DIELECTRIC PHENOMENA IN SOLIDS With Emphasis on Physical Concepts of Electronic Processes
DIELECTRIC PHENOMENA IN SOLIDS With Emphasis on Physical Concepts of Electronic Processes
Kwan Chi Kao Professor Emeritus of Electrical and Computer Engineering University of Manitoba
AMSTERDAM • BOSTON • HEIDELBERG • LONDON NEW YORK • OXFORD • PARIS • SAN DIEGO SAN FRANCISCO • SINGAPORE • SYDNEY • TOKYO
Elsevier Academic Press 525 B Street, Suite 1900, San Diego, California 921014495, USA 84 Theobald’s Road, London WC1X 8RR, UK This book is printed on acidfree paper.
Copyright 2004, Elsevier, Inc. All rights reserved. No part of this publication may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopy, recording, or any information storage and retrieval system, without permission in writing from the publisher. Permissions may be sought directly from Elsevier’s Science & Technology Rights Department in Oxford, UK: phone: (+44) 1865 843830, fax: (+44) 1865 853333, email:
[email protected] You may also complete your request online via the Elsevier Science homepage (http://elsevier.com), by selecting “Customer Support” and then “Obtaining Permissions.” Library of Congress CataloginginPublication Data Kao, Kwan Chi. Dielectric phenomena in solids: with emphasis on physical concepts of electronic processes / Kwan Chi Kao. p. cm. Includes bibliographical references and index. ISBN 0123965616 (alk. paper) 1. Dielectrics. I. Title. QC585.K36 2004 537¢.24–dc22 2003070901 British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library ISBN: 0123965616 For all information on all Academic Press publications visit our website at www.academicpress.com Printed in the United States of America 04 05 06 07 08 9 8 7 6 5
4
3
2
1
Dedicated to my aunt, Hui Jien, my sister, Chih Hai, and my daughter, Hung Jien, whose love has contributed so much to my strength and faith.
Contents Preface 1 INTRODUCTION 1.1 Maxwell’s Equations 1.1.1 Ampere’s Law 1.1.2 Faraday’s Law 1.1.3 Inseparable Magnetic Poles 1.1.4 Gauss’s Law 1.2 Magnetization The Orbital Motion of Electrons around the Nucleus of an Atom The Rotation of Electrons about Their Own Axis in an Atom The Rotation of Protons and Neutrons inside the Nucleus 1.2.1 Diamagnetism 1.2.2 Paramagnetism 1.2.3 Ferromagnetism 1.2.4 Magnetostriction 1.2.5 Magnetic Materials 1.2.6 Magnetic Resonance Nuclear Magnetic Resonance (NMR) Electron Paramagnetic Resonance (EPR) Electron Spin Resonance (ESR) 1.2.7 Permanent Magnets 1.2.8 Magnetic Memories 1.3 Electromagnetic Waves and Fields 1.4 Dimensions and Units 1.4.1 Length 1.4.2 Mass 1.4.3 Time 1.4.4 Electric Charge 1.4.5 Derived Units 1.4.6 Cgs System of Units and Cgs/SI Conversion
1.4.7 The Unit of Debye 1.4.8 The Chemical Unit of Mole References
xiv 1 2 3 5
ELECTRIC POLARIZATION AND RELAXATION 2.1 Fundamental Concepts 2.1.1 Electric Charge Carriers and Their Motion 2.1.2 Electromechanical Effects The Force Acting on the Boundary between Two Different Dielectric Materials The Force Acting on Conductor Surfaces The Force Elongating A Bubble or A Globule in A Dielectric Fluid The Dielectrophoretic Force The Electrostriction Force The Torque Orientating A Solid Body 2.1.3 Electrostatic Induction 2.2 Electric Polarization and Relaxation in Static Electric Fields 2.2.1 Vacuum Space 2.2.2 Conducting Materials 2.2.3 Dielectric Materials 2.3 The Mechanisms of Electric Polarization 2.3.1 Electronic Polarization (Also Called Optical Polarization) Classical Approach Quantum Mechanical Approach 2.3.2 Atomic or Ionic Polarization (Vibrational Polarization) 2.3.3 Orientational Polarization
38 38 38
2
8 9 9
11
12
12 13 15 18 23 23 26 27 28 30 30 30 32 34 34 35 35 35 35 36 vii
41 41 41 44
47 47
48 49 49 50 51
52 53 53 54 58
59 59 64
65 67
viii
Contents
2.3.4 Spontaneous Polarization 2.3.5 Space Charge Polarization Hopping Polarization Interfacial Polarization 2.4 Classification of Dielectric Materials 2.4.1 Nonferroelectric Materials (Normal Dielectric or Paraelectric Materials) Nonpolar Materials Polar Materials Dipolar Materials 2.4.2 Ferroelectric Materials 2.5 Internal Fields 2.5.1 Local Fields for Nondipolar Materials The Clausius–Mosotti Equation The Lorentz–Lorenz Equation 2.5.2 The Reaction Field for Dipolar Materials The Debye Equation The Onsager Equation StatisticalMechanical Approaches and the Kirkwood Equation The Frohlich Equation 2.6 Electric Polarization and Relaxation in TimeVarying Electric Fields 2.6.1 The TimeDomain Approach and the FrequencyDomain Approach 2.6.2 Complex Permittivity 2.6.3 Time Dependent Electric Polarization Case A Case B 2.6.4 Kramers–Kronig Equations 2.6.5 Debye Equations, Absorption, and Dispersion for Dynamic Polarizations The Effects of the Local Field The Effects of DC Conductivity
74 75 75 77
79
2.6.6 The Cole–Cole Plot 2.6.7 Temperature Dependence of Complex Permittivity 2.6.8 Field Dependence of Complex Permitivitty Semiconducting Materials Ferroelectric Materials Insulating Materials 2.7 Dielectric Relaxation Phenomena 2.7.1 The Hamon Approximation 2.7.2 Distribution of Relaxation Times 2.7.3 The Relation between Dielectric Relaxation and Chemical Structure References
80
3
78
78 78 78 78 79 79
80 81 82 83
84 85 86
86 86 87 89 89 91
92 94 94
OPTICAL AND ELECTROOPTIC PROCESSES 3.1 Nature of Light 3.1.1 Corpuscular Theory The Outstanding Difference between Photons and Electrons or Protons Frequency, Energy and Momentum of Photons 3.1.2 Wave Theory Principle of Superposition Interference and Interferometry Diffraction Polarization, Reflection and Refraction 3.2 Modulation of Light 3.2.1 Double Refraction and Birefringence QuarterWave Plate (QWP) Optical Activity 3.2.2 ElectroOptic Effects The Pockels Effect or Linear ElectroOptic Effect The Kerr Effect or Quadratic ElectroOptic Effect ElectroOptic Ceramics 3.2.3 The Photorefractive Effect 3.2.4 The MagnetoOptic Effect The Faraday Effect The Voigt Effect
95 97 100 100 101 102 105 105 108
110 112
115 115 115
115 115 116 117 118 121 123 128 128 130 131 131
131 133 136 138 142 142 142
Contents
3.2.5 The AcoustoOptic Effect 3.3 Interaction between Radiation and Matter 3.3.1 Generation of Radiation Thermal Radiation Luminescent Radiation Units of Light 3.3.2 The Franck–Condon Principle 3.3.3 Radiative and Nonradiative Transition Processes MultiplePhonon Transition Auger Recombination Processes Nonradiative Transition due to Defects Nonradiative Transition in Indirect Bandgap Materials 3.3.4 Absorption and Dispersion 3.3.5 The Franz–Keldysh Effect 3.3.6 Formation and Behavior of Excitons Exciton Transport Processes Exciton Interactions 3.4 Luminescence 3.4.1 Photoluminescence Fluorescence Phosphorescence and Phosphors 3.4.2 Electroluminescence Classical Electroluminescence Injection Electroluminescence 3.5 Photoemission 3.5.1 Photoemission from Electrical Contacts From a Metal into Wide Bandwidth Semiconductors From a Narrow Bandwidth Emitter into Wide Bandwidth Semiconductors From a Metal into Narrow Bandwidth Crystals
143 144 144 144 145 145 146 146 150 150 152
152 154 157 158 161 162 164 165 165
3.5.2 Photoemission from Crystalline Solids Effects of Surface Conditions Effects of Defects in Crystals Energy Distribution of Emitted Electrons Multiquantum Processes 3.6 Photovoltaic Effects 3.6.1 Bulk Photovoltaic Effects The Dember Effect The PhotoelectroMagnetic (PEM) Effect 3.6.2 Contact Potential Photovoltaic Effects Schottky Barrier Photovoltages MIS Solar Cells Photovoltaic Behavior of PN Junctions PIN Structures for Amorphous Sibased Photovoltaic Devices 3.6.3 Photosynthesis Photovoltaic Effects 3.6.4 Anomalous Photovoltaic Effects References
185 188 188 189 189 191 191 192 194 194 194 196 196
201 203 206 207
4 169 171 171 173 181 181
182
184 184
FERROELECTRICS, PIEZOELECTRICS, AND PYROELECTRICS 4.1 Introductory Remarks 4.2 Ferroelectric Phenomena 4.2.1 General Features 4.2.2 Phenomenological Properties and Mechanisms BaTiO3Type Ferroelectrics KH2PO4Type Ferroelectrics KNaC4H4O6 • 4H2O (Rochelle Salt)Type Ferroelectrics (NH2CH2COOH)3 • H2SO4Type Ferroelectrics Alloys of PbO, ZrO2, and TiO2 (PZT alloys)Type Ferroelectric Ceramics
ix
213 213 216 216 221 221 227
228 229
230
x
Contents
PVDF [(CH2CF2)n]Type Ferroelectric Polymers 4.2.3 Thermodynamic Theory Ferroelectric Transition Antiferroelectric Transition 4.2.4 Formation and Dynamics of Domains 4.2.5 Ferroelectric Materials 4.2.6 Applications of Ferroelectrics Capacitors ThermoAutostabilization Nonlinear Dielectric Elements (TANDEL) HighEnergy Electrical Pulse Generators Memories 4.3 Piezoelectric Phenomena 4.3.1 Phenomenological Approach to Piezoelectric Effects 4.3.2 Piezoelectric Parameters and Their Measurements 4.3.3 Piezoelectric Materials 4.3.4 Applications of Piezoelectrics Gas Igniters Delay Lines Piezoelectric Positioners and Actuators Piezoelectrc Transformers 4.4 Pyroelectric Phenomena 4.4.1 Phenomenological Approach to Pyroelectric Effects 4.4.2 Pyroelectric Parameters and Their Measurements 4.4.3 Pyroelectric and Thermally Sensitive Materials NTC Materials PTC Materials 4.4.4 Applications of Pyroelectrics Pyroelectric Radiation Detectors Pyroelectric Burglar Alarm Systems Pyroelectric Thermometry Pyroelectric Energy Conversion References
234 236 238 241 242 246 249 249
252 252 255 257 257 262 264 266 266 267 267 268 269 270 271 272 273 274 275 275 278 278 279 279
5 ELECTRETS 5.1 Introductory Remarks 5.2 Formation of Electrets 5.2.1 ThermoElectrical Method 5.2.2 LiquidContact Method 5.2.3 Corona Discharge Method 5.2.4 ElectronBeam Method 5.2.5 Electromagnetic Radiation Method 5.3 Charges, Electric Fields and Currents in Electrets Case I: The Electret Has Only Surface Charges Case II: The Electret Has Both Surface Charges s(d) and Volume Charges r(x) 5.4 Measurements of Total Surface Charge Density and Total Charges 5.4.1 Total Surface Charge Density Compensation Method Capacitive Probe Method 5.4.2 Total Charges per Unit Planar Area QT Electrostatic Induction or Faraday Pail Method Thermal Pulse Method 5.5 Charge Storage Involving Dipolar Charges 5.5.1 Basic Poling Processes 5.5.2 Relaxation Times of Dipoles and the Thermally Stimulated Discharge Currents (TSDC) Technique 5.5.3 Spatial Distribution of Dipolar Polarization 5.5.4 Isothermal Polarization Decay Processes 5.6 Charge Storage Involving Real Charges 5.6.1 Spatial Distributions of Trapped Real Charges Sectioning Method Electron Beam Sampling Method Pulsed ElectroAcoustic Method
283 283 284 284 287 288 289 290 290 292
293 294 294 294 295 296 296 296 297 297
298 302 302 303 303 303 304 305
Contents
Other Methods 5.6.2 Energy Distribution of Trapped Real Charges 5.6.3 Isothermal Real Charge Decay Processes Stage 1: For t £ tto Stage 2: for t ≥ tto 5.6.4 Distinction between Dipolar Charges and Real Charges 5.7 Basic Effects of Electrets 5.8 Materials for Electrets 5.8.1 General Remarks 5.8.2 Physical Properties 5.9 Applications of Electrets 5.9.1 Electret Microphones 5.9.2 Electromechanical Transducers 5.9.3 Pyroelectric Detectors 5.9.4 Other Applications References CHARGE CARRIER INJECTION FROM ELECTRICAL CONTACTS 6.1 Concepts of Electrical Contacts and Potential Barriers 6.1.1 Electrical Contacts, Work Functions, and Contact Potentials Contact Potential Measurements Photoelectric Emission Method Thermionic Emission Method 6.1.2 Types of Electrical Contacts Neutral Contacts Blocking Contacts Ohmic Contacts 6.1.3 Surface States 6.2 Charge Carrier Injection through Potential Barriers from Contacts 6.2.1 Potential Barrier Height and the Schottky Effect Neutral Contacts Blocking Contacts 6.2.2 Thermionic Emission Effect of Effective Mass
308 308 310 311 311
312 313 316 316 316 321 321 322 322 323 323
6
327 327
328 330
Correction due to Drift and Diffusion of Carriers in the Depletion Region Effects of Phonon Scattering and QuantumMechanical Reflection Other Factors 6.2.3 Field Emission Without the Effects of Defects in Solids With the Effects of Defects in Solids 6.2.4 ThermionicField Emission 6.3 Tunneling through Thin Dielectric Films between Electrical Contacts 6.3.1 Analysis Based on a Generalized Potential Barrier For T = 0 For T > 0 6.3.2 Elastic and Inelastic Tunneling 6.3.3 Tunneling Through a MetalThin Insulation Film–Semiconductor (MIS) System 6.3.4 Effects of Space Charges and Traps on Tunneling Efficiency and Impurity Conduction 6.4 Charge Transfer at the MetalPolymer Interface References
xi
350
352 352 354 354 358 363 364
364 366 366 367
371
374 376 378
330 7 330 334 334 336 336 341 345 345 345 347 350 350
ELECTRICAL CONDUCTION AND PHOTOCONDUCTION PART I: ELECTRICAL CONDUCTION 7.1 Introductory Remarks 7.2 Ionic Conduction 7.2.1 Intrinsic Ionic Conduction 7.2.2 Extrinsic Ionic Conduction 7.2.3 Effects of Ionic Conduction 7.3 Electronic Conduction 7.3.1 Electrical Transport Band Conduction DefectControlled Conduction Electrical Transport by a Tunneling Process
381 381 381 382 383 385 385 387 389 389 398 399
xii
Contents
Electrical Transport by a Hopping Process 401 Polaron Conduction 402 7.3.2 Lifetime and Relaxation Electrical Conduction 403 Lifetime Regime 403 Relaxation Regime 404 7.4 Bulk Limited Electrical Conduction 406 7.4.1 Basic Concepts Relevant to Space Charge Limited Electrical Conduction 406 7.4.2 SCL Electrical Conduction: One Carrier (Single) Planar Injection 408 Theoretical Analyses 408 The Scaling Rule 420 The Effect of Carrier Diffusion 422 7.5 Bulk Limited Electrical Conduction Involving Two Types of Carriers 423 7.5.1 Physical Concepts of Carrier Trapping and Recombination 423 Capture Rates and Capture CrossSections 425 Recombination Rates and Recombination CrossSections 426 Demarcation Levels 427 Coulombic Traps 430 Characteristic Times 432 7.5.2 Kinetics of Recombination Processes 433 BandtoBand Recombination without Involving Recombination Centers or Traps 434 With a Single Set of Recombination Centers but without Traps 435 7.5.3 SpaceCharge Limited Electrical Conduction: TwoCarrier (Double) Planar Injection 437 Without Recombination Centers and without Traps 438 With Recombination Centers but without Traps 440 7.6 HighField Effects 443
7.6.1 Filamentary ChargeCarrier Injection in Solids Filamentary OneCarrier (Single) Injection Filamentary TwoCarrier (Double) Injection 7.6.2 The Poole–Frenkel Detrapping Model 7.6.3 The Onsager Detrapping Model 7.6.4 FieldDependent Carrier Mobilities 7.7 Transitions between Electrical Conduction Processes 7.7.1 Basic Transition Processes A Solid between Similar Contacts A Solid between Dissimilar Contacts 7.7.2 Transition from BulkLimited to ElectrodeLimited Conduction Process 7.7.3 Transition from ElectrodeLimited to BulkLimited Conduction Process 7.7.4 Transition from SingleInjection to DoubleInjection Conduction Process 7.8 Current Transient Phenomena 7.8.1 SpaceCharge Free (SCF) Transient Case 1: In the Absence of Traps and Diffusion Case 2: In the Absence of Diffusion but with Traps 7.8.2 SpaceCharge Limited (SCL) Transient Case 1: In the Absence of Traps and Diffusion Case 2: In the Absence of Diffusion but with Traps 7.8.3 SpaceCharge Perturbed (SCP) Transient Carrier Generation by a Strong Light Pulse Carrier Generation by a Weak Light Pulse
443 444 446 447 449 451 455 455 455 459
460
461
462 463 466 466 466 468 468 470 470 470 471
Contents
7.9 Experimental Methodology and Characterization 7.9.1 Simultaneous Measurements of Charging Current and Photocurrent Transients 7.9.2 Alternating Measurements of the I–V and C–V Characteristics 7.9.3 Measurements of Surface Potentials 7.9.4 Capacitance Transient Spectroscopy PART II: PHOTOCONDUCTION 7.10 Quantum Yield and Quantum Efficiency for Photoconduction 7.11 Generation of Nonequilibrium Charge Carriers 7.11.1 Energy Distribution of Nonequilibrium Charge Carriers 7.11.2 Spatial Distribution of Nonequilibrium Charge Carriers 7.11.3 Lifetimes of Nonequilibrium Charge Carriers Linear Recombination Quadratic Recombination Instantaneous Lifetimes 7.12 Photoconduction Processes 7.12.1 Intrinsic Photoconduction 7.12.2 Extrinsic Photoconduction Photocurrent—Voltage Characteristics Light Intensity Dependence Light Wavelength Dependence Temperature Dependence Effects of Surface Conditions and Ambient Atmosphere 7.12.3 Homogeneous and Nonhomogeneous Photoconduction Homogeneous Photoconduction Nonhomogeneous Photoconduction 7.12.4 Photoresponse Times
472
7.13 Photosensitization 7.14 Transient Photoconduction References
503 505 509
8 472
472 477 478 480 480 482
484
484 486 486 488 489 490 490 490 491 494 495 496
497
497 497 499 500
ELECTRICAL AGING, DISHCARGE, AND BREAKDOWN PHENOMENA 8.1 Electrical Aging 8.1.1 Theory 8.1.2 Measurements of Electrical Aging Electron Paramagnetic Resonance (EPR) Spectroscopy Infrared (IR) Absorption Spectroscopy Surface Potential Measurements Small Angle Scattering of XRays (SASX) Spectroscopy Lifetime Evaluation Other Measurements 8.1.3 Remedy for Electrical Aging Emission Shields Radical Scavengers 8.2 Electrical Discharges 8.2.1 Internal Discharges Fundamental Features of Internal Discharges in a Cavity Discharge Current Impulses, Recurrence, Discharge Magnitudes, Discharge Energy, and Power Losses 8.2.2 Electrical Treeing Prebreakdown Disturbances and Light Emission Mechanisms and Characterization of Electrical Treeing Some Special Features of Electrical Treeing Inhibition of Electrical Treeing Electrical Treeing Initiated by Water Trees
xiii
515 515 515 520
521 522 523
523 524 525 525 525 526 528 528
529
530 540 540
542 543 545 545
xiv
Contents
8.2.3 Surface Discharges and Corona Discharges 8.2.4 Detection of Partial Discharges 8.3 Electrical Breakdown 8.3.1 Electrical Breakdown in Gases Townsend Discharges Streamer Discharges Discharges in Electronegative Gases Paschen’s Law 8.3.2 Electrical Breakdown in Liquids
546 547 549 549 551 553 555 555 557
8.3.3 Electrical Breakdown in Solids Thermal Breakdown Electrical Breakdown 8.3.4 Similaritiy in Breakdown Mechanisms for Gas, Liquid, and Solid Dielectrics References
567 569
Index
573
559 559 560
Preface responsible for the macroscopic electrical and optical properties of the materials. In dielectric materials, carrier traps arising from various structural and chemical defects and their interactions with charge carriers injected from electrical contacts or other excitation sources always play major roles in dielectric phenomena. In today’s high technology era, the trend of electronics has been directed to the use for some solidstate devices of some dielectric materials, such as ceramics, which have good insulating properties as well as some special features such as spontaneous polarization. Therefore, a chapter dealing with ferroelectric, piezoelectric, pyroelectric, and electrooptic phenomena, as well as a chapter dealing with electrets, are also included in this book. The theoretical analyses are general. We have endeavored throughout this book to keep the mathematics as simple as possible, and emphasized the physical insight of the mechanisms responsible for the phenomena. We use the international MKSC system (also called the SI system, the International System of Units [Systeme Internationale]) in which the unit of length is meter (m), the unit of mass is kilogram (kg), the unit of time is second (s), and the fourth unit of electrical charge is Coulomb (C), because all other units for physical parameters can easily be derived from these four basic units. It should be noted that to deal with such vast subjects, although confined to the area of dielectric phenomena in only nonmetallic and nonmagnetic materials, it is almost unavoidable that some topics are deliberately overemphasized and others discussed minimally or even excluded. This is not because they are of less importance, but rather, it is because of the limited size of this book. However, an understanding of dielectric phenomena requires knowledge of the basic physics of Maxwell’s equations and the general electromagnetic
The word dielectric is derived from the prefix dia, originally from Greek, which means “through” or “across”; thus, the dielectric is referred to as a material that permits the passage of the electric field or electric flux, but not particles. This implies that the dielectric does not permit the passage of any kind of particles, including electrons. Thus, it should not conduct the electric current. However, a dielectric is generally considered a nonconducting or an insulating material. There is no ideal dielectric in this planet. The perfect vacuum may be considered to be close to the ideal dielectric, but a perfect vacuum cannot be obtained on Earth. A vacuum of 1014 torr still consists of about 300 particles per cubic centimeter. All real dielectric materials are imperfect, and thus permit, to a certain degree, the passage of particles. We have to coexist with the imperfections. This book deals mainly with the phenomena resulting from the responses of the solid dielectric materials to external applied forces such as electromagnetic fields, mechanical stress, and temperature. The materials considered are mainly nonmetallic and nonmagnetic materials, which are generally not considered as dielectric materials. There is no clear demarcation between dielectrics and semiconductors. We can say that the major difference lies in their conductivity and that the dominant charge carriers in semiconductors are generated by the thermal excitation in the bulk, while those in dielectric materials come from sources other than the thermal excitation, including carrier injection from the electrical contacts, optical excitations, etc. This book will not include semiconductors as such, but certain dielectric phenomena related to semiconductors will be briefly discussed. Dielectric phenomena include induced and spontaneous electric polarizations, relaxation processes, and the behavior of charge carriers xv
xvi
Preface
theory. Thus, in the first chapter, Introduction, we have described rather briefly the basic concepts of the magnetization and the ferromagnetism that are analogous to the counterpart of the electric polarization and the ferroelectricity, and also the electromagnetic waves and fields. The reader may be familiar with much of the content of that chapter, but may still find it useful as background knowledge for the main topics of dielectric phenomena in the following chapters. I would like, first, to thank gratefully my former colleagues and students for their cooperation and encouragement, and particularly, Professor Demin Tu of Xi’an Jiaotong University for his longterm collaboration with my research team on many projects related to prebreakdown and breakdown phenomena. I would like to express my appreciation to the Faculty of Engineering at the University of Manitoba for the provision of all facilities in the course of the writing of this book. I wish especially to thank my sons Hung Teh and Hung Pin, and my daughters Hung Mei and Hung Hsueh, and their families for all the love
and support; Hung Pin and his wife Jennifer Chan for their weekly “good wishes” by telephone from California. I am also very thankful to Hung Hsueh and the staff of the Sciences and Technology Library of the University of Manitoba for obtaining all the references I needed for the writing. I also want to thank some of my close friends, and in particular, Chang Chan, SiuYi Kwok, HungKang Hu, PiChieh Lin, JiaYu Yang, and FengLian Wong for their unfailing constant care and support, which have contributed so much to my patience and confidence in dealing with the writing. Finally, I am deeply indebted to Ms. Karin Kroeker for her skillful typing and her patience in typing the mathematical expressions, and to the editors, Mr. Charles B. Glaser and Ms. Christine Kloiber of Academic Press for their helpful cooperation and prompt actions. Last but not least, I would like to acknowledge gratefully the publishers and societies for permission to reproduce illustrations. The publishers and societies are listed in the following table.
Publisher or Society American Institute of Physics
Book or Journal J. Appl. Phys.
American Institute of Physics American Institute of Physics
Appl. Plys. Lett. J. Chem. Phys. Soviet Phys.—Solid State Phys. Rev
American Physical Society
American Chemical Society American Vacuum Society American Ceramic Society IEEE Dielectrics and Electrical Insulation Society John Wiley and Sons
J. Amer. Chem. Soc. J. Vac. Sci. Tech Amer. Ceram. Soc. Bull. J. Amer. Ceram. Soc. IEEE Trans. Electr. Insul. IEEE Electrical Insulation Magazine
Figure 322, 351, 616, 619, 623, 624, 632, 725, 726, 743, 745, 747, 748, 759(b), 86, 87, 88, 810, 811, 812 423 346, 737, 754 369 337, 363, 411, 412, 417, 418, 425, 628, 630, 635, 718, 719, 759(a) 218 840 320 420 520, 822, 823 519
J. Appl. Polymer Sci. J. Polymer Sci.—Physics
738, 85, 89, 813 516
Preface
Publisher or Society
Institute of Physics (London) Physical Society of Japan Australian Chemical Society Physica Status Solidi Steinkopff, Darmstadt Electrochemical Society Pergamon Press
MOSES King (Cambridge) Materials Research Society IEEE Dielectric and Electrical Insulation Society American Institute of Physics Clarendon (Oxford)
North Holland (Amsterdam) SpringerVerlag (New York) Elsevier
Plenum (New York) Springer Verlag (New York) Dover Academic Press MacMillan (New York) Clarendon (Oxford)
Clarendon (Oxford)
Book or Journal J. Polymer Science—Polym. Phys. Ed. J. Phys. D: Appl. Phys. J. Phys. Soc. Japan Aust. J. Chem. Phys. Stat. Sol. Kolloid Z. J. Electrochem. Soc. Solid State Commun. Solid State Electronics J. Phys. Chem. Solids Science MRS Bulletin 2000 IEEE International Symposium on Electrical Insulation Proc. 1965 International Symposium on Thin Film Physics Theory of Dielectrics (H. Frohlich) HighField Transport In Semiconductors (E.M. Conwell) Ferroelectricity (E. Fatuzzo and W.J. Merz) Electrets (G.M. Sessler) Thermally Stimulated Discharge of Polymer Electrets (J. Van Turnhout) Principles of Fluorescence Spectroscopy (J.R. Lakowicz) Electroluminescene (J.I. Pankove) Optical Processes in Semiconductors (J.I. Pankove) Piezoelectric Ceramics (B. Jaffe, W.R. Cook and H. Jaffe) Ferroelectric Crystals (F. Jona and G. Shirane) Electronic Process in NonCyrstalline Materials (N.F. Mott and E.A. Davis) Ionized Gases (A. Von Engel)
xvii
Figure 442 75, 76 421 734 736 242 834 352, 825 345, 625, 626, 727 347, 348 422 368 435
615 214 237 238 514 515, 523
340 344 370 419, 441 413, 414, 415, 416 634
829
Kwan Chi Kao Winnipeg, Manitoba, Canada
1
Introduction
Learning without thought is labor forgone; thought without learning is perilous. Confucius (600 BC)
such as bits of chaff. In Greek, “amber” was referred to as electricity. However, it is now well known that many substances possess this property to some extent. A glass or metal rod, after being rubbed with a polyester sheet, will attract a light piece of paper. This attraction phenomenon may be considered due to the charge on the rod tip polarizing the paper nearby. The electric polarization produces an opposite charge on the paper surface close to the charged rod tip, resulting in this attraction. Any electromagnetic wave will induce polarization in dielectric materials and magnetization in magnetic materials. Both the polarization and the magnetization also produce their own fields, which interact with the external fields, resulting in a vast scope of dielectric and magnetic phenomena. However, dielectric phenomena did not receive much attention until the middle of the 18th century, although the Leyden jar condenser, which could store charges, was discovered in 1745 by the Dutch physicist van Musschenbrack, of the University of Leyden.1 About 90 years later (in 1837) Faraday, in England, was the first to report2 that the capacitance of a condenser was dependent on the material inside the condenser. At that time, he called the ratio of the capacitance of the condenser filled with a dielectric material to that of the same condenser, empty inside (free space), the specific inductive capacity, which is now called the permittivity. In 1873, following the discovery of Coulomb’s law on forces between charges, Ohm’s law on electrical conductivity, Faraday’s law, and Ampère’s law on magnetic and electric induction, Maxwell3 welded these
The basic distinction between a semiconductor and a dielectric (or insulator) lies in the difference in the energy band gap. At the normal ranges of temperatures and pressures, the dominant charge carriers in a semiconductor are generated mainly by thermal excitation in the bulk because the semiconductor has a small energy band gap; hence, a small amount of energy is sufficient to excite electrons from full valence band to an upper empty conduction band. In a dielectric, charge carriers are mainly injected from the electrical contacts or other external sources simply because a dielectric’s energy band gap is relatively large, so a higher amount of energy is required for such bandtoband transitions. A material consists mainly of atoms or molecules, which comprise electrons and nuclei. The electrons in the outermost shell of atoms, bound to the atoms or molecules coupled with the free charges, interact with external forces, such as electric fields, magnetic fields, electromagnetic waves, mechanical stress, or temperature, resulting in the occurrence of all dielectric phenomena. For nonmagnetic dielectric materials, the dielectric phenomena include mainly electric polarization; resonance; relaxation; energy storage; energy dissipation; thermal, mechanical, and optical effects and their interrelations; and electrical aging and destructive breakdown. The discussion of these phenomena is the scope of this book. Dielectric phenomena, like other natural phenomena, were noticed long before the time of Christ. As early as 600 bc, the Greek philosopher Thales discovered that amber, when rubbed with cloth, attracted light objects 1
2 Dielectric Phenomena in Solids
discoveries together to formulate a unified approach. He developed four equations, known as Maxwell’s equations, to govern all the macroscopic electromagnetic phenomena. Obviously, dielectric phenomena are part of the electromagnetic phenomena, which result from the interaction of the material with electromagnetic fields. Therefore, it is very important to understand the meaning of these four equations.
1.1
Maxwell’s Equations
Maxwell’s four equations are —¥H =J+ —¥F=
∂D ∂t
∂B ∂t
(11) (12)
—•B= 0
(13)
—•D= r
(14)
where F, D, H, and B are four vectors denoting, respectively, the electric field, the electric flux density (or electric displacement), the magnetic field, and the magnetic flux density (or magnetic induction); J is also a vector denoting the electric current density; and r is a scalar quantity denoting a net charge density. These equations imply that at any point inside a material there exist four vectors—F, D, H, and B— when that material is subjected to an external electromagnetic field, and that the distribution of the electric current may be considered the conservation of the electric charges, which give rise to the electromagnetic field. In other words, Maxwell’s equations describe the coupling between the electric field and the magnetic field and their interaction with the material, resulting in all electromagnetic phenomena. The parameter B may be linked to parameter H, and so D to F and J to F, by the following relations: B = mH
(15)
D = eF
(16)
J = sF
(17)
where m, e and s are, respectively, the permeability, the permittivity, and the conductivity of the material (medium). Microscopic theory may deduce the physical properties of a material from its atomic structure, which may be generally represented by these three parameters: m, e, and s. The nature of these parameters is directly associated with the aggregate effect of the deformation of the atomic structure and the movement of electric charges caused by the electromagnetic field, which is mainly due to magnetization, polarization, and electrical conduction. We shall discuss the polarization and electrical conduction in some detail in later chapters. As we shall confine ourselves to dealing only with nonmagnetic materials, we will discuss magnetization only briefly in this chapter, with the aim of clarifying the difference between magnetic and nonmagnetic materials. In this world, there is no lossless material as such. All materials are lossy. Only in a perfect vacuum can there be there no loss and, hence, no dispersion in the presence of an electromagnetic field. In practice, we cannot achieve a perfect vacuum on earth. Even at the pressure of 1014 torr, the lowest pressure (or the best vacuum) that today’s technology can achieve, there are still about 300 particles per cubic centimeter. However, at the normal range of temperatures and pressures, the gas media can be considered to be very close to the socalled free space. In free space, we have mo = 4p ¥ 10 7 henry m 1 = 1.257 ¥ 10 6 henry m 1
According to wave theory, the velocity of electromagnetic waves (light) in free space is c = ( moe o )1 2 = 2.998 ¥ 108 ms 1 = 3 ¥ 108 ms 1
From this, eo in free space is e o = 8.854 ¥ 10 12 farad m 1 = (36p ¥ 10 9 )1 farad m 1
Obviously, in free space s = 0 and J = 0. In isotropic media, we would expect that at any point D and J are parallel to F, and B is
Introduction
parallel to H. The beauty of the Maxwell’s equations is that a vast scope of electromagnetic phenomena can be described with only a few variables. Usually, we use the relative values of m and e, which are expressed as mr = m mo
(18)
er = e eo
(19)
mr and er are called, respectively, the relative permeability and the relative permittivity (or simple dielectric constant). The parameters mr, er, and s generally characterize the electromagnetic properties of materials. Thus, information about the dependence of these parameters on some physical variables, such as density, temperature, field intensity, and frequency, would shed much light on the internal structure of matter. As Maxwell’s equations govern both the electrical and the magnetic properties of matter, as well as all electromagnetic phenomena in any medium, it is important to understand the physics and the historical development behind these equations. Faraday discovered not only the dependence of the capacitance of a condenser on the material filled between the two metallic plates, but also the induction law, which involves a voltage induced in a coil when a timevarying magnetic field is in the region surrounded by the coil. At about the same time, Henry, in the United States, discovered the selfinduction of the electric current, which led to the development of electromagnets. In fact, about 10 years before this discovery, in 1820, the Danish scientist Oersted observed the magnetic effect of an electric current.1 After the announcement of Oersted’s discovery, the French scientist Ampère discovered, in about 1824, the circuital law: the line integral of the magnetic field intensity around any closed path is equal to the total current linked with that path. 1.1.1 Ampère’s Law Suppose we have an iron core with a gap filled with air or a nonmagnetic material, with a uniform crosssection area A, and a mean magnetic flux path length m around the iron core
3
and a length a across the gap, as shown in Figure 11(a). When the coil of N turns around the core carries a current i, then (ignoring any flux leakage traversing the path for mathematical simplicity) the magnetomotance (usually called the magnetomotive force, mmf ) Um can be expressed by Um = Hm l m + Ha l a = Ni
(110)
where Hm and Ha are, respectively, the magnetic field intensities in the iron core and the gap. Since the magnetic flux f is continuous, as is the magnetic flux density B, f and B are the same in the iron core and in the gap. Thus, B = Bm = Ba =
f A
(111)
and Equation 110 may be written in the form Ni = B
Ê lm ˆ Ê mm la ˆ 1+ Ë mm ¯ Ë ma l m ¯
(112)
This shows that for a fixed magnetizing current i, the smaller the gap length la, the larger the magnetic flux density B. This is the general feature of electromagnets. We can write Equation 110 in general form as
ÂH l
i i
(113)
= Ni
i
A coil with N turns carrying a current i is the same as a coil with only one turn but carrying a current I = Ni. Since the north and south magnetic poles are inseparable, the magnetic flux lines must close on themselves. Considering these facts, Equation 113 can be written as
Ú Hdl = I = Ú J • nds c
a
(114)
where n is the unit vector normal to the surface. According to Stokes’s theorem, the line integral of a vector around the boundary of a surface with an area S is equal to the surface integral of the curl of the same vector over the area bound by the path of this vector, as illustrated in Figure 11(b). So we can write
Ú (— ¥ H )• nds = Ú Hdl s
c
(115)
4 Dielectric Phenomena in Solids f Iron Core
m a
i
V
Gap Filled with Air or Nonmagnetic Material
N
N Turns
S
Cross Section A
Total Coil Resistance R
(a) Cross Section a J
Th
a
e
Pa
th
of
M
ag
m
ne
tic
Fl
ux
f
1 Turn
Enclosed Surface with Area S
(b) Figure 11 Schematic diagrams illustrating (a) Ampère’s circuital law and an electromagnet and (b) Stokes’s theorem based on the flux path in (a).
The surface can be an arbitrary surface, provided that it includes the current passing through the surface. This implies that Ú J • n ds = Ú J • n ds. Thus, from Equations 114 and 115 we obtain
Ú (— ¥ H )• n ds = Ú J • n ds s
s
(116)
These two surface integrals are equal; thus, we have —¥H=J
(117)
This equation is valid for both the steady current (DC) and the timevarying current (AC, or pulse or transient current). For the steady current (DC), f becomes constant, and hence,
Introduction
df = 0, but for the timevarying current (such dt as AC), the total current may also involve the ∂D displacement current . If this is the case, ∂t Equation 117 must be written as ∂D —¥H =J+ ∂t
(118)
This is the Ampère’s circuital law, which forms the first equation of Maxwell’s equations. Depending on the situation, Equation 118 may ∂D =0 involve only conduction current, with ∂t (such as the magnetic fields in electrical machines), or it may involve only displacement current with J = 0 (such as the electromagnetic waves in free space). It should be noted that — ¥ H = 0 does not happen, because this means mathematically4–6 that there exists a scalar field such that H is equal to — (scalar field), but such a scalar field does not exist in magnetic circuits. This also implies that the north and south magnetic poles are inseparable. 1.1.2 Faraday’s Law Electromagnetic induction is a very interesting and important phenomenon, so we include here a brief discussion about the physics behind it. Let us return to the electromagnet system shown in Figure 11(a). Suppose the coil of copper wire, with a total resistance R, is connected to a DC voltage V through a switch. As soon as the switch is turned on, a magnetic flux will be induced in the magnetic circuit. During the time internal dt, energy equal to Vidt will be supplied to the system from the DC source, of which i2Rdt energy (as heat loss) will be consumed in the coil, leaving (Vi  i2R)dt in energy stored in the magnetic field dWm = (V  iR)idt
(119)
During the time interval, the magnetic flux changes with time: df/dt. This change in magnetic flux, according to Faraday’s induction law, will produce voltage equal to XN df/dt. Thus, during dt, the stored energy dWm should be
df dWm = i Ê N ˆ dt Ë dt ¯
5
(120)
From Equations 119 and 120, we obtain df dt = V + Vi R R
VN i=
(121)
where Vi is the induced voltage, which is Vi =  N
df dt
(122)
Equation 122 means that whenever the current or its accompanying magnetic flux changes with time, a voltage Vi will be generated in the circuit, called the induced voltage, with the polarity opposite to the source voltage and the magnitude equal to the time rate of change of the flux. This is Lenz’s law, which is the consequence of the principle of conservation of energy. Vi can also be written in terms of time rate of change of the current as Vi = 
d di ( Li ) =  L dt dt
(123)
where L is a constant generally called the selfinductance of the circuit. From Equations 122 and 123, we have L=N
df di =  Vi dt di
(124)
The selfinductance L in the electromagnetic system is analogous to the capacitance C in the dielectric system in which i = C dV/dt. The latter will be discussed in Chapter 2. Because of the parameters R and L in the magnetic circuit, when the switch is turned on, it takes some time for the current to establish its final, steady value. Based on the simple equivalent circuit, the system shown in Figure 11(a), we can write V = Ri + L
di dt
(125)
For magnetic materials, L is not always a constant, so f is not a linear function of i based on Equation 124. However, L can be considered a constant for nonmagnetic materials and can be assumed to be approximately constant for
6 Dielectric Phenomena in Solids
magnetic materials if the magnetic flux density is sufficiently low or the magnetizing current is sufficiently small. When L is constant, the solution of Equation 125, using the initial boundary condition, when t = 0, i = 0, gives i=
VÈ R 1  exp Ê  t ˆ ˘˙ Ë L ¯˚ R ÎÍ
(126)
The variation of i with t is shown in Figure 12. Theoretically, i never rises to its final value I = V/R, but practically this is usually accomplished in a rather short time. From Equations 124–126, t = L/R is a time constant. Initially, i rises linearly with time, but the rate of the current rise gradually decreases because when i rises, there is an increasing storage of energy in the magnetic field. By multiplying Equation 125 by idt, we have Vidt = Ri 2 dt + Lidi Energy stored Energy supplied Energy to the magnetic dissipated in the magnetic system as heat field loss in the coil
(127) When t = t, the current reaches about 63% of its final value I = V/R. The rate di/dt gradually decreases, implying that the induced voltage Vi decreases gradually, but the current and hence f gradually increase to their final values. When i reaches its final value I, the induced voltage t
V/R
=I
L di R dt
(Rising) i i
+ i
V
RL
–
Ri R L
di
L dt
t (time) Figure 12 The current rise in an inductive circuit— equivalent circuit of the electromagnet system shown in Figure 11(a)
approaches zero, and the total energy stored in I 1 the magnetic field will be Ú Lidi = LI 2 . This i 2 phenomenon is analogous to the response of a C and R series circuit representing a dielectric system. In this case, the time constant is CR. When the voltage across the capacitor approaches the value of the applied DC voltage V, the charging current will approach zero. By this time, the energy stored in the capacitor is 1 CV 2. 2 For a large electromagnet, the amount of energy stored in the system could be quite large. If the switch is suddenly opened to disconnect the system from the source, there is an induced voltage, which is theoretically infinite because di/dt Æ • if there is no protective resistor RL across the coil. In this case, the huge induced voltage may cause a spark across the switch or damage in the coil insulation. To protect the system, a protective resistor RL is usually connected across the coil, as shown in the inserted circuit in Figure 12. This resistor, in series with the coil resistance R, will absorb the energy released from the system when and after the switch is opened. Having discussed the concept of the electromagnetic behavior under a DC condition, we now turn to what is different under a timevarying current condition. Let us use the system shown in Figure 13(a), in which we have a closed iron core with a cross section area A and mean flux path length m, a coil of N1 turns on one side, and a coil of N2 turns on the other side. This system is similar to that shown in Figure 11(a), except there is no gap in the core (a = 0). Note that the following analysis is valid for the core with or without a gap. We chose the core without a gap in order to use this system to illustrate the principle of transformers. If the coil with N1 turns is connected to an AC voltage source, the + sign means the positive polarity, i.e., the positive halfcycle of the AC voltage at the coil terminal at a particular moment as a reference. At that particular moment, the current i1 will flow in coil 1 (primary coil) and induce a flux f circulating the iron core, as shown in Figure 13(a).
Introduction
– i1
Secondary
F
Primary
+
+
Va
7
V2
N2
N1
Iron Core (Cross Section A)
(a) F = BA
DVi
Iron Core (Cross Section A)
Vi = N (DVi)
Enclosed Surface with an Area S Surrounded by One Turn
(b) Figure 13 Schematic diagrams illustrating (a) Faraday’s law and the transformer principle, and (b) Stokes’s theorem based on the flux path in (a) for one turn.
According to Faraday’s law and Lenz’s law, this induced flux f will also induce a voltage Vi opposite to the applied voltage V1 and equal in magnitude to Va  R1i1, where R1 is the resistance of coil 1 in order to oppose any change of the flux. Vi is given by Vi = Va  R1i1 = V1 = N1
df dt
(128)
The same flux is also linked with coil 2 (secondary coil) of N2 turns. This flux will induce a voltage in coil 2, which is given by V2 =  N2
df dt
(129)
It is desirable to give a careful definition of the polarity of the coil terminals in relation to the flux. A positive direction of the flux is arbitrarily chosen as a reference; the terminals are then labeled in such a way that the winding of the coil running from the positive to the negative terminal constitutes a righthanded rotation
about the positive direction of the flux, as shown in Figure 13(a). Now let us consider only one turn. The voltage induced in one turn will be —Vi = 
df d =  Ú Bn ds dt dt s
(130)
The line integral of the electric field F around the coil of only one turn is equal to DVi. Thus, —Vi = Ú Fdl =  Ú c
s
∂B • n ds ∂t
(131)
This is an expression of Faraday’s law of magnetic induction. Applying Stokes’s theorem [see Figure 13(b)], the left side of Equation 131 can be expressed as
Ú Fdl = Ú — ¥ F • n ds c
s
(132)
Substitution of Equation 132 into Equation 131 gives
Ú — ¥ F • n ds =  Ú s
s
∂B • n ds ∂t
Direction of Force
8 Dielectric Phenomena in Solids
(133)
because the surface S is an arbitrary surface bounded by the loop C. Therefore, the two surface integrals are equal, so we can write —¥F=
∂B ∂t
(134)
This is an expression of Faraday’s law and is also the second equation of Maxwell’s equations in differential form. It is obvious that Figure 13(a) is the basic arrangement of a transformer, which can transform a low voltage to a high voltage simply by adjusting the turn ratio N2/N1 > 1, or vice versa. The timevarying magnetic flux can be achieved by many means. For example, with stationary north and south magnetic poles arranged alternatively in a chain with a small gap between the north and south poles, a copper coil moving along this chain will be linked by the magnetic flux, which changes with time from the north to the south pole and then to the north pole again, and so on. A voltage will be generated in the coil due to df/dt. Alternatively, the same effect would result if the coil were kept stationary and the magnetic pole chain were moving through the coil. A coil or a wire carrying a current placed in a magnetic field will experience a force acting on it. This is the magnetic force given by F = qv ¥ B
(135)
where v is the velocity of the electrons moving in the coil or wire. The direction of this force is perpendicular to both B and v . This is why the electric motor works. The direction of this force follows Fleming’s socalled lefthand rule, as shown in Figure 14(a). This rule states that if the forefinger points in the direction of the magnetic field and the middle finger points in the direction of the current flowing in the conductor (coil or wire), then the thumb will point in the direction of the force which tends to make the coil or wire move. In fact, this phenomenon can be visualized by the crowding of the magnetic flux, which tends to push the conductor from the region with dense flux to the region of less flux, as shown in Figure 14(b).
N
S Direction of Magnetic Field
Direction of Current
(a) N Direction of Force
+
Direction of Current Pointing on the Surface of the Page
Crowding Magnetic Flux
(b) Figure 14 (a) Fleming’s lefthand rule, and (b) crowding magnetic flux pushing the conductor from a highflux density region to a weakflux density region.
The principles of all DC and AC machines— stationary (e.g., electromagnets and transformers) or nonstationary (e.g., generators and motors)—are simply based on these three laws—Ampère’s, Faraday’s, and Lenz’s— coupled with magnetic forces. 1.1.3 Inseparable Magnetic Poles The third of Maxwell’s equations, — • B = 0, merely states the fact that magnetic flux lines are continuous. In other words, the number of magnetic flux lines entering any given volume of a region must equal the number of flux lines leaving the same volume. This means that the magnetic flux lines always close themselves, because the north and south magnetic poles are inseparable, no matter how small the magnets are. Electrons, protons, and neutrons produce their own magnets, and each always comes with both a north pole and a south pole.
Introduction
Breaking a magnet in two just gives two smaller magnets, not separated north and south poles. No magnetic monopoles exist. Thus, the magnetic effects in a material must originate from the magnetism of the constituent particles as an immutable fact of nature. 1.1.4 Gauss’s Law Divergence of a flux means the excess of the outward flux over the inward flux through any closed surface per unit volume. For electric flux density D, the — • D means
Ú D • n ds = Ú — • DdV = Ú r dV S
V
= 0 if Q ( the net charge) is located outside the surface S = Q if Q is inside the volume V enclosed by the surface S.
(136) If the region enclosed by the surface S has a net charge Q that is equal to Úr dV, then we can write (137)
—• D = r
This is Gauss’s law; it is also the fourth of Maxwell’s equations. If the permittivity of the region e is independent of the field and the material is isotropic, then Equation 137 can be written as —•F =
r e
(138)
This is Poisson’s equation. Since (139)
F = —V
where V is the scalar potential field in the region. In terms of scalar parameters, Poisson’s equation can be written as — •(—V ) = — 2V = 
r e
(140)
If Q = 0, that is, if the region is free of charges, then Equation 140 reduces to — 2V = 0
(141)
Equation 141 is known as Laplace’s equation. Both Poisson’s equation and Laplace’s equation will be very useful in later chapters when we
9
are dealing with space charges and related subjects. The parameters e, m, and s in Equations 15 through 17 depend on the structure of materials. Therefore, information about the dependence of these parameters on the field strength, frequency, temperature, and mechanical stress may reveal the structure of the materials, as well as the way of developing new materials. Equation 17 is Ohm’s law, discovered by German scientist Ohm in 1826, referring mainly to metallic conductors at that time. In fact, all of these parameters are dependent on field strength and frequency, even at a constant temperature and pressure condition. It can be imagined that to solve Maxwell’s equations with the fielddependent and frequencydependent e, m, and s would be quite involved. For nonmagnetic materials, we can assume that m = mo and is constant, but e and s are always field and frequencydependent. In subsequent chapters, we shall deal with these two parameters and discuss how they are related to all dielectric phenomena.
1.2
Magnetization
In this book, we shall deal only with nonmagnetic materials. What kind of materials can we consider nonmagnetic? All substances do show some magnetic effects. In fact, many features of the magnetic properties of matter are similar or analogous to the dielectric properties. Induced magnetization is analogous to induced polarization. For some materials, atoms or molecules possess permanent magnetic dipoles, just as other materials do with permanent electric dipoles. Some materials possess a spontaneous magnetization, just as other materials possess a spontaneous polarization. However, there is a basic difference between magnetic and dielectric behaviors. Individual electric charges (monopoles) of one sign, either positive or negative charges, do exist, but the corresponding magnetic monopoles do not occur. This was explained briefly in Section 1.1.3. We have mentioned that magnetism is the manifestation of electric charges in motion based on Ampère’s and Faraday’s laws, so we
10 Dielectric Phenomena in Solids
can expect that the electrons circulating around the nucleus and the electrons spinning themselves in the atom, as well as the spinning of protons and neutrons inside the nucleus, will produce magnetic effects. Before discussing the physical origins of the magnetism, we must define some parameters that are generally used to describe the properties of matter. Polarization P describes dielectric behavior, and magnetization; M describes magnetic behavior. P is defined as the total electric dipole moments per unit volume. The same goes for M, which is defined as the total magnetic dipole moments per unit volume. Let us consider a cubeshaped piece of material with a unit volume cut out from the iron core, as shown in Figure 13. We can see in this cube that there is a magnetization M, as shown in Figure 15. A cube of magnetized material contains of the order of 1022 magnetic dipoles, which tend to line up just like a compass needle when they are magnetized in a magnetic field. For electric polarization, the electric flux inside a polarized material has two components: One component is for setting up an electric field and the other component is due to the polarization. (See Chapter 2, Electric Polarization and Relaxation in Static Electric Fields.) In a similar manner, the magnetic flux inside a magnetized material also has two components: One component is for setting up a magnetic field H, and the other is due to the magnetiza
M South Poles S
h S
North Pole (+p) mm = ph (magnetic dipole ANALOGOUS TO moment) South Pole (–p)
(b)
(142)
The magnetization M has the same dimension as H, which is ampere per unit length. M can be expressed as M = Total magnetic dipole moments volume = N( m m ) = N( ph) = Nh( p) (143)
where N is the number of atoms or molecules per unit volume. The elementary magnetic dipoles are in fact the atoms or molecules, which are the constituent particles of the material. They can become magnetic dipoles pointing in one direction under the influence of a magnetic field. Thus, mm = ph is the magnetic dipole moment, where h is the distance between the north and south magnetic poles. Since the dimension of M is ampere per unit length (or amperelength1), the dimension for the pole strength p is amperelength and that for the magnetic dipole moment ph becomes amperelength2. It is easy to understand the charge q in the electric dipoles. But what is meant by p in the magnetic dipoles? To understand p, we must look into the mechanisms responsible for the magnetic effect of the constituent particles, which are atoms or molecules. Before doing so, return to Equation 142. From this equation we have B Ê m H =  1ˆ H = ( mr  1)H Ë mo ¯ mo (144) = c m H = N m m = N ph
M=
cm =
(a)
N
B = mo H + mo M
where · Ò denotes the average value of mm over the whole ensemble, and cm is the magnetic susceptibility in analogy to the dielectric susceptibility.
North Poles N H
tion M. Thus, under an applied magnetic field we have
+ qd d
– –qd
u = qdd
(c)
Figure 15 Schematic diagrams illustrating (a) magnetization, (b) magnetic dipole of the magnetic dipole moment um = ph, and (c) electric dipole of the electric dipole moment u = qdd.
M = mr 1 H
(145)
Obviously, cm reflects the degree of magnetization. In free space, or in gases at normal temperatures and pressures, we can consider cm = 0, implying that there is no magnetization: M = 0. Depending on the values of cm, all materials can be divided into three major groups: diamagnetic materials with ur very slightly less than unity, (i.e., cm < 0); paramagnetic materials with mr very slightly greater than unity (i.e., cm >> 0); and ferromagnetic materials with ur enormously
Introduction
greater than unity (i.e., cm >> 0). The physical origins of these three kinds of materials are briefly discussed in the following sections. The Orbital Motion of Electrons around the Nucleus of an Atom The orbital motion of each electron constitutes a current i circulating around the nucleus, following the path of the orbit of radius r and taking time Tor to complete one revolution. Thus, the orbital current i can be expressed as i=
q qv qw ==Tor 2pr 2p
(146)
where v and w are, respectively, the circumferential velocity and the angular velocity (radians/second), and q denotes the electronic charge, which is always positive. Thus, an electron’s charge is q, while a proton’s charge is +q. It is important to remember the sign to avoid confusion. This current i will produce an orbital magnetic moment (called an orbital dipole moment), which is given by Bor a h mo i = Hor ah = Ê ˆ ah = ia Ë h¯
mor = ph =
(147)
where Hor and Bor are, respectively, the magnetic field and the magnetic flux density produced by i, and a is the area of the orbit. The revolving electron under the influence of centrifugal force also produces an orbital angular momentum, which is given by Lor = mvr = mwr 2
(148)
where m is the electron mass. Substituting Equations 146 and 148 into Equation 147, we have qw ˆ 2 Ê qwr 2 ˆ Ê q ˆ mor = Ê (pr ) = = Lor Ë 2p ¯ Ë 2 ¯ Ë 2m ¯
(149) The value of : The corresponding orbital type: The number of possible orbitals in one type: The corresponding value of m:
11
The orbital magnetic moment mor is proportional to the orbital angular momentum Lor. Both are normal to the plane of the current loop, but they are in opposite directions, as shown in Figure 16(a). The coefficient (q/2m), i.e., the ratio of mor /Lor, is called the gyromagnetic ratio.7 It is very important to understand that electrons of an atom are entirely quantummechanical in nature. The classical approach can help us to visualize qualitatively the mechanism, but for quantitative analysis, we must use quantum mechanics. Equation 148 gives only the classic angular momentum. In quantum mechanics, the angular momentum is given by h Lor = ml Ê ˆ = ml h Ë 2p ¯
(150)
where h is Planck’s constant and h = h/2p is generally called the hbar; m is a quantum number. To describe electron behavior in an atom, we need four quantum numbers, defined as follows: n:
The shell quantum number, defining the energy level of the shell. It takes integers, 1, 2, 3, 4, . . . : The orbital or the azimuthal quantum number, defining the orbital type in each shell. It takes integers, 0, 1, 2, . . . (n  1). m: The magnetic orbital quantum number, defining the possible ways of electron motion in the orbit. It takes integers with the values limited by  £ m £ +. s: The spin quantum number, defining the possible ways of electron rotation about its own axis. It takes either +1/2 or 1/2. The relation between and m is as follows: 0 1 2 3 4 . . . . . . . . . . (n  1) spdfg.......... 1 3 5 7 9 . . . . . . . . . . (2 + 1) 0 (1, 0, +1) (2, 1, 0, +1, +2) and so on following the relation  £ m £ +
12 Dielectric Phenomena in Solids uor S
i
us
S
N Spinning
Lor
Electron with –q
N
S us
Upspin Spin Quantum Number: s = 1/2 u Spin Magnetic Moment: S = –uB Spin Angular Momentum: S = + h/2
(a)
is also proportional to its angular momentum and the directions of spin magnetic momentum and orbital magnetic momentum are opposite to each other, as shown in Figure 16(b), following the relation
S Downspin s = –1/2 uS = +uB S = – h/2
(b)
Figure 16 Schematic diagrams showing (a) orbital magnetic dipole moment uor created by an electric current i due to the electron orbiting around the nucleus, and orbital angular momentum Lor of the electron and (b) spin magnetic dipole moment us and the associated spin angular momentum s for the upspin and the downspin.
A piece of material contains a large number of atoms or molecules. Each orbital electron has a magnetic moment mor, but the directions of all the magnetic moments are oriented in a random manner, and their magnetic effects tend to cancel each other out. Thus, the material does not exhibit any magnetic effect because there is no net magnetization in any particular direction without the aid of an external magnetic field. It should also be noted that, if there is only one electron in the s orbital (or s state), the orbital angular momentum Lor = 0 and hence the orbital magnetic moment mor = 0, such as hydrogen (1s1). In this case, the magnetic moment is only that of the electron spin. If there are only two electrons in the s orbital, as in helium (2s2), both the orbital and the spin magnetic moments are zero because in this case, the angular momentum Lor = 0, and the magnetic moments due to the upspin and the downspin tend to cancel each other out. The Rotation of Electrons about Their Own Axis in an Atom The electron’s rotation about its axis, generally referred to as the electron spin, also produces a spin magnetic moment us and the accompanying spin magnetic momentum S. The spin motion is entirely quantum mechanical. Similar to orbital electrons, the spin magnetic moment
q ms = Ê  ˆ S Ë m¯
(151)
where S is the spin angular momentum. The spin gyromagnetic ratio (q/m) is twice that for orbital electrons. According to quantum mechanics, the spin angular momentum is given by h S = s Ê ˆ = sh Ë 2p ¯
(152)
As has been mentioned, the spin quantum number s can take only +1/2 (upspin) or 1/2 (downspin). Thus us can be written as q qh ˆ h ms = Ê  ˆ Ê + ˆ = Ê Ë m¯Ë 2¯ Ë 2m ¯ =  m B for up  spin
or
(153)
q qh ˆ h ms = Ê  ˆ Ê  ˆ = + Ê Ë m¯Ë 2¯ Ë 2m ¯ = + m B for down  spin
The quantity (q h/2m) is called the Bohr magneton uB, which is equal to 9.3 ¥ 1024 amperem2. For m = ±1, L = ± h the orbital magnetic moment uor is equal to the spin magnetic moment uor = ms = uB. The Rotation of Protons and Neutrons inside the Nucleus The rotation of protons and neutrons also contributes to magnetic moments, but their magnetic effect is much weaker than electrons. Magnetic moments of protons and neutrons are of the order of 103 times smaller than the magnetic moments of electrons.8 In the following discussion, we shall ignore the magnetic effect due to protons and neutrons for simplicity. In any atoms, the electrons in inner closed shells do not have a net magnetic moment because in these shells all quantum states are filled and there are just as many electron orbital
Introduction
and electron spin magnetic moments in one direction as there are in the opposite direction, so they tend to cancel each other. Only the electrons in partially filled shells (mainly in outermost shells) may contribute to net magnetic moments in a particular direction with the aid of an external magnetic field. In the following section, we shall discuss briefly the mechanisms responsible for the three kinds of magnetization. 1.2.1 Diamagnetism In most diamagnetic materials, atoms have an even number of electrons in the partially filled shells, so that the major magnetic moments are due to electron motion in orbits, the spin magnetic moments (one in upspin and one in downspin) tend to cancel each other. Under an external magnetic field, the field will exert a torque, acting on the electron. This torque is given by t=
d Lor = m or ¥ B dt
(154)
The direction of the torque vector is perpendicular to both uor and B. This torque tends to turn the magnetic dipole to align with the external magnetic field in order to reduce its potential energy. By rewriting Equation 154 in the form dL Ê q ˆ = L¥B dt Ë 2 m ¯
(155)
or q dL = Ê  ˆ L ¥ Bdt Ë m¯
it is clear that dL is perpendicular to L and B. Since B is constant, the only possibility that the momentum can change with time is for it to rotate or precess about the B vector, as shown in Figure 17. Thus, Equation 154 can be written as dL qB = L ¥ = L ¥ w p 2m dt
where wp is wp =
qB 2m
(156)
13
B z axis Precession Circle wp dL L and B L = Angular Momentum
wp
q wp
w
w
Orbit S r N –q, m, w uor Duor (Electron) Magnetic Moment Projected Electron Orbit on the x–y r Plane Nucleus Coulomb Force i
i
Lorentz Force q(v X B)
Figure 17 Larmor procession of an electron orbit about a magnetic field H = uoB.
which is known as the Larmor frequency. Theoretically, the magnetic dipole does not tend to align itself with the magnetic field, but rather to precess around B without even getting close to the direction of the magnetic field. In a pure Larmor precession, no alignment would take place. However, the precession always encounters many collisions, and the dipole would then gradually lose energy and approach alignment with B because under the condition of alignment, the potential energy uorB becomes a minimum. Because of the torque, the orientational potential energy of the magnetic dipole can be written as q ˆ Uor =  mor B =  Ê LB Ë 2m ¯ q ˆ =Ê ( m h)B = ml m B B Ë 2m ¯ l
(157)
For example, if = 1, m takes the value 1, 0, and +1. This implies that the atomic energy level under the influence of an applied magnetic field B is split into three levels. This splitting caused by a magnetic field was first discovered
14 Dielectric Phenomena in Solids
by Zeeman; therefore, it is generally called the Zeeman effect or Zeeman splitting. The difference between two adjacent split levels in this case is DUor = m B B
(158)
The lowest level, m = 1, in this case, refers to the minimum potential energy corresponding to the orientation of uor toward the alignment with the magnetic field B; the highest energy level, m = +1, refers to the maximum potential energy corresponding to the orientation of uor toward the direction opposite to B. The Zeeman effect also occurs in spin magnetic dipoles, but in this case the potential energy level is split into only two levels: one associated with s = 1/2 and the other with s = +1/2. The difference between these two levels is DUs = 2m B B
(159)
At this point, it is desirable to go back to the classical approach because it is easier to visualize the mechanism of precession. In a magnetic field, the motion of the electrons around the nucleus is the same as that in the absence of the field, except that the angular frequency is changed by wp due to precession. Thus, the new angular frequency w is w = wo  w p
(160)
where wo is the angular frequency in the absence of the field. The reason for the slight decrease in angular frequency is that in the presence of the field B, the orbital electron will experience a Lorentz force q ( v ¥ B) = q(wrB), as shown in Figure 17. This is a radially outward force, which tends to reduce the original centrifugal force by qwrB, and the new centrifugal force is given by
which would be of the order of 107 radians/sec for H = 100 amperes/m. In this case wo /wp = 109. So, wp is extremely small compared to wo. However, the motion of the electron has been slowed down, resulting from this reduction in angular frequency. This implies that the orbital magnetic moment is also decreased by the following amount: qw o r 2 Ê qwr 2 ˆ  Ë 2 2 ¯ 2 qw p r q qB ˆ 2 == Ê r 2 2 Ë 2m ¯ q 2 Br 2 =4m
Dmor = 
For the electron circulating counterclockwise, the induced magnetic moment is parallel to B, but its direction is opposite to B, as shown in Figure 17. It should be noted that the electron is not orbiting in one circle, but orbiting around a spherical surface. If we choose B in z direction, the orbital magnetic moment mor of a current loop is iA. The projected area of the loop on the x–y plane is pr2 with a new radius, r. Thus, the mean square of the radius can be written as ·r2Ò = ·x2Ò + ·y2Ò, which is the mean square of the distance of the orbiting electron normal to the magnetic field (zaxis) through the nucleus. But the orbiting electron is circulating the spherical surface; the mean square of the distance of the electron from the nucleus is ·r2Ò = ·x2Ò + ·y2Ò + ·z2Ò. For a spherically symmetrical distribution of the electron charge, we 3 have ·x2Ò = ·y2Ò = ·z2Ò. Thus, ·r2Ò = ·r2Ò. 2 Suppose a material has N atoms per unit volume and Z electrons per atom, which are undergoing Larmor precession. From Equation 162, we can write the magnetization M by replacing r with r, since we refer to the electron circulating on the x–y plane, as
mw 2 r = mw o2 r  qwrB M = NZ Dmor = 
which leads to wp =
qB 2m
(161)
It is desirable to have some feeling for the order of magnitude of the angular frequencies. wo is of the order of 1016 radian/sec, wp 1.05 ¥ 105 H,
(162)
2 2 Ê q Br ˆ NZ Ë 4m ¯
(163)
and hence, to the susceptibility as mo q 2 r 2 NZ M mo NZ Dmor = =4m H B (164) mo q 2 r 2 NZ =6m
cm =
Introduction
Diamagnetic susceptibility is negative, resulting in mr < 1. For example, for N = 1023 cm3, Z = 2, and r = 1A = 108 cm, cm is of the order of 106. In general, a diamagnetic material does not have permanent magnetic dipoles; the induced magnetization tends to reduce the total magnetic field. This is why cm is negative. Materials with complete shells, such as ionic and covalent bonded crystals, are diamagnetic. Their diamagnetic behavior is due mainly to the distortion of the electron orbital motion by the external magnetic field. Dielectric solids, such as insulating polymers involving ionic and covalent bonds, are mainly diamagnetic. Diamagnetic materials generally have an even number of electrons, so the magnetic effects due to the up and downspins tend to cancel each other out. In a case such as hydrogen, where there is only one electron in the s orbital (or s state), the orbital motion’s contribution to the magnetic effect is zero, and the diamagnetic moment is mainly that of the spin. In some materials, such as semiconductors and metals, free electrons also contribute to diamagnetic behavior because in the presence of a magnetic field the electrons will experience a magnetic force (qv ¥ B), and their quantum
15
states and motion will be modified. When this happens, they will produce a local magnetic moment that tends to oppose the external magnetic field, according to Lenz’s law. This contributes to a negative magnetization and a negative value of cm. Some values of cm are cm (copper) =  0.74 ¥ 106; cm (gold) = 3.7 ¥ 105; cm (silicon) =  0.4 ¥ 105; cm (silicon dioxide) = 1.5 ¥ 105. As cm is extremely small, we can consider all diamagnetic materials as nonmagnetic materials because ur = 1 and u = uo.
1.2.2 Paramagnetism As has been mentioned, substances having an even number of electrons in the shells are inherently diamagnetic. In some substances, however, atoms have nonpaired electrons or an odd number of electrons. In such cases, the magnetic effect due to the total electron spins cannot be zero. An atom of this kind will have a permanent magnetic moment, which arises from the combination of the orbital and the spin motions of its electrons, as shown in Figure 18(a). The resultant magnetic moment is given by um = g(  q 2 m) J
(165)
J L S uor us q uav
um
(a) Level 2 B=0
mj 1/2
1.0 N1/N 0.5 N2 /N 0
DU = guBB –1/2 Level 1 B>0
Lower State
Upper State uBB/kT
(b) Figure 18 (a) The spinorbit interaction forming a resulting magnetic dipole moment and (b) Zeeman splitting into two potential energy levels and the population of these levels as a function of temperature.
16 Dielectric Phenomena in Solids
where J is the resultant angular momentum, and g is a constant known as the Lande factor. For a pure orbital magnetic moment, g = 1; for a pure spin magnetic moment, g = 2. The value of g depends on the relative orientation of both the orbital and the spin angular momenta and must be determined by quantum mechanics. Further discussion about its value is beyond the scope of this book. However, following the quantummechanical approach, as in Equations 150 and 152, J can be written as J = mjh
(166)
where mj is the resultant quantum number defining the possible ways of the combined electron orbiting and spinning motions, and j is an equivalent azimuthal quantum number. The permanent magnetic moments of atoms or molecules are randomly distributed, with just as many pointing in one direction as in another in the absence of a magnetic field. With an external magnetic field, all the momenta precess about the magnetic field B with precessional angular velocities, which results in a Zeeman splitting. Following Equation 157, the potential energy of the dipole can be written as U = um B =  gm j uB B
N = N1 + N2
(170)
N2 N1 = exp( U kT ) = exp(  guB B kT )
(171) From these two equations, we can rewrite Equation 169 as M = N um tanh( guB B kT )
(172)
The ratios of N1/N and N2/N are also shown in Figure 18(b). Obviously, the condition for M = 0 is either B = 0 or T being very high, so that N1 = N2. It should be noted that the axis of the total angular momentum J is generally not the same as that of the total magnetic moment um, as shown in Figure 18(a). However, the J axis represents the rotation axis of the physical system formed by an electron which is orbiting as well as spinning. For low magnetic fields, guBB/kT << 1, tanh (guBB/kT) = guBB/kT, Equation 172 can be simplified to
(167)
For a simple case with only a single spin magnetic moment, then mj = ms = +1/2 or mj = ms = 1/2, and g = 2, and the Zeeman splitting will produce two levels, as shown in Figure 18(b). The difference in potential energy between these two levels is DU = g(1 2)uB B  g( 1 2)uB B = guB B (168)
The lower level, corresponding to mj = 1/2, is associated with the magnetic dipole moment in parallel with the magnetic field B because the potential energy of the dipole is a minimum, while the upper level, corresponding to mj = +1/2, is associated with the magnetic dipole moment in the direction opposite to the magnetic field. Thus, we can write the magnetization M as M = um ( N1  N2 )
of the magnetic dipoles with the direction n parallel to and that opposite to the magnetic field B in zdirection. By denoting N as the total concentration of atoms or molecules and following the Boltzmann statistics, we can write
(169)
where ·umÒ is the average dipole moment, and N1 and N2 are, respectively, the concentrations
M = N um ( guB B kT )
(173)
Thus, the magnetic susceptibility can be expressed as c m = M H = Muo B = Nuo um guB kT
(174) For general cases involving both the orbital and the spin magnetic moments, the Lande factor g should be between 1 and 2, following the relation8 g = 1+
j( j + 1) + s( s + 1)  l( l + 1) 2 j( j + 1)
(175)
A classical approach to evaluating cm is Langevin’s method.9 Atoms or molecules with a permanent magnetic dipole moment experience a torque in the presence of a magnetic field B, tending to orient themselves toward the direction of the field. However, the ensemble of atoms or molecules will gradually attain a statistically quasi equilibrium. Langevin, in 1909,
Introduction
17
z 1 L(um B/kT)
B
r q
0
dq
3 um B/kT
Figure 110 The Langevin function as a function of umB/kt.
2p(1  cos q) steradians, so dW = 2p sin qdq. Substituting Equation 177 into Equation 178 and changing dW in terms of dq, we obtain Figure 19 The element of the spherical shell between solid angle W and W + dW. W = solid angle = 2p(1  cos q) steradians. dW = 2p sin qdq.
was the first to develop a method of calculating the orientational magnetic susceptibility for paramagnetic materials. Later, Debye used the same method for its electrical analog in dipolar dielectric materials.10 The mean permanent dipole moment in the direction of the magnetic field is um = um cosq
(176)
where q is the angle between the dipole moment and the magnetic field B. Thus, the potential energy of the dipole at angle q is umBcos q. So, the probability of finding a dipole in the direction q from the zaxis (direction of the magnetic field B) is governed by the Boltzmann distribution function f (q ) = exp( U kT ) = exp(um B cosq kT )
(177) Thus, the mean dipole moment can be determined by the following equation um
Úu =
m
cosq f (q )dW
Ú f (q )dW
(178)
As shown in Figure 19, the solid angle W formed by the circular cone is equal to
um = um L(um B kT ) = um cosq
(179)
where L(umB/kT) is known as the Langevin function, which is given by L(um B kT ) = cosq =
Ú
p
o
exp(um B cosq kT )cosq sin qdq
Ú
p
o
exp(um B cosq kT )sin qdq
= Coth(um B kT )  (um B kT )1
(180) L(umB/kT) as a function of (umB/kT) is shown in Figure 110. For low values of umB/kT, Equation 180 can be simplified to L(um B kT ) = cosq = um B 3kT
(181)
From Equations 179 and 181, the magnetization M can be written as M = N um = N(um )2 B 3kT
(182)
and the magnetic susceptibility cm as c m = Nuo (um )2 3kT = Nuo ( gm j uB )2 3kT
(183) in which um = gmjuB, and gmj can be considered as the effective number of Bohr magnetons per magnetic dipole moment. Notice that the derivation of Equation 174 is based on the simplest type of Zeeman
18 Dielectric Phenomena in Solids
splitting, involving only two levels. If j is larger than 1/2, then the number of levels would be 2j + 1, and Equation 174 may be written as cm =
Nuo ( gm j uB )( guB ) 3kT
(184)
ferromagnetic behavior are complicated and must be treated quantum mechanically. To do so would be far beyond the scope of the present book. However, for completeness we shall discuss briefly, and only qualitatively, the origins of ferromagnetic behavior, which may have some bearing on later chapters. General ferromagnetic properties are summarized as follows:
It can be seen that cm, derived on the basis of the quantum mechanical approach, is very close to that derived on the basis of the classical approach. If N = 1023 atoms per cm3 and each atom has only one magnetic moment and T = 300 K, then cm = 0.87 ¥ 104. For any actual atoms or molecules in a real material, the value given by Equation 183 must be adjusted in accordance with the number of orbital and spinformed permanent magnetic dipoles involved to give the magnetic moment um per atom as a whole. We can replace N with NZ, with Z denoting the number of permanent magnets per atom. For example, cm (aluminum) = 0.21 ¥ 104, cm (platinum) = 2.9 ¥ 104, cm (oxygen gas) = 1.79 ¥ 106. Note that the magnetic effect given for paramagnetism is stronger than the inherent diamagnetic effect, which is always there. However, the resultant magnetic moment is always in the same direction as the external magnetic field, resulting in ur as slightly larger than unity and cm as positive, even though its value is very small, of the order of 104. Because of the extremely small values of cm, we can also consider the paramagnetic materials as nonmagnetic materials, and we can assume ur 1 for these materials.
• The magnetization may reach a saturation value by a weak magnetizing field. • The material may have zero magnetization at zero (or very small) magnetic fields, and the magnetization remains after the removal of the magnetic field. Thus, when the applied magnetic field is changed from a positive polarity to a negative polarity, and then back to the positive polarity, a hysteresis loop will be formed in the relation of B and H, resulting in energy loss due to the rotation of the dipoles. The area enclosed by the hysteresis loop represents the energy loss involved. • The ferromagnetic behavior (i.e., the spontaneous magnetization) completely disappears at temperatures higher than a critical temperature, called the Curie temperature Tc. At T > Tc, spontaneous magnetization is destroyed, and the material becomes paramagnetic, not ferromagnetic.
1.2.3 Ferromagnetism We have discussed, to some extent, diamagnetism and paramagnetism. The purpose of including these topics in the present book is twofold: to show what kind of materials can be considered nonmagnetic materials, and to show that the mechanisms of magnetization are similar to those of electric polarization. With a basic knowledge of magnetism, the reader may better appreciate the discussion in the later chapters about dielectric phenomena. Ferromagnetic materials are magnetic materials; the mechanisms responsible for magnetization and related
The commonly used ferromagnetic materials are iron (Fe), cobalt (Co), nickel (Ni), and their alloys, which are of importance to technical applications. Two other rareearth metals, gadolinium (Gd) and dysprosium (Dy), are of less practical interest because of their low Curie temperatures. The Curie temperatures for Fe, Co, Ni, Gd, and Dy are, respectively, 1043 K, 1400 K, 630 K, 280 K, and 105 K. However, the elemental metals and their alloys are metallic in nature, and their electric conductivity is generally very high. For some applications, insulating or semiinsulating ferromagnetic materials are preferable. Some oxides, such as
• The magnetization is spontaneous. • The relative permeability attains very high values, as high as 106 in some solids.
Introduction
CrO2, MnOFe2O3, and FeOFe2O3, have low electric conductivity and also possess spontaneous magnetization under suitable circumstances. They have a reasonable range of Curie temperatures much higher than normal room temperature. In all of the elemental metals, spontaneous magnetization arises from an incomplete 3d shell for Fe, Co, and Ni, and an incomplete 4f shell for Dg and Dy. In this section, we use Fe as an example to discuss the mechanisms of ferromagnetic behavior. The same mechanisms apply to other elements with incomplete 3d or 4f shells. An iron atom has six electrons in the 3d shell; a fully filled 3d shell should contain ten electrons. Of these six electrons in the 3d shell, five spin in the same direction and only one spins in the opposite direction. This makes the spin magnetic dipole moment of one atom equal to 4uB. Why are these six electrons in the 3d shell divided in such a way that five electrons have the same spin and only one electron has the opposite spin, producing a net spin magnetic moment of 4uB? In other words, why must these six electrons form a magnetized state (with five electrons in one spin and one in opposite spin), instead of having a nonmagnetized state (three electrons in one spin and the other three in opposite spin)? This can only be explained through quantum mechanics. The exchange energy principle, coupled with the Pauli’s exclusion principle, shows that the potential energy of the electrons in the magnetized state is lower than when they are in the nonmagnetized state.11–13 This conclusion can also be realized on the basis of band theory, by considering that the electrons with upspin form one band and those with downspin form another. These two bands would be completely filled if there were ten electrons in the 3d shell per atom, i.e., five electrons with upspin and the other five with downspin. However, iron atoms have only six electrons in the 3d shell. For the unmagnetized state, we would expect three electrons in the upspin band and the other three in the downspin band. In this case, both bands are partially filled. For the magnetized state, we would expect five electrons with same
19
spin in one band, which is completely filled, and one electron with opposite spin in the other band, which is partially filled. By comparing these two states, it can be imagined that the magnetized state is more stable than the unmagnetized one. This also implies that the potential energy is lower in the magnetized state than in the unmagnetized state, because for the former, one band is completely filled, while for the latter, each band is only partially filled. However, the difference in potential energy between these two states, referred to as the exchange energy, is small; it is of the order of 0.1 eV. Thermal agitation tends to destroy such a magnetized state (the state with a minimum potential energy) and hence, the spontaneous magnetization. Thus, we would expect that there is a critical temperature, at or above which the magnetized state would become an unmagnetized state, and spontaneous magnetization would be completely destroyed. This critical temperature is called the Curie temperature Tc. Its value is different for different magnetic materials, as mentioned previously. Ferromagnetic materials, such as Fe, Co, and Ni, have definite types of crystalline structure, such as bodycentered cubic for Fe, hexagonal for Co, and facecentered cubic for Ni. In such crystals, there are certain principal directions, which are (100), (110), and (111), assigned according to the Miller system of indices. In general, for bodycentered cubic Fe, magnetization is easy in the (100) direction, medium in (110), and hard in (111). Most magnetic materials are polycrystalline, i.e., the material is composed of a large number of very tiny single crystals, called grains. Between grains, there exist grain boundaries. In each grain, there are many spin magnetic dipoles. Even their magnetic moments tend to be parallel to the easy direction, but there are six possible easy directions in a cubic unit cell: ± x, ± y, and ± z. In order to reduce the dipole interaction energy (i.e., magnetostatic or magnetic field energy) to a minimal or lowest level, the grain must be divided into many small regions called domains. In each domain, the net spin magnetic moments are pointing in one easy direction, which is termed the parallel direction”; or in the
20 Dielectric Phenomena in Solids
(a)
(b)
I
II
III
IV
(c) Figure 111 Schematic diagrams showing the directions of spin magnetic moments in the domains inside a piece of ferromagnetic material (a) net magnetic moment pointing in only one direction with a large potential energy, (b) each domain having its magnetic moment pointing in different directions with a total minimal potential energy, and (c) some possible configurations, the magnetic moment pointing into the plane of the page and the magnetic moment pointing out of it. The potential energy is lower with the magnetic moments of neighboring domains pointing in opposite directions.
reverse easy direction, which is termed the antiparallel direction. At T = 0, all spins in one domain will be pointing in the parallel direction, and this domain is said to be spontaneously magnetized to the maximum degree without the aid of any external magnetic fields. The formation of domains inside a crystal is a natural process to minimize the potential energy of the system, which contains a large number of spin magnetic dipole moments. It can be imagined that, if the crystal had only one domain with a net magnetic moment pointing in one direction, this magnetic moment would be large and produce a large external magnetic field; therefore, a large amount of energy is involved, as shown in Figure 111(a). However, if the crystal is divided into four or more domains with the magnetic moments in the
domains tending to cancel one another out, as shown in Figure 111(b), then a lower energy for the crystal can be achieved. The mutual reaction force between the dipoles pointing in one direction acts as a driving force to cause the formation of more domains, with the magnetic moments pointing different directions so that they can cancel one another, thus reducing the potential energy of the system. The partial distribution of domains tends to assume the configuration so that adjacent domains have opposite magnetic moments. Some possible configurations are shown in Figure 111(c). The potential magnetic energy in Figure 111(c) part I is smaller than that in Figure 111(a), and the potential energy in Figure 111(c) parts III and IV is much smaller than that in Figure 111(c) part II. It seems that the larger
Introduction
the number of domains formed, the lower the energy associated with the system. But when domains are formed, block walls (or domain walls) are required to separate the domains. Energy is required to create a wall between domains. This, in turn, results in an increase of the energy in the system. It is likely that the increase in energy for the creation of domain walls balances the decrease in energy due to the formation of domains. There must be an optimal point at which the number of domains is limited by the minimization of the total energy of the system. In other words, the number and the configuration of domains in a magnetic material are determined by the minimization of the magnetic field energy and the domain wall energy. We have already mentioned the reduction of magnetic field energy by the formation of many domains. The domain wall energy arises from both the exchange energy and the isotropy energy; the former is related to the energy difference between the unmagnetized state and the magnetized state, while the latter is related to the energy involved for magnetization in one direction relative to the crystal axes and in another direction. In a material as a whole, there are many tiny crystals (grains), and each grain has many domains. The magnetic moments are pointing randomly in all directions, resulting in a zero net magnetization, as shown in Figure 111(c). It is desirable to have a general picture about the sizes of grains and domains. Suppose a piece of iron of one cubic centimeter (cm3) has about 1023 atoms, which may contain about 104 tiny single crystals (grains), and each grain may be divided into about 105 domains in average. This means that in average, there are about 1019 atoms per grain and about 1014 atoms per domain. Assuming that both the grain and the domain are cubic in shape, the linear dimensions would be about 5 ¥ 102 cm for a grain and about 103 cm for a domain. Note that the sizes of the grains and the domains may be different from grain to grain and from domain to domain, and their shape is not necessarily cubic. The example given here is only to establish a feeling about the average sizes of a grain and a domain.
21
Let us now consider the influence of an applied magnetic field on the orientation of the magnetic moments in the domains toward the direction of the magnetic field H to produce an overall magnetization of the whole material. Suppose that we apply a magnetic field H to a nonmagnetized ferromagnetic solid, starting with zero field and gradually increasing the field in steps. We can see the gradual increase of the magnetization (or the magnetic flux density B), as shown in Figure 112(a). The B–H curve has four regions, each is related to different magnetization processes: • Region I: Magnetization by translation increasing the size of the magnetized domains parallel to H and reducing the size of those with magnetization antiparallel to H, as shown in Figure 112(b). • Region II: B increases in a series of jerky steps with increasing H, corresponding to jerky rotation of domains from the original “easy” crystal direction to other “easy” direction more nearly parallel to H. This phenomenon is known as the Barkhausen effect. • Region III: The magnetic moments in all domains rotate gradually from the “easy” direction toward the direction of H. • Region IV: Further increase in H will make the magnetic moments of all domains parallel to H, implying that the magnetization has reached a saturation value. Now we start to reduce the magnetic field H, also in steps. As can be seen in Figure 112(a), B at point 5 is almost the same as at point 4, but with further decrease of H to zero, B does not go back to zero, but decreases following a different curve and reaches a finite value BR at H = 0. BR is referred to as the remanent flux density. To bring B to zero, we need a reverse magnetic field HC, which is generally called the coercive force or demagnetizing field. This is the magnetic field opposite to the magnetization field, required to bring the magnetization to the vanishing point. The formation of a hysteresis loop implies that the magnetization of a ferromagnetic material is irreversible. The
22 Dielectric Phenomena in Solids 5 4
B BR
3
6
2
1 Barkhausen Effect
12
7 HC
0
H 0–1 Region I Translation 1–2 Region II Rotation
11
8 9
2–3 Region III Rotation 3–4 Region IV Rotation
10
(a) H=0
H
Demagnetized
I H
II
H
III & IV
(b) Figure 112 (a) The B–H hysteresis loop of a typical ferromagnetic material, and (b) the magnetization processes in Regions I, II, III, and IV.
paths 3–4 and 4–5 are almost identical, indicating that the domains’ rotation from an “easy” to a “hard” direction is reversible. However, the paths 0–1–2–3 and 5–6–7 are quite different, indicating that the domain motion is irreversible because of the unavoid
able presence of all kinds of defects: structural defects and chemical defects or impurities in a real material. The domain walls move in a series of jerky steps or in a jerky rotation due to the collision with various defects, which consume energy.
Introduction
When a magnetization process consumes energy, this process will be irreversible, and this is why a hysteresis loop is formed. For the hysteresis loop around the loop 5–6–7–8–11– 12–5, the hysteresis loss is equal to the loop area, which is given by Wm = Ú HdB
joules m 3  cycle
(185)
when H is in ampere/m and B in Webers/m2. The power loss is proportional to the frequency of the magnetization field. Thus, the total power loss, i.e., the total hysteresis energy loss per second, is P=
[ Ú HdB] f ¥ (volume of the material)
(186)
where f is the frequency of the magnetic field. Note that the magnetic moment in one direction in one domain does not change abruptly to the reverse direction in a neighboring domain because of the exchange energy, which tends to keep the angle between adjacent magnetic moments small. Thus, the domain wall is a transitional region, enabling a gradual change in the spin direction, as shown in Figure 113. The domain wall width WB that minimizes the
N WB Domain B
S
Domain A
WB = Block Wall Thickness ~ ~ 300 Lattice Constants
Figure 113 Gradual change of spin direction inside the domain wall.
23
total energy—exchange energy and anisotropy energy—is about 300 lattice constants (1000 A). The wall energy involved is about 107 joule cm2 for a wall separating domains magnetized in opposite directions (a 180degree wall). It can be imagined that the transition due to the motion of the domain walls can only be made with the expenditure of work. This constitutes the hysteresis loss for each cycle of an alternating magnetic field. In fact, hysteresis loss is a major component of power losses in electrical machines. To reduce this loss, we must use very soft magnetic materials with a very narrow B–H loop and also laminate the material in order to reduce the eddy current loss. 1.2.4 Magnetostriction It may be said that all mechanical forces developed inside a material are originated by the interaction of electric charges. This is also true for magnetostriction, which is the magnetic counterpart of electrostriction. The spontaneous magnetization of a domain in a ferromagnetic material is always accompanied by an elongation or contraction in the direction of the magnetizing field. This physical deformation phenomenon is called magnetostriction. It is associated with the inherent anisotropy of the crystal structure and the preferred direction of magnetization in certain crystallographic directions. Magnetostriction is fundamentally a result of crystal anisotropy. Any physical deformation due to mechanical forces, such as expansion or contraction, will result in an increase in strain energy. Magnetostriction transforms electrical energy into mechanical energy in magnetostrictive transducers,8 but it also causes damage by introducing serious vibrations in the magnetic cores of the electrical machines and humming noise in transformers. 1.2.5 Magnetic Materials In terms of the arrangement of spin magnetic moments in the fully magnetized state, there are four general arrangements, as shown in
24 Dielectric Phenomena in Solids
(a)
(b)
(c)
(d)
Figure 114 The arrangement of spin magnetic moments in four different types of magnetic materials: (a) ferromagnetic, (b) antiferromagnetic, (c) ferrimagnetic, and (d) garnet ferromagnetic (a mixture of spin and orbital magnetic moments: —— spin magnetic moments,  orbital magnetic tmoments).
Figure 114. These general arrangements, briefly discussed, are as follows: • In ferromagnetic materials such as Fe, Co, and Ni, the spins of neighboring atoms are parallel to each other, which would result in a great increase in potential energy of the system. To reduce this energy, the formation of many tiny domains, with their magnetic moments tending to cancel each other is necessary in nature, as explained in the previous section. • In antiferromagnetic materials including chromium, manganese, MnO, and FeO, the spin magnetic moments alternate atom by atom as a result of the exchange interaction, which is essentially based on Pauli’s exclusion principle. These materials are still magnetic from a behavioral point of view, but they do not produce an external magnetic effect, because the magnetic moments tend to cancel each other. Therefore, they are of no technical interest. • Ferrimagnetism occurs only in compound materials. In such materials, there are two sets of spin magnetic moments that are unequal in magnitude and antiparallel to each other in direction, as shown in Figure 114(c). For most practical ferrimagnetic materials, the resultant spin magnetic moments are quite large. The materials behave like ferromagnetic materials but generally have a lower saturation value of magnetization. Ferrimagnetic materials are
generally referred to as ferrites. They have a very important feature, i.e., they are insulators, so ferrites are sometimes called the ferromagnetic insulators. They have very small eddy current losses, so they are suitable for high frequency applications. Ferrites are mainly transitionmetal oxides. One of the commonly used ferrites is MOFe2O3, where M is a metal, typically Fe, Ni, Al, Zn, or Mg. If M is Fe, the material becomes FeOFe2O3 or Fe3O4, which is the mineral magnetite, also known as lodestone, which has been exploited in navigation for centuries It is the best known ferrite. • The typical example of the garnet ferromagnetic materials is yttriumiron garnet (Y3Fe5012), also known as YIG. In this material, the spin magnetic moments of the yttrium atoms are opposite to the spin magnetic moments of iron atoms, but yttrium atoms also have orbital magnetic moments, which are larger than the spin magnetic moments. Thus, this compound is ferromagnetic. The garnet structure is very tight. All the large cages between oxygen ions are occupied by positive ions. As a result, these materials are very stable compared to spinel ferrites. Furthermore, very thin garnet films can be fabricated by the epitaxial technique on a suitable substrate for memory or storage on magnetic tapes or discs. Based on the magnitude of the coercivity, magnetic materials can also be divided into two major classes: soft magnetic materials and hard magnetic materials, as shown in Figure 115. Soft magnetic materials refer to the materials that can provide a large magnetic flux density at a small magnetizing field with a high differential relative permeability (ur)max, which is defined as (ur )max =
1 dB mo dH
(187)
as shown in Figure 115. Soft materials have a low coercivity (or demagnetizing field Hc) and hence, a small area enclosed by the B–H loop, thus giving a low hysteresis loss per cycle of an applied magnetic field. These materials are
Introduction
25
B slope = mmax
B Bmax +BR
Bs BR B = m0H
–Hc Hc
–Hc Hc
H
(a)
H
(b) (BH )
(BH )max
H
(c) Figure 115 (a) Typical B–H curve for soft magnetic materials, (b) typical B–H curve for hard magnetic materials, and (c) typical BH product as a function of H for the portion of the B–H curve where B is positive and H is negative (demagnetizing).
generally used for transformer cores, electrical machines, electromagnets, inductors, etc., which require easy magnetization and low energy losses. The most commonly used soft material is not pure iron, because practical iron contains various impurities and its properties depend on its fabrication processes. In practice, to reduce the coercivity, some suitable impurities are introduced into iron to make the motion of domain walls easier. For example, for iron, the easy magnetizing direction is along the (100) crystal direction, while for nickel, the easy magnetizing direction is along the (111) crystal direction. It can be imagined that an alloy made of Fe and Ni would be magnetized in any direction between (100) and (111) crystal directions, making domain motion much easier. Furthermore, the deformation sign of the magnetostriction of iron is opposite to that of nickel. An alloy of Fe and Ni with 70–80% of Ni is called permalloy, with a negligible net magnetostriction effect. It is a very soft material, easy to magnetize and demagnetize. Permalloys with 22% of Fe and 78% of Ni have
ur = 105, and those with 16% of Fe, 79% of Ni, and 5% of Mo have ur as high as 106. These materials are used for highquality transformers and other electromagnetic apparatus. However, these materials have a very high electrical conductivity, and therefore, they have a high eddycurrent loss, particularly at high frequencies. We need a material with high ur but a low electrical conductivity. Silicon–iron alloy, with about 2% of silicon to reduce the electrical conductivity, has been used for most electrical machines. Some ferrites with a very low electrical conductivity have also been used for electromagnetic apparatus. Some commonly used soft magnetic materials are listed in Table 11. Hard magnetic materials are used for permanent magnets, storage media in tapes and discs, etc. In order to have a large coercivity, we need a flat B–H curve. The figure of merit generally used to characterize the hard magnetic materials is the maximum value of the B–H product, i.e., (BH)max in the second quadrant of the B–H curve, as shown in Figure 115. The larger the
26 Dielectric Phenomena in Solids Table 11 Some soft magnetic materials and their properties. Curie Temperature TC (K)
Saturated BS (Wb m2)
Coercive HC (Am1)
Relative Permeability mr
Resistivity r (W  m)
Fe
1043
2.15
4
5 ¥ 103
1.0 ¥ 107
Fe (with 3% Si)
1030
1.97
12
4 ¥ 104
6.0 ¥ 107
800
1.08
4
1 ¥ 105
1.6 ¥ 107
0.80
0.16
1 ¥ 106
6.0 ¥ 107
0.25
0.80
2 ¥ 103
0.2
Soft Magnetic Material
Permalloy (22% Fe and 78% Ni) Supermalloy (16% Fe, 79% Ni and 5% Mo) ManganeseZinc Ferrite [MnZn(Fe2O3)2]
Table 12
570
Some hard magnetic materials and their properties.
Hard Magnetic Material
TC (K)
Remanent BR (Wb m2)
HC (Am1)
Magnetite [FeO Fe2O3] (Iron Ferrite—Lodestone)
850
0.27
25 ¥ 103
0.90
4 ¥ 103
8 ¥ 102
Carbon Steel (With 0.9% C and 1% Mn)
(BH)max (AWb m3)
Alnico 5 (51% Fe, 8% Al, 14% Ni, 24% Co and 3% Cu)
1160
1.35
64 ¥ 103
2 ¥ 104
Barrium Ferrite [BaO(Fe2O3)6] (Ferroxdur)
720
0.35
160 ¥ 103
12 ¥ 104
value of (BH)max, the harder the magnetic material. To have a larger coercivity, the material must have a large anisotropy and contain impurities, which make domain motion difficult, so that after the removal of the magnetizing field H, the magnetized material will still provide a magnetic flux density BR and not relax back to its original thermal equilibrium state with the magnetic moments randomly arranged. Carbonincorporated steel and a series of alnico alloys are good hard magnetic materials. Alnico alloys are composed mainly of Fe, Al, Ni, Co, and Cu, such as alnico 5, which consists of 51% Fe, 8% Al, 14% Ni, 24% Co, and 3% Cu and yields a very high coercivity. Ferrites are also good hard magnetic materials. Some com
monly used hard magnetic materials are listed in Table 12. 1.2.6 Magnetic Resonance So far, we have dealt with only the magnetic effects under static DC or low frequency AC magnetic fields. There is much more information that can be obtained using high frequency AC magnetic fields. The term resonance generally refers to the condition in which a system involving oscillation with its natural frequency will absorb a maximum energy from a driving force source when it is driven at the frequency equal to the natural frequency. In other words, the response of a physical system to a periodic
Introduction
excitation is greatly enhanced when the excitation frequency approaches the natural frequency of the system. In fact, resonance is commonly evidenced by a large oscillation amplitude, which results when a small amplitude of a periodic driving force has a frequency approaching one of the natural frequencies of the driven system. We have mentioned that the rotation of electrons and spins in the atoms, and the rotation of protons and neutrons inside the nuclei, will produce magnetic moments. Application of a magnetic field H(= B/mo) will cause a Larmor precession of the magnetic moments around the field axis at a Larmor frequency wp (Equation 156). It can be imagined that the Larmor precession under a static field will become gradually attenuated, but the superposition of a small alternating field will make it start a precession again around the static field axis. Magnetic resonance occurs when the frequency of the exciting field is equal to the Larmor frequency of the system (i.e., the natural frequency of the system). There are several types of magnetic resonance, depending on whether the magnetic effects are associated mainly with the spin angular momentum of nuclei or of electrons. These are nuclear magnetic resonance (NMR), electron paramagnetic resonance (EPR), electron spin resonance (ESR), nuclear quadrupule resonance (NQR), ferromagnetic resonance (FMR), antiferromagnetic resonance (AFMR), etc. Most commonly used are NMR, EPR, and ESR. In this section, we shall discuss only briefly the basic principles of NMR, EPR, and ESR, which are widely used for many diagnostic and analytical applications. Nuclear Magnetic Resonance (NMR) As mentioned, for ferromagnetic materials, the magnetic effect due to atomic nuclei can be neglected because it is extremely small compared to that due to electrons, which is a thousand times stronger and plays the key role in ferromagnetism. However, for nonferromagnetic materials, the magnetic dipole moment of the nucleus resulting from the intrinsic
27
moments of the protons and neutrons, plus the moment of the current loop formed by the orbiting protons, exhibits some features different from those due to electrons. Magnetically, all electrons are identical, but all nuclei are not. Different nuclei have different magnetic moments and spins. Following Equation 165, the resultant magnetic moment of a nucleus may be written as (188)
uN = gN ( q 2 m p )I
where gN is the nucleus g factor analogous to the Lande g factor, mp is the mass of the proton, and I is the resultant angular momentum of the nucleus. Following the quantum mechanical approach, as used in Equation 166, the nuclear angular momentum I must be quantized in the same way as any other angular momentum. Thus, we can write I = mi h
(189)
where mi is the quantum number for the nuclear spin and assumes the value mi = i, (i  1), . . .  (i  1),  i
(190)
where i is the spin quantum number for the nucleus. The magnetic moments and spins depend on the structure of the nucleus.12,14–16 The magnetic moments and the spin quantum numbers for some nuclei are listed in Table 13. The isotope number is the total number of protons and neutrons in the nucleus. Similar to electrons, the number of allowed quantum energy levels is 2i + 1. For i = 3/2, mi Table 13 Nuclear magnetic moments and spins for some nuclei. Nucleus (Isotope Number)
Magnetic Moment (in Nuclear Magnetons)
Spin (i)
Hydrogen (1) Carbon (13) Oxygen (17) Sodium (23) Silicon (29) Phosphorus (31) Copper (63)
+ 2.79 + 0.70  1.89 + 2.22  0.55 + 1.13 + 2.22
1/2 1/2 5/2 3/2 1/2 1/2 3/2
28 Dielectric Phenomena in Solids
can be 3/2, 1/2, 1/2, or 3/2. The potential energy of the dipole is given by U N = uN B = gN ( q 2 m p )Iuo H = gN ( q 2 m p )( mi h)uo H = gN uNM mi uo H
mi = 3/2
DU Energy of the Levels
(191)
where uNM = q h/2mp is called the nuclear magneton, in analogy to the Bohr magneton uB. For i = 3/2, the energy difference between two levels, as shown in Figure 116, is
mi = 1/2 DU B = uoH
0
mi = –1/2 DU
DU = gN uNM (3 2  1 2)uo H = gN uNM uo H
(192) mi = –3/2
If the nucleus is excited by an alternating electromagnetic field to make a transition from one energy level to the other, the frequency of the electromagnetic field must, based on hf = gNuNMuoH, be
Figure 116 Splitting of 2i + 1 energy levels in a magnetic field B for a nucleus with i = 3/2.
imaging. For example, NMR is used in measuring the concentration of protons in tissues, the decay time of absorption using short rf pulses for the diagnosis of cancer tumors, etc.
(193)
f = gN uNM uo H h
Energy Absorption
Since mp (proton mass) is much larger than m (electron mass), the frequency required for nuclear magnetic resonance is usually in the megahertz range for a suitable choice of the magnetic field B (= uoH). The basic experimental arrangement for NMR measurements is shown in Figure 117. NMR has been a powerful tool for studying the physical properties of solids. It is also a very useful technique in nuclear physics, chemistry, and biology. A recent and fastgrowing application of NMR is in the area of medical
f
Electron Paramagnetic Resonance (EPR) In principle, energy absorption from the highfrequency electromagnetic field in EPR is strikingly similar to that in NMR. However, in paramagnetic systems, the interaction between dipoles due to electrons is weak. So, when a material containing atoms with quantum number j π 0 is subjected to a magnetic field
Electromagnet
Electromagnet Microwave Cavity
f = DU/h r f Coil
To r f Generator and Detector for Energy Absorption Measurements
Microwave Generator
Detector
Specimen
Specimen
Electromagnet
Electromagnet
(a)
(b)
Figure 117 Schematic diagrams showing the basic experimental arrangements for the measurements of (a) the nuclear magnetic resonance (NMR) in the radio frequency (rf) megahertz region, and (b) the electron paramagnetic resonance (EPR) in the microwave frequency gigahertz region.
Introduction
B (= uoH), all atoms will have some magnetic moments parallel to the direction of the magnetic field. The possible magnetic moment of the dipole is given by (see Equations 165 and 166). (194)
um = gm j uB
where mj = j, ( j  1), . . .  ( j  1), J, and j = 0, 1, 2, 3, . . . The possible potential energy of an atom in a magnetic field is governed by Equation 167, depending mainly on the value of mj. There are 2j + 1 energy levels. For example, if j = 1, there are three levels corresponding to mj = 1, mj = 0, and mj = 1. Thus, the separation between levels for j = 1 is (195)
DU = guB B = guBuo H
The splitting of the 2j + 1 energy levels for j = 1 is shown in Figure 118. If such a paramagnetic material is subjected to a static magnetic field superposed with a small microwave field with frequency f, when the frequency reaches a value such that hf = DU or f = DU/h (which is equal to the Larmor frequency or natural frequency of the system), the incident energy will excite the dipole from a lower energy level to a higher energy level. At the same time, the energy will be absorbed by the system from the incident microwave source. There is a dip in the transmission spectrum, indicating the paramagnetic resonant absorption, as shown in Figure 119.
29
The basic experimental arrangement for EPR measurements is similar to that shown in Figure 117, except that the range of the incident excitation frequencies for EPR is in the microwave gigahertz region simply because m for electrons is much smaller than mp for protons. The EPR phenomenon was first observed by Zavoisky in 1945 on the paramagnetic salt (CuCl2 • 2H2O).17,18 Studies of paramagnetic resonance in crystalline solids provide a great deal of information about the crystalline structure.18 The technique of EPR has been widely used in physics, chemistry, biology, and other fields. It is one of the important tools employed in the analysis of matter,18–20 such as the measurements of free radicals, trapped electrons, and excited molecules in dielectric materials. For example, there is no electron spin resonance in pure and perfect ionic crystals, since all electron shells are completely filled. Imperfections, including impurities in such crystals, however, usually create uncompensated spins, thus producing an absorption line or lines. An F color center (F refers to Farbe, the German word for color) in an alkali halide crystal is considered an electron trapped at a negative ion vacancy, the electron being shared by the six surrounding positive ions. Such electrons will exhibit electron spin resonance.21
DU mj = 0 B = uoH
0
Transmission
Energy of the Levels
mj = 1 1
DU
mj = –1 Figure 118 Splitting of 2j + 1 energy levels in a magnetic field B for an electron in an atom resulting from spinorbit interaction with j = 1.
f
0 f = DU/h
Figure 119 Transmission of electromagnetic waves as a function of frequency. The dip indicates the resonant absorption at f = DU/h.
30 Dielectric Phenomena in Solids
Electron Spin Resonance (ESR) ESR can be considered a special case of EPR only if the spin of the electron plays the key role in magnetic resonance. The ESR technique is widely used as a tool to analyze chemical reactions. When chemical bonds break up, electrons may be left unpaired. Such fragments may possess spins and are usually called free radicals. The magnetic resonant absorption from the electromagnetic excitation source indicates the presence of free radicals, and the magnitude of the absorption peaks can serve as a measure of their concentration. 1.2.7 Permanent Magnets Lodestone was possibly the first natural permanent magnet, discovered on the earth long before Christ. Chinese scientists invented the compass and called it the “southpointing needle”—a magnetized needle, possibly made of lodestone, having the composition Fe3O4 (magnetite), mounted on a pivot to permit the needle to swing freely in the horizontal plane. To fabricate a permanent magnet, we first must granulate a hard magnetic material into very small particles, each no larger than the domain (about 20–100 nm). These particles are then suspended in a substance solution, which itself need not be ferromagnetic. When an external magnetic field is applied, these suspended particles will orient to make themselves parallel to the direction of the magnetic field. As soon as this magnetization process is completed, the substance solution is gradually hardened, and the magnetized particles become frozen inside the substance to form a permanent magnet. There is another fabrication process called sintering. In this process, the granular magnetic particles are first subjected to an external magnetic field, so that they are aligned in one direction. Then they are heated to a high temperature to allow them to stick together. After that, the temperature is gradually lowered to consolidate the stuck particles, forming a solid permanent magnet. The most commonly used material for permanent magnets is alnico 5 (see Table 12). A permanent magnet with tiny, needlelike parti
cles of Fe in a nickel and aluminum matrix can be formed by controlled heat treatment and by annealing in a magnetic field. Single domain particles with a high uniaxial anisotropy should have a large coercivity. Barrium ferrites called Ferroxdur [BaO (Fe2O3)6] belong to this kind of large coercivity material. These materials have been used to form ceramic permanent magnets by sintering (or bonding in a matrix) the finely powdered barium ferrites under a magnetic field. Under this guideline, many new materials have recently been developed for sophisticated permanent magnets, including samariumcobalt (SmCo5), Nd2Fe14B, etc. The permanent magnets formed by single domain particles are often referred to as ESD magnets because the particles are elongated single domain particles.22–25 1.2.8 Magnetic Memories The discussion of various applications of magnetic materials is far beyond the scope of this book. However, it is worth mentioning a few, such as the use of magnetic materials for storing information. It is also good for the reader to think whether the dielectric materials can have a function similar to or better than magnetic materials. In fact, the sales of audio and video tapes, computer discs, and other magnetic information products in the United States exceeded those for all other hightechnology products. Storage capacity has been greatly improved in the past decade, an upperbound density has reached about 1014 bits m2. The basic principle for storage of information as patterns of magnetization in a magnetic material has been well established for more than 100 years. The main difference between the old and the new magnetic memories lies in technology—in materials and recording methods. In general, to write is simply to use an electromagnet moving relative to the recording tape or disc. After recording (writing), to read is to move the tape or disc that has already been stored with information. This moving tape or disc will give rise to varying magnetic flux, which will induce voltages in a coil and convert the signal to the original information. For tapes
Introduction
and discs, magnetic particles of sizes substantially less than one micron, with carefully tailored magnetic properties, are deployed in a passive binder on a flexible polymeric sheet, such as polyethylene terephthalate (PET or trade name Mylar) or on a rigid aluminum disc. To promote high coercivity, it is necessary to make a certain magnetization direction preferable to the others (easy axis). Particles commonly used for tapes and discs are g iron oxides including g Fe2O3, Co g Fe2O3, CrO2, BaO(F2O3)6, etc. Synthetic g iron oxide is the oxide containing g iron that has a facecentered cubic structure. g iron oxides can be used to produce needleshaped particles. For more information about this field, see references 23–25. Semiconductor memories are presently preferred for shortterm information storage, mainly because of low cost, easy handling capacity, fast access time, and small size. Magnetic tapes and discs, on the other hand, are chosen for longterm, largescale information storage, and particularly, for the fact that no electrical energy is needed to retain information storage. However, conventional tapes and discs do have some shortcomings: recording and playback heads are easily worn down, and coercivity decreases as packing density increases. Thin film technologies were developed to reduce the bit size so as to increase the bit density and make the reader easier to read by putting the thin film medium closer to the head. About four decades ago, small, bulk ferromagnetic ferrite cores were dominantly employed as computer memory elements; now, magnetic films deposited in the presence of a magnetic field exhibit a square hysteresis loop capable of switching from one state to another as a bistable element. Thin magnetic films consisting of Co, Ni, and Pt; Co, Cr, and Ta; or Co (75%), Cr (13%), and Pt (12%) are frequently used for hard disc memories. They may be deposited on an aluminum substrate by means of vapor deposition, sputtering, or electroplating. Such films are subsequently covered with a thin carbon layer about 40 nm thick for lubrication and protection against corrosion. These films can have coercivities ranging from 60 to 120 kA m1 and are capable of providing a density of 1.8 Mbits mm2.
31
Thin films can also be used for optical recording. In fact, magnetooptical recording relies on thermomagnetic effects. Suppose that a small region of a magnetic film is heated to a temperature higher than its Curie temperature and then allowed to cool in the presence of an external magnetic field. This small region would become magnetized to the direction of the magnetic field. If this heating and cooling process were carried out by means of a focused laser beam, the whole operating process could be very fast, within a microsecond. This could be considered as the “write” step in a recording system. The information stored in the magnetized regions of a thin film can be read by using the Kerr or Faraday magnetooptic effects by means of polarized light. By analyzing the direction of rotation of the polarization plane, it is easy to find the magnetized regions that hold the stored information. Several amorphous alloys, including TbFe, GdCo, GdFe, GdTbFe, GdTbCo, etc., have been used for magnetooptic memories because they have a larger Kerr rotation angle and hence a better signaltonoise ratio.25–27 There is another magnetic storage device, which is based on magnetic bubbles. This device was first demonstrated in 1967. A great deal of research was carried out for a while, but this technology is presently not much in use. Single crystal mixed garnets, such as yttriumirongarnet (Y3Fe5O12), are used for magnetic bubble media. Basically, a thin film of a few mm in thickness, consisting of such a magnetic material, can be epitaxially grown on a suitable substrate. Such a film has a highly uniaxial and anisotropic feature, implying that there is an easy axis for the generation of bubbles, perpendicular to the plane of the film. In this film are tiny cylindrical domains, each about 1 mm in diameter. All the domains can be aligned in a weak magnetic field normal to the film. However, by applying a strong, localized magnetic field in the opposite direction, it is possible to produce a cylindrical domain called a magnetic bubble with its magnetic axis inverted. Such a bubble will be stable after the strong field is removed because of its large domainwall coercivity. If the north pole of the
32 Dielectric Phenomena in Solids
bubble is on the top surface of the film, a small, southpole magnetic field placed near the bubble will attract it, causing it to move. This small magnetic field can be produced simply by employing soft magnetic permalloy overlays on the top surface of the film. The actual devices are fairly complicated. Our intention here is to describe briefly the basic principle of how magnetic bubbles can be generated, persuaded to move from one place to another, and erased by magnetic fields. The crystals are transparent to red light. Thus, by viewing the transparent film through crossed polarizers, it is easy to find the domain from the direction of rotation of the plane of polarization (Faraday effect in transmission or Kerr effect in reflection). Each such domain constitutes one bit of stored information. For more details about magnetic bubbles, see references 26–30.
1.3 Electromagnetic Waves and Fields There are two kinds of waves: longitudinal and transverse. In longitudinal waves, the oscillatory movement is in the direction of wave propagation, as in sound waves; in transverse waves, the oscillatory movement is perpendicular to the direction of wave propagation, as in waves on the surface of water. An electromagnetic wave is a transverse wave with its electric field F and magnetic field H perpendicular to each other and also perpendicular to the direction of wave propagation, as shown in Figure 120.
F c
x
H
From Maxwell’s equations, the following can be seen: • Wherever there exists a timevarying electric field, there must also exist a timevarying magnetic field, and vice versa. • An electrostatic field does not induce a magnetic field, and a magnetostatic field does not induce an electric field. • Electric flux lines terminate on charges. • Magnetic flux lines do not end, and their associated magnetic fields are solenoidal. In general, space containing air only is essentially equivalent to free space, as far as electromagnetic wave propagation is concerned. We consider the medium to be air in which e = eo, u = uo, s = o and r = 0. The variables F and H produce each other, so, for simple presentations, we can keep one variable and eliminate the other by the following process: Taking the curl of Equation 12, we have — ¥ (— ¥ F ) = —(— • F )  — 2 F ∂ =  mo (— ¥ H ) ∂t
(196)
Since r = 0, — • F = 0. Substitution of Equation 11 into Equation 196 yields — 2 F = e o mo
∂ 2F 1 ∂ 2F = ∂ t 2 c2 ∂ t 2
(197)
This is the wave equation for free space (or in air medium), and c is the velocity of light, which is (eomo)1/2. Equation 197 provides information about the electric field F at any position and at any time. The amplitude of its electric field intensity vector will vary with respect to x, y, z and t if Cartesian coordinates are employed. For simplicity, if we consider only the y component Fy and assume that there is no variation in H with respect to y and in F with respect to z directions, then Equation 197 reduces to ∂ 2 Fy 1 ∂ 2 Fy = 2 2 c ∂ t2 ∂x
(198)
The general solution of Equation 198 is Figure 120 Schematic diagram of a traveling plane electromagnetic wave.
Fy = f1( x + ct ) + f2 ( x  ct )
(199)
Introduction
If we are interested principally in sinusoidal function, then the solution of Equation 198 can be expressed simply as
33
Ú Pda . The rate of decrease of the stored d È1 (eF + mH )dV ˘˙ , energy would be dt ÍÎ 2 Ú ˚ as
a
2
2
V
Fy = A cos(wt  kx )
(1100)
where k is the wave factor, which is given by k=
w ∂ p f 2p = = v lf l
(1101)
which depends on the wavelength or the velocity of the electromagnetic wave. In other words, it depends on e and m, which are inherent in the properties of matter. Equation 1100 represents a component of F in y direction, which varies with time. Because the variation is perpendicular to the direction of wave propagation, which is in x direction, the wave is a transverse wave, as shown in Figure 120. It is also a plane wave, because a surface passing through all points of equal phase would be a plane, which is perpendicular to the x direction for the present case. From Equations 11 and 1100, it can easily be shown that the associated magnetic field in z direction is given by Hz = A(e o uo )1 2 cos(w t  kx )
(1102)
The ratio of Fy to Hz is the intrinsic impedance of the medium Z=
Fy Ê mo ˆ = Hz Ë e o ¯
12
(1103)
For free space, Z = 377 ohms. Both the electric field and the magnetic field represent the stored energy of the electromagnetic wave. By considering an enclosed surface with a volume V, the energy stored in the electric field is UF =
eo 2
Ú
V
F 2 dV
(1104)
and the energy stored in the magnetic field is UH =
uo 2
Ú
V
H 2 dV
(1105)
By denoting the power conveyed by the electromagnetic wave or power flow in the direction of wave propagation per unit area and per unit time as P, the total power flow out of the enclosed surface per second can be expressed
which must be equal to the outflow of the power. Thus, d È1
Ú Pda =  dt ÍÎ 2 Ú (eF a
V
2
+ mH 2 )dV ˘˙ ˚
(1106)
From Equations 11 and 12 it can easily be shown that
Ú Pda = Ú — •( F ¥ H )dV a
V
(1107)
Based on Gauss’ law
Ú — •( F ¥ H )dV = Ú ( F ¥ H )da V
a
(1108)
Thus, the power flow per unit area can be written as (1109)
P=F¥H
This is called the Poynting vector, showing that the direction of the power flow is the same as the direction of wave propagation. Wave theory can explain many optical phenomena, such as reflection, diffraction, and interference, but it cannot explain phenomena related to the exchange of energy, including the emission and absorption of light, photoelectric effects, etc. According to Einstein and Planck, electromagnetic wave or light energy is emitted or absorbed in multiples of a certain minimum energy particle, which is called a quantum or a photon.31,32 Depending on the frequency of the electromagnetic wave, the energy of a quantum or a photon is given by E = hu = h
c l
(1110)
where u is the frequency. (Note that the frequency is sometimes denoted by f.) It is generally accepted that electromagnetic waves or light apparently has a dual nature. Depending on the situation, the particle nature dominates when dealing with the exchange of energy, while the wave nature dominates when dealing with reflection, diffraction, etc. Figure 121 shows the electromagnetic spectrum. Equation 1110 can be written for the photon energy in free space in a simple form as E=
1.24 l
(1111)
34 Dielectric Phenomena in Solids l (m)
f (Hz)
10 kHz 103
E (eV) 10–12
105
104 10 105
4
103 km
MHz 106 10
Radio
2
107
10–11 Very Low Frequency VLF
10–10
Low Frequency LF
10–9
Medium Frequency MF
10–8 10–7
10 108
Television
Very High Frequency VHF
10 Radiant Heating
Ultra High Frequency UHF
109
10–1
THz 10
11
12
1013 10 Illumination
10–5
10–2
10–4
Extremely High Frequency EHF 10–3 mm
10–3
10–4
10–2
10–5
Infrared
10–6 mm 10
–7
16
Sun Lamps
1 Ultraviolet
1018
102
10–9 nm
103
10–10
Xray 1019
Cosmic Ray
Xray
10–11
1020
10–12 pm
1021
10–13
1022
10
10–8
1017
Gamma Ray
650 nm
600 nm Yellow 550 nm Green 500 nm Blue 450 nm Violet 400 nm
104 10
Gamma Ray
Orange
10–1
14
1015 10
Red
Super High Frequency SHF
1010
Radar
700 nm
10–6
1m GHz
Infrared (IR)
High Frequency HF
Visible Light
Audio
Spectral Region
6
5
106
Ultraviolet (UV)
107 Cosmic Ray
Figure 121 Electromagnetic spectrum. The wavelength l depends on the medium in which the electromagnetic wave propagates. In this figure, the medium is air, so the wavelength is for e = eO and u = uO.
in which E is in eV and the wavelength l in mm.
1.4
Dimensions and Units
Length, mass, time, and electric charge are generally used as the fundamental dimensions for describing physical quantities. On the basis of the International System of Units (Système Internationale, SI), the units for the four fundamental dimensions are L (length): . . . . . . . . . . . . . . . M (mass): . . . . . . . . . . . . . . . T (time): . . . . . . . . . . . . . . . . Q (electric charge): . . . . . . . .
m (meter) kg (kilogram) s (second) C (coulomb)
1.4.1 Length The unit for length is m (meter), but sometimes it is more convenient to use smaller units, particularly for microscopic dimensions. The commonly used smaller units are 1 cm (centimeter) = 10 2 m 1 mm ( millimeter) = 10 3 m 1 mm ( micron) = 10 6 m = 10 4 cm 1nm ( nanometer) = 10 9 m = 10 7 cm 1 Å ( Angstrom) = 10 10 m = 10 8 cm 1 pm ( picometer) = 10 12 m = 10 10 cm
Some old publications sometimes use British units: inch, foot, or yard. The conversion of British units to SI units is
Introduction
1 inch = 0.0254 m = 2.54 cm 1 foot = 12 inches = 0.3048 m = 30.48cm 1yard = 3 feet = 0.9144 m = 91.44 cm 1mile = 5280 feet = 1609.344 m
1.4.2 Mass The unit for mass is kg (kilograms). Again, it is sometimes more convenient to use smaller units. Those most commonly used are 1 g (gram) = 10 3 kg 1mg (milligram) = 10 6 kg = 10 3 g 1 mg (microgram) = 10 9 kg = 10 6 g 1ng (nanogram) = 10 12 kg = 10 9 g
British units for mass are ounce and pound. The conversion is as follows:
So, an electron has a negative charge q and a proton has a positive charge +q.
1.4.5 Derived Units Many derived units are also generally used to shorten the dimensional expressions for many physical parameters, including the ampere, volt, ohm, etc. The derived units can be easily expressed in terms of the fundamental units. However, it is important to understand the meaning of the derived units when analyzing any dielectric phenomena. 1.
1.4.3 Time The unit for time is s (second). The commonly used smaller units are 1 ms ( millisecond) = 10 3 s 1 ms ( microsecond) = 10 6 s 1 ns ( nanosecond) = 10 9 s 1 ps ( picosecond) = 10 12 s
1.4.4 Electric Charge The fourth unit is C (coulomb). Smaller units are also frequently used, namely mC (microcoulomb), nC (nanocoulomb), and pC (picocoulomb). The smallest existing charge, called the elementary charge, is the charge of an electron, which is 1.602 ¥ 1019 C. We use q to denote this charge q = 1.602 ¥ 10 19 C
Current I: The unit is ampere. 1 A ( Ampere) = 1Cs 1
2.
(T1Q)
Force F: The unit is newton. 1 N (newton) = 10 5 dynes = 1kg m s 2 (LMT2)
1 ounce (avoirdupois) = 28.3495 g = 28.3495 ¥10 3 kg 1pound (avoirdupois) = 16 ounces = 453.59 g = 0.45359 kg = 1lb (from Latin Libra) 1 ton (short ton, S.T.) = 2000 pounds = 907.18 kg 1 ton (long ton, L.T.) = 2240 pounds = 1016.04 kg
35
3.
Pressure X: The unit is Pa (pascal). 1 Pa (pascal) = 1 newton m 2 = 1 kg m 1 s 2 (L1MT2)
One conventional unit frequently used in the literature is torr, which is 1 torr = 1 mm Hg = 1.01325 760 bar 1bar = 10 6 dynescm 2 1 torr = 1.01325 ¥ 10 6 760 = 1330 dynescm 2 = 133Pa
Standard temperature and pressure (STP) refers to the condition at one atmosphere (760 mm Hg) and 270 K (0° C). 4.
Energy E: The unit is J (joule). 1 J ( joule) = 1 Nm = 1kgm 2 s 2
(L2MT2)
7
1 J ( joule) = 10 erg
One most frequently used unit is eV (electronvolt). 1 eV = 1.602 ¥ 10 19 coulomb ¥ 1V = 1.602 ¥ 10 19 joule 1 keV = 10 3 eV 1 MeV = 10 6 eV
There is another unit frequently used by chemists, calorie, called the thermochemical unit.
36 Dielectric Phenomena in Solids
11. Magnetic flux f: The unit is Wb (weber).
1 cal (calorie) = 4.184 J ( joule) 1 J (joule) = 0.2389 cal (calorie)
1 Wb ( weber) = Vs = 1C 1 kg m 2 s 1 (L2MT1Q1)
Thermal energy is also expressed in eV, such as kT (at 300 K) = 0.0259 eV. British thermal unit is called the btu, 1 btu = 252 calorie.
Magnetic flux density (or called magnetic induction) B: The unit is T (tesla).
5.
1 T ( tesla) = 1Wbm 2 = 1C 1 kgs 1
Power P: The unit is W (watt). (L2MT3)
(MT1Q1)
Electric Potential (voltage) V: The unit is V (volt).
B is frequently expressed in cgs unit, that is gauss.
1 W ( watt) = 1 J s 1 = 1 kg m 2 s 3
6.
1 V ( volt) = 1 WA 1 = 1C 1 kg m 2 s 2 (L2MT2Q1)
7.
Resistance R: The unit is W (ohm).
1 gauss = 10 4 Wbm 2 = 10 8 Wb cm 2 (MT1Q1)
12. Inductance L: The unit is H (henry). 1 H ( henry) = 1 Wb A 1 = 1C 2 kgm 2
1 (ohm) = 1 VA 1 = 1C 2 kg m 2 s 1
(L2MQ2)
(L2MT1Q2)
8.
Conductance G: The unit is S (siemens). 1S (siemens) = 1 W 1 = 1C 2 kg 1 m 2 s (L2M1TQ2)
Electric flux y: The unit is C (coulomb) or electric flux lines. Electric flux density D: The unit is Cm2 or electric flux lines per m2. (L2Q) 10. Capacitance C: The unit is F (farad). 9.
1 F ( farad) = QV 1 = 1C 2 kg 1 m 2 s2 (L2M1T2Q2)
A list of SI units for some physical parameters frequently encountered is given in Table 14. 1.4.6 Cgs System of Units and Cgs/SI Conversion The basic units of the cgs system are cm (centimeter), g (gram), and s (second). But, the fourth unit depends on whether it is based on the cgs electrostatic system of units (esu) or based on the cgs electromagnetic system of units (emu). For the esu system, the permittivity in free space is assigned to be 1 (unra
Table 14 SI units for some physical parameters frequently used. Physical Parameter Temperature Frequency Force Pressure Energy Power Current Electric Potential Resistance Conductance Electric Flux Electric Flux Density Capacitance Magnetic Flux Magnetic Flux Density Inductance
Symbol
SI Unit
Dimensions
T f or v F X E P I V R G y D C f B L
K (kelvin) Hz N (newton) Pa (pascal) J (joule) W (watt) A (ampere) V (volt) … (ohm) S (siemens) C (coulomb) C/m2 (coulomb/m2) F (farad) Wb (weber) T (tesla) H (henry)
K s1 (T1) kg/m/s2 (LMT2) N/m2 (L1MT2) N/m (L2MT2) J/s1 (L2MT3) C/s1 (T1Q) W/A1 (L2MT2Q1) V/A1 (L2MT1Q2) A/V1 (L2M1TQ2) C (Q) C/m2 (L2Q) Q/V1 (L2M1T2Q2) V/S (L2MT1Q1) Wb/m2 (MT1Q1) Wb/A1 (L2MQ2)
Introduction
tionalized dielectric constant), the fourth basic unit is statcoulomb, and each unit is designated by prefixing the syllable stat to the name of the corresponding unit. For the emu system, the permeability uo in free space is assigned to be 1 (unrationalized magnetic constant), the fourth basic unit is abampere, and most units are designated by prefixing the syllable ab to the name of the corresponding units, exceptions are the maxwell, gauss, oersted, and gilbert. In the statcgs (esu) system, eo = 1 (unrationalized), the electric flux is defined in such a manner that 4p lines of electric flux emanate from each statcoulomb of charge. That is
In the unrationalized abcgs (emu) systems, uo = 1. Following the same procedure, we can write the magnetic flux density B in terms of mks–(SI) units and that in terms of ab cgs–(emu) units as follows: B(in webers m 2 ) B(in maxwells cm 2 ) uour H(in amperes m 1 ) 1ur H(in gilberts cm 1 ) webers gilberts centimeters = maxwells amperes meters =
or uo [in mks–(SI) units] = 4p ¥ 10 7 henry per meter
y = 4pQstat
Thus, the rationalized statcgs (esu) system is characterized by the fact that the electric flux density is expressed as statcoulomb per cm2. Based on this relation, we can write the electric flux density D in terms of mks–(SI) units and that in terms of stat cgs–(esu) units as follows: D(in coulomb m 2 ) e o e r (in volts m 1 ) = 2 D(in cgs lines cm ) 1e r F(in statvolts cm 1 )
= 1.254 ¥ 10 6 Hm 1 = 1.254 ¥ 10 6 C 2 kg m (LMQ2)
The following is the transformation of the quantities between the mks (SI) and the cgs (emu) units: Charge:
abcoulomb = 10 1 coulomb abfarad = 10 9 farad
Capacitance:
or e o (in mks – SI units ) coulombs statvolts centimeters = 4p statcoulombs volts meters 1 = farad meter 1 36p ¥ 10 9 = 8.854 ¥ 10
12
Fm
1
2
= 8.854 ¥ 10 C 2 kg 1 m 3 s 2 (L3 M 1T 2 Q 2 )
The following is the transformation of the quantities between mks (SI) and cgs (esu) units: Charge:
statcoulomb = 3 ¥ 10 9 coulomb
Resistance: Voltage:
statohm 1 = ohm 9 ¥ 1011
statvolt 1 = volt 300
Capacitance: Current:
37
statfarad = 9 ¥ 1011 farad
statampere = 3 ¥ 10 9 ampere
Voltage:
abvolt = 108 volt
Magnetic flux:
maxwell = 10 8 weber
abampere = 10 1 ampere Magnetic flux density:
Current:
gauss(maxwell cm 2 ) = 10 4 weber m 2 Resistance:
abohm = 10 9 ohm
Magetomive force ( mmf ): abampere turn ( gilbert ) 4p = ampere turn 10 abhenry = 10 9 henry Magnetic field strength: Inductance:
abampere cm 1 (oersted ) 4p = 3 ampere m 1 10
Based on the above relations, we obtain
38 Dielectric Phenomena in Solids
e o (esu) = c2 e o (emu) 1 uo (esu) = 2 uo (emu) c
Similarly, the number of SiO2 molecules per cm3 is NSiO2 = (6.022 ¥ 10 23 mole 1 60 grams mole 1 ) ¥ 2.22 g cm 3 = 2.23 ¥ 10 22 molecules cm 3
1.4.7 The Unit of Debye The unit of debye is frequently used in the literature to give a numerical value of dipole moments. One debye is one unit of dipole moment formed by positive and negative charge of the charge equal to q (electron charge), which is 4.803 ¥ 1010 statcoulomb, and the positive and negative’s charge separation of 0.2A = 2 ¥ 109 cm. Thus, 1 debye = 4.803 ¥ 10 10 statcoulomb ¥ 2 ¥ 10 9 cm 10 18 esu
In terms of SI units, we have 1 debye = 1.602 ¥ 10 19 coulomb ¥ 2 ¥ 10 11 m = 3.2 ¥ 10 30 cm 1 3 ¥ 10 29 cm
where 2.33 g cm3 and 2.22 g cm3 are, respectively, the densities of Si and SiO2.
References 1. 2. 3. 4. 5. 6.
1.4.8 The Chemical Unit of Mole The definition of Avogadro’s number of 6.022 ¥ 1023/mole is the number of atoms or molecules per one gram atomic weight. For one gram atomic weight of hydrogen with atomic weight of one gram, one mole of hydrogen contains 6.022 ¥ 1023 hydrogen atoms. For one gram atomic weight of oxygen with atomic weight of 16 grams, one mole of oxygen also contains 6.022 ¥ 1023 oxygen atoms. Similarly, for one gram atomic weight of silicon with atomic weight of 28 grams, one mole of silicon still contains 6.022 ¥ 1023 silicon atoms. Thus, one mole of silicon oxide (SiO2) with a molecular weight of 28 + 2 ¥ 16 = 60 grams contains 6.022 ¥ 1023 SiO2 molecules. To transform this number into practical units in terms of the number of atoms or the number of molecules per cm3, we need to know the density of the material r (grams per cm3). For example, the number of silicon atoms per cm3 is NSi = (6.022 ¥ 10 23 mole 1 28 grams mole 1 ) ¥ 2.33 g cm 3 = 5 ¥ 10 22 atoms cm 3
7. 8. 9. 10. 11. 12. 13. 14. 15.
16. 17.
H.H. Skilling, Exploring Electricity (Ronald Press, New York, 1948). M. Faraday, Phil. Trans. 128, 1, 79, 265 (1837/38). J.C. Maxwell, Treatise on Electricity and Magnetism (Dover, New York, 1954). R.P. Feynman, R.B. Leighton, and M. Sands, The Feynman Lectures in Physics (AddisonWesley, New York, 1989). W.R. Smythe, Static and Dynamic Electricity (McGrawHill, New York, 1950). J.A. Stratton, Electromagnetic Theory (McGrawHill, New York, 1941). A.R. von Hippel, Molecular Science and Molecular Engineering (John Wiley and Sons, New York, 1959). C. Kittel, Introduction to Solid State Physics, 5th Edition (John Wiley and Sons, New York, 1976). P. Langevin, J. Phys. 4, 678 (1905). P. Debye, Polar Molecules (Dover, New York, 1945). R.M. Bozorth, Rev. Mod. Phys., 19, 29 (1947) and also Ferromagnetism (Van Nostrand, New York, 1951). A.H. Morrish, Physical Principles of Magnetism (John Wiley and Sons, New York, 1965). C. Kittel and J.K. Galt, “Ferromagnetic Domains,” Solid State Physics, 3, 437 (1956). A. Abragam, Nuclear Magnetism (Oxford University Press, Oxford, 1961). G.E. Pake, “Nuclear Magnetic Resonances” in Solid State Physics, Ed. by F. Seitz and D. Turnbull, Vol. 2 (Academic Press, New York, 1956). R.T. Schumacher, Introduction to Nuclear Magnetic Resonance (W.A. Benjamin Publishers, New York, 1970). E.K. Zavoisky, J. Phys. U.S.S.R., 9, 211, 245, and 447 (1945), and also 10, 170, and 197 (1946).
Introduction
18. 19. 20. 21. 22. 23. 24.
B. Bleany and K.W.H. Stevens, Rep. Progr. Phys., 16, 108 (1955). G.E. Pake, Paramagnetic Resonance (W.A. Benjamin Publishers, New York, 1962). W. Low, in “Paramagnetic Resonance in Solids,” Solid State Physics Supplement 2 (Academic Press, New York, 1962). A.F. Kip, C. Kittel, R.A. Levy, and A.M. Portis, Phys. Rev., 91, 1066 (1953). H.H. Stadelmaier and E. Th. Honig, Permanent Magnetic Materials, J. of Metals, 43, 32 (1991). R.E. Hummel, Electronic Properties of Materials, 2nd Edition (SpringerVerlag, New York, 1993). J.C. Anderson, Magnetism and Magnetic Materials (Chapman and Hall, London, 1968).
25. 26. 27. 28. 29. 30. 31. 32.
39
N. Braithwaite and G. Weaver, Electronic Materials (ButterworthHeinemann, London, 1990). J.C. Mallionson, The Foundation of Magnetic Recording, (Academic Press, New York, 1987). M. Ohring, The Materials Science of Thin Films (Academic Press, New York, 1992). A.H. Bobeck and E. Della Torre, Magnetic Bubbles, (NorthHolland, Amsterdam, 1975). G.S. Almasi, Proc. IEEE., 61, 438 (1972). E.A. Giess, Science, 208, 938 (1980). A.R. von Hippel, Dielectrics and Waves (John Wiley and Sons, New York, 1954). E. Goldin, Waves and Photons: An Introduction to Quantum Optics, (John Wiley and Sons, New York, 1982).
2 Electric Polarization and Relaxation The task of science is both to extend the range of our experience and to reduce it to order. Only by experience itself do we come to recognize those laws which grant us a comprehensive view of the diversity of phenomena. The classical theories have contributed so fundamentally to our knowledge of atomic structure. Neils Bohr
2.1
Fundamental Concepts
F is determined by the magnitudes and the locations of all other charges, as well as the surrounding medium. For a singlepoint charge with total net charge +Q in free space, F can be written as
We can say that all dielectric phenomena arise from an electric force which is primarily due to the attraction and the repulsion of electric charges. The action of the force tends to reduce the potential energy of the whole electrically stressed system to a minimum. This is a universal law of nature. Photocopies stick together, dust collects on television screens, dirty particles adhere to outdoor power transmission line insulators, etc.: Such phenomena are caused by this force. In the following sections, we shall discuss the origin of this force.
F=
(22)
where r is the distance between the location of +Q and a point P, and eo is the permittivity of the medium. From Equations 21 and 22, it can be seen that the force acting on the charge q can either be attractive or repulsive, depending solely on the relative polarity of Q and q, as shown in Figure 21. In a neutral atom or molecule, or any neutral particle, the number of electrons is equal to the number of protons. When such a neutral entity loses one electron, it becomes a positive ion (i.e., the entity has one proton which is not neutralized by the electron); when the entity receives an electron, it becomes a negative ion. Free ions are just like free electrons and will move in the presence of an electric field. A charged particle moving due to an electric force will have an acceleration a, based on Newton’s law, given by
2.1.1 Electric Charge Carriers and Their Motion The most important electric charges are electrons and protons, which are the major elementary particles of any atom of any material. Both the electron and the proton are the elementary charges; they are equal in magnitude, but opposite in charge polarity. An electron has a negative charge q, and a proton has a positive charge +q, where q = 1.602 ¥ 1019 C. An electric field can be considered a region in which a particle with a charge q would experience an electric force acting on it. This force, denoted by F, is given by F = qF
Q 4pe o r 2
a=
F qF = M M
(23)
Since the charged particle is accelerated in the direction of the field, it exhibits a kinetic energy
(21)
where F is the electric field strength at the point the particle is placed. The electric field strength
1 Mv 2 = Ú F dr = Ú qFdr 2 41
(24)
42 Dielectric Phenomena in Solids
where M is the mass, v is the velocity of the particle, (i.e., charge carrier), and r is the length of the path along which the particle has traveled. In a nonuniform field, such as that produced by a point charge +Q, the velocity of the charge carrier varies from point to point. Supposing that the charge carrier is an electron and it is placed at point P at t = 0, v = 0, and r = r1, then its velocity at point P¢ where r = r2 can be expressed as 12
2q v = ÈÍ Ú Fdr ˘˙ Îm ˚
12
2 qQ r2 dr ˘ = ÈÍ Î 4pe o m Úr1 r 2 ˙˚
12
qQ Ê 1 1 ˆ ˘ = ÈÍ Î 2pe o m Ë r1 r2 ¯ ˙˚
(25)
that produced by a point charge +Q shown in Figure 21. In this case, the neutral particle will be polarized, shifting the normally symmetrical electron clouds of atoms or orienting existing permanent dipoles, if any, toward the direction of the field. Electric polarization processes will be discussed in Section 2.3. This neutral particle, polarized by the field, will become an overall large dipole consisting of two charges equal in magnitude but opposite in polarity, +qd and qd, separated by a small distance d. At point P¢, where this dipole is located, the charge qd will experience an attractive force given by F1 = qF =  qd
It can be seen from Equations 24 and 25 that the velocity and the kinetic energy of an electron or a negative ion increase as it travels toward a convergent field, and decrease when it travels in a divergent field. Suppose now we place a neutral particle with a permittivity e2 in a nonuniform field such as F
F2 = qF = + qd
–q –
F –q +
+q P'
F
– +
–qd +qd
Figure 21 Nonuniform electric field F produced by a single point charge +Q, and the force between +Q and various charged particles. Electron with a charge q. Negative ion with a charge q. Positive ion with a charge +q. Dipole formed by a polarized neutral particle with a net negative charge qd on one end and a net positive charge of +qd on the other at a separation of d. Y The direction of the force.
(27)
In this case, F1 is larger than F2 by an amount equal to
=
+Q r=0
Q 4pe o ( r + d )2
DF = F1  F2 =
F
(26)
and the charge +qd will also experience a force, which is repulsive, given by
F
P
Q 4pe o r 2
qd Q d 2pe o r 3
qd Q Ê 1 1 ˆ Á ˜ 4pe o Ë r 2 ( r + d )2 ¯
(28)
since r is much larger than d. This force always tends to move the particle from the weak field region to a strong field region. It should be noted that, apart from this force, there is another force arising from the release of some stored potential energy of the system: in the present case, the permittivity of the particle e2 > eo. This force also helps to move the particle to a strong field region because this action would reduce the potential energy of the system. This is why dust is attracted to television screens and dirty particles are collected on the surface of power transmission line insulators, which may lead to a very harmful effect. This force depends on the relative magnitude of the permittivity of the particles and that of the medium. We shall discuss this force further in a later section. Now let us consider the case with a constant uniform electric field F. Such a uniform field can be produced simply by connecting a steady DC voltage supply across two parallel metallic
Electric Polarization and Relaxation x=d
ss
+Q
D
A
F
Electron x=0
–Q
Ion –
Figure 22 Uniform electric field F produced inside a capacitor by the uniformly distributed charge +Q on plate A and Q on plate B, the separation between two parallel plates being d and the area of each plate being A.
plates and charging this system as a capacitor. After charging, the supply is disconnected and removed from the system, leaving positive charge +Q on plate A and a negative charge Q on plate B, as shown in Figure 22. The electric field created by the charges on the plates can be considered to be uniform in the region between the plates if the edge effect is ignored. This field F can be written as Q ss D F= = = eA e e
(29)
where e is the permittivity of the medium, A is the area of the plates, ss is the surface charge density on the plates, and D is the electric flux density in the medium, which is equal to ss if the medium is free space. Now, if we place an electron or a negative ion at a point very close to x = 0, as shown in Figure 22, this charge carrier will move freely from x = 0 to x = d if the medium is free space with e = eo. This carrier will be accelerated along the field direction without encountering any collision. Thus, we can write F = qF = Ma qF a= M
(210)
where M is the mass of the carrier, and M = m if it is an electron. The acceleration a is equal to dv/dt, thus the velocity of the carrier can be expressed as t
v = Ú adt = at o
increases with t, the time required to travel a unit distance decreases as x increases from 0. Suppose it takes td time for the carrier to travel to x = d from x = 0, then the velocity of the carrier at x = d can be expressed as (212)
vd = atd B
(211)
where a is constant since F is constant, but v increases linearly with traveling time t. Since v
43
Thus, the average velocity can be written as v=
atd 2
(213)
Since t d = d v, the average velocity can be expressed in the form qFd ˆ v =Ê Ë 2M ¯
12
(214)
The mobility of the carrier is defined as the velocity per unit electric field strength, so the average mobility of the carrier u is the average velocity per unit field strength. Thus, u=
v Ê qd ˆ = F Ë 2 MF ¯
12
(215)
The average velocity of the carrier in this case is proportional to (F)1/2, while the average mobility of the carrier is inversely proportional to (F)1/2. Now we will consider the case for solids, such as semiconductors or dielectric materials. In this case, there are about 1022 to 1023 atoms or molecules per cm3. It can be imagined that in solids, a charge carrier will not move freely as in free space. It will suffer many, many collisions with phonons and impurities during its movement from x = 0 to x = d in the same electrode configuration shown in Figure 22. Based on Equation 29, for the same charges on plates A and B, F will be smaller by a factor of e = e r . An electron (or a hole) will react with eo the lattice vibrations (i.e., phonons) and other imperfections in the material, and its quantum state is governed by Pauli’s exclusion principle. To take into account the effects of the inertia due to all the interactions and to make the motion of electrons or holes to follow the classical Newton’s law, we use the effective mass m* instead of the conventional electron mass mo in free space, which is practically equal to the rest mass of the electron because, for most
44 Dielectric Phenomena in Solids
cases, the electron velocity is much smaller than the light velocity, so the relativistic effect can be ignored. The electric field exerts on the electron an electric force qF, but the electron encounters a friction force (called an inertia force or a viscous force) due to the collisions with phonons and imperfections (structural defects and chemical defects or impurities). Assuming that this friction force, which opposes the electric force, has the form m*v/t, where v is the drift velocity of the electron and t is the collision time, then based on Newton’s law, we can write m*
dv v = qF  m * dt t
(216)
The friction force tends to retard the motion of the electron. In the steady state condition, dv/dt = 0, and Equation 216 reduces to v=
qt F = mF m*
(217)
where m is called the electron mobility, which is defined as the drift velocity per unit field strength m = dv dF =
qt m*
(218)
Electrons in a solid also have their thermal velocity vth, due to thermal agitation. The direction of thermal velocity is random, and hence the random motion of electrons does not contribute to electrical conductivity. Drift velocity leads the electrons to move in the direction of the electric field and hence contributes to the electrical conductivity, which is defined as the electrical current density J per unit electric field strength. Thus, the electrical conductivity s is given by s=
J qnv = = qmn F F
(219)
where n is the concentration of electrons. Both thermal velocity and drift velocity are temperature dependent. Thermal velocity is given by Ê 2 kT ˆ vth = Á ˜ Ë 3m * ¯
12
(220)
which is proportional to (T)1/2. It is usually much larger than the drift velocity. The temperature dependence of drift velocity or mobility is mainly due to the temperature dependence of t. The collision time t is sometimes called the mean free time or relaxation time. It is really the time between collisions. Based on the quantum mechanics, an electron has a wave character. Thus, a wave passing through a perfect periodic lattice should travel freely without scattering (or collision).1 However, the lattice is far from perfect periodicity because thermal agitation causes lattice vibrations (or atomic vibrations), which generate phonons, and also various defects (structural and chemical) in the material form scatterers to collide with electrons. In general, the probability of electron collision with phonons increases with increasing temperature, while the probability of electron collision with defects decreases with increasing temperature. That the mobility decreases with increasing temperature is mainly due to the decrease of t with temperature. Ions are much larger in size than electrons. It can be imagined that it would be much more difficult for ions to move in solids. Small ions may be able to move by jumping from one interstitial site to the next, but large ions must move from one lattice site to the next, which must be vacated for their occupation. Thus, the probability of ion movement depends on the probability of the creation of a vacancy next to the moving ion. For large ions, the activation energy for their movement involves several eV. Donors or acceptors in semiconductors or insulators, when ionized, become positive or negative ions, respectively. These ions, for most practical cases, cannot move at normal temperature. Charge carrier transport processes will be discussed in Ionic Conduction and Electronic Conduction in Chapter 7. 2.1.2 Electromechanical Effects In an electrically stressed system, there is always a force tending to reduce the stored potential energy of the system. For a simple capacitor, shown in Figure 22, the force tends to increase the capacitance in order to reduce
Electric Polarization and Relaxation
the potential between the two charged plates so as to reduce the potential energy, since the decrease in V would result in a decrease in potential energy, which is equal to QV/2 or CV2/2. If the medium inside the capacitor is air, such a force would tend to attract any substance with a permittivity larger than eo into the capacitor to replace the air medium. In the following discussion, it is assumed for mathematical simplicity that the dielectric system is isotropic and linear, and heat losses and other effects, such as thermal agitation and gravitation, are ignored. If the initial charges in the system are fixed, then any mechanical work done for the reduction of the potential energy of the system must be at the expense of the stored energy in the system. The change of the stored potential energy DU in the system, due to the introduction of a dielectric body of volume V2 and permittivity e2 into a dielectric system of volume V1 and permittivity e1, can be evaluated by DU =
1 (e 2  e1 )F1 F2 dV 2Ú
Medium 1 of permittivity e1 and medium 2 of permittivity e2 separated by a plane boundary.
The field in the media parallel (or tangential) to the boundary, as shown in Figure 23(a). For this case, the tangential fields in the two media are equal. (222)
F2 t = F1t
Case i (b):
F2 n =
The field in the media normal (or perpendicular) to the boundary, as shown in Figure 23(b). For this case, the relation of the fields in both sides is given by
e1 F1n e2
Case i (c):
(221)
where F1 is the electric field in the region of the dielectric medium in the system of permittivity e1 where a dielectric body of permittivity e2 is subsequently introduced, and F2 is the electric field in the dielectric body itself.2 The stored potential energy of the system after the introduction of the body into the system is decreased when DU is positive, and increased when DU is negative. Using Equation 221, we have derived the electromechanical forces resulting from the change of the stored energy of the system for the following cases.3 Before presenting our analysis of the cases, it is desirable to review briefly some formulas about the field distribution inside and outside a dielectric body of permittivity e2 placed in a medium of permittivity e1, which is stressed in a uniform static electric field F1. The field inside the dielectric body F2 depends on the geometric shape of the body. The formulas for some common configurations shown in Figure 23 are summarized as follows.4–6 1.
Case i (a):
45
(223)
The field inclined with an incident angle q1 incident on the boundary, as shown in Figure 23(c). For this case, we have
F1t = F1 sin q1 , F2 t = F2 sin q 2 ,
F1n = F1 cosq1 F2 n = F2 cosq 2
Based on Equations 222 and 223, we have tan q1 e1 = tan q 2 e 2
2.
This is the law of refraction (see Wave Theory in Chapter 3). A dielectric sphere with a radius a. For this case, the field inside the sphere is given by F2 =
3
3e1 F1 2e1 + e 2
(224)
F2 < F1 for e2 > e1, as shown in Figure 23(d) and F2 > F1 for e2 < e1, as shown in Figure 23(e). A dielectric ellipsoid with its major axis 2c and 2 equal minor axes 2a and 2b, i.e., a prolate spheroid with c > a = b. Case iii (a): The field in the medium parallel to the major axis. For
46 Dielectric Phenomena in Solids
F1n
e1
e1 F1t
F2t
e1
e2
F1t
q1
e2
e2
(a)
F1
F1n
F2t q2
F2n
(b)
(c)
Sphere with e2 > e1
Sphere with e2 < e1
(d)
(e)
Spheroid with field parallel to major axis 2c and e2 > e1
(f)
F2n
F2
Spheroid with field normal to major axis 2c and e2 > e1
(g)
Figure 23 Electric field distribution in two media separated by a boundary. (a) Tangential field parallel to a plane boundary, (b) normal field perpendicular to a plane boundary, (c) inclined field with an incident angle q1 incident on a plane boundary, (d) a sphere of radius a having permittivity e2 in a medium having permittivity e1 with e2 > e1, (e) same as (d) but with e2 < e1, (f) a spheroid of major axis 2c having permittivity e2 in a medium of permittivity e1 with e2 > e1 and the field parallel to the major axis 2c, and (g) same as (f) but with the field normal to the major axis 2c.
this case, the field inside the spheroid is given by F2 =
e1 F1 e1  (e1  e 2 )G//
(225)
where G11 is given by G// =
a2c • ds 2 Ú0 ( s + c 2 )3 2 ( s + a 2 )
Case iii (b):
F2 =
e1 F1 e1  (e1  e 2 )G^
(227)
where G^ is given by
(226)
1 In this case, G// < , F2 < F1 3 for e2 > e1, as shown in Figure 23(f).
The field in the medium normal to the major axis. For this case, the field inside the spheroid is given by
G^ =
ac 2 2
Ú
•
0
ds (s + a ) (s + c2 ) 2 32
(228)
In this case, G > 1/3, F2 < F1 for e2 > e1, as shown in Figure 23(g).
Electric Polarization and Relaxation
47
With these formulas, we can now analyze the following cases.
tivity. Because of the presence of this force, we would expect the occurrence of the following electromechanical effects:
The Force Acting on the Boundary between Two Different Dielectric Materials At the boundary between two different materials 1 and 2, the electric flux is usually refracted, and the tangential components of the electric field F1t and F2t, as well as the normal components, F1n and F2n, follow the relationship based on Equations 222 and 223, which are
• If material 1 is air with e1 = e0, and material 2 is a dielectric solid or liquid with e2 > e1, there is always a pulling force to pull material 2 into the space of air. Since the force is proportional to F2, a big mechanical impact on the dielectric solid may occur when the insulation system is subjected to a high voltage transient or switching surge. • If material 1 is a dielectric fluid, such as transformer oil or hydrocarbon liquids with e1 > eo, and material 2 is a particle with e2 < e1, then under a nonuniform electric field, such as that shown in Figure 21, the particle may be ejected from the strong field region because the force given by Equations 233 and 234 is more dominant than the force given by Equation 28. In this case, these two forces are present but, in opposite directions. For example, in the strong field region near the high voltage windings of a power transformer, in which transformer oil is generally used for both heat transfer and insulation purposes, we would expect that any gas bubbles formed in the transformer oil would be ejected from the strong field region, and any particles with e2 > e1 and conductive particles, particularly moistureabsorbed particles, would be attracted to the strong field region, resulting in many insulation problems in power transformers.
F1t = F2 t
(229)
F1n = e 2 F2 n e1
(230)
where e1 and e2 are, respectively, the permittivities of materials 1 and 2. According to Equation 221, there is a force acting on the boundary with the tendency of expanding material 2 into material 1 if e2 > e1. The decrease in stored energy due to the expansion of a small volume dV of material 2 into material 1, due to the tangential component of the field, is then dUt =
1 (e 2  e1 )F12t dV 2
(231)
Thus, the force acting normally on the boundary is dFt = —( dUt ) =
1 (e 2  e1 )—F12t dV 2
(232)
since dFt /dV = —pt, where pt is the mechanical stress, which is the mechanical force per unit area. Therefore, the mechanical stress due to the tangential components of the field can be written as pt =
1 (e 2  e1 )F12t 2
(233)
Similarly, it can easily be shown that the mechanical stress due to the normal components of the field is Pn =
1 e1(e 2  e1 ) 2 F1n 2 e2
(234)
Both pt and pn are normal to the boundary, tending to cause the dielectric material having a higher permittivity to move into the space occupied by the other, having a lower permit
The Force Acting on Conductor Surfaces The attractive force between two parallel metal plates with opposite electric charges, in contact with a dielectric material of permittivity e, will bring about deformation within the volume of the dielectric material in order to reduce the stored energy of the system. The decrease in stored energy resulting from a reduction of the volume of the material by a small amount of dV due to this compressive force can be written as dU =
1 2 eF dV 2
(235)
where F is the electric field strength produced by the charges on the metal plates. Following
48 Dielectric Phenomena in Solids
the same derivation procedure, the compressive pressure acting on the dielectric material is Pc =
1 2 eF 2
(236)
This mechanical stress will result in a compression of the dielectric material, and its effect on the breakdown strength of polymers has been reported by several investigators.7,8 For example, a dielectric material, such as an insulating polymer, having a relative permittivity of 4 stressed at a field of 2 MV cm1, may suffer a compressive pressure of about 273 newtons cm2. This pressure, which increases proportionally with permittivity and the square of applied electric field, may be sufficient, especially under transient overvoltage conditions, to cause reduction of thickness or fracture of the insulation, followed by dielectric breakdown. The Force Elongating a Bubble or a Globule in a Dielectric Fluid A small bubble of gaseous or vapor phase or a globule of liquid phase of permittivity e2 in a dielectric fluid of permittivity e1 always takes on a spherical shape because of surface tension. In the presence of an electric field F1 in the dielectric fluid, the field strength inside a spherical bubble or globule is given by Equation 224. Thus, by substituting Equation 224 into Equation 221, we would obtain the change in stored energy in the electrically stressed dielectric fluid due to the introduction of a bubble or globule, which is DUs =
1 È 3e1(e 2  e1 ) ˘ 2 Ê 4 3 ˆ F1 pr ¯ 2 ÎÍ 2e1 + e 2 ˚˙ Ë 3
(237)
where r is the radius of the spherical bubble or globule, and F1 is the field strength in the region of the fluid which the bubble or globule subsequently occupies. It is assumed that a spheroidal shape is a good approximation to that into which a spherical bubble or globule may be expected to deform, and that the volume of the bubble or globule remains unchanged while its shape deforms from a sphere into a spheroid. As the field strength inside a spheroidal bubble or globule is given by Equation 225, substitu
tion of Equation 225 into Equation 221 gives the change in stored energy in the electrically stressed dielectric fluid due to the presence of a spheroidal bubble or globule, which is DUe =
1 È e1(e 2  e1 ) ˘ 2 Ê 4 3 ˆ F1 pr ¯ 2 ÍÎ e1  (e1  e 2 )G ˙˚ Ë 3
(238)
Thus, the work done at the expense of the stored energy for the deformation of the bubble or globule is DU = DUe  DUs =
1 È e1(e 2  e1 )2 (1  3G) ˘ 2 ÍÎ (2e1 + e 2 )[e1  (e1  e 2 )G] ˙˚ 4 • F12 Ê pr 3 ˆ Ë3 ¯
(239)
When DU is positive, the stored energy is further reduced after the bubble or globule is degenerated into a spheroid. For DU > 0, G must be less than 1/3, according to Equation 226. This corresponds to a prolate spheroid, implying that the spherical bubble or globule is elongated along the direction of the applied field, irrespective of whether the permittivity of the globule is larger or smaller than that of the fluid. The force involved in the elongation can be derived as follows: By assuming that the volume of the bubble or globule is unchanged during elongation (we make this assumption purely for mathematical simplicity; there should be some change during the elongation process), we can write r 3 = ca 2
(240)
When the sphere is slightly deformed by elongation of the major axis from the original 2r to 2(r + dc), then we have c = r + dc
(241)
and hence 3dc a2 r3 = 1 2 ( r + dc)3 c r
(242)
the terms of higher powers in the binomial expansion being ignored. Substituting Equation 242 into Equation 226 and then integrating it, we obtain
Electric Polarization and Relaxation
G=
1 dc 3 r
(243)
Substitution of Equation 243 into Equation 239 gives the decrease in stored energy due to a bubble or globule with its major axis elongated from 2r to 2(r + dc) d(DU ) =
(244) Thus, the elongation force is Fe =
Ê 4 pr 3 ˆ Ë3 ¯
(245)
The elongation phenomenon was first predicted based on a simple analysis by Kao,3,9 and later verified experimentally by Kao10 and further analyzed rigorously by Garton and Krasucki.11 Electric breakdown of dielectric liquids has been attributed to the formation and subsequent elongation of vapor bubbles in the liquids.12 The Dielectrophoretic Force Unlike electrophoresis, in which the motion of particles depends on the charge of the particles, dielectrophoresis is defined as the motion of neutral particles in a nonuniform electric field, depending only on the force acting on polarized particles. The dielectrophoretic force tends to draw the particles whose permittivities are larger than that of the dielectric medium from the weak field to the intense field region, and to reject those with lower permittivities from the intense field to the weak field region in the same manner described in Section 2.1.2. On the assumption that the particles are spherical in shape, the change in stored energy due to the presence of spherical particle of radius a and permittivity e2 in a dielectric medium of permittivity e1 and stressed at a field F1 can be calculated from Equation 237. Thus, the dielectrophoretic force can be written as Fd = —(DUd ) 1 3e1(e 2  e1 ) ˘ 2 Ê 4 3 ˆ = ÈÍ pa —F1 Ë3 ¯ 2 Î 2e1 + e 2 ˙˚
Consider a nonuniform field, such as that produced by a single point charge Q given by Equation 22; the dielectrophoretic force can be expressed as Fd =
1 È 3e1(e 2  e1 ) ˘Ê 4 3 ˆ È Q2 ˘ pa Í 2 2 5 ˙ ¯ Î 4p e 1 r ˚ 2 ÍÎ 2e1 + e 2 ˙˚Ë 3
(247)
9 È e1(e 2  e1 )2 ˘ 2 Ê 4 3 ˆ dc F1 pr ¯ r 2 ÍÎ (2e1 + e 2 )2 ˙˚ Ë 3
d(DU ) dc 9 È e1(e 2  e1 )2 ˘ F12 = Í 2 Î (2e1 + e 2 )2 ˙˚ r
49
(246)
This force depends on the distance from the point charge r and is opposed by a viscous drag of the medium, which, according to Stokes’s law, is 6ph av, where h is the viscosity of the medium and v is the velocity of the particle. Hence, the velocity of the particle in such a nonuniform field can be approximately evaluated by v=
1 È 3e1(e 2  e1 ) ˘Ê 2 a 2 ˆ È Q2 ˘ 2 ÎÍ 2e1 + e 2 ˚˙Ë 9h ¯ ÍÎ 4p 2e 21 r 5 ˙˚
(248)
The dielectrophoretic effect may be used to produce pumping action of nonconducting liquids, to cause separation of the components in suspension in a dielectric fluid, to cause precipitation, or to produce mixing.13 The Electrostriction Force Electrostriction is defined as the elastic deformation of a dielectric material under the force exerted by an electric field. A dielectric material can be thought of as consisting of dielectric particles (atoms or molecules) uniformly distributed throughout a vacuum space. Thus, the local field acting on each particle is higher than the apparent or measured field by an amount resulting from the polarization field of the surrounding polarized particles. This local field is given by Floc =
e + 2e o F 3e o
(249)
where e and eo are the permittivities of the dielectric material and vacuum, respectively. (See Section 2.5.) The polarization involves the displacement of electric charges, shifting the originally symmetrical charge distribution to an nonsymmetrical one. This implies that the polarization tends to elongate the particles in the direction of the field, i.e., to cause the
50 Dielectric Phenomena in Solids
material to expand in the direction parallel to the field and to contract in the direction perpendicular to the field. This process is accompanied by a slight decrease in volume of the material and hence a slight increase in density of the material. Suppose a material of volume V suffers a slight decrease in volume by dV and hence a slight increase in density by dr, due to elongation; then from Equation 221, the decrease in stored energy of this piece of material due to the decrease in volume by dV is d(DU )v =
1 È (e  e o )(e + 2e o ) ˘ 2 F dV 2 ÎÍ 3e o ˚˙
(250)
Hence, the torque exerted on the body is d(DUT ) dq 2pca 2e1(e 2  e1 )2 (Gy  Gx )sin 2q 2 F1 = 3[e1  (e1  e 2 )Gx ][e1  (e1  e 2 )Gy ]
T=
(253) where Gx =
•
0
ds ( s + c 2 )3 2 ( s + a 2 )
(a c ) [1  (a c ) ]
2 32
Ï ÔÔ Ì2 1  a c Ô ÔÓ
[
2 12
2
Gy =
ca 2 2
Ú
•
0
2
1 = 4
DUT =
2pca 2e1(e 2  e1 )2 (Gy  Gx )sin 2 q 2 F1 3[e1  (e1  e 2 )Gx ][e1  (e1  e 2 )Gy ]
(252)
¸ Ô 12 ˝ Ô ˛
(254)
ds ( s + c 2 )1 2 ( s + a 2 )2
(a c ) [1  (a c ) ]
2 32
[
2 12
[ ( )] + log 1 + [1  ( a c ) ] 1 1 ac
12
( )] ( )
Ï2 1 a 2 Ô c Ì 2 a Ô c Ó
2
The Torque Orienting a Solid Body If a body is not symmetrical about its center, it will experience a torque, tending to orient itself in such a manner that the stored energy in the electric field will become minimal. For simplicity, a prolate spheroidal shape is chosen as the approximation to the general shape of a solid body, and its principal axes, which follow the relationship c > a = b, form a rectangular coordinate frame, x directing the major axis 2c, y and z, the minor axes 2a and 2b. If one of the minor axes is originally in the direction of the field, the decrease in stored energy when its major axis orients and causes an angular displacement q, from Equations 221 and 225, is
2 12
( )]
[ ( )] + log 1 + [1  ( a c ) ] 1 1 ac
(251)
It should be noted that most solids are incompressible because the particles (atoms or molecules) are rigidly bonded together. For slightly compressible materials—such as some liquids, polymers, or ceramics—electrostriction phenomenon may be detectable. Also, the hydrostatic pressure may become significant for materials with high dielectric constants.
Ú
2
1 =2
Therefore, the hydrostatic pressure tending to contact the material is d(DU )v (e  e o )(e + 2e o ) 2 Pv = = F dV 6e o
ca 2 2
¸ Ô 12 ˝ Ô ˛
(255)
F1 is the field strength in the region of the dielectric medium where the solid body is subsequently placed, and e1 and e2 are the permittivities of the medium and the body, respectively. The torque tends to orient the major axis of the body to the direction of the field and is independent of the relative magnitudes of e1 and e2. The magnitude of the torque depends on the size and the position of the body. It is zero when the major axis of the body is perpendicular to the field, and is maximal when it is at the angle of 45° to the field. The torque exerted on the solid particles may accentuate the effect of impurities on the dielectric breakdown of liquids, but on the other hand, it may be used as a means to determine the permittivity of a dielectric sample of known shape. These six electromechanical forces may be appreciable when the impressed electric fields
Electric Polarization and Relaxation
are large. The directions of these forces are independent of the directions of the fields, implying that unidirectional and alternating fields will produce the same effects. 2.1.3 Electrostatic Induction Before discussing electric polarization and relaxation, it is desirable to review briefly the electrostatic induction phenomenon. Suppose that we have a positively charged insulator A with the charge distribution, as shown in Figure 24(a). If we now place an uncharged conductor B near the charged insulator A, the electrostatic field produced by A will shift the free electrons in B toward the surface close to A, resulting in the formation of a negative charge on one side and a positive charge on the opposite side, where there is a deficit of electrons, as shown in Figure 24(a). This phenomenon is referred to as electrostatic induction. The electric field inside B is zero because this field is composed of two components: one is the original field from A, which should always exist inside B, and the other is the field produced by the induced negative and positive charges in B, which is opposite to that
51
produced by A. If we now connect the conductor B to ground by a conducting wire, electrons will flow to B from the ground to make up the deficit of electrons on the positivecharge side, as shown in Figure 24(b). This is equivalent to saying that some positive charge flows out from B to ground. Thus, the negative charge on the side close to A is called the bound induced charge, while the positive charge on the opposite side is called the free induced charge. When the free induced charge disappears, both the magnitude and the distribution of the negative bound charge will change in such a way that the electric field inside B remains zero. Now, if the ground connecting wire is cut off and the conductor B is removed from the field produced by A, then the conductor B becomes an isolated negatively charged conductor, and the bound induced charge becomes free to move to redistribute itself on the surface in such a way that the electric field inside B is zero and the electric flux outside B is perpendicular to the surface of B, because any tangential components of the electric field would cause the movement of surface charges. The charge distribution is dependent solely on the geometric shape of the conductor B. It should be noted
Bound Charge Free Charge Uncharged Conductor + + + + A + + + + +
– + – + – B + – ++ –
– – – B – –
+
+ + A + + + + +
F=0 Charged Insulator Uncharged Conductor Charged Insulator
(a)
F=0
(b) Dipoles – – – – – – –
+ + + + + + + + D Charged Insulator Insulator + + A + + + +
–
+
(c) Figure 24 Electrostatic induction: (a) positively charged insulator A and uncharged conductor B (isolated), (b) positively charged insulator A and uncharged conductor B (grounded), and (c) positively charged insulator A and isolated insulator D.
52 Dielectric Phenomena in Solids
that any change in charge distribution in conductor B due to different arrangements does not affect the charge distribution in the charged insulator A, simply because charges in insulator A cannot freely move. However, if A is a charged conductor instead of a charged insulator, then the induced charge in conductor B will also cause a change in charge distribution in charged conductor A, in order to make the electric field inside both A and B be zero. A conductor, or a conducting material, generally refers to the material consisting of a great many mobile free charge carriers, such as a metal in which the concentration of free electrons (mobile charge carriers) is of the same order as that of atoms, i.e., about 1022 to 1023 cm3, and electrolytes in which ions are the charge carriers. In those conducting materials, the electrostatic induction phenomenon prevails. But in other materials, such as semiconductors and dielectric materials, the number of mobile charge carriers is far less than the number of atoms. Although an electric field would cause the movement of mobile charge carriers to produce space charge polarization in a manner similar to electrostatic induction, space charge polarization usually plays an insignificant role because it involves only a small number of mobile charge carriers, as compared to electric polarization, which involves all atoms. Now, suppose the uncharged conductor B, shown in Figure 24(a), is replaced by an isolated uncharged insulator D of the same shape, shown in Figure 24(c). In this case, the field produced by the charged insulator A will not induce charge in D because there are practically no mobile free charge carriers in insulator D. Instead, the field will polarize the material by shifting slightly the normally symmetrical distribution of electron clouds of atoms and by orienting dipolar molecules toward the direction of the field to form dipoles. So, each atom or molecule contributes a tiny dipole to form a big dipole, as shown in Figure 24(c). If we remove the insulator D after it has been completely polarized, the polarized insulator D will undergo relaxation and gradually become depolarized, due to thermal agitation. Electric
polarization and relaxation processes are discussed in the following sections.
2.2 Electric Polarization and Relaxation in Static Electric Fields Electric polarization refers to a phenomenon of the relative displacement of the negative and positive charges of atoms or molecules, the orientation of existing dipoles toward the direction of the field, or the separation of mobile charge carriers at the interfaces of impurities or other defect boundaries, caused by an external electric field. A detailed account of various polarization processes will be given in Section 2.3. Electric polarization can also be thought of as charge redistribution in a material caused by an external electric field. The work done for the charge redistribution and the energy loss involved in the redistribution process require an energy supply. Where does this energy come from? We can say that the whole polarization process is performed at the expense of the potential energy released from this process, because the total potential energy of the system in an electric field is smaller after electric polarization than before it. We shall apply Gauss’s law to explain some dielectric phenomena resulting from electric polarization. As discussed in Gauss’s Law in Chapter 1, Gauss’s law simply states that the electric flux outward from a volume is equal to the total net charge enclosed inside it. We use a simple system consisting of two metal plates parallel to each other with an area A each and a separation d, which is much smaller than the linear dimension of the plates, so that the fringing effect at the edges can be ignored by approximation. Suppose we introduce a positive charge +Q on the upper plate and a negative charge Q of the same magnitude on the lower plate. This can be easily done by connecting a steady DC voltage supply across the plates and charging the system as a capacitor, and then disconnecting the supply from the system as soon as the charge has been accumulated to the desired value Q. These
Electric Polarization and Relaxation
charges on the plates will create a potential difference between the plates V that is proportional to Q. Thus, we can write Va Q Q V= or Q = CV C
(257)
Q ssA A = =e V Fd d
ss F
(258)
Where e is the permittivity of the material filled between the two plates, which is equal to the ss ratio of . In the following sections, we shall F discuss this ratio for three general cases. 2.2.1 Vacuum Space By true vacuum space, or free space, we mean that in the space there are no detectable particles, although there may be a hypothetical ether, thought of as the medium for the propagation of electromagnetic waves in free space. However, a true vacuum is not available on the earth. The best vacuum system that can be produced by today’s technology can achieve only a vacuum of about 1014 torr, in which there are still about 300 particles per cm3. Assuming that the space between the plates is free space, sso is equal to the electric flux density Do based on Gauss’s law, as shown in Figure 25. So we can write s so = Do = e o Fo
or
The volume containing Fo free surface charges of density sso
Plate B
From this we obtain e=
Do = e 0Fo
(256)
where F is the electric field strength, which is simply equal to V/d. From Equation 257 we can express C in the form C=
+Q
Plate A
where C is the proportionality constant, generally called the capacitance. By denoting the surface charge density on the plates as ss, the charge Q can be expressed as Q = C( Fd ) = s s A
53
–Q Figure 25 The electric field Fo and the associated electric flux density Do produced by the free surface charges of density sso on the plates in vacuum space (free space).
eo =
s so Fo
(259)
where Fo is the electric field strength in the vacuum space, which is equal to Q/Vo and Vo is the potential between two plates created by the charge Q; and eo is the permittivity of vacuum or free space, which is practically the same as the permittivity of dielectric gases, such as air, at normal pressure and temperature. The permittivity of gases, depending on the molecular structure, has only negligibly small deviation from the ideal value of eo at normal pressure and temperature.14 2.2.2 Conducting Materials A conducting material, or a conductor, refers to a material containing many mobile free charge carriers. For example, in a piece of copper or sodium, each atom contributes one free electron, making the total electron concentration equal to the concentration of atoms, i.e., 1022 to 1023 cm3. These electrons move freely and randomly and distribute themselves with statistical uniformity in the bed of regularly arranged positive ions. If such a piece of metal with the thickness of d2s were inserted into the space between the two charged plates, with a small gap s to separate the plates and the metal conductor, then the charge on the plates would cause the electrons in the conductor to move toward the surface close to the positively charged plate but could not leave the surface, resulting in a nonuniform distribution of the net
54 Dielectric Phenomena in Solids
charge. This creates a net negative space charge on one surface and a net positive space charge on the other in a manner similar to the electronic polarization of a neutral atom. Thus, in this case, we can say that charge Q on plate A induces a negative charge equal in magnitude but opposite in polarity on one surface of the metal close to plate A. Similarly, a positive charge is induced on the other surface of the metal by the negative Q on plate B. So, in the vacuum space between plate A and the metal surface, or between plate B, and the other surface of the metal, we have
es =
2.2.3 Dielectric Materials One of the important electrical properties of dielectric materials is permittivity (or relative permittivity, which is generally referred to as the dielectric constant). For most materials, the dielectric constant is independent of the electric field strength for fields below a certain critical field, at or above which carrier injection into the material becomes important. The dielectric constant depends strongly on the frequency of the alternating electric field or the rate of the change of the timevarying field. It
which is the same as that as given by Equation 259. The response in the vacuum space is exactly the same as that described in Section 2.2.1. However, inside the metal there is no electric flux based on Gauss’s law, as shown in Figure 26, and hence, F = 0.
Free Electron Distribution
The volume containing a positive charge on the plate surface of density Q/A and an induced negative charge on the conductor surface of density –Q/A, so the total net charge is zero.
Net Charges on the Surfaces of Metallic Conductor
(a)
Vacuum space d – 2s
s
s
(260)
In metal, the permittivity is • under static fields only. Under a timevarying field or an alternating field, the charges induced on the metal surfaces may not follow instantaneously the timevarying field. In this case, the permittivity is not infinite, but a finite value. We shall discuss this phenomenon further in later sections.
s so = Do = e o Fo s so eo = Fo
Positive Ion Distribution
ss Æ• F
Metal
F=0
Vacuum space
(b) Figure 26 (a) Induced net charges on the surfaces of a metallic conductor in the presence of a static electric field, and (b) the charge on the plate with the surface charge density sS inducing a charge equal in magnitude but opposite in polarity on the surface of the conductor, resulting in zero electric field inside the conductor. The vacuum space s is exaggerated for clarity.
Electric Polarization and Relaxation
also depends on the chemical structure and the imperfections (defects) of the material, as well as on other physical parameters including temperature and pressure, etc. This chapter is devoted to the discussion of electric polarization and relaxation under various conditions. A dielectric material is made up of atoms or molecules that possess one or more of five basic types of electric polarization: 1. 2. 3. 4. 5.
Electronic polarization Atomic or ionic polarization Dipolar polarization Spontaneous polarization Interface or space charge polarization.
Each type of polarization requires time to perform; this is why the degree of the overall polarization depends on the time variation of the electric field. In the present section, we consider only the polarization under static fields. In the first place, we consider a perfect dielectric material. The socalled “perfect” material implies that inside the material no mobile charge carriers (electrons or ions) are present. If a piece of such a dielectric material is put near the system shown in Figure 25, the system will tend to attract this piece of material into the vacuum space between the two plates in order to reduce the potential energy of the system. Suppose now that the piece of the material is inside the space between the metal plates with the original surface of density ss unaltered, as shown in Figure 27. This causes the potential between the plates produced by the original charge Q on the plates to decrease to a smaller value. In fact, with Q on the plates remaining constant, the ratio of the electric field in free space Fo to that filled with the dielectric material F is the socalled dielectric constant or relative static permittivity, esr = es /eo. With the dielectric material, one portion of ss is used to compensate the polarization charges on the surfaces of the material in contact with the metal plates. This portion of sb is bound at the locations with its charge opposite in polarity and equal in magnitude to the polarization charges of the material, as shown
55
The volume containing free surface charge of density ss – sb and bound surface charge of density sb, which is for compensating the polarization surface charge of the dielectric material.
P
eoF
Figure 27 The surface charge of density sS consisting of two portions: the bound charge sb and the free charge sS sb. The free charge portion produces the electric Field F and the electric flux density of eoF, while the bound charge portion produces polarization P. + and  denote the free and positive and negative charges, respectively, and denote the bound positive and negative charges, respectively.
in Figure 27. This portion of charge is termed the bound charge density sb. By denoting the number of atoms (or molecules) per unit volume of the material as N, and the average separation between charges +qd and qd of each dipole (each atom or molecule produces one dipole) as d, we can write s b = N qd d
(261)
The other portion ss  sb is the free surface charge density, which acts in exactly the same manner as that in a vacuum, creating an electric flux density Do = eoF. Thus, we can write s s = (s s  s b ) + s b = D = Do + P = e s F = e o F + (e s  e o )F
(262)
Therefore, polarization P can be expressed as p = (e s  e o )F = s b = polarization Bound charge = = N qd d Surface area Number of Induced Dipole Moments = Volume =N u
(263) where · u Ò is the average value of the dipole moment, which is given by
56 Dielectric Phenomena in Solids
u = qdd = a F loc
(264)
where a is called the polarizability and is a scalar quantity if the constituent particles (atoms or molecules) in a material are spherically symmetrical in shape and · u Ò is in the direction of F. However, if the particles (atoms or molecules) are not spherically symmetrical in shape, particularly those with permanent dipoles, then · u Ò is not exactly in the direction of F. In this case, a becomes a tensor. Throughout this book, we are interested mainly in physical concepts and, therefore, to maintain clarity and simplicity rather than to involve lengthy mathematics, we consider only homogeneous materials and electric fields that are independent of space coordinates, although they may vary with time. However, it should be noted that · u Ò depends on the local field at which the individual particle is polarized. This field Floc is different from the applied external field F; therefore, by making · u Ò proportional to F, the polarizability a must be related to the local field. From Equations 263 and 264, we can also write a=
es  eo N
(265)
We can also say that the polarizability a of a particle in a dielectric material is induced by the local field. We will see this point more clearly in Section 2.3. It is sometimes convenient to use the relative permittivity esr (i.e., the dielectric constant) to describe the dielectric properties e sr =
es Ê Na ˆ = 1+ = 1+ c Ë eo eo ¯
(266)
Na is called the electric susceptieo bility, which can also be written as where c =
P Do Bound surface charge density on the plates = Free surface charge density on the plates
c = e sr  1 =
(267) c is the electric counterpart of the magnetic susceptibility described in Magnetization in Chapter 1.
It should be noted that this discussion is limited to the phenomena under a static field. This means that the charges +Q and Q already put on the plates are constant and that the dielectric material has been inserted into the vacuum space for a time period long enough for all types of polarization to settle down to their steady state values. Now, supposing that it takes a negligibly small amount of time for the insertion of the dielectric material into the vacuum space, we can assume that at time t = 0 the material is already inside the vacuum space and starts to be polarized by the field created by the charges on the metal plates. The polarization due to the elastic displacement of electron clouds of the particles (atoms and molecules) requires a very little time, while the polarization involving the movement of the particles, such as the orientation of permanent dipoles or the migration of charge carriers (electrons or ions), requires a much longer time to perform. All types of polarization encounter some inertia counteracting the change and, therefore, involve some dielectric loss, as shown in Figure 28. In the system being considered, ss on the plates is constant, but the permittivity starts to rise from e = eo and the corresponding field to decrease from F = Fo at t = 0. It takes a very little time for e to increase to e• and for F to decrease to E• due to the polarization contributed by the elastic displacement of electron clouds of atoms or molecules (electron and atomic polarization). The time involved in this polarization is of the order of 1014 to 1013 second. We shall discuss e• further in Section 2.6. However, for the permittivity to increase from e• to its steady state value es and for the corresponding field to decrease from F• to its final value Fs, a considerably larger amount of time is required, because this change is caused by the polarization associated with the inelastic movement of particles such as the sluggish collective orientation of dipoles or the migration of charge carriers to form space charges near the electrodes or grain boundaries. Ignoring the small loss due to elastic displacement of electron clouds, the transition from P• = (e•r  1)eoF• to Ps = (esr  1)eoFs involves some
Electric Polarization and Relaxation
57
Polarization due to inelastic movement of charged particles esr –1
Fo F∞ Electric Field F
Susceptivity er – 1
er – 1
F
e∞r –1 0
Fs 0
t
ts
(a)
Polarization due to elastic displacement of electron clouds of particles
Polarization P
P
Loss
Dielectric Loss
Ps
P∞ 0
0
t
ts
(b) Figure 28 (a) The variation of the susceptivity er  1 and the electric field F with time, and (b) the polarization P = (er  1) eoF and the dielectric loss with time, where P• = (e•  1) eoF•, and PS = (eSr  1) eoFS.
energy loss, which must be consumed to overcome the inertia resistance. This energy loss is called the dielectric loss, which always accompanies timevarying electric fields. At static fields, it appears only during the transient period in which the electric field across the dielectric material is timevarying, although the charges on the metal plates are constant. This loss per unit time will become zero when the polarization has reached its final steady value e = es. The loss is proportional to the PF product; thus the loss per unit time becomes maximal when the PF product is maximal, as shown in Figure 28(b).
After the overall polarization process is completed, we shortcircuit the two metal plates. Under this shortcircuiting condition, the charges on plate A and plate B will be immediately neutralized, leaving only the polarized particles in the dielectric material to be gradually depolarized. It would take some time, depending on the environmental temperature, for all polarized particles to become completely depolarized, particularly for those whose polarization involves the orientation of permanent dipoles or the migration of charge carriers. After the shortcircuit current, due to the neutralization of the charges on the metal plates, a
58 Dielectric Phenomena in Solids
reverse depolarization current will follow, due to the depolarization of the polarized particles. The thermally activated depolarization process will be discussed in Charge Storage Involving Dipolar Charges in Chapter 5, which deals with electrets. In reality, there is no perfect dielectric material. All real dielectric materials contain, more or less, some mobile charge carriers. If such a real material has the total charge carriers n per unit volume, each carrying a charge q and having an average mobility un, then the conductivity of this material s is qunn. For a dielectric material with low conductivity, we can use an equivalent circuit, shown in Figure 29, to describe the response of this material under an electric field produced by two charged metal plates similar to that shown in Figure 27. As mentioned, the parameters e and Rd are derived directly from the polarization process. Thus, at t = 0, just after the insertion of the material into the vacuum space, e Æ e• and Rd Æ •, and at t = ts, e Æ es and Rd Æ •. The value of the resistance Rd is finite only during the period 0 < t < ts. But the leakage current through the leakage resistance Rc will continue to drain the charge from plate A to plate B, making ss decay with time. By expressing the voltage between the two plates as Fd =
ds s Rc dt ss = Q/A
Rc
C
Rd
Figure 29 The equivalent circuit of a real dielectric material. Rc = rd is the leakage resistance of the material where r is the resistivity; C = e/d is the capacitance per unit area, where e varies with time; Rd is the resistance per unit area derived directly from the polarization process and varies with time.
or ds s s s (t ) ˘ ( rd ) = ÈÍ d dt Î e s ˚˙
(268)
using the boundary condition ss (t = o) = ss (o), the solution of Equation 268 gives s s (t ) = s s (o)e  t t d
(269)
where td = res is the dielectric relaxation time and r is the resistivity of the material. td is the time required for the originally induced charge to decay to 36.7% of its original value. td can be very large for materials with a very high resistivity (i.e., low conductivity). So, it is quite dangerous to touch an electrically disconnected capacitor, because some charges may still remain on the electrodes even though the capacitor may have been deenergized for some time. For example, if es = 3eo and r = 1018W  cm, then td = 2.65 ¥ 105 seconds = 3 days. This means that it may take many days for the charges to be completely neutralized.
2.3 The Mechanisms of Electric Polarization The polarizability defined by Equation 264 implies that if · u Ò is proportional to the local field Flocal at which the particles are polarized, then ·uÒ is expressed as · u Ò = aFlocal and the polarizability a depends only on the mechanism of polarization and can be defined simply as the average dipole moment per unit field strength of the local field Flocal, which is different from the externally applied field F. But if · u Ò is expressed as · u Ò = aeffF, i.e., · u Ò is proportional to F, in this case, aeff should also be defined similarly to the effective dipole moment per unit field strength of the applied field F. However, aeff depends not only on the mechanism of polarization, but also on the factor of Floc /F. We shall consider first the mechanisms responsible for the polarizability, a, and the local field later. There are three major mechanisms of electric polarization. At moderate electric fields (i.e., at fields much lower than the inner atomic or molecular fields), and for materials with a
Electric Polarization and Relaxation
very low conductivity (i.e., the concentration of charge carriers inside the materials is so low that its effect can be neglected), these mechanisms prevail. • Electronic polarization (also called optical polarization): The electric field causes deformation or translation of the originally symmetrical distribution of the electron clouds of atoms or molecules. This is essentially the displacement of the outer electron clouds with respect to the inner positive atomic cores. • Atomic or ionic polarization: The electric field causes the atoms or ions of a polyatomic molecule to be displaced relative to each other. This is essentially the distortion of the normal lattice vibration, and this is why it is sometimes referred to as vibrational polarization. • Orientational polarization: This polarization occurs only in materials consisting of molecules or particles with a permanent dipole moment. The electric field causes the reorientation of the dipoles toward the direction of the field. Both the electronic polarization and the atomic polarization are due mainly to the elastic displacement of electron clouds and lattice vibration within the atoms or molecules. Their interaction is an intramolecular phenomenon, and the restoring force against the displacement is relatively insensitive to temperature, so electronic and atomic (or ionic) polarization processes are only slightly dependent on temperature. However, orientational polarization is a rotational process, which encounters not only the resistance due to thermal agitation, but also that due to the inertia resistance of the surrounding molecules, giving rise to mechanical friction. The rotation of a dipole in a material is like a small ball, or any body, rotating in a viscous fluid. Under an external force, it tends to change from its original equilibrium state to a new, dynamic equilibrium state, and when the force is removed, it then relaxes back to its original equilibrium state. This process is generally referred to as the relaxation process. This
59
polarization involves the inelastic movement of particles, and its interaction is an intermolecular phenomenon; hence, orientational polarizability is strongly temperaturedependent. At higher fields, carrier injection becomes important. For materials consisting of a high concentration of charge carriers (i.e., with a high conductivity), polarization due to the migration of charge carriers to form space charges at interfaces or grain boundaries becomes important. This type of polarization is called space charge polarization. Thus, the total polarizability of material a comprises four components a = ae + ai + ao + ad
(270)
where ae, ai, ao, and ad are the polarizabilities due to electronic, atomic, orientational, and space charge polarizations, respectively. For ferroelectric materials, there is also a component, called spontaneous polarization, under certain conditions. The following sections discuss the mechanisms responsible for these polarizations.
2.3.1 Electronic Polarization (Also Called Optical Polarization) There are two ways to calculate electronic polarizability: the classical approach and the quantummechanical approach. We will first discuss the classical approach. Classical Approach The polarizability ae depends on the atomic number of the atom and predominantly on the number of electrons in the outermost shell. The noble gas atoms, such as He, Ne, Ar, Kr, Xe, and Ra, whose shells are completely filled (effectively screening the nucleus from the influence of the applied fields), have the lowest polarizabilities for their atomic numbers. The Group I elements, such as H, Li, Na, K, Rb, and Cs, with only one electron in the outermost shell, have the highest polarizabilities for their atomic numbers, possibly due to the ease of polarization of a single electron in the outermost orbit.15,16 Electronic polarizability can be
60 Dielectric Phenomena in Solids
The dipole moment is given by
Floc
ue = a e Floc = Zqd = 4pe o R3 Floc
(275)
Therefore, the electronic polarizability is R
a e = 4pe o R3 = 3e oVa
d Figure 210 The displacement of the electron cloud relative to the nucleus of positive charges Zq due to the polarization by the local field Floc.
measured in monoatomic gases. Suppose that the electron cloud of charges Zq is uniformly distributed in a sphere of radius R and that its center of gravity originally coincided with that of the nucleus, and suppose that it is displaced by the field to a distance d from the center of the nucleus, as shown in Figure 210. There is a coulombic force tending to bring the electron cloud back to its original position. According to Gauss’s law, the coulombic force is only exerted on the electron cloud that does not surround the positive nucleus charges +Zq. This portion of the electron cloud is contained in the sphere of radius d and it is Qd =
Zq( 4pd 3 3) =  Zqd 3 R3 4pR3 3
(271)
Thus, the coulombic force is F =
Zq • Zqd 3 R3 = ( Zq )2 d 4pe o R3 4pe od 2
(272)
This force must balance the displacement force, which is Fd = ZqFloc
(273)
By setting Equation 272 equal to Equation 273, we obtain d = 4pe o R3 Floc Zq
(274)
(276)
where Va is the volume of the atom. ae is proportional to the volume of the atom. For the hydrogen atom, R is about 0.50 Å, ae = 1.57 ¥ 1024eo cm3. For Floc = 104 V cm1, d = 1014 cm. The displacement distance d is extremely small, only of the order of twomillionths of the radius of the atom. The susceptibility ce = N·uÒ/eoFloc = N4pR3 = 1.57 ¥ 1024N. For the ideal gas under normal conditions (0°C and 760 mm Hg), the number of particles per unit volume is 2.687 ¥ 1019 cm3, which is also known as the Loschmidt number, and xe = 1.57 ¥ 1024 ¥ 2.687 ¥ 1019 = 4.22 ¥ 105. These numerical data give us a feeling for the orders of magnitude involved in the microscopic parameters. There is another classical method that can be used for the calculation of ae, i.e., using Bohr’s model with the electrons revolving around a circular orbit instead of using a uniform electron cloud density up to radius R as just shown. This displacement of the electrons Dx, resulting from electronic polarization, always generates an elastic restoring force tending to bring the electrons back to their equilibrium position. This restoring force is proportional to the displacement Dx, resulting from the interaction of the electron with the bare nucleus and with other electrons screening the nucleus. The electron orbiting the nucleus is like a harmonic oscillation with a natural frequency wo. Thus, the motion of the electrons is governed by the following equation: m
d 2 Dx = gDx  ZqFloc dt 2
(277)
where m is the electron mass, q is the electronic charge, Z is the number electrons involved, Floc is the local field acting on the atoms, and g is the force constant. By assuming, for simplicity, that when the centroid of the negatively charged electrons is displaced by Dx from that of the positively charged nucleus, the
Electric Polarization and Relaxation
coulumbic force is the restoring force, which can be expressed as 3
2
Dx ( Zq ) Zq • Zq Ê ˆ = Dx = gDx Ë R¯ 4pe o (Dx )2 4pe o R3
(278)
and hence the electronic polarizability is ae =
g =
( Zq ) 4pe o R3
ae =
(279)
The restoring force can also be expressed in terms of the natural oscillation frequency wo by the following relation: gDx = mw o2 Dx
(280)
Thus, g wo = Ê ˆ Ë m¯
12
(281)
However, there must be some loss or damping mechanisms to limit the forced oscillation. The oscillation of an electron is equivalent to an oscillating dipole and would radiate energy according to the electromagnetic theory of radiation. Thus, radiation can be considered one of the damping mechanisms. Therefore, a term dx b , representing the retarding force, should dt be included in Equation 277. By including this term and substituting Equation 281 into Equation 277, we obtain m
d 2 Dx dx + mw o2 Dx =  b  ZqFloc dt 2 dt
(282)
where b is the damping coefficient. Damping mechanisms will be discussed further in Section 2.6. If the field is an alternating field with the frequency w expressed as Floc = Fo (loc )e  jw t
(283)
then the solution of Equation 282 gives the net displacement of the electrons by the applied field, which is Dx =
ZqFloc m(w o2  w 2 ) + jbw
(284)
The induced dipole moment is
(285)
(286)
( Zq )2 mw o2
(287)
Based on Bohr’s model of an electron revolving around a circular orbit about the nucleus, the potential energy of the electron is given by E = hw o =
mq 4 ( 4pe o )2 h 2
(288)
and the radius of the groundstate orbit of Bohr’s atom is given by R=
( 4pe o )h 2 mq 2
(289)
where h = h/2p and h is Planck’s constant. When Z = 1, by expressing the parameters m and wo in terms of R and eo, and substituting them into Equation 287, we obtain ae =
q2 = 4pe o R3 mw o2
(290)
Amazingly, Equation 290 turns out to be the same as Equation 276, although the two equations are derived on the basis of different assumptions. For the hydrogen atom, ae = 1.57 ¥ 1024eo cm3. Taking q = 1.6 ¥ 1019C and m = 9.11 ¥ 1031 kg, we have estimated the value of wo from Equation 290; it is 4.5 ¥ 1016 radians sec1. The average electronic polarizability is obtained by the summation of the contributions of all atoms divided by the number of atoms. We can consider only the contributions of the outermost electrons of each atom, and ignore the negligibly small contribution of inner electrons. From Equation 266, the electronic susceptivity is given by ce =
( Zq )2 Floc u= = a e Floc = a e(eff ) F m(w o2  w 2 ) + jbw
( Zq )2 m(w  w 2 ) + jbw 2 o
In static fields, w = o, and the static electronic polarizability becomes
In this case, the restoring force constant is 2
61
Na e N È ( Zq )2 ˘ = Í eo e o Î mw o2 ˙˚
(291)
and the relative permittivity, or dielectric constant, is
62 Dielectric Phenomena in Solids
er = 1 + ce = 1 +
N ( Zq )2 e o mw o2
(292)
the natural frequency wo should vary from atom to atom. However, for gases, the separation between atoms is large enough, and it is quite acceptable to assume that the local field Floc, at which the atom is polarized, is equal to the applied field F and that the interaction of the outermost electrons between atoms is negligibly small and can be completely ignored. So, in this case, we can assume that each atom has the same wo and hence, the same ae. Equation 292 indicates that the dielectric constant increases with the increase of the density of atoms. For a hydrogen atomic gas, N is about 2.7 ¥ 1019 atoms cm3 at the standard temperature and pressure. Thus, the dielectric constant for the hydrogen atomic gas is er = 1 + 2.7 ¥ 1019 ¥ 1.57 ¥ 1024 = 1 + 4.24 ¥ 105. N of gases is much smaller than that of solids, which is of the order of 1022 to 1023 cm3. Furthermore, in solids, the interaction of outermost electrons between atoms cannot be ignored. It should be noted that only in inert gases, such as He, A, etc., the quantum states of the outermost shell are completely filled, so the inert gases are atomic gases. In other gases, including hydrogen, oxygen, etc., the gases are formed by molecules such as H2, and O2 instead of H or O. In this case, the particles are no longer spherical in shape, but prolate ellipsoidal or spheroidal, and we shall see that geometric shape does play an important role in determining ae.
F
F
Single atoms in gases may be considered spherical in shape, but molecules, each comprising two or more atoms, are generally not spherical. In this case, the geometric shape does play an important role in determining ae. We will choose a diatomic molecule with a prolate spheroidal shape to demonstrate the calculation of the electronic polarizability of this molecule. We assume that the two atoms are identical; each has an electron polarizability ae, which is proportional to its volume, as given in Equation 276. There are two extreme possible arrangements, as shown in Figure 211(a) and (b): the molecular axis ab is parallel to the applied field (ab//F), or the axis ab is perpendicular to F (ab^F). For the case ab//F, the dipole of each atom consists of two components, one due to the applied field F and the other due to the field produced by the other polarized atom, which is in the same direction as F. Thus, we have Ê u// ˆ u// = a e Á F + 2˜ Ë 2pe o ab ¯
(293)
Rearrangement of Equation 293 gives u// =
ae 1  a e 2pe o ab
3
F = a e¢ F
(294)
where ab is the distance between the two atoms and a¢e is the effective polarizability of each atom. Thus, the electronic polarizability of this diatomic molecule is a // = 2a e¢ =
2a e 1  2( R ab)3
> 2a e
(295)
F Major Axis u// q
a
u
b
a
b
u^ F//
F^ F
(a)
(b)
(c)
Figure 211 (a) The major axis ab of a spheroidal molecule parallel to the applied field F, (b) the major axis ab of a spheroidal molecule perpendicular to F, and (c) the major axis ab of a spheroidal molecule at an angle q with respect to F.
Electric Polarization and Relaxation
In this case, a// is larger than twice the polarizability of a single atom. For the case ab^F, the dipole of each atom also consists of two components, one due to the applied field F, and the other due to the field produced by the other polarized atom, but this field is in the opposite direction to F. Thus, we have Ê u^ ˆ u^ = a e Á F 3˜ Ë 4pe o ab ¯
(296)
Rearrangement of Equation 296 gives u^ =
ae F = a e¢¢F 1 + a e 4pe o ab 3
(297)
where a≤e is the effective polarizability of each atom. Thus, the electronic polarizability is a ^ = 2a e¢¢ =
2a e 1 + ( R ab)3
< 2a e
(298)
In this case, a^ is smaller than twice the polarizability of a single atom. Obviously, a// > a^. If the molecular axis is neither parallel nor perpendicular to F, but has an angle q with respect to F, as shown in Figure 211(c), the total dipole moment is r r r u = u// + u^ r r = a // F// + a ^ F^
(299)
and the dipole moment in the direction of F is r r r uF = u// cosq + u^sin q = (a // cos 2 q + a ^sin 2 q )F
(2100)
The potential energy of a dipole induced by the field is therefore 1 W =  (a // F//2 + a ^ F^2 ) 2 1 =  (a // cos 2 q + a ^ sin 2 q )F 2 2 1 =  [a //  (a //  a ^ )sin 2 q ]F 2 2
63
in liquids or gases, they will tend to align their major axes with the applied field. It should be noted that the induced dipoles in the molecules due to electronic polarization also involve the orientation of the molecules in a manner similar to the orientation of the permanent dipoles.17 The field strength produced by the nucleus charges and experienced by the electrons is Zq/4peoR2 is larger than 109 V/cm. This field strength is far larger than the applied field. This may be the reason why the induced dipole moment for electronic polarization is proportional to the applied field and independent of frequency, because the time required for this polarization to occur is of the order of 1015 sec (wo1). This type of polarization is also called optical polarization, because it does not vary until the frequencies are in the optical range (visible region). Equations 276 and 287 are, of course, only a very rough approximation, because we have used a model that ignores the complications involving quantum mechanics. We have mentioned that in gases we can assume quite reasonably that the interaction between outermost electrons of atoms can be ignored and that the local field is equal to the applied field. However, in a condensed phase (i.e., in liquids or solids) the interaction between electrons of different atoms becomes very important. According to Pauli’s exclusion principle, there should be many values of wo, since each electron is allowed to occupy only its own state. Therefore, the electric susceptibility should be obtained by the summation of the contributions of all outermost electrons of all atoms in a piece of dielectric solid. The electric susceptibility can be written as N
(2101)
Equation 2101 indicates that when q = 0 or p, the potential energy is minimal, corresponding to the most stable position; when q = p/2, W is maximal, corresponding to the most unstable condition. If the molecules are free to rotate, as
1 Ê ( Zq )2 ˆ Ê Floc ˆ Á ˜ Ë mw o2i ¯ Ë F ¯ i =1 e o
ce = Â
(2102)
where N denotes the total number of atoms per unit volume. Furthermore, because the surrounding polarized atoms will modify the applied field, in this case each atom is polarized in the socalled local field, which is generally larger than the applied field. We shall discuss the local field in Section 2.5.
64 Dielectric Phenomena in Solids
Quantum Mechanical Approach The motion of electrons in an atom is governed by quantum mechanical rules. On the basis of the quantum mechanical approach, electron cloud density is assumed to vary from zero at the center of the atom to zero at far distance, with a peak around the Bohr radius R. The electronic polarizability, derived by van Vleck in 1932, is given by a e (w ) =
q2 Ê f10 ˆ m Ë w102  w 2 ¯
(2103)
where w10 = (E1  Eo)/ h is the proper oscillation frequency for two energy levels, Eo denotes the energy level of the ground state, E1 denotes the energy level of one of the allowed excited states, and f10 represents the strength of the oscillator associated with the coupling between the wave function in the ground state and that in the allowed excited state.18,19 Its value is of the order of unity. It is amazing that Equation 2103, based on the quantum mechanical approach, is similar to Equation 286, based on the classical approach. By setting w = 0, we have the static electronic polarizability 2
a e ( o) =
q f10 m w102
(2104)
which is again similar to Equation 287. If an atom has several excited levels, then Equation 2103 must be written in generalized form, as a e (w ) =
q2 m
Âw j πo
2 jo
f10 w2
(2105)
and
an isolated atom, may be applicable to gases because a gas may be considered an assembly of isolated atoms with negligible interaction among them. Equation 2105 is not applicable to solids, where the binding force between atoms affects the movement of valence electrons, and also the energy levels are no longer discrete but form continuous bands. However, wjo is directly related to Eg = Ec  Ev, where Ec and Ev are, respectively, the energy levels of the conduction and the valence band edges, and Eg is the forbidden energy gap. Qualitatively, we can think from Equation 2106 and would expect that the smaller the forbidden gap, the larger is the electron polarizability and hence, the static dielectric constant, as shown in the following table20,21:
Crystal
C
Si
Ge
Eg (eV) esr
5.2 5.68
1.1 12
0.7 16
It should be noted that in crystalline solids with covalent bonds, such as Si and Ge, the calculation for ae is quite involved,18.19 since the wave functions in the crystal are quite different from those in isolated atoms because of the involvement of valence electrons in the binding of atoms to form a solid. However, in ionic crystals, such as NaCl, the valence electrons are strongly localized in each ion. In this case, the electronic polarizability can be calculated simply by Â Nia ei, where Ni and aei are, i
q2 a e ( o) = m
f Â wjo2jo j πo
(2106)
where wjo = (Ej  Eo)/ h and j refers to the jth excited level. Nonpolar solids are generally elemental solids, and they consist of only one kind of atom, such as diamond (C), silicon (Si), and germanium (Ge). In these materials, there are no permanent dipoles or ions. The only polarization they have is electronic polarization. In general, Equation 2105 for ae, derived on the basis of the displacement of electron clouds in
respectively, the concentration of ith ions and the electronic polarizability of each ith ion. For example, for NaCl ionic crystal, the energy band gap Eg = 7 eV, the values of electronic polarizability21,22 for Na+ and Cl are, respectively, 0.20 ¥ 1040 and 2.65 ¥ 1040 farad m2. From Equation 266, we have calculated the relative permittivity (dielectric constant) to be about 2.28 by assuming the concentration of NaCl molecules N = 4 ¥ 1028 m3 and a = (0.20 + 2.65) ¥ 1040 farad m2. This value is very close to the experimental value of 2.25. Note that the static dielectric constant of NaCl
Electric Polarization and Relaxation
crystals is 5.62. The difference between 5.62 and 2.28 is due to the contribution of ionic polarizability, which will be discussed in the following section. Similarly, in molecular solids where the atoms or molecules are bonded by weak van der Waals forces, each particle (atom or molecule) can be considered a quasiisolated particle. In this case, the electronic polarizability of the solid can also be calculated by Â Nia ei, where Ni is the concentration of ith i
particles and aei is the electronic polarizability of each ith particle. For condensed matter (liquids or solids) made of single inert (or noble) atoms, such as He, neon, or argon, the total electronic polarizability can be simply calculated by Nae. In this case, N is just the concentration of atoms in the material.
2.3.2 Atomic or Ionic Polarization (Vibrational Polarization) A dielectric material consisting of polyatomic molecules usually has electronic polarization and ionic polarization, and in some cases, also orientational polarization when it is subjected to an electric field. In general, there are two groups of ionic solids. One group does not possess permanent dipoles, such as NaCl, which forms a simple cubic lattice so that the lattice symmetry and the overall charge neutrality ensure that electric dipoles formed by each ion pair everywhere cancel each other. The other group possesses permanent dipoles, because the crystal lattice in this case is less symmetrical, as with HCl. In fact, the internal field at the positive ion sites is generally different from that at the negative ion sites. In general, most ionic solids are asymmetrical and the electronegativities of both ions are different. They possess permanent dipoles, but these dipoles are foreseen in the solid state and cannot be aligned by an electric field. This is why in most ionic solids belonging to this group, the permanent dipole moments do not contribute to the polarizability in the solid state although the materials possess them. Quantitative analysis of the ionic polarization is quite involved.22–24 In this section, we
65
will consider only a simple case to illustrate the basic concept of atomic polarization. Suppose we have a molecule consisting of two atoms: A and B. Atom A is ready to give part of its valence electrons to atom B in order to make the outermost shells of both atoms more fully completed. This tendency is, in fact, the force that produces the socalled ionic bond. In this case, atom A is more electropositive and atom B more electronegative. NaCl is a good example, in which atom A is Na and atom B is Cl. The one electron in the outermost shell of Na is not completely given to Cl (Na gives, on average, about 78% of the electron to Cl). However, Cl receives some of the valence electron from Na and becomes a negative ion; Na becomes a positive ion. Let us consider a linear chain of ions A and ions B placed at equal distances along the x direction, as shown in Figure 212(a). In thermal equilibrium and in the absence of an electric field, the positive ions A at x2n, x2n+2, x2n2, etc., and the negative ions B at x2n+1, x2n+3, x2n1, etc., will always undergo lattice vibrations, but their interatomic distance is x2n+1  x2n = a, on average. Now if a stepfunction electric field is applied in the x direction, the electron clouds immediately shift to the left, and it takes only about 1015 sec to produce electronic polarization, as shown in Figure 212(b). In about 1013 sec after the application of the field, the positive ion at x2n and the negative ion at x2n+1 tend to attract and move toward each other, making the interatomic distance Dx1 = x2n+1  x2n < a and Dx2 = x2n  x2n1 > a. The same tendency prevails in other ions. The displacement in both the electron clouds and the ions themselves produces electronic polarization, as well as ionic polarization, as shown in Figure 212(c). Displacement of the atoms (i.e., ions) from their equilibrium sites by Dx will generate a force that tends to bring them back to their original thermal equilibrium sites. Within the approximation of harmonic oscillation, the elastic restoring force is proportional to the difference between displacements of neighboring ions. Thus, from Figure 212(c), we can write
66 Dielectric Phenomena in Solids x2n–2 a
(a)
F=0
(b)
F>0
(c)
F>0
MA +
a MB –
a MA +
a MB –
Dx1
+ZqFloc –ZqFloc
x2n
x2n–1
x2n+1 a
MA +
x2n+2 a
MB –
a MA +
MB –
Dx2 >a
Figure 212 Illustrating a linear chain of atoms A with mass MA and atoms B with mass MB placed at equal spacing a along the x direction. (a) In the absence of an electric field F = 0, (b) in the presence of an electric field F > 0, only electron clouds are shifted to the left, and (c) also in the presence of an electric field F > 0, but in this case the positive ions and the negative ions tend to move toward each other, resulting in ionic polarization, which involves both the displacement of electron clouds and the movement of ions.
the equations of motion for ions MA and MB as follows: MA
MB
d 2 x2 n = g i [( x2 n +1  x2 n )  a] dt 2  g i [( x2 n  x2 n 1 )  a] = g i [ x2 n +1 + x2 n 1  2 x2 n ]
(2107)
corresponding to the equilibrium sites, and the second term is the elastic restoring force 2 Z A ZBq 2 • Dx = g i Dx 4pe o a 3
(2110)
In general, ZA = ZB = Z. For NaCl, Z = 0.78. So the force constant is
d 2 x2 n 1 = g i [( x2 n  x2 n 1 )  a] dt 2  g i [( x2 n 1  x2 n 2 )  a] = g i [ x2 n + x2 n 2  2 x2 n 1 ]
gi =
(2108) where gi is the restoring force constant, which is different from g in Equation 279. gi can be calculated on the basis of only the electrostatic interaction between the ion and its nearest neighbors. Suppose, for simplicity, the positive and the negative ions have net charges ZAq and ZBq, respectively, and the net displacement from their equilibrium sites is Dx, then the coulombic force between the two ions is Z A ZBq 2 Z A ZBq 2 2 Z A ZBq 2 + Dx 2 4pe o ( a  Dx ) 4pe o a 2 4pe o a 3
(2109) since Dx << a. We retain only the first two terms. The first term is the force of interaction
2 Z 2q2 4pe o a 3
(2111)
Equations 2107 and 2108 are equations of phase waves and therefore have the solutions of phase wave form x2 n = x I exp[ jk(2 n)a]
(2112)
x2 n 1 = x II exp[ jk(2 n  1)a]
(2113)
where xI and xII are periodic functions of time and the exponential is a phase factor. These equations indicate that the phase of the elastic wave changes by 2ka from one ion to the nearest ion of the same kind, such as from MA at x2n2 to another MA at x2n. k is the wave number, which may be taken as 2p/l with l as the wavelength of the elastic wave. For lattice vibrations, in the visible and infrared regions, l is of the order of 3 ¥ 105 cm, which is considerably larger than the interatomic distance of
Electric Polarization and Relaxation
about 3 ¥ 108 cm. So we can say that ka is extremely small and is much smaller than unity for the frequency range associated with the lattice waves. Substituting Equations 2112 and (2113 into Equations 2107 and 2108, and bearing in mind that exp ( jka) is equal to cos ka (which can be practically considered as coska 1), we obtain d 2 xI M A 2 = 2g i ( x I  x II ) dt
(2114)
d x II = 2g i ( x II  x I ) dt 2
(2115)
Under an electric field, the equations of motion for ions should include both the elastic force and the electric force, as well as the damping or retarding force. Therefore, the above equations must be modified to MA
MB
d 2 xI = 2g i ( x I  x II ) dt 2 d( x I  x II ) b + ZqFloc dt
(2116)
d 2 x II = 2g i ( x II  x I ) dt 2 d( x II  x I ) b  ZqFloc dt
(2117)
Equation 2117 ¥ MA minus Equation 2116 ¥ MB yields Mr
d 2 Dx dDx = 2g i Dx  b  ZqFloc dt 2 dt
(2118)
where Mr = MAMB/(MA + MB) is the reduced mass and Dx = DxII  DxI is the relative displacement of positive and negative ions. Following the same principle for Equation 281, we can express gi in terms of the natural oscillation (or lattice vibration) frequency wo as 2gi = Mrw 2o. If the applied electric field is an alternating field with the frequency w, as given by Equation 283, then the solution of Equation 2118 gives Dx =
ZqFloc Mr (w o2  w 2 ) + jbw
The induced ionic dipole moment is
mi = ZqD x =
(2119)
(2120)
Thus, the ionic (or atomic) polarizability is ai =
( Zq )2 Mr (w  w 2 ) + jbw 2 o
(2121)
In static fields, w = 0 the static ionic polarizability becomes ai =
2
MB
( Zq )2 Floc Mr (w o2  w 2 ) + jbw = a i Floc = a i (eff ) F
67
( Zq )2 Mrw o2
(2122)
The expression for ai is similar to that for ae. It should be noted that the distinction between electron and ionic polarizations is not sharp, because a displacement of ions is always accomplished by a displacement of electrons. Generally, it is much easier to measure the electronic polarizability than the ionic polarizability. Usually, the electronic polarizability is determined by measuring the refractive index in the visible or ultraviolet region, and the ionic polarizability is then determined by extrapolating the refractive index spectrum to frequencies much lower than the visible region—generally, in the infrared region, in which both ae and ai are the dominant polarizabilities. The time required for electronic polarization is about 1015 sec, and that required for the ionic polarization is about 1013 sec, simply because ions are heavier than electrons by more than 103 times. This is why the resonances for these two polarizations occur in different frequency regions.
2.3.3 Orientational Polarization To begin, it may be desirable to show why some molecules possess permanent dipole moments and some do not. For a molecule with two atoms A and B, atom A gives some of its valence electrons to atom B, then atom A becomes a positive ion and atom B becomes a negative ion. This ionic bond molecule obviously possesses a permanent dipole moment, which is the product of the charge of the portion of the valence electrons transferred from atom A to atom B and the interatomic distance. If a
68 Dielectric Phenomena in Solids
great many such molecules form an ionic crystal, such as an NaCl crystal, the vector sum of all the dipole moments vanishes, because they tend to cancel each other. So, the crystal itself is not a dipolar material. For some materials, a molecule consists of three atoms in the form AB2 or A2B. For example, CO2 is in the form of AB2. In this molecule, the bonding structure is symmetrical, so the centroids of the positive and the negative charges are coincident, thus the resultant dipole moment is zero, as shown in Figure 213(a). Similarly, molecules consisting of similar atoms, such as H2, O2, and N2, carry no permanent dipole moments. However, H2O is in the form of A2B, but in this case, the bonding structure is asymmetrical, so the centroid of the negative charge is not coincident with that of the positive charge, thus resulting in a net permanent dipole moment, i.e., the vector sum of the two individual dipole moments gives a resultant dipole moment, as shown in Figure 213(b). In the presence of an electric field F, the molecules carrying a permanent dipole moment O
C
O
+8
+6
+8
up = 0 u No permanent dipole moment
u
(a) H Centroid of + charges
O
H
+8
Centroid of – charges
+1
+1
q = 105° u
u up = 2u sin(q/2) With permanent dipole moment
(b) Figure 213 The formation of dipole moments for two typical molecules: (a) molecule CO2 having no net permanent dipole moment and (b) molecule H2O having net permanent dipole moment.
will orient to align the permanent dipole moments along the direction of F. This process is referred to as orientational polarization, which occurs only in dipolar materials possessing permanent dipoles. It is obvious that orientation of a molecule involves the energy required to overcome the resistance of the surrounding molecules, so the orientation process is strongly temperature dependent. In general, nonmagnetic dielectric materials can be considered paraelectric materials, the counterpart to paramagnetic materials, in which the induced electric susceptibility c > o is always positive. There is no counterpart to diagmagnetic materials in dielectric materials, in which c should be negative. In paraelectric materials, ae and ai can be considered practically independent of temperature for the normal temperature range in most applications, because the electronic structure does not change in the normal temperature range. However, the orientational polarizability ao is strongly temperature dependent. Figure 214 shows the total polarization of some vapors as a function of temperature. The data are from the references.25–28 It can be seen that C2H2 and molecules with a similar symmetrical and linear structure, such as CH4, CCl4, and CO2, do not possess permanent dipole moments and therefore are not dipolar. Those with an asymmetrical structure are dipolar, such as H2O, in which two OH bonds make an angle of 105°, resulting in the formation of a permanent dipole moment. This is why the total polarization in which the orientational polarization is dominant decreases with increasing temperature, as shown in Figure 214. It should be noted that for gases at normal temperature and pressure, susceptibility is of the order of 104 to 103. The difference in susceptibility reflects the difference in the number of atoms per unit volume. However, for solids, susceptibility is generally much higher than unity. Molecules having a permanent dipole moment experience a torque in an electric field, tending to orient themselves to the field direction, but thermal agitation tends to put them back into random orientation. However, the ensemble of molecules will gradually attain a
Electric Polarization and Relaxation F
F +
F
69
+
–
–
8
q
+
–
CH3Cl
(er – 1) ¥ 103
(a)
(b)
(c)
6 Figure 215 The orientation of a dipole: (a) stable position, (b) unstable position, and (c) orienting to the field direction.
CH2Cl2 4 CHCl3 CCl4
F
2 CH4 0 2.5
3.0
r
dq
3.5
1/T (K –1) ¥ 103
x q
Figure 214 The susceptibility (er  1) as a function of temperature for some polar and nonpolar gases at the normal pressure of 1 atmosphere.
statistical quasiequilibrium. The method of calculating orientational polarizability was first developed for permanent magnetic moments in paramagnetic materials by Langevin29 and later applied to permanent dipole moments in dielectric materials by Debye.30,31 Supposing that the permanent dipole moment uo of the molecule is not affected by the applied electric field and temperature, and that the density of molecules in the gas medium as an ensemble is so small that the dipole–dipole interaction is very small compared to the thermal equilibrium energy kT; the moment of the permanent dipole in the direction of the applied field F, as shown in Figure 215, can be written as uF = uo cosq
(2123)
where q is the angle between the dipole moment and the applied field, and < > represents the statistical ensemble average. At zero applied field, the number of dipoles having an inclination of their axes to the axes
Figure 216 The calculation of the number of dipoles having the inclination of their axes to the xaxis between q and q + dq.
located between q and q + d q, as shown in Figure 216, is dN = N
2pr sin qrdq 1 = N sin qdq 4pr 2 2
(2124)
With an applied field F and the effect of temperature, Equation 2124 is changed to the following form, according to Boltzmann’s statistics, 1 dN = A exp( U kT ) sin qdq 2
(2125)
where U is the potential energy of the dipole at q, which is given by U = uo F cosq
(2126)
Thus, the average dipole moment in the field direction is
70 Dielectric Phenomena in Solids
uF =
Úu
o
L( z ) = cosq = 1  1 z
cosqdN
Ú dN
= uo
Ú
p o
exp(uo F cosq kT )cosq sin qdq
Ú
p o
exp(uo F cosq kT )sin qdq
= uo cosq
(2127)
However, as F/T increases, the dipole of the molecule becomes more parallel to the applied field. In practical and most cases, uoF/kT << 1. Thus, substitution of Equation 2131 into Equation 2123 gives uF =
By introducing y = cosq
(2128)
z = uo F kT
(2129)
we obtain +1
cosq =
Ú Ú
exp( yz )ydy
1 +1 1
(2130)
exp( yz )dy
= cothz  1 z = L( z )
The function L(z) is called the Langevin function, which is shown in Figure 217 as a function of z = uoF/kT. At low values of z, L(z) varies almost linearly, with z following the relation (2131)
L( z ) = cosq = uo F 3kT
For example, a dipole moment uo = 108 qC cm at a field of 106 V/cm and a temperature of 300 K gives uoF/kT 0.4, which is smaller than 1. There is no possibility for < cos q > to reach unity at room temperature. Only at very low temperatures may it approach unity at high fields. For z << 1, Equation 2131 is reasonably accurate, and for z >> 1, L(z) can be estimated by
L(z)
1 z /3
0
1
2
3
4 5 z = uoF/kT
Figure 217 The Langevin function.
6
7
(2132)
uo2 F 3kT
(2133)
and the orientational polarizability is ao =
uo2 3kT
(2134)
In general, orientational polarizability is much larger than electronic and atomic polarizabilities at normal conditions, since ae and ai are practically independent of temperature (i.e., their temperature dependence at normal conditions is not significant) but ao is strongly temperature dependent. Thus, ao can be easily distinguished from ae and ai by the temperature dependence measurement of er. There are two factors that have not been taken into account in the derivation of ao. One is the effect of electron spins, which cause spin paramagnetism and may affect the results. To take this effect into account, the quantum mechanical approach must be used. The other factor is that the permanent dipole moment uo for multiatomic molecules is not independent of temperature because in this case, the permanent dipole moment is the result of several moments, and their internal orientation is dependent on their individual activation energies and hence on the temperature. In solids, the dipoles do not rotate freely as do dipoles in liquids or gases. The rotation of dipoles in solids is constrained to a few discrete orientations, which are influenced by the crystalline field determined by the interaction of the dipole with neighboring ones. Thus, to describe the dielectric constant in terms of the dipole moments uo of individual dipoles (molecules), it is necessary to know the crystal structure of the material in the solid state. The potential energy of a dipole in a crystalline solid depends on the direction of the dipole relative to the crystal axes. In other
Electric Polarization and Relaxation Solid
71
Liquid
40
Solid
Liquid
20 30
16
er er 12
20
Melting point
8 10 4 m.p. 0
0 270
280
290 T (K )
300
(a)
80
To
120
160 T (K )
200 Tm
(b)
Figure 218 Variation of dielectric constant (measured at low frequency 5 kHz) with temperature for (a) nitrobenzene (C6H5CO3), and (b) hydrogen sulfide (H2S).
words, the potential energy is directly related to the crystalline field acting on the dipole and is therefore temperature dependent. In some solids, dipoles at temperatures below the melting point are frozen, and their rotation is inhibited even under an electric field. In such solids, the contribution of ao to the total polarization is zero, ie., ao = 0, as in nitrobenzene (C6H5CO3), shown in Figure 218(a). The dielectric constant decreases abruptly from the value of 35 (in liquid state) to a value of about 3 (in solid state) at 278 K, the melting point of this material. For T < 278 K, only ae and ai contribute to er. For T > 278 K, the material is in the liquid state; ae, ai, and ao all contribute to er, and er decreases with increasing temperature following Equation 2134. However, in some other solids, the dielectric constant is still increasing with decreasing temperature at temperatures below the melting point, i.e., in the solid state. This rise in dielectric constant continues until a critical temperature To, at and below which the dipoles become frozen. H2S is a typical example of this kind of material. Figure 218(b) shows that, for temperatures between the melting point Tm (188K) and the critical temperature To (103 K), the dielectric
constant of H2S in the solid state increases with decreasing temperature, but at To = 103 K, er drops abruptly from about 20 to about 3, indicating that the dipoles at To are frozen and become immobile, resulting in ao Æ 0. The experimental results are from Smyth and Hitchcock.32,33 To explain why H2S and some other materials, such as HCl, still have the temperature dependence of ao in the solid state within a certain range of temperatures between Tm and To, we can assume that the average potential energy of a dipole due to shortrange interaction, which creates the crystalline field, has a profile similar to that shown in Figure 219. The bottom of the potential wells represents the equilibrium state of the dipoles in which the potential energy of the dipoles reaches the minimum value. In the absence of an electric field, a dipole has the same probability of orienting to the right or to the left, so there is no net polarization. But when the material is present in an electric field, the well at q = 0 is lowered by an amount of uoF, and that, at q = p, is deepened by the same amount of uoF, as shown by the dashed line in Figure 219. The direction of the dipoles orienting to the right
72 Dielectric Phenomena in Solids
The term exp(2uoF/kT) can be expanded into a series because uoF << kT. This leads to
F
2uo F 1 Ê 2uo F ˆ + kT 2 Ë kT ¯ 3 1 2uo F ˆ  Ê + ... Ë ¯ 3! kT
2
exp( 2uo F kT ) = 1 
uoF uoF
0
p 2
By keeping only the first two terms, we obtain u o ( parallel to F ) =
p
2uo2 F kT
(2139)
This leads to the polarizability Figure 219 Schematic diagram showing the potential energy of a dipole as a function of the orientation angle q in the solid state. Solid curve—in the absence of an electric field and dashed curvein the presence of an electric field.
corresponds to the orientation of the dipoles toward the direction of the applied field, and that to the left corresponds to the orientation of the dipoles opposite to the field. Denoting the probability of the dipoles at q = p orienting to the left as w, then 1  w is the probability of the dipoles at q = 0 orienting to the right, and according to the Boltzmann statistics, we can write w = exp[ 2uo F kT ] 1 w
(2135)
This leads to w=
exp( 2uo F kT ) 1 + exp( 2uo F kT )
(2136)
In general, uoF is much smaller than kT under most practical conditions. For uoF << kT, Equation 2136 can be simplified to w=
1 exp[ 2uo F kT ] 2
(2137)
Based on this model, the percentage of a dipole moment uo in the direction opposite to the applied field is w, than the percentage of the dipole moment in the direction parallel to the field is 1  w. Thus, we can write u o ( parallel to F ) = uo (1  w )  uo ( w ) = uo (1  2 w ) = uo [1  exp( 2uo F kT )]
(2138)
ao =
u 2uo2 = F kT
(2140)
which is in the same form as that of Equation 2134 derived on the assumption that the dipoles rotate freely in the material. However, the difference between these two equations explains that at T = Tm, ao in the solid state is larger than in the liquid state, as shown in Figure 218(b). The transition from one form of the solid state at To < T < Tm to the form at T < To can be considered the transition from a disordered state to an ordered state. At T = 0, all dipoles are in a completely ordered state. That at T = 0, ao = 0 implies that the number of dipoles pointing in one direction is equal to that pointing in the opposite direction, so the net polarization vanishes. As the temperature increases, the number of dipoles in the ordered state will tend to move to the disordered state. Considering that the dipoles have their lowest potential energy in the completely ordered state, there exists a potential difference U(T) between two equilibrium states, as shown in Figure 220(a). It can be imagined that the probability for a dipole having its direction at q = 0, termed the right direction, is w, then a lower probability (zero at T = 0) for the dipole having its direction at q = p, termed the wrong direction, is 1  w, as shown in Figure 220(a). Similarly, another dipole may behave oppositely; its direction at q = 0 is the wrong direction, and that at q = p is the right direction,28,34,25 as shown in Figure 220(a). We can use the same approach for the polarization at To < T < Tm; the probability for a dipole in the wrong direction
Electric Polarization and Relaxation
is 1  w, which is governed by the following relation: w = exp[ U(T ) kT ] 1 w
(2141)
Hence, we have w=
exp[ U(T ) kT ] 1 + exp[ U(T ) kT ]
(2142)
The calculation of U(T) is very involved, even by means of approximation methods.28,36 We shall not give details about the calculation here.
A qualitative picture of U(T) as a function of T, as shown in Figure 220(b), is sufficient to explain the temperature dependence of er at T < To. Since U(T) >> kT, the energy of the dipole due to the applied field uoF is negligibly small compared to U(T); therefore, the field F does not affect the order–disorder transition for T £ To. According to Equation 2142 and Figure 220(c), w is very small for T £ To and becomes 1/2 at T = To, at which U(T) = 0, as shown in Figure 220(b). This means that w = 1/2 for T ≥ To, implying that the probability for the dipoles pointing to the right or to the left is
U (T )
0
73
U (T )
p 2
p
0
p 2
p
(a)
W U (T ) 1 2
To
(b)
T
To
(c)
Figure 220 (a) Potential energy profiles of two different types of dipoles in the lattice, (b) U(T) as a function of temperature, and (c) the probability W as a function of temperature.
74 Dielectric Phenomena in Solids
equal. Under this situation, the applied field will start to play an important role in causing polarization, as discussed earlier for T between To and Tm. 2.3.4 Spontaneous Polarization Electronic polarization is always present in atoms or molecules in all kinds of materials; ionic polarization is present only in materials made of two or more different kinds of atoms that form ions due to the sharing of the valence electrons of one or more atoms with the others. For both electronic and ionic polarizations, the dipole moments are induced by electric fields, so they are classified as induced dipole moments. In short, both electronic and ionic polarizations are due to the translation (or deformation) of the valence electron clouds from their original thermal equilibrium state to a new equilibrium state. These types of polarization are only slightly dependent on temperature because they are intramolecular phenomena. However, orientational polarization occurs only in the materials composed of molecules with an asymmetrical structure in which the centroid of the negative charge (mainly electrons) and that of the positive charge (mainly nuclei) are not coincident, so they possess permanent dipole moments in the absence of external fields. The directions of these permanent dipole moments are randomly distributed in the material. An electric field will cause them to reorient toward the direction of the field, resulting in orientational polarization. The net polarization will return to zero after the removal of the external field because thermal agitation tends to randomize the alignment. This is why polarization decreases with increasing temperature. However, there is another kind of polarization, called spontaneous polarization. By analogy to magnetization, electric polarization can be grouped into two major polarizations: • Paraelectric polarization, which includes mainly electronic, ionic, and orientational polarizations, with c always positive • Ferroelectric polarization, with c very large, similar to ferromagetization
There is no counterpart to diamagnetization in dielectric materials, with c in negative values. Spontaneous polarization occurs in materials whose crystalline structure exhibits electrical order. This implies that spontaneous polarization occurs only in single crystals or crystallites in polycrystalline materials with a noncentrosymmetic structure, because only in a noncentrosymmetic structure does the centroid of the negative charges not coincide with that of the positive charges. In ferroelectric materials, electric polarization occurs spontaneously due to a phase transition at a critical temperature called the Curie temperature, Tc, without the help of an external electric field. At and below Tc, the crystal undergoes a phase transition, usually from a nonpolar cubic structure to a polar structure. BaTiO3 is a typical example of a ferroelectric crystal. At T > Tc, the BaTiO3 crystal assumes a cubic structure in which the centroid of the negative charges and that of the positive charges coincide, so the molecule does not form a dipole moment. However, at T £ Tc, the cubic structure is slightly distorted, resulting in a slight displacement of Ba2+ and Ti4+ ions. This displacement, though very small (only about 0.15Å), is enough to cause the centroid of the negative charges to be different from that of the positive charges, thus forming an electric dipole moment. Each unit cell carries a reversible electric dipole moment spontaneously oriented parallel to the dipole moment of neighboring cells. This chainreaction process is referred to as spontaneous polarization. The buildup of such dipole moments pointing along one crystal axis will gradually form a domain and will gradually increase the free energy of the system. This process cannot continue; the domain will stop growing when it has reached a certain size, and another domain with dipole moments pointing in the opposite direction will be formed in order to reduce the free energy of the system. In a single crystal or a crystallite, there are many domains with moments pointing in various directions. But the vector sum of the dipole moments of all domains vanishes. Each domain can be considered as a large dipole. Under an external
Electric Polarization and Relaxation
electric field, all of these randomly arranged domains tend to move toward the direction of the field, resulting in a net total spontaneous polarization. Upon the removal of the field, spontaneous polarization does not vanish but remains inside the material. The fieldpolarization relation forms a hysteresis loop similar to the hysteresis loop for ferromagnetic materials. This topic will be discussed in more detail in Ferroelectric Phenomena in Chapter 4.
75
F
EA
EB DEo DE
2.3.5 Space Charge Polarization The induced, orientational, and spontaneous polarizations discussed previously are due to the bound positive and negative charges within the atom or the molecule itself, which are linked intimately to each other and which normally cannot be separated. However, electric polarization may also be associated with mobile and trapped charges. This polarization is generally referred to as space charge polarization, Pd. This occurs mainly in amorphous or polycrystalline solids or in materials consisting of traps. Charge carriers (electrons, holes, or ions), which may be injected from electrical contacts, may be trapped in the bulk or at the interfaces, or may be impeded to be discharged or replaced at the electrical contacts. In this case, space charges will be formed, field distribution will be distorted, and hence, the average dielectric constant will be affected. In the following sections, we shall consider two possible ways in which space charge polarization may result. Hopping Polarization In a dielectric material, localized charges (ions and vacancies, or electrons and holes) can hop from one site to the neighboring site, creating socalled hopping polarization.16 These charges are capable of moving freely from one site to another site for a short time, then becoming trapped in localized states and spending most of their time there. Occasionally, these charges make a jump surmounting a potential barrier to other sites. In fact, the movement of ions or vacancies in ionic crystals and the movement of electrons and holes in glasses and amorphous
r A
B
Figure 221 A double potential well illustrating hopping polarization due to the hopping of the charged particle over the barrier from one well to the other.
semiconductors are essentially due to the hopping process.37 Depending on the width and the height of the potential barrier, a charged particle on one site may hop or tunnel to the other site. A simple, doublewell potential barrier is shown in Figure 221. In thermal equilibrium, the timeaveraged probability for a charged particle (for example, a negatively charged particle) to hop from site A to site B, leaving a positive charge in site A and creating a negative charge in site B to form a dipole, is Po ( AÆB) = C exp(  EA kT )
(2143)
where C is a constant and EA is the activation energy for the hopping transition. Similarly, the probability for the charged particle to hop in the reverse direction from site B to site A is Po ( BÆA) = C expÊ Ë
 EA  DEo ˆ ¯ kT
(2144)
where DEo is the difference between EA and EB, which is positive when EA > EB, zero when EA = EB, or negative when EA < EB. An applied field changes the potential barrier profile, making the hopping of the particle from site B to site A much easier than from site A to site B (for the case shown in Figure 221). Thus, the probabilities under an applied field become
76 Dielectric Phenomena in Solids
P( AÆB) = C exp[ ( EA + aDE ¢) kT ]
(2145)
If qrF/kT << 1, p¢ can be approximated to p¢ po ( AÆB) po ( BÆA) ( qrF cosq kT )
and
the random hopping dipole moment is
P( BÆA) = C exp{[ EA  (1  a)DE ¢] kT }
(2146) where DE¢ = DE  DEo is the potential barrier height difference created by the applied field F, a(DE¢) is the increase in potential barrier height in site A, and (1  a)DE¢ is the decrease in potential barrier height in site B. Obviously, the magnitude of DE¢ depends on the direction of the vector r (the axis joining site A and site B) relative to F. Therefore, DE¢ can be written as DE ¢ = DE  DEo = qFr cosq
(2147)
This implies that DE¢ = qFr when q = 0, i.e., the vector r is in the field direction; DE¢ = 0 when q = p/2, i.e., the vector r is perpendicular to the field direction. In this case, the applied field does not modify the original potential barrier height. In terms of probabilities, we can write p( AÆB) = po ( AÆB)  p¢
(2148)
p( BÆA) = po ( BÆA) + p¢
(2149)
and
The hopping dipole moment may be considered similar phenomenally to the orientational dipole moment, but in nature, they are different. The orientational dipole moment refers to the permanent dipole moment formed by bound charges within the particle, while the hopping dipole moment is the moment formed by the transition of a separate charged particle from one potential well to another potential well. Following the same concept in treating the orientation of permanent dipoles (Equation 2123), the hopping dipole moment in the direction of the applied field can be written as
(2151) Assuming that the particle must be located either in site A or in site B, then po ( AÆB) + po ( BÆA) = p( AÆB) + p( BÆA) = 1
(2152) From Equations 2148 and 2152, we obtain p¢ = po ( AÆB) po ( BÆA) 1  exp( qrF cosq kT ) Ï ¸ ¥Ì ˝ Ó 1  po ( BÆA) [exp( qrF cosq kT )  1] ˛
(2153)
(2156)
uhF = uh p¢ cosq
where the factor p¢ means that it is the fieldinduced excess probability p¢ that produces the hopping polarization. Using Equation 2127, we have p¢ cosq =
Ú p¢ cosqdN Ú dN p Ú p p
o
o ( AÆB ) o ( BÆA )
( qrF cosq kT )
1 ¥ (cosq ) N sin qdq 2 = p 1 Úo 2 N sin qdq qrF ˆ = po ( AÆB) po ( BÆA) Ê Ë 3kT ¯
(2150)
p( BÆA) = exp(DE kT ) = exp[(DEo + DE ¢) kT ] p( AÆB)
(2155)
uh = qr
The applied field causes a decrease in hopping probability from site A to site B by an amount p¢ and an increase in hopping probability from site B to site A by p¢. From Equations 2143 and 2147 we have po ( BÆA) = exp(DEo kT ) po ( AÆB)
(2154)
(2157) Substitution of Equation 2157 into Equation 2156 gives uhF =
q2r 2 F po ( AÆB) po ( BÆA) 3kT
(2158)
Thus, the hopping polarizability is ah =
q2r 2 po ( AÆB) po ( BÆA) 3kT
(2159)
where po ( AÆB) po ( BÆA) denotes the ensemble average of the product of these two probabilities, because EA and EB may vary from site to site.
Electric Polarization and Relaxation
Interfacial Polarization The space charge, or interfacial polarization, is produced by the separation of mobile positively and negatively charged particles under an applied field, which form positive and negative space charges in the bulk of the material or at the interfaces between different materials. These space charges, in turn, modify the field distribution. Suppose that we have a composite dielectric specimen comprising two parallel sheets of different materials, and that this dielectric specimen is inserted into the space between two parallel metallic plates of unit area, as shown in Figure 222. In this case, under AC fields the admittance is Y=
Y1Y2 Y1 + Y2
(2160)
t = (e1r d2 + e 2 r d1 )e 0 (s 1d2 + s 2 d1 )
(2161)
Y2 = (s 2 + jwe 2 re 0 ) d2
(2162)
where e1r and e2r are the dielectric constants, s1 and s2 are the conductivities, and d1 and d2 are the thicknesses of sheets 1 and 2, respectively. Substitution of Equations 2161 and 2162 into Equation 2160 gives 2 È Ê 1  w t 1t 2 ˆ Ê wt 1 + wt 2 ˆ ˘ Í Á + w 2 t 1t ˜ + j Á + w 3t 1t 2 t ˜ ˙ ˜ ˜ Á ÍÁ 2 Ë  wt ¯ ˙ s 1s 2 ˙ Í Ë + w t 2t ¯ Y= ˙ s 1 d2 + s 2 d1 Í 1 + w 2t 2 ˙ Í ˙ Í ˚ Î
(2163)
where t 1 = e1re o s 1
(2164)
t 2 = e 2 re 0 s 2
(2165)
(2166)
Y can also be written as Y = s d + jwe re 0 d
(2167)
By comparing Equation 2167 with Equation 2163, we obtain the overall dielectric constant and conductivity of this composite dielectric as follows: er =
1 Ê s 1s 2 d ˆ t 1 + t 2 + w 2t 1t 2t  t e 0 Ë s 1d2 + s 2 d1 ¯ 1 + w 2t 2
(2168) s 1s 2 d ˆ 1  w 2t 1t 2 + w 2t 1t + w 2t 2t s =Ê Ë s 1d2 + s 2 d1 ¯ 1 + w 2t 2
(2169) Under static DC fields, w = 0. Thus, the static overall dielectric constant and conductivity are
in which Y1 = (s 1 + jwe1re 0 ) d1
77
s 1s 2 d ˆ Ê t 1 + t 2  t ˆ e rs = Ê Ë s 1d2 + s 2 d1 ¯ Ë ¯ e0
(2170)
and ss =
s 1s 2 d s 1d2 + s 2 d1
(2171)
At high frequencies, the space charges cannot follow the change of the field and hence do not produce space charge polarization. By setting w Æ •, we obtain e r• =
e1re 2 r d e1r d2 + e 2 r d1
s • = s s (t 1t 2 + t 1t + t 2t ) t 2
(2172) (2173)
We can consider er• to be mainly the contribution of electronic and atomic polarizations. Thus, the total polarization is P = (e rs  1)e o F = NaF
(2174)
and the polarization due to electronic, atomic, and orientational contributions is P¢ = (e r • + e ro  1)e o F = N(a • + a o )F
~
d
s1, e1
d1
s1/d1
e1r eo /d1
(2175)
s2, e2
d2
s2/d2
e2r eo /d2
Therefore, P  P¢ is the polarization due to the space charge contribution. Thus,
Figure 222 A composite dielectric material between two parallel metal plates of unit area.
Pc = P  P¢ = (e rs  e r •  e ro )e o F = N(a  a •  a o )F
(2176)
78 Dielectric Phenomena in Solids
and the space charge polarizability is a c = a  a •  a o = (e rs  e r •  e ro )e o N
(2177) where N is the number of molecules per unit volume of the composite dielectric. It should be noted that if this composite dielectric also involves hopping polarization, then the space charge polarizability ad = ah + ac is the combination of both the hopping and the interfacial polarizabilities. Since these two types of polarization involve the movement of charged particles, there is no easy experimental method to separate these two different mechanisms.
2.4 Classification of Dielectric Materials Dielectric materials may be classified into two major categories: nonferroelectric (or normal dielectric or paraelectric) materials and ferroelectric materials. The former may be divided into three classes, as the following sections show. 2.4.1 Nonferroelectric Materials (Normal Dielectric or Paraelectric Materials) In materials of this category, electric polarization is actuated by external electric fields. Based on the mechanisms of electric polarization, we have three classes: nonpolar, polar, and dipolar materials. Nonpolar Materials In materials of this class, an electric field can cause only elastic displacement of electron clouds (mainly valence electron clouds), so they have only electronic polarization. Such materials, which are generally referred to as elemental materials, consist of a single kind of atom, such as silicon (Si), diamonds (C), inert elements in gas, liquid, or solid phase. For these materials, the appreciable absorption occurs at the resonance frequency wo, which is in the visibletoultraviolet region. For frequencies lower than the resonance frequency, the
dielectric constant should be independent of frequency and equal to the static dielectric constant. According to Maxwell’s relation, the refractive index of such materials can be written as n = (e rs )1 2
(2178)
The total polarizability is a = ae
(2179)
Polar Materials In materials of this class, an electric field will cause elastic displacement of the valence electron clouds, as well as elastic displacement of the relative positions of ions, so such materials have both electronic and ionic polarization. The material may be composed of molecules, and each of the molecules is made of more than one kind of atom without permanent dipole moments. Examples of such materials are ionic crystals, including alkali halides, some oxides, paraffins, benzene, carbon tetrachloride, etc. The appreciable absorption occurs at two resonant frequencies: one in the optical frequency region (corresponding to electronic polarization) and the other in the lower resonance frequency—(the infrared region corresponding to ionic polarization). In this case, the total polarizability is a = ae + ai
(2180)
Dipolar Materials The materials of this class have all three fundamental polarizations: electronic, ionic, and orientational. Thus, the total polarizability is a = ae + ai + ao
(2181)
Materials whose molecules possess a permanent dipole moment belong to this class. An electric field will cause spatial orientation of the permanent dipoles, resulting in orientational polarization. The orientation process occurs predominantly in liquids and gases, and in some solids within a certain range of temperatures, such as solid hydrochloric and sulfuric acids. However, in the solid state, there exists
Electric Polarization and Relaxation
a critical temperature at and below which all dipoles are frozen in and lose their capability to contribute orientational polarizability. But for most materials, the dipoles are frozen in below the melting point of the material. It should be noted that dielectric materials, in general, are not single crystals; they are either amorphous or polycrystalline, containing a large quantity of various traps. Furthermore, they are not nonconductive and always involve charge carriers (electrons, holes, or both) injected from electrical contacts. Therefore, in this case, the total polarizability should include the space charge polarizability a = ae + ai + ao + ad
(2182)
where ad in the space charge polarizability includes ah + ac. 2.4.2 Ferroelectric Materials A ferroelectric material is normally in single crystalline or polycrystalline form and possesses a reversible spontaneous polarization over a certain temperature range. There is a critical temperature, called the Curie temperature, which marks the transition from the ordered to the disordered phase. At this temperature, the dielectric constant may reach values three to four orders of magnitude higher than in the disordered phase. The order–disorder phase transition involves the displacement of atoms so that crystals or crystallites exhibiting ferroelectric phenomena must be noncentrosymmetric. This implies that a phase transition will induce a mechanical strain, tending to change not only the volume and the shape of the material body, but also the optical refractive index. Thus, ferroelectric materials exhibit not only ferroelectric phenomena, but also piezoelectric, pyroelectric, and electrooptic effects, which can be used for many technological applications. In general, ferroelectric materials also have electrically induced polarizations, but these are negligibly small compared to spontaneous polarization. For most practical cases dealing with ferroelectric phenomena, electrically induced polarization can be ignored. More details about the properties and applications of
79
ferroelectric materials are given in Ferroelectric Phenomena in Chapter 4.
2.5
Internal Fields
Only in gases or in dilute phases, in which the interaction between atoms or molecules can be neglected, the internal or local field, Floc, acting on the atomic or molecular sites, can be assumed to be the same as the applied field F. However, the local field in condensed phases (solids and liquids) is higher than F because of the polarization of the surrounding particles. In this section, we shall briefly discuss local fields for nondipolar and dipolar materials. Local Fields for Nondipolar Materials To understand the concept of local fields, imagine a small sphere of dielectric material removed from around the site of the atom or molecule to form a cavity, as shown in Figure 223. The local field Floc is composed of four components Floc = F0 + F1 + F2 + F3
(2183)
where F0 is the externally applied field in the cavity, which is assumed to be a vacuum, acting on A and is related to the applied field in the bulk F by D = e 0 F + P = e 0 F0
(2184)
or F0 = F + P e 0
F1 is the depolarization field resulting from polarization charges (bound charges) on the surface of the specimen, which is given by F1 =  P e 0
(2185)
In fact, F0 + F1 is equal to the applied field F. F2 is the Lorentz field due to polarization charges on the inside surface of the spherical cavity,6,27 which is given by F2 =
(e r  1) F 3
(2186)
F3 is the field of the adjacent dipoles due to the molecules inside the spherical cavity. In
80 Dielectric Phenomena in Solids +
+
+
+
+
+
+ Dipole
F
dA + + dA + q q P P A
dF2 =
dF2 – – –
F2 =
dF – 2 –
–
–
–
–
–
–
–
u
Pcosq dA 4peor 2 Pcos2qdA 4peor 2 p
=
– +
P cos2q 2pr 2sinqdq 4peor 2
= P/3eo = (er – 1)F/3
Figure 223 The model for the calculation of the Lorentz field.
general, we assume that the cavity is ideally formed without disturbing the state of polarization of the surrounding material and that the fields contributed by all dipoles inside the cavity tend to compensate each other. This assumption leads to (2187)
F3 = 0
Thus, the local field can be written as Floc = F0 + F1 + F2 + F3 =
er + 2 F 3
(2188)
The ClausiusMossotti Equation From Equations 263, 264, and 2188, we obtain e r  1 Na = e r + 2 3e 0
(2189)
This is the well known ClausiusMossotti equation. The number of atoms or molecules per unit volume N is related to the number of atoms or molecules per mole (Avogadro’s number N0) by N0 =
NM = 6.023 ¥ 10 23 per mole r
rial. Substitution of Equation 2190 into Equation 2189 gives the molar polarization in terms of polarization per mole e r  1 M N0a = er + 2 r 3e 0
(2191)
This is the Clausius–Mossotti equation expressed in terms of M and r. Using either Equation 2189 or Equation 2191, a can be determined because all other parameters are generally known or can easily be measured. It should be noted that the Clausius–Mossotti equation can be used only for nonpolar materials because F3 cannot be assumed to be zero for polar materials, which will be discussed in later Na sections. It should also be noted that when 3e 0 approaches unity, er approaches infinity, and when r is larger than a certain critical value, er tends to be negative. This phenomenon is generally called the Clausius–Mossotti catastrophe, indicating that Equations 2189 and 2191 are reasonable only for a low a, a low r, and nondipolar materials.
(2190)
where M and r are, respectively, the atomic or molecular weight and the density of the mate
The Lorentz–Lorenz Equation The Clausius–Mossotti equation can be used for dipolar materials in highfrequency AC
Electric Polarization and Relaxation
fields in which orientational polarization cannot follow the timevarying fields but electronic and atomic polarizations are still present. For optical frequencies, only electronic polarization is dominant, and in this case er = n2, where n is the refractive index. In the optical frequency range, Equations 2189 and 2191 can be rewritten as n 2  1 Na = n 2 + 2 3e 0
(2192)
n 2  1 M N0a = n2 + 2 r 3e 0
(2193)
These equations are sometimes called the Lorentz–Lorenz equation because they were first derived independently by H.A. Lorentz in Holland and L. Lorenz in Denmark in 1880.27 At high frequencies, which are so high that no orientational polarization can occur but still low enough to include both the electronic and atomic polarizations, er is termed er•. In this case, er•  n2 is the contribution of atomic polarization. We can also estimate the orientational contribution. The electronic and atomic polarizability can be estimated from e r•  1 N(a e + a i ) = e r• + 2 3e 0
(e rs  e r • ) Na o = (e rs + 2)(e r • + 2) 9e 0
cavity of radius a, it produces a field that polarizes the cavity’s surrounding molecules. The reaction field Fr is the field created inside the cavity by the charges of these polarized molecules on the cavity surface. Thus, in the absence of the applied field F = 0, the effective dipole moment of a dipolar molecule in a condensed dipolar material is
where u0 is the permanent dipole moment of an individual molecule and a is the total polarizability of the material. The permanent dipole moment and Fr are in the same direction. This reaction field is given by Fr =
2.5.2 The Reaction Field for Dipolar Materials In Section 2.5.1, we derived an expression for the local field based on the assumption that there is no contribution to the field from the molecules inside the spherical cavity. If a dipolar molecule is located at the center of the
2ueff Ê e r  1 ˆ = fueff 4pe 0 a 3 Ë 2e r + 1¯
(2197)
where f=
1 Ê er  1 ˆ 2 N Ê er  1 ˆ = 2pe 0 a 3 Ë 2e r + 1¯ 3e 0 Ë 2e r + 1¯
(2198) 3
1 6
since N = (4pa /3) . Then, from Equations 2196 and 2197, we obtain ueff =
u0 1a f
(2199)
With an applied field F, the field inside the empty spherical cavity is given by Fi =
3e r F = hF 2e r + 1
(2200)
3e r 2e r + 1
(2201)
where h=
(2195)
where ers denotes the static dielectric constant.
(2196)
ueff = u0 + aFr
(2194)
The total polarizability can be obtained by measuring er under static DC fields. Thus, subtracting Equation 2194 from Equation 2189 gives the polarizability contributed by orientational polarization if both the hopping and the space charge polarizations are absent. This gives
81
Thus, the effective induced dipole moment of a dipolar molecule inside the cavity due to the cavity field Fi and the reaction field Fr in the direction of the applied field F, as shown in Figure 224, becomes ¢ = a( F i + fueff ¢ ) ueff
or ¢ = ueff
ah F 1a f
(2202)
82 Dielectric Phenomena in Solids F=0
F
F ueff
Fr ueff
q
Fi
uo
¢ ueff
¢ ueff and ueff
Fi = hF
Fr = fueff = fuo /(1 – a f )
Figure 224 Schematic diagrams illustrating the concept of the reaction field Fr, the cavity internal field Fi, the effective dipole moment of a polar molecule ueff, and the effective induced dipole moment of a polar molecule u¢eff in a condensed polar material.
The total dipole moment in the cavity is the sum of the permanent dipole moment and the induced dipole moment in the direction of F uF
¢ uF = ueff cosq + ueff Polarized by the reaction field at F=0
Polarized by the cavity field at applied field F
(2203) To obtain the mean value of uF, we use the Boltzmann statistics with a weight factor W (q ) ˘ exp ÈÍ, in which W(q) is the activation Î kT ˙˚ energy for the rotation of a dipole toward the field direction and is given by W (q ) = u eff • F = 
hueff F cosq kT
(2204)
Since only ueff must rotate but not u¢eff, which is already in parallel to F, we have
uF =
Ú (ueff cosq + ueff¢ ) ¥ exp( hueff F cosq kT )dW Ú exp(hu
eff
F cosq kT )dW
ÈÊ u0 ˆ
(2205)
where dW = 2p sin qdq is the solid angle corresponding to dq. Following the same approach for L(z) (Equation 2127) and substituting Equations 2199 and 2202 into Equation 2205, we obtain
ah
˘
Ú ÍÎË 1  af ¯ cosq + 1  af F ˙˚ ÈÊ hu0 ˆ ˘ F cosq kT ˙2p sin qdq ¥ exp Í ÎË 1  af ¯ ˚ = ÈÊ hu0 ˆ ˘ Ú exp ÍÎË 1  af ¯ F cosq kT ˙˚2p sin qdq h È u02 ˘ F a+ = Í 1  af Î 3(1  af )kT ˙˚
(2206) The Debye Equation Assuming that ah = ac = 0 (or ad = 0) and expressing the total polarizability as a = ae + ai +
uo2 3kT
(2207)
substitution of Equation 2207 into Equation 2189 gives er  1 N Ê uo2 ˆ = ae + ai + e r + 2 3e o Ë 3kT ¯
(2208)
This is called the Debye equation. The molar polarization can be expressed in a form similar to Equation 2191 e r  1 ˆ M No Ê uo2 ˆ p =Ê = ae + ai + Ë e r + 2 ¯ r 3e o Ë 3kT ¯
(2209) In fact, the Debye equation is similar to the Clausius–Mossotti equation; the only differ
Electric Polarization and Relaxation
ence is that the former introduces ao = u2o/3kT into the equation. Both equations were derived on the basis of the internal local field rather than the reaction field. The Debye equation is in poor agreement with experiments for dipolar liquids and solids, possibly due in part to the fact that for dipolar liquids and solids, the Lorentz internal field is not applicable. The Onsager equation improves on the Debye equation by using the reaction field instead of the Lorentz internal field. Theoretically, the molar polarization deduced from the Debye equation should be a constant at a fixed temperature and independent of pressure. This means that Equation 2191 should have the same value for the material whether in the gaseous phase or in the liquid phase. Experimentally, this is not true for dipolar liquids. However, for gases in which er  1 << 1, the Debye equation gives a reasonably accurate prediction. Based on the Debye equation, (ae + ai) and uo can be determined by measuring er at different temperatures. Furthermore, the Debye equation gives reasonable results for diluted solutions of dipolar molecules in nondipolar solvents. In general, dipolar materials can be classified into three groups based on the permanent dipole moments of their molecules: • Weakly dipolar materials in which uo < 0.5 debye • Medium dipolar materials in which 0.5 debye < uo < 1.5 debye • Strongly dipolar materials in which uo > 1.5 debye The Onsager Equation In the static DC or lowfrequency fields, we have 3e rs 2e rs + 1 2 N Ê e rs  1 ˆ f Æ fs = 3e 0 Ë 2e rs + 1¯
h Æ hs =
(2210)
On the basis of the definition of the polarization, we obtain P = (e rs  1)e 0 F = N uF
(2211)
83
At zero and low frequencies, all types of polarization are taking place, so a = ae + aa + ao (hopping and space charge polarizations are assumed to be absent). However, in the highfrequency fields, in which orientational polarization does not occur, uo = 0. Then we have 3e r • 2e r • + 1 2 N Ê er•  1 ˆ f Æ f• = 3e 0 Ë 2e r • + 1¯
h Æ h• =
(2212)
The polarization becomes P• = (e r •  1)e 0 F = N uF•
(2213)
Hence, we obtain e r•  1 N(a e + a i ) = e r• + 2 3e 0
(2214)
This equation is, in fact, the same as the ClausiusMossotti equation. By subtracting Equation 2213 from Equation 2211, we obtain (e rs  e r • )(2e rs + e r • ) Nu02 = 2 e rs (e r • + 2) 9e o kT
(2215)
This is the well known Onsager equation.38 This equation enables the computation of uo of a dipolar molecule from ers of a pure dipolar liquid or solution, if its density and er• are known. The Onsager equation was first derived on the assumption that the molecules are spherical in shape and that there are no interactions between the molecules (or between the dipoles). However, uo of nonassociating organic compounds (with weak interactions between molecules) agrees reasonably with those computed from Onsager equation. For associating organic compounds (with strong interactions between molecules), the difference between the measured and the computed values of uo is large, indicating that Onsager’s model is inadequate for associating organic compounds.39 This is mainly due to the following reasons: • The model assumes that the surrounding medium of any molecule is a continuum. This means that it does not take into account the interactions between the molecule and its neighbors. In other words, only long
84 Dielectric Phenomena in Solids
range interaction is considered; shortrange interaction energy has been neglected. • The model does not take into consideration the electrostatic interaction between nearest dipoles. • The model does not take into account the nonpolar molecular interactions, which may be significant in some liquids and solids. Several investigators6,24,28 have attempted to modify the Onsager equation by using an ellipsoid instead of a spheroid in the shape of the cavity, and also by taking into account the anisotropy of the polarizabilities of the molecules. However, their modified models do not improve much. The improvement must take into account the intermolecular interactions, and to this end, we must use the statistical–mechanical approach. Statistical–Mechanical Approaches and the Kirkwood Equation Both Debye and Onsager used a statistical method to solve only part of the polarization problem by considering the whole dielectric medium as a continuum where there is no correlation between molecules (molecular interactions) in deformational (or induced) polarization and in orientational polarization. Statistical–mechanical approaches to the polarization problem, taking into account the interaction between nearest dipoles, were first used by Kirkwood.40 He developed a general method of solving the problem that had some influence on all the subsequent polarization theories. Kirkwood had taken into account the shortrange correlation in orientational polarization, but he ignored the correlation in deformational polarization between molecules. In Kirkwood’s final equation, the terms due to deformational polarization were added empirically. Later, Frohlich28 developed a more rigorous expression, taking into account the correlation between molecules in both orientational and deformational polarizations by means of a statistical–mechanical approach. The equations derived by these and other investigators include a correlation factor g, which is related to the effects of molecular interactions. When g = 1, no correlation between molecules is taken
into account. This is true only for systems of nonassociating molecules. Therefore, the Clausius–Mossotti, Debye, and Onsager equations can apply only to systems of nonassociating molecules and, as a result, they are not satisfactory for condensed systems, such as polymeric materials. Kirkwood40 developed his theory of static polarization by taking into account the shortrange interaction between molecules in the liquid state. The Kirkwood equation is (e rs  1)(2e rs + 1) N Ê guo2 ˆ = ae + ai + 9e rs 9e o Ë 3kT ¯
(2216) where g is the correlation factor. The correlation factor is a measure of the local ordering in the material. g = 1 indicates that the average dipole moment of a finite spherical region around one reference molecule, which is held fixed in an infinite size of the material specimen, is about equal to the moment of the fixed molecule. This implies that the location of one dipole does not influence the positions of the other dipoles. If a fixed dipole tends to make the neighboring dipoles line up in a parallel direction, then the effective moment is larger than uo and hence g > 1. Conversely, if the fixing dipole tends to line up with the neighboring dipoles in an antiparallel direction, then g < 1.34 If the reference molecule (the fixing dipole) is surrounded by z neighboring molecules and cos F is the average of cos F made between the reference molecule and one of its z nearest neighbors, then g may be expressed as39,40 g = 1 + z cosf
(2217)
The correlation factor is supposed to characterize the molecular interaction and the shortrange structure. Up to the present, no good method is available for determining the value of g accurately. In general, it is roughly estimated from the measured value of the dielectric constant or the dipole moment. This is one of the major shortcomings of the Kirkwood equation. Furthermore, Kirkwood used the approximate formula for the internal field, which also makes Kirkwood’s equation inaccurate.
Electric Polarization and Relaxation
The Frohlich Equation In the model of Frohlich,28 both the shortrange interaction between molecules and the deformational polarization are taken into account. Frohlich also considered a spherical region within an infinite, homogeneous dielectric continuum of static dielectric constant ers. This region contains dipoles whose behavior is governed by statistical–mechanical laws. Frohlich also treated the internal and reaction fields in a macroscopic manner, which is more realistic than the Onsager model. The general Frohlich equation is (e rs  e r • )(2e rs + e r • ) Ngu 2 = e rs (e r • + 2)2 9e o kT
(2218)
where Nv
g = 1 + Â cosfij
(2219)
j
j π1
Nv is the number of the dipoles within the spherical region of volume V, and thus, N = Nv /V is the number of dipoles per unit volume, and cosf oj is the average of cos Fij made between the reference molecule i and the jth nearest neighbor. Equation 2218 becomes identical with the Onsager equation (Equation 2215) when g = 1. However, the definition of u in the Frohlich equation differs from that in the Onsager equation.28 If ers >> er•, the Kirkwood equation and the Frohlich equation do not differ significantly. In polymeric liquids or solids, the polymer chains are entangled. The appropriate way to deal with such molecules is to choose a small, repeating unit of a chain as a basic dipole unit; each of these basic units contributes equally to the average polarization of a macroscopic sphere of the dielectric in an applied field. Based on this consideration, the Frohlich equation can be used for polymers, provided that g is replaced by x
x
g¢ = 1 + Â cos fij¢ + Â cos fik¢¢ j
(2220)
k
j π1
where cos f ij¢¢ is the average of cos f≤ij made between the reference unit i and the jth unit
85
within the same polymer chain, and cos f ik¢¢ is the average of cos f≤ij made between the reference unit i and a kth unit in the polymer chains that do not contain the reference unit i.39 It is also assumed that the polymer chain contains x repeating dipole units and the polymer has a high molecular weight, so the contribution to the overall polarization made by the end groups can be neglected. In contrast to Frohlich’s approach, Harris and Adler41 considered a macroscopic sphere immersed not in an infinite macroscopic dielectric continuum but in a vacuum, in order to simplify the evaluation of the energy of the interaction between the specimen and the field. Their results predicted dielectric constants larger by a factor roughly equal to (2e rs + 1)(e r • + 2) . However, because of many 3(2e rs + e r • ) shortcomings to their approach, several investigators42–46 have proposed different approaches in order to correct them. Buckingham45 has pointed out that the Onsager relation between ueff and uo is a sufficiently good approximation for many polar liquids. By taking into account the discrete nature of the particles surrounding the reference molecule and the shortrange interactions, Buckingham, in his derivation for the dielectric constants, arrived at the same expression as the Frohlich equation (Equation 2218). As mentioned earlier, the statistical theories of polarization may enable the determination of the effective dipole moment and the correlation factor, which characterize the molecular interactions. It has been shown that the value of the effective dipole moment in polymers depends on the internal rotation in polymer chains, which is greatly hindered due to the presence of strong molecular interactions.47 A study of the dielectric polarization of polymers certainly will provide useful information about molecular interaction in polymers. As regards polymers, it is not possible to eliminate the interaction between polar groups belonging to the same chain; even polymers are dissolved in a nonpolar solvent with an infinite dilution. In alcohol, g is large (g > 3 for butyl alcohol at 0°C) because of the high degree of correlation between the alcohol molecules due to the
86 Dielectric Phenomena in Solids
existence of hydrogen bonds, which leads to the parallel orientation of dipole moments. Replacing the OH radical with a halogen in butyl alcohol leads to a big change in g. For example, g = 0.76 for butyl bromide and g = 0.85 for butyl chloride at 0°C. The value of g < 1 indicates that the correlation in orientation makes the dipole moments antiparallel and cancel one another. The study of g as a function of temperature and pressure in polar substances, and as a function of the concentration in polar solution, is important to understanding molecular interactions with respect to structural changes.
2.6 Electric Polarization and Relaxation in TimeVarying Electric Fields Atoms, molecules, and ions are so small that even a macroscopically tiny region in a solid contains very large numbers of such particles. The discrete nature of matter, and the behavior and interaction of those particles, can be manifested through their response to timevarying electric fields with wavelengths comparable to the distances between particles (interparticle distances). In condensed matter—solids and liquids—the interparticle distances are of the order of a few angstroms; electric fields with wavelengths of this order would be in the region of xrays, which have energies capable of ionizing the particles. In this section, we will deal with the dynamic response of the dielectric material involving electric fields with wavelengths much larger than the interparticle distances, so the dielectric material can be treated as a continuum. 2.6.1 The TimeDomain Approach and the FrequencyDomain Approach In the previous section, we discussed the static response of dielectric materials under static electric fields with w = 0. However, the dynamic response under timevarying electric fields provides much more information about the structure of the material and its dielectric behavior for fundamental studies, as well as for technological applications. To measure the
dynamic response, we can use either the timedomain approach or the frequencydomain approach. These two approaches are equally powerful methods for studying dielectric phenomena. From the viewpoint of measuring techniques, the timedomain approach is simpler than the frequencydomain approach, but from the viewpoint of data analyses, the timedomain approach is more complex. In the timedomain approach, we measure the timedependent polarization immediately after the application of a stepfunction electric field, or we measure the decay of the polarization from an initial steady state value to zero after the sudden removal of an initial polarizing field. This decay is generally referred to as dielectric relaxation. In the frequencydomain approach, we mainly measure the dielectric constants at various frequencies of alternating excitation fields. Both approaches should be intimately connected and should yield, in principle, the same results. 2.6.2 Complex Permittivity When a timevarying electric field is applied across a parallelplate capacitor with the plate area of one unit and a separation of d between the plates, then the total current is given by JT = J +
dD dF = J + e* dt dt
(2221)
where J is the conduction current and e* is defined as the complex permittivity, which is introduced to allow for dielectric losses due to the friction accompanying polarization and orientation of electric dipoles. This may be written as e * = e  je ¢ = (e r  je r¢ )e o
(2222)
in which er is called the dielectric constant and e¢r the loss factor. An arbitrary timevarying field can be resolved into sinusoidal AC fields of a spectrum of frequencies by means of the Fourier transformation. For simplicity, we consider the applied field to be monochromatic and a sinusoidal function of angular frequency w, which can be expressed as F = Fm exp( jwt )
(2223)
Electric Polarization and Relaxation
Substitution of Equations 2222 and 2223 into Equation 2216 yields JT = sF + jw (e  je ¢)F = (s + we ¢)F + jwe F
(2224) where s is the electric conductivity of the material. The first term on the right is a loss component due to the inelastic scattering of conducting charge carriers with scatterers during their migration, which is present at all frequencies, including w = 0 (DC fields); the second term is also a loss component due to the friction in the polarization processes, which disappears when w = 0 and increases with w; and the third term is a lossless component which is, in fact, the displacement current. For dielectric polymers, s is normally extremely small, and in most cases the contribution of the first term can be neglected. By ignoring the first term, the tan d is given by (2225)
tand = e r¢ e r
which is generally called the loss tangent, as shown in Figure 225. If e¢r /er << 1 then tand = e r¢ e r d
(2226)
This is generally called the loss angle. The instantaneous energy absorbed per second per cm3 by the material is given by JT (t)F(t). Thus, on average, the amount of energy per cm3 per second absorbed by the material is W=
1 2p
2p
Ú J (t )F(t )d(wt ) T
(2227)
0
87
2.6.3 TimeDependent Electric Polarization In general, the time required for electronic and atomic polarization and depolarization is very short (<1012 sec). This deformational polarization process is also referred to as the resonance process because it involves vibrating modes. Resonance of a vibrating system occurs when an excitation field oscillates at a frequency close to the natural frequency of the system. The time required for orientational, hopping, or space charge polarization and depolarization is quite long and varies in a wide range, depending on the dielectric systems; such polarization processes are sometimes referred to as relaxation processes because they involve a relaxation time. A relaxation phenomenon occurs when restoring action tends to bring the excited system back to its original equilibrium state. Ignoring, for simplicity, hopping and space charge polarization, the total polarization of an arbitrary dielectric system is (2228)
P = Pe + Pi + Po
Since the response time for electronic and atomic polarization is so short and can be assumed to be practically constant for all frequencies from 0 to about 1012 Hz, we can group these two polarizations as P• = Pe + Pi = (er•  1)eoF. These two types of polarization can be considered to follow instantaneously the excitation field F without time lag; in other words, P• and F can be considered to be in phase. Thus, we can write P = P• + Po = (e r •  1)e o F + (e rs  e r • )e o F
(2229)
2 r 0 m
= we ¢e F 2
JT
weF JT jwe
we ¢
s
d
sF
we ¢F
Figure 225 The response of a parallel plate capacitor with the plate area of one unit and its equivalent circuit under an alternating electric field.
88 Dielectric Phenomena in Solids
It is Po that has a time lag with F; therefore, there is a phase difference between Po and F. Supposing that the orientational polarization takes time to respond to the applied excitation field F, and that at the removal of the excitation field making F = 0 at t = 0, the polarization will decay at a rate proportional to its change from its equilibrium state (as shown in Figure 226), then we can write dPo (t ) Po (t ) =dt to
(2230)
where to is the macroscopic relaxation time. Using the boundary condition that at t = 0, Po = (ers  er•)eoF, the solution of Equation 2230 is Po (t ) = (e rs  e r • )e o F exp( t t o )
(2226)
So, dPo(t)/dt gives the depolarization rate for this case, in which the excitation field is a stepfunction, F = constant up to t = 0. Similarly, if a stepfunction excitation field F is applied to the dielectric system at t = 0, then Po(t) = 0 at t = 0, and Po(t) increases with time. Following the same method, we obtain
Po (t ) = (e rs  e ra )e o F[1  exp( t t o )] (2232)
In this case, dPo(t)/dt gives the polarization rate. The approximate time required for polarization is shown in Figure 227. Supposing that during the time interval between u and u + du, an excitation field F(u) is applied to the dielectric system, and that F = 0 for t < u and t > u + du (as shown in Figure 228), then Po(t) will take time to respond and will change for t > u. As soon as Po(t) reaches the value of Po(u + du) at u = t + du, the polarization will decay gradually. During the polarization period u < t < u + du, the change of the polarization can be written as dPo (t  u) t  uˆ˘ = (e rs  e r • )e o ÈÍ1  expÊ dF(u) Ë t o ¯ ˙˚ Î
(2233) in which 1  exp[(t  u)/to] is a response function. The total P consists of two parts: P•, which can follow the excitation field immediately, and Po(t), which is governed by Equation 2233. Thus, we can write
F
0
t
0
t
Polarization
Depolarization
P• + Po P• P Po(t )
Po(t )
P•
0
t
0
t
Figure 226 Time dependence of polarization and depolarization under a stepfunction electric field F.
+
89
Space Charge Polarization
Hopping Polarization
Orientational Polarization
Atomic Polarization
Electronic Polarization
Polarization P
Electric Polarization and Relaxation
+ + + +
+ – + +
– + – + –
+ – – –
–
+
10–15
10–10
10–5 Time (second)
1
105
Figure 227 The variation of different types of polarization with time under a stepfunction electric field F.
dP(t  u) = dP• (t  u) + dPo (t  u) = (e r •  1)e o dF(u) + (e rs  e r • ) t  uˆ˘ ¥ e o ÈÍ1  expÊ dF(u) Ë t o ¯ ˚˙ Î
(2234) According to the superposition principle, the total polarization at time t is a superposition of all increments dP, so we have
Case A If F is a stepfunction electric field with F = 0 at t = 0 and F = F at t = 0+, then from Equation 2236 we have P = (e r •  1)e o F + (e rs  e r • )e o F[1  exp( t t o )]
(2237)
The variation of P with time t is shown in Figure 226.
P = (e r •  1)e o F(t ) t t  uˆ˘ + (e rs  e r • )e o Ú ÈÍ1  expÊ dF(u) 0Î Ë t o ¯ ˙˚
(2235) Integrating by part, we obtain
F = Fm cos wt = Re[ Fm exp( jwt )]
P = (e r •  1)e o F(t ) + (e rs  e r • )e o Ú
Case B If F is a sinusoidal AC field with
F(u) exp[ (t  u) t o ]du 0 t o t
(2236) where exp[(t  u)/to] is a decay function that tends to approach zero at t Æ •. In the following cases, we shall discuss two general cases.
(2238)
where Re refers to the real part of Fm exp( jwt), P• can follow the field immediately, but Po has a time lag, i.e., Po has a phase shift. To analyze this case, we must assume that P has reached its dynamic steady state at t = 0, so that the bottom limit of the integral in Equation 2236 must be changed to •, where P = 0. From Equation 2236 we obtain
90 Dielectric Phenomena in Solids
F (t )
F (u)
u
P (t )
u + du
Po
t
P• Po (t )
P•
u
u + du
t
Figure 228 The time response of P(t) to a delta function electric field F(u) of strength F(u) within the time period of u £ t £ u + du.
t
È ˘ Fm Re Í Ú exp( jwt )exp[ (t  u ) t o ]du ˙ to Î• ˚ È exp( jwt ) ˘ = (e r •  1)e o Fm cos wt + (e rs  e r • )e o Fm Re Í Î 1  jwt o ˙˚ (e rs  e r • )e o Fm cos wt (e rs  e r • )wt o e o Fm sin wt + = (e r •  1)e o Fm cos wt + 1 + w 2 t o2 1 + w 2 t o2 In plase with the Lag by p 2 from the applied field applied field
P = (e r •  1)e o Fm cos wt + (e rs  e r • )e o
The component in phase with the applied field is the lossless component, while the component with p/2 out of phase with the applied field is the loss component. It is obvious that for
(2239)
w >> 1/to the dipoles cannot follow the field variation; hence, the polarization gradually decreases to zero as w increases. The loss component, in fact, represents the dielectric losses
Electric Polarization and Relaxation
P
91
long time that D has been settled to be a periodic function of time, we can write
P• + P1
D  e r•e o Fm cos wt
P1 P1/2
[Ú G( x)coswt coswxdx + Ú G( x )sin wt sin wxdx ] •
= (e rs  e r • )e o Fm
P2
0
•
P•
0
w = 1/to
0
(2243)
w
Figure 229 The variation of P•, P1, and P2 with frequency.
in the form of energy absorption. This term is maximum at wo = 1/to and decreases gradually as w increases or decreases from the point wo = 1/to. Using P•, P1, and P2 to denote the three components, Equation 2234 can be written as P = ( P• + P1 )cos wt + P2 sin wt
2.6.4 Kramers–Kronig Relations Equation 2231 can be used to derive the relations between the dielectric constant er(w) and the loss factor e¢r(w). These relations are known as the Kramers–Kronig relations.48,49 By writing the decay function in a more generalized 1 form G(t  u) to replace exp[ (t  u) t o ], to Equation 2231 can be written as P = (e r •  1)e o F(t ) t
(2241)
0
Since D = Do + P = eoF(t) + P, we have t
D = e r•e o F(t ) + (e rs  e r • )e o Ú F(u)G(t  u)du 0
D = Re[e r*e o F ] = Re[(e r  je r¢ )e o Fm exp( jwt )] = e o Fm [e r cos wt + e r¢ sin wt ]
(2244) Comparing Equation 2243 with Equation 2244, it follows that •
(2240)
These components as functions of frequency are shown in Figure 229. The variation of the dielectric parameters, such as P and e*, with frequency is known as the dispersion of the dielectric material, and it is one of the most important properties of all materials.
+ Ú (e rs  e r • )e o F(u)G(t  u)du
By expressing the AC field in the form of Equation 2238, D can be considered to be the real part of the product e*F. Thus,
(2242)
By introducing a new variable x = t  u and assuming that the material has been subjected to the AC field F(t) = Fm cos wt for a sufficiently
(e r  e r • ) = (e rs  e r • )Ú G( x )cos wxdx 0
•
e r¢ = (e rs  e r • )Ú G( x )sin wxdx
(2245) (2246)
0
These two equations indicate that the real and imaginary parts of complex permittivity depend on the same decay function G(x). According to the Fourier theorem, G(x) can be expressed in the following form: G( x ) =
2 p
Ú
0
G( x ) =
2 p
Ú
0
•
e r (u)  e r• cos uxdx e rs  e r•
(2247)
e r¢(u) sin uxdx e rs  e r•
(2248)
or •
These two equations must be equal, so er must be related to e¢r. Substituting Equation 2248 into Equation 2245, we obtain 2 p 2 = p 2 = p
e r (w)  e r • =
Ú [Ú •
•
0
0
•
Ú
0
Ú
0
•
]
e r¢(u)sin uxdu cos wxdx
[sin ux cos wxdx ]e r¢(u)du e ¢(u)u du u2  w 2
(2249) Similarly, substitution of Equation 2247 into Equation 2246 yields
92 Dielectric Phenomena in Solids
e r¢(w ) =
2 p
Ú
• 0
[e r (u)  e r • ]
w du (2250) u2  w 2
Equations 2249 and 2250 are called the Kramers–Kronig relations. These relations are very useful under certain situations because they enable the determination of the value of one parameter (er or e¢r) from the other parameter (e¢r or er) at any frequency. This is particularly important when, for some reason, one of the parameters cannot be measured. These relations are valid for any type of polarization, and from them a complete spectrum of er and e¢r over a wide range of frequencies can be obtained—provided that one of the parameters (er or e¢r) can be measured throughout the same frequency range. If we set w = 0 for the case of DC fields, Equation 2249 becomes 2 p 2 = p
e rs  e r• =
Ú Ú
• 0 • 0
e r¢(u)
du 2 = u p
Ú
• 0
e i (w )
dw w
By expressing Fm cos wt = Fm exp ( jwt), Fm sin wt can be expressed as Fm sin wt = Fm exp[ j(wt  p 2)] =  jFm exp( jwt )
and Equation 2239 can be rewritten as (e rs  e r • ) ˘ P = ÈÍe r •  1 + e o Fm exp( jwt ) 1 + w 2t o2 ˙˚ Î (e rs  e r • )wt o ˘  j ÈÍ e o Fm exp( jwt ) Î 1 + w 2t o2 ˙˚
(2253) From Equations 268 and 2222, P can also be expressed as P = (e r*  1)e o F = [(e r  1)  je r¢ ]e o Fm exp( jwt )
e r* = e r  je r¢ = e r• +
e ¢(w )d( lnw )
•
e ¢(w )d( lnw ) =
p (e rs  e r • ) 2
(2251)
This implies that the total area under the curve of e¢r vs nw is simply related to ers  er•, the extreme values of the dielectric constants, and is independent of their dispersion mechanisms. We shall return to this interesting feature in the Section 2.7, which deals with the distribution of relaxation times. 2.6.5 Debye Equations, Absorption, and Dispersion for Dynamic Polarizations Strictly speaking, no material is free of dielectric losses, and therefore, no material is free of absorption and dispersion. This implies that there is no material having frequencyindependent er and e¢r. In fact, the dispersion in er and e¢r is an intrinsic property of all dielectric materials, and all other properties have to coexist with it. In this section, we shall first show the derivation of the Debye equations and then discuss the absorption and dispersion phenomena.
e r¢ =
e rs  e r• 1 + jwt o
(2255)
e rs + e r• 1 + w 2t o2
(2256)
(e rs  e r • )wt o 1 + w 2t o2
(2257)
e r = e r• +
0
(2254)
By comparing Equation 2253 with Equation 2254, we have
or
Ú
(2252)
and tan d =
e r¢ (e rs  e r • )wt o = er e rs + e r•w 2t o2
(2258)
Equations 2255 through 2257 are generally called the Debye equations for dynamic polarization with only one relaxation time to.31,50,51 These equations are based on the assumption that the decay function is exponential. Similar to the situation for static polarization, Debye equations are satisfactory only for the condition ers  er• < 1, which can be fulfilled only in dilute solutions because the derivation of Equations 2255 through 2257 has not taken into account the interaction between particles. er and e¢r are temperature dependent through the temperature dependence of (ers er•) and to. We can easily find the frequency at which e¢r de r¢ and tan d are maximal by setting = 0 and dw
Electric Polarization and Relaxation
93
d(tan d ) = 0. The maximum value of e¢r occurs dw at wo when
eliminating wto from these two equations, we obtain
(2259)
(2267)
w ot o = 1
At this frequency, er, e¢r and tan d are given by er
w =w o
e rs + e r• = 2
¢ e r¢ w =w o = e (max) = tand
w =w o
=
(2260)
e rs  e r• 2
(2261)
e rs  e r• e rs + e r•
(2262)
However, the value of tan d at wo is not maximal. The maximum value of tan d occurs at wd when w d t o = (e rs e r • )1 2 > 1
(2263)
At this frequency, tan d is given by tan d
w =w d
= tan d (max) =
e rs  e r• 2(e rse r • )1 2
(2264)
The values of er, e¢r, and tan d as functions of w are shown in Figure 230. Equations 2256 and 2257 can be written as e r  e r• 1 = e rs  e r• 1 + w 2t o2
(2265)
e r¢ wt o = e rs  e r• 1 + w 2t o2
(2266)
These two equations are the parametric equations of a circle in the er  e¢r plane. By
2
Ê e  e rs + e r• ˆ + e ¢ 2 = Ê e rs  e r• ˆ r Ë Ë r 2 ¯ 2 ¯
2
Of course, only the semicircle of Equation 2267, over which e¢r is positive, as shown in Figure 231, has physical significance. The major disadvantage of this method for finding er or e¢r is that the frequency, which is the independent variable and is the parameter most accurately measured, is not explicitly shown in the Argand diagram. It should also be noted that the derivation of Equations 2255 through 2257 is based on the following assumptions for simplicity: The local field is the same as the applied field F; the conductivity of the materials is negligible; and all dipoles have only one identical relaxation time to. The effects of these assumptions on er and e¢r will be discussed later in this section. Debye equations emerge directly from the Kramers–Kronig relations. They show explicitly the frequency dependence of er and e¢r. The type of dispersion shown in Figure 230 is generally considered the normal dispersion. All types of polarization may be grouped into two major regimes: the resonance regime and the relaxation regime. Polarizations associated with vibrations of electrons (i.e., electronic or optical polarization) or with vibrations of atoms or ions (i.e., atomic or ionic polarization) belong to the resonance regime because in the e¢r
ers er
e¢r (max) = (ers – er•)/2
(ers + er•)/2
w = wo = 1/to w
er e¢r tand
(ers – er•)/2 e¢r
e•
w
tand w
w = 1/to
wd = (ers /er•)
1/2
(to
)–1
Figure 230 er, e¢r and tan d as functions of w for cases with negligible contribution of s due to carrier migration.
• er
(e rs
–
(ers + er•)/2
)/2 e r•
w=0 ers
er
Figure 231 Argand diagram of er  e¢r relation for cases with only one relaxation time to.
94 Dielectric Phenomena in Solids
polarization a resonance will occur when the frequency of the excitation field is close to the natural frequency of the vibration or oscillation system. Polarizations involving the movements of charges either by orientation (i.e., orientational polarization) or through the migration of charge carriers (i.e., hopping or space charge polarization) belong to the relaxation regime because during the polarization or depolarization processes, a relaxation phenomenon occurs due to the time required for the charge carriers to overcome the inertia arising from the surrounding medium in order to proceed in their movement. The variation of er and e¢r with frequency shown in Figure 230 illustrates schematically the typical dispersion behavior for polarizations in the relaxation regime. However, in the resonance regime, the optical constants, i.e., the complex refractive index n*, which consists of the refractive index n and the extinction coefficient (or called the absorption index) k, can be expressed in terms of the complex dielectric constant as n* = n  jk = (e r*)1 2 = (e r  je r¢ )1 2
valid in dilute gases. In Section 2.5, we discussed the internal field or the Lorentz field (Equation 2188). By taking into account the local field based on the Lorentz field, Equations 2255 through 2258 and other equations are still valid if to is replaced with t¢o, which is given by17 t o¢ =
e r = n2  k 2
(2269)
e r¢ = 2 nk
(2270)
The frequency dependence of er and e¢r in the optical frequency range, i.e., f > 1011 Hz, and the dispersion of er and e¢r (or n and k) are anomalous. So this type of dispersion is sometimes referred to as anomalous dispersion. Figure 332 in Chapter 3 shows schematically this anomalous dispersion phenomenon, and Figure 333 shows the variation of er and e¢r with frequency for various types of polarization in both the resonance and the relaxation regimes. For more details, see Absorption and Dispersion in Chapter 3.
(2271)
In general, the measured relaxation time based on the Cole–Cole plot is higher than the real relaxation time, possibly due to the local field effect. Note that the local field given by Equation 2193 is not applicable to condensed polar polymer materials, as explained in Section 2.5.2. The Effects of DC Conductivity If the DC conductivity s is not negligibly small, then s will contribute to the imaginary part of complex permittivity. The total complex permittivity becomes
(2268)
Rearrangement of Equation 2268 leads to
e rs + 2 to e r• + 2
s s ˆ˘ e * = e  j Ê e ¢ + ˆ = ÈÍe r  j Ê e r¢ + eo Ë Ë w¯ Î we o ¯ ˚˙
or e r* = e r  je r¢  j
s w
(2272)
Taking the DC conductivity into account, the Debye equation (Equation 2255), for example, becomes e r*  e r• =
e rs  e r• s j 1 + jwt o we o
(2273)
and Equations 2257 and 2258 become e r¢ =
s (e rs  e r • )wt o + we o 1 + w 2t o2
tan d =
(2274)
we o (e rs  e r • )wt o + (1 + w 2t o2 )s we o (e rs + e r •w 2t o2 )
(2275) The Effects of the Local Field So far in Section 2.6, all equations derived are based on the assumption that the local field is the same as the applied field. This, of course, is
When wto << 1, Equations 2274 and 2275 reduce to e r¢ =
s we o
(2276)
Electric Polarization and Relaxation
tand =
s we oe rs
(2277)
When wto ª 1, Equations 2274 and 2275 reduce to e r¢ =
(2278)
e o (e rs  e r • ) + 2st o e o (e rs + e r • )
(2279)
When wto >> 1, Equations 2274 and 2275 reduce to e rs  e r• ˆ e r¢ = Ê Ë wt o ¯ tan d =
the basis of the suggestion of Cole and Cole, Equation 2282 can be written as 1 + (wt )1a sin ap 2 e r  e r• = e rs  e r• 1 + 2(wt )1a sin ap 2 + (wt )2 (1a )
(2283)
e rs  e r• st o + eo 2
tan d =
(2280)
e o (e rs  e r • ) + st o wt oe oe r•
(2281)
The variation of e¢r and tan d with w, including the effect of DC conductivity, is shown in Figure 232, and the Argand diagram of er  e¢r relation showing this effect in Figure 233.
(wt )1a cosap 2 e r¢ = e rs  e r• 1 + 2(wt )1a sin ap 2 + (wt )2 (1a )
(2284) When a = 0, Equations 2283 and 2284 reduce back to the Debye equations. The dispersion curve with a > 0 is broader than that for a single relaxation time but still symmetrical about wt de r¢ = 0, we can find that the = 1. By setting dw maximum loss also occurs at wt = 1. By eliminating wt from Equations 2283 and 2284, we obtain 2
Èe  (e rs + e r • ) ˘ + Èe ¢ + (e rs  e r • ) tan ap ˘ ÍÎ r ˙˚ ÍÎ r 2 2 2 ˙˚ = ÈÍ Î
2.6.6 The Cole–Cole Plot Debye equations (Equations 2256 and 2257) based on a single relaxation time do not suffice to describe the relaxation phenomena for most dielectric materials, e.g., polymers. In this case, a distribution of relaxation times is necessary to interpret the experimental data. In Section 2.7, we shall discuss the approach based on a distribution of relaxation times. However, to take into account the effect of a distribution of relaxation times, Cole and Cole52 have proposed that an Argand diagram, in which e¢r is plotted as a function of er, can be constructed following the empirical relation e r*  e r• = e r  e r•  je r¢ =
95
e rs  e r• 1 + ( jwt o )1a
(2282) where a is the parameters with 0 < a < 1. In fact, many materials, particularly polymers with long chains, have a broader e¢r  nw dispersion curve and a lower maximum loss than would be expected from the Debye semicircle shown in Figure 231.39 In such cases, the er e 1r arc will fall inside the Debye semicircle. On
e rs  e r• ap ˘ sec 2 2 ˚˙
2
2
(2285)
This equation represents a circle with the center e rs  e r • (e rs  e r • ) ap ˘ at ÈÍ and the ,tan 2 2 ˙˚ Î 2 È e rs  e r • sec ap ˘ radius of Í . This is shown in 2 ˙˚ Î 2 Figure 234. The Cole–Cole plot exhibits a depressed semicircle because of a > 0. Some experimental results agree well with Equations 2283 and 2284 with a > 0.39 Debye’s er  e¢r semicircle is based on a = 0, which represents the materials’ having only one single relaxation time. In general, there exists a distribution of relaxation times in all solid materials because there are always some nonuniformities in local domains, which would alter the individual dipoles or charges in addition to existing dipoles in the material. If the relaxation times are due to several different mechanisms, then the er  e¢r arc will be asymmetrical.53,54 Several investigators53–56 have put forward suggestions to modify the Cole–Cole empirical equations. Some of the equations are listed below for comparison purposes:
96 Dielectric Phenomena in Solids
e¢r Dominant s Effect
w
Negligible s Effect
w = to
tand
tand(max) Dominant s Effect
w
Negligible s Effect
1/2
w = (ers /er•)
Figure 232 e¢r and tan d as functions of w, taking into account the effect of DC conductivity.
/to
Electric Polarization and Relaxation e¢r D C B
A
er∞
er
ers
Figure 233 The effect of DC conductivity on the er  e¢r arc. (A) s = 0, (B) s = s1 > 0, (C) s2 > s1, (D) s3 = s2.
e¢r e¢r (max)
w (ers + er•)/2
er• (ers – er•)tan(ap /2) 2
ap /2
ap /2
ers
er
Debye equation e r*  e r• =
e rs  e r• 1 + jwt
(2255)
Cole–Cole equation e r*  e r• =
e rs  e r• 1 + ( jwt )1a
(2282)
Davidson–Cole equation e r*  e r• =
e rs  e r• (1 + jwt )b
e rs  e r• [1 + ( jwt )1a ]b
2e r¢(max) (wt )l + (wt )l
(2288)
where l is the parameter with the value 0 < l < 1, and e¢r(max) is the maximum value of the loss factor when wt = 1. On a logarithmic frequency scale, the e¢r  (nw) relation exhibits a symmetrical bellshaped curve about a central frequency w = 1/t, which is broader than the corresponding Debye curve (Equation 2257), but very similar in shape to, although not identical with, that based on the Cole–Cole equation (Equation 2284). The difference can be seen by comparing these two equations. Cole57,58 has discussed the correlation between these two equations in some detail.
(2286)
Havriliak–Negami equation e r*  e r• =
equation will reduce to the Debye equation for b = 1. But, with b < 1, the er  e¢r arc will become asymmetrical, as shown in Figure 235(a). It has been found that several materials obey the Davidson–Cole equation, such as glycerol triacetate55 and Pyralene (a fluid mixture of chlorinated diphenols in chlorobenzene).17 However, the Havriliak–Negami equation gives a much better fit to most experimental results if a and b are properly chosen. The er  e¢r arc for a = 2/3 and b = 1/2 is shown in Figure 235(b). In the Havriliak–Negami equation, the parameters a and b are not based on the physics of the dielectric polarization, although the modification of the original Cole–Cole equation empirically may make the equation better fit experimental results. The modification does not lead to a better understanding of the physics behind the distribution of relaxation times. Fuoss and Kirkwood56 have also put forward a semiempirical equation, called the Fuoss–Kirkwood equation, to relate only the imaginary part e¢r of the complex dielectric constant with frequency, which is given by e r¢(w ) =
Figure 234 The Cole–Cole plot for dielectric material with a set of relaxation times.
97
(2287)
All of these equations depend on the values of a and b chosen within the ranges 0 < a < 1 and 0 < b < 1. Obviously, the Davidson–Cole
2.6.7 Temperature Dependence of Complex Permittivity Complex permittivity is a complex function of both the frequency and the temperature, apart from the dependence of other parameters such as pressure, etc. We have briefly discussed the frequency dependence of er and e¢r. The
98 Dielectric Phenomena in Solids e¢r w to = 1
w bp /4 ers
er•
er
(a) e¢r
w w to = 1 (1 – a)bp /4 er•
ers
er
(b) Figure 235 The er  e¢r arcs based on (a) the Davidson–Cole equation for b = 1/2, and (b) the Havriliak–Negami equation for a = 1/3 and b = 1/2.
temperature dependence of er and e¢r is mainly through the temperature dependence of the relaxation time which can, for a single relaxation time, be expressed as t = t h exp( H kT )
(2289)
where th is a preexponential factor and H is the activation energy.28 By replacing to with a temperaturedependent t, the Debye equations (Equations 2256 and 2257) can be written as e r = e rT• +
e  e rT• 1 + w t exp(2 H kT )
e r¢ = (e rsT  e rT• )
T rs 2 2 h
(2290)
wt h exp( H kT ) 1 + w 2t h2 exp(2 H kT )
(2291) T where e Trs and e r• are the value of ers and er• at temperature T. It can be seen from these two equations that the dielectric constant er and the loss peak e¢r(max) decrease with increasing temperature, and the loss peak shifts toward higher temperatures, as shown in Figure 236. If
(ers  er•) for nondipolar materials is not temperature dependent, then the area beneath the e¢r vs 1/T curve depends only on the activation energy H and does not depend explicitly on frequency, based on the following equation:
Ú
• 0
1 k p e r¢d Ê ˆ = (e rs  e r • ) Ê  tan 1 wt ˆ ËT¯ ¯ HË2
(2292) For tan1 wt < p/2, the area beneath the e¢r vs 1/T curve is practically independent of frequency. However, for dipolar materials with dipolar T molecules, (e rsT  e r• ) is temperature dependent. According to the theories of Onsager, Frohlich, and Debye (see Section 2.5.2), we can write (e rsT  e rT• ) =
A T
(2293)
where A is a constant. In this case, the area beneath the e¢r vs 1/T curve is more complicated, and it is given by39,59
Electric Polarization and Relaxation
99
T1
er
w1
T2 > T1
w 2 > w1
w1
e¢r
er
T2 > T1
e¢r
er
T1 w 2 > w1
e¢r w
Tmax
(a)
T
(b)
tand
w1
w 2 > w1
T max ¢
T
(c) Figure 236 (a) er and e¢r as functions of w for fixed temperatures T1 and T2 with T2 > T1, (b) er and e¢r as functions of temperature for fixed frequencies w1 and w2 with w2 > w1, and (c) tan d as a function of temperature for fixed frequencies w1 and w2 with w2 > w1. For the same frequency, Tmax for e¢r(max) is higher than T¢max for tand(max).
Ú
• 0
1 e r¢d Ê ˆ ËT¯
Ú
( 1) (wt ) Ak È plnwt +Â (2 r + 1)2 H ÍÎ 2 r =1 •
2
=
r
2 r +1
˘ ˙˚
(2294) By denoting Tmax as the temperature at which e¢r is maximum, then (e rsTmax  e rT•max ) =
A Tmax
t Tmax = t h exp( H kTmax )
(2295) (2296)
In general, wtTmax differs little from unity.60 Thus, for the frequency range normally encountered in practice (wt < 1), Equation 2294 can be approximated to
• 0
1 pk e d¢ d Ê ˆ = (e rsTmax  e rT•max ) ËT¯ 2H
(2297)
For wt < 1, Equation 2297 differs from EquaT tion 2292 only in the (e rsT  e r• ) term. Thus, the area beneath the e¢r vs 1/T curve is still practically independent of the frequency, as shown in Figure 236. It should be noted that for the same w, T¢max, for tan d to be maximum, is lower than Tmax for e¢r to be maximum. The same concept for temperature dependence of er and e¢r can be applied to other empirical equations—the Cole–Cole equation, the Davidson–Cole equation, and the Havriliak– Negami equation. The measurement of e¢r as a function of frequency at a fixed temperature is equivalent to the measurement of e¢r as a
100
Dielectric Phenomena in Solids
function of temperature at a fixed frequency. Both methods should provide similar information provided that there is no change in the specimen and the DC conductivity is negligible over the temperature range for the measurements. 2.6.8 Field Dependence of Complex Permittivity From Equations 268 and 2224, it can be seen that if the relationship between the polarization P and the electric field F is linear and the electrical conductivity s is constant, then the dielectric constant er and the loss factor e¢r should be independent of electric field. This is true only when the total field during the measurement of these parameters is low. However, when the specimen is biased with a strong field, s may not be constant or the P–F relationship may become nonlinear, then er and e¢r, measured with a smallsignal AC voltage, will be fielddependent. Since the total current density in a material specimen under an AC field is given by dF = sF + j(e r  je r¢ )e o F dt (2298) = (s + e r¢e o )F + je re o F
JT = J + e *
the complex relative permittivity, including the electrical conductivity s, can be expressed as s ˆ ¢ = e r  j Ê e r¢ + e r* = e r  je rT Ë we o ¯
(2299)
where J is the conduction current, e¢rT is the total loss factor, including the loss factor due to the loss involved in the polarization processes and the loss due to the electrical conduction involving the movement of charge carriers. In the following sections, we shall discuss the effects of strong electric fields on complex permittivity for three categories of materials: semiconducting, ferroelectric, and insulating.
Semiconducting Materials In semiconductors, the concentration of free charge carriers and hence the conductivity are high. The value of the conductivity s at
microwave fields of frequencies of the order of 10 GHz (10 ¥ 109 Hz) or higher may become complex. Only at AC fields of frequencies low enough for the current capable of following the field, the conductivity would have the value appropriate to that at a DC field of the same magnitude. If the total field applied to a semiconductor specimen is F = FDC + FAC coswt
(2300)
with FAC << FDC. For AC fields not high enough to heat the charge carriers, the current may no longer follow the field at frequencies for which wt is comparable to unity, where t can be taken as the mean free time between collisions. Obviously, t depends on both the temperature and the applied field magnitude; it decreases with increasing temperature and with increasing field magnitude. So we can describe the situation by expressing the AC conductivity as a complex conductivity s*(w) with the real part s(w) representing the inphase conductivity, which means the current capable of following the field, and the imaginary part s¢(w) representing the outofphase conductivity (p/2 lagging the field). For a simple band structure, the AC conductivity at low AC fields is given by s *(w ) =
nq 2 È DEavet m m * ÍÎ DEave (1 + w 2t m2 ) wt m DEavet m ˘ j DEave (1 + w 2t m2 ) ˙˚
(2301)
= s (w ) + js 1(w )
where DEave is the average energy of the carrier, n is the carrier concentration, q is the electronic charge, m* is the effective mass of the carrier, and tm is the momentum relaxation time, which is the average time required for a component of the carrier momentum in any direction to be reduced to 1/e of its value.61,62 The t mentioned above can be considered to be identical to tm.61 The symbol · Ò indicates the average values to be taken over the carrier distribution in the specimen. The outofphase current (p/2 lagging FAC) may be thought of as a contribution to the displacement current, so that we can write the dielectric constant and the loss factor
Electric Polarization and Relaxation
101
20 15.5
15 78 K
10
15.0 SmallSignal Dielectric Constant
SmallSignal Dielectric Constant
300 K
5 0 –5 –10
14.5
Apparent Dielectric Constant of Intrinsic Germanium
14.0 13.62 13.5
Observed Dielectric Constant Dielectric Constant Deduced from Absorption Data
13.0
–15
12.5
–20 0
2.5
10 12.5 5.0 7.5 Electric Field (kV/cm)
15
(a)
0
1
2 3 4 Electric Field (kV/cm)
(b)
Figure 237 The variation of smallsignal dielectric constant with DC bias field: (a) for nGe specimen of lowfield resistivity of 1.9 ohmcm at 300 K and smallsignal frequency of 70 GHz, and (b) for nGe specimen of low field resistivity of 4.7 ohmcm at 300 K and small signal frequency of 35 GHz.
for semiconductors at high frequency AC fields as e rT (w ) = e r (w ) +
s 1(w ) we o
(2302)
¢ (w ) = e r¢(w ) + e rT
s (w ) we o
(2303)
Since s ¢(w) is negative, the contribution of the carriers to the dielectric constant is also negative. This implies that s ¢(w) tends to decrease the dielectric constant, and it may even make the dielectric constant negative for high carrier concentrations. Using a smallsignal AC field FAC cos wt superimposed on a DC bias field FDC, as given by Equation 2300, the field dependence of the dielectric constant for n type germanium specimens with lowfield resistivity of 1.9 ohmcm and the smallsignal frequency of 70 GHz is shown in Figure 237(a). The results are from Conwell, Fowler, and Zucker.62,63 At T = 300°K and FDC = 0, erT does not lie much below er, which is about 16, because of the small value
of wtm(wtm £ 0.1). However, at T = 78°K and FDC = 0, tm becomes larger, making wtm close to unity. In this case, the carrier contribution becomes large enough to result in a large negative value of erT. The DC bias field tends to reduce the value of tm and hence the value of wtm, thus reducing the carrier contribution to the dielectric constant, as shown in Figure 237(a). Similar results have also been observed for ntype germanium specimens with lowfield resistivity of 4.7 ohmcm and the smallsignal frequency of 35 GHz, as shown in Figure 237(b). The results are from Gibson, Granville, and Pagie.62,64 Obviously, the loss factor e¢rT is also field dependent through the field dependence of tm, as indicated in Equations 2301 and 2303. Ferroelectric Materials For ferroelectric materials, the applied electric field has a marked effect on complex permittivity. In Thermodynamic Theory in Chapter 4, we mention that the application of a suitable
5
102
Dielectric Phenomena in Solids
DC field can shift the Curie point temperature of BaTiO3 to a higher temperature, converting the paraelectric state to the ferroelectric state; this converted ferroelectric state will return to the paraelectric state when the electric field is removed. However, dielectric constant is field dependent in the paraelectric state at temperatures above the Curie point temperature Tc. Typical results for triglycine sulphate (TGS) and potassium dihydrogen phosphate (KDP) are shown in Figure 238. In the measurements of the effects of an applied electric field, the electric field used to induce the polarization P was a 200 Hz sinusoidal field, while for the measurements of the dielectric constants a smallsignal AC field was used and kept constant and low at a fixed frequency of 50 kHz. The results shown in Figure 238(a) for TGS are from Triebwasser,65 and those in Figure 238(b) for KDP are from Baumpartner.66 When no electric field is applied to the specimen, the polarization P is equal to zero. When a finite electric field F is applied, it induces a finite value of the polarization P. For T > Tc and F = 0, the dielectric constant follows closely the Curie–Weiss relation (see Chapter 4) er =
C T  Tc
(2304)
where C is known as the Curie constant. In ferroelectric materials, there exists an intrinsic bias, which produces just the same effects on the dielectric constant as an applied bias.67 Since the applied electric field along the ferroelectric axis is opposite in sign to the intrinsic bias, the net dielectric constant decreases with increasing applied field, as shown in Fig. 2.38. Insulating Materials Insulating materials generally refer to the materials with a large bandgap, a low concentration of free charge carriers, a small carrier mobility, and hence an extremely small conductivity. Therefore, for these materials we can ignore the effects of electrical conuctivity s because it would be negligibly small. The field dependence of the complex permittivity is associated mainly with the nonlinear field dependence of the polarization. Excluding the hopping and
the space charge polarizations for simplicity, the major types of the polarization are electronic polarization (Pe), atomic polarization (Pi), and orientational polarization (Po). For Pe and Pi, the polarizationfield relationship should remain linear even at high fields. But for Po, the polarizationfield relationship is linear only at low fields and becomes nonlinear at high fields. Dipolar molecules in a material are similar to balls with a positive charge on one end and a negative charge of the same magnitude on the other end in a viscous fluid. They are in motion due to thermal agitation. When an electric field is applied across a material specimen between two electrodes, these dipolar molecules will orient toward the direction of the field, with the end of positive charge facing the negative electrode (cathode) and the end of negative charge facing the positive electrode (anode), resulting in orientational polarization. The magnitude of the polarization depends on the angle made between the dipole axis and the field direction, which, in turn, depends on the applied field strength and the temperature. The degree of polarization is governed by the Langevin function, as discussed in Section 2.3.3. It should be noted that molecules are generally not spherical in shape, but rather ellipsoidal. So, even in nondipolar materials, the molecules are not dipolar but are ellipsoidal in shape; the molecules will still orient under an applied electric field in order to reduce their potential energy. In fact, a molecule can be considered a configuration built up of a number of charges; it will be distorted in an elastic system under an external electric field. Including its distortion, any molecule can be represented by an ellipsoid with three principal polarizabilities related to the three perpendicular axes. If such a molecule is placed in a field, the axis of highest polarizability will orient toward the direction of the field to reduce its potential energy to a minimum. Therefore, there will exist an orientation effect in a manner similar to the dipolar molecules (see Classical Approach in Section 2.3.1). It can be imagined that in a high electric field, all individual molecules will be largely oriented, so that there can be little extra polarization from the further orientation of dipolar or nondipolar
1.2
er (F )/er (O)
Tc = 49°C
0.8
T – Tc = 2.0°C 0.4
T – Tc = 0.5°C
0
T – Tc = 1.0°C
2
4
6
F (kV/cm)
(a) 10000 F=0 Tc = –150°C 5000 4000 3000 500
F (V/cm)
1500 1000 1000 2000 3000 4000 5000 6000
Dielectric Constant (er)
2000
500 400
8000
300
12000 200
18000
150
0.1
0.2
0.3
0.5
1.0 T – Tc (°C)
2.0
3.0
5.0
100 10.0
(b) Figure 238 The variation of smallsignal dielectric constant with DC bias field, with the field applied along the ferroelectric axis at temperatures above the Curie point temperature TC for (a) triglycine sulphate (TGS) [(NH2CH2COOH)3H2SO4], for which er(F) is normalized to er(F = 0), and (b) potassium dihydrogen phosphate (KDP) [KH2PO4] plotted as a function of temperature at various DC bias fields.
104
Dielectric Phenomena in Solids
molecules when the field is further increased. Under this situation, the polarization becomes saturated; this phenomenon is known as dielectric saturation. Several investigators68–72 have observed experimentally that the static dielectric constant of dipolar solution decreases as the applied electric field is increased, and that the amount of the decrease in dielectric constant is approximately proportional to the square of the field strength. It should be noted that in order to observe the dielectric saturation phenomenon, the material used must be in fluid state so that molecules have freedom to orient; in a material in solid state, the molecules are frozen, losing their ability to move. Several investigators have studied this phenomenon theoretically and proposed equations to elucidate quantitatively the behavior of the dielectric constant at high fields. The first was Debye.31 Later, van Vlect,18,72 Böttcher,6 and several others74–79 also put forward their approaches based on their assumptions. All of the theoretical equations are derived on the basis of some assumptions, but none of them is very satisfactory. It is obvious that the tremendous local fields existing around ions and dipoles in the solution must have large effects on the dielectric behavior. An accurate method to calculate such local fields is still not available. We shall not include the discussion of various analyses for this dielectric saturation phenomenon here. The reader interested in this topic is referred to the references cited above. In the following, we shall present a simple analysis with the aim of showing the physical concept of this phenomenon. In a dielectric solution under a high electric field, the average dipole moment in the direction of the field is given by [see Equations (2.123), (2.129) and (2.130)] uF = uo L( z )
z=
uo Floc kT
L( z ) = coth z 
(2306)
(2307)
Here, we must use the local field Floc instead of the applied field F. The local field is always larger than F by a local field correction factor B, so Equation 2302 can be rewritten as z=
uo BF kT
(2308)
At high fields (HF) for which z > 1, we must include higher power terms of L(z). For simplicity, we take only the terms up to z3. Thus, the polarization can be written as P( HF ) = [(e r •  1) + e ro( HF ) ]e o F Buo2 F È = N Ía e BF + a i BF + 3kT Î 3 uo uo BF ˆ ˘  Ê 45 Ë kT ¯ ˙˚
(2309)
Assuming that for the same high field, the dielectric constant remains the same as that obtained at low fields, based on the linear part of the Langevin function shown in Figure 217, the polarization can be written as P = [(e r •  1) + e ro ]e o F Buo2 F ˘ È = N Ía e BF + a i BF + 3kT ˙˚ Î
(2310)
The difference between P(HF)  P in Equation 2309 and Equation 2310 gives the difference between ero(HF) and ero due to the effects of high fields. Thus, we have DP = P( HF )  P = [e ro( HF )  e ro ]e o F =
Nuo Ê uo BF ˆ 45 Ë kT ¯
3
(2311)
and the decrease in dielectric constant as
(2305)
where L(z) is the Langevin function, which can be expressed in the form of a series as 1 z 3 2z5 È1 z z ˘ 1 =Í + +  ... ˙ Î z 3 45 945 ˚ z 3 5 2z z z = +  ... 3 45 945
in which z is
De r = 
4 2 Ê Nuo F ˆ 3 B Ë 45e o k 3T 3 ¯
(2312)
Depending on the local field correction factor B, Der is proportional to the square of the applied field and inversely proportional to T3. If the local field, based on Lorentz’s approach, is used, B is given by B=
e rs + 2 3
(2313)
Electric Polarization and Relaxation
If the reaction field, based on Onsager’s approach, is used, B is given by B=
3(e rs  e r • )(2e rs + e r • ) e rs (e r • + 2)2
(2314)
The basic difference among the different expressions put forward by other investigators lies mainly in the different expressions for B. However, this simple analysis, though not accurate, does provide a way to understand this phenomenon.
2.7 Dielectric Relaxation Phenomena Using the timedomain approach, measurements of the growth or the decay of the polarization when a stepfunction electric field is suddenly applied or removed from the specimen will yield information about the relaxation behavior equivalent to that from the measurements of er and e¢r as functions of frequency based on the frequencydomain approach. In the previous section, we discussed the relation of the dielectric constant and absorption, with frequency based on the frequencydomain approach. In the present section, we shall use the timedomain approach to deal with relaxation phenomena. In general, the timedomain response provides conspicuous information about the nonlinearity of the dielectric behavior simply by varying the amplitude of the applied stepfunction field. The basic experimental arrangement for the measurements of the timedomain response, (i.e., the transient charging or discharging current, resulting from the application or the removal of a step DC voltage) is shown schematically in Figure 239(a). This arrangement was originally used by Williams.80 The circuit is selfexplanatory. The switch S1 has two positions: one for turning on the step DC voltage to start the flow of the charging current, the other for shortcircuiting the specimen to allow the discharging current to flow after the specimen has been fully charged to a steadystate level. The switch S2 is used to shortcircuit R1 to provide a path for surge currents for a very short period of time to
105
protect the circuit; it also gives a chance to adjust the amplifier to a null position before recording the transient current. It is important to make the time constant of the amplifier, which depends on the stray capacitance in shunt with R1, much smaller than the time during which the transient current is flowing. The specimen has the guard and the guarded electrodes, the outer guard electrode being connected to ground to eliminate surface leakage currents from the specimen. The charging or discharging current is measured as a voltage appearing across R1 by means of a DC amplifier. The voltage drop from point A to ground is made zero by a negative feedback in the amplifier circuit, which produces a voltage across R2 equal and opposite to that across R1, thus making the applied step voltage across the specimen only. The step voltage, and the charging and discharging current as function of time, are schematically shown in Figure 239(b), in which Io is the steady DC component of the charging current and the width of the step voltage is 63 seconds. 2.7.1 The Hamon Approximation In principle, the equivalent frequencydomain response of a dielectric material can be obtained from a timedomain response by a Fourier transformation which extracts all the separate harmonic components from the charging or the discharging current. For a linear dielectric material in a capacitor of unit area in crosssection and d in thickness, as shown in Figure 239(a), the complex dielectric constant can be expressed as •
e r*(w ) = e r• + Ú f (t )e  jw tdt  j o
so we o
(2315)
where so is the steady DC electrical conductivity and f(t) is the decay function of the transient current J(t).81 Thus, f(t) can be written as f (t ) =
J (t ) eo F
(2316)
where F is equal to V/d. Note that f(t) does not include the contribution to the observed tran
106
Dielectric Phenomena in Solids a S1 b Specimen A
Amplifier
V R1
S2
B Meter
R2
(a) Step Voltage V
t = 63 sec
t=0
I (mmA)
Charge
I0
Discharge
10
20
30
40
50
60
120
Time (sec)
(b) Figure 239 Schematic diagrams illustrating (a) the basic experimental arrangement for the measurements of the charging and the discharging current resulting from the application and the removal of a step voltage, and (b) the step voltage and the charging and the discharging current as functions of time. Io is the steady DC component of the charging current.
sient current J(t) from the steady DC conductivity of the specimen. By considering only the relaxation component of the transient current, the complex dielectric constant should not include the term so /weo, although it is part of the total loss factor. Thus, we have
For a simple relaxation process involving only one single relaxation time based on the Debye theory, the decay function is f (t ) = A exp( t t o )
where A = (e rs  e r • ) t o
•
e r*(w ) = e r (w )  je r¢(w ) = e r• + Ú f (t )e  jw tdt u
(2317)
(2318)
(2319)
However, for relaxation processes involving a distribution of relaxation times, as in poly
Electric Polarization and Relaxation
mers, f(t) would be a complicated function of time, and an explicit expression for the spectra of er(w) and e¢r(w) cannot be deduced by analytical integration of Equation 2317. Of course, if f(t) can be determined experimentally over the entire range of time, numerical solution of Equation 2317, with the aid of a computer, would provide information about er(w) and e¢r(w). However, the frequencydomain response for the case with a distribution of relaxation times can be expressed by empirical equations (see Equations 2282 and 2286 through 2288), hinting that the timedomain response can also be expressed by an empirical equation such as J(t ) = At  r
(2320)
From Equation 2316, the decay function can be written as f (t ) =
J (t ) = Bt  r eo F
e r¢(w ) =
(2322) e r¢(w ) = Bw r 1G(1  r )cos rp 2 , 0 < r < 2
(2323) where G(1  r) is the gamma function.16,39 If B and r are known, er(w) and e¢r(w) at any desired value of w can be obtained from Equations 2322 and 2323. To simplify the calculation, Hamon82 has proposed an approximation method, generally referred to as the Hamon approximation. Equation 2323 for e¢r(w) may be rearranged to the form e r¢(w ) =
(2324)
J (t ) we o F
(2325)
This criterion implies that G(1  r )cos rp 2 =1 (wt ) r
or w t = [ G(1  r )cos rp 2]1 r
(2326)
Hamon found that for 0.1 < r < 1.2, the righthand side of Equation 2326 is approximately constant at a value of p/5 = 0.63 at an accuracy of about 3%. Based on the Hamon approximation, the loss factor can be expressed simply as e r¢(w ) =
e r (w ) = e • + Bw r 1G(1  r )sin rp 2 , 0 < r < 1
Bt  r È G(1  r )cos rp 2 ˘ ˙˚ w ÍÎ (wt ) r J(t ) È G(1  r )cos rp 2 ˘ = ˙˚ we o F ÍÎ (wt ) r
The basic criterion for the Hamon approximation is that at a certain value of t in Equation 2324 e¢r (or) value of t in Equation 2324, e¢r(w) at any desired value of w can be obtained simply by the following expression
(2321)
in which B = A/eoF. At a fixed constant temperature, the constant A (and hence the constants B and r) can be determined for a specific dielectric material by a direct fitting of Equation 2320 to the experimental data of the charging or the discharging current. Substitution of Equation 2321 into Equation 2317, followed by integration, yields
107
J(t = 0.63 w ) we o F
(2327)
This equation indicates that the observed transient current J(t) at t = 1 sec and 10 sec corresponds to the frequency f = w/2p = 0.63/2pt = 0.1/t = 0.1 Hz for t = 1 sec, and 102 Hz for t = 10 sec. That means that we can obtain e¢r(w) at f = 0.1 Hz and 102 Hz using the value of J(t) at t = 1 sec and at 10 sec, respectively. The dielectric constant er(w), based on the Hamon approximation, can be deduced from Equations 2322 through 2324. It is e r (w ) = e r• + e r¢(w )tan r p 2 , 0.1 < r < 1
(2328) The Hamon approximation is not rigorous, since Equation 2321 does not hold in practice over the entire range of times. Williams83 has shown that the Hamon approximation can be derived more rigorously for lowfrequency long relaxation time or highfrequency short relaxation time for dielectric materials following the Cole–Cole empirical relation (see Equation 2282). Later, Hyde84 treated this timefrequency transformation problem based on the data of the timeintegral of the transient current, i.e., the charge Q(t). The measurement of the charge on the capacitor plates rather than the
108
Dielectric Phenomena in Solids
current through the specimen has some advantages in principle. The decay function for Q(t) can be obtained directly, and Q(t) is usually bound at short times, while J(t) involves a much longer time to reach a steady level though the current is much easier to measure. Hyde’s approach may be more accurate, but it involves more computations. Using inline computation, Hyde’s method can provide a rapid means of determining er(w) and e¢r(w) over the frequency range of 104 to 106 Hz.84 The Fourier transformation technique has been extended to obtain very high frequency (108 to 1010 Hz) data. The experimental method is usually referred to as timedomain spectroscopy. It involves the use of a waveguide and very shortduration pulses with fast rise times, the reflected or the transmitted pulses being observed with a sampling oscilloscope.85 However, the Hamon approximation is useful for a rapid appraisal of the dielectric losses and the dielectric constant from the polarization or the depolarization current in practical dielectric materials, such as polymers.
H for dipole orientation and hence the relaxation time t, as well as the preexponential factor th based on Equation 2289. In polymers, the molecules are complex; the orientation of the polar group related to the link segment along a polymer chain may involve many relaxation times. For example, in polyvinyl chloride, the degree of rotation of the polar groups about the C–C axis depends on the position and the angle of the section of the C–C links. If a system has more than one type of dipole, the relaxation times will be distributed. Supposing that N is the number of dipoles of one type per unit volume, than we can write (2329)
N = No f (t )
where No is the total number of dipoles of all different types per unit volume, f(t) is the distribution function of the relaxation time t or the probability density of t. Thus, f(t)dt represents the probability density of f(t) in the interval between t and t + dt. So, we can write •
Ú f (t )dt = 1
(2330)
0
2.7.2 Distribution of Relaxation Times Dipoles (permanent or induced) are generally present in inorganic, organic, and biological materials. Orientational polarization plays a decisive role in dielectric phenomena in materials. The behavior of a polar molecule in a material is similar to a body of ellipsoidal shape in a viscous fluid. If these bodies in the fluid are not all identical in size, then their orientations will involve more than one relaxation time. Since molecules are generally ellipsoidal in shape, the friction coefficients of the three axes are different; hence, three different relaxation times may exist. Many reasons exist for the relaxation times to be distributed in solids, the most obvious being the presence of inhomogeneities. It is likely that not all dipoles in a solid are situated in the same environment, so some are more free to rotate than others. Even in a single crystal, dipoles may find certain orientations more favorable than others and certain transitions between orientations easier than others. The variation of such local transition probabilities reflects the variation of the activation energy
Taking into account the distribution of relaxation times, the Debye equations, (Equations 2255 through 2258) become •
f (t )dt 1 + w 2t 2 0
e r = e r• + (e rs  e r • )Ú
(2331)
•
wt f (t )dt 1 + w 2t 2 0
e r¢ = (e rs  e r • )Ú
(2332)
•
e r¢ tan d = = er
wt f (t )dt 1 + w 2t 2 0
(e rs  e r • )Ú
•
e r• + (e rs  e r • )Ú 0
f (t )dt 1 + w 2t 2
(2333)
If t is distributed, then the peak value of e¢r decreases and the spread width of e¢r increases, as shown in Figure 240. The area beneath the curve in Figure 240 can be expressed as •
S=
•
Ú e ¢d(lnw ) = Ú e ¢ r
r
•
0
•
•
dw w
dw w tf (t )dt = (e rs  e r • )Ú w Ú0 1 + w 2t 2 0
(2334)
Electric Polarization and Relaxation
109
times makes e¢r(max) decrease, Fuoss and Kirkwood56 have proposed a parameter l with 0 < l < 1 to modify Equation 2257 to take into account the effect of the distribution of relaxation times empirically. They have changed Equation 2257 to the following form:
A e¢r B
l(e rs  e r • ) (wt )l + (wt )l 1 = (e rs  e r • )Sech[lln(wt )] 2
e r¢ =
When wt = 1, the maximum value of the loss factor, termed e¢r(max), occurs. It is
n w n w = n (l/to) Figure 240 The e¢r  n w curves (A) involving only one relaxation time, and (B) involving a set of relaxation times, each having its Debyetype loss peak.
By changing the integration order, we have •
•
S = (e rs  e r • )Ú t f (t )dt Ú 0
0
dw 1 + w 2t 2
(2335)
Since •
dw
Ú 1+ w t
2 2
0
=
p 2t
•
Ú f (t )dt = 1 0
e r¢(max) = l(e rs  e r • )
n
(2336)
This equation implies that the area is not related to the distribution function f(t). This means that the area beneath the e¢r  nw curve for any number of relaxation times is identical irrespective of the dispersion mechanisms of t and irrespective of f(t). The quantity De r = e rs  e r• =
2 p
•
Ú e ¢d(lnw ) = r
•
2S (2337) p
is called the relaxation strength, which is an important physical parameter in relaxation processes. Since f(t) is unknown, we cannot determine er(w) and e¢r(w) from Equations 2331 and 2332. Because the distribution of relaxation
(2339)
Substitution of Equation 2339 into Equation 2338 gives the expression exactly the same as Equation 2288—the Fuoss–Kirkwood equation. When l = 1, Equation 2338 returns to the Debye equation in the case of only one relaxation time. So l < 1 implies that the relaxation processes involve more than one relaxation time. Thus, the smaller the value of l, the higher the number of different relaxation times, the wider the spread of e¢r(w), and hence the smaller the value of e¢r(max). This implies that the distribution function f(t) covers a wide range of frequencies. To find f(t), we can rewrite Equation 2332 to the form86
Equation 2330 reduces to p S = (e rs  e r • ) 2
(2338)
e r¢ = (e rs  e r • )Â i =1 j =1
w it j f (t j )Dt j 1 + w i2t 2j
(2340)
If the summation is represented by a matrix M, then e¢r = Mf(t), where the elements of the matrix are È w it j Dt j ˘ Aij = (e rs  e r • )Í 2 2˙ Î1 + w i t j ˚
(2341)
So the distribution function f(t) can be expressed in terms of the inverse matrix as f (t ) = M 1e r¢
(2342)
If e¢r is known, f(t) may be determined. However, this method is suitable for the continuous distribution of the relaxation times. Great errors may result if the relaxation process involves only a few, discrete relaxation times.
110
Dielectric Phenomena in Solids
If all dipoles follow Debye’s relaxation model, f(t) may be expressed as f (t ) =
1 exp( t t ) t
(2343)
If the distribution of the relaxation times assumes a Gaussian type of distribution, then we have f (t ) = ( b p 2t )exp{[ bln(t t o )]2 }
(2344)
where b is a constant and to is the central and the most probable relaxation time. The empirical relation developed by Cole and Cole52 corresponds to the distribution function52,56 f (t ) =
sin ap 2[cos h( lnt t o ) + cos lp ]
(2345)
Based on Equation 2289, we can write DH ˘ t H  Ho ˘ = exp ÈÍ = exp ÈÍ Î kT ˚˙ Î kT ˚˙ to
(2346)
The distribution function for activation energies for dipole orientation G(H) can be written as G( H )d(DH ) = f (t )d( lnt t o )
(2347)
This expression represents the fraction of dipoles having activation energy for orientation between H  d (DH)/2 and H + d (DH)/2. A great deal of work has been carried out in studying the distribution functions for the relaxation times and their associated activation energies. However, the molecular processes leading to such various distributions are still not well understood. We still rely on some empirical approaches. It is possible that a collective and cooperative mechanism may be involved. 2.7.3 The Relation between Dielectric Relaxation and Chemical Structure This is a huge topic, and we shall not include a detailed review of it in this chapter. There are several excellent reviews dealing with this topic, and the reader who is interested in more details is referred to these reviews.26,39,87–94 Here, we shall briefly discuss the relation between dielectric relaxation and chemical structure, taking polymers as an example.
In polymers, there are mainly two types of dielectric relaxation: dipolar segmental relaxation and dipolar group relaxation. The dielectric relaxation processes of these two types exhibit loss peaks on the curves of the temperature or frequency dependence of e¢r. In amorphous polymers, the most intensive peaks of e¢r or tan d occur in the region of the transition from the glassy to the rubbery (high elastic) state, i.e., near the glass transition temperature Tg. Dielectric losses caused by dipolar segmental relaxation are associated with the microBrownian motion of segments in polymeric chains, while dielectric losses caused by dipolar group relaxation are associated with the localized movement of molecules. Several distinct dielectric relaxation processes are usually present in solid polymeric materials. They can be observed by means of the thermally stimulated relaxation technique.94 As the temperature is raised, the mobility of various types of molecules becomes successively enhanced, making it easier for dipolar orientation to occur. Usually, dielectric relaxation processes are labeled by a, b, g, d, and so on, beginning at the hightemperature end. Figure 241 illustrates schematically the a, b, and g peaks on the curve of the loss factor e¢r as a function of temperature at a fixed frequency. In this convention, the dipolar segmental relaxation corresponds to the a relaxation, and the dipolar group relaxation processes correspond to the b, g, d, relaxations. The hightemperature a relaxation is mainly a
b
e¢r g
Temperature Figure 241 Schematic illustration of the loss factor e¢r as a function of temperature showing the a, b, and g loss peaks.
Electric Polarization and Relaxation
associated with the microBrownian motion of whole chain (segmental movement). The dielectric loss peak in the region of b relaxation is mainly due to the movement of side groups or small units of main chains. The relative strength of the a and b dielectric relaxation depends on the degree of the orientation of dipolar groups through the limited mobility allowed by the b process before the more difficult, but more extensive, mobility for the a process comes into play. There is a partitioning of the total dipolar alignment among the molecular rearrangement processes. The mechanisms for the b process may depend on the nature of the dipolar group concerned and its position on the polymeric chain. Among the most important mechanisms are the following91,92: • Relaxation of a side group about a C–C chain, • Conformational flip of a cyclic unit involving the transition from one chain form to another, altering the orientation of a polar substituent, • Local motion of a segment of the main chain, since the small segment of a (CH2)n chain can have such motion without involving the rest of the chain. At lower temperatures, there is a g relaxation peak due mainly to the movement of small kinetic units of the main or the side chains, which consist of a sequence of several carbon atoms, such as the movement of several CH2 or CF2 groups. Another possible mechanism for the g relaxation is due to the crankshaft rotation95 below the glass transition temperature. The g relaxation process has been observed in polyethylene, aliphatic polyamides, polyester, and some polymethacrylates containing linear methylene chains in side branches.95 The presence in the polymeric chain of runs of three or more CH2 units, each of which is linked to immobile groups, would lead to the crankshaft rotation, thus resulting in g relaxation in various polymers.93,96 However, the available experimental evidence indicates that g relaxation due to crankshaft rotation is possible only in amor
111
phous polymers, or in amorphous regions of crystalline polymers, because crankshaft rotation can only occur about two collinear bonds. This condition is not fulfilled in crystalline regions, where the sequences of methylene groups form mainly transconformations. Relaxation processes at very low temperatures have a quantum nature.93 To study the dielectric relaxation processes, apart from the measurement of the thermally stimulated relaxation as a function of temperature, we need also the data from isothermal scans of the dielectric constant er and the loss factor e¢r as functions of frequency, so that the effective dipole moments and activation energies may be obtained. Typical results from such measurements for polyvinyl chloride in the a relaxation region are shown in Figure 242. The results are from Ishida.97 Such plots are sometimes referred to as dielectric spectra. From a series of such plots, the relaxation times can be determined for the individual relaxation processes as functions of temperature. The a relaxation peak at T = Tg of an amorphous polymer is much narrower than the b relaxation peak. Also, the temperature dependence of the a process is much steeper than that of the b process, indicating that a greater thermal activation energy is required for the motion. The a relaxation process near Tg is largely dependent on free volume. Molecular structure greatly affects the glass transition temperature and hence the dielectric relaxation times. Thus, a bulky side group would cause the Tg to decrease, thus preventing the chains from packing together tightly. Tg can also be deliberately reduced by doping a plasticizer into the polymer, such as diphenyl doped into polyvinyl chloride, which affects the a relaxation process because of the decrease of Tg.98 The effect of the degree of crystallinity on the dielectric properties of polymers has been extensively studied. The socalled crystalline polymers always consist of many fully crystalline and fully amorphous regions. So, the overall dielectric relaxation processes may be regarded as a superposition of the relaxation processes in fully crystalline and in fully amorphous regions in the polymer. Usually, the
112
Dielectric Phenomena in Solids 2.0
8
5° 1. 12 14° 1 8° 10
8°
5° 4. 11 8° 10
12
7 er
128° 125°
1.5
9
e¢r 1.0
10
6 5
.5°
4
10
1.
95
5°
95
1.
.5°
0.5
85°
5°
85°
3 0 2
3
4 5 logf (Hz)
6
2
3
(a)
4 5 logf (Hz)
6
(b)
Figure 242 (a) The dielectric constant er and (b) the loss factor e¢r as functions of frequency at temperatures in the a relaxation region for polyvinyl chloride.
amorphous regions make the major contribution to both er and e¢r. As a result, er and e¢r will decrease with an increasing degree of crystallinity. Such a dependence of the dielectric properties on the degree of crystallinity is usually observed at temperatures higher than Tg of the amorphous regions. When the temperature is lowered further to the level at which t becomes so large that wt >> 1, then the dielectric constant becomes dominated by er•. Since the value of er• for a number of nonpolar (e.g., polyethylene and polytetrafluoroethylene) and polar (e.g., polyamids) polymers differs little, at very low temperatures, the dielectric constants of these polymers are almost identical. Thus, when the relaxation spectra are frozen at low temperatures, the difference between nonpolar and polar polymers will disappear— at least, as far as the value of er is concerned. This phenomenon has been experimentally observed.93 Polymers may exist with linear, branched, and crosslinked chain structures. Linear polymers usually have long chains composed of a large number of repeating units, such as polyethylene and polytetrafluoroethylene. Branched polymers have side chains attached to the main chain, such as polymethyl methacrylate. Crosslinked polymers have a threedimensional
space network formed by chemical bonds. They are sometimes called the network polymers. There are many ways to cause the formation of a crosslinked network. Polyethylene undergoes crosslinking under the action of ionizing radiation. Crosslinking can greatly restrict certain kinds of molecular movement and hence can affect the dielectric relaxation processes. In general, dielectric losses will diminish with an increasing degree of crosslinking. This tendency appears more prominently in the region of the transition from the glassy to the rubbery state. Thus, as the degree of crosslinking increases, the magnitude of the principal a relaxation peak decreases. Obviously, the incorporation of any impurities into the polymer in order to modify the dielectric properties will also affect the relaxation processes and hence the values of er and e¢r. Examples include plasticizer to lower the glass transition temperature and polar impurities to increase the dielectric relaxation for nonpolar polymers.
References 1.
L. Brillouin, Wave Propagation in Periodic Structures, (Dover, New York 1953). 2. J.A. Stratton, Electromagnetic Theory, (McGrawHill, New York, 1941), p. 113.
Electric Polarization and Relaxation
3. 4. 5. 6. 7. 8. 9.
10. 11. 12. 13. 14.
15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26.
K.C. Kao, Brit. J. Appl. Phys., 12, 629 (1961). W.R. Smythe, Static and Dynamic Electricity, (McGrawHill, New York, 1950). J.H. Jeans, The Mathematical Theory of Electricity and Magnetism, (Cambridge University Press, Cambridge, 1925). C.J.F. Böttcher, Theory of Electric Polarization, (Elsevier, Amsterdam, 1978). R. Cooper and A.A. Wallace, proc. Phys. Soc., B66, 1113 (1953). K.H. Stark and C.G. Garton, Nature, 176, 1225 (1955). K.C. Kao, “The Bubble Theory for Electrical Breakdown of Liquid Dielectrics,” A.I.E.E. Conference Paper No. CP 60–84 (American Institute of Electrical Engineers, New York, January 1960). K.C. Kao, Nature, 208, 279 (1965). C.G. Garton and Z. Krasucki, Proc. Royal Soc. (London), 208A, 211 (1964). K.C. Kao and J.B. Higham, J. Electrochem. Soc., 108, 522 (1961). H.A. Pohl, Dielectrophoresis, (Cambridge University Press, Cambridge, (1978), and J. Appl. Phys., 29, 1182 (1958). R.H. Cole, “Theories of Dielectric Polarization and Relaxation”, in Progress in Dielectrics, Vol. 3, (Heywood, London, 1961) pp. 47–100. R.E. Teachout and R.T. Pack, Atomic Data, 3, 195 (1971). A.K. Jonscher, Dielectric Relaxation in Solids, (Chelsea Dielectric Press, London, 1983). R. Coelho, Physics of Dielectrics, (Elsevier, Amsterdam, 1979). J.H. van Vleck, Theory of Electric and Magnetic Polarizabilities, (Oxford Univeristy Press, Oxford, 1932), p. 203. N.F. Mott and I.N. Sneddon, Wave Mechanics and Its Applications, (Clarendon, Oxford, 1948), p. 166. A.J. Dekker, Electrical Engineering Materials, (Prentice Hall, Englewood Cliffs, NJ, 1961). A.J. Dekker, Solid State Physics, (MacMillan, London, 1963). I. Pirenne and E. Kartheuser, Physica, 20, 2005 (1964). M. Born and K. Huang, Dynamical Theory of Crystal Lattices, (Clarendon, Oxford, 1954). B.K.P. Scaife, Principles of Dielectrics, (Clarendon, Oxford, 1984). R.J.W. LeFevre, Dipole Moments, (Methuen, London, 1953). C.P. Smyth, Dielectric Behavior and Structure, (McGrawHill, New York, 1955).
27. 28. 29. 30. 31. 32. 33. 34.
35. 36. 37. 38. 39.
40. 41. 42. 43. 44. 45. 46. 47. 48.
49. 50. 51.
113
A.R. Von Hippel, Dielectrics and Waves, (John Wiley and Sons, New York, 1954). H. Frohlich, Theory of Dielectrics, (Clarendon, Oxford, 1958). P. Langevin, J. Physique, 4, 678 (1905); Ann. Chim. Phys., 5, 70 (1905). P. Debye, Physik Zeit., 13, 97 (1912). P. Debye, Polar Molecules, (Dover, New York, 1945). C.P. Smyth and C.S. Hitchcock, J. Amer. Chem. Soc., 55, 1290 (1933). C.P. Smyth and C.S. Hitchcock, J. Amer. Chem. Soc., 56, 1084 (1934). N.E. Hill, “Theoretical Treatment of Permittivity and Loss” in Dielectric Properties and Molecular Behaviour, Ed. N.E. Hill, W.E. Vaughan, A.H. Price, and M. Davies (Van Norstrand Reinhold, London, 1969). J.C. Slater, Insulators, Semiconductors and Metals, (McGrawHill, New York, 1955). F.C. Nix and W. Shockley, Rev. Mod. Phys., 10, 1 (1938). N.F. Mott and E.A. Davis, Electronic Processes in NonCrystalline Materials, (Clarendon, Oxford, 1974). L. Onsager, J. Am. Chem. Soc., 58, 1486 (1936). N.G. McCrum, B.E. Read, and G. Williams, Anelastic and Dielectric Effects in Polymeric Solids, (John Wiley and Sons, New York, 1967). J.G. Kirkwood, J. Chem. Phys., 7, 911 (1939). F.E. Harris and B.J. Adler, J. Chem. Phys., 21, 1031 (1952). H. Frohlich, Physica, 22, 898 (1956). J.J. O’Dwyer, J. Chem. Phys., 26, 878 (1957). B.K.P. Scaife, Proc. Phys. Soc. (London), B70, 314 (1957). A.D. Buckingham, Proc. Roy. Soc. (London), A238, 235 (1956); also, Trans. Faraday Soc., 52, 1035 and 1551 (1956). R.H. Cole, J. Chem. Phys., 27, 33 (1957). G.P. Mikhailov, in Physics of NonCrystalline Solids, (North Holland, Amsterdam, 1965), p. 270. H.A. Kramers, Atti del Congresso Internazionali dei Fisici, Como 2, 545 (1927), Collected Sci. Papers, (North Holland, Amsterdam, 1956), p. 333. R. de L. Kronig, J. Optical Society of America, 12, 547 (1926). P. Debye and W. Ramm, Annalen der Physik, 28, 28 (1937). P. Debye, The Collected Papers of Peter J.W. Debye, (Wiley Interscience, New York, 1954).
114
Dielectric Phenomena in Solids
52.
R.H. Cole and K.S. Cole, J. Chem. Phys., 9, 341 (1941); ibid., 10, 98 (1942). D.W. Davidson and R.H. Cole, J. Chem. Phys., 18, 1417 (1950); ibid., 19, 1484 (1951). S. Havriliak and S. Negami, J. Polymer Sci., Pt. C. 14, 99 (1966); also, Polymers, 8, 161 (1967). A.M. Rad and P. Bordewijk, Rec. Trav. Chim., 90, 1055 (1971). R.M. Fuoss and J.G. Kirkwood, J. Amer. Chem. Soc., 63, 385 (1941). R.H. Cole and P.M. Cross, Rev. Sci. Instru., 20, 252 (1949). R.H. Cole, J. Chem. Phy., 23, 493 (1955). B.E. Read and G. Williams, Polmyers, 2, 239 (1961); also, Trans. Faraday Soc., 57, 1979 (1961). A. Schallamach, Trans. Faraday Soc., 42A, 495 (1946). C. Herring, Bell System Tech, J., 34, 237 (1955). E.M. Conwell, High Field Transport in Semiconductors, (Academic Press, New York, 1967). E.M. Conwell, V.J. Fowler, and J. Zucker, Report on Contract AF19 (604)–5714 (Air Force Cambridge Res. Center, Cambridge, Massachusetts, 1960). A.F. Gibson, J.W. Granville, and E.G.S. Paige, J. Phys. Chem. Solids, 19, 198 (1961). S. Triebwasser, IBM J. Res. Develop., 2, 212 (1958); also, Phys. Rev., 118, 100 (1960). H. Baumpartner, Helv. Phys. Acta, 23, 651 (1950); ibid., 24, 326 (1951). E. Fatusso and W.J. Merz, Ferroelectricity, (North Holland, Amsterdam, 1967). S. Ratnowsky, Vorhandl deut Physik. Ges., 15, 497 (1913). J. Herweg, Z. Physik, 3, 36 (1920). J. Herweg and W. Potzsch, Z. Physik, 8, 1 (1922). J. Malsch, Physik Z., 29, 710 (1928). G.P. Jones and M. Gregson, Total Dielectric Saturation Observed in a Dipolar Solution, Chem. Phys. Lett., 4, 13 (1969). J.H. van Vleck, J. Chem. Phys., 5, 556 (1937). A.D. Buckingham, J. Chem. Phys., 25, 428 (1956). J.J. O’Dwyer, Proc. Phys. Soc. (London), A64, 1125 (1951).
53. 54. 55. 56. 57. 58. 59. 60. 61. 62. 63.
64. 65. 66. 67. 68. 69. 70. 71. 72. 73. 74. 75.
76. 77. 78.
79. 80. 81. 82. 83. 84. 85. 86. 87.
88. 89. 90. 91. 92. 93. 94. 95.
96. 97. 98.
A. Anselm, Acta Physicochim, U.S.S.R., 19, 400 (1944). J.B. Hasted, D.M. Ritson, and C.H. Collie, J. Chem. Phys., 16, 11 (1948). S. Lielich, in Dielectric and Related Molecular Processes, Vol. 1, (The Chemical Society, Burlington House, London, 1972), (1972). G.P. Jones, ibid., Vol. 2 (1975). G. Williams, Polymers, 4, 27 (1963). M.F. Manning and M.E. Bell, Rev. Mod. Phys., 12, 215 (1940). B.V. Hamon, Proc. IEE, (London), 99, 151 (1952), and also Austral. J. Phys., 6, 304 (1953). G. Williams, Trans. Faraday Soc., 58, 1041 (1962); ibid., 59, 1397 (1963). P.J. Hyde, Proc. IEE. (London), 117, 1891 (1970). A. Suggett, in Dielectric and Related Molecular Processes, Vol. 1 (Chemical Society, London, 1972), p. 100. D.R. Uhlmann and R.M. Hakim, J. Phys. Chem. Solids, 32, 2652 (1971). N.E. Hill, W.E. Vaughan, A.H. Price, and M. Davies (Eds.), Dielectric Properties and Molecular Behaviour, (Van Nostrand Reinhold, London, 1969). A.M. North, Chem. Soc. Rev., 1, 49 (1972). P. Hedvig, Dielectric Spectroscopy of Polymers, (Adam Hilger, Bristol, 1977). P.E. Karasz (Ed.), Dielectric Properties of Polymers, (Plenum, New York, 1972). A.R. Blythe, Electrical Properties of Polymers, (Cambridge Universtiy Press, Cambridge, 1979). I.I. Perepechko, An Introduction to Polymer Physics, (Mir Publisher, Moscow, 1981), English Translation by A. Beknazarov). I.I. Perepechko, Low Temperature Properties of Polymers, (Mir Publisher, Moscow, and Pergamon Press, Oxford, 1980). P. Bräunlich, Thermally Stimulated Relaxation in Solids, (SpringerVerlag, Berlin, 1979). T.F. Schatzki, J. Poly. Sci., 57, 496 (1962); also, Meeting of Am. Chem. Soc. Div. Polymer Chem., Atlantic City, September 1965, Polymer Preprints, 6, 646 (1965). B.J. Wunderlich, J. Chem. Phys., 7, 10 and 2429 (1962). Y. Ishida, Kolloid. Z., 168, 29 (1960). R.M. Fuoss, J. Am. Chem. Soc., 63, 378 (1941).
3 Optical and ElectroOptic Processes We can conceive darkness without thought of light, but we cannot conceive light without thought of darkness. Christopher Morley
Optical and electrooptic processes are mainly associated with the interaction of light with matter. Light is simply energy and energy is intangible, being apprehended only on its interaction with matter, which acts as an origin or as a detector of energy. In this chapter, we shall discuss such interaction processes.
3.1
3.1.1 Corpuscular Theory The Outstanding Differences between Photons and Electrons or Protons There are several significant differences between photons and electrons or protons.1 • Photons may be created and annihilated, whereas electrons or protons are conserved. • Photons do not interact with each other, and they obey Bose–Einstein statistics; electrons or protons do interact with each other and obey Fermi–Dirac statistics. • Photons do not have electrostatic charges, spin moments, or rest mass; these are possessed by electrons or protons. • All photons have a common constant velocity c in free space (constant velocity v = c/n in materials), whereas the velocities of electrons or protons are variable, depending on the accelerating voltage. • Photons have diffraction wavelength ld equal to their radiation (conversion) wavelength lE, whereas electrons or protons have ld • V 1/2 but lE • V 1, where V is the accelerating voltage. • Photons have momentum p and kinetic energy Ek, depending on their frequency, whereas electrons or protons have momentum and kinetic energy, depending on their velocity.
Nature of Light
Optical radiation is electromagnetic radiation covering a wide range of wavelengths, as was shown in Figure 121. As mentioned in Electromagnetic Waves and Fields in Chapter 1, light can be described by corpuscular theory or by wave theory. The two theories are not in conflict but complementary. According to quantum mechanics, radiation is absorbed or emitted as particles, called photons, having discrete values of energy in quanta. Thus, photon energy can be written as E = hu =
hc l
(31)
where h is the Planck constant, c is the speed of light, and u and l are, respectively, the frequency and the wavelength. Energy is itself intangible; it can be apprehended only through its interaction with matter. The interaction of light with solids may produce diffraction or photoelectricity, leading to the concept of radiant energy, which can be described in terms of photons or quanta. Light, like matter, is composed of infinitesimal particles whose probable behaviors are describable by wave equations similar to those used for describing other waves. So, light is energy and apparently has a dual nature.
Frequency, Energy, and Momentum of Photons On the basis of Einstein’s relativistic mechanics, the relation between mass m and energy E, and momentum p of a particle can be expressed as 115
116
Dielectric Phenomena in Solids
E = mc 2 = p = mv =
mo c 2 (1  v 2 c 2 )1 2
mo v (1  v 2 c 2 )1 2
(33)
in which mo is the rest mass of the particle, and m is the mass of the particle when it is moving at a velocity v. If v << c, Equation 32 can be simplified to E = mo c 2 +
1 1 mo v 2 = Eo + mo v 2 2 2
(34)
2
of which Eo = mc is the rest mass energy and 1 mo v 2 is the kinetic energy of the particle. 2 For photons, we have the following relation based on Equations 32 through 34: E 2 = mo2 c 2 + c 2 p2
v=
(32)
(35)
Since the photon has no mass, so mo = 0, the momentum of a photon is E = cp
c n
(39)
where n is the refractive index of the medium, which is given by n = (ure r )1 2
(310)
and ur = u uo er = e eo
where eo and e are, respectively, the permittivities of free space and the medium, and uo and u are, respectively, the permeabilities of free space and the medium. In describing optical phenomena, we usually deal with the electric field vector, because the magnetic field vector behaves in the same way as the electric field vector. In a onedimensional case, Equation 37 can be written as ∂ 2F 1 ∂ 2F = ∂ x 2 c2 ∂ t 2
(311)
The solution of the above equation is
or p=
F( x, t ) = Fo cos(w t  kx + f )
E h = c l
(36)
It can be imagined that a particle like a photon, whose rest mass is extremely small (m Æ 0) and whose velocity is extremely large (v Æ c), will have a finite momentum and energy. 3.1.2 Wave Theory Light as an electromagnetic wave can be characterized by Maxwell’s wave equation 2
—2 F =
1 ∂ F c2 ∂ t 2
(37)
—2 H =
1 ∂ 2H c2 ∂ t 2
(38)
where F and H are, respectively, the electric and magnetic fields. F and H are transverse waves, as shown in Figure 120. In free space, the waves propagate at a speed of light c. In other material media, the propagation speed is given by
(312)
where k = wave vector =
2p (the wave number l
usually used is l1) f = phase T = one period of the time for one cycle = 1 2p = v w Figure 31 illustrates the variation of F with the traveling distance x and the time t. Wavefronts or wavesurfaces are the surfaces with a constant phase, implying that on the wavefronts, F is a constant magnitude. This means w t  kx + f = constant
(313)
This leads to dx w = = vl = c dt k
which is called the phase velocity.
(314)
Optical and ElectroOptic Processes F
l
tan f =
Fo cos(w t + f)
Fo 0
x
wt + f k
(a) F Fo cosf
Fo 0
t
T
(b) Figure 31 The variation of the electric field vector F with distance in xdirection and time t. (a) F as a function of x at a fixed value of t (say t = 0) and (b) F as a function of t at a fixed value of x (say x = 0).
F10 sin f1 + F20 sin f 2 F10 cos f1 + F20 cos f 2
117
(320)
Equation 318 implies that the resultant of two sinusoidal waves of the same frequency is itself a sinusoidal wave with the same frequency as the original waves. In general, it is not possible in practice to produce perfectly monochromatic light. Usually, light consists of a group of waves of closely similar wavelength, moving in the form of a packet. To illustrate the concept of the wave packet, we use two waves, for simplicity, to demonstrate how the two waves form a packet. Let the two waves be F1 = Fo cos(w t  kx )
(321)
F2 = Fo cos[(w + dw )t  ( k + dk ) x ]
(322)
Based on the principle of superposition, these two waves can be added to form a resultant wave. This resultant wave is F = F1 + F2 = 2 Fo cos[(w + dw 2)t
(323)
 ( k + dk 2) x ]cos(dw t 2  dkx 2)
Principle of Superposition According to the principle of superposition, two or more waves can be added to form a resultant wave. For example, by adding two waves of the same frequency, but with different amplitudes and phases, such as F1 = F10 sin(w t  kx + f1 )
(315)
F2 = F20 sin(w t  kx + f 2 )
(316)
the resultant wave becomes F = F1 + F2 = ( F10 cos f1 + F20 cos f 2 )sin(w t  kx ) + ( F10 sin f1 + F20 sin f 2 )cos(w t  kx )
(317) which can be written in the form F = Fo sin(w t  kx + f )
(318)
Fo2 = F102 + F202 + 2 F10 F20 cos(f1  f 2 )
(319)
with
As we assume dw << w and dk << k, Equation 323 can be simplified to F = 2 Fo cos(dw t 2  d kx 2)cos(w t  kx ) = Fo¢ cos(w t  kx )
(324)
This is the wave of the same form as the original waves, but it has the amplitude Fo¢ = 2 Fo cos(dw t 2  d kx 2)
(325)
It is also a traveling wave. However, it can be seen from Equation 325 that there are maxima (antinodes) occurring at dwt/2  dkx/2 = mp with m = 0, 1, 2, 3, . . . and minima (nodes) at p dw t 2  d kx 2 = m ¢ with m¢ = 1, 3, 5, 7, . . . . 2 These maxima and minima are generally referred to as the beats. The propagation velocity of a specific beat is the signal velocity or group velocity vg of the modulated wave. Thus, by setting dwt/2  dkx/2 = constant (the plane of constant amplitude), we obtain
118
Dielectric Phenomena in Solids
vg =
dx dw = dt dk
and most light detectors are not sensitive to electric field or magnetic field vectors; they are sensitive to the power density of light, which is the flow of energy per unit time per unit area and is generally referred to as the irradiance I. I is, in fact, the Poynting vector. For the present case, the irradiance Ir can be written as
(326)
Figure 32 illustrates this phenomenon of beats. From Equations 39 and 314, using v instead of c for phase velocity for general cases because in solids v = c/n, we can write (327)
w = kul = kv
Ir = FH • F 2 •
and obtain the group velocity in the form vg =
d ( kv) dv = vl dk dl
(328)
A cos(w t  kr ) r
I = Fo2 = F102 + F202 + 2 F10 F20 cos(f1  f 2 )
(331) If E10 = E20, then I becomes
(329)
I = 2 F102 [1 + cos(f1  f 2 )]
where A is the strength of the light source and r is the distance from the light source. Equation 329 implies that the amplitude of the electric field vector F is proportional to r1. Human eyes
= 4 F102 cos2 [(f1  f 2 ) 2]
Fo cosw t
+
t
(332)
It can be seen that as (f1  f2)/2 varies from 0 2 to p, I will vary from 4F 10 to zero and then from
Fo cos(w + Dw)t
0
(330)
Interference and Interferometry When two or more waves with different amplitudes and phases are mixed, they will interfere with each other. For example, when two waves, such as those given by Equations 315 and 316, are mixed, the resultant wave is given by Equation 318, with Fo given by Equation 319. In this case, the resultant irradiance can be written as
Group velocity and phase velocity are identical only in media in which the propagation velocity is independent of frequency, that is, the wave propagation in nondispersive dielectric media. Note that in most cases, the light source is a point source of light radiating in all directions. The wavefronts are then a series of concentric spherical shells. So, the electric field vector is given by F=
1 r2
0
t
2Fo coswt cosDwt /2
2Fo cosDwt /2
t 0
p Dw
3p Dw
Figure 32 Schematic diagrams showing the beats produced by two waves of slightly different frequencies for x = 0.
Optical and ElectroOptic Processes 2 zero to 4F 10 . If F10 π F20, then I varies between 2 (F10 + F20) and (F10  F20)2, as (f1  f2) varies between 0 and p. In general, interference produces the socalled interference fringes, which are the variation of the resultant amplitude and hence the relative energy and illumination (or brightness) from point to point in the field of view. They are mainly caused by the different paths between the interfering beams of light. The conditions for the occurrence of interference are as follows:
• The sources of light must be coherent. This means that the waves emanating from the sources, while they need not be exactly in phase, must keep their phase relationship unaltered during the period of interference. • The amplitudes of two wavefronts must be similar. • The wavelengths of the light from the sources must be the same. • The ways for obtaining interference in accordance with the above conditions can be divided into two groups: division of wavefront and division of amplitude.2,3 Division of Wavefront
The earliest experiment about interference caused by the division of wavefront was performed by Thomas Young in 1802.4 The experiment basically involves two slits S1 and S2 with a separation d between them, and light from a monochromatic source A illuminating a narrow slit S, which then acts as a light source to illuminate simultaneously S1 and S2, as shown in Figure 33. Then the two narrow beams of light of different cylindrical wavefronts from S1 and S2 will fall upon the screen B. Generally, the narrower the slit as compared with d, the greater the illuminated area, because of diffraction at the slits. The distances D1 and D2 determine the phase difference f1  f2 between the two waves. Thus, the phase difference between the two waves on the screen can be written as f1  f 2 =
2p ( D1  D2 ) l
(333)
119
B (Screen) p D1 y S A
d
S1 S2
q
x
q
D2 O
S¢2
D Figure 33 Schematic diagram showing the basic arrangement of Young’s doubleslit experiment on interference.
Obviously, at point O on the screen, D1 = D2, both light waves from S1 and S2, are exactly in phase (i.e., f1  f2 = 0); bright fringe will appear at point 0 on the screen. When x = l/2, as shown in Figure 33, the two waves will be exactly out of phase and tend to cancel each other, so there will be no light (i.e., there will be darkness) at point p on the screen. Bright fringes occur when f1  f2 = ±2mp, that is, when D1  D2 = ml, and the dark fringes occur when f1  f2 = (2 m + 1)l ±(2m + 1)p, or when D1  D2 = ± , 2 where m is any integer, 0, 1, 2, 3, . . . . To find a point on the screen at a distance y from point 0, we assume that both d and y are much smaller than D. For this case, bright fringes occur at the points p located at a distance y from point 0 when y = ±2mlD/d.5 Similarly, dark fringes occur for the points at y = ±(2m + 1)lD/d. Division of Amplitude
The various colors appearing in a soap bubble, or those reflected from the oil film on the top surface of a pool of water, are examples of interference encountered daily. This phenomenon is due to the interference caused by the division of amplitude. The simplest example of interference caused by the division of amplitude is the interference from a thin film of refractive index n2 deposited on a substrate of refractive index n3. This system is placed in a medium of refractive index n1 (usually in air with n1 = 1), as shown in Figure
120
Dielectric Phenomena in Solids
34. The beams emerging from A and B at the interface between the medium and the film are parallel; a lens is therefore required to bring them together to produce interference. The beam from A is due directly to the reflection of the incident beam, while the beam from B is due to the reflection of the refracted beam on the rear surface of the film. For simplicity, we choose n1 = 1. The difference in optical path between the beam from B and that from A is given by3 Ldiff = n2 ( AD + DB)  AC
(334)
= 2 n2 AD  AC
Using Snell’s law, n1sinq1 = n2sinq2, we obtain AC = 2 AD sin q 2 sin q1
(335)
= 2 n2 AD sin 2 q 2
Substituting Equation 335 into Equation 334, we obtain Ldiff = 2 n2 d cos2 q 2
(336)
So, bright fringes occur when 4p n2 d cos q 2 = 2 mp l
(337)
or 2 n2 d cosq 2 = ml
and dark fringes occur when 4p n2 d cos q 2 (2 m + 1) = p l 2 Interference pattern appearing on the focal plane C
q1
2 n2 d cosq 2 =
(2 m + 1) l 2
q2 q2
Nonreflecting Surface—It is possible to deposit or to insert a thin dielectric layer on the surface of any object, when reflection of the incident wave is not desired. Such a thin layer or thin film, as shown in Figure 35, is sometimes called an antireflection coating. The incident wave reflected from the interface between the film and the medium (usually the air with n1 = 1), called wave A, and the wave reflected from the interface between the film and the object of refractive index n3, called wave B, will interfere with each other. In order to make them to interfere destructively, the optical thickness of the thin film must be equal to l/4, so that the optical path difference between wave A and wave B is equal to l/2, or their phase difference equal to p. To satisfy this condition, the following relation, based on Fresnel’s reflection equation, must be satisfied3:
Incident Wave
Lens
D
n1
B n2
(338)
where m is any integer, 0, 1, 2, 3, . . . . Applying the same principle of analysis for two beams, it is quite straightforward to extend the case for two beams to the cases for multiple beams. Multiple beams will produce interference caused either by the division of wavefront or by the division of amplitude. For more details about this subject, the reader is referred to two very good references.3,4 Many applications are derived from the interference phenomenon. Here, we just mention a few examples.
n1
A d
or
n2 (Thin Film)
d
n3
n3 Transmitted Wave
Figure 34 Schematic diagram showing the interference caused by the division of amplitude due to beams of light emerging from a thin film of refractive index n2 with n2 > n1.
Figure 35 Nonreflecting surface produced by insertion of a dielectric film with thickness d = l/4 and refractive index n2 = (n1n3)1/2.
Optical and ElectroOptic Processes
n2  n1 n3  n2 = n2 + n1 n3 + n2
(339)
LP A
This leads to n2 = (n1n3 )1 2
121
(340)
F
Appreciable reduction in the reflected irradiance has been found with films of magnesium fluoride or cryolite on the glass surface. Interferometers—The various types of interferometers may be divided into two main groups based on their operational principles:
• On the basis of the division of wavefront by means of a number of apertures similar to that used in Young’s experiment, or by means of prisms and mirrors. • On the basis of the division of amplitude by means of semireflecting surfaces, part of the light being reflected and part being transmitted. The classical Michelson interferometer belongs to this group. The basic principle of interferometers is to bring the reflected or transmitted beams together to produce bright and dark interference fringes. Based on the difference in the optical paths and the associated bright and dark interference fringes, it is possible to determine the distance between two points or the thickness of a thin film. The classical method for measuring the distance is the Michelson interferometer, and in fact, nearly all other interferometers are variations of this basic instrument.6–8 Because our aim is to show the basic principle of the interferometer, we have chosen a simple one, called the Fizeau interferometer, because the essential design of this instrument is originally due to Fizeau, but the arrangement shown in Figure 36 is based on a more recent development.9,10 In this instrument, light from a quasimonochromatic source Lp is collimated by the lens L and falls on the film T at nearly normal incidence. The light reflected from the top and bottom surfaces of the film returns through L and converges to an apparatus A, which produces the bright and dark interference fringes on the focal plane F. Usually, a black cloth is placed at the base S of the instrument
L
T S
Figure 36 The basic arrangement of the essential parts for the Fizeau interferometer.
to absorb the transmitted light. The bright and dark fringes appearing on the focal plane F provide the information about the optical thickness of the film. Diffraction If an opaque object is placed between a beam of light and a screen, the shadow cast on the screen is not perfectly sharp. Some light is also present in the dark zone. Similarly, a beam of light that emerges from a small aperture or a narrow slit is observed to spread out. In daily experience, we may have noticed that the beams of a car’s headlights are spread out by the mist on a foggy night; the mist is composed of water particles, which scatter the light beams. This phenomenon is called diffraction. If the particles are extremely small, such as atoms arranged in the lattice of a crystal, an
122
Dielectric Phenomena in Solids
incident beam striking the crystal will undergo Bragg diffraction. The arrangement of the atoms and the structure of the crystal can be determined by examining the angle and the intensity of the diffracted beams. Since the separation between atoms (lattice constant) is extremely small, the wavelength of the incident beam must be small. This is why xrays must be used. This is well known as xray diffraction spectroscopy. The basic theory of diffraction is that of Huygens and Fresnel, which is so far the most powerful and adequate theory for treating most problems encountered in optical instruments.11 Based on this theory, every point of a wavefront may be considered a center of a secondary disturbance which gives rise to many spherical wavelets spreading out in all directions. Secondary wavelets also mutually interfere with each other. The waves of such spherical wavelets from the center of the disturbance will be superposed to form a new wavefront. Because of the diffraction effect, images of any object through a lens or a microscope always have some defects, implying that the images always have some distortion in shape from the actual object. This may be caused by diffraction, aberration, or optical noise. Here, we will consider only the effect of diffraction. Let us take the resolution of a microscope as an example. Airy was the first to compute the diffracted image,12 showing in 1834 that for a diffraction at a circular aperture of diameter D, the angle a between the first maximum (measured from the center) and the first dark ring is given by sin a =
1.22l D
(341)
where l is the wavelength of the light. The maxima are separated by the minima, which occur at the angle of diffraction. For a circular aperture, the pattern would consist of a central bright area surrounded by concentric dark and bright rings. According to Airy, about 84% of the light is concentrated within the central spot, which is called the Airy or diffraction disk, as shown in Figure 37(a). For instance, when
A
D
B
S
L q L
a I x
Image of Object B I
Image of Object A x
(a)
(b)
Figure 37 (a) Diffraction at the aperture of a lens showing an Airy disk, and (b) the resolution limit of an optical microscope.
light from a lamp, through a small pinhole, falls on a cardboard sheet located at a distance of several meters, we can see a bright spot and also dark rings. The same kind of pattern can be observed when a pointed object is imaged by a microscope. Generally, a microscope is commonly used to determine the separation between two small objects. This is exactly what photolithography does in today’s microelectronic technology. In this case, we may have three possible resolutions: • The two objects produce an overlapping image, so we can see only one object through the microscope. • The two objects can be observed distinguishably, but their relative positions are not distinguished. • The two objects are clearly resolved. However, the demarcation between the “resolved” and the “not resolved” is not perfectly sharp. The Rayleigh criterion imposes the condition that the two objects can be clearly distinguished when the central maximum, created by object A, coincides with the first minimum created by the other object B, as shown in Figure 37(b). Thus, for a distinguishable image, the separa
tion S between the two objects should follow the criterion 1.22 2 n sinq
y
(342)
W av e
S=
where n is the refractive index of the medium. This means that for the two objects in the image are just resolved, S must be the value not smaller than that limited by Equation 342. The numerical aperture (NA) is given by
x H
NA = n sinq
So
F
F
S=
0.6l NA
123
Pr op ag at io n
Optical and ElectroOptic Processes
(343)
Thus, the higher the value of NA of a lens, the higher the quality of the lens. Based on this criterion, if the system is placed in dry air, n = 1, values of NA up to 0.95 have been used. However, if the system is immersed in oil, the value of NA can be higher than 1.45. Thus, for l = 5500A, the minimum value of S having good resolution is about 3.5 ¥ 105 cm in dry air and about 2.5 ¥ 105 cm in oil. So there is some advantage to placing the system in a medium having a high n and hence high NA. Polarization, Reflection, and Refraction Any beam of ordinary light comprises many individual waves, so the planes of the vibration of the electric field vectors are randomly oriented. Such a beam of light is unpolarized, and the resultant electric field vector changes its orientation randomly in time. A beam of light with its electric field vector vibrating only in a specific plane is referred to as planepolarized, as shown in Figure 38. The wave propagates in the z direction, while the electric field vector F vibrates in the x–z plane (i.e., y = 0) and the magnetic field vector H vibrates in the yz plane (i.e., x = 0). We have mentioned that in describing optical phenomena, we usually consider only the electric field vector F because the magnetic field vector H behaves in the same way as F. The simplest form of polarization is plane polarization. There are other forms of polarization. Suppose that we have two plane waves,
z
H
Figure 38 Planepolarized light wave with the electric field vector F vibrating in the x–z plane (y = 0) and the magnetic field vector H vibrating in the y–z plane (x = 0).
one with Fx vibrating in the xz plane and the other with Fy vibrating in the yz plane (see Figure 38), then we can write Fx = Fxo cosw t
(344)
Fy = Fyo cos(w t + q )
(345)
By eliminating wt and combining Equations 344 and 345, we obtain 2
2 Ê Fx ˆ  2 Fx Fy cosq + Ê Fy ˆ = sin 2 q Á ˜ Ë Fxo ¯ Ë Fyo ¯ Fxo Fyo
(346) There are three special cases. p First, if Fxo π Fyo and q = ± , then Equation 2 4.46 can be simplified to 2
2 Ê Fx ˆ + Ê Fy ˆ = 1 Ë Fxo ¯ ÁË Fyo ˜¯
(347)
This is an elliptically polarized wave. p Second, if Fxo = Fyo and q = ± , then 2 Equation 446 becomes Fx2 + Fy2 = Fxo2
(348)
This is a circularly polarized wave. Third, if Fxo π Fyo and q = ±p, then Equation 346 becomes
124
Dielectric Phenomena in Solids
Fy Fx + =0 Fxo Fyo
(349)
This is a linearly polarized wave. Of course, if q were different from 0, p/2, and p, the shapes of the polarized waves would be different from the three cases just mentioned. Polarizers
Certain sources provide polarized light without the use of polarizers, such as light from lasers and light from the blue sky, which is partially polarized. However, planepolarized light may be produced from unpolarized light in a number of ways. The earliest experiment to produce planepolarized light from ordinary, unpolarized light is due to Malus.3,14 He used two parallel, unsilvered mirrors, such as glass plates, as shown in Figure 39. The light is strongly reflected from G1. If mirror G2 is turned in such a direction to reflect most of the light out of the x–y plane, then mirror G1 makes the light strongly reflected in the x–y plane and not in the direction perpendicular to the x–y plane. In other
G2
G1 y x
Figure 39 Malus’s successive reflection experiement employing two parallel transparent mirrors G1 and G2.
words, the first mirror G1 polarizes the light, and the second mirror G2 reveals that it is polarized. An apparatus that can produce a beam of planepolarized light from a beam of unpolarized light is called a polarizer. This is similar to a filter, which allows only a narrow band of frequencies to pass through and filters out all other frequencies. An apparatus that can detect planepolarized light is called an analyzer. Generally, an apparatus capable of being a polarizer is also capable of being an analyzer, and vice versa. We shall consider two commonly used polarizers: one is by reflection and the other by transmission; both are based on the condition of no reflection at the Brewster angle. The former suffers a great loss of light, since only a fraction of the incident beam is reflected, while the latter does not give complete polarization, though a pile of glass plates is used.
Light Polarized by Reflection—When a beam of unpolarized light strikes the boundary between two media, the incident beam on the plane of incidence perpendicular to the boundary will be partly reflected and partly refracted, thus changing the direction of propagation, amplitude, and phase, as shown in Figure 310(a). The electric field vector F of the incident beam may be vibrating in any direction, such as along the rdirection but in the rr1 plane. However, F can be resolved into two components: one vibrating in the plane of incidence (i.e., parallel to the plane of incidence), termed Fp, and the other vibrating perpendicular to the plane of incidence (i.e., normal to the plane of incidence), termed Fn, as shown in Figure 310(b). The symbol used for Fp is —  and that for •••• . Thus, the symbol for an unpolarized Fn is — •••• beam, with F mixed with Fp and Fn, is —  . The normal reflection and refraction for an unpolarized light wave is shown in Figure 310(c). However, when the angle of incidence is equal to Brewster angle qB, (i.e., q1 = qB) if the incident beam is a normally planepolarized beam, the reflected beam and the refracted beam are both normally planepolarized, as shown in Figure 311(a). When the incident beam is parallel planepolarized, the incident
Optical and ElectroOptic Processes
Medium 1
125
r1 q1 q r1¢ 1
F
Fn
r
0
Medium 2
0
Plane of Incidence
q2
Fp
r2
(a)
(b)
q1 q1 n1 n2 q2
(c) Figure 310 Schematic diagrams showing (a) the plane of incidence and the angles of incidence q1, of reflection q1, and of refraction q2, (b) the normal component Fn and the parallel component Fp of the electric field vector F, and (c) the reflection and refraction of an unpolarized beam at any angle of incidence q1.
qB
qB
n1 n2 q2
(a)
(b)
(c)
Figure 311 The reflection and refraction for the incident beam striking the boundary between two media at the angle of incidence q1 = qB (Brewster angle): (a) for the normal planepolarized beam, (b) for the parallel planepolarized beam, and (c) for the unpolarized beam.
beam and the refracted beam are parallel planepolarized, but there is no reflected beam, as shown in Figure 311(b). For the incident unpolarized beam, the refracted beam is still partially unpolarized, but the reflected beam is highly planepolarized. In this case, the planepolarized reflected beam is polarized in the direction normal to the plane of incidence. Therefore, this method can be used to produce a normally planepolarized beam from an unpolarized beam.
From Figure 311, it can be seen that only for the incident beam parallel planepolarized at q1 = qB, there is no reflection. When q1 = qB, then q2 = p 2  q B
(350)
Based on Snell’s law, n1 sin q1 = n2 sin q 2
(351)
so from Equations 350 and 351, qB can be expressed as
Dielectric Phenomena in Solids
q B = tan 1 (n2 n1 )
(352)
If medium 1 is air, n1 = 1, and medium 2 is glass, n2 = 1.5, then qB = 56.3°. For the reverse case— medium 1 is glass and medium 2 is air—then qB = 33.7°. At this critical angle qB, the reflectance from the boundary is equal to zero for parallel planepolarized light.15,16 No reflection occurs, because the electric field vector Fp in medium 2 sets the atomic electrons into oscillation. This oscillation of atomic electrons acts like that of Hertian oscillators, which radiate energy only in the direction perpendicular to the direction of the oscillation but radiate no energy in the direction of the oscillation. That is why there is no reflection in medium 1 in the direction parallel to the direction of the oscillation of the atomic electrons in medium 2. The reflectance, which is defined as the ratio of the reflected to the incident energy, is given by Rp =
( F1rp )2 ( F1i p )2
(353)
for a parallel planepolarized wave, and Rn =
( F1rn )2 ( F1in )2
(355)
where n is the refractive index and k is the absorption index or the extinction coefficient, which represents the attenuation of the wave per unit wavelength. The calculation for the reflectance in general is quite mathematically involved. For the simple case, assuming that medium 1 is a transparent material with n*1 = n1 and k1 = 0, and medium 2 is an absorbing material with n*2 = n2  jk2, then the reflectance can be expressed as17 Rp =
Rn =
(n22 + k22 )  2 n1n2 cosq1 + n12 cos2 q1 (n22 + k22 ) + 2 n1n2 cosq1 + n12 cos2 q1
(357) Only for normal incidence (i.e., q1 = 0), Rp = Rn. Otherwise, Rp and Rn are different. The reflectance as a function of the angle of incidence is shown in Figure 312. It can be seen that only for Rp there is a Brewster angle qB, at which Rp = 0. Light Polarized by Transmission—Figure 311(c) shows that some of the light polarized normal to the plane of incidence is reflected; all of the light parallel planepolarized is transmitted to medium 2. If a pile of glass plates is used for this polarizing process, it is possible to filter out the light normally planepolarized, leaving the portion parallel planepolarized to pass through, as shown in Figure 313. After passing through a pile of glass plates, the transmitted light becomes a highly planepolarized light, but in this case, the light is polarized parallel to the plane of incidence.
(354)
for a normally planepolarized wave. Both Rp and Rn depend on the angle of incidence q1 and on the optical constants of the medium. In general, the optical constants should be expressed in complex form because of the dispersion of the material. The complex refractive index is given by n* = n  jk
and
(n22 + k22 )cos2 q1  2 n1n2 cosq1 + n12 (n22 + k22 )cos2 q1 + 2 n1n2 cosq1 + n12
(356)
1.0 0.9 0.8 0.7 Reflectance
126
0.6 0.5 0.4 0.3 Rn 0.2 0.1
Rp 0
10
20
30 40 50
60 70
80
90
Angle of Incidence (degrees) Figure 312 Reflectance as a function of angle of incidence for the lightpolarized parallel (Rp) and normal (Rn) to the plane of incidence for the light reflected from water surface.
Optical and ElectroOptic Processes
Unpolarized Beam
qB
Glass Plate
Polarized Beam
Figure 313 Polarization by transmission through a pile of glass plates with the incident unpolarized beam striking the surface of the first glass plate at the Brewster angle.
Total Internal Reflection
Based on Snell’s law, it is possible to make the angle of refraction q2 = p/2 by changing the angle of incidence to a critical angle termed qc. For this to occur, n1 must be larger than n2, (i.e., n1 > n2). So, when a light beam in medium 1 strikes the surface of medium 2, which is a less dense medium, at the critical angle qc, which is q c = sin 1 (n2 n1 )
(358)
then the incident beam will be totally reflected. Usually, the incident beam is not reflected at the striking point on the boundary surface, but penetrates some distance into medium 2 before it is reflected. The reflecting surface of the reflected beam is displaced slightly behind the real reflecting surface. This is known as the Goos–Hanchen effect.18 The total internal reflection is important in optical fiber waveguides. Dispersion
A pulse or signal of any electromagnetic waves may be constructed to form wave packets by superposition of all harmonic waves covering a frequency interval with prescribed amplitudes. The velocities, with which the constant phase surface of these component waves are propagated, depend on the parameters e (permittivity), m (permeability), and s (conductivity) of the medium. If the medium is nonconducting and e and m are independent of the frequency of the waves, then the phase velocity is constant and the signal is propagated
127
without distortion. Such a medium is not dispersive. On the other hand, if the medium is conducting, then the propagating harmonic waves suffer attenuation, relative displacements in phase in the direction of propagation, and the signal arrives at a distant point in a distorted form. Such a medium, in which the phase velocity is frequencydependent, is dispersive. At optical frequencies, a material may exhibit this dispersive phenomenon even when the conductivity due to free charges is totally negligible. In nonmagnetic dielectric materials, the phase velocity is related to the refractive index n = (er)1/2. Strictly speaking, however, there is no material free of dielectric losses; therefore, there is no material completely free of dispersion. Dispersion is an intrinsic property of all dielectric materials, and all other properties must coexist with it. So, the refractive index must be in complex form, as given by Equation 355. A dielectric solid may be considered an assembly of oscillators (each atom or molecule is an oscillator) set into forced vibration by the excitation force or by the radiation of optical frequencies. Under an applied electric field or the electricfield vector of the incident electromagnetic wave of radiation, the bound electrons (or ions) will be displaced from their equilibrium positions, giving rise to polarization. These bound electrons (or ions) will also experience a restoring force proportional to the displacement Dx and a damping force proportional to the velocity d(Dx)/dt. Thus, the motion of an electron (or an ion) is governed by the following equation m
d 2 Dx dDx + mG + mw o2 Dx = qFx exp( jw t ) dt 2 dt
(359) where m is the mass of the electron (or the ion), wo is the natural frequency of the oscillator, G is the force constant, and Fx exp( jwt) is the excitation field in the x direction. The solution of Equation 359 is Dx =
qFx m[(w 2  w o2 ) + jGw ]
(360)
Thus, we have the complex relative permittivity (or dielectric constant)
128
Dielectric Phenomena in Solids
e r* = 1 + = 1+
N ( qDx ) e o Fx Nq Ï qFx ¸ Ì ˝ e o Fx Ó m[(w 2  w o2 ) + jGw ] ˛
(361)
Thus, we can write e r* = e r  je r¢ = (n  jk )2 = (n 2  k 2 )  j 2 nk
(362) This is the dispersion equation. It implies that any light beam passing through a dielectric medium will suffer attenuation and hence dispersion. More details about this topic will be given in Section 3.3.4.
3.2
Modulation of Light
If optical beams are used as information carriers, then transmission of the information requires the optical beams to be modulated. This process of placing information onto an information carrier is referred to as modulation, and the converse process is referred to as demodulation (the recovery of the information). Optical beams can be modulated by varying one or more of the wave parameters: frequency, amplitude, phase, polarization, and propagation direction. Frequency, amplitude, and phase modulations are well known in radio and microwave communications. Polarization and propagation direction are related to the variation of the refractive index. In this section, we shall discuss several important effects that lead to the modulation of light. 3.2.1 Double Refraction and Birefringence In Section 3.1.2, we mentioned that the superposition of two waves, one with the electric field vector vibrating in the x direction and the other vibrating in the y direction, will produce elliptical, circular, or linear polarizations, depending on the relative values in amplitude and phase of the two waves. There are some materials in which the refractive index for light linearly polarized in one direction (e.g., in the x direction) is different from that for the light linearly polarized in another (e.g., in the y
direction). This implies that such materials are anisotropic and that the light with the electric vector in one direction travels faster than that in another. Some materials consist of nonspherical, long molecules, and these molecules may be arranged with their long axes parallel to each other. Because of the structure of the molecules, it is possible that the electrons respond more easily to the electric field oscillation in the direction parallel to the long axes of the molecules than they would respond to the electric field perpendicular to these axes. Such materials, which have double refractive indices, are said to be birefringent. If a light beam is incident normally on such birefringent materials, the beam will be split in two upon refraction, except in certain preferred directions. Since the xdirected and the ydirected electric field vectors travel with different velocities, their phases change at a different rate as the light propagates through the material. Although on the material surface the xdirected and the ydirected electric field vectors are in phase, the phase difference between these two electric field vectors inside the material becomes proportional to the depth the light has traveled into the material. Anisotropic materials, such as Calcite (CaCO3), quartz (SiO2), and KDP (potassium dihydrogen phosphate, KH2PO4), belong to this kind of material. If a narrow beam of unpolarized light is incident normally on the surface of a birefringent plate, the beam will be split into two refracted beams: the ordinary ray (O ray) and the extraordinary ray (E ray), as shown in Figure 314(a). The O ray passes through the plate, but the E ray diverges as it passes through the plate and then emerges parallel to the original beam direction. If the emergent beam from Plate I is allowed to fall on Plate II, whose optic axis is parallel to that of Plate I, the result is shown in Figure 314(b). The combination of these two plates behaves like a single plate of the thickness equal to the sum of the thicknesses of the two plates (i.e., 1d + d/2 = 1.5d). If Plate II is rotated through an angle of p about the direction of the incident beam, the deflections in the two plates are of opposite signs. Thus, the combination of these two plates behaves like a single plate of the
Optical and ElectroOptic Processes
thickness equal to the difference in thickness between the two plates, (i.e., 1d  d/2 = d/2), as shown in Figure 314(c). The direction of polarization of the O ray is perpendicular to that of the E ray. According to Huygens,3 since there are two rays, the wave should consist of two equiphase wavefront surfaces, one for the O ray and the other for the E ray. The O ray obeys Snell’s law in all directions, indicating that the surface to represent its equiphase wavefront surface is a sphere, while for the E ray, the surface to represent its equiphase wavefront surface should be an ellipsoid of revolution. Huygens also assumed that all birefringent crystals can be considered uniaxial and that the spheroid touches the sphere either externally, as shown in Figure 315(a), or internally, as shown in Figure 315(b), depending on whether the uniaxial crystal is positive
129
or negative. In either case, the whole surface is formed by revolving the curves about the line joining the points of contacts. If the wave propagation is along this line, both the O ray and the E ray have the same propagation velocity. This line is called the optic axis. The two rays have mutual perpendicular polarization. The plane containing the optic axis and the O ray is called the principal plane for the O ray, and that containing the optic axis and the E ray is called the principal plane for the E ray. The O ray is polarized perpendicular to the principal plane of the O ray, while the E ray is polarized in the principal plane of the E ray. For positive uniaxial crystals, the refractive index for the O ray no is smaller than that for the E ray nE (i.e., no < nE), as in quartz (SiO2), while for negative uniaxial crystals, the refractive index for the O ray is larger than that for the E ray (i.e., no > nE).
E (E Ray)
(a)
O (O Ray)
E1E2 (E Ray)
E1 O1
(b)
O1O2 (O Ray)
E1 E1E2 (E Ray) O1O2 (O Ray)
O1
(c)
d
d/2
Plate I
Plate II
Figure 314 (a) Double refraction of light (birefringence) in an anisotropic crystal plate, (b) double refraction in two parallel plates with the same orientation of the crystal axes, and (c) double refraction in two parallel plates, but in this case, the second has been rotated through an angle of p about the direction of the incident light beam.
130
Dielectric Phenomena in Solids Optic Axis
Optic Axis
E Ray
O Ray
O Ray
E Ray
q1
q1
n1
n1
no, nE
no, nE
O Ray
E Ray
E Ray
(a) Positive Uniaxial Crystal no< nE
O Ray
(b) Negative Uniaxial Crystal no > nE
Figure 315 Equiphase wavefront surfaces for ordinary and extraordinary rays for (a) positive uniaxial crystal and (b) negative uniaxial crystal.
Suppose that a point source of light is radiating uniformly inside the crystal; the O ray component is polarized with its electric field vector perpendicular to its principal plane and has a spherical equiphase wavefront surface. This is why the O ray propagates at the same velocity in all directions and the crystal for the O ray behaves like an isotropic crystal. The E ray is polarized in its principal plane and orthogonally to the O ray. Its equiphase wavefront surface is a spheroid, and this is why the velocity of the E ray propagation varies with direction. Only along the optic axis, its propagation velocity is the same as that of the O ray. At right angles to the optic axis, the propagation velocity of the E ray is either a maximum
for the negative uniaxial crystal, in which no > nE, or a minimum for the positive uniaxial crystal, in which no < nE, as shown in Figure 315. If an unpolarized light beam is incident on the surface of a birefringent material, there are two refracted beams inside the material: the O ray and the E ray. Their refraction angles depend on the value of no and nE, as shown in Figure 315. QuarterWave Plates (QWP) It can be seen from Figure 315 that when a light beam propagates along the direction perpendicular to the optic axis in a uniaxial crystal, the difference in velocity between the O ray and
Optical and ElectroOptic Processes
the E ray is the greatest. Therefore, there will be a phase difference between the two beams. After these two beams have traveled a distance d inside the crystal, the phase difference is Df =
2p (no d  nE d ) l
a magnetic field, optical radiation, or mechanical stress. This leads to many ways to produce light modulation. In the following sections, we shall discuss some commonly used methods for making material optically active.
(363)
Suppose we have a uniaxial crystal plate of thickness d. If the difference in optical paths (no  nE) d = l/4 (quarter wavelength), then the phase difference between the O ray and the E ray becomes Df = p 2
131
(364)
Thus, the combination of these two rays will have a resultant electric field vector that will trace an ellipse on the exit facet of the crystal. Based on the same principle, we can also produce halfwave or wholewave plates. In addition, we can adjust the direction of the incident beam relative to the optic axis. If the angle between the direction of the incident beam and the optic axis is 45°, the emergent beam will be circularly polarized. However, a variety of the forms of polarization can be obtained using uniaxial crystal plates. Such plates are often used in light modulation systems.
Optical Activity When a beam of planepolarized light passes through certain types of crystals, the light remains planepolarized but rotates about the direction of polarization, either in clockwise rotation (called righthand or positive rotation) or in counterclockwise rotation (called lefthand or negative rotation). Such crystals are generally referred to as optically active materials, and such an intrinsic phenomenon is referred to as natural optical activity. Obviously, only anisotropic crystals may have this property. Some birefringent crystals exhibit a gyration phenomenon due to this natural rotation of the polarization plane. However, optical activity can be induced by an external excitation force. Some materials, which are normally isotropic in their optical properties, may become anisotropic and optically active by an external force, such as an applied electric field,
3.2.2 ElectroOptic Effects This section deals with the ways of making some crystals optically active by means of an applied electric field. An applied electric field across a crystal will alter the normal distribution of electrons in it and hence cause changes in polarization P and refractive index n. Thus, the field dependence of the refractive index can be written as nF = n + aF + bF 2 + . . .
or Dn = nF  n = aF + bF 2 + . . .
(365)
where n is the refractive index in the absence of an applied field (i.e., F = 0), Dn is the change of the refractive index, and a and b are electrooptic constants. The effect of the electric field on the change of the refractive index is referred to as the electrooptic effect. It is evident that if a crystal has a center of symmetry or a material has a random structure, there is no electrooptic effect. Only crystals that are noncentrosymmetric exhibit the electrooptic effect. In the following sections, we shall discuss two well known electrooptic effects commonly used in lightmodulation systems.
The Pockels Effect or Linear ElectroOptic Effect The Pockels effect is the first order electrooptic effect, which was first discovered by F. Pockels in 189319 and is now probably the most useful element in modulation applications.20 Let us consider a threedimensional dielectric ellipsoid, as shown in Figure 316, whose shape varies with the electric field. In the absence of an applied electric field (F = 0), the refractive index is isotropic, and the ellipsoid should be a sphere. Suppose a beam of planepolarized light is propagating in the z direction
132
Dielectric Phenomena in Solids
involves tensors. A linear electrooptic effect in quartz was first analyzed by F. Pockels in 1893.19 For the details about the derivation, see references 5 and 19–23. The basic arrangement of a Pockels light modulator is shown in Figure 317. Since the two beams travel at different velocities in the crystal, the emergent beams will have a phase difference given by
z
n3
0 n1
n2
y
x
Figure 316 An ellipsoid for a biaxial crystal used for explaining the effect of an applied electric field.
through an electrooptic crystal such as KDP, and also an electric field F is applied across the crystal along the z direction. The refractive index does not change in the z direction but changes in the transverse direction. For KDP, if F is along the z direction, then the original principal axes of the ellipsoid are rotated through 45° into new principal axes x¢ and y¢, due to the induced optical activity. The refractive index changes in such a way that the refractive index for the polarization in the x¢ direction changes by +Dn and that for the polarization in the y¢ direction by Dn, so we can write nx¢ = n + Dn ny¢ = n  Dn
(366)
where Dn =
n3 rF 2
(367)
and r is the electrooptic coefficient for the Pockels effect and n is the refractive index in the absence of an applied electric field. The derivation of the Pockels coefficient r is based on the dependence of the refractive index on the electric polarization P, and the analysis
2p ( n x ¢  ny¢ ) d l n3 2p = (2 d ) rF l 2 2p 3 = n rV l
Df =
(368)
where d is the thickness of the crystal and V is the applied voltage (V = Fd). With this phase difference, the emergent beam is generally elliptically polarized. This elliptically polarized beam is then made horizontally planepolarized by an analyzer before it is transmitted to the other optical transmission system. Since the electric field vectors Fx¢ and Fy¢ of the beam emerging from the electrooptic crystal depend on the phase difference Df, we can write Fx¢ =
Fx¢o cos(w t + Df 2) 2
(369)
Fy¢ =
Fy¢o cos(w t  Df 2) 2
(370)
It can easily be shown that the total electric field vector FT = Fx¢ + Fy¢, after passing through the horizontal polarizer (analyzer), is in a form similar to Equations 318 and 319. The transmitted light intensity (i.e., irradiance) is I•F T2. It can be shown that the transmitted light intensity is given by I = Io sin 2 (Df 2) p = Io sin 2 Ê n3rV ˆ Ël ¯
(371)
where Io is the irradiance (i.e., intensity) of the light incident on the electrooptic crystal.5 The irradiance of the output light varies with applied voltage, and there is a maximum output, which occurs at V = Vm when
Optical and ElectroOptic Processes
133
x¢
z y¢ d x¢
Unpolarized
x
Light Beam
y
Emergent Beam (Elliptically Polarized) y¢
Vertical Plane Polarizer
Transmitted Light
Horizontal Plane Polarizer (Analyzer) V Applied Voltage ElectroOptic Specimen
Figure 317 The basic arrangement of the compenents of a Pockels light modulator.
p 3 p n rV = 2 l
(372)
or when V = Vm =
l 2 n 3r
The variation of I/Io with V is shown in Figure 318(a). If the applied voltage V is superimposed on a small signal, the transmitted light will be modulated according to the small signal, as shown in Figure 318(b). Obviously, the Pockels electrooptic cell can be used as a light switch. We can adjust the irradiance of the light output from its maximum value by increasing the applied voltage to the value of Vm, and we can turn off the light by reducing the applied voltage to zero, as indicated in Figure 318(a).
The Kerr Effect or Quadratic ElectroOptic Effect The Kerr effect is the second order electrooptic effect. In 1875, John Kerr was the first to show that many isotropic materials behave like a uniaxial crystal with the optic axis in the direction of the electric field.24 When an electric field
is applied across the material in the direction perpendicular to the incident light beam, however, birefringence will be induced. Kerr used glass at that time to show this effect.3,20,24 If the applied field F or the applied voltage (V = FL) is in the direction perpendicular to the incident light beam, the change in refractive index is given by Dn = n p  nn = KlF 2
(373)
where K is the Kerr constant (or the birefringence coefficient) and l is the wavelength of the incident light in free space. The dimension of the Kerr constant is mV 2. If an optically inactive, transparent, dielectric liquid is composed of long asymmetric molecules and these molecules are polar, possessing permanent dipoles, then at zero applied field, the dipoles are randomly oriented; however, at high applied fields, the molecules will be polarized and the dipoles will tend to line up, making the liquid become anisotropic and birefringent, and exhibit optical activity. This means that under a high applied field, the propagation velocity of the incident light polarized in the direction parallel to the optical axis is different from that normal to the optical axis. The applied electric field F produces two effects:
134
Dielectric Phenomena in Solids 1.0
I Io
0.5
V
0
2Vm
Vm
(a) 1.0 Transmitted Irradiance I Io
0.5
time, t
Q
0 Vm
Voltage
Modulating Voltage time, t
(b) Figure 318 (a) The ratio of output light irradiance to input light irradiance as a function of applied voltage and (b) the variation of the irradiance of the modulated output light with time corresponding to the variation of the modulating signal voltage with time.
The first effect is the orientation of the dipolar molecules (dipoles) with their axes of greatest polarizability in the direction of the field, and the other effect is the orientation of these dipoles. In nonpolar materials, only the first effect is present, but in polar materials, both effects will occur, with the second effect usually dominant. The field dependence of the difference between the refractive index np when the electric field vector of the light wave Fp is parallel to the applied field F, and nn when the field vector Fn is normal to F, is shown in Figure 319. It can be imagined that molecular dipoles are very sluggish in responding to the periodic change of the electric field vector of the light beam, whose frequency is of the order of 1014 Hz. This implies that it is the applied electric field F that causes the orientation and polarization of the molecules, resulting in the change of the refractive index. In the Fundamental Concepts section of Chapter 2, we assumed the
electric susceptibility c and polarizability a to be independent of applied electric field. However, in nonlinear optics, the polarization P is no longer just equal to ceoF, but should be written as P = ( c + aF + bF 2 + . . . )e o F
(374)
If we consider only the quadratic field dependence, P may be simplified to P = e o ( cF + bF 3 )
(375)
Based on this field dependence of the polarization, the Kerr constant K has been derived to find the permittivity of the material at the optical frequency.5,25,26 This constant is given by K=
N Ê uo2 ˆ Da + 30e o kT Ë kT ¯
(376)
where N is the number of molecules per unit volume, uo is the dipole moment of the molecular dipole, Da = ap  an, and ap and an are, respectively, the induced polarizability along
Optical and ElectroOptic Processes
Applied Voltage
135
V x¢
x¢ y¢
L
z
Plane Polarized Beam
y¢ Emergent Beam (Elliptically Polarized)
d ElectroOptic Specimen
(a) V = FL
V = FL
Fp
Light Beam
Fn
The electric field vector Fp is polarized in the plane of incidence, so Fp is parallel to the applied field F and the refractive index is np.
Light Beam
The electric field vector Fn is polarized normal to the plane of incidence, so Fn is perpendicular to the applied field F and the refractive index is nn.
(b) Figure 319 Schematic diagrams showing (a) the basic arrangement for a Kerr effect light modulater and (b) the definition of np and nn.
the optic axis and that perpendicular to the optic axis. For more details about the Kerr effect, see references 25–28. The electric field that induces optical anisotropy can be either a static or a timevarying field. In the former case, the Kerr effect can be used for light modulators or light switches; in the latter case, the Kerr effect can provide information about molecular reorientation. The Kerr effect can also be used as a method for measuring the spatial distribution
of space charges or electric field in fluids with high Kerr constants.29 If the field for inducing the Kerr effect is in the optical frequency range, the effect is called optically induced birefringence. This effect has been theoretically studied and experimentally observed in several liquids by several investigators.30,31 This effect can be used for selffocusing of laser beams, because the intense field vector of the beams can enhance the refractive index.32 In polar materials, the optically induced birefringence is
136
Dielectric Phenomena in Solids
smaller than the static field–induced birefringence for the same field intensity, since in the optical frequency fields, the orientation of the molecules is due only to the anisotropy of the polarizability, while in the static fields the orientation of the permanent dipoles becomes more important. Liquid Kerr cells containing CS2, nitrobenzene, or other similar liquids have been used either as a light modulator or as a light switch. Practical Kerr cells usually employ one of the molecular liquids, since the reorientation of the molecules in those liquids under an applied electric field can produce a large change in refractive index. However, even though those liquids have a high value of the Kerr constant K, a high voltage of the order of 25 kV is sometimes required to produce sizable amplitude modulation. This is why most of electrooptic light modulators used with lasers are Pockels cells, which use one of the noncentrosymmetric crystals and produce birefringence through the second order nonlinearity, which induces a linear rather than a quadratic birefringence, as discussed earlier. Adequate modulation can be achieved in most applications with the modulation voltage of a few kV or less. The most important materials for Pockels cells are potassium dihydrogen phosphate (KDP) and ammonium dihydrogen phosphate (ADP), or Lithium niobate (LiNbO3). ElectroOptic Ceramics Before closing this subsection, it is worth mentioning the electrooptic effect in ceramic materials. About 1960, highly transparent ceramics in the PbZrO3  PbTiO3  La2O3 (PLZT) system were developed.33–35 These materials have a remarkable facility for changing their polar state under an applied electric field. Since these materials are made of many compounds, a highly homogeneous mixture is necessary for electrooptic applications in order to avoid scattering due to local variation in composition and to ensure uniform electrooptic properties. This is why material fabrication processes are extremely important for producing PLZT ceramics for optical applications. For details
about ceramic fabrication processes, see references 36–38. The optical transparency of the PLZT ceramics is highly dependent on the concentration of lanthanum oxide (La2O3) in the material. The specific concentrations of La that yield high optical transparency are dependent on the concentration ratio of Zr/Ti. For Zr/Ti = 65/35, the concentrations of La expressed in atomic percentage should be in the range of about 5 to about 16 atomic percentage. The type of hysteresis loop depends on the composition of the PLZT ceramics. For a Zr/Ti ratio of about 65/35 and a concentration of La of about 5 atomic percentage percent, the hysteresis loop is a square loop with a low coercive field, as shown in Figure 320(a), while for a Zr/Ti ratio of about 35/65 and a concentration of La of about 8 atomic percentage, the hysteresis loop is also a square loop, but with a high coercive field, as shown in Figure 320(b). By increasing the concentration of La to about 11 atomic percentage for the case of a Zr/Ti ratio of about 65/35, the hysteresis loop becomes a slim loop exhibiting fieldenhanced ferroelectric behavior, as shown in Figure 320(c). The corresponding variations of the change in refractive index Dn = (nE  no), with the applied electric field for the three main types of characteristics, are also shown in Figure 320. The experimental data are from Haertling.36,39,40 Ferroelectric materials are noncentrosymmetric and possess the property of birefringence. These materials have one optic axis. A light beam traveling in the direction of the optic axis with its electric field vector vibrating in the direction perpendicular to the optic axis has a phase velocity c/no, while a beam traveling in the direction perpendicular to the optic axis with its electric field vector vibrating in the direction parallel to the optic axis has a phase velocity c/nE, in which no and nE are the same as those defined for the ordinary and extraordinary rays. Let us go back to Figure 320. The hysteresis loop shown in (a) is suitable for memory applications (see Ferroelectric Materials and Application of Ferroelectrics in Chapter 4). However, the PLZT with the hysteresis loop
Optical and ElectroOptic Processes
137
Dn (10–3)
–2 P (C m )
8
0.3 6 4 –2
–1
1 2 F (MV m–1)
2
–0.3 –1.0 –0.5
0.5
1.0
–1 F (MV m )
(a) P (C m–2)
Dn (10–3) 3
0.3
2
F (MV m–1) –2
–1
1
1
2 –1.5
–0.3
–0.5
0.5
1.5 –1 F (MV m )
(b) –3 Dn (10 ) 8
–2 P (C m )
6
0.3
4 –2 –1
2
1 2 F (MV m–1)
–0.3
–1.5
–0.5
0.5
1.5 F (MV m–1)
(c) Figure 320 The hysteresis loops and the variation of the change in a refractive index with the applied electric field for (a) a square loop with a low coercive field, (b) a square loop with a high coercive field, and (c) a slim loop of PLZT ceramics.
shown in (b) exhibits a linear electrooptic effect similar to the Pockels effect. The composition of this PLZT system is rich in the concentration of PbTiO3. A high concentration of PbTiO3 favors tetragonal distortion from the cubic structure, and a high tetragonality yields a high coercivity. The hysteresis loop shown in (c) is a slim loop; the PLZT exhibits a quadratic electrooptic effect similar to the Kerr effect.
The composition of this PLZT system lies close to the ferroelectric rhombohedraltetragonal boundary (see the phase diagram for the PZT system, Figure 419, in Phenomenological Properties and Mechanisms in Chapter 4). For more information regarding the properties and applications of electrooptic materials, the reader is referred to some excellent references, 36–43.
138
Dielectric Phenomena in Solids
3.2.3
The Photorefractive Effect
Some materials’ refractive index will change when they are subjected to light radiation. This phenomenon is referred to as the photorefractive effect. Several investigators discovered in 1966 that an intensive blue or green laser beam irradiating LiNbO3 or LiTaO3 crystals caused a change in refractive index of these materials.44 They also found that such crystals, after their refractive index was changed by irradiation, could be returned to their original homogeneous and equilibrium state by being heated to about 200°C in a short period of time. Since then, many investigators have studied this effect in three directions: the mechanisms responsible for this effect, the materials exhibiting this effect, and the applications of this effect.45–50 The photorefractive effect simply refers to the optically induced changes of the refractive indices. This effect has been observed in a variety of electrooptic materials, including BaTiO3, KNbO3, CdS, etc. Depending on the band gap of the material, the refractive index changes may be induced not only by visible light but also by infrared or ultraviolet light. The basic experimental arrangement for detecting the optically induced changes of refractive indices in crystals is shown in Figure 321(a). Both LiNbO3 and LiTaO3 have a large linear electrooptic effect and large spontaneous polarization of the order of 60 mC cm2.51,52 The laser beam is illuminating the specimen in the direction perpendicular to the caxis (the polar axis of the crystal), and only a small region of the specimen is illuminated. For the specimen with a size of about 1.25 cm along the aaxis, 0.25 cm along the caxis, and 0.25 cm along the baxis, the diameter of the illuminating beam is about 102 cm. Usually, the incident beam is linearly polarized, with the plane of polarization at 45° from the caxis of the crystal. The incident light beam in this case is found to split into three beams inside the crystal: one beam (the ordinary ray) does not change the direction, while the other two beams (extraordinary rays) are displaced from each other. The splitting of the light beam
indicates that the laser beam has caused the changes of refractive indices most for the extraordinary rays and least for the ordinary ray, resulting in nE < no for LiNbO3. The change of the refractive index Dn = nE  no is the highest at the center of the caxis (i.e., the region in which the intensity of the laser beam is the highest) and Dn gradually decreases along both sides of the caxis and the baxis from the center, as shown schematically in Figure 321(b). The refractive index changes Dn = nE  no within the illumination region increase linearly with increasing laser beam intensity and also with increasing the light exposure time, as shown in Figure 322. The experimental results are from F.S. Chen.46 When a crystal specimen is illuminated by a light beam, the illumination inside the specimen is not uniform. The amount of photogenerated charge carriers depends on the concentration of suitable donors present in the specimen, as well as the intensity of the light beam. Most of the crystals of interest are transparent to visible light, so electrons and holes excited from impurities present in the crystal are important. All charge carriers generated by light will diffuse from the region of high light intensity to the region of low light intensity, or to the region without illumination. These charge carriers may also move by drift due to the photovoltaic effect. The migration of the charge carriers will form space charges along the caxis and the baxis, and hence create an internal field (called a space charge field). This internal field causes the changes of refractive indices based on the electrooptic effect. The basic difference between the conventional electrooptic effect and the photorefractive effect lies in the fact that for the former, the change of the refractive index is caused by an externally applied electric field, while for the latter, it is caused by the internal field created by space charges and the photovoltaic effect due to the optical excitation. However, for a large photorefractive effect, suitable donors, traps, and efficient charge carrier movement are essential. In crystals, traps are present due either to structural defects or to chemical defects (irregular composition or
Optical and ElectroOptic Processes
139
c
a b
Laser
Slit
Lens
Lens
LiNbO3
Analyzer
Polarizer Compensator
Photodetector
(a) c(x )
a(z )
Direction of the Incident Laser Beam
b(y )
c
c
Dn CrossSection Area of the Laser Beam
0 Dn
–c
b
–b
–b
0
b
–c
(b) Figure 321 (a) The basic experimental arrangement for detecting the optically induced changes of refractive indices, and (b) the schematic diagrams showing the spatial variation of the changes of refractive indices along the caxis and along the baxis.
impurities). Materials doped with Fe impurities have a high photorefractive effect since Fe acts as a donoracceptor trap via intervalence exchanges, such as Fe2+ X Fe3+. The ion Fe2+ acts as a donor, and Fe3+ acts as an acceptor, which may act as an electron trap to capture an electron from the conduction band or as an acceptor to produce a hole in the valence band. The change of refractive index is more concentrated in the illuminating region along the caxis, as shown in Figure 321(b). This
may indicate that a higher internal field may be created not only by space charges similar to the Dember photovoltaic effect, but also by anomalous photovoltaic effect, due to an asymmetric charge transfer process and Franck–Condon shifts of the excited ions along the polar axis (caxis) of pyroelectric crystals, such as LiNbO3.48 It has been reported that even in pure ferroelectric or electrooptic materials, electronphonon coupling and collective Franck–Condon relaxation processes
140
Dielectric Phenomena in Solids
B
10
A
dn dx dn = qun( Fph + Fsc ) + ukT dx
j = qun( Fph + Fsc ) + qD
8 Dn (¥10–3)
multiplying it by (hu)1 or (hc/l)1, where hu is the energy of each photon). The current flow equation is
6
(378)
The continuity equation is ∂r sc ( x, t ) ∂ j( x, t ) = ∂t ∂x
4
(379)
and Poisson’s equation is 2
dFsc r sc ( x, t ) = e re o dx
0 0
100 200 300 Beam Intensity (mW)
400
Figure 322 The change of the refractive index Dn of LiNbO3 crystals as a function of the intensity of the illustrating laser beam. The beam diameter is 102 cm. The exposure time is 0.02 sec for A and 0.1 sec for B.
may produce an anomalous photovoltaic effect.53,54 We will consider a simple case to illustrate the factors controlling the photorefractive effect, assuming that only electrons in the conduction band are mobile carriers, that the donors and other impurities or traps are immobile, and that the formulation is for the onedimensional case (i.e., along the caxis [xaxis]). The equations governing the behavior of the photorefractive effect are as follows. The equation for the rate of photoionization is ∂ N D+ = SI ( N D  N D+ )  RnN D+ ∂t
(377)
where ND and ND+ are, respectively, the concentrations of the total donors and the ionized donors, n is the mobile electron concentration, R is the recombination coefficient, S is the crosssection of photoionization, and I is the incident light intensity expressed in the number of photons per unit area and per unit time (I expressed in mW cm2 must be converted to the number of photons per cm2 and per second by
(380)
where Fph and Fsc are, respectively, the photovoltaic field and the space charge field; D is the diffusion coefficient, which is equal to ukT/q based on Einstein relation; rsc(x, t) is the space charge density, which is q(n  ND+ + NA); and N A is the concentration of trapped electrons captured by traps other than the ionized donors, which also act as electron traps. Even if we ignore the photovoltaic field Fph, to obtain Fsc by solving Equations 377 through 380, we need to know the spatial distribution of N D+ , n, and u. It is much easier to solve this problem if we use a light source having a definite spatial distribution of its light intensity. In the following, we describe briefly a simple doublebeam coupling system that can provide a stable spatial distribution of the incident light intensity. With two light beams of intensities I10 and I20 incident on the specimen surface at an angle q from the aaxis, as shown in Figure 323, the spatial distribution of the resultant light intensity is given by I ( x, t ) = Io exp( a z cosq )[1  m cos Kx ]
(381) along the xaxis (caxis) for the onedimensional case, where a is the light absorption coefficient, K = 2p/L is the spatial frequency, L = l/2 sin q is the interference fringe spacing, Io = I1 + I2, and I1 and I2 are, respectively, the light intensities of the two incident interfering beams (I10 and I20) with a modulation index m.49,55 The value of m is given by
Optical and ElectroOptic Processes
change of refractive index for the linear electrooptic crystals induced by the photorefractive effect can be estimated by
c(x )
a(z )
no3r13 Fsc 2 nE3 r33 Fsc DnE = 2 Dno = 
b(y )
I10
I2
q q
I1 d
I20
Figure 323 A doublebeam coupling system for producing a stable spatial distribution of light intensity.
12
2( I1 I2 ) ˘ m = ÈÍ cos 2q Î I1 + I2 ˚˙
(382)
With this doublebeam coupling system, the generation of photoinduced electrons can be considered to be uniform over the crystal length along the z direction. The generation rate of photoinduced electrons along the x direction (caxis) can be written as g( x ) = go (1 + m cos Kx )
(383)
where go is given by ba Io ba Io l go = = hu hc
(384)
where b is the quantum efficiency for exciting a charge carrier from the donor. Using the doublebeam coupling system, several investigators have solved Equations 377 through 380 for the space charge field Fsc. By ignoring the contribution from the anomalous photovoltaic effect, the space charge field along the caxis (xaxis) is given by Fsc = m
kT È K ˘ cos 2q q ÍÎ (1 + K Ko )2 ˙˚
(385)
where Ko2 =
141
qN D+ ( av ) [ N D  N D+ ( av ) ] qkTN D
(386)
+ and ND(av) is the mean value of ND+ distributed along the xaxis.49,56 Once Fsc is known, the
(387)
These expressions are similar to that for the Pockels effect. The electrooptic coefficients r13 and r33 are related to the relative direction of the O ray and that of the E ray to the direction of Fsc. For most crystals, r33 > r13. For example, BaTiO3 has r13 = 10 pmV 1 and r33 = 93 pmV1.57,58 Since the discovery of the photorefractive effect, a great deal of effort has been devoted to insight into the microscopic mechanisms responsible for this photorefractive phenomenon and the factors controlling its behavior under various conditions. Details about developments in this area are beyond the scope of this book. However, before closing this subsection, we would like to mention some general information about the materials and applications. Up to the present, the materials exhibiting the photorefractive effect may be placed into three groups: Group 1: This group includes mainly ferroelectric materials. The oxygenoctahedral materials, particularly those containing Fe, exhibit the largest electrooptic effect, such as LiNbO3, LiTaO3, KNbO3, and BaTiO3. Highly transparent ferroelectric ceramics of the PZT family, with the perovskite structure with part of lead ions substituted by lanthanum ions, form a (Pb1xLax) (ZryTiz)O3 or PLZT system. Group 2: This group includes mainly nonferroelectric or paraelectric materials, such as Bi12SiO20, and Bi12GeO20. They possess electrooptic and photoconductive properties. Group 3: This group includes mainly semiconducting materials such as GaAs, InP, and CdTe. These materials are transparent up to the infrared frequency region, so they exhibit the photorefractive effect in the infrared frequency range.
142
Dielectric Phenomena in Solids
To select material for a specific application, it is important to consider the following factors: • Photorefractive sensitivity • The range of the refractive index changes • The phase shift between the refractive index and light intensity distributions • Photorefractive signal recording time and erasure time • Spatial frequency dependence • Electric field dependence • Light wavelength (i.e., photon energy) for inducing refractive index changes • Resolution • Signaltonoise ratio • Operation temperature Similar to the electrooptic effect, there are a variety of applications of the photorefractive effect.49,59 Here we just mention a few because of the limited space of this subsection. Some important applications are volume hologram storage,47,49,60 realtime holography and interferometry,61,62 realtime information processing,63,64 and coherent light amplification.49,65
3.2.4 The MagnetoOptic Effect In general, any method that can change the refractive index of a crystal can be used to deflect a light beam and hence to modulate a light beam. Obviously, the electrooptic effect is a more efficient and convenient means for modulating light than the magnetooptic effect. The magnetic field may also change the optical properties of some materials, but the handling of an electric field is much easier than the handling of a magnetic field, so any optical devices based on the electrooptic effect are preferred to those based on the magnetooptic effect. The Faraday Effect Faraday discovered in 1848 that when a planepolarized light beam passed through a glass plate in the direction of an applied magnetic field, the plane of polarization was rotated.66,67
The amount of rotation in angle is proportional to the magnetic field H and is given by q = VHL
(388)
where L is the path length in the material and V is the socalled Verdet constant, whose dimension is the rotation per unit path length and per unit magnetic field. The Faraday effect is usually small and depends on the wavelength of the light beam. For example, the rotation in quartz at a magnetic field of 104 oersteds and the wavelength of the light beam of 5900Å is only about 2°46¢ for a path length of 1 cm. A planepolarized light beam will become circularly polarized when the crystal is subjected to a strong magnetic field along the direction of the light beam propagation. Depending on the electric field vector direction, the circularly polarized wave can be a righthand circularly polarized (RHCP) wave or a lefthand circularly polarized (LHCP) wave. As a result, the two counterrotating circularly polarized waves propagating along the direction of the magnetic field in the z direction have different phase velocities, c/nR and c/nL, where nR and nL are, respectively, the refractive indices for the RHCP and the LHCP waves. So q can also be expressed in terms of nR and nL as q=
2p ( nR  nL ) L l
(389)
It can be seen from Equations 388 and 389 that nR  nL depends on H. Thus, by varying the magnetic field H, we can modulate the light beam for various applications. The Voigt Effect Voigt found in 1905 that a magnetic field may also induce birefringence for a planepolarized light beam passing through a crystal in the direction perpendicular to the magnetic field. The component of a linear polarized light beam with the electric field vector parallel to the magnetic field travels at a phase velocity different from that with its electric field vector perpendicular to the magnetic field, thus causing the emerging light beam from the crystal to become
Optical and ElectroOptic Processes
143
elliptically polarized.68,69 We may consider the Faraday effect as the magnetic counterpart to the Pockels effect and the Voigt effect as the magnetic counterpart to the Kerr effect.
Substitution of Equations 394 and 395 into Equation 393 yields
3.2.5 The AcoustoOptic Effect The refractive index of a medium can be changed by the mechanical strains caused by the passage of an acoustic wave through the medium. The relation between the change of the refractive index and the change of the mechanical strain and stress is rather complicated.70 However, we may explain this effect from the Lorentz–Lorenz equation (see Chapter 2, Equation 2192), which is given by
The change of the refractive index Dn is directly proportional to the mechanical strain h. The acoustooptic effect is sometimes referred to as the elastooptic effect or the photoelastic effect, referring mainly to the change induced in the relative dielectric impermeability tensor by mechanical strain.71 The relative dielectric impermeability tensor is defined as Bij = (e1 r )ij, which is a secondrank tensor. The impermeability Bij is symmetrical, so Bij = Bji. For a weak strain, such as that caused by an acoustic wave, the change of the tensor can be considered as a linear function of strain. However, since the relative dielectric impermeability tensor and the strain tensor each involves nine tensor components, the solution of this problem for the acoustooptic effect would be quite complicated. Because it is beyond the scope of this book, we shall not discuss the mathematical involvement further. When a light beam enters an elastic medium in which an acoustic wave has already produced a sinusoidal variation of elastic pressure in the medium, the portion of the light wavefronts near the pressure maxima will encounter a higher refractive index and hence travel at a lower phase velocity than the portion of the wavefronts near the pressure minima. Thus, the light wavefronts in the medium exhibit a wavy variation according to the variation of the acoustic wave. The velocity of an acoustic wave (i.e., a sound wave) is much lower than that of a light wave. So, we may ignore the small wave variation of the wavefront and consider the variation of the refractive index to be stationary in the medium. In general, acoustooptic modulation cells are produced by means of moving gratings in an elastic medium produced by the strain accompanying acoustic waves. The light beam passing through the gratings will suffer diffraction; the light beam will then be spatially deflected, and the deflected beams have phases different from each other. There are two types
n 2  1 Na = n 2 + 2 3e o
(390)
The basic mechanism responsible for the change of the refractive index is the change of the density of the molecules by DN due to the mechanical strain produced by the acoustic wave. So we can write ( n  Dn)2  1 ( N  DN )a = ( n  Dn)2 + 2 3e o
(391)
From Equations 390 and 391, the change of the refractive index may be expressed as71 6nDn DNa = ( n 2 + 2 )2 3e o
(392)
or expressed in the form of Dn =
n3 È (n 2  1)(n 2 + 2) ˘ DN ˙˚ N 2 ÍÎ 3n 4
(393)
The acoustic wave causes only the locally elastic change in the density of the molecules in the region where the wave passes through. There is no change in the total mass of the medium, so the acoustic wave causes only a fractional change in volume of the medium DV. So, we can express the tensile strain h as h=
DV DN = V N
(394)
The photoelastic constant is given by p=
(n 2  1)(n 2 + 2) 3n 4
(395)
Dn =
n3 ph 2
(396)
144
Dielectric Phenomena in Solids
of diffraction: Raman–Nath diffraction and Bragg diffraction. For Raman–Nath diffraction, the grating is thin so that the light beam will be diffracted producing deflected beams. The amplitude of the deflected beam depends on the deflection angle from the direction of the incident light beam. If only the deflected beam in the same direction as that of the incident beam is considered, then the modulated beam will follow the modulating signal directly. For Bragg diffraction, we consider a planepolarized light beam incident on the grating planes at an angle of incidence q in a manner very similar to the Bragg diffraction of xrays from the planes (layers) of atoms in a crystal. The grating planes can be considered stationary acoustic wavefronts, so the incident beams are scattered from the successive planes. Constructive interference is formed by mixing the beams reflected from each of the planes (the grating planes imply a thick grating). So, the amplitude of the modulated beam is directly related to the modulating signal. Here, we have used a simple approach to describe the basic concept of the interaction between light waves and acoustic waves. For more details, the reader is referred to some excellent references, 5 and 71–74.
3.3 Interaction between Radiation and Matter The interaction between radiation and matter deals primarily with the processes of energy exchange between radiation and atoms. There are discrete energy levels in an atomic (or molecular) system. The system can make a transition from a state at a lower level E1 to a state at a higher level E2 by the absorption of a photon of energy DE = E2  E1 = hu. The system can also reverse the process; that is, an atom in a state of energy level E2 may change to a state of lower energy level E1 by the emission of a photon of the same energy DE = E2  E1. The optical spectra are associated with the motion of the outermost valence electrons of atoms or molecules and with the motion of the atoms or molecules, which occur in the microwave, infrared, visible, or ultraviolet frequency regions. The optical spectra provide informa
tion about the behavior of the outermost valence electrons of an atom,75–77 while Xray spectra give information about the inner electrons in the atom.77,78 This is a huge subject. In the limited space of this chapter, we shall deal only briefly with the topics related to dielectric phenomena. 3.3.1 Generation of Radiation Radiation generated from candlelight, the fire in a fireplace, or sunlight is common in our daily lives, and we often overlook its presence and importance. But life could not exist without radiation. There are two outstanding processes by which a material can generate radiation after absorbing suitable extraneous primary energy. The energy thus given to the electrons in solids may be transformed into thermal energy by collisions with neighboring atoms or molecules, resulting in thermal radiation. The energy given to the electrons may also be used to raise them from a state at a relatively lower energy level to another state at a relatively higher energy level, resulting in luminescent radiation. Thermal Radiation Radiation can emerge from a small hole in a highly polished cavity, as shown in Figure 324(a). It should be noted that almost every heated metal, such as tungsten filament, produces a radiation spectrum. The spectral radiation pattern depends on the radiator temperature. The ability of a body to radiate is closely related to its ability to absorb radiation. This is to be expected, since a body at a constant temperature in thermal equilibrium with its surroundings must absorb energy from those surroundings at the same rate as it emits energy. Generally, we consider an ideal body that absorbs all radiations incident upon it, regardless of frequency. Such a body is called a blackbody. The cavity shown in Figure 324(a) is a good approximation of an ideal blackbody. A small fraction of the thermal radiation can escape through a small hole in the wall of the cavity. Both the density and the wavelength of the emerging radiation can be measured by
Optical and ElectroOptic Processes
145
30 25
Cavity at T r(l)
20 1100° K
15
1000° K
10
Thermal Radiation
900° K
5
lm
0 0
1
2
3
4
5
6
7
8
9 10
Wavelength l (¥10–4 cm)
(a)
(b)
Figure 324 (a) The cavity approximates an ideal blackbody showing schematically the thermal radiation emitted from a small hole on the wall of the cavity, and (b) the distribution function of the radiation energy as a function of wavelength.
standard apparatus. In order to obtain emission of thermal radiation from a solid in the visible frequency region, the temperature of the solid must be raised to a temperature higher than 900 K to achieve an appreciable probability of getting 1.7 eV (or greater) for electronic excitation by the accumulative action of phonons. The thermal radiation of a solid approximates closely the thermal radiation of an ideal black body. Thus, the total energy (for all wavelengths) emitted in unit time per unit area of the wall of the cavity, according to Stefan’s law,3,79 is given by E =aT4
(397)
where a is Stefan’s constant, which is 5.67 ¥ 108 Wm2K4 for an ideal blackbody. Most hot material surfaces only approach the ideal; therefore, a would be smaller than this value. The distribution of energy with wavelength can be described by a function r(l). This means that the total energy, with a wavelength range between l and l + dl, is r(l)dl. This function r(l), according to Planck’s radiation law, is given by r (l ) =
8phc È 1 ˘ l5 ÍÎ exp(hc lkT )  1 ˙˚
(398)
or in term of frequency u instead of wavelength 3
r (u ) =
l 8phu È 1 ˘ r (l ) = u c 3 ÍÎ exp(hu kT )  1 ˙˚
(399)
The radiation energy distribution r(l) as a function of wavelength for three different temperatures is shown in Figure 324(b). It can be seen that r(l) has a peak value at lm, and the wavelength for the occurrence of the peak is inversely proportional to temperature T, according to Wien’s displacement law, given by lm T = constant
(3100)
Luminescent Radiation Strictly speaking, luminescence is a process whereby matter generates nonthermal radiation. This implies that luminescence affords photon emission in excess of that produced entirely by thermal radiation. Luminescence is generally produced by the excitation of a solid by primary photons or charge particles in a material having individual energies ranging from about 1 eV to over 106 eV and affording emitted photons with energies in excess of 1 eV. The luminescence process as a whole includes excitation, temporary storage of the energy, and radiation (or emission). Various processes for producing luminescence will be discussed in Section 3.4. Units of Light In Gauss’s law in Chapter 1, we discussed the fundamental and derived units of the SI system. Here we describe just briefly the units for light.
146
Dielectric Phenomena in Solids
The method of measuring the energy of electromagnetic radiation, when all frequencies involved are treated equally, is called radiometry. The watt is a radiometric unit. Light is a form of energy, and radiant energy and power are measured in joules and watts, respectively. Radiant power is sometimes referred to as flux. The amount of flux per unit area delivered to a surface is the irradiance I. In fact, this unit is often referred to as radiation intensity. In SI units, however, it is called irradiance and expressed in watts. If the light is from a point light source, the irradiance I is not expressed in watts alone because the irradiance measured at point P depends on the distance r from point P to the point light source, so it must be expressed in watts per unit solid angle: radiant power per unit area within a unit solid angle (i.e., watts per steradian [W/sr1]). Photometry was the method used to measure the radiation energy or power in the past. The fundamental difference between radiometry and photometry is that in radiometry, the measurements are made with electronic instruments, while in photometry, the measurements are based on the human eye. Therefore, different units are used in photometry for radiant power. The unit is lumens (lm) instead of watts. The unit for power density is lux (lumens per square meter) instead of watts per square meter. In this book, we use mainly the SI units based on radiometry. 3.3.2 The Franck–Condon Principle The concept of the configuration diagram, based on the Franck–Condon principle, is useful in explaining the nonradiative transition. In the Born–Oppenheimer approximation, the total wave function of a vibronic state Y can be expressed as the product of electronic wave function fe and vibrational wave function fv. Thus, we may write y li = f le ( q, r )f li (r )
(3101)
as the total wave function of the i vibronic state, where i indicates the ith vibrational state of the lower electronic state , and y mj = f me ( q, r )f mj (r )
(3102)
as the total wave function of the mj vibronic state, where j indicates the jth vibrational state of the higher electronic state m, and q and r are, respectively, the electronic and nuclear coordinates. According to the Franck–Condon principle, there are no changes in the nuclear coordinates during an electronic transition, and therefore, the most probable vibronic transitions are vertical because the time (less than 3 ¥ 1014 sec) required for an electronic transition is negligibly small compared to the period of nuclear vibration. Electronic transitions are most probable when the kinetic energies of the nuclei are minimal (that is, at the end points of their vibrations; for example, at a2c2 and a*2c*2 in Figure 325). The lowest vibrational levels may be possible exceptions to this principle.80 If the molecule is in its ground state E with vibrational energy corresponding to lowest sublevel aoco, as shown in Figure 325, the electron may be excited from this level to state Em at vibrationallevel end point a*2 by absorption of a proton with energy EA = huA. The excited molecule then vibrates between a*2 and c*2 and may emit phonons and relax to sublevel a*oc*o. Then, it may proceed back to state E at sublevel a2c2 by emitting a photon of energy EB = huB The molecule can relax to its lowest sublevel a*oc*o by emitting phonons. The energy emitted EB is lower than the energy absorbed EA. The difference between these two energies is called the Franck–Condon shift. In general, the degradation of optical energy is called the Stokes shift. Thus, the Franck–Condon shift is a Stokes shift due to the displacement of the molecule Dr. The absorption spectrum depends on the relative position of the minimum potential energy level and on whether the molecules are in vapor or in solution, as shown in Figure 325. 3.3.3 Radiative and Nonradiative Transition Processes The emission of radiation is the inverse of the absorption process. An electron occupying a quantum state at a level relatively higher than it would under thermal equilibrium conditions, will tend to make a transition to an empty state
Optical and ElectroOptic Processes
Ee* + (5/2)Emi
a2*
Ee* + (3/2)Emi
c2*
a1*
Ee* + (1/2)Emi
c1* a0*
EA = hnA
Energy Ee + (5/2)Ei Ee + (3/2)Ei Ee + (1/2)Ei
2 1 0
EB = hnB
c0*
147
a2
c2 a1
2
c1 a0
1
c0
0
r
Absorption
0–2 0–1 0–0
Wavelength Figure 325 Franck–Condon configuration diagram and absorption spectrum for a diatomic molecule. In the absorption curves, the dashed curve is for molecules in solution and the solid lines are for molecules in vapor form. EA is the absorption at the Franck–Condon maximum, and EB is the emission at the Franck–Condon minimum; r is the nuclear separation.
at a lower energy level, and all or most of the energy released due to this transition will be emitted as electromagnetic radiation. The radiative transition rate is determined by the product of the density of the occupied upper states and the density of the empty lower states, and also the probability P per unit volume for one carrier in the upper state to make a radiative transition to one lower empty state. Thus, the radiative transition rate can be written as
R = Pnu nl
where nu and n are, respectively, the densities of the occupied upper states and the empty lower states. The Franck–Condon configuration diagram indicates that the phonon emission process may accompany radiative transition when the electron is excited from the ground state at the ao level to the excited state at the a*2 level; the
148
Dielectric Phenomena in Solids
system will then partly relax to the a*o before making the transition to return to its ground state, as shown in Figure 325. This involves a displacement Dr of the atom. The excited electron loses some energy in this process, and the energy thus lost is dissipated in the atomic displacement, that is, in the form of phonon emission. When the electron returns to the ground state at the c2 level, a new atomic displacement will take place for c2 Æ co, again in the form of phonon emission. However, whether the transition made by an electron from an excited state at level m to a state at a lower level is radiative or nonradiative depends on the transition moment (or matrix elements of the electric dipole moment) between two states yi and ymi given by Equations 3101 and 3102, based on the Franck– Condon principle. The transition moment can be expressed as MmjÆli = y mj M y li = f me M f le f mi f li
(3103)
= Mml Smj ,li
where M is the electric dipole operator, Mml is the mean electronic transition moment, and Smj,i is the vibrational overlap integral. The FranckCondon maximum, which represents a vertical transition on the configuration diagram, corresponds to a maximum overlap integral (Smj,i). The probability of the radiative transition from a state corresponding to wave function ymj to a state corresponding to wave function yi is proportional to the square of the electronic transition moment pmrÆl µ MmjÆli 2
2
= Mml Smj ,li
2
(3104)
= AmÆl F
where F is the Franck–Condon factor, which is equal to Smj,i2; AmÆ is Einstein’s coefficient of spontaneous emission, which is equal to  M m2 and is given by 3 3 3 AmÆl = (8p hu mj Ælih c ) BmÆl
(3105)
in which h is the Plank constant, h is the refractive index of the medium where a molecule undergoes a transition, c is the light
velocity, umjÆi is the radiative frequency corresponding to the energy difference between the states mj, and i, BmÆ is Einstein’s coefficient for induced absorption or induced emission.70,81 The probability of nonradiative transition from a state of wave function ymj to a state of wave function yi is proportional to the electronic factor pmnrÆl µ Hmj Æli
2
2
(3106)
= Jml F
where HmjÆli = f mj Jml f li
(3107)
in which Jml = f me J N f le 2
(3108)
where Jm is the electronic factor and JN is the nuclear kinetic energy operator.81 Nonradiative transition processes always compete with radiative transition processes, and are therefore very important in energy transfer processes and luminescent phenomena. Unfortunately, these processes are poorly understood. Both Mm2 and Jm2 involve the wave functions of the initial and the final electronic states, so nonradiative transitions are subject to the same multiplicity, symmetry, and parity selection rules as radiative transitions.81 So far, we have discussed only the transitions in a completely isolated molecule. But the analysis of a solid containing interreacting molecules or atoms involves a complete Hamiltonian and would therefore become formidable. As our aim is to understand the basic concept of radiative and nonradiative transitions, we will use a simple model to show the rules governing the transition processes. We consider one electron in a onedimensional box, whose behavior is governed by the timedependent Schrodinger equation. In the box, there are quantum states of various discrete energy levels. Let us look into the behavior of this electron between any two states: one state n at an energy level higher than the other state, called state m. When the electron in state n makes a transition to state m, starting at time t = 0, how does this electron move during the time inter
Optical and ElectroOptic Processes
val (0 < t < t), where t is the time required for the electron to reach state m? By solving the Schrodinger equation for this simple case, it can be shown that the wave function y(x,t) of this electron during the time interval of transition is given by y ( x, t ) = y n cos
pt pt + y m sin , 2t 2t
0
(3109) where yn and ym are, respectively, the wave functions of the electron in state n and in state m. They are yn =
np x 2 sin exp( jEn t h) L L
(3110)
ym =
mp x 2 sin exp( jEm t h) L L
(3111)
The electron is in state n at t = 0, and in state m at t = t. The average value (or the expectation value) of the energy for the electron is L
E = Ú y jh o
∂ ydx ∂t
(3112)
pt = Em + ( En  Em )cos 2t
where y is the complex conjugate of y. Similarly, the average position (or the expectation position) of the electron in the box is
L
x = Ú y ¥ ydx o
=
pt ( En  Em )t L 4L + sin cos h 2 p2 t 4nm ¥ 2 ( n  m 2 )2
(3113)
where m and n are integers signifying the energy levels of the quantum states. By examining Equations 3112 and 3113, it can be concluded that when n  m is an odd number, the position of the electron ·xÒ oscillates about its average position at ·xÒ = L/2, and the oscillation frequency is (En  Em)/h during transition, as shown in Figure 326. This implies that the transition generates photons and is thus radiative, producing luminescence. Based on the classical theory of radiation, an electron oscillating in space will radiate electromagnetic waves. If n  m is an even number, ·xÒ = L/2, implying that there is no time change of the electron position during transition. This means that the transition generates phonons whose energy is dissipated as energy loss to the lattice vibration. The above model, though very simple, shows the transitions typical to electric dipole transitions governed by the selection rules. The performance of a laser depends on a particle (electron, atom, ion, or molecule) chang
t=0
En
149
En
E
E
Em
Em
t=t
0
L/2
L
t
0 t
x
(a)
(b)
Figure 326 Schematic diagrams showing (a) the displacement (oscillation) of an electron in a onedimensional box during the transition from state n to state m, and (b) the average energy of the electron in the box during transition from t = 0 at state n to t = t at state m.
150
Dielectric Phenomena in Solids
ing its energy state; in so doing, a photon can be generated. There are two basic types of solidstate lasers: one consists of rather wellisolated ions embedded in a host crystal, and the other is generally a semiconductor. The former can be considered a molecule with tightly bound electrons having discrete energy levels, somewhat similar to the simple model just discussed. In general, there are five processes for radiative transitions in solids82: 1. 2. 3. 4. 5.
Bandtoband transitions Transitions via shallow donor or acceptor levels Donoracceptor transitions Transitions via deep recombination centers Exciton transitions
In inorganic semiconductors, processes 1–4 may be dominant. However, in organic semiconductors, process 5 is the most important transition process. The quantum yield of luminescence depends on the relative probability of radiative and nonradiative transitions, and the relative efficiency of producing radiative excitons. There are many possible processes for nonradiative transitions. In inorganic semiconductors, multiphonon transition and Auger recombination processes are the dominant nonradiative transition processes.83 In organic semiconductors, however, again the process of exciton transitions leading to nonradiative transitions is the most important nonradiative transition process. In the following sections, we shall discuss briefly some nonradiative transition processes. The radiative transition processes will be discussed in Section 3.4, dealing with luminescence. MultiplePhonon Transition The excited electron in the Franck–Condon configuration diagram, shown in Figure 327, can be excited from point A at the lower level at ra to point B at a higher level at rb by thermal excitation at a higher temperature. At such a high temperature, the electron at point B may have enough energy to cross over to the ground
E
B Excited State
A
Ground State C
rc
ra
rb
r
Figure 327 Schematic diagram showing a nonradiative multiplephonon transition.
state, and then relax to a lower level in the ground state by the emission of phonons. This type of multiplephonon nonradiative transition process may occur in narrow bandgap materials, such as Ge and Si.84,85 For more information about multiplephonon transition, see the original work on this process.86,87 Auger Recombination Processes A number of Auger recombination processes are possible, depending on the nature of the transition and the concentration of carriers. This is a threebody collision event. Figure 328(a) shows the processes without involving localized states in the band gap; it is a bandtoband recombination but requires first the collision of two electrons in the conduction band or two holes in the valence band. Figure 328(b) shows the processes involving one level of localized states, which may be near either the conduction band or the valence band, and (c) shows the processes involving two levels of the localized states. The illustrations are selfexplanatory. For example, in the case of bandtoband recombination, after electron–electron collision, one electron will recombine with a hole in the valence band, and the energy
Optical and ElectroOptic Processes
Hot Electron
2¢ (High Energy Level)
Ec
Electron–Electron Collision 1 2
Ec
1
151
Phonons
2 Ec Recombination
Ev
Ev
Ev
Ec
Ec
Ec Recombination
Ev
1
Ev
2
2
1
Ev
Hole–Hole Collision
Phonons 2¢ (Low Energy Level)
(a)
Ec
Ec
Ec
Ev
Ev
Ev
(b)
(c)
Figure 328 Schematic diagrams showing the Auger recombination processes: (a) bandtoband transitions without involving localized states in the bandgap, but involving either electron–electron collision in the conduction band or hole–hole collision in the valence band, (b) the transition involving one level of localized states either near the conduction band or near the valence band, and (c) the transitions involving two levels of localized states.
released due to this recombination will be transferred to another electron, making it a hot electron. This hot electron will then relax to a low energy level by emission of multiple phonons.
The Auger effect depends mainly on carrier– carrier interaction. Thus, this effect increases with increasing concentration of carriers.88 Since the concentration of carriers increases
152
Dielectric Phenomena in Solids
with increasing temperature, this effect also increases with increasing temperature. The Auger effect is an important nonradiative transition process. It plays an important role in the electrical discharge and breakdown processes in dielectric materials. It accounts for the nonradiative trapping and recombination of the carriers injected from the electrical contacts at high fields, thus causing gradual degradation of the material.89 Nonradiative Transition due to Defects There are always surface states at the surface of a crystal or the interface between two different materials, such as the metal–semiconductor interface, because of the presence of dangling bonds. These surface states create shallow and deep traps in the band gap. This makes bandtoband recombination unable to take place near the surface, implying that the recombination nearby must go via the surface states, thus rendering the recombination nonradiative. This effect occurs also in the internal interface between the inclusion (e.g., foreign particle) and the host material. A crystal always consists of various defects, either structural or chemical, such as microvoids or pores, grain boundaries, dislocations, a cluster of vacancies, or precipitates of impurities. Such defects cause nonradiative transitions. Nonradiative Transition in Indirect Bandgap Materials Group IV elemental semiconductors and some III–V compounds belong to the category of indirect bandgap materials. In the energy band structure of direct bandgap materials, the wave vector kc of the conduction band edge (the bottom of the conduction band) and the wave vector kv of the valence band edge (the top of the valence band) are the same, so the law of the conservation of wave vectors (momenta) for optical transition is automatically satisfied. Since the wave vector of electrons is of the order of p/a, where a is the lattice constant, and the wave vector of photons is 2p/l, where l is the wavelength of the light wave, the photon
wave vector is much smaller than the electron wave vector for visible light or even higher optical frequencies. So, an electron must make a transition between states having the same wave vector. This means that only vertical transition is allowed, so both the optical absorption and the emission are a direct transition process. However, in indirect bandgap materials, the wave vector kc of the conduction band edge and kv of the valence band edge are not the same, so the law of the conservation of momenta for optical transition is not satisfied. For this case, absorption or emission of phonons is required to provide momenta to satisfy the momentum conservation law. Such a transition involves either absorption or emission of phonons in an indirect transition process. In general, an electron may be excited without change of wave vector from the top of the valence band to the conduction band by direct transition in an indirect band gap material, as shown in Figure 329(a). This transition creates a hole at the top of the valence band, but the electron in the conduction band is in a state with a higher energy than that at the conduction band edge (the bottom of the conduction band). This electron will quickly make a transition to the state at the bottom of the conduction band with emission of phonons. If the photon energy hu is less than Eg or higher than Eg, optical transition is still possible. For the case hu < Eg the transition process is as follows: Eg = hu + DE1
or hu = Eg  DE1
involving absorption of a phonon. If the photon energy is Eg < hu < Eg + DE2, then we have Eg = hu  DE2 ,
or hu = Eg + DE2
involving emission of a phonon. These optical absorption processes are shown in Figure 329.
Optical and ElectroOptic Processes
153
E DE Eg
k
(a) E
E
DE
DE Eg
kv
Eg
kc
k
(b)
kv
kc
k
(c)
Figure 329 Optical absorption processes in indirect bandgap semiconductors (a) direct transition requiring a photon of energy hu = Eg + DE, and the excited electron moving quickly to the bottom of the conduction band, (b) indirect transition involving absorption of a phonon of energy DE1, and (c) indirect transition involving emission of a phonon of energy DE2.
Similarly, we can easily write the processes for radiative emission. Suppose now that an electron in the bottom of the conduction band makes a transition to recombine with a hole in the valence band, but the hole is available only at the top of the valence band. In this case, absorption or emission of a phonon is again required to satisfy the momentum conservation law. If the emitted photon has energy hu smaller than Eg, then Eg = hu + DE1 ,
or hu = Eg  DE1
involving emission of a phonon. If the energy of the emitted photon is larger than Eg, then we have Eg = hu  DE2
or hu = Eg + DE2
involving absorption of a phonon.
These optical emission processes are shown in Figure 330. Phonon energies are of the order of 0.01 eV, much smaller than Eg. The phonon energies are mainly from the lattice vibrations. The indirect transition involves three particles—electron, hole, and phonon—and the three particles must match each other perfectly before the transition would become radiative. Furthermore, any transition involving the absorption of more than one phonon is very improbable. Obviously, it is highly improbable that the three particles will match each other perfectly to produce radiative transition. This is why the probability of radiative bandtoband recombination p is very small for indirect bandgap materials. The probability of bandtoband radiative transition for indirect bandgap materials, such as Si and Ge, is some 106 times smaller than that for direct bandgap materials, such as GaAs. This implies that the bandtoband carrier recombination in indirect bandgap materials is mainly nonradiative. For more details about this subject, the reader is referred to references 90–92.
154
Dielectric Phenomena in Solids E
E DE
DE Eg
Eg
kv
kc
k
k
(a) Indirect transition with
(b) Indirect transition with
phonon emission
phonon absorption
Figure 330 Optical emission processes in indirect bandgap semiconductors (a) involving emission of a phonon of energy DE1, and (b) involving absorption of a phonon of energy DE2.
For more information about nonradiative transition processes, see references 93 and 94.
3.3.4 Absorption and Dispersion Suppose a monochromatic light beam of intensity Ii is incident perpendicularly on the flat surface of an absorbing material, as shown in Figure 331. This light beam will be partly reflected from the surface and will partly enter the material. The intensity of the light beam entering the material is thus (3114)
I ( z ) = Ii  Ir
where Ir is the intensity of the reflected light. Because of the absorption of the material, the intensity of the light will decrease with the distance it has traveled. The probability (or
dz
Ir n* = n – jk
0

dI( z ) µ I( z ) dz

dI ( z ) = aI ( z ) dz
or
z
z + dz
(3115)
where a is the absorption coefficient. Using the initial boundary condition I(z) = Io at z = 0, the solution of Equation 315 gives I ( z ) = Io exp( a z )
(3116)
The dimension of the absorption coefficient is cm1, and it depends on the wavelength of the light and the material. The complex dielectric constant of dielectric materials is given by e r* = e r  je r¢
I (z )
Ii
the rate) of absorption in any element dz is constant, so the decrease of the light intensity is dI(z)/dz, and it is proportional to the light intensity at z. Thus, we can write
(3117)
where er is the dielectric constant (or relative permittivity) and e¢r is the loss factor (see The Complex Permittivity in Chapter 2). Since ur = 1 for nonmagnetic dielectric materials, the complex refractive index n* can be written as n* = n  jk = e r* = (e r  j e r¢)1 2
(3118)
This equation leads to Figure 331 The incident II, the reflected Ir, and the transmitted I(z) light beams from a transparent medium to an absorbing material.
n2  k 2 = e r 2 nk = e r¢
(3119)
Optical and ElectroOptic Processes
From Equation 3119 we can obtain n and k as a function of er and e¢r, and they are 12
2 er¢ ˘ ÔÏ 1 È n = Ì e r Í1 + Ê ˆ ˙ Ë er ¯ ˚ ÓÔ 2 Î
12
e r ¸Ô + ˝ 2 ˛Ô
12
12
2 ÏÔ 1 È er¢ ˘ k = Ì e r Í1 + Ê ˆ ˙ ÔÓ 2 Î Ë e r ¯ ˚
(3120)

e r ¸Ô ˝ 2 Ô˛
(3121)
For lossless materials, e¢r = 0 and k = 0, then n = er . Consider a planepolarized light beam propagating in the z direction in the absorbing material. The velocity of the light wave inside the material is v=
c n*
or 1 n k = j v c c
(3122)
The electric field vector F(z,t) of the propagating wave can be written as F( z, t ) = Fo exp[ jw (t  z v)] = Fo exp[ jw (t  nz c)]exp( wkz c)
(3123) The term exp (wkz/c) is a damping factor, representing the attenuation of the amplitude of F(z,t) with z due to the absorption of the electromagnetic energy of the light wave by the material. Thus, the light intensity at point z can be determined by the following relation: I(z) F 2 (z) = = exp( 2w kz c) = exp( a z ) Io Fo2
(3124) Comparing Equation 3124 to Equation 3116, the absorption coefficient can be expressed in terms of wavelength and the absorption property of the material a=
2w k 4p k = c l
(3125)
In Section 3.1.2, we mentioned the dispersion phenomenon. Strictly speaking, there is no material free of dielectric loss; therefore, there
155
is no material free of dispersion. This means that there is no material with completely frequencyindependent er and e¢r. In fact, the dispersion of er and e¢r is an intrinsic property of all materials, and all other properties must coexist with it. Also in Section 3.1.2, we mentioned that a dielectric solid can be considered an assembly of oscillators set into forced vibration by the external excitation force. The electric field vector of an electromagnetic wave of a light beam of frequency w may cause the bound electrons or ions to be displaced from their equilibrium positions, giving rise to polarization. Equation 359 is the equation governing the displacement of the bound electrons or ions, and Equation 361 gives the complex dielectric constant resulting from this displacement by the electric field Fx. In The Complex Permittivity in Chapter 2, we assumed that electronic and atomic polarization can immediately follow the electric field, and there is practically no time lag between Pe (or Pa) and F. This is true only at frequencies much lower than 1013 Hz. In the optical frequency region, the time lag becomes significant. In this case, there is a component of Pe (or Pa) with p/2 lagging from the applied electric field. This component contributes to the dielectric losses. Obviously, the damping force results in such losses due to mechanical friction. In the optical region, e*r is still a complex quantity, which is given by Equation 361. From Equations 361 and 362, we obtain Nq 2 ˆ w 2  w o2 e r = n2  k 2 = 1 + Ê Ë me o ¯ (w 2  w o2 ) + w 2 G 2
(3126) e r¢ = 2 nk =
2 wG Ê Nq ˆ Ë me o ¯ (w 2  w o2 )2 + w 2 G 2
(3127) where N is the density of oscillators (atoms or molecules). These equations indicate that in the neighborhood of w = wo there is an absorption maximum and that n increases rapidly on decreasing w through this region. With continuing decrease in w, n will pass a maximum and then fall asymptotically as w goes further away from wo. The resonance frequency wo is actu
156
Dielectric Phenomena in Solids
ally the frequency at which the AC conductivity 2wnk is maximum, or at which the absorption or the dielectric loss is the highest. The force constant or the damping factor G can be interpreted in this way: the AC conductivity is half the maximum value when w  wo is about G/2. Thus, G is about the bandwidth of the resonance curve, as shown in Figure 332. As w Æ 0,e¢r and hence k approaches zero, n becomes no = [1 + Nq 2 me ow o2 ]1 2
(3128)
This is the undispersed refractive index, generally referred to as the refractive index of a material for w << wo; n2o is also referred to as the highfrequency dielectric constant. However, in general no is different from the static or lowfrequency (or nonoptical) dielectric constant. In Figure 333, the dielectric constant and the loss factor are plotted as functions of frequency. When the loss factor exhibits a maximum at wo, the material in this frequency region is opaque to the electromagnetic wave of frequency in this region. As w rises from values lying below wo, the dielectric constant (or the refractive index) reaches a peak at w1 and then falls off rapidly to a value less than unity at w2, whence it increases again with frequency w and finally approaches unity, as shown in Figure 332. In the region from w1 to w2, an increase in fre
quency results in a decrease in refractive index and an increase in phase velocity. This type of dispersion is generally referred to as anomalous dispersion. In fact, dispersion introduced by the conductivity of the materials is anomalous. Anomalous dispersion occurs pronouncedly in gases. In liquids and solids, the general form of the dispersion curves is not greatly affected. It should be noted that Equations 3126 and 3127 are derived on the basis of a single oscillator, which described well the behavior of er and e¢r in the neighborhood of a single resonance frequency. Actually, a molecule is a complicated dynamic system possessing many natural frequencies, each affecting the reaction of the molecule to the incident field. Furthermore, the interaction between molecules in condensed materials also plays a role in affecting the reaction of the system to the incident field. The location of the natural frequency wo cannot be determined accurately by the classical approach. However, the development of the quantum mechanical theory of dispersion is based on the assumption that the interaction between the excitation field and the absorbing atoms can be represented by a set of linear oscillators, each of which has a resonance frequency corresponding to an optical absorption. Based on this theory, er and e¢r are given by N
2 (w 2  w i2 ) Ê q fi ˆ 2 2 2 2 Ë ¯ i =1 me o (w  w i ) + w Gi
e r = n2  k 2 = 1 + Â
(3129) n
k
n k
w1/wo 1 w2/wo Relative Frequency (w/wo) Figure 332 Refractive index n and extinction coeffiecient k as functions of frequency.
N
2 w Gi Ê q fi ˆ 2 2 2 Ë ¯ 2 i =1 me o (w  w i ) + w Gi
e r¢ = 2 nk = Â
(3130) where fi is the ith oscillator strength, measuring the magnitude of the contribution of this oscillator. For details, see references 91 and 95–98. Equations 3129 and 3130 are closely similar to Equations 3126 and 3127, indicating that the equations involving a set of linear oscillators give a more satisfactory agreement with experimental results over a wide range of frequencies. It can be seen in Figure 333 that the frequencies corresponding to photon energies lower than 1019 Hz cannot excite the electrons
Optical and ElectroOptic Processes
Electronic Polarization Atomic Polarization Orientational Polarization Hopping Polarization Space Charge & InterC facial Polarization
B
157
A
er
1
10–2
1
102
104 (wo)h
106
108
1010
(wo)o
1012 1014 1016 (wo)a (wo)e
1018
Resonance Regime
Relaxation Regime Absorption Band er¢
A
w
(wo)h
0.707 A
(wo)o
(wo)a
(wo)e
Figure 333 The relative permittivities (dielectric constant and loss factor) as functions of frequency.
in the inner shells; thus, these inner electrons will not contribute polarization to the material for frequencies lower than 1019 Hz. In region A, the polarization is due completely to electron polarization. In region B, it is due to the combination of electronic and atomic polarization, and so on. The frequency spectra of er and e¢r are selfexplanatory. 3.3.5 The Franz–Keldysh Effect For narrow bandgap materials, electrons in the valence band may be able to tunnel to the conduction band under a very high electric field. This is referred to as the Zener effect (see Chapter 8, Electrical Breakdown in Solids). The Franz–Keldysh effect is that the electron tunneling probability can be increased by absorption of photons from an illuminating
light beam.99–102 The wave function of a tunneling electron is y 1 = u1 exp ( jkx ) = u1 exp (  k1 x )
(3131)
where k1 is an imaginary wave vector for the electron in the band gap.103 This means that k1 becomes a damping factor in the bandgap. If the wave function y1 decays to a very low value before reaching the conduction band edge, the tunneling probability (or the electron transfer to the conduction band) is very small. This tunneling probability depends on barrier width, which is Dx, and barrier height, which is DE, as shown in Figure 334. Thus, we can write qFD x = D E
or
158
Dielectric Phenomena in Solids
imaginary values of k1 and k2 occur only in the band gap in the longitudinal direction, that is, in the tunneling direction, which is also parallel to the applied field, and they become zero at the band edges. For optical transition, only the transverse (i.e., the vertical momentum) must be conserved. For more details about the treatment of electron tunneling involving photon absorption, see references 102, 108, and 109.
DE ′ hn
DE
x
Conduction Band
Dx′ Dx
Valence Band Figure 334 Schematic illustration showing the photonassisted electron tunneling—The Franz–Keldysh effect.
Dx =
DE qF
(3132)
where F is the applied electric field. It is clear that Dx decreases with increasing applied field F. The wave function of the tunneling electron before reaching the conduction band edge in the band gap is y 2 = u2 exp[  k2 (D x  x )]
(3133)
The overlap of the two wave functions y1 and y2 determines the probability of tunneling. Without light illumination, the barrier width is Dx and the barrier height is DE. However, with photons of energy, hu from light illumination, the barrier width will change to D x¢ =
D E  hu qF
(3134)
The barrier height is also reduced by the illumination, as shown in Figure 334. This implies that the overlap of y1 and y2 is increased, thus increasing the tunneling probability. This phenomenon has been observed in Si, Ge, GaAs, and CdS.104–107 Note that electron tunneling involves only the longitudinal component of the momentum. The
3.3.6 Formation and Behavior of Excitons Absorption and reflectance spectra often show the structure for photon energies below the energy band gap, indicating that there are excited states of energy levels below Ec and above Ev. If the excited states are located at energy level Eex, then the excited electron at this level is electrostatically bound with the hole in the valence band to form an exciton. The binding energy of the exciton is Ec  Eex referred to as a free electron and a free hole, and the absorption or excitation energy is Eex Ev, which is smaller than Ec  Ev = Eg. Excitons are unstable with respect to the ultimate recombination, in which the electron drops into the hole, producing either a photon or phonons. Excitons can be formed in almost any insulating crystals, although some types of excitons are intrinsically unstable with respect to dissociation into free electrons and holes. Excitons can be generated by direct optical, indirect optical, and carrier injection (double injection) processes. In general, when the electron and hole group velocities are equal, the electron and hole may be bound by their coulombic attraction to form an exciton. Excitons can be classified into two groups, based on two different limiting approximations: One group is based on the tightbinding approximation, which was first investigated by Frenkel110 and Peierls,111 and is generally referred to as Frenkel excitons; and the other group is based on the weakly binding approximation, which was first proposed by Wannier112 and Mott,113 and is generally referred to as Wannier excitons. In the former, an excited state of a molecule is a state
Optical and ElectroOptic Processes
in which an electron has been removed from the filled orbital and occupies a previously empty orbital of higher energy, leaving a hole in the original orbital (ground state); the excitation is confined within or near the molecule. In the latter, the molecules (or atoms) are packed so closely that interaction among molecules is strong, which reduces the coulombic interaction between the electron and the hole and hence increases their separation, as shown schematically in Figure 335. In molecular crystals, the covalent binding of atoms within a molecule is much stronger than the van der Waals binding between molecules. This is indicated by the fact that electronic excitation lines of an isolated molecule appear also in the crystalline solid with the same molecules, with only a slight shift in frequency. At low temperatures, the excitation lines are quite
+ (a)
+
(b) Figure 335 Schematic illustration of (a) the Frenkel exciton and (b) the Wannier exciton.
159
sharp, although there may be more structures to the lines in the crystal than in the isolated molecule, due to Davydov splitting.114 On this basis, the Frenkel model of excitons has been used extensively to explain luminescent phenomena. However, Wannier excitons are most common in inorganic materials with covalent or ionic bonds, in which the interaction energy is large and the dielectric constant is high. In dealing with the motion of electrons in a perfect crystal, we usually ignore the mutual repulsion of the electrons. The mutual interaction of the electrons gives rise to scattering and leads to attraction between a hole and an electron, thus forming a Wannier exciton with excited states of various energy levels just below the conduction band. It corresponds, in a sense, to an excited state of an atom of the crystal being passed on to neighboring atoms by quantum mechanical resonance.112 For Frenkel excitons, the exciton radius is of the order of one lattice constant, while for Wannier excitons, the exciton radius is of the order of several lattice constants. This implies that for a tightly binding Frenkel exciton model, the atoms or molecules are well separated, such as those in molecular crystals. In this case, the electron and hole are close to one another and interact by way of coulombic and exchange energies. This means that the excited states of the Frenkel exciton can be characterized by atomic parameters. For the weakly binding Wannier exciton model, a dielectric medium is involved between the excited electron and the hole. This reduces the coulombic interaction between the electron and the hole by er times, implying that the orbit of the excited electron encloses more atoms. This means that the excited states of the Wannier exciton must be characterized by coulombic interaction energy in a dielectric medium. Thus, the optical transition for largeradius Wannier excitons inside the solid should resemble the Rydberg transition in the hydrogen atom. Ignoring, for simplicity, the motion of the center of mass of the electron and hole, the energy levels of the excited states of the Wannier exciton can be written as
160
Dielectric Phenomena in Solids Wavelength (A) 3800
Conduction Band n=3 n=2 n=1
300 n=2
k=0 Valence Band
Figure 336 Schematic illustration of the energy levels of excited states of Wannier excitons.
Cu2O
200
100
0 2
mr e 1 Eex = EH Ê ˆ Ê ˆ 2 Ë m ¯ Ë eo ¯ n
(3135)
where m is the rest mass of the electron and mr is the reduced mass of the electron and the hole, which is given by mr =
me*mh* me* + mh*
(3136)
in which m*e and m*h are, respectively, the effective masses of the electron and the hole; eo and e are, respectively, the permittivities of free space and the material; n = 1, 2, 3, . . . signifies the energy level; and EH is the Rydberg energy, which is the energy of the ground state of the hydrogen atom, that is, when n = 1, which is given by115 EH =
3900
n=3
Excited States Absorption Coefficlent (cm–1)
Energy Levels
mq 4 = 13.53 eV 8e o2 h 2
(3137)
The energy levels of the excited states of the Wannier exciton are shown schematically in Figure 336. So, in inorganic dielectric materials or semiconductors, the excited states of the Wannier excitons appear as additional structure in the energy region below that of the fundamental absorption edge. The absorption spectrum of cuprous oxide (Cu2O) at 77 K is a good example, illustrating the energy levels of the excited states of the Wannier exciton, as shown in Figure 337. The result is from Baumeister.116 The dielectric constant and the reduced mass of Cu2O are 10 and 0.7 m, respectively. Similar
2.15
2.10 Energy (eV )
2.05
Figure 337 Absorption spectrum of an annealed thin Cu2O film.
absorption spectra have also been observed in CdS, CdI2, PbI2, and AgI2.117 In general, the absorption lines created by Wannier excitons can be observed at very low temperatures, because at high temperatures the excitons may be thermally dissociated into free electrons and holes. Between the smallradius Frenkel excitons and the largeradius Wannier excitons is an intermediate case, in which the excited electron remains correlated with the hole and both are located on the same molecule site. But the excited states occur when the excited electron is transferred to the nearest or nextnearest neighboring molecule site and still remains correlated with its parent hole. Such a correlated electron–hole pair with a spatial separation of one or two lattice constants is referred to as a chargetransfer (CT) exciton. In homomolecular crystals, consisting of only one kind of molecules, the absorption line of the CT exciton is very weak, since the energy involved in the optical transition is too close to that for Frenkel excitons. However, in heteromolecular crystals, consisting of more than one kind of molecules (such as CT complexes involving donors and acceptors), the absorption lines are much
Optical and ElectroOptic Processes
stronger. The excited states correspond to the transfer of one electron from the donor (D) to the acceptor (A), implying that the optical transition involves the motion of an electron in the highest occupied orbital of the donor in the molecule of one kind to the lowest unoccupied orbital of the acceptor on the molecule of the other kind, such as hu AD+ A  DAD ææ Æ ADAD+ A  D
Polymers containing donor and acceptor groups may form donoracceptor (DA) complexes with suitable monomers. However, CT excitons can be considered the intermediates in carrier recombination. A CT exciton that is a nearestneighbor pair of an electron and a hole, can move through the lattice and occasionally be dissociated by thermal excitation into a free electron and a free hole; then they recombine, producing luminescence. For more information about CT excitons, see references 118–120. Most organic dielectric materials have weak bonding between molecules, like molecular crystals. In these materials, such as polymers and organic semiconductors, Frenkel excitons play a very important role in optical transition processes. In the following section, we shall discuss briefly the behavior of excitons with particular reference to Frenkel excitons. Exciton Transport Processes Excitation can transfer energy, but not charges, in wave packets of excitation. Excitons consisting of electron–hole pairs can move, implying that the energy can be transported by excitons a certain distance from where they are formed. We mentioned earlier that when the electron and hole group velocities are equal, the coulombic attraction between the electron and hole may form an exciton. If both the electron and hole concentrations are high, the electron–electron and hole–hole coulombic repulsions are large, which tends to reduce the attractive coulombic interaction. The internal field created by the potential fluctuations of the band edges due to high concentrations of both
161
types of carriers tends to separate the electrons and the holes, causing the dissociation of excitons. However, if the internal field is due to a deformation potential, the direction of the force acting on the electron will be the same as that acting on the hole, thus causing the exciton to move as an entity from a large energygap region to a low energygap region. Generally, there are three basic mechanisms of exciton energy transport: Electromagnetic wave packet transport: The energy is transported by a polariton, which is an intimate mixture of a photon and an exciton. When a photon contributes one quantum of excitation to the electromagnetic flux, it will travel as a wave packet inside a crystal.120,121 Hopping transport: If the exciton is selftrapped, it might jump to another site of the perfect lattice along a chain of molecules (e.g., anthracene molecules) until it falls into a trap (e.g., tetracene molecule), as in sensitized luminescence.122,123 Longrange resonance transport: This transfer process is based on the dipole–dipole coupling mechanism, in which it is not necessary to have a chain of molecules to carry the energy. Suppose that an acceptor molecule A undergoes an absorption transition which coincides in energy with luminescent transiton of a donor molecule D, then both may occur simultaneously without involving radiative emission. This implies that the excitation energy is transferred from D to A due to coupling between these two systems. In other words, the photon is absorbed by A before D has finished emitting.124,125 In molecular crystals, the overlap between molecules is small and the electrons are highly localized. This implies that intermolecular interaction is small, and carriers or excitons do not move easily through the solid. However, there are two limiting cases generally used for analyzing exciton transport problems— coherent transport and incoherent transport: Coherent Transport: In coherent transport, the time required for an exciton to transfer from
162
Dielectric Phenomena in Solids
one molecule to another tet is much shorter than the displacement time required for molecules to change from the old to the new equilibrium positions tmd under a change in the force of interaction between neighboring molecules upon excitation of one molecule in the solid. This means that the motion of an exciton is not accompanied by a local lattice deformation, and therefore, can be described using a band model because its mean free path is greater than the lattice spacing, and it can move coherently over several lattice spacings before being scattered. In general, coherent exciton motion may be expected to occur only in ultrapure organic crystals at low temperatures, at which both impurities and phonons are ineffective in limiting the exciton mean free path. Incoherent Transport: The wavelength of the light that is absorbed to create excitons in a crystal is much larger than both the absorption length and the intermolecular separation in most cases. A typical example is l = 5000 Å, a1 = 100 Å, and a = 10 Å. Therefore, it would be expected that some coherence in all excitons should exist at the time of their creation. It probably does exist for a very brief instant, but in most situations, the initial coherence associated with the photon’s spatial extent is washed out by vibrational broadening. Electron–phonon interaction is strong. For incoherent transport in the case of the slow exciton limit, the exchange energies of the exciton are small compared to phonon dispersion energies, and the transfer of the electron between adjacent molecules is ratedetermining. In this slow exciton limit case, the hopping diffusion coefficient decreases with decreasing temperature. However, at low temperatures, coherent diffusion becomes important. In the case of the slow phonon limit, the electron exchange energies are large compared to the phonon dispersion energies, and the transfer of the electron between adjacent molecules is limited by the rate of the phonon transfer. In this case, the hopping diffusion coefficient increases with decreasing temperature.
The overall diffusion coefficient is the sum of the coherent and incoherent contributions. However, it is generally agreed that coherent transport prevails at low temperatures and incoherent transport is dominant at high temperatures. Exciton Interactions There are several possible ways in which an exciton can interact with another exciton or other particles. We shall discuss briefly various exciton interactions that are directly associated with photoluminescence and electroluminescence.
Free Exciton–Free Exciton Interactions
The collision of two free excitons will produce fluorescence or phosphorescence and phonons. Let us take anthracene crystals as an example. The singlet–singlet exciton interaction processes can be described by S1 + S1 Æ S1* + So Æ S1 + So + phonons
fluorescence
or S1 + S1 Æ e + h (autoionization)
or S1 + S1 Æ T1* + T1* (fission)
where S1 and So are, respectively, the excited singlet state (exciton) and the ground states; S*1 and T*1 are, respectively, the singlet and the triplet at high vibronicelectronic levels (hot excitons); and e and h are, respectively, the electrons and holes. The above processes are selfexplanatory. Similarly, we can write the triplet–triplet interaction processes as T1 + T1 Æ S1* + So Æ S1 + So + phonons
fluorescence
or T1 + T1 Æ T1* + So Æ T1 + So + phonons
phosphorescence
Optical and ElectroOptic Processes
These interaction processes have been observed experimentally in anthracene and naphthalene by several investigators.126–129 Free Exciton–Trapped Exciton Interactions
In real crystals, there are always traps capturing excitons. Exciton traps are sites capable of holding the energy that otherwise propagates through the lattice. These traps are generally localized and nonperiodic states in the crystals. Thus, the radiative transiton rate is determined by the specific electronic structure of the trap site. The presence of traps changes the spectral energy distribution, especially the fluorescence and electroluminescence, and also changes the time dependence of exciton population and depopulation. In molecular crystals, three types of traps have been identified: guest molecules, such as tetracene doped in anthracene; defects or lattice imperfections—(structural defects); and selftrapping due to a lattice relaxation induced by excitons.130,131 In general, the molecule that transfers the energy is referred to as the sensitizer, and the molecule that receives the energy is the activator. Either a host molecule or an impurity (guest) molecule can be the sensitizer. Energy transfer implies exciton migration through sensitizers, and the energy eventually given to an activator is referred to as exciton trapping. Let us take free singlet–trapped singlet interaction as example. The interaction process can be written as S1 + ( S1 )trap Æ S1G + So + phonons
non  radiative or radiative transition
For more details about the singlet exciton energy transfer processes, the reader is referred to a comprehensive review [132]. Exciton–Charge Carrier Interactions
Again, we use anthracene as an example. The interactions of singlet excitons or triplet excitons with free electrons or holes, or with trapped electrons or trapped holes, can lead to their annihilation. When the interaction involves trapped electrons or trapped holes, it
163
will give rise to detrapping of trapped carriers, resulting in an increase of photoconduction. Such nonradiative destruction of excitons has been observed by several investigators.133,134 Obviously, exciton–charge carrier interactions lead to a decrease in both fluorescence intensity and exciton lifetime. However, such interactions provide an additional channel for nonradiative exciton decay. In other words, excitons can be quenched by charge carriers.133,134 Exciton–Surface Interactions
There are two processes for quenching the mobile molecular excitons at the boundary between a molecular crystal and an electrode: Charge transfer: An exciton can transfer an electron to an adjacent trapping center at the interface, producing a free hole in the crystal (for example, oxygen molecules adsorbed at the surface can act as electron trap centers). Energy transfer: An exciton can transfer its energy to the acceptor molecules present at or adjacent to the surface of the molecular crystal. Usually, such an electron transfer is a rather slow process compared to the energy transfer between the crystal and an electrode. A metal on the surface of a molecular crystal can influence the electronic states of the surface molecules in two ways: First, it can modify their energetic position; secondly, it can affect the lifetime of excited states. The first effect results from the discontinuity of the dielectric constant across the interface, which leads to a change in the molecular polarization energy. If the polarization is enhanced, surface molecules may act as traps for excitons. The second effect results from nonradiative transitions induced by metallic electrodes. In general, the exciton quenching zone at the surface is very narrow (about 20 Å).135 In the case of electroluminescence, the excitons are generated from electron–hole recombination, and the recombination zone is of the order of 103 Å. Thus, in this case, exciton–surface interactions may not be so important, compared to other nonradiative transitions. However, in the
164
Dielectric Phenomena in Solids
case of photoconduction, the dissociation of excitons at the boundary generates free carriers and is therefore one of the important processes for photocarrier generation. The behavior of excitons in contact with a metal surface has been studied theoretically and experimentally in some detail by several investigators.136,137
Exciton–Photon Interactions
Exciton–photon interactions lead to photoionization of excitons. The photoionization of either singlet excitons or triplet excitons will produce free electrons and holes. This process of producing free electrons and holes by photoionization may compete with the exciton– exciton interactions, which may also produce free electrons and holes by autoionization mentioned earlier.
Exciton–Phonon Interactions
The effects of the interaction between Frenkel excitons and phonons arising from intramolecular vibrations can be summarized as follows138: • The main effect is the reduction of the bandwidth relative to the free exciton value; in general, the upper half of the band is compressed much more than the lower half. • The effective mass of the exciton increases with increasing exciton–phonon coupling because exciton motion is retarded by nuclear displacements. • The wider the free exciton band, the less effective is the exciton–phonon coupling. • Exciton–phonon coupling affects the electronic transition intensity spectrum. The intermolecular vibrations or lattice vibrations interact with phonons, causing a broadening and a shift of exciton energy levels.138 Exciton–phonon coupling greatly affects exciton migration. In extremely pure crystals, the energy transfer rate constant increases with increasing temperature, indicating that exciton– phonon coupling is the dominant pathlimiting mechanism. The nature and the effects of
exciton–phonon interactions are not yet fully understood. However, for details of the present state of knowledge in this area, see references 120, 138, 139.
3.4
Luminescence
Luminescence was known and studied long before the discovery of the quantum picture of atoms by Rutherford and Bohr. Luminescent spectra can provide information about the nature, structure, and excited states of an atom or a molecule in a solid. Luminescence and its related phenomena have been technically employed for various optical devices, including scintillation counters, electroluminescent devices, etc. The process of luminescence is the deexcitation of excited atoms or molecules (or the annihilation of excitons through recombination) by reemission of the absorbed energy as light. Whatever the form of the energy input to the luminescent materials, the final stage in the process is an electronic transition between two energy levels. There are many types of luminescence, depending mainly on the methods of excitation: Photoluminescence: The excited atoms or molecules are produced by the absorption of photons. Cathodoluminescence: The excited atoms or molecules are produced by the bombardment of highenergy electron beams. Many display devices are based on the cathodoluminescent process, employing a luminescent screen made of a layer of small phosphor granules adhering to a glass faceplate, as in cathode ray tubes and television screens. Electroluminescence: Luminescence is due to the recombination of the electrons and holes injected from electrical contacts. Triboluminescence (or sonoluminescence): Excited atoms or molecules are produced by mechanical disruption, such as friction, grinding, or sound and shock waves. Thermoluminescence: Excited atoms or molecules are produced by heat, converting thermal energy to optical energy.
Optical and ElectroOptic Processes
Chemiluminescence: Light emission is due to chemical reactions. Bioluminescence: Excited molecules are produced by biochemical reactions or biological processes, including the motion of electrons, the vibrational energy of nuclei, and the rotational energy of molecules in the macromolecular system. Ionoluminescence (or radioluminescence): Excited molecules are produced by a particles or ions. We discussed thermoluminescence in Section 3.3.3. In this section, we shall confine ourselves to a discussion of photoluminescence and electroluminescence. 3.4.1 Photoluminescence In general, after or during absorption of light photons, a luminescent material will be excited to excited states. The deexcitation will then produce photoluminescence. Photoluminescence is the emission of photons from electronically excited states. It is generally divided into two types—fluorescence and phosphorescence—depending on the nature of the excited states and the ground states. Suppose that a luminescent material is excited by optical excitation from the ground state to the excited state, as shown in Figure 338. If the return of the excited state to the ground state takes place by a spontaneous transition and emits light at a time of about 108 sec after excitation, as shown in Figure 338(a), this luminescent phenomenon is referred to as fluorescence. If, on the contrary, the emission of light takes place with the intervention of a metastable state, followed by the return to the excited state due to the addiEx
Ex Absorption
Metastable State Emission
Absorption Emission Gr
(a)
Gr
(b)
Figure 338 Schematic diagrams showing the absorption and emission processes of (a) fluorescence and (b) phosphorescence.
165
tion of energy, as shown in Figure 338(b), the emission will persist for a period of time ranging from milliseconds to seconds after the excitation ends. This way of emitting light is referred to as phosphorescence. This also implies that for fluorescence, the rate of emission is 108 sec1 and the fluorescence lifetime is 108 sec; while for phosphorescence, the rate of emission is about 1103 sec1 and the phosphorescence lifetime is about 1031 sec. The lifetime is the average period of time an excited electron remains in the excited state. In the excited state of a singlet, the electron in the higher energy orbital has the opposite spin orientation as the electron in the lower energy orbital, that is, the two electrons are paired. In this case, the transition of the electron in the higher energy orbital to the lower one is quantummechanically allowed, thus resulting in the emission of fluorescence. In contrast, for a triplet state, these two electrons, one in the higher and the other in the lower energy orbitals, have the same spin orientation, that is, they are unpaired, so the return of the electron from the higher to the lower energy orbital is not allowed. This implies that a change in spin orientation is needed for the transition of an electron from the triplet excited state to the singlet ground state. Thus, depending on the deexcitation processes, the rate of light emission is small and hence the lifetime is long for phosphorescence. Fluorescence Singlet excitons can be generated not only directly by absorption of light but also indirectly by triplet–triplet annihilation, as discussed in the previous section. Since there is a great difference in lifetime between singlet and triplet excitons (e.g., for anthracene they are about 108 and 102 sec, respectively), fluorescence produced by singlet excitons generated directly by absorption of light or other external means is referred to as prompt fluorescence, and that produced indirectly through triplet– triplet annihilation as delayed fluorescence. The absorption and emission of light in most organic crystals can be described by a simple
166
Dielectric Phenomena in Solids
Autoionization
Internal Conversion
S2
* S1
Internal
S1
T1*
rescence
Weak Absorption S0
Phospho
T1
Fluorescence
Absorption
S1G
Conversion
T2
Intersystem Crossing
T1G
S0
Figure 339 Schematic diagram showing the energy levels of various excited states. S0 is the ground state of the singlet; S1 and S2 are, respectively, the first and second excited singlet states; S*1 is the high vibronic level of S1; S1G is the trapped singlet state; T1 and T2 are, respectively, the first and second excited triplet states; T *1 is the high vibronic level of T1, and T1G is the trapped triplet state. Æ Radiative transition; ~~~> Nonradiative transition; Vibronic levels; — Electronic levels.
energy level diagram, shown in Figure 339. Absorption and emission of photon energy by a bound electron occur between the allowed energy levels and must obey certain selection rules. Important firstorder selection rules are summarized as follows: The change of the orbital angular momentum quantum number must not exceed ±1, that is, D = ±1. The change of the resultant orbital angular momentum quantum number of all the electrons in an atom L must not be beyond 0, +1, that is, DL = 0, + 1 and L = 0 Æ L = 0 is not allowed. The change of the resultant spin angular momentum quantum number of all the electrons in an atom S must be zero, that is, DS = 0.
The total angular momentum quantum number J, that is, the resultant of L and S so that L  S £ J £ L + S, may change by 1, 0, 1, except for J = 0 Æ J = 0, which is forbidden. The value of S is called the multiplicity. For a singlet, S = 0; for a doublet, S = 1/2; and for a triplet, S = 1. All optical transitions between electronic levels are vertical, since this process occurs in about 1015 sec, a time too short for significant displacement of nuclei based on the Franck– Condon principle. In general, fluorescence is the result of a threestage process in fluorescent materials, which are generally called the fluorophors or fluors. These three stages are
Optical and ElectroOptic Processes
Excitation: The fluorophor must absorb a photon of energy sufficiently large to create an excited electronic singlet state. Excited state lifetime: The excited state exists for a period of time of about 109 to 108 sec. During this short period of time, the fluorophor undergoes interactions with surrounding molecules, resulting in two possible changes: intersystem crossing to transfer some of its energy to the triplet state, or internal conversion to bring, by emission of phonons, the excited singlet state to the lowest level S1, which produces fluorescence. Emission: Because part of the energy is taken away during the excitation lifetime and part is dissipated in nonradiative transition, the energy left over for fluorescence is lower; therefore, in the absorption and emission spectra, the wavelength of the emitted fluorescence is longer than that of the excitation (absorption). The difference between the excitation energy huEX and the emission energy huEM is referred to as the Stokes shift. Thus, the quantum yield for the fluorescence ffl can be written as
Number of photons emitted during fluorescence f fl = Number of photons absorbed during excitation
450
490
530 570
1.00
32000 0.80 24000
Perylene in Benzene 0.60
16000
Absorption
Emission 0.40
8000
0.20
00.0 28800
26800 24800 22800 20800 Wave Number
(cm–1
18800
)
Figure 340 Absorption and fluorescence emission spectra of perylene in benzene.
Normalized Fluorescence Intensity
Absorption Coefficient (cm–1)
370 390 410
(3138)
Fluorescence spectra vary widely, depending on the structure and the defects of the fluorophor and also on the solvent in which the fluorophor is dissolved. The typical fluorescence emission spectrum for perylene dissolved in benzene is shown in Figure 340. For perylene, the spectrum shows structure due to the individual vibronic energy levels of the excited and the ground states. The absorption spectrum appears at a lower wavelength than the emission spectrum because of the Stokes shift.140 After optical excitation, the emitted fluorescence will decay with time. The decay process depends on whether it involves one body or two. The former, having the firstorder kinetics, is referred to as the monomolecular or unimolecular mechanism; the latter, with the secondorder kinetics, is referred to as the bimolecular mechanism. These terms are taken from chemical kinetics as synonymous for such processes. A monomolecular reaction involves only one molecule, while a bimolecular reaction
Wavelength (nm) 350
167
168
Dielectric Phenomena in Solids
involves the combination of two molecules. In photoconducting luminescent materials, there occur in all cases monomolecular and bimolecular recombinations. These two kinds of recombination processes are now briefly described. Monomolecular or Unimolecular Mechanism
The rate of decrease of the number of excited electrons n is proportional to n. Thus, we can write dn = a n dt
(3139)
where a is a constant that represents the probability for the annihilation of the excited electrons for luminescence. The solution of Equation 3139 gives n = no exp( a t )
(3140)
where no is the initial value of n, that is, the value just before the excitation ends. Luminescence intensity I = dn/dt, so I can be expressed as I = Io exp( a t ) = a n
(3141)
When a molecule inside a crystal is excited or ionized, the excited or emitted electron is still close to the molecule. It is possible that such an electron will undergo geminate recombination, but the yield would be very low and depends markedly on the electric field. Generally, the emitted electron tends to diffuse away from its parent molecule, as suggested by Onsager.141 However, if the excited electron comes from the molecules inside the crystal and returns to the ground state of the molecules, as in the return of excited singlet state S1 to its ground state So, the process is monomolecular. Bimolecular Mechanism
The rate of decrease of the number of excited electrons n is proportional to n2, since the probability for the annihilation of the excited electrons for luminescence (or recombination) is also proportional to the number of available centers for the recombination. Thus, we can write
dn = bn 2 dt
(3142)
where b is a constant related to the probability of the annihilation of excited electrons. The solution of Equation 3142 yields n=
no (1 + no b t )
(3143)
In this case, n decreases hyperbolically with time. The luminescence intensity is dn = bn 2 dt Io = (1 + Io b t )2
I=
(3144)
The luminescence decays more rapidly as the excitation intensity is increased.142 Recombination processes may involve one body, two bodies, or three bodies. The socalled bodies may mean the quasiparticles that obey the Fermi–Dirac statistics, such as electrons and holes. The recombination that involves one free carrier at a time, such as indirect recombination through a recombination center (e.g., an electron captured by a recombination center and then recombined with a hole, each process involving only one carrier), is generally referred to as monomolecular recombination. The recombination that involves two free carriers simultaneously, such as direct bandtoband recombination, is generally referred to as bimolecular recombination. The recombination that involves three free carriers simultaneously, such as a threebody collision in the Auger intrinsic recombination (in which one electron in the conduction band recombines with a hole in the valence band and the energy released is taken up by a third particleelectron), is generally referred to as trimolecular recombination or threebody recombination (or simply as Auger or impact recombination). So far, we have discussed prompt fluorescence. As shown in Figure 339, some light may be absorbed in the excitation of triplets to their excited states, particularly for the light photons of lower energy—lower than the lowest energy required for creating excited singlets S1 but higher than that for creating excited triplets
Optical and ElectroOptic Processes
T1, although the absorption is very low due to the fact that the optical transition (absorption and emission) is generally forbidden by the firstorder selection rules. However, there is always some way to circumvent the selection rules, so optical transition in triplets is never zero.1 It is possible that the interaction of two triplet excitons leads to indirect creation of an excited singlet by triplettriplet annihilation, resulting in delayed fluorescence emission.143,144 The interaction process can be simply described as follows: T1 + T1 Æ S1* + So Æ S1 + So + Phonons
Delayed Fluorescence
The delay time is approximately of the order of the lifetime of the excited triplet state. The delayed fluorescence intensity is proportional to I 2ex, where Iex is the intensity of the excitation light and depends on the traps in the crystal.118 Furthermore, the interaction between excitons and charge carriers always results in quenching of delayed fluorescence.133,145 Fluorescence spectra under various temperatures and applied electric fields provide a great deal of information about the structure of the material, including structural and chemical defects, as well as charge carriers. Therefore, fluorescence spectroscopy has been widely used for investigating the properties of biological macromolecules.140,146,147
the singlet ground state, producing the socalled alpha phosphorescence. Phosphorescence may be considered a temporary storage of potential luminescence energy in the form of trapped excited electrons or electrons in metastable states. Electrons in metastable states are not allowed to make radiative transitions to lower, unoccupied states by the firstorder selection rules. However, electrons in metastable states may be raised to higher levels, where radiative transitions to lower levels are allowed. In this respect, metastable states are similar to traps. An electron in a particular trap may have to be thermally excited to another, higher level, where it may be able to travel to meet a hole appearing nearby to make a radiative transition. Metastable states acting as traps are responsible for the persistence of phosphorescence. A trapped electron may remain in a trap for some time. It may be released from the trap for a while and then be retrapped in another trap. In this case, the ultimate phosphorescence will be further delayed. In general, thermal excitation is required to release a trapped electron from the trap, as shown in Figure 338(b). The thermal energy comes from phonon interaction with the surroundings. The number of escapes per second for the thermal release of a trapped electron depends on the energy level of the trap and temperature, which, according to the general thermal activation law, can be expressed as p = s exp(  Et kT )
Phosphorescence and Phosphors Shortpersistent fluorescence emission involves transition between states with the same multiplicity, whereas longpersistent phosphorescence involves delays in the quasimetastable states having different multiplicities from the ground state. In this case, there is still a low but appreciable probability of a spontaneous transition to the ground state, producing the socalled beta phosphorescence.1 Metastable states are presumed to be the lowest triplet state in the molecule in which it is possible for an electron to absorb thermal energy to raise the system to a nonmetastable singlet state, whence it can make a delayed fluorescence transition to
169
(3145)
where Et is the energy level of the trap below the conduction band (or the excited state), and s is a constant approximately equal to the rate of natural fluorescence emission, which is of the order of 108 sec1. It can be seen that p decreases with increasing depth of the traps and with decreasing temperature. As the delay time for phosphorescence emission after the original excitation t is equal to 1/p, so the delay time t increases with increasing depth of the traps and with decreasing temperature. For example, for Cudoped ZnS crystals, Et = 0.65 eV below the conduction band edge, the delay time is about three minutes at 18°C and becomes about one day at 50°C.142
170
Dielectric Phenomena in Solids
Materials exhibiting phosphorescence are referred to as phosphors. Since most organic luminescent materials have instability problems at elevated temperatures, low absorption power, and short afterglow, most phosphors are inorganic materials. Artificial inorganic phosphors are not only much more efficient, versatile, and stable than naturally occurring minerals, they are also better defined and hence more suitable for practical applications. Generally, artificial phosphors depend on the presence of some impurity ions, called activators, inside the crystal for persistent luminescence. Such impurity ions usually substitute some of the host ions in the crystal lattice. If the charge of the doped activator ions is not identical to that of the host ions, then it is necessary to introduce other impurity ions, called coactivators, into the crystal to balance the charges. The persistence of the luminescence is directly related to the lifetime of the excited state of the activators. For atomic electric dipole transition, the persistence time is of the order of 108 sec. But for phosphorescence transition, the persistence time can be much longer, as mentioned earlier. For phosphors, the activators and the coactivators are usually considered acceptorlike electron traps and donorlike traps, respectively. There are two types of luminescence: Characteristic luminescence: Excitation, emission, and persistence depend on the activators. Noncharacteristic luminescence: Excitation, emission, and persistence depend on the action of both the host atoms in the crystal
(a)
lattice and the activators, as well as the coactivators. For characteristic luminescence, an electron in the ground state can be excited directly to the activator, and the electron in the activator can make a direct transition to the ground state, producing luminescence. For noncharacteristic luminescence, activators are generally chosen with multiplicity different from that of the ground state, so the direct transition from the activator to the ground state is not allowed. In this case, optical absorption first creates electron–hole pairs in the host lattice. The excited electrons will quickly be trapped in the activators and the holes in the coactivators. The trapped electrons may remain in the traps for some time before being released thermally. The time that an electron spends in the trap depends on the depth of the trap energy level below the conduction band and temperature, governed by Equation 3145, as mentioned earlier. For phosphors involving activators only (i.e., when the charge of the activator is identical to that of the host atom it replaces), some of the thermally released electrons may make a transition to the valence band, producing luminescence, and some may go on to be retrapped before being detrapped again to make a luminescent transition, as shown in Figure 341(a). For phosphors involving both activators and coactivators, the thermally released trapped electrons may have a better chance to recombine with holes trapped in the coactivators, as shown in Figure 341(b). It should be noted that transition between donors and acceptors can be very efficient. Many phosphors have activators
Ec Eact
Ec Eact
Ev
Ecoa Ev
(b)
Eact
Ec
Ecoa Ev
(c)
Figure 341 Schematic diagrams showing the optical absorption and emission process in (a) phosphors involving activators only, (b) phosphors involving activators and coactivators, and (c) phosphors involving donoraccepted recombination.
Optical and ElectroOptic Processes
as acceptors and coactivators as donors. These two impurity atoms can be thought of as an impurity molecule formed by their coulombic interaction, as shown in Figure 341(c). The electron in the activator can recombine with the hole in the coactivator, producing luminescence hu = Eg  ( Eact + Ecoa ) +
q2 4per
(3146)
where r is the separation between the donor and the acceptor, and e is the permittivity of the phosphor. Obviously, the emission spectrum would be broad, due to the large range of the possible impurity atom separations. In fact, the emission of red light from GaP is due to Zn substituting for Ga and 0 substituting for P in the GaPdoped crystal, with Zn and 0 forming a donoracceptor complex.148 Group II–VI compounds are an important class of luminescent materials. ZnS is one of these materials that has been extensively studied. In general, the electronic properties of group II–VI compounds are between those of group I–VII and group III–V compounds. For example, the energy band gap of ZnS is about 3.7 eV, as compared to about 9.4 eV for KCl and 1.4 eV for GaAs. Regarding the bonding of atoms, the ZnS lattice is about 75% ionic, compared to predominantly ionic KCl and predominantly covalent GaAs. Most widely used phosphors are made of group II–VI compounds activated by suitable impurities as activators and coactivators. As mentioned earlier, the charge balance is important when choosing impurities to replace the host atoms. For example, ZnS:Cu means ZnS activated by Cu activators, Cu+ to replace Zn2+ creates a charge imbalance problem. So, it is necessary to introduce another impurity ion, such as Ga3+, into the crystal as coactivator to compensate for the charge difference. In this case, one Cu+ and one Ga3+ replace two Zn2+. Alternatively, a halide ion, such as Cl, can be used to replace S2. In this case, the Cu+ and Clpairs do not produce any charge imbalance problem. On the basis of the basic principles for phosphors given here, the properties of phosphors, including persistence and the luminescence
171
spectrum, can be tailored to suit any particular applications by selecting suitable impurities for activators and coactivators. For example, the phosphors used for the color displays involve the production of three primary colors: blue, green, and red. The phosphors commonly used for this purpose are ZnS:Ag for blue, ZnxCd1xS:Cu for green, and Y2O2S:Eu,Tb for red.5 For more details about phosphors and luminescence in general, see references 103, 142, and 148–150.
3.4.2 Electroluminescence Electroluminescence in a broad sense is the phenomenon of converting electrical energy into light energy. This implies that luminescence can be produced by electrical activation. There are two major types of electroluminescence. One type does not involve carrier injection from electrical contacts; this type is generally referred to as classical electroluminescence. The other type involves carrier injection and is generally referred to as injection electroluminescence.
Classical Electroluminescence Without involving charge carriers injected externally through electrical contacts, this type of electroluminescence is sometimes referred to as intrinsic electroluminescence. In this case, the excited electrons must be produced by electrical activation. The idea of intrinsic electroluminescence was first proposed and developed in 1936 by Destriau, who used a thin layer of phosphor powder suspended in an insulating medium.151 The early structure of this type of electroluminescence (EL) device is very simple. The phosphor powder (usually ZnS:Cu phosphor particles) is suspended in a transparent insulating medium and sandwiched between two electrodes, one of which is transparent. Later, instead of using the phosphorpowder dispersion method (which has many disadvantages, such as short life, low stability and brightness), the techniques of producing thin phosphor films by vacuum deposition or
172
Dielectric Phenomena in Solids
other methods were developed.152–154 We shall discuss briefly the performance of such thin phosphor film EL devices, but before doing so, we would like to mention two possible mechanisms that may be responsible for intrinsic electroluminescence: electron tunneling and impact ionization.155
Electron Tunneling Mechanism
If the phosphor film is thin and the applied electric field is sufficiently high, electrons at the acceptor level may be able to tunnel to the conduction band and subsequently recombine with the hole (empty acceptor) nearby, producing luminescence, as shown in Figure 342(A).
Photon
Ec
Electron Energy
Ec
Ev
Ev Distance
(a)
(b)
(A)
Electron Energy
Photon Ec
Ec
Ev
Distance
Ec
Ev
(a)
(b)
Ev
(c)
(B) Figure 342 Schematic diagrams showing possible mechanisms for producing electroluminescence, (A) involving tunneling: (a) an electron in the acceptor state may tunnel to a state in the conduction band of the same energy, and (b) this electron may then fall into an empty acceptor state, resulting in radiative emission; (B) involving impact ionization: (a) an electron moving in the high electric fields may acquire sufficient energy to produce an electron–hole pair by impact ionization, (b) the hole may recombine with an electron in the acceptor state, and (c) the electron may then fall into the empty acceptor state just created by (b), resulting in radiative emission.
Optical and ElectroOptic Processes
Impact Ionization Mechanism
Electrons in the conduction band that are accelerated under a sufficiently high field may acquire enough energy to cause impact ionization in the material, producing electron–hole pairs. The holes will quickly be trapped at the acceptor sites nearby, while the electrons in the conduction band will move until they find suitable empty acceptor sites and then recombine with holes there, producing luminescence, as shown in Figure 342(B). This phenomenon has been observed in the ZnS:Mn phosphor film EL devices. The typical thinfilm EL device is the LUMOCEN (LUminescence from MOlecular CENters). This EL device consists of phosphor with special luminous centers, made of rare earth–halide molecules.153 Figure 343 illustrates schematically a representative structure of a LUMOCEN device. Normally, ZnS phosphor is used as the host phosphor material and TbF3 as the luminous centers. The SnO2 film serves as the transparent electrode. However, this structure has not been developed further for practical applications because of many inherent shortcomings. Several better thinfilm EL devices have been developed, including ZnS:Mn thinfilm EL devices, radiofrequency sputtered ZnS:Mn, Cu thinfilm EL devices, ZnS:Mn thinfilm EL devices with double insulating layer structure, etc.154,156 We use the ZnS:Mn thinfilm EL device with a double insulating layer structure as an example to show the typical performance of classical electroluminescence devices. Figure 344(a) illustrates schematically the fundamental structure of the EL active film sandwiched between two insulating layers. These two insu1 2 3 4 5 Figure 343 Schematic diagram showing the basic structure of a LUMOCEN device. 1: metal electrode (Al); 2: ZnS:TbF3 film (1500 Å); 3: HO2 film (3000 Å); 4: SnO2 film (2000 Å); 5: glass substrate.
173
lating layers prevent leakage current from flowing through the EL film and keep the applied electric field for producing luminescence across the active element of ZnS:Mn phosphor. The materials for the insulating layers must have a high breakdown strength and a high dielectric constant, so that they do not take away a large portion of the applied field, and they must be transparent. Usually, Y2O3, Si3N4, or Al2O3 is used for insulating layers. The general performance of this device is good and has a long life of operation. This device emits bright, yellowishorange light under an AC field. The luminescence spectrum is not affected by the amplitude of the driving AC field and frequency. The typical brightnessvoltage characteristics of this device are shown in Figure 344(b). The brightness depends strongly on the applied voltage in the lower voltage region and tends to saturate in the higher voltage region. The brightnessvoltage characteristics shift to higher voltages as time elapses, but the saturation value does not change. This shift is not due to the degradation of the device but to a kind of stabilization process similar to the thermal annealing process. After the completion of such a stabilization process, the device becomes extremely stable for three years, without any change in brightness. The stabilization process can be accelerated by elevating the temperature and applying a suitable voltage on the device at the same time. For example, if a voltage in the saturation region is applied across the device at 200°C, the time required to complete the stabilization process is within one hour.156 Injection Electroluminescence Injection electroluminescence is sometimes referred to as extrinsic electroluminescence, because the electrons and holes undergoing radiative recombination are supplied externally by carrier injection through electrical contacts. Light emission from electrical contacts is, of course, very similar to light emission from p–n junctions, on which most lightemitting diodes (LED) and semiconductor lasers are based. However, for many luminescent materials, such
174
Dielectric Phenomena in Solids
5 6
2,140 hrs t = 80,90,10
4
t = 16
3
102
t=1
2
t=0
1
Brightness (arbitrary units)
103
10
(a)
5 kHz
1 150
200
250
300
Applied Voltage (Volts)
(b) Figure 344 (a) Schematic diagram showing the ZnS:Mn thinfilm electroluminesence device with a doubleinsulating layer structure, 1: metal electrode (Al); 2: insulating layer (2000 Å); 3: active layer ZnS:Mn film (5000 Å); 4: insulating layer (2000 Å); 5: SnO2 transparent electrode; 6: glass substrate, and (b) the brightnessapplied voltage characteristics of the ZnS:Mn thinfilm device.
as molecular crystals and II–VI compounds, p–n junctions are not feasible. In such cases, other methods of carrier injection must be used. In the following sections, we shall discuss briefly some commonly used methods of carrier injection. Carrier Injection from Electrical Contacts
Filamentary ChargeCarrier Injection in Solids in Chapter 7 discusses the theory of filamentary double injection in solids. It is likely that multiple current filaments may simultaneously exist between two parallel plane electrodes. In such a case, we can always consider that within a domain of radius rd is enclosed only one current filament and that the total current between the plane electrodes may be expressed as IT = Idomain1 + Idomain 2 + . . . = Â In HI n
(3147)
This means that the total current can be represented by the current in one domain I multiplied by a constant H. We can also assume that the current is uniformly distributed within the area of pr 2d, provided that rd is small enough to satisfy this condition. In molecular crystals—for example, in undoped and doped anthracene—both the electron and hole mobilities are generally small and the recombination rate constant is large, resulting in a small space charge overlap. Thus, the simultaneous injection of electrons and holes from the contacting electrodes will produce twocarrier space charge limited currents within the filament, and lead to electroluminescence when two types of carriers meet and recombine radiatively. After the onset of electroluminescence in a molecular crystal with a fixed emission spectrum, the electroluminescent brightness is gov
Optical and ElectroOptic Processes
erned by the external quantum efficiency,148 hq, given by hq = hihghe = hinthe
(3148)
where hi is the carrier injection efficiency, which is the ratio of the current due to minority carriers to the total current. If it is assumed that Jn is the current due to minority carriers, then hi = Jn ( Jn + J p )
(3149)
hg is the light generation efficiency; hint = hihg is the internal quantum efficiency, which is a function of the total current density and temperature of the electroluminescence specimen; and he is the light extraction efficiency, which is defined as the ratio of power loss due to the light transmission within the electroluminescence specimen to the total power losses, which consist of both the losses in the bulk and on the surface. This can be considered fixed for a given specimen. For double injection, the recombination of the injected electrons with the injected holes in the molecular crystal will yield singlet and triplet excitons. It is generally accepted that the singlet excitons producing fluorescence are partly generated directly by electron–hole recombination and partly generated indirectly by triplet–triplet recombination in pairs, according to the following relation157,158: 20(e + h) Æ 5 [ S ]dir + 15 [T ] Æ 5 [ S ]dir + 3 [ S ]ind
where e and h represent, respectively, the electron and the hole; [S]dir and [S]ind represent, respectively, the singlet excitons produced by the direct and the indirect processes; and [T] represents the triplet excitons. It is the efficiency of generating [S]dir and [S]ind and their subsequent population in the crystal that governs the electroluminescent intensity, but the threshold voltage is mainly governed by local field effects on the electrode surfaces. Since there is a great difference in lifetime between the singlet and the triplet excitons in molecular crystals (for example, in anthracene they are 108 and 102 sec, respectively), the total electroluminescence consists of prompt
175
electroluminescence due to [S]dir and delayed electroluminescence due to [S]ind and exhibits time constants corresponding to both of these decays. In the steady state, however, electroluminescence is the combination of these two. Through a semitransparent planer electrode, Hwang and Kao have observed that electroluminescence in anthracene occurs within a single filament, and its brightness decreases with increasing distance from the center of the filament in a manner similar to the variation of the current density with radial distance described in Filamentary ChargeCarrier Injection in Solids in Chapter 7.159 As the applied voltage is increased, multiple filaments are observed and the overall electroluminescent brightness increases. Since the normal parallelplane electrodes have sharp edges, the filaments are generally formed near the edges, because the field is higher there.159 Electroluminescent intensity (or brightness) is dependent on the injection current density. At a high injection level, bimolecular decay is dominant, so the electroluminescent brightness is proportional to the injection current. At a low injection level, monomolecular decay becomes dominant, so the electroluminescent brightness is proportional to the square of the injection current.131,159,160 Some typical results for the total brightness BT as a function of the injection current I for anthracene are shown in Figure 345. The experimental results are from Williams and Schadt161; Schwob and ZschokkeGranacher163; Kawabe, Masuda, and Namba164; and Hwang and Kao.159 If the currentvoltage (IV) characteristics are known, the relationship between electroluminescent brightness and applied voltage can easily be deduced. It is most likely that prior to the onset of observable electroluminescence, the current is dominated by one type of charge carrier from one electrode, the other being a neutral or blocking contact. But when the applied voltage V > Vth, the space charge built up near the blocking contact becomes sufficient to turn on the carrier injection; therefore, the current increases sharply to another regime. In this regime, both types of carriers, holes and electrons, play almost equally important roles in the conduction current, and both electrodes
176
Dielectric Phenomena in Solids 10
Brightness (arbitrary units)
BT •1 1
BT •1 10–1 BT •12 10–2 BT •12 10–3 10–8
10–7 10–6 Current (A)
10–5
Figure 345 Electroluminescent brightness as a function of current for (a) undoped anthracene crystals and (b) anthracene crystals doped with tetracene. Solid curves are based on the theory and experimental results are from Williams and Schadt,161 , Mehl and Funk, ,162 Schwob and ZschokkeGränacher ,163 Kawabe, Masuda, and Namba ,164 and Hwang and Kao, 159
under such a condition can be assumed to be ohmic contacts, but the effects of fieldenhanced detrapping and reabsorption of electroluminescence are excluded. If these effects are taken into account, it would be expected that I and hence BT would increase more rapidly with V. This trend of BT V relationship has been observed in anthracene.159 Electroluminescent intensity is also dependent on temperature. The temperaturedependent phenomenon may be explained in terms of three processes: • Exciton–trapped exciton interactions • Exciton–carrier interactions • Exciton–surface state interactions, which control the electroluminescent intensity and are temperaturedependent The surface states at the interface between the contacting electrode and the anthracene crystal
quenches singlet excitons, and the quenching rate decreases with increasing temperature. However, the effect of surface states may be very small compared to those of processes 1 and 2,145 and for most cases, process 3 may be ignored. If the temperature for peak electroluminescent brightness is defined as the brightness characteristic temperature Tb, then it is possible that for temperatures lower than Tb, process1 is dominant, and for temperatures higher than Tb, process 2 becomes important. Tb can be thought of as the characteristic temperature of these processes, at which the singlet excitonattemptescape frequency is equal to the carriersinglet exciton reaction rate.159 For temperatures lower than Tb, brightness increases with increasing current. Since BT is proportional to I in the highinjection case, the temperature dependence of BT can be explained in terms of the temperature dependence of I. For temperatures higher than Tb, brightness decreases although the current still increases with increasing temperature, and electroluminescence disappears at a certain temperature, depending on the applied voltage. It has been experimentally observed that the interaction of singlet excitons165 or of triplet excitons133 with charge carriers quenches fluorescence. The change of temperature may not greatly affect the carrier injection from the electrodes, but it would greatly affect the ratio of the free carrier density to the total carrier density, which includes both free and trapped carriers. Typical temperaturedependent electroluminescence results are shown in Figure 346. The experimental data are from Hwang and Kao.159 It should be noted that the nature of exciton–trapped exciton interactions and carrier–exciton interactions is still not fully understood. However, the argument here serves, at least, to explain qualitatively this temperaturedependent phenomenon. Electroluminescence consists of two components: the fast component (generally referred to as prompt electroluminescence) and the slow component (generally referred to as delayed electroluminescence). The “fast” light transient
Optical and ElectroOptic Processes
1.6 1.4
a
Brightness (arbitrary units)
1.2 1.0 0.8
b
0.6 0.4 0.2 0 –40
–20
0
20 40 60 Temperature (°C)
80
100
Figure 346 Electroluminescent brightness as a function of temperature for undoped anthracene crystals of about 1 mm in thickness for (a) 1.2 kV applied voltage and (b) 1.0 kV applied voltage.
marks the time when the two leading carrier fronts meet in the specimen, while the “slow” light transient involves triplettriplet annihilation and electron and hole detrapping processes. The time dependence of the “fast” current transient enables the determination of the carrier recombination rate constant, and the “slow” current transient can be used to monitor any change of exciton generation rate that may arise from a decrease of mobile carriers due to trapping. The steady state (or DC) electroluminescence spectrum is independent of the electrode material but depends on temperature and crystal preparation. Under pulse voltage conditions, however, a carrierinjection mechanism of a normally blocking contact becomes apparent. Electroluminescence first appears at the time, after the application of a voltage pulse, corresponding to the transit time of d2/ (mn + mp)V in cases of both electroninjecting and holeinjecting contacts. But in cases of one electroninjecting contact and one normally holeblocking contact, electroluminescence appears at the time corresponding to the transit
177
time of electrons alone, that is, on the arrival of the electron space charge front at the anode to enhance the hole injection. In cases with two carrierinjecting contacts, electroluminescent intensity is proportional to the current, irrespective of the current level, while in cases with only one carrierinjecting contact and one normally blocking contact, the relationship between the electroluminescent intensity and the current depends on the current level.161 Electroluminescent intensity depends on the frequency under applied sinusoidal AC fields. Using a sodium electrode as the electroninjecting contact and a silver electrode as the holeinjecting contact (a silver electrode is a holeblocking contact at low fields and can become a holeinjecting contact only at high fields), Kunkel and Kao have studied electroluminescence under continuously sinusoidal AC fields at various temperatures.166 The typical wave forms of the AC voltage applied across the specimen and the corresponding electroluminescence produced in it are shown in Figure 347. It can be seen that electroluminescence appears only when the silver electrode is at the positive voltage halfcycles, indicating that neither the sodium electrode injects holes nor the silver electrode injects electrons, that there is a time delay (td) between the time when the voltage is applied and the time when the electroluminescence appears, and that there is also a phase shift (q) between the peak of the applied voltage and the peak of the electroluminescent intensity. Peak electroluminescent brightness as a function of frequency for various temperatures is shown in Figure 348. Brightness decreases monotonically with increasing frequency. Brightness increases with increasing temperature, reaches a peak at a certain critical temperature, and then decreases with increasing temperature in a manner similar to that for DC electroluminescence, discussed earlier. The delay time (td) shown in Figure 347 is also frequencydependent, as shown in Figure 348 in a dashed curve. The phase shift q also increases with increasing frequency; it is not noticeable at 20 Hz but becomes significant at 5000 Hz. The leading portion of the wave form of
Dielectric Phenomena in Solids
td
q
1.6 4
1.4 1.2
3
1.0 0.8 0.6 0.4 0.2 0
1.0
a b
2
c d e
1
2.0 3.0 4.0 Frequency, kHz
Delay time, msec
Peak brlghtness (arbltrary units)
178
5.0
(a) Figure 348 The peak electroluminescent brightness (solid curves a–e) and the delay time (dashed curve) as a functions of frequency of the applied sinusoidal AC voltage of 1600 V peak to peak at various temperatures, a: 20°C, b: 30°C, c: 40°C, d: 0°C, e: 20°C. The delay time is measured at 40°C.
Carrier Injection through P–N Junctions
(b) Figure 347 Oscillograms illustrating the waveform of AC voltages and that of corresponding electroluminescence, which appears only when the silver electrode is at the positivevoltage half cycle, td is the time delay and q is the phase shift. (a) frequency: 500 Hz, temperature: 40°C, vertical scale: voltage, 400 V/div; brightness, 0.5 V/div; horizontal scale: time, 0.5 msec/div; (b) frequency: 5000 Hz, temperature: 20°C, vertical scale: voltage, 400 V/div; brightness, 0.1 V/div; horizontal scale: time, 0.05 msec/div.
electroluminescence is similar in shape to that of the applied voltage for all frequencies, but the tailing portion is different. There is a significant exponential tail developed on the trailing edge at high frequencies, as shown in Figure 347(b). Usually, when the applied voltage reaches the zero point, the electroluminescence wave form becomes exponential, since beyond this point light output results predominantly from delayed fluorescence.
Most LEDs and semiconductor lasers are based on the principle of p–n junctions under forwardbias conditions. Several p–n junction structures formed by luminescent materials produce injection electroluminescence.167 In this section, we will briefly describe some of the most commonly used p–n junction devices for electroluminescence. P–N Homojunction Devices—Since group IV elements, such as Si and Ge, are not luminescent materials, and group II–VI compounds cannot be readily doped to form n or ptype materials, group III–V compounds are the major luminescent materials for p–n junctions. For example, p–n junctions are readily formed in GaAs by doping with Si as donors by replacing Ga, or as acceptors by replacing As. Similarly, p–n junctions can be formed by diffusing Zn into pulled crystals of nGaAs. P–n junctions can be made as step (or abrupt) junctions, in which the ptype semiconductor is uniformly doped with acceptor impurities and the ntype semiconductor is uniformly doped with donor impurities up to the metallurgical junction. P–n junctions can also be made as
Optical and ElectroOptic Processes
graded junctions, in which the concentration of the doped acceptor and donor impurities are distributed either linearly or following a particular distribution function up to the metallurgical junction. However, when a p–n junction is formed, the requirement of the constant Fermi level throughout the device in thermal equilibrium results in the formation of a depletion region due to the transfer of electrons and holes across the junction, as shown in Figure 349. A full discussion of the p–n junctions is beyond the scope of this book. For details, see the standard references, such as reference 168. Here, we will use abrupt p–n junctions to illustrate the basic concept of p–n junctions’ production of light emission. The basic normal p–n junction is shown in Figure 349(a). For example, GaAs has an energy bandgap of 1.43 eV corresponding to the wavelength of 861 nm. The most probable energy of the electrons in the conduction band is kT/2; thus, the wavelength of the emitting light due to bandtoband transition is slightly shorter than 861 nm. Furthermore, the light produced will be attenuated due to selfabsorption during its travel to the surface of the semiconductor (i.e., the semiconductor–air interface). The light intensity will be reduced by exp(a), where is the length of the semiconductor. Reaching the surface, part of the light will be reflected according to the reflection coefficient R given by Equation 357. So, the external quantum efficiency hq can be written as hq = hint (1  R)(1  cosq c )exp( al)
(3150)
where qc = sin1(1/n), n is the refractive index of the semiconductor, and hint is the internal quantum efficiency, which is given by hint =
Radiative Transition Ê Radiative Transition + ˆ Ë Nonradiative Transition¯
(3151)
In general, all recombination processes involve both radiative and nonradiative transitions. For radiative transition, the effective carrier lifetime is tR, and for nonradiative transition it is tNR. The internal quantum efficiency can also be expressed as
1 tR 1 t R + 1 t NR 1 = 1 + (t R t NR )
179
hint =
(3152)
Thus, to achieve high hint, the tNR must be made as long as possible. However, although hint may be close to 100%, the actual hq in practical LEDs is generally less than 10%. Since radiative transition is not limited to bandtoband recombination, depending on the dopants and their concentration, radiative transition may take place between the conduction band and the acceptor level or between the valence band and the donor level. In this case, the peak of the light emission spectrum may not occur at 861 nm but at a longer wavelength. For example, the peak of the electroluminescent emission spectrum for an Sidoped GaAs LED occurs at wavelengths between 910 and 1020 nm. In general, light emission intensity is proportional to forwardbiased current I at high current levels, that is, under high forwardbias conditions, in which the radiative transition occurs mainly outside the depletion region due to diffusion current. At low current levels, that is, under low forwardbias conditions, the radiative transition takes place mainly in the depletion region; hence, the light emission intensity is proportional to I2 due to the recombination current in the depletion region. To reduce the reabsorption (or selfabsorption) of the emitting light in the semiconductor, p–n junction LEDs usually have one side much more heavily doped, as shown in Figure 349(b), or both sides heavily doped, as shown in Figure 349(c), since the emitting photons have an energy of Eg lower than the reabsorption energy level, which is Eg + DE. When both sides of the junction are heavily doped, the nside becomes n+ degenerate material and the Fermi level lies inside the conduction band. Similarly, for the p+ degenerate material on the p side, the Fermi level lies inside the valence band. In this case, when the junction is forwardbiased with a voltage nearly equal to Eg/q, the numbers of electrons and holes injected across the junction are sufficient
180
Dielectric Phenomena in Solids
In Thermal Equilibrium PType
With Forward Bias NType
PType
NType
Metallurgical Junction Ec
EC
EC EF
hn EC
EF EV
EF
EF
hu
EV
hn EV
EV
Neutral Region
Depletion Region
Neutral Region
(a) EC
EC
DE EF EV
EF
EF
EC
EV
EF EC
hu EV
EV
(b) EC
EC
DE EV EF
EC
hn EV
EF
DE
EF
hu
EF EV
EC
EV
(c) Figure 349 Schematic diagrams illustrating p–n junctions for injection electroluminescence, (a) the normal p–n junction, (b) the p–n junction with the n–side heavily doped, and (c) the p–n junction with both the n–side and the p–side heavily doped.
to create a population inversion in a narrow region, called the active region. The thickness of the active region is approximately of the order of the minority carrier diffusion length. The radiation produced by recombination in
that region may interact with valence electrons and be absorbed, or interact with electrons in the conduction band, thereby stimulating the production of further photons of the same energy. If the injected carrier concentration
Optical and ElectroOptic Processes
becomes large enough, the stimulated emission can exceed the absorption, so the optical gain can be achieved in the active region, resulting in laser oscillations.
made either ntype or ptype by adjusting the value of x.168
3.5 P–N Heterojunction Devices—When the ptype material and the ntype material, having different energy bandgaps, form a p–n junction, such a junction is called the p–n heterojunction, as shown in Figure 350(a). When a forwardbias voltage across the junction is sufficient to flatten the valence band edges, as shown in Figure 350(b), holes are injected freely into the ntype semiconductor without a barrier. But it is difficult for the minority electrons to be injected into the ptype semiconductor because of the large barrier height. Obviously, radiative recombination will then occur in the lowergap semiconductor, as shown in Figure 350(b). For example, in the p(GaAs)n(GaSb) heterojunction, the injection electroluminescence occurs at about 0.7 eV, which is near the energy bandgap of nGaSb. The largergap semiconductor side. such as pGaAs is, in general, transparent to the radiation generated in the lowergap semiconductor and therefore serves as a window for transmitting the radiation. In practice, heterojunctions suffer from interfacial problems. In order to make a compromise with this interfacial difficulty, p–n heterojunctions can be made from different compositions of miscible alloys having similar lattice constants, such as Al1xGaxAs. This alloy can be
PType
181
Photoemission
Photoemission is generally referred to as emission of electrons into a vacuum from a solid, or injection of electrons or holes from a solid into another solid, resulting from an interaction between photons and a solid. The photoemission of carriers from a solid into a vacuum is referred to as external photoemission, while that from a solid into another solid (such as from a contact electrode to a semiconductor) is referred to as internal photoemission. Photoemission has been extensively studied as a tool to study energy levels, particularly ionization energies of molecular crystals,169,170 as well as to obtain information about the injecting contact, potential barriers, surface states, and electronic structures of solids.171–173 In this section, we shall discuss photoinjection from a contacting electrode to a crystalline solid and photoemission from a crystalline solid to a vacuum. 3.5.1 Photoemission from Electrical Contacts An extensive compilation of experimental data on this subject is available in the literature for inorganic semiconductors,171,174 as well as for organic semiconductors.173 Metallic contacts
NType
PType
NType
Ec
Ec
Ec EF
Eg1 Ec EF
EF Ev
Eg2
Hole Emitter
EF Ev
qV
hu
Ev
Ev Luminescent Region
(a)
(b)
Figure 350 Schematic diagrams illustrating a p–n heterojunction for injection electroluminescence: (a) in thermal equilibrium and (b) with forward bias to bring the valence band edges of both sides to the same level.
Dielectric Phenomena in Solids
can be roughly classified into two groups: ohmic contacts and blocking contacts.175 An ohmic contact can be considered a reservoir of carriers that are always ready to supply as many carriers as needed. Usually, at a given field, the ohmic contact can supply more carriers than the bulk material can carry. Thus, the current is bulklimited. Further increase in currentinjection by photoexcitation does not affect the current; therefore, no photoemission current can be observed. A blocking contact can inject only a very few carriers—much less than the bulk material can carry. Thus, the current is contact limited. If a light of energy hu ≥ fB (where fB is the potential barrier height—the difference between the Fermi level of the metal and the conduction band edge of the semiconductor, as shown in Chapter 6, Figure 64) illuminates the metallic contact, photoinjection from the contact will take place. The photoemission, without taking into account the effects of scattering and relaxation, can be written, according to the Fowler theory176,177 as J ph = C( hu  f B )2 for hu ≥ f B
(3153)
This equation is valid only for fB ≥ 0.5 eV, that is, if hu  fB is greater than some multiple of kT (>6 kT) or hu £ 1.5fB. Beyond this range, the assumptions for the simple Fowler theory are no longer valid.178 Furthermore, Equation 3153 is valid only for photoinjection from a metal to a semiconductor having wide energy bands (with bandwidths larger than 0.5 eV). Most metals, inorganic semiconductors, and insulators can satisfy these conditions. For materials and conditions for which Equation 3153 is valid, the measurements of Jph as a function of hv, and then the extrapolation of the plot of J 1ph2 versus hv to Jph = 0, yields fB. However, Equation 3153 cannot be applied to narrow energy band materials, such as most lowmobility organic semiconductors (e.g., anthracene). In narrow energy band materials, an electron injected into the narrow band can diffuse only a few angstroms (about 5 Å) and would then be captured in a bound state of the coulomb image potential (see Figures 612 and 613). There
fore, an injected electron must have a sufficient momentum perpendicular to the surface before it can escape from the image force to enter the conduction band. From a Metal into Wide Bandwidth Semiconductors This is the most common case, and it has been treated in detail by investigators.177–179 As mentioned before, in this case, photoemission measurements would directly yield the barrier height of the blocking contact fB. For semiconductors for which the imageforce effect is negligible, the photoemission method is reasonably accurate for determining fB. A typical example is given in Figure 351 for a gold contact to a CdS crystal specimen, in which fB = 0.7 eV is obtained for this contact potential barrier height. The experimental data are from Goodman.180 A similar agreement to the Fowler theory has also been reported for Si and for other inorganic semiconductors.181 By measuring the threshold energy hv0 = fB for electron emission and that for hole emission, the sum of these two threshold energies gives the energy band gap of the semiconductor. For example, the threshold energy for electron emission from Au to nGaP is 1.30 eV182 and that for hole
(Relative photocurrent/incident photon)1/2
182
10 9 8 7 6 5 4 3
fB + = 0.7 ev
2 1 0 0.6
0.7
0.8 0.9 hu (eV )
1.0
1.1
Figure 351 (Relative photocurrent per incident photon)1/2 as a function of photon quantum energy for an evaporated gold contact to a cadmium sulfide crystal specimen.
Optical and ElectroOptic Processes
emission from Au to pGaP is 0.72 eV.183 The sum of these is 2.02 eV, which is about the energy band gap of GaP, which is 2.18 eV.184 It should be noted that the barrier heights determined by means of photoemission measurements depend on the specimen’s surface conditions. The effects of surface states have been discussed by several investigators.180,181 For large bandgap materials, the Fowler plot at hu close to hu0 is usually not linear, which means (Jph)1/2 is not proportional to (hu  fB), or deviates from the linear Fowler plot. Figure 352 shows a typical (Jph)1/2 versus hu curve for an MIM (metalinsulatormetal) structure; the results are from Kadlec and Gundlach.185 The asymmetry of AlAl2O3Al (f1 > f2) shown in Jpn
f1
fB
f2
30
AI
S AI oxide
AI
20
1/2
Jph (arb. units)
Xm
183
the inset of Figure 352 is probably due to the different prehistories of the two interfaces. This nonlinear behavior or deviation has been observed by many investigators,186,187 and makes it difficult to determine accurately the value of fB. Several factors may be responsible for this deviation178: • The electron distribution may be smeared out about the Fermi level, but the deviation is too large to be explained by this effect. • The scattering of electrons in the conduction band may play a role, but it is likely that it can be important for thick specimens and not for films thinner than 50 Å. • The quantum mechanical transmission coefficient, which affects the photocurrent, is not equal to zero for Ex < fB, because some of the electrons can tunnel through the potential barrier, and is not equal to 1 for Ex > fB, because some of the electrons are reflected, where Ex = mv2x /2 and v* is the electron velocity in x direction. • It is possible that the barrier height is not uniform over the whole area of the interface. It should be noted that the barrier height may depend on specimen thickness and light intensity, possibly due to space charge effects.188 Obviously, because of the image force effect, the barrier height is field dependent. Berglund and Powell189 have derived the expression for the photoemission current versus applied voltage characteristics for an MIM structure. It is given by
10
Ï È q J ph a Ìhu  f B  Í Ó Î 4peS 1
p
xm ˘ 2 ¸Ô ¥ ( qV + f1  f 2 )˙ ˝ expÊ  ˆ Ë l¯ ˚ ˛Ô
0 1.5
2.0 fB
2.5 hn (eV )
Figure 352 (Photoemission current)1/2 as a function of incident photon quantum energy for an Al (1000 Å) Al2O3(30 Å)  Al(200 Å) structure with the 200 Åthick top electrode illuminated. The corners of the barriers are rounded off due to the image force, as shown in the inset.
(3154)
where S is thickness of the specimen, xm is the distance from the illuminated electrode to the location of the maximum barrier height, l is the mean free path, and p is a parameter depending on the kind of electron excitation and lies 1 < p < 3. If the insulator is too thin, the incident light illuminating the first electrode can
184
Dielectric Phenomena in Solids
also reach the second electrode (opposite to the first) and excite carriers there. Consequently, the photoemission current is composed of two types of currents (electrons and holes) under an applied field. Unless the component from the opposite electrode is negligibly small, the photoemission consisting of two types of carriers would influence the thickness and hu dependence of Jph. Furthermore, the electron–electron and electron–phonon interactions also play an important role in this dependence. All these effects on the internal photoemission—as well as the application of various internal photoemission experiments for the determination of barrier height, potential barrier shape, charge distribution in the insulator, topographical distribution of the barrier height, trap distribution in the barrier, and the mean free paths and energy losses of the carriers—have been critically reviewed by Kadlec and Gundlach.178,186,190 From a Narrow Bandwidth Emitter into Wide Bandwidth Semiconductors A degenerate ntype or ptype silicon or similar semiconductor can act as a narrow bandwidth emitter. Photons with energies hu0 or hu1 can excite electrons from the conduction band, and those with energy hu2 can excite electrons from the valence band of a degenerate ntype semiconductor into the conduction band of an insulator, as shown in Figure 353. For a given photon energy hu, the excited electrons are distributed over only a narrow band of the width
hu2 hu1 Narrow Bandwidth Emitter
hu0 Ec Ev
fB
Ec
Eg
Degenerate Ntype Semiconductor
Ev Insulator
Figure 353 Various possible transitions for photoemission of electrons from a degenerate n–type semiconductor into an insulator.
within a few kT of the bottom of the conduction band, far narrower than those excited from the metal. Thus, within the range of photon energies fB £ hu £ fB + Eg, the photoemission current (or the quantum yield for photoemission) as a function of photon energy is simply J ph = C( hu  hu o )
(3155)
For the SiSi02 system, the experimental results fit Equation 3155 if the photon energies hv are less than fB + Eg, and then fit Equation 3153 (rather than Equation 3155) when hv > fB + Eg, because at higher photon energies, the electrons excited from the valence band become dominant, as shown in Figure 353. From a Metal into Narrow Bandwidth Crystals The narrow band can be considered a delta function. This means that within the band, the energy distribution of excited holes (or excited electrons) is uniform and implies that the quantum yield for photon energies above the threshold hv0 is independent of photon energy, as shown in Figure 354(a). In organic crystals, there are usually several narrow bands separated by roughly equally spaced levels, due to molecular vibrations. For example, in anthracene, the molecular vibration has frequencies corresponding to energies of approximately 0.2 eV, but the electronic bandwidth is about 0.02 eV. For clarity, only two such narrow valence bands are shown in Figure 354(b). Each band gives rise to a stepfunction of photoemission current, starting at different photon energies. The combination of these stepfunctions gives a staircase quantum yield Y, and the derivative dY/d(hv) gives a clear picture of energylevel splitting by molecular vibration, as shown in Figure 354(b). Figure 354(b) gives only the basic concept of the behavior of narrow bands. In fact, the quantum yield of the ith narrow band should be proportional to (hv  fBi), since the number of excited carriers that can surmount the potential barrier fBi is proportional to (hv  fBi), as shown in Figure 354(c). See also the top energy diagram of Figure 354(b). The total quantum
Optical and ElectroOptic Processes Ec
Ec hn2
fB = hno Metal
185
hn1 hno
hno + hnv Evo
Ev
Narrow Band Insulator
Ev1 Narrow Band Insulator
Metal
hno + hnv
hno Quantum Y Yield
Y hn
hno
Y hn
dY d (hn)
dY d (hn) hn
(a)
hn
dY d (hn) hn
(b)
hn
(c)
Figure 354 Schematic diagrams illustrating photoemission from metal into narrowband crystals: (a) with one narrow band when the acceptance angle is not considered; (b) with two narrow bands when the acceptance angle is not considered; (c) with two narrow bands when the acceptance angle is taken into account.
yield Y from all the vibrationally split levels should be the sum of the linear ramps, as shown in Figure 354(c). In this case, the derivative dY/d(hv) gives a series of stepfunctions, starting at different photon energies. For photoemission from a metallic contact to an organic crystal, the quantum yield Y should follow the relation schematically shown in Figure 354(c) and Yµ(hv  fB)2, rather than those shown in Figure 354(b) with Ya (hv  fB). Several investigators have reported that the quantum yields for the photoemission of holes into organic semiconductors, measured as functions of photon energy using various metallic electrodes, are in good agreement with the theoretical prediction discussed here.171–174,191,192 Obviously, these arguments for photoemission of holes from metal to narrow band crystals apply equally well to cases of photoemission of electrons from metal to narrowband crystals. It should also be noted that, from the arguments given earlier in this chapter in Photoemission from Electrical Contacts, it is possible to estimate the photoemission spectrum in cases of a narrow bandwidth emitter into crystals with a series of narrow bands.
3.5.2 Photoemission from Crystalline Solids In general, photoemission from crystalline solids means volume photoemission resulting from optical absorption in the bulk, which should be distinguished from surface photoemission resulting from optical absorption at the surface. The contribution from excitation of surface states is small, because the total number of surface states is small compared to the number of states in the bulk that can participate in photoemission processes. Therefore, photoemission is mostly a volume effect. The photoemission quantum yield increases with increasing specimen thickness and reaches a saturation value when specimen thickness exceeds the penetration (or absorption) depth or the escape depth. If specimen thickness is smaller than penetration depth, photoemission may exhibit a roughly periodic nature of its variation with specimen thickness, going through a minimum at thicknesses equal to an odd number of quarterwavelengths and through a maximum at thicknesses equal to an integral number of halfwavelengths of the
186
Dielectric Phenomena in Solids
incident light.193 To simplify matters, such an interference effect is ignored in the following discussion, and photoemission is assumed to be a bulk phenomenon. Photoemission consists of three steps: 1. 2. 3.
Excitation of an electron to a highenergy state by the absorption of a photon The scattering of the excited electron on its way to the vacuumsolid interfaces The escape of the electron over the potential barrier at the surface of the solid
RIo
Surface states may affect volume photoemission indirectly through band bending. However, for the sake of simplicity, we will neglect the bandbending effects. Figure 355 illustrates the three steps, the band diagram, and the relative energy levels for photoemission from an organic crystal into a vacuum. The light intensity of the excitation with photon energy hu at the same distance x from the vacuumsolid interface is I(u , x ) = Io (1  R)exp( a x )
(3156)
Io(1 – R )exp (–a x)
Io hn
Scattering
Emitted Electron x
dx d x=0 Vacuum
Organic Crystal
Vacuum Level
Vacuum Level c Ec
hn1 hno
Ev Ev1 Ev2 E
E x
k
Figure 355 Schematic diagrams illustrating excitation, scattering, and escape of an excited electron, the hole bands EV, the vibrationally excited hole bands EV1, EV2, and so on. The conduction band is assumed to be parabolic, and the valence bands are assumed to be almost independent of k vector. Localized states in the energy gap due to imperfections are not shown for the sake of clarity.
Optical and ElectroOptic Processes
where Io is the light intensity in vacuum; R and a are, respectively, the reflection and the absorption coefficients of the crystal, which depend on light wavelength. I(v,x) can be defined as the number of photons of energy hv arriving at x per second. Before going to organic crystals, we will take a simple inorganic semiconductor as an example to illustrate the procedures of deriving an expression for the photoemission yield Y. Supposing that the energy of incident photons hv is larger than Eg + c, then the concentration of photocarriers generated within dx at x is dn = PaI (v, x )dx = PaIo (1  R)exp( a x )dx
(3157)
where P is the probability that a photon absorbed will excite an electron to a highenergy state. The energy hv > (Eg + c) may excite some electrons to a highenergy state above the vacuum level, but it may also excite some to a level below the vacuum level if the electrons being excited are located much lower than Ev in the valence band. Clearly, only those above the vacuum level can lead to photoemission. Furthermore, even though some excited electrons at x may have energies above the vacuum level, they will lose part of their energies by the scattering processes during their motion toward the vacuumsolid interface. Thus, by the time they reach the interface, some may have lost so much energy that their energies become lower than the vacuum level, and they will not be able to escape over the potential barrier. The probability for an excited electron at x to escape to contribute to photoemission can be written as194 Pesc (u , x ) = B(u )exp(  x Lesc )
(3158)
where B(u) is constant and Lesc is the escape depth. Both B(u) and Lesc are dependent on electron energy. The total photocarriers emitted from the crystal specimen are then •
n = Ú PaIo (1  R)exp( a x )B exp(  x Lesc )dx o
=
PaBIo (1  R) a + 1 Lesc
(3159)
187
The quantum yield is defined as Y=
n PB = Io (1  R) 1 + 1 aLesc
(3160)
Since B and Lesc are functions of electron energy, they must be directly related to scattering mechanisms and absorption processes (direct transition, without a change in momentum, or indirect transition, involving a change in momentum). Kane has analyzed theoretically the quantum yield versus photon energy characteristics near the threshold for a general band structure and for a variety of photocarrier generation and scattering mechanisms involving volume and surface states (volume and surface scattering processes) in semiconductors.195 The initial fastrising portion of the Y hv curve can be expressed in the form Y = A( hv  Eth )S
(3161)
where A and S are constants and Eth is the threshold energy required for photoemission. For intrinsic and lightly doped semiconductors Eth = c + Eg. Depending on the photocarrier generation and scattering mechanisms, S varies from S = 1 to S = 5/2.195 For cases that do not involve surface scattering, the values of S are as follows: S = 1 for direct transition without volume scattering S = 2 for direct transition involving elastic scattering S = 5/2 for indirect transition with or without elastic scattering In practical cases, photocarriers suffer both volume and surface scattering. However, that S = 1 in the highenergy region and S = 3 in the region near the threshold has been experimentally observed in IIIV compounds, such as InSb, GaSb, InAs, and GaAs.196 Kane’s theory, however, depends on the shape of the edge of the valence band. Therefore, it cannot be applied to organic crystals with narrow valence bands. In organic molecular crystals, excitons are generally the intermediate states in the photocarrier generation processes. Also, the molecu
188
Dielectric Phenomena in Solids
lar vibrations split each valence band into many wellseparated narrow bands with an energy separation of one vibrational quantum, hvv. The electron escape probability Pesc involves both the scattering probability and the surface transmission probability. Near the threshold, Pesc may be considered due mainly to surface transmission probability, because scattering probability varies slowly in this energy region.170 On the basis of this consideration, several investigators170,197,198 have derived a relation between the quantum yield and the photon energy near the threshold, which is given by Y µ ( hu  Eth )S
Vacuum Level Vacuum Level
Eth DE
EC
Eth DEo
EC
EF
EF
EV
EV
Figure 356 The effect of band bending on the threshold for photoemission.
(3162)
with 1/2 £ S £ 3. This expression is similar to Equation 3161. However, for a large number of molecular crystals, the experimental results on the quantum yield near the threshold are in agreement with Equation 3162 with S = 3, such as anthracene, tetracene, and pentacene.170,199 It should be noted that, because many factors may affect the value of S, it is often possible to obtain fits to the experimental data versus hu with S other than 3. When photon energy is in the abovethreshold region, the value of S may become 1/2. It is likely that the extrapolation of the plot of Y 2 as a function of hu to Y 2 = 0 yields the value of Eth corresponding to the first maximum in the photoelectron energy distribution spectrum (from the most probable position of the first valence band to the vacuum level), while the cubic law extrapolation gives the value of Eth corresponding to the onset of photoemission.198 For more details about photoemission in molecular crystals, see references 198–200. Effects of Surface Conditions In the preceding analysis, the energy bands are assumed to be flat up to the surface. In fact, there are always surface states present at the surface that induce space charge near it, causing the band to bend up or down, as shown in Figure 356. Gases such as oxygen adsorbed on the surface may result in a change of the order of 1 eV in Eth. If the space charge causes the
band to bend up by DE the threshold energy for photoemission Eth = Ethflat band + DE. Conversely, if the band is bent down by DE then Eth = Ethflat band  DE. To include the effects of surface conditions, we must know the variation of Ev with x measured from the vacuum level. Of course, the analysis for the Y  hu relation will be very mathematically involved. Effects of Defects in Crystals Obviously, defects in a crystal will affect the photoemission spectrum. It is likely that the adsorbed gases in the crystal lead to the formation of deep traps, particularly in the surface layers of the solid. Electron acceptors, such as O2, produce electron traps, while electron donors, such as H2, produce hole traps. Local changes in polarization energy and impurities with low ionization energy present in the crystal lattice would cause changes in the photoemission spectrum. In general, the defects tend to broaden the low energy tails, causing a decrease in the threshold. Thus, in studying photoemission from solids, there are two intricate problems: the determination of the threshold photon energy, and the identification of the origin of the emitted electrons. For example, the values of Eth change as oxygen is incorporated into tetracene,194 or for alkali metals such as caesium, potassium, and sodium doped into anthracene crystals.201
Optical and ElectroOptic Processes
Energy Distribution of Emitted Electrons The energy distribution of the emitted electrons can be measured by several techniques. The most commonly used technique is the retarding potential method. This method simply employs a bias, acting as a retarding potential VR, which collects only those emitted electrons with a kinetic energy Ek greater than the retarding potential energy qVR. By sweeping the retarding potential over a range of bias, a complete energy distribution curve (EDC) can be obtained.202,203 All energies above the vacuum level (see Figure 355) are available as kinetic energy for the emitted electrons. So, the incident photon energy Ep must be at least equal to the energy between the valence band edge Ev and the vacuum level Evac. Thus, the minimum retarding potential VR(min) that can completely block the photoemission current should be VR(min) = ( E p  Evac ) q
(3163)
From the EDC, it is possible to determine the band structure in the crystal,204 as well as to obtain information about the density of states in the valence and the conduction bands. Figure 357 shows schematically the variation of the photoemission current I and the number of emitted electrons per unit times per unit energy N with retarding potential VR. For the latter, N can be expressed as N=
1 dI 1 dI = 2 q d ( qVR ) q dVR
(3164)
It can be seen that N = 0 when VR = VR(sat) and VR = VR(min). N increases with VR from VR(sat), as expected, since the attenuation of the absorbed optical energy varies exponentially with the depth from the surface of the solid specimen. So, a greater fraction of excited electrons lies in the region close to the surface. Fewer electrons are excited deeper inside the crystal; these electrons will find greater difficulty in emerging because their kinetic energy is close to zero. Thus, electrons excited closer to the surface will be greater in number and their energies close to the maximum kinetic energy. The peak of the N  qVR curve occurs at qVR = EA, imply
189
ing that the loss of electron energy for qVR < EA results in a decrease in the number of emitted electrons with kinetic energies less than EA. There are many possible causes of the loss of electron energy. For example, the loss may be due to the excitation of bound molecular states by the electrons before they emerge from the crystal. The width of the peak at EA could be due to a variety of causes; for example, not all of the emitted electrons travel in the direction perpendicular to the surface of the collecting electrode [see the insert of Figure 357(a)] due either to scattering, to the excitation of bound molecular states, or to a particular distribution in the intrinsic density of states. Furthermore, the vibrational modes of the molecular ions, as well as the fluctuation of intermolecular electronic polarization, may also cause N to decrease for qVR greater and smaller than EA. The second peak at qVR = EB may be due to the structure of the crystal. Depending on the incident photon energy and the structure of the crystal, the N  qVR curve may exhibit one peak, two peaks, or one peak with several shoulders. For example, for the inorganic cesiated GaAs crystal, the N  Ek curve exhibits one peak if it is excited by photons of about 1.4 eV. But at photon energies greater than 1.7 eV, the valleys can take electrons. If the photoemission time is comparable to the intervalley relaxation time, then the crystal will exhibit two peaks in the N  Ek curve.205 For the organic anthracene crystal, there are many shoulders before the occurrence of the peak in the N  Ek curve.170 A wide variety of phenomena can be studied using the experimental data on the photoemission of electrons with a definite kinetic energy. Multiquantum Processes So far, our discussion has been limited to phenomena based on onequantum processes. For example, when an anthracene crystal is excited by light of the energy hv < 5 eV there is still photoemission below the ionization threshold, which is 5.7 eV. But in this case, the quantum yield Y varies as the square of the incident photon energy. This phenomenon was first
190
Dielectric Phenomena in Solids I
hn
VR
I DI DVR
VR(sat)
VR(min)
VR
(a)
N
qVR(sat)
EA
EB
qVR(min)
(b) Figure 357 Schematic diagrams illustrating (a) the variation of the photoemission current with the retarding potential and the simple setup for this measurement and (b) the corresponding variation of the number of emitted electrons per unit time per unit energy N with their kinetic energy represented by qVR.
discovered by Pope et al.206 It can only be explained by the doublequantum processes. If the rate of photoemission is proportional to light intensity, excitation is a onephoton process; if it varies quadratically with light intensity, excitation is a twophoton process. The mechanisms that may contribute to this
doublequantum process are direct twophoton excitation, exciton photoionization, exciton– exciton collision ionization, exciton–conduction electron ionization, and conduction electron ionization. The excitons involved could be neutral singlet or triplet excitons or ionic excitons.169
Optical and ElectroOptic Processes
3.6
Photovoltaic Effects
Photovoltaic effects generally refer to phenomena resulting from the conversion of light energy into electrical energy. This conversion process can be considered the reverse of electroluminescence. However, the criteria for achieving the conversion are different. For electroluminescence, only radiative recombination produces light, and the carriers involved in producing light can be free or bound carriers. But for photovoltaic effects, optical absorption must produce free carriers, and the carriers involved in generating photovoltages must be free (mobile) carriers. A photovoltaic device is a photodiode in which electron–hole pairs can be generated by photon absorption, and they will be separated by a force due either to the diffusion of these photogenerated carriers with different mobilities in the bulk, to the contact potential (or diffusion potential) associated with the contact between two different materials, or to photosynthesis. We may detect this charge separation in two ways. If the device under photon radiation is left on an open circuit, then the potential between two terminals can be measured as the opencircuit voltage. This is known as the photovoltaic mode of operation. On the other hand, if the device under photon radiation is shortcircuited, then an external current can be measured under the shortcircuit condition or through a small resistance. This is known as the photoconductive mode of operation. Photovoltaic effects in solids may therefore be caused by Bulk photovoltaic effects: A photovoltage arises due to the diffusion of nonequilibrium photogenerated carriers with different electron and hole mobilities in the bulk of the solid. Contact potential photovoltaic effects: A photovoltage arises due to the potential barrier at the interface between two different materials, such as the Schottky barrier at the metalsemiconductor or metalinsulator contacts; the p–n junction between a ptype and an ntype semiconductor; or the p–i–n
191
structure, with an insulator between a ptype and an ntype semiconductor. Photosynthesis photovoltaic effects: A photovoltage arises due to the photosynthesis of a dye sensitizer and an electrolyte. Anomalous photovoltaic effects: A photovoltage arises due to a combination of several mechanisms, such as the Dember effect in microregions, photovoltaic effects at p–n junctions, Schottky barriers or strains at grain boundaries. Any photovoltaic effects occurring in a solid involve • Light absorption in the solid • Mobile charge carriers generated by the absorption • An internal discontinuity or nonuniform distribution of impurities or defects giving rise to the creation of an internal electric field to separate the two types of carriers • Electrical contacts In this section, we shall discuss briefly various photovoltaic effects.
3.6.1 Bulk Photovoltaic Effects As early in 1931, Dember observed an electric potential developed across a cuprous oxide specimen when subjected to illumination with a strong light in the absorption region of this material. Later, this phenomenon was referred to as the Dember effect 207 and was soon found also in diamond and zinc sulfide,208 in Ge and Si,91,209,210 in CdS,211 and in organic crystals.212 This phenomenon is attributed to the diffusion of photogenerated electrons and holes with different mobilities. In general, the spectral distribution of the photovoltage amplitudes correlates closely to the absorption spectrum, and the change in light intensity changes only the photovoltage amplitude; it does not affect this correlation. Photovoltaic behavior is sensitive to the surface condition of the device. Adsorption of oxygen on the crystal surface may reduce greatly the photovoltage amplitude.
192
Dielectric Phenomena in Solids
The Dember Effect
leaving a positive space charge near the illuminated surface and a negative charge within the bulk of the specimen. The internal electric field set up by this charge distribution tends to oppose the electron flow and to assist the hole flow, so the carriers drift in a manner that reduces the space charge. For lowresistivity materials, the Debye length is small, implying that the length over which a charge imbalance is neutralized by the majority of carriers is small. In other words, the overall internal field created is considerably smaller than would be obtained for highresistivity materials. Thus, for highresistivity materials, the excess photogenerated carrier concentration is larger than the thermal equilibrium carrier concentration. For this case, the opencircuit photovoltage, usually called the Dember voltage, can be derived on the basis of large signal theory. It is given by
The lightinduced creation of a photovoltage in the bulk of a solid is referred to as the Dember effect. Conditions necessary for this effect to occur are nonuniform illumination, which gives rise to a concentration gradient of the photogenerated carriers, and photogenerated carriers with different mobilities. Under these conditions, when the surface of a solid specimen is illuminated with a light of high intensity, a high concentration of photogenerated electron–hole pairs will be produced near the illuminated surface, as shown in Figure 358(a). In general, the mobility of electrons is higher than that of holes for most inorganic semiconductors (usually, the reverse is true for most organic semiconductors). If this is the case, electrons will diffuse more rapidly than the holes,
Holes
Electrons
Transparent Electrode (SnO2)
Electrode
Light Beam
VD
(a) Light Beam
Iye
Ixh t
Ixe
Fx
Iyh d Bz VPEM
(b) Figure 358 Schematic diagrams illustrating the basic arrangements for measurements of (a) the Dember voltage VD and (b) the photoelectromagnetic (PEM) voltage VPEM.
Optical and ElectroOptic Processes
VD =
kT mn  m p È ( mn + m p )Dn ˘ ln 1 + q mn + m p ÍÎ mn no + m p po ˙˚
(3165) where mn and mp are the mobilities of electrons and holes, respectively; no and po are the concentrations of thermally equilibrium electrons and holes; and Dn = Dp is the photogenerated excess electron concentration (equal to the excess hole concentration).99 It should be noted that there are always traps in solids, and that the electrical contacts to the solid specimen are usually not ohmic, resulting in the formation of a surface potential barrier. The electric field associated with such a barrier would partially separate the electrons and holes, which are injected to the specimen due to optical illumination in the vicinity of the surface. This would create a photovoltage indistinguishable from the Dember voltage. However, the Dember voltage is usually very small, and the Dember effect has so far received little attention because of its low efficiency for use as solar cells. Most photovoltaic effects are based on other, more efficient ways of photogeneration of free carriers and their separation for the creation of a high internal electric field. The PhotoelectroMagnetic (PEM) Effect The photoelectromagnetic (PEM) effect, which is also called the photomagnetoelectric (PME) or the magnetophotovoltaic (MPV) effect, was originally discovered in cuprous oxide by Kikoin and Noskov in 1934213 and later studied by many investigators.91,214,215 The PEM effect is illustrated schematically in Figure 358(b). When a slab of photoconductor is illuminated perpendicularly with light within the intrinsic absorption band of the material, electron–hole pairs are generated in a layer close to the illuminated surface. These photogenerated electrons and holes will set up a concentration gradient and diffuse in the direction of the illumination. If a magnetic field B is applied in the z direction transversely to the diffusion current, the electrons and holes will be deflected in the opposite x direction, resulting in the creation of an electric field in the x direc
193
tion. This will, in turn, produce Jsc if the two electrodes are shortcircuited, or produce an opencircuit photovoltage VPEM between the two electrodes, which is just sufficient to prevent the current flow. The photovoltaic phenomenon, unlike the Dember effect, occurs even if mn = mp. Based on a simple phenomenological theory, an approximate expression for the shortcircuit current per unit width of the slab in the magnetic field direction has been derived,69,91 and it is given by Jsc = IB [2 kTtqmn m p ( mn + m p )]1 2
(3166)
The opencircuit photovoltage is given simply by the product of the resistance of the slab and Jsc, so that the PEM opencircuit photovoltage can be expressed as VPEM =  Jsc d s t
(3167)
where I is the light intensity, expressed in quanta (photons) per second per unit area absorbed by the slab; B is the magnetic field in flux density; t is the lifetime of the photogenerated carriers; s is the conductivity of the slab; and d and t are, respectively, the length and the thickness of the slab. It can be seen from Equations 3166 and 3167 that both Jsc and VPEM increase linearly with light intensity and magnetic field. It is interesting to note that for the PEM, Jsc depends on (t)1/2, while for photoconduction, the current usually depends linearly on t. It should also be noted that Jsc and VPEM depend on surface recombination, which has been ignored in deriving these approximate expressions. However, for the validity of the expressions, the thickness t of the slab must be small compared to the carrier diffusion length, so bulk recombination can be neglected. For the configuration shown in Figure 358(b), the direction of the illuminating light and that of the magnetic field are mutually perpendicular. This arrangement will develop a voltage Vx, which creates an opencircuit circulating current lying completely in the x–y plane perpendicular to the magnetic field. So, there is no net mechanical force produced due to this interaction if the field is homogeneous.
194
Dielectric Phenomena in Solids
However, if the applied magnetic field is tilted in the x–z plane instead of being perpendicular to the x direction, then the Bx component will interact with the opencircuit circulating current in the slab, creating a torque. This phenomenon is called the photomechanical effect.214 Measuring PEM torques instead of PEM photovoltages, no electrodes are required and thus, the effects due to electrical contacts can be eliminated. This is an important advantage when using the PEM effect for studying bulk properties of a material. 3.6.2 Contact Potential Photovoltaic Effects To produce a photovoltage in a device, it is necessary to have mobile photogenerated electron–hole pairs and an internal electric field to separate the two types of carriers and to enable them to flow to the external contacts of the device. The contact potential at the interface between two different materials provides an efficient means for this requirement. Since the contact potential is associated with the bending of the energy bands near the interface, the contact potential’s magnitude and sign depend strongly on the surface states at the interface. Schottky Barrier Photovoltages There are three possible photoeffects that can take place at the Schottky barrier: Process 1: Light absorbed in the metal will raise electrons in the metal to energy levels high enough to surmount the barrier, as shown in Figure 359(a). The threshold for this to occur is the measure of the barrier height fB. Electrons with sufficient energy to enter the solid will make it acquire negative charges, thus creating a photovoltage across the barrier. Process 2: Light with hv ≥ Eg can generate electron–hole pairs in the depletion region. The high electric field in the depletion region will separate the photogenerated carriers, as shown in Figure 359(a), resulting in a photovoltage between the metallic electrode and the bulk of the solid.
fB 1
2
3 3
2 1 W W
(a)
(b)
Figure 359 Energy band diagrams for (a) the ntype semiconductor with an elecron Schottky barrier and (b) the ptype semiconductor with a hole Schottky barrier, and three carrier generation processes for photovoltaic effects.
Process 3: Light with hv ≥ Eg may also be absorbed deep in the bulk of the solid and generate electron–hole pairs there. One type of carrier (minority carriers) diffuses to the junction, as shown in Figure 359(a). This also contributes to the total photovoltage across the barrier. In general, the contribution from process 1 is small because the electrons require momentum conservation (phonons) for their crossing.216 The major contribution to the photovoltaic effects is from processes 2 and 3. Process 1 is, in fact, similar to photoemission, which was discussed in Section 3.5.1. Electrons injected from a metal into a semiconductor experience a force directed away from the contact. Of course, the probability of the occurrence of photoemission depends on the thickness of the metal film that is the illuminated electrode. If the electron attenuation length is sufficiently long compared to the thickness of metal film, then the photoresponse is proportional to (hv  fB)2.217 Processes 2 and 3 occur when hv ≥ Eg. A typical curve showing the spectral dependence of the photoresponse is shown in Figure 360. Thus, measurements of the threshold energies at which these processes occur may be used to determine the barrier height fB and the energy gap of the semiconductor Eg.181 When the photon energies
Optical and ElectroOptic Processes
Photovoltaic Response (arbitrary units)
105
104
B
103
102 A 10
1
Eg Photon Energy (hn)
Figure 360 Spectral dependence of photovoltaic response. A: photoemission from the metal. B: the bandtoband transition.
are much larger than Eg, the electron–hole pairs are generated very close to the interface between the illuminated electrode and the semiconductor because of the high absorption there. The decrease of photoresponse at high photon energies is due to the strong surface recombination. For hv ≥ Eg, and on the assumption that the energy band diagram of the Schottky barrier is as shown in Figure 359(a) without interface states, the photocurrent due to process 2 (photocarriers generated in the depletion region) for the exciting light of wavelength l is given by218 Jdr = qT (l )I(l )[1  exp( a w )]
(3168)
and the photocurrent due to process 3 (photogenerated holes collected from the bulk) is given by218
195
where T (l) is the transmission of the metal film into the underlying semiconductor, I (l) is the incident photon flux, a is the absorption coefficient, S is the surface recombination velocity, d is the semiconductor specimen thickness, Lp is the diffusion length of holes, and w is the width of the depletion layer and is given by Equation 6.27 (see Chapter 6). The total photocurrent is the sum of Jdr and Jp. Several effects that would affect the photocurrent are not included in the derivation of Equations 3168 and 3169: the surface states at the metal–semiconductor interface, the reflection from the illuminated electrode surface, the image potential, and the interfacial dielectric layer. To include these effects would make the analysis intractable. If the photocurrent under the shortcircuit condition is Jsc = Jdr + J p
(3170)
then when the two electrode is not shortcircuited, but connected with a resistive load with the resistance R between them, the photocurrent collected externally can be written as Jph = Jsc  Jo [exp( qVph kT )  1]
(3171)
in which the second term is the normal forwardbias current at the voltage Vph for a Schottky barrier diode and Jo is the reverse bias saturation current, which is Jo = AT 2 exp( f B kT )
(3172)
where A is the Richardson constant, which is normally equal to 120 A cm2K2, and fB is the Schottky barrier height.219 When the photocurrent Jph is flowing, a photovoltage Vph = JphR will be developed across the diode, producing a forwardbias current in the direction opposite to the photocurrent. Thus, the opencircuit voltage can be deduced simply by setting Jph = 0 in Equation 3171, which is
(SL p Dp ){cosh[(d  w ) L p ]  exp[ a (d  w )]} + ˆ Ê sinh[(d  w ) L p ] + aL p exp[ a (d  w )] qIaL p Á ˜ Jp = T exp ( a w ) ¥ Á aL p ˜ ( SL D ) sinh[( d w ) L ] + cosh[( d w ) L ] (a 2 L2p  1) p p p p Á ˜ Ë ¯
(3169)
196
Dielectric Phenomena in Solids
Voc = =
kT Ê Jsc ˆ ln +1 Ë Jo ¯ q kT Ê Jsc ˆ ln Ë Jo ¯ q
(3173)
since Jsc >> Jo. MIS Solar Cells If Si or any covalent bonded crystal is used as the semiconductor for solar cells, dangling bonds exist at the surface of the crystal due to the interruption of the perfect periodicity of the crystal lattice. These dangling bonds create surface states, which may overlap the states in the valence and the conduction bands, but only those within the forbidden gap play a role in the behavior of the metal–semiconductor contacts. The dangling bonds tend to capture electrons to complete the bonds. Theoretically, the number of surface states created by dangling bonds should be approximately equal to (1023 cm3)2/3 = 1015 cm2. But the experimental data show the surface state density being of the order of 1012 cm2, implying that there exists mutual saturation of unsaturated bonds of neighboring atoms, and that there may be an oxide layer of about 20 Å in thickness formed on the semiconductor surface due to the preparation and exposure of the surface to the atmosphere containing oxygen before the deposition of the metallic electrode.219 This would result in the formation of an MIS structure with a very thin insulating layer (I) between metal (M) and the semiconductor (S), as shown in Figure 361. The insulating layer (oxide) screens the semiconductor surface from the metal and helps saturation of unsaturated bonds. The opencircuit photovoltage Voc decreases with increasing Jo, as shown in Equation 3173. Jo for Schottky barrier diodes is a few orders of magnitude higher than for p–n junction diodes, so Voc for Schottky barrier solar cells is significantly smaller than that of p–n junction solar cells. Jo represents the majority carrier thermionic current flowing in the direction opposite to the photogenerated current. The thin insulating layer between the metal and the semiconductor also serves to reduce Jo, thus increasing the magnitude of Voc.220 The thin insulating layer with a thickness of the order of 20 Å will be no
barrier for the photogenerated minority carriers. They can tunnel through a thin layer. Photovoltaic Behavior of P–N Junctions A simple p–n junction diode is shown in Figure 362. In general, a very thin semitransparent metallic film (usually gold film of 50–100 Å in thickness) is vacuumdeposited on one side of the semiconductor surface for the light illumination; the front contact, with a thick metallic grid, is then deposited. To minimize surface reflection at the metal–air interface, an antireflective film is coated on the surface, as shown in Figure 362(a). For such simple p–n junction diodes, the currentvoltage characteristic for the abrupt junction case is given by168 J = Jo [exp( qV kT )  1]
(3174)
where Jo is the reverse bias saturation current, which is Jo =
qDn n po qDp pno + Ln Lp
(3175)
where Dn and Dp are, respectively, the diffusion coefficients for minority electrons and minority holes; Ln and Lp are, respectively, the diffusion lengths of minority electrons and minority holes; npo and pno are, respectively, the concentrations of the minority electrons in the ptype and the minority holes in the ntype semiconductors. It can be seen from Figure 362(b) that an electric field exists in the space charge (depletion) region even without bias. Incident photon illumination creates electron–hole pairs in the space charge region, as well as in the neutral regions of the ntype and ptype semiconductors. For the latter, however, only those electrons and holes within the diffusion length from the edge of the depletion region have a chance to diffuse to the depletion region. These carriers in the depletion region will be swept out, producing the photocurrent Jph in the reversebias direction, as shown in Figure 362(c) and (d). Similar to Schottky barrier solar cells, the photocurrent will produce a voltage drop across the load resistance R, which produces a forward bias across the p–n junction. This forwardbias voltage Vph in turn produces a forwardbias current J, as given by Equation
Optical and ElectroOptic Processes
197
Antireflective Coating Sunlight Contact Grid
Semitransparent Thin Metal Film
Oxide Layer Semiconductor
Back Contact
fB
EC EF
EV
Metal
Semiconductor Insulation Layer (SiO2)
Figure 361 Schematic diagrams showing the basic structure of an MIS solar cell and its energy band diagram.
3174. Thus, the photocurrent under shortcircuit condition is Jsc = Jph (Vph = 0)
(3176)
With a load resistance R instead of shortcircuiting, the net photocurrent becomes Jph = Jsc  Jo [exp( qVph kT )  1]
Voc =
kT Ê Jsc ln + 1ˆ Ë Jo ¯ q
(3178)
This equation is similar to Equation 3173, but Jo for p–n junctions is much smaller than Jo for Schottky barrier diodes. The power delivered to the load is
(3177)
There are two limiting cases. One is when R = 0, Vph = 0, we have Jsc, which is the highest photocurrent that can be obtained. The other is when R Æ •, then Jph = 0. From Equation 3177, the opencircuit photovoltage Voc can be written as
P = Jph Vph = { Jsc  Jo [exp( qVph kT )  1]}Vph
(3179) By setting dP/dVph = 0, we can obtain the condition under which the maximum power can be delivered to the load, which is
198
Dielectric Phenomena in Solids Front Contact Antireflective Coating
Back Contact
Depletion Region
Sunlight
n+
P
Semitransparent Thin Metallic Electrode
(a) J Without Light
EC EC
V
Eg Voc
Io
EF EV
EF EC
qV
ph
EF EV
Jm With Light
Vm Jsc
EV
(b) In Thermal Equilibrium
(c) Under light Illumination
(d)
Figure 362 Schematic diagrams showing (a) the basic structure of an n+–p junction solar cell, (b) the energy band diagram in thermal equilibrium, (c) the energy band diagram under light illumination generating a photovoltage Vph, and (d) the J  V characteristic.
qVm ˆ Jm Ê Ê qVm ˆ Á1 + ˜ exp Á ˜ = 1+ Ë Ë kT ¯ kT ¯ Jo
(3180)
where Vm and Jm are, respectively, the photovoltage and the photocurrent, at which the power delivered to the load is maximal. Vm and Jm can be determined by the trialanderror method. The maximum power is JmVm product, which is the area of the rectangle formed within the boundary of the Jph  Vph curve, as shown in Figure 362(d). The energy conversion efficiency is given by (3181)
h = JmVm Pin
where Pin is the incident optical power. The maximum possible photocurrent is Jsc, and the maximum possible photovoltage is Voc. The fill factor is defined as Fill Factor =
JmVm JscVoc
(3182)
This simple analysis shows the basic principle of an ideal p–n junction solar cell. For practical p–n junction solar cells, one side of the semiconductor (n or pside, but usually the nside) is heavily doped to the n+ level, so that the Fermi level of the n+ side is inside the conduction band because of its degeneracy. This would make it easy for photons with the energy of the order of Eg to reach the depletion region. The heavy doping of the n+ side also makes it easy to produce an ohmic contact with the deposited thin semitransparent metallic electrode for the admission of the incident light. The energy conversion efficiency depends on the wavelength of the incident photons. A photon with energy greater than Eg will contribute to the solar cell output power, but a fraction of the energy (typically hu  Eg) will be dissipated as heat, while a photon with energy less than Eg will not contribute much to the solar well output power.
Optical and ElectroOptic Processes
ance depends on the doping level. A heavily doped semiconductor reduces the minority carrier lifetime and diffusion length. So, the doping level and the junction depth must be adjusted to arrive at the optimal comprise. The effect of series resistance Rs on the Jph  Vph characteristics is shown in Figure 363. The experimental result of the GaAs p–n junction is from Janny, Loferski, and Rappaport.222 Thus, taking Rs into account, Equation 3177 must be written as Jph = Jsc  Jo (exp[ q (Vph  Jph Rs ) kT ]  1)
(3183) and Equation 3178 as Voc =
kT Ê Jsc ln + 1ˆ Ë Jo ¯ q
(3184)
which is the same as Equation 3178, implying that series resistance does not affect the opencircuit voltage. Incomplete absorption: A small absorption coefficient means a deep penetration of the incident photons, implying that most of the photons eventually transmit through the material because of insufficient interaction between the photons and the bound electrons inside the material. Thus, the absorption properties of photovoltaic material determine, to a great extent, the amount of the incident radi
600 Load Line 500 Rs = 0 400 Iph (mA)
The following list points out the limitations of photovoltaic solar energy converters, along with some possible improvements in their efficiency: Reflection losses: The surface of the n+ side semiconductor should be texturized to produce pyramids (roughnesses) before metallization. After the deposition of the thin semitransparent electrode, a thin antireflective coating is then deposited to provide further antireflection. A good antireflective coating should have a refractive index of about two and should be as transparent as possible in the solar energy spectrum. The optimal thickness is of the order of 800 Å. Typical materials for antireflective coating are TiO2, Ta2O3, and Si3N4. Several methods can be used to deposit the antireflective coating, such as vacuum evaporation, spinon or sprayon techniques (spinning or spraying a liquid containing TiO2 or Ta2O3 on the surface), or screenprinting techniques.221 Collection losses: Only those electron–hole pairs generated within the diffusion length from the edge of the depletion region have a chance to contribute to electrical energy. Thus, the larger the diffusion length, the better the conversion efficiency. But both the diffusion coefficient and the lifetime of the minority carriers decrease with increasing concentrations of the doping impurities or unwanted defects, so the diffusion length is limited and cannot be increased much. Voltage factor: The opencircuit voltage Voc is smaller than Eg /q simply because EFn  EFp < Eg. Only when the injection level becomes extremely high may Voc approach the value of Eg /q, but such a high injection level can never be reached from sunlight. Effect of series resistance: For p–n junctions, series resistance is the sum of the contact resistance and the bulk resistance of the semiconductor. The voltage drop across the series resistance reduces the effective potential across the junction, increases the internal power dissipation, and decreases the fill factor. In general, the contact resistance can be reduced to a negligible value, but the bulk resist
199
300
Rs = 200Wcm Maximum Power Rectangle
Rs > 200Wcm
200 100 0
0.1 0.2 0.3 0.4 0.5 0.6 Vph (v)
Figure 363 The effect of the series resistance RS on the photocurrent (Iph)  photovoltage (Vph) characteristics. Solid lines are theoretical curves; xxx represent the experimental data from a GaAs photovoltaic device.
200
Dielectric Phenomena in Solids
ation that can be converted into electrical energy. The absorption coefficient of a material depends on the wavelength of the incident radiation. The absorption of light in a semiconductor is determined by several mechanisms, of which the two most important are fundamental absorption and free carrier absorption. Fundamental absorption refers to the absorption by which a photon with energy equal to or larger than Eg will generate one electron–hole pair with the excess energy, DE = hu  Eg, if any, being dissipated as thermal energy and thus lost for photovoltaic conversion. Free carrier absorption refers to the absorption by free carriers to raise their energy level in the conduction or the valence band without contribution to energy conversion. Total absorption coefficient a (l) is defined as the reciprocal of the distance for the energy to fall by a factor of e. Thus, a (l) is a (l ) = a f + a fc
(3185)
where af and afc are, respectively, the fundamental and the free carrier absorption coefficients. The absorption coefficient a (l) depends strongly on whether the semiconductor is crystalline or amorphous, and in the case of a crystalline semiconductor, whether it is a direct or indirect gap semiconductor. In a crystalline semiconductor, both energy and momentum must be conserved when an electron makes a transition from the valence band to the conduction band. In a direct gap semiconductor, such as GaAs, optical transition does not need a change in momentum, so it has a large absorption coefficient. In an indirect gap semiconductor, such as Si, an optical transition for an electron with the energy even equal to Eg is only possible if, at the same time, a suitable phonon is available to help the electron to satisfy the momentum conservation for the transition. In this case, the probability of light absorption is much smaller; hence, Si has a much lower absorption coefficient. Possible ways to improve conversion efficiency: Sunlight consists of photons having different energies and associated wave
lengths. For p–n junctions with a constant energy gap, the maximum conversion efficiency for Si crystal p–n junction solar cells is 21.6%, and that for GaAs is 23%. Several methods may lead to the improvement of conversion efficiency: • We may use a proper doping impurity grading to increase the absorption of those photons with energies lower than Eg. • We may use multitransition materials with two or more trapping levels in the energy band gap, as shown in Figure 364. • We may use suitable heterojunction structures, inlcuding nSipGaAs, pGa1xAlx As– pGaAsnGaAs, etc.223,224 A typical heterojunction solar cell is shown schematically in Figure 365. The basic principle is that the two junctions can occur in materials of different energy gaps, so that each can make efficient use of a different portion of the solar spectrum. Usually, the large energy gap material is on top and absorbs the short wavelength radiation first. The longer wavelength radiation is captured by the smaller energy gap material. Reduction of cost per unit power generated by solar cells: Thin film solar cells have been developed to reduce fabrication cost and increase the exposure area of the solar cell to incident sunlight. The most promising material for high conversion efficiency and lowcost thin film solar cells is cadmium telluride (CdTe). The cell consists of a heterojunction between II–IV compounds, such as between ptype copper telluride (Cu2Te) and ntype CdTe. The behavior is very similar to a heterojunction between ptype CdTe and ntype CdS solar cell. The conversion Conduction Band
EC Et 1 (First Trap Level)
Possible Transitions
Et 2 (Second Trap Level) Valence Band
EV
Figure 364 Schematic illustration of a material having multitrap levels in the energy band gap for increasing the light absorption in different wavelengths.
Optical and ElectroOptic Processes
201
hu
p–AxGa1–x As p–GaAs
n–GaAs
(a) Ec hu
Eg1 p–AxGa1–x As
Eg2
Voc
p–GaAs Ev
n–GaAs
(b) Figure 365 Schematic diagrams illustrating (a) the basic structure of pAlXGao(1x)As–pGaAs–nGaAs heterojunction solar cell, and (b) the energy band diagram for this solar cell with Eg1 > Eg2.
efficiency of such II–VI compound thin film solar cells has reached about 17%.225 Most thin films are polycrystalline. For further cost reduction, amorphous siliconbased solar cells may provide the solution. This will be discussed in the next section.
PIN Structures for Amorphous SiBased Photovoltaic Devices It is important to understand the basic concept of why amorphous silicon (aSi) has the potential for lowcost photovoltaic devices and why a pin structure must be used for such devices. Amorphous materials have no longrange order; the concept of crystal momentum is not
applicable, and they are not conserved in optical transition as they are in crystals. The lack of longrange order results in two important features: • The absorption coefficient in the solar light energy spectrum for aSi is about an order of magnitude higher than that for crystalline Si at the maximum solar light wavelength near 5000 Å. • A high concentration of defects exists in the energy gap. In crystalline Si photovoltaic devices, the p–n junction structure is generally used, in which the space charge (depletion) region width is generally between 0.1% and 1.0% of the device
202
Dielectric Phenomena in Solids
thickness. Almost all of the carriers are photogenerated in the neutral (fieldfree) regions outside the space charge region; therefore, the minority carrier lifetime must be longer than the time required for them to travel to the space charge region edge, so that they can be collected at the terminals. In amorphous Si photovoltaic devices, the carrier collection process is quite different. Amorphous Si has a high absorption coefficient but a low mobility, implying a low diffusion length. In order to eliminate the dangling bonds for obtaining good electronic and optical properties, aSi must be incorporated with hydrogen and become aSi:H. Generally, the optical gap and the diffusion length decrease with increasing impurity content. This implies that the p–n junction structure is not suitable for aSi:H–based photovoltaic devices. It is necessary to adopt a pin structure to provide an undoped ilayer in which an internal field is created so that the carriers photogenerated in the ilayer are strongly attracted toward the regions in which they are the majority carriers. The thicknesses of the three layers are typically 0.5 mm for the ilayer and 0.01 mm for both the n and the players. The ilayer normally refers to an insulating layer, but here, it refers to an intrinsic or undoped aSi:H layer. Because of the large internal field, photogenerated carriers can be collected even though their lifetime is small, since the collection mechanism does not depend strongly on carrier lifetime. It is a drift transport throughout almost the entire device, thus yielding a good collection efficiency. In aSi:H pin structures, diffusion outside the field region is less important. Figure 366 illustrates the basic structure of an aSi:H pin homojunction solar cell and the energy band diagrams at thermal equilibrium and under solar radiation. In the crystalline Si p–n homojunction, the diffusion current is larger than the drift current, whereas in the aSi:H p–i–n homojunction, the drift current is larger than the diffusion current. This may be the basic difference between these two types of solar cells. In aSi:H pin solar cells, the carrier transport is characterized by the drift length, which is mFt, where F is the internal
field in the ilayer and m and t are the carrier mobility and lifetime, respectively. For good collection efficiency, the drift length must be larger than the ilayer thickness. However, the high absorption in the front ptype aSi:H or ntype aSi:H thin layer reduces the light penetration into the ilayer. To overcome this disadvantage, a heterojunction structure has been developed by employing a wide bandgap, borondoped aSiC:H layer as a front window, as shown in Figure 367. It is important to increase the light input to the ilayer and also to increase the absorption of the long wavelength portion of the solar light spectrum. The latter can be achieved by using a narrow bandgap material such as aSiGe:H behind the ilayer.227 The advantage of using aSiC:H is that the optical gap of this material can be adjusted from 1.8 eV to 2.8 eV simply by adjusting the value of x in the gas mixture [SiH4(1x) CH4x] when fabricated by a highfrequency glow discharge technique in a plasma reaction chamber, the optical gap increasing with increasing x. Unlike crystalline materials, where there is no latticematching problem, aSi:H can form junctions with any material. By carefully reducing the unwanted impurities using an ultrahigh vacuum (UHV) chamber of 109 torr, Nakano et al.228,229 have achieved a conversion efficiency of 11.7% for a cell of 1 cm2 and 9.72% for a cell module of 100 cm2 size of a pin heterojunction structure, as shown in Figure 367. The ilayer usually consists of a large amount of unwanted impurities (1019 to 1021 cm3) such as O, N, C. These impurities have a strong influence on film properties, space charge density, and lightinduced degradation. The concentrations of such impurities depend on the method used for film fabrication. It has been found that there are two types of lightinduced degradation—one related to impurities and the other to structural defects— and that the reduction of the oxygen and SiH2 contents will result in improvement of conversion efficiency.228,229 For more details about the p–n junction and amorphous pin junction photovoltaic devices and solar cells, see references 168, 218, 221, 226, and 230–236.
Optical and ElectroOptic Processes
203
Indium Tin Oxide (ITO) Glass
Al Electrode hn
n+
p+
i Layer
(a) EC
EF
EV
(b) EC EFn Voc hu EFp
EV
(c) Figure 366 Schematic diagrams showing (a) the basic structure of an amorphous silicon aSi:H pin solar cell, (b) the energy band diagram at thermal equilibrium, and (c) the energy band diagram under light illumination.
3.6.3
Photosynthesis Photovoltaic Effects
In general, photosynthesis refers to a process utilizing light (usually sunlight) to convert carbon dioxide and water into carbohydrates and oxygen. This usually occurs in green plants. In living systems, chlorophyll and the lipid membrane are liable to change, but they are continuously renewed to maintain a dynamic stability. For photovoltaic devices, we may use a similar photosynthesis process, but we must use a more stable sensitizer to react with light in a manner similar to chlorophyll or the lipid membrane. In inorganic materials, which are generally more stable than organic materials, it has been found that transition metal complexes are very stable and have good
light absorption properties. Titanium dioxide (TiO2) is one of these inorganic materials. It is a semiconductor with a large band gap, but it does not absorb visible light. So, a thin TiO2 film consisting of TiO2 particles of a few nanometers size, coated with a monolayer of charge transfer dye, will form a sensitizer. Usually, the film is about 5 mm thick, deposited on a transparent conductive layer of fluorinedoped thin oxide, as shown in Figure 368(a). In the case of ntype TiO2 film, electrical current is produced when light absorbed by the dye molecules generates electrons, which are then injected into the conduction band of the semiconductor TiO2. The minority carriers (holes in the present case) do not participate in the photovoltaic conversion. However, to complete the
204
Dielectric Phenomena in Solids Glass
ITO
hn
i Layer (aSi : H)
p
pSi1–xCx : H
Back Contact (Stainless Steel)
n
nSiGe : H
(a) EC
Eg1
EC EFn
Eg2 hu
Voc
EFp
Eg3
EV
EV Eg1 > Eg2 > Eg3
(b) Figure 367 Schematic diagrams showing (a) the basic structure of an amorphous pSi1xCX:H–iSi:HnSiGe:H heterojunction pin solar cell and (b) the energy band diagram for this solar cell with Eg1 > Eg2 > Eg3 under light illumination.
current flow circuit, the dye must be regenerated. This is done by the transfer of the electrons from redox species in the electrolyte to the dye. The counter electrode will collect the electrons from the semiconductor and then return them to the electrolyte. In the electrolyte–dye region, the electrolyte is reducing (Red) when there is electron transfer from the electrolyte to the dye, because reducing means an increase in negative charge or a gain of electrons in the dye. Similarly, the electrolyte is oxidizing (Ox) when there is electron transfer from the dye to oxidized species in the electrolyte, because oxidation means a decrease in negative charge or a loss of electrons in the dye. A redox reaction may be simply expressed by Ox + e  X Red
The Red species is equivalent to an occupied electron state in the valence band, whereas the Ox species is equivalent to an empty electron state in the conduction band. The Red and Ox species are separated by an energy gap, thus
energy is required for an electron to transfer from the former to the latter. This energy gap is analogous to the energy band gap in an intrinsic semiconductor. Figure 368(b) illustrates schematically how electrons are photogenerated and then injected from the dye to the TiO2 semiconductor under sunlight radiation. The electrons are transported from the semiconductor to the counter electrode and then return to the electrolyte, which has transferred electrons to recombine with holes photogenerated in the dye, thus completing the electron flow circuit. This device operates entirely on majority carriers (electrons in the present case), in contrast to conventional p–n junctions, whose photovoltaic performance depends almost entirely on minority carriers and their diffusion lengths. Between the counter electrode and the sensitizer is an electrolyte containing a redox couple, that is, iodine and iodide. The electrons reduce iodine to iodide ions, which diffuse from the counter electrode to the sensitizer, where they regenerate the cations in the dye;
TiO2 Colloidal Layer
Electrolyte Conducting Glass
Dye
hu
Fluorinedoped SnO2
Transparent Conducting Layer
Load
(a) Dye
Electrolyte
Conducting Glass Electrode
TiO2 Semiconductor E
(S +/S –) e– 3
Vph
2 1
hu 4 (R /R –) e– 5
e–
(S +/s )
e–
e–
e–
e– Load
(b) Figure 368 Schematic diagrams showing (a) the basic structure of a photosynthesis phovoltaic device and (b) the photosynthetic process for producing photovoltaic voltages.
Dielectric Phenomena in Solids
simultaneously, the iodide is oxidized back to iodine. The cycling of the redox species enables the conversion of light into electrical current. The photovoltage Vph generated by this process is the difference between the Fermi level of the TiO2 under light illumination and the Nernst potential of the redox couple in the electrolyte. At this time, the conversion efficiency of this type of photovoltaic solar cell has reached about 10%, and the cost is expected to be much lower than that of conventional silicon solar cells. However, more research and development are required to make this new idea feasible for practical applications. For more details about this type of photovoltaic device, see references 237–242. 3.6.4 Anomalous Photovoltaic Effects Some semiconductors in thin film form exhibit a high photovoltage when exposed to intense light, and in some cases the photovoltages may reach a value as high as 5000 V, for example, in III–V compound semiconductor films.243 Such an anomalous photovoltaic phenomenon has been observed in many semiconductor films, such as germanium,244,245 silicon,246 and many compound semiconductors.99 The semiconductor films exhibiting such anomalous behavior are usually fabricated using an oblique vapor deposition technique. This means that when a film is grown, the insulating substrate must be inclined with respect to the plane normal to the direction of evaporating vapor for deposition. In general, the angle of inclination between the direction of evaporation and the direction normal to the substrate plane must be in the range of 30 to 60 degrees. This phenomenon is sensitive to film preparation processes. Apart from the inclination of evaporation direction, this phenomenon depends on the substrate temperature during oblique deposition, which should be in the range of 50–100°C, and also on the pressure and the composition of the gases in the deposition chamber in which the film is fabricated. It may also depend on the substrate material and its surface treatment, film thickness, adsorption of oxygen, etc.99 Opencircuit photovoltages as
functions of light intensity for some semiconductors are shown in Figure 369. The experimental results are from Adirovich, Rubinov, and Yuabov.247 Photovoltage generally increases with decreasing temperature. Several models have been put forward to explain such anomalous phenomena. However, none of them can account for all observed phenomena. It is generally believed that the large photovoltage along the length of the film is due to the addition of photovoltages generated in microelements connected in a series arrangement. Such microelements could be micro p–n junctions, the Dember effect in microcrystals separated by grain boundaries, or both. It is also believed that surface recombination, which may lead to anomalous photogenerated carrier distribution, is responsible for the photovoltage polarity and the spectral sensitivity of the films.248,249 Obviously, anomalous photovoltaic effects are interesting and may be important for device applications. However, further work, both experimental and theoretical, is needed to clarify the ambiguities. Obliquely deposited semiconductor films generally exhibit the same polarity of photovoltages regardless of the angle of the incident
500
CdTe
400 Vph (volts)
206
300 GaAs
200
100
Si Ge 0
100
200
300
I ¥ 10–3 (Lux) Figure 369 The photovoltage of Vph as a function of incident light intensity I for various semiconductor thin films fabricated with an oblique vapor deposition technique.
Optical and ElectroOptic Processes Voc (Volts)
3.0
Light Beam q
Broad Beam
2.0 1.0
Narrow Beam
–20 –10
Film
207
–80 –70 –60 –50 –40 –30
10 20 30 40 50 60 70 80 –1.0
q (degrees)
Substrate –2.0 –3.0
(a)
(b)
Figure 370 (a) The experimental arrangement for the observation of the anomalous photoangular effect and (b) the variation of the photovoltaic opencircuit voltage (VOC) with the angle (q) of the incident light beam.
light direction with respect to the film, even when the film is illuminated through its substrate. However, there is another anomalous photovoltaic effect. In this case, the films are relatively thicker (≥2 mm) and polycrystalline. The film is usually deposited by a vapor deposition technique, with the vapor traveling across a small gap between the vapor source and the substrate. The deposition is normal to the substrate, so that the structure of such films should be quite different from obliquely deposited films. When such a film is illuminated normally with a light beam, no photovoltage appears, but as the light beam is tilted with respect to the normal direction, as shown in Figure 370(a), a photovoltage will be generated and increases with increasing tilting angle, as shown in Figure 370(b). The polarity of the photovoltage along the film depends on the direction of the light beam. The photovoltage appears only when the light beam is illuminating the film surface directly. No photovoltage appears if the film is illuminated indirectly through the substrate.250 This angularly anomalous photovoltaic effect may be associated with the existence of an array of angular ridges on the film surface, and the development of the photovoltage due to nonuniform concentration of photogenerated carriers in the ridges. This phenomenon may be similar to the Dember effect occurring in an angularly shaped crystal, observed by Dember in 1932.207 A more detailed account of anomalous photovoltaic effects can be found in reference 99.
References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18.
H.W. Leverenz, An Introduction to Luminescence of Solids, (Dover, New York, 1968). R.A. Wheadon, Principles of Light and Optics, (Longmans, London, 1980). R.W. Ditchburn, Light, Vols. I and II, (Academic Press, New York, 1976). M. Born and E. Wolf, Principles of Optics, 5th ed. (Pergamon, Oxford, 1975). J. Wilson and J.F.B. Hawkes, Optoelectronics, (Prentice Hall, New York, 1989). A.A. Michelson, Amer. J. Science, 22, 120 (1881); Phil. Mag., 13, 256 (1882) and 31, 338 (1891), and 34, 280 (1892). Lord Rayleigh, Phil Mag., 34, 407 (1892). W.E. Williams, Applications of Interferometry, (Methuen, London, 1957). H. Fizeau, Ann. Chim. Phys., 66, 429 (1862). F.H. Rolt, Engineering, 144, 162 (1937). C.F. Meyer, The Diffraction of Light, Xrays, and Material Particles, (University of Chicago, Chicago, 1934). G.B. Airy, Phil. Mag., 2, 20 (1833); also Ann. Phys. und Chem., 41, 512 (1837). M. Spencer, Fundamentals of Light Microscopy, (Cambridge University Press, Cambridge, 1982). E. Malus, Optique Diotrique, J. Ecole Polytechn., 7, pp. 1–44, 84129 (1805). D. Brewster, Phil. Trans., 125 (1815). A.R. Von Hippel, Dielectrics and Waves, (Wiley, New York, 1954). O.S. Heavens, Optical Properties of Thin Films, (Dover, New York, 1965). F. Goos and H. Hanchen, Ann. Phys., 6, 1 (1947).
208
19. 20. 21. 22. 23. 24. 25. 26.
27.
28.
29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42.
Dielectric Phenomena in Solids
F. Pockels, Lehrbuch de Kristalloptik, (Taubner, Leipzig, 1906); also Ann. d. Physik, 87, 158, (1889). F.A. Jenkins and H.E. White, Fundamentals of Optics, (McGrawHill, New York, 1976), Chapter 32. A. J. Moulson and J.M. Herbert, Electroceramics, (Chapman and Hall, London, 1990). A. Yariv and P. Yeh, Optical Waves in Crystals, (Wiley, New York, 1984). P. Lorrain and D. Corson, Electromagnetic Fields and Waves, 3rd Edition, (Freeman, New York, 1988), Chapter 9. J. Kerr, Phil. Mag., 4 (50), 337 (1875). R. Coelho, Physics of Dielectrics, (Elsevier, Amsterdam, 1979). C.J.F. Bottcher and P. Bordewijk, Theory of Electric Polarization: Dielectrics in Time Dependent Fields, (Elsevier, Amsterdam, 1978). C.G. Le Fevre and R.J. Le Fevre, “The Kerr Effect” in Techniques of Chemistry, Vol. 1, edited by A. Weissberger and B.W. Rossiter (Wiley, New York, 1972), p. 399. S. Kielich, “ElectroOptic Properties of Dielectrics” in Dielectric and Related Molecular Processes, Vol. 1 (The Chem. Soc., London, 1972), p. 278. M. Zahn, IEEE Trans. Dielectrics and Elect. Insul., DEI6, 627 (1998). A.D. Buckingham, Proc. Phys. Soc., B69, 344 (1956). G. Mayer and F. Gires, Compt. Rend., B258, 2039 (1964). C.C. Wang, Phys. Rev., 152, 149 (1966). G. Haertling, Am. Ceram. Soc. Bull., 43, 875 (1964). C. Land and P. Thatcher, Proc. IEEE, 57, 751 (1969). P. Thatcher and C. Land, IEEE Trans. Electron. Devices, ED16, 515 (1969). R.C. Buchanan (Ed.), Ceramic Materials for Electronics, (Marcel Dekker, New York, 1986). L.M. Levinson (Ed.), Electronic Ceramics, (Marcel Dekker, New York, 1988). J.M. Herbert, Ferroelectric Transducers and Sensors, (Gordon and Breach London, 1982). G. Haertling, Am. Ceram. Soc. Bull., 49, 564 (1970). G. Haertling and C. Land, Ferroelectrics, 3, 269 (1972). T.S. Narasimhamurty, Photelectric and ElectroOptic Properties of Crystals, (Plenum, New York, 1981). M.E. Lines and A.M. Glass, Principles and Applications of Ferroelectrics and
43. 44. 45. 46. 47. 48. 49. 50.
51. 52. 53. 54. 55. 56. 57. 58. 59. 60. 61. 62. 63. 64. 65. 66.
Related Materials, (Clarendon, Oxford, 1977). J.C. Purfoot and G.W. Taylor, Polar Dielectrics and Applications, (Macmillan, London, 1979). A. Ashkin, G.D. Boyd, J.M. Dziedzik, R.G. Smith, A.A. Ballman, and K. Nassau, Appl. Phys. Lett., 9, 72 (1966). F.S. Chen, J. Appl. Phys., 38, 3418 (1967). F.S. Chen, J. Appl. Phys., 40, 3389 (1969). F.S. Chen, J.T. LaMcChia, and D.B. Fraser, Appl. Phys. Lett., 13, 723 (1968). A.M. Glass, D. von der Linde, and T.J. Negran, Appl. Phys. Lett., 25, 233 (1974). P. Gunter, Physics Report, 93, (No. 4), 199 (1982). P.S. Brody, U. Efron, J. Feinbery, A.M. Glass, R.W. Hellwarth, R.R. Neurgaonkar, G. Rakuljic, G.C. Valley, and C. Woods, “Photorefractive and Liquid Crystal Materials” in “Research on NonLinear Optical Materials: An Assessment,” Applied Optics, 26, 211 (1987). E.H. Turner, Appl. Phys. Lett., 8, 303 (1966). S.H. Wemple, M. DiDonenico, Jr., and I. Connlibel, Appl. Phys. Lett., 12, 209 (1968). G. Chanussot and A.M. Glass, Phys. Lett., 50A, 405 (1976). G. Chanussot, Ferroelectrics, 20, 37 (1978). H. Kogelnik, Bell Syst. Tech. J., 48, 2909 (1969). N.V. Kukhtarev, V.B. Markov, S.G. Odulov, M.S. Soskin, and V.L. Vinetskii, Ferroelectrics, 22, 949 and 961 (1979). M.D. Ewlank, R.R. Neurgaonkar, and W.K. Carg, J. Appl. Phys., 62, 374 (1987). J. Bodriguez, A. Sichnakoun, and G. Salano, Appl. Optics, 26, 1732 (1987). A.M. Glass, Optical Engineering, 17, 470 (1978). D.I. Staebler and J.J. Amodei, J. Appl. Phys., 43, 1042 (1972). J.P. Huignard, J.P. Herriau, and T. Valentin, Appl. Optics, 16, 2796 (1977). J.P. Huignard and J.P. Herriau, Appl. Optics, 16, 180 (1977). J.P. Huignard, J.P. Harriau, and F. Micheron, Appl. Phys. Lett., 26, 256 (1978). J.P. Huignard, J.P. Herriau, and F. Micheron, Ferroelectrics, 11, 393 (1976). V. Harkov, S. Odulov, and M. Soskin, in Optics and Laser Technology, (April 1979), p. 95. B. Lax and S. Zwardling, Progress in Semiconductors, 5, 251 (1966).
Optical and ElectroOptic Processes
67. 68. 69. 70. 71. 72. 73. 74. 75. 76. 77. 78. 79.
80. 81. 82. 83. 84. 85. 86. 87. 88. 89. 90. 91. 92. 93.
L.M. Roth, Phys. Rev., 133A, 542 (1964). W. Voigt, Phys. Z., 8, 612 and 815 (1905). T.S. Moss, G.J. Burrell, and B. Ellis, Semiconductor OptoElectronics, (Wiley, New York, 1973). A. Yariv, Quantum Electronics, (Wiley, New York, 1975). C.L. Chen, Elements of OptoElectronics and Fiber Optics, (Erwin, Chicago, 1996). R. Adler, IEEE Spectrum, 4, 42 (1967). I.C. Chang, IEEE Trans. Sonic and Ultrasonics, SU23, 2 (1976). A. Korpel, Proc. IEEE, 69, 48 (1981). G. Herzberg, Atomic Spectra and Atomic Structure, (Dover, New York, 1944). G.N. Lewis, Valence and the Structure of Atoms and Molecules, (Dover, New York, 1966). A.E. Ruark and H.C. Urey, Atoms, Molecules and Quanta, Vols. I and II, (Dover, New York, 1964). A.H. Compton, Xrays and Electrons, (Van Nostrand, New York, 1926). A.C.G. Michell and M.W. Zemansky, Resonance Radiation and Excited Atoms, (Cambridge Univ. Press, Cambridge, 1971). E.U. Condon, The FranckCondon Principle and Related Topics, Am. J. Phys., 15, 365 (1947). J.B. Birks, PhotoPhysics of Aromatic Molecules, (Wiley, New York, 1970). C.H. Gooch, Injection Electroluminiescent Devices, (Wiley, New York, 1973). P.T. Landsberg, Phys. Stat. Sol., 41, 457 (1970). C. BenoitalaGuillauma and J. Cernogora, J. Phys. Chem. Solids, 24, 383 (1963). V. Kryukova, Soviet Phys. Solid State, 7, 2060 (1966). M. Lax, J. Phys. Chem. Solids, 8, 66 (1959). M. Lax, Phys. Rev., 119, 1502 (1960). J.S. Blackemore, Semiconductor Statistics, (Pergamon, Oxford, 1962). K.C. Kao, J. Appl. Phys., 55, 752 (1984). D.L. Greenaway and G. Harbeke, Optical Properties and Band Structure of Semiconductors, (Pergamon, Oxford, 1968). T.S. Moss, Optical Properties of Semiconductors, (Butterworths, London, 1959). R.A. Smith, Semiconductors, (Cambridge Univ. Press, Cambridge, 1978). P.T. Landsberg, Lectures—Theor. Phys. Summer Institute, (Univ. of Colorado Press, Boulder, 1966), 8A, p. 313.
94. 95. 96. 97.
98. 99. 100. 101. 102. 103. 104. 105. 106. 107. 108. 109. 110. 111. 112. 113. 114.
115. 116. 117. 118. 119. 120. 121.
209
V.L. BonchBruevich and E.G. Landsberg, Phys. Stat. Sol., 29, (1968) pp. 9–43. L. Rosenfeld, Theory of Electrons, (North Holland, Amsterdam, 1951). P. Norzieres and D. Pines, Phys. Rev., 109, 741 (1958). R.W. Ditchburn, Eye Movement and Visual Perception, (Oxford Univ. Press, Oxford, 1973); also Light, (Blackie, London, 1952). J.T. Houghton and S.D. Smith, Infrared Physics, (Clarendon, Oxford, 1966). J.L. Pankove, Optical Processes in Semiconductors, (Dover, New York, 1975). W. Franz, Z. Naturforsch, 13A, 484 (1958). L.V. Keldysh, Soviet Physics, (JETP), 7, 788 (1958). L.V. Keldysh, J. Exptl. Theoret. Phys. (U.S.S.R.), 47, 1945 (1965); English translation: Soviet Phys. JETP, 20, 1307 (1965). S. Wang, Solid State Electronics, (McGrawHill, New York, 1966), p. 369. T.S. Moss, J. Appl. Phys., Supplement, 32, 2136 (1966). G.S. Paige and H.D. Rees, Phys. Rev. Lett., 16, 444 (1966). A. Frova and P. Handler, Phys. Rev., 137A, 1857 (1965). R. Williams, Phys. Rev., 117, 1487 (1960). E.O. Kane, J. Phys. Chem. Solids, 12, 181 (1959). T.N. Morgan, Phys. Rev., 148, 890 (1966). J. Frenkel, Phys. Rev., 38, 309 (1931). R. Peierls, Ann. Phys. 13, 905 (1932). G.H. Wannier, Phys. Rev., 52, 191 (1937). N.F. Mott, Trans. Faraday Soc., 34, 500 (1938). A.S. Davydov, Theory of Molecular Excitons, translated by M. Kasha and M. Oppenheimer, (McGrawHill, New York, 1962). F.O. Rice and F. Teller, The Structure of Matter, (Wiley, New York, 1949). P.W. Baumeister, Phys. Rev., 121, 359 (1961). E.F. Gross and A. Kaplianski, Zh. Tekh, Fiz., 25, 2061 (1955). H. Meier, Organic Semiconductors, (Verlag Chemie, Weinheim, Germany, 1974). M. Pope and C.E. Swenberg, Electronic Processes in Organic Crystals, (Clarendon, Oxford, 1982). D.L. Dexter and R.S. Knox, Excitons, (Wiley, New York, 1965). R.S. Knox, Theory of Excitons, Solid State Physics Supplement 5, (Academic Press, New York, 1963).
210
122. 123. 124. 125. 126. 127. 128. 129. 130. 131. 132. 133. 134. 135. 136. 137. 138.
139. 140. 141. 142. 143. 144. 145. 146.
147.
Dielectric Phenomena in Solids
M. Trlifaj, Czech, J. Phys., 8, 510 (1958). R.W. Munn and W. Siebrand, J. Chem Phys., 52, 47 (1970). R.C. Powell and Z.G. Soos, Phys. Rev., B5, 1547 (1972). D.L. Dexter, J. Chem Phys., 21, 836 (1953). M. Pope, J. Chem. Phys., 47, 2197 (1967). G.R. Johnston and L.E. Lyon, Chem. Phys. Lett., 2, 489 (1968). C.L. Braun and G.M. Dobbs, J. Chem. Phys., 53, 2718 (1970). S. Singh, W.J. Jones, W. Siebrand, B.P. Stoicheff, and W.G. Schneider, J. Chem. Phys. 42, 330 (1965). W. Helfrich and F.R. Lipsett, J. Chem. Phys., 43, 4368 (1965). H.C. Wolf and K.W. Benz, Pure Appl. Chem., 27, 439 (1971). R.C. Powell and Z.G. Soos, J. Luminescence, 11, 1 (1975). N. Wakayama and D.F. Williams, J. Chem. Phys., 57, 1770 (1972). M. Schott and I. Berehar, Mol. Cryst. Liq. Cryst. 20, 13 (1973). M. Pope, J. Burgos, and N. Wotherspoon, Chem. Phys. Lett., 12, 140 (1971). R.R. Chance and A. Prock, Phys. Stat. Sol. (b), 57, 597 (1973). M.E. MichelBeyerle, W. Harengel, and R. Haberkorn, Mol. Cryst. Liq. Cryst., 25, 323 (1974). S.A. Rice and J. Jortner, “Comments on the Theory of the Excited States in Molecular Cyrstals,” in Physics and Chemistry of Organic Solid State, edited by D. Fox, M.M. Labes, and A. Weissberger, 3, (1967) pp. 199–497. M.G. Sceats and S.A. Rice, J. Chem. Phys., 62, 1098 (1975). J.R. Lakowicz, Principles of Fluorescence Spectroscopy, (Plenum, New York 1983). L. Onsager, Phys. Rev., 84, 554 (1938). D. Curie, Luminescence in Crystals, (Methuen, London, 1963). P. Avakian and R.E. Merrifield, Mol. Cryst., 5, 37 (1968). W. Seibrand, J. Chem. Phys., 42, 3951 (1965). M. Pope and R. Selsby, Chem. Phys. Lett., 14, 226 (1972). T.G. Dewey (Ed.), Biophysical and Biochemical Aspects of Fluorescence Spectroscopy, (Plenum, New York, 1991). W.T. Mason, Fluorescent and Luminescent Probe for Biological Activity, (Academic Press, New York, 1993).
148. 149. 150. 151. 152. 153. 154. 155. 156. 157. 158. 159. 160. 161. 162. 163. 164. 165. 166. 167. 168. 169. 170. 171.
A.A. Bergh and P.J. Dean, LightEmitting Diodes, (Oxford University Press, Oxford, 1976), Chapter 5. K. Gillessen and W. Schaiver, Light Emitting Diodes—Introduction, (Prentice Hall International, London, 1987). H.F. Ivey, “Electroluminescence and Related Effects,” Advan. Electron. Phys., Supplement 1, 1963. G. Destriau, J. Chem. Phys., 33, 620 (1936). A. Vecht, J. Vac. Sci. Technol., 10, 789 (1973). D. Kahng, Appl. Phys. Lett., 13, 210 (1968). J. Russ and D.I. Kennedy, J. Electrochem. Soc., 114, 1066 (1967). H.K. Henisch, Electroluminescence, (Pergamon, Oxford, 1962). T. Inoguchi and S. Mito, in Electroluminescence, edited by J.I. Pankove, (Springer Verlag, Berlin, 1976). W. Helfrich and W.G. Schneider, Phys. Rev, Lett., 14, 29 (1965). W. Helfrich and W.G. Schneider, J. Chem. Phys., 44, 2902 (1966). W. Hwang and K.C. Kao, J. Chem. Phys., 60, 3845 (1974). A. Suna, Phys. Rev., Bl, 1716 (1970). D.F. Williams and M. Schadt, J. Chem. Phys., 53, 3480 (1970). W. Mehl and B. Funk, Phys. Lett., 25A, 364 (1967). H.P. Schwob and I. ZschokkeGranacher, Mol. Cryst. Liq. Crys., 13, 115 0(1971). M. Kawabe, K. Masuda, and S. Namba, Japan J. Appl. Phys., 10, 527 (1971). N. Wakayama and D.F. Williams, Chem. Phys. Lett., 9, 45 (1971). H.P. Kunkel and K.C. Kao, J. Phys. Chem. Solids, 37, 863 (1976). H.F. Ivey, “Electroluminescence and Semiconductor Lasers,” IEEE J. Quantum Electron., QE2, 713 (1966). S.M. Sze, Physics of Semiconductor Devices, (Wiley Interscience, New York, 1981). F. Gutmann and L.E. Lyons, Organic Semiconductors, (Wiley, New York, 1967). M. Kochi, Y. Harada, I. Hirooka, and H. Inokuchi, Bull. Chem. Soc. Japan, 43, 2690 (1970). R. Williams, “Injection by Internal Photemission,” in Semiconductors and Semimetals, edited by R.K. Willardson and A.C. Beer, Vol. 6, (1970) pp. 97– 139.
Optical and ElectroOptic Processes
172. 173. 174. 175. 176. 177. 178. 179. 180. 181. 182. 183. 184. 185. 186. 187. 188. 189. 190. 191. 192. 193. 194. 195. 196.
197.
G. Vaubel and H. Basessler, Phys. Stat. Sol., 26, 599 (1968). J.M. Caywood, Mol. Cryst. and Liq. Cryst., 12, 1 (1970). W. Ruppel, “The PhotoconductorMetal Contact,” in Semiconductors and Semimetals, 6, (1970) pp. 315–345. A. Rose, Concepts in Photoconductivity and Allied Problems, (Wiley, New York, 1963). R.H. Fowler, Phys. Rev., 38, 45 (1931). A. L. Hughes and L.A. DuBridge, Photelectric Phenomena, (McGrawHill, New York, 1932). J. Kadlec and K. H. Gundlach, Phys. Stat. Sol., (A) 37, 11 (1976). F. Abeles (Ed.), Optical Properties of Solids, (North Holland, Amsterdam and New York, 1972). A. M. Goodman, J. Appl. Phys., 35, 573 (1964). C.A. Mead and W.G. Spitzer, Phys. Rev., 134A, 713 (1964); also Appl. Phys. Lett., 2, 74 (1963). A.M. Cowley and H. Heffner, J. Appl. Phys., 35, 255 (1964). H.G. White and R.A. Logan, J. Appl. Phys., 34, 1990 (1963). J.J. Tietjen and J.A. Amick, J. Electrochem. Soc., 113, 724 (1966). J. Kadlec and K.H. Gundlach, Solid State Commun., 16, 621 (1975). K.H. Gundlach and J. Kadlec, J. Appl. Phys., 46, 5286 (1975). G. Lewicki, J. Maserjian, and C.A. Mead, J. Appl. Phys., 43, 1764 (1972). K.H. Gundlach and J. Kadlec, Appl. Phys. Lett., 20, 445 (1972). C.N. Berglund and R.J. Powell, J. Appl. Phys., 42, 573 (1971). J. Kadlec and K.H. Gundlach, J. Appl. Phys., 47, 672 (1976). R. Williams and J. Dresner, J. Chem. Phys., 46, 2133 (1967). J. Dresner, Phys. Rev. Lett., 21, 356 (1968). E.G. Ramberg, Appl. Optics, 6, 2163 (1967). W.E. Spicer, Phys. Rev., 154, 385 (1967). E.O. Kane, Phys. Rev., 127, 131 (1962). G.W. Gobeli and F.G. Allen, “Photoelectric Threshold and Work Function,” in Semiconductors and Semimetals, edited by R.K. Willardson and A.C. Beer, Vol. 2, (Academic Press, New York, 1966), pp. 263–300. J. Sworakowski, Phys. Stat. Sol. (a) 13, 381 (1972).
198. 199. 200.
201. 202.
203. 204. 205. 206. 207. 208. 209. 210. 211.
212. 213. 214. 215. 216. 217. 218.
219.
211
J. Sworakowski, Phys. Stat. Sol. (a) 22, K73 (1974). K. Seki, T. Hirooka, Y. Kamura, and H. Inokuchi, Bull. Chem. Soc. Japan, 49, 904 (1976). M. Cardona and L. Ley (eds), Photoemission in Solids, Vol. 1 (1978) and Vol. 2 (1979), (SpringerVerlag, New York, 1978 and 1979). S. Yoshimura, J. Phys. Soc. Japan, 28, 701 (1970). B.H. Schechtma, S.F. Lin, and W.E. Spicer, Phys. Rev. Lett., 34, 667 (1975); and also; B.H. Schechtman, Ph.D. thesis, Stanford University, 1968. T. Hirooka, K. Tanaka, K. Kuchitsu, M. Fujihara, H. Inokuchi, and Y. Harada, Chem. Phys. Lett., 18, 390 (1973). W.E. Spicer and R.E. Simon, J. Phys. Chem. Solids, 23, 1817 (1962). R.C. Eden, J.L. Moll, and W.E. Spicer, Phys. Rev. Lett., 18, 597 (1967). M. Pope, H. Kallmann, and J. Giachino, J. Chem. Phys., 42, 2540 (1965). H. Dember, Physik Zeits, 32, 554 and 856 (1931); and 33, 209 (1932). R. Robertson, T.T. Fox, and A.M. Martin, Nature, 129, 579 (1932). T.S. Moss, L. Pincherle, and A.M. Woodward, Proc. Phys. Soc. (London), 66B, 743 (1953). T. Tauc, Rev. Mod. Phys., 29, 308 (1959). H. Kallmann, “Energy Transfer Processes,” in Comparative Effects of Radiation, edited by M. Burton, J.S. Kirby Smith and J.L. Magee, (Wiley, New York, 1960). H. Kallmann and M. Pope, J. Chem. Phys., 30, 585 (1959). I.K. Kikoin and M.M. Noskov, Phys. Z. Sowjet, 5, 586 (1934). O. Garreta and J. Grosvalet, Progress in Semiconductors, Vol. 1, 165 (Heywood, London, 1956). W. Van Roosbrook, Phys. Rev., 101, 1713 (1956). C.A. Mead, Solid State Electron., 9, 1023 (1966). C.R. Crowell, W.G. Spitzer, L.E. Howarth, and E.E. Labate, Phys. Rev., 127, 2006 (1962). H.J. Novel, “Solar Cells” in Semiconductors and Semimetals, Vol. 11, edited by R.F. Willardson and A.C. Beer (Academic Press, New York, 1975). E.H. Rhoderick, Metal–Semiconductor Contacts, (Clarendon Press, Oxford, 1978).
212
220. 221.
222. 223. 224. 225. 226. 227. 228.
229. 230. 231. 232. 233.
234.
Dielectric Phenomena in Solids
H.C. Card and E.S. Yang, Appl. Phys. Lett., 29, 51 (1976). R.J. Van Overstraeten and R.P. Mertens, Physics, Technology and Use of Photovoltaics, (Adam Hilger, Bristol and Boston, 1986). D.A. Jenny, J.J. Loferski, and P. Rappaport, Phys. Rev., 101, 1208 (1956). A.K. Sreedhar, B.L. Sharma, and R.K. Purohit, IEEE Trans. Electron. Devices, ED16, 309 (1969). H.J. Hovel and J.M. Woodall, J. Electrochem. Soc., 120, 1246 (1973). D.A. Cusano, Solid State Electron., 6, 217 (1963). D.E. Carlson, “Solar Cells” in Semiconductors and Semimetals, Vol. 21, Part D (Academic Press, New York, 1984). G. Nakamura, R. Sato, and Y. Yukimoto, Japan J. Appl. Phys., 21, Suppl. 297 (1982). S. Nakano, H. Tarui, T. Takahama, M. Isomura, T. Matsuyama, H. Haku, M. Nishikuni, S. Tsuda, M. Ohnishi, Y. Kishi, and Y. Kuwano, Proc. 7th EC Photovoltaic Solar Energy Conference, Seville, Spain, 1986, p. 27; also Jpn. J. Appl. Phys., 25, 1936 (1986). A. Nakano, S. Ikegama, H. Matsumoto, H. Uda, and Y. Komatsu, Solar Cells, 17, 233 (1986). K. Takahashi and M. Konsgai, Amorphous Silicon Solar Cells, (Wiley, New York, 1986). M. Wolf, Proc. IRE, 48, 1246 (1960). M.A. Green, High Efficiency Silicon Solar Cells (Trans. Tech. Publications, Brookfield, 1987). Y. Hamakawa, “Amorphous Silicon Solar Cells,” in Current Topics in Photovoltaics edited by T.J. Coutts and J. Meakin (Academic Press, New York, 1985), pp. 111–165. C.E. Backus, ed., Solar Cells, (IEEE Press, New York, 1976).
235.
236.
237. 238.
239. 240.
241. 242. 243. 244. 245. 246.
247. 248. 249. 250.
M.A. Green, Solar Cells: Operating Principles, Technology and System Application, (Prentice Hall, New Jersey, 1982). W.C. Sinke, ed., “The Photovoltaic Challenge,” in MRS Bulletin of October 1993 (Materials Research Society, Pittsburgh, 1993), pp. 18–66. B. O’Regan and M. Gratzel, Nature, 353, 737 (1991). M. Gratzel, “Nanocrystalline Thin Film PV Cells,” in MRS Bulletin of October 1993 (Materials Research Society, Pittsburgh, 1993), p. 61. B. O’Regan, J. Moser, M. Anderson, and M. Gratzel, J. Phys. Chem., 94, 8720 (1990). M.K. Nazeeruddin, A. Kay, J. Rodicio, R. HumphreyBaker, E. Muller, P. Liska, N. Vlachopoulos, and M. Gratzel, J. Am. Chem. Soc., 115, 6382 (1993). A. Kay and M. Gratzel, J. Phys. Chem., 97, 6272 (1993). G. Hodes, I.O.F. Howell, and L.M. Peter, J. Electrochem. Soc., 130, 3136 (1992). E.I. Adirovich, T. Mirzamakhmudov, V.M. Rubinov, and Yu. M. Yuabov, Sov. Phys.— Solid State, 7, 2946 (1966). H. Kallmann, G.M. Spruch, and S. Trester, J. Appl. Phys., 43, 469 (1972). W. Ma, R.M. Anderson, and S.J. Hruska, J. Appl. Phys., 46, 2650 (1975). H. Kallmann, B. Kramer, E. Maidemanakis, W.J. McAleer, H. Barkemeyer, and P.I. Pollak, J. Electrochem. Soc., 108, 247 (1961). E.I. Adirovich, Y.M. Rubinov, and Yu. M. Yuabov, Sov. Phys.—Solid State, 6, 2540 (1965). M.I. Korsunskii and M.M. Sominskii, Soviet Phys.—Semicon., 7, 342 (1973). H. Onishi, S. Kurokawa, and K. Leyansu, J. Appl. Phys., 45, 3205 (1974). F.H. Nicoll, J. Electrochem. Soc., 110, 1165 (1963).
4 Ferroelectrics, Piezoelectrics, and Pyroelectrics The whole of science is nothing more than a refinement of everyday thinking. Science is the attempt to make the chaotic diversity of our sense experience correspond to a logically uniform system of thought. Albert Einstein
4.1
Introductory Remarks
The prefix piezo in the word piezoelectrics is derived from a Greek word, piezein, meaning pressure. Piezoelectrics are materials in which electricity can be generated by an applied mechanical stress or a mechanical stress can be produced by an applied electric field. This interconvertible behavior was first discovered by Pierre and Jacques Curie in 1880 in certain crystals, such as quartz, zinc blends, tourmaline, and Rochelle salt.4,5 The term piezoelectricity has been used by scientists since 1881 to distinguish the piezoelectric phenomena from electrostriction. The piezoelectric phenomena occurs in both the ferroelectric and the nonferroelectric states.2,3 The prefix pyro in the term pyroelectrics means heat in Greek. Thus, pyroelectricity means heatgenerated electricity. This effect is also convertible. This implies that heat can be generated by electricity resulting from the change of the state of electric polarization, such as electrothermal and electrocalorie effects. Pyroelectric phenomena were in fact discovered much earlier. Theophrast discovered the pyroelectric phenomena in tourmaline in 314 bc, and the word pyroelectricity has been used since 1824, first by Brewster.6 The theory of the pyroelectric effect was first formulated by W. Thomson (Lord Kelvin) in 1878 and further developed by Voigt in 1897 and later by Born, based on his famous crystal lattice dynamics in 1921 and 1928.7 In general, all materials undergo a small change in dimension when subjected to an external force, such as an applied electric field, a mechanical stress, or a change in temperature
The term ferroelectrics arose by analogy with ferromagnetics, mainly because they have similar characteristics: under electric fields for ferroelectric phenomena and under magnetic fields for ferromagnetic phenomena. The prefix ferro derived from ferum, which means iron in Latin. The term is perfect for ferromagnetics, since all ferromagnetic phenomena are associated with the special type of spin arrangement of the iron atoms. But in ferroelectrics there are no iron atoms, so the prefix does not mean iron. Rather, it implies the similarity in characteristics to ferromagnetics. Like ferromagnetics, ferroelectrics exhibit a spontaneous electric polarization below the Curie temperature, a hysteresis loop, and an associated mechanical strain. However, ferroelectrics differ from ferromagnetics in their fundamental mechanisms and also in some of their applications. In Europe, ferroelectrics are sometimes called Seignette electrics. This term is somewhat misleading, because Seignette did not discover the ferroelectric phenomena. Instead, in 17thcentury Rochelle, France, he discovered Rochelle salt (potassiumsodium tartrate– tetrahydrate, KNaC4H4O6–4 H2O), a colorless crystalline compound with an orthorhombic structure. At that time, the material was used as a laxative. More than 200 years later, in 1921, Valasek discovered the ferroelectric phenomena in the same material.1–3 Ferroelectrics were discovered much later than ferromagnetics. However, there are now more than 1,000 solid materials possessing ferroelectric properties. 213
Dielectric Phenomena in Solids
(heat). Depending on the material structure, such a small change in dimension may result in a change in electric polarization and hence give rise to the occurrence of the ferroelectric, piezoelectric, or pyroelectric effects. It can be imagined that materials exhibiting these effects must be polar and have an electrical order, implying that they must be crystals or polycrystalline materials composed of crystallites. A crystal or a crystallite must have a definite chemical composition, with the molecules made up of positive ions (atoms sharing part of their valence electrons with others) and negative ions (atoms receiving part of electrons from others) occupying lattice sites to constitute a crystal structure lattice. The smallest repeating unit of the lattice is called the unit cell, and the specific symmetry of the unit cell determines whether the crystal exhibits ferroelectric, piezoelectric, pyroelectric, or electrooptic effects. On the basis of the symmetry elements of translational position and orientation, there are 230 space groups. Ignoring translational repetition, these 230 groups break down into 32 classes, known as the 32 point groups. Point groups are based on orientation only.8,9 Any point may be defined by coordinates x, y, and z, with respect to the origin of symmetry. A centrosymmetric crystal is a crystal in which the movement of each point at x, y, z, to a new point at x, y, z, does not cause a recognizable difference. This implies that centrosymmetric crystals are nonpolar and thus do not possess a finite polarization or dipole moment. Of the 32 classes (or point groups), 11 classes are centrosymmetric and 21 classes are noncentrosymmetric, possessing no center of symmetry. The latter is the necessary requirement for the occurrence of piezoelectricity. However, one of the 21 classes, though classified as the noncentrosymmetric class, possesses other combined symmetry elements, thus rendering no piezoelectricity. So, only 20 classes of noncentrosymmetric crystals would exhibit piezoelectric effects. In 10 of these 20 classes, polarization can be induced by a mechanical stress, while the other 10 classes possess spontaneous polarization, so they are permanently polar and thus can have piezo
electric as well as pyroelectric effects. There is a subgroup within these 10 classes that possesses spontaneous polarization and reversible polarization; this subgroup can exhibit all three effects—ferroelectric, piezoelectric, and pyroelectric. In fact, the ferroelectric effect is an empirical phenomenon distinct from piezoelectric and pyroelectric effects in that it exists with a reversible polarization. The relationship between polarization behavior and crystal structure is shown in Figure 41. The 32 point groups are subdivisions of seven basic crystal systems, which are based on the degree of symmetry. In the order of ascending symmetry, these seven basic crystal systems are triclinic, monoclinic, orthorhombic, tetragonal, trigonal (rhombohedral), hexagonal, and cubic. For a more detailed description of these seven systems, see references 8 and 9. Based on the optical properties, these systems can be classified into three major optical groups, as shown in Table 41. The optical biaxial group refers to the crystals in which the molecules are not spherical, with the long axis longer than the axes perpendicular to it. Depending on the structure of the crystal, if the index of refraction in the direction along the long axis is different from that along the direction of the short axis, the crystals are optically biaxial and exhibit birefringence. If the indices of refraction in the two axes are identical, then the crystals are optically uniaxial. However, some Table 41 The seven basic crystal systems. Crystal System
Optical Group
Order of Symmetry
Triclinic
Biaxial
Very Nonsymmetric
Monoclinic
Biaxial
Orthorhombic
Biaxial
Tetragonal
Uniaxial
Trogonal (Rhombohedral)
Uniaxial
Hexagonal
Uniaxial
Cubic
Optically Isotropic
Increasing
214
Very Symmetric
Ferroelectrics, Piezoelectrics, and Pyroelectrics
215
32 Classes Crystal Symmetry Point Groups
21 Classes
11 Classes
Noncentrosymmetric Groups
Centrosymmetric Groups
1 Class
10 Classes
Possessing Other Symmetric Elements (Nonpolar)
Piezoelectric Effect (Polarized under Mechanical Stress)
10 Classes Piezoelectric Effect Pyroelectric Effect (Spontaneously Polarized)
Subgroup of the 10 Classes Ferroelectric Effect Piezoelectric Effect Pyroelectric Effect (Spontaneously Polarized with Reversible Polarization)
Figure 41 Classification of crystals showing the classes with piezoelectric, pyroelectric, and ferroelectric effects.
crystals with their constituent molecules being close to spherical particles in shape; then in such cases the index of refraction is identical in all directions and the crystals are optically isotropic. Apart from the crystals with the structures just described, some synthetic and biological polymers with different structures also exhibit piezoelectric, pyroelectric, and ferroelectric phenomena.10–15 In view of the complex molecular, crystalline, and morphological structures
of polymers, there may exist a possibility that the combined collective and coordinate effects of the structure would satisfy the requirements for the occurrence of piezoelectric, pyroelectric, and even ferroelectric phenomena. Polyvinylidene fluoride (PVDF) polymer is a good example that complies with such requirements under certain conditions. However, polymers are potential materials suited particularly for many practical applications because of their easy processability into
216
Dielectric Phenomena in Solids
thin, tough, and flexible films. We shall discuss polymers having these properties later. In the present chapter, we shall deal only with ferroelectric, piezoelectric, and pyroelectric effects. Electrooptic effects were discussed in Chapter 3.
4.2
properties are also very small. However, there are a number of crystals with a nonsymmetrical structure (see Figure 41) that exhibit a large polarization, with the dielectric constant up to 105, under certain conditions. Obviously, such a large magnitude of polarization has attracted many researchers to study it theoretically and to develop various practical applications. A ferroelectric crystal shows a reversible spontaneous electric polarization and a hysteresis loop that can be observed in certain temperature regions, delimited by a transition point called the Curie temperature, Tc. At temperatures above Tc, the crystal is no longer ferroelectric and exhibits normal dielectric behavior. Ferroelectric materials usually, but not always, exist in a nonpolar state at temperatures above Tc, and have anomalously high dielectric constants, especially near the Curie temperature. Typical dielectric constant–temperature and polarization–temperature characteristics are shown in Figure 42. The dielectric constant increases very rapidly to a very high peak value at Tc. The anomalously high value of er in the neighborhood of Tc is generally referred to as the anomalous value. At T > Tc, anomalous
Ferroelectric Phenomena
Ferroelectricity is one of the most fascinating properties of dielectric solids. Materials exhibiting ferroelectric properties must be either single crystals or polycrystalline solids composed of crystallites; they must also possess reversible spontaneous polarization. In this section, we shall discuss the various features of ferroelectrics, the mechanisms responsible for the appearance of these features, and ferroelectric materials and their applications. 4.2.1 General Features The polarization induced by an externally applied field in normal dielectric materials is very small, with the dielectric constant usually less than 100, and its effects on other physical
er
Tc
T
Tc
T
Tc
T
Barium Titanate
KDP
Rochelle Salt
(a) Tc = 120°C.
(b) Tc = –150°C.
(c) Tc = 24°C.
Ps
Tc
T
Tc
T
Tc
T
Figure 42 Schematic illustration of the variation of the dielectric constant er and the spontaneous polarization of PS with temperature for three typical ferroelectric crystals: (a) Barrium titanate (BaTiO3) with Tc = 120°C, (b) Potassium dihydrogen phosphate (KDP, KH2PO4) with Tc = 150°C, and (c) Potassium Sodium tartratetetrahydrate (Rochelle Salt, KNaC4H4O64H2O) with Tc = 24°C.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
behavior follows closely the Curie–Weiss relation er =
C T  Tc
(41)
where C is known as the Curie constant. In fact, anomalous behavior always appears near any transition point between two different phases, even at T below Tc. At the transition points, there are anomalies not only in the dielectric constant and polarization, but also in piezoelectric and elastic constants and specific heat, because of the change in crystal structure. Ferroelectrics have reversible spontaneous polarization. The word spontaneous may mean that the polarization has a nonzero value in the absence of an applied electric field. The word reversible refers to the direction of the spontaneous polarization that can be reversed by an applied field in opposite direction. The spontaneous polarization Ps usually increases rapidly on crossing the transition point and then gradually reaches a saturation value at lower temperatures. The most prominent features of ferroelectric properties are hysteresis and nonlinearity in the relation between the polarization P and the applied electric field F. The simplest method for measuring spontaneous polarization is the Sawyer and Tower method,16 as shown in Figure 43, in which C is the capacitance of the ferroelectric specimen and Co is the standard capacitor. The voltage across C should be sufficiently large to render a saturation in polarization, so Vo should be proportional to the polarization charge, Vo = AP/Co,
where A is the area of the specimen. V is the applied voltage, which is usually an AC signal voltage of low frequencies. Thus, the applied field across the specimen is F = Vc /d = (V Vo)/d. A typical hysteresis loop is shown schematically in Figure 44. When the field is small, the polarization increases linearly with the field. This is due mainly to fieldinduced polarization, because the field is not large enough to cause orientation of the domains (portion 0A). At fields higher than the lowfield range, polarization increases nonlinearly with increasing field, because all domains start to orient toward the direction of the field (portion AB). At high fields, polarization will reach a state of saturation corresponding to portion BC, in which most domains are aligned toward the direction of the poling field. Now, if the field is gradually decreased to zero, the polarization will decrease, following the path CBD. By extrapolating the linear portion CB to the polarization axis (or zerofield axis) at E, 0E represents the spontaneous polarization Ps and 0D represents the remanent polarization Pr . The linear increase in polarization from Ps to Pp is due mainly to the normal fieldinduced dielectric polarization. Pr is smaller than Ps because when the field is reduced to zero, some domains may return to their original positions due to the P Pp
K
Ps
Vc
B
A
R
F
0
d
C
E D
Pr
C
217
V H Co
Vo G
Figure 43 The Sawyer–Tower method for the measurement of the polarizationelectric field (P–F) characteristics.
Figure 44 Schematic diagram of a typical ferroelectric hysteresis loop.
218
Dielectric Phenomena in Solids
strain situation, thus reducing these domains’ contribution to the net polarization. For most ferroelectric materials, the component due to the normal fieldinduced dielectric polarization is very small compared to the spontaneous polarization; therefore, for most applications, this component can be ignored. The magnitude of the difference between Pp and Ps in Figure 44 is exaggerated for the purpose of clear illustration. The field required to bring the polarization to zero is called the coercive field Fc (portion 0R on zero polarization axis). Fc depends not only on temperature, but also on the measuring frequency and the waveform of the applied field. When the field in the opposite direction decreases to zero, the polarization is reversed, indicating that domains (see Section 4.2.4) have already been formed before poling and that the motion of the domain walls results in the change of direction of polarization. The hysteresis arises from the energy needed to reverse the metastable dipoles during each cycle of the applied field. The area of the loop represents the energy dissipated inside the specimen as heat during each cycle. In general, the hysteresis loop is measured with AC fields at low frequencies, 60 Hz or lower, to avoid heating the specimen. In general, ferroelectricity is harder to demonstrate in polycrystalline materials composed of crystallites, such as ceramics, than in a single crystal because of the random orientation of crystallites. This is why in some single crystals the polarization reverses quite abruptly
to form a square loop, as shown in Figure 45(a), while in most ceramics the loop is rounded, as shown in Figure 45(b), because of the more sluggish reversal, which is due partly to the axes of the unit cells in the randomized arrangement of the nonuniform crystallites. Ferroelectric materials exhibit ferroelectric properties only at temperatures below Tc because they are polar; at temperatures above it, they are not polar. Obviously, the shape of the hysteresis loop depends on temperature. Figure 46 shows the shape of the hysteresis loop for Rochelle salt at two different temperatures. The loop becomes gradually diminished at T > Tc, eventually degenerating to a straight line at T much larger than Tc, when the ferroelectric behavior disappears completely. However, some ferroelectric materials can be driven from the paraelectric state to a ferroelectric state at T > Tc by an applied field larger than a certain critical value Ft . In other words, the applied electric field larger than Ft tends to shift the Curie point to a higher temperature. The higher the temperature above Tc, the higher the field required to induce ferroelectricity. If a ferroelectric material is subjected to a large AC field at a temperature slightly higher than Tc, two small hysteresis loops may appear, as shown schematically in Figure 47. A double hysteresis loop has been observed in BaTiO3 at a temperature a few degrees above Tc.17,18 For the transition from the tetragonal structure to the orthorhombic structure at the transition temperature of 5°C for BaTiO3 at an AC field P
P
P
F
F
P (mC cm–2)
0.50
A 0.25
B
0
F
–0.25 –0.50 –800
–400
0 F (V
(a)
400
800
cm–1)
(b)
Figure 45 Schematic diagrams of (a) the “square” and (b) the “rounded” hysteresis loops.
Figure 46 Temperature dependence of the hysteresis loop for Rochelle salt with Tc = 24°C. (A) T = 19°C < Tc, and (B) T = 42°C > Tc.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
higher than Ft, a triple hysteresis loop, consisting of one main loop and two small loops, has also been observed.19 Using the circuit shown in Figure 43, the voltage across C is proportional to the polar
P
–Fc 2 –Ft
–Fc1 Fc1
Ft
Fc 2 F
Figure 47 Schematic diagram showing a typical double hysteresis loop at T slightly higher than Tc and at F larger than a critical value Ft.
ization P, which is the dipole moments per unit volume and is also equal to the surface charge density on the electrode. During polarization, a current j = dP/dt will flow through the specimen per unit area. Suppose that the wave shape of the switching signal voltage is as shown in Figure 48(a) for two cases: one with the voltage (or field) increasing linearly with time and the other with the field decreasing linearly with time. In this case, the resulting current flowing through the specimen, for a normal linear dielectric, is constant, as shown in Figure 48(b). But if the specimen is a ferroelectric material, the current will be a short pulse, as shown in Figure 48(c). This is one of the simplest ways to distinguish ferroelectric from nonferroelectric materials. The size of the unit cell and the force of ions in the lattice of a crystal are temperature dependent. As the temperature changes, there exists a critical temperature (i.e., the transition temperature), at which a particular structure becomes unstable and tends to transform to a more stable one. Although the transition involves only small ionic movements, they cause a marked change in properties. A change in dimensions of a crystal or a crystallite will
F
(a) Waveform
0
(b) Dielectric
j
F t
0
t
j
P 0
219
t
0
t
F
(c) Ferroelectric P
j
j 0
t
0
t
F
Figure 48 Schematic diagrams showing (a) the waveforms of the linearly timevarying electric field (b) the corresponding current j flowing through the lossfree dielectric material, and (c) the corresponding current j flowing through the ferroelectric material.
220
Dielectric Phenomena in Solids
create internal stresses, particularly at the boundaries between crystallites in polycrystalline materials, such as in ceramics. Under certain conditions, the magnitude of such stresses may be large enough to cause internal cracks. Transition from one crystal structure to another usually involves a change in entropy and volume. In general, there are two different orders of transition. When the spontaneous polarization goes from zero to a finite value, or from one value to another, the change in polarization may be continuous or discontinuous. If there is discontinuity in the change of the polarization, the transition is referred to as a firstorder transition, as in BaTiO3 and KNbO3. See Figure 49(a) and (c). In this case, the entropy changes at a constant temperature (e.g., T = Tc), and consequently the latent heat also changes. If the change of the polarization is continuous, the transition is referred to as a secondorder transition, as in KH2PO4 and Rochelle salt. See Figure 49(b) and (d). In this case, there is no change in entropy and latent heat at the transition temperature. It is interesting to note that at the Curie temperature, the transition in ferromagnetic materials does not involve changes in crystal structure but only a small change in the
coupling forces between the outer electrons of neighboring magnetic ions. Since the dielectric constant of ferroelectric materials is extremely high near the transition temperature, the polarization induced in the paraelectric (nonpolar) region at T > Tc by an applied electric field along the ferroelectric axis goes gradually over into the spontaneous polarization region upon cooling below Tc. The effect of this field tends to shift Tc to a higher temperature, as shown in Figure 49. The polarization–temperature curve shifts to a higher temperature as the applied field is increased. However, the concept of the Curie temperature cannot be applied to ferroelectric materials under the electrically biased condition.18,20 In general, if the direction of the applied field is parallel to the polar direction of any phase, it favors the existence of that phase and extends its temperature range. At Tc, the ferroelectric phase is favored by an applied field; therefore, the Curie temperature is raised. A change in crystal structure and crystal volume caused by any external forces, such as electric fields, mechanical stresses, or hydrostatic pressures, will affect the phase transition. A shear stress is essentially equivalent to an electric field along the ferroelectric axis and Ps
Ps
F2 > F1
F2 > F1 F=0 0
Tc
F1 > 0 T
F=0 0
F1 > 0
Tc
T
Tc
T
(b)
(a)
Ps
Ps T lowering T returning up 0
Tc
(c)
T
0
(d)
Figure 49 Schematic diagrams illustrating the effect of applied electric field on (a) first order transition and (b) second order transition, and the shift of the transition point when the temperature is returning up (increasing), (c) Tc shifts to a higher temperature for the first order transition, and (d) there is no shift for the second order transition.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
therefore would have a similar effect on the polarization–temperature curve, as shown in Figure 49. It should be noted that in Equation 41 the Curie temperature Tc coincides with the actual transition temperature at which spontaneous polarization begins to rise if the transition is of the second order. For firstorder transitions, Tc is generally slightly lower than the actual transition temperature by several degrees (typically ~10 K). Because the difference is very small, and for general uses, Tc is usually considered the actual transition temperature. When the temperature decreases through Tc, the polarization rises from zero continuously over several degrees of temperature if the transition is of the second order. However, when the polarization rises abruptly from zero at Tc following the firstorder transition, then the rise involves a change of the latent heat, implying that the process is equivalent to supercooling. When the temperature is reversed—that is, increases through the transition point—the process becomes superheating, and a collective or cooperative action among the dipoles and surrounding ions tends to hold the spontaneous polarization until a slightly higher temperature is reached, as shown in Figure 49(c). A similar phenomenon occurs at any transition point if the transition is of the first order. (See Figures 411 and 412.) But this phenomenon does not occur if the transition is of the second order, as shown in Figure 49(d).
4.2.2 Phenomenological Properties and Mechanisms This section discusses the phenomenological behaviors and their mechanisms of six typical ferroelectric materials: • Barium titanate (BaTiO3)–type ferroelectrics • Potassium dihydrogen phosphate (abbreviated KDP, KH2PO4)–type ferroelectrics • Potassiumsodium tartrate tetrahydrate (Rochelle salt, KNaC4H4O6•4H2O)–type ferroelectrics • Triglycine sulphate (abbreviated TGS, (NH2CH2COOH)3H2SO4)–type ferroelectrics
221
• Alloys of lead, zirconium, and titanium oxide (abbreviated PZT, alloys of PbO, ZrO2, and TiO2)–type ferroelectrics • Polyvinylidene fluoride (abbreviated PVDF, –(CH2CF2)n–type ferroelectrics. BaTiO3Type Ferroelectrics BaTiO3 belongs to the family of ABO3 Perovskite mineral (CaTiO3) structures, in which A and B are metals. The total charge of the A and B positive ions must be +6, and A and B must be of quite different sizes; the smaller ion, with a larger charge, must be a transition metal. For BaTiO3, Ti is a 3d transition element and has the d orbital for electrons to form covalent bonds with its neighbors. The radius of Ti4+ ion is about 0.68 Å, and that of Ba2+ is about 1.35 Å. These ions form nice octahedral cages, with the O2 ions held apart. At temperatures higher than the Curie temperature (>120°C), Ti4+ stays in the cage, rattling around it to make the unit cell maintain a symmetrical cubic structure, as shown in Figure 410(a). However, the structure of the unit cell is temperature dependent. At a certain transition temperature, the particular structure of the unit cell becomes unstable and must transform to a more stable one. So, at the Curie temperature Tc, the octahedral cages distort and the positive ions move to offcenter positions. The crystal takes a tetragonal form, resulting from the stretching of the cubic unit cells along one edge, as shown in Figure 410(b). In fact, the Ba2+ ions shift 0.05 Å upward from their original position in the cubic structure; Ti4+ ions shift upward by 0.1 Å, and the O 2 ions downward by 0.04 Å to form the tetragonal structure. As a result of the ion shifts, the centroid of the positive charges no longer coincides with the centroid of the negative charges; therefore, the unit cells become permanently polarized and behave as permanent dipoles, leading to spontaneous polarization. The direction of the displacement can be reversed by a sufficiently high electric field of opposite polarity. This possibility of dipole reversal distinguishes ferroelectric materials from nonferroelectric ones. At temperatures
222
Dielectric Phenomena in Solids Ti4+ O2– Ba2+
Ti4+
O2–
Ba2+
Ti4+
O2–
Ti4+
O2– Ba2+
Ba
(a)
O
Ti4+
Ti
(b)
The unit cell of BaTiO3
PS
PS
PS
c
The ion displacements due to the cubictetragonal distortion in BaTiO3
a2
a1 Rhombohedral, Stable below –90°C
(c)
Orthorhombic, Stable between 5°C & –90°C
Ba2+
Tetragonal, Stable between 120°C & 5°C
a a
a
Cubic, Stable above 120°C
The temperature dependence of the structure of the unit cell
Figure 410 Schematic diagrams showing (a) the unit cell of BaTiO3, (b) the ion displacement due to the cubictetragonal distortion in BaTiO3, and (c) the temperature dependence of the structure of the unit cell.
below Tc and between 120°C and 5°C, the structure is tetragonal and the polar axis (i.e., the direction of the spontaneous polarization) is along the caxis of the unit cells, in which c > a. At about 5°C, the tetragonal unit cells undergo a transition for a higher stability to the orthorhombic structure, which is formed by stretching the cell along the facediagonal direction with the polar axis also along the same direction. This structure will remain stable for temperatures between 5°C and 90°C. Similarly, at around 90°C, a rhombohedral structure, formed by stretching the unit cell along the bodydiagonal direction, becomes preferred, as shown in Figure 410(c). The direction of spontaneous polarization is
always along the direction of the unit cell’s elongation, that is, the stretching direction. This is also referred to as the ferroelectric polar axis. BaTiO3type ferroelectrics are nonpiezoelectric in the unpolarized state. The cubic symmetry implies that, depending on the temperature, spontaneous polarization may occur along several axes. For example, there is a set of three (100) axes, a set of six (110) axes, and a set of four (111) axes. The three sets are nonequivalent.
Dielectric Constants
Dielectric constants are usually measured with small AC signals. At low frequencies,
Ferroelectrics, Piezoelectrics, and Pyroelectrics Rhombohedral
Orthorhombic
Tetragonal
Cubic
10,000
Dielectric Constant
piezoelectric deformation can follow the change of the applied electric field, and the crystal can be considered mechanically unconstrained. In this case, the dielectric constant measured is under the free crystal condition. However, at frequencies higher than the piezoelectric resonance frequency of the crystal, piezoelectric deformation cannot follow the change of the applied AC field due to inertia effects, and the dielectric constant measured is under the clamped crystal condition. In nonpiezoelectric crystals, such as BaTiO3 (which is nonpiezoelectric in the unpolarized state), the dielectric constant is practically independent of frequency at temperatures near or higher than Tc. But in piezoelectric crystals, such as KDP and Rochelle salt, the dielectric constant is strongly frequencydependent and may differ by several orders of magnitude, depending on the frequency used for the measurement. Obviously, the frequency dependence of er of BaTiO3 is expected to be different in the various phases. In the tetragonal phase, er, measured at low frequencies under the free crystal condition, is expected to be higher than that measured at frequencies higher than the piezoelectric resonance frequency under the clamped crystal condition. At still higher frequencies, an additional drop in er may occur, possibly due to dielectric relaxation. In general, the frequency range used for measurements of er is from zero to microwave frequencies in which the crystal can still be considered a free crystal. The dielectric constant–temperature (erT) characteristics for BaTiO3 under the free crystal condition are shown is shown in Figure 411. The data are from Merz.17,18 The special features of this erT relationship are discussed as follows. For temperatures above the Curie temperature Tc, the crystal assumes a cubic structure and is in the paraelectric unpolarized state. The dielectric constant decreases with increasing temperature, following closely the Curie–Weiss relation given by Equation 41. Xray analysis has indicated that the dipole moment is associated with the distortion of the molecular system and the cooperative alignment of the dipoles, resulting in spontaneous polarization. BaTiO3 is
223
8000 6000 aaxis 4000 2000 caxis 0 –200 –160 –120 –80 –40
0
40
80
120
Temperature (°C) Figure 411 Dielectric constant of BaTiO3 as a function of temperature measured along the caxis and along the aaxis (perpendicular to the caxis).
a multiaxial ferroelectric, and its basic molecular structure, as shown in Figure 410(a), is an octahedral arrangement of oxygen ions around a central Ti4+ ion. Above the Curie point, the Ti4+ ion is rattling around from its symmetrical position. Each shift will create a dipole moment along that shifting direction, but this ion can also shift in the opposite direction, due mainly to thermal agitation, which is randomized. However, when a small AC signal field is applied to the crystal along one axis for the measurement of er, the ions will be inclined to shift along the direction of the applied field, thus producing net dipole moments, provided that the driving force from the field is larger than the thermal agitation force. This can happen only at a temperature close to, but above, the Curie point. This shift obviously depends on the local field and the temperature the ions experience. The local field, derived on the basis of Lorentz’s internal field, is for nonpolar materials (see Internal Fields in Chapter 2). At T > Tc, however, BaTiO3 would become polar, due to the shifting of the ions under an applied field. This mechanism is different from atomic polarization in ionic crystals and also from the orientational polarization in dipolar materials in which permanent dipoles are present. So far, there is no satisfactory method available to calculate the local field and the average dipole moment in ferroelectric materials for T > Tc. By assuming that the ionic shifting in producing dipole moments is equivalent
Dielectric Phenomena in Solids
where mo is the dipole moment of the permanent dipole in the material and Flocal is the local field. Again, we borrow the formula for local field based on Lorentz’s internal field, which is given by Flocal =
er + 2 F 3
(43)
Since the polarization is given by P = (e r  1)e o F = N m F
(44)
where N is the number of molecules per unit volume, then from Equations 42 through 44 we obtain the famous Clausius–Mossotti equation: er  1 Nmo2 = e r + 2 9e o kT
(45)
Rearrangement of Equation 45 yields the dielectric susceptibility c = er  1 =
3 N ( mo )2 9e o k 3Td = er T  N ( mo )2 9e o k T  Td
(46) because er >> 1. This equation is similar to Equation 41. This indicates that er diverges as T approaches Tc, and that the system becomes unstable and must make a transition to a new phase. The divergence of er at T = Tc, based on Equation 46, is generally referred to as the Clausius–Mossotti or polarization catastrophe. It is important to note that Td = N(mo)2/9eok is definitely not Tc and cannot be used to evaluate Tc, nor can 3Td be used to estimate the Curie constant C for ferroelectric materials, simply because for T > Tc, there are no permanent dipoles as such in BaTiO3. It appears that research in the derivation of the Curie–Weiss equation based on the ionshifting mechanism (which is similar to ionic polarization but not quite the same and has a different form of local
30 Ps
25 20 15 10 5
–140 –120–100 –80 –60 –40 –20
0
2
Fc
1
20 40 60
80 100
Coercive field Fc (kV/cm)
(42)
Tetragonal
mo2 Flocal 3kT
Orthorhombic
mF =
field) could be very rewarding. A thermodynamic approach to this phenomenon will be discussed in Section 4.2.3. At Tc, the dielectric constant for BaTiO3 is typically of the order of 10,000, and the ions are moving into a difference phase, corresponding to spontaneous polarization. Consequently, an applied electric field will be able to produce relatively large shifts. This action results in a big change in dipole moment, corresponding to a high dielectric constant. When T is lowered just below Tc, the structure of the unit cell changes from the cubic form to a tetragonal one, as shown in Figure 410(b) and (c). Once the structure begins to change or spontaneous polarization to arise, the net dipole moment in the direction of the applied AC field, and hence the dielectric constant, will start to decrease, as shown in Figures 411 and 412. At T < Tc, the dielectric constant is strongly anisotropic in the ferroelectric phase for all crystals. For multiaxial ferroelectrics such as BaTiO3, the dielectric behavior, which is isotropic in the cubic nonpolarized phase, becomes strongly anisotropic in the polarized phase. The dielectric constant measured along the principal ferroelectric axis (caxis in the tetragonal structure) is lower than that normal to it (i.e., aaxes). This big difference can be observed only in singledomain crystals.17,18 This is readily understandable because the spontaneous polarization along the caxis is saturated, while the polarization along the aaxes is not. For uniaxial ferroelectrics, such as KDP
Rhombohedral
to the dipole orientation (although in fact, they are quite different), we can borrow Debye’s formula originally derived for dipolar materials. Then, the average dipole moment per molecule in the direction of the applied field can be written as
Spontaneous polarization Ps (mC/cm2)
224
Temperature (°C) Figure 412 Spontaneous polarization and coercive field of a BaTiO3 single crystal as functions of temperature measured along the tetragonal [001] direction (caxis).
Ferroelectrics, Piezoelectrics, and Pyroelectrics
and Rochelle salt, the dielectric constant measured along the principal ferroelectric axis is much larger than that normal to it, simply because the ions shift only along one principal ferroelectric axis and do not shift in any direction other than the principal axis. For example, for KDP, the dielectric constant along the principal axis is about 1100, while that normal to it is only 12. For Rochelle salt, the corresponding dielectric constants along and normal to the principal axis are 1000 and 10, respectively. In general, pure crystal specimens have a lower Tc than the impure ones. Also, the electrical conductivity of a material has a screening effect on the cooperative force that leads to the ferroelectric behavior. Other ferroelectric materials, which are similar to BaTiO3 in their chemical structure (PbTiO3, KNbO3, KTaO3, etc.), have similar dielectric and structural properties to those of BaTiO3, except that their Curie temperatures and Curie constants are different.
Spontaneous Polarization and Coercive Field
The temperature dependence of the spontaneous polarization Ps and the coercive field Fc for BaTiO3 single crystals is shown in Figure 412. The data are from Merz.17,18 The measurements were made along the caxis of the tetragonal structure, that is, along the (001) direction.18,21 The Ps value along the (110) facediagonal direction of the orthorhombic structure can be obtained by multiplying the corresponding value along the caxis by 2 . Similarly, the Ps value along the (111) bodydiagonal direction of the rhombohedral structure can be obtained by multiplying the corresponding value along the caxis by 3. The transition at Tc is of the first order for single, pure BaTiO3 crystals. However, if the crystals are not pure, the expected firstorder transition may become a secondorder transition, and the value of Ps would also be lowered, due to the hindering of the motion of domain walls by impurities or other defects. The coercive field Fc is temperature dependent, as shown in Figure 412. Fc depends also on the time required for the polarization to reverse its direction. According to Merz22 and
225
Landauer,23 the rate of the reversal of the polarization P can be expressed as dP = f ( P)exp[ a F(t )] dt
(47)
where the function f(P) is related to the switching rate. For most hysteresis loop measurements, the applied field varies sinusoidally with time (i.e., F(t) = Fosin wt), and a is a parameter depending on temperature. Equation 47 implies that the coercive field depends on the rise rate of the applied field. For slow rates, the crystal can have enough time to reverse its polarization so that the reversal can be completed before the peak field is reached. For fast rates, however, the crystal may not have sufficient time to complete the reversal process. In this case, a larger Fc is needed to bring Ps to zero. In other words, Fc is not a constant physical parameter; it depends on both the value of Fo and the frequency w of the applied field.24,25 The coercive field depends also on the thickness of the ferroelectric specimens. The thicker the specimen, the smaller the coercive field. The experimental results follow the thicknessdependence relation26 Fc = Fco + G d
(48)
where Fco is the coercive field for very thick specimens, d is the specimen thickness, and G is a constant. Based on the experimental results for BaTiO3, G turns out to be 2.2 V. Polarization reversal is a process of nucleation and growth of antiparallel domains, which is thickness dependent.22,27 The coercive field can be considered the field at which the reversal process can proceed easily. Before ending this section, it is worth mentioning that upon repeated switching of the polarization of the crystals, notably BaTiO3, spontaneous polarization becomes clamped or decreases, and the coercive field increases. This phenomenon is referred to as the fatigue or decay of the crystal,28,29 and it has been attributed to the buildup of the space charge near the crystal surfaces and the interaction of this space charge with domain walls. The degree of the fatigue depends on several factors including the ambient atmosphere, the elec
226
Dielectric Phenomena in Solids
trode material, and the waveform of the applied switching field. The decay is more rapid with pulsed fields than with lowfrequency AC fields.28–30 Ferroelectric ceramics exhibit also fatigue behavior. Apart from the factors previously mentioned, pores, impurities, and microcracking may also play important roles in this phenomenon. The displacement current observed during the reversal of spontaneous polarization is often accompanied by transient pulses. Such noiselike pulses were first observed in ferromagnetic materials by Barkhausen in 1919, and the analog of this phenomenon in ferroelectric materials still bears his name. The processes of domain nucleating or coalescing produce sharp discontinuities in the change of polarization. These are picked up from the electrode as Barkhausen pulses. This phenomenon has been studied by many investigators.31–33 In BaTiO3, there are typically 105 to 106 pulses during a complete polarization reversal, and the average pulse height is of the order of 1012 coulomb. The total number of pulses of all sizes does not vary with the applied field, but pulse heights increase with increasing field. Similar features of this phenomenon appear in other ferroelectric materials, including TGS, Rochelle salt, etc. Experiments have revealed that Barkhausen pulses are associated with the nucleation and growth of domains. However, this phenomenon provides an additional avenue for the study of polarization reversal processes under various conditions.
the intrinsic conductivity at room temperature is thousands of millions of times smaller than the real electrical conductivity of BaTiO3, which is of the order of 1014 (ohmcm)1 and of the ntype. So, the contribution from the intrinsic condition is negligible and the electronic conductivity must be extrinsic (see Electronic Conduction in Chapter 7). For this finite ntype electronic conductivity, we must find the source of the electrons. The mechanism of electrical conduction for BaTiO3 is similar to that for titanium oxide TiO2 (rutile) or other oxides, such as ZnO, etc. It is almost impossible to obtain stoichiometric BaTiO3. Crystal specimen fabrication processes are never perfect. There is always a possibility for the fourvalent Ti4+ ions to reduce to the threevalent Ti3+ or even to the twovalent Ti2+ ions. Each titanium atom can give four electrons to oxygen atoms, and each oxygen atom can take only two electrons. If the oxide is oxygendeficient (or metalrich), then not all the titanium atoms have shed four electrons. Some must be left in a lower valency state of Ta3+ or Ta2+ in order to maintain an overall neutrality of the system. This situation results in a few Ta3+ or Ta2+ in a sea of Ta4+, and a few of oxygen vacancies in the lattice of O2 ions. The Ta3+ or Ta2+ ions act like electron donors, ready to provide electrons for electronic conduction, while O2ions may also diffuse via the vacancies for ionic conduction. So, the electrical conductivity consists of electronic conductivity sn and ion conductivity si. Thus, s = s n + s i = qmn n + qmi ni
Electrical Conductivity and Breakdown Strength
In oxide crystals, bonds are formed by the complete transfer of the electrons from the metal atoms to the nonmetal atoms, such as oxygen atoms. Each atom then becomes an ion with an inert gas atomic structure. These ions are so stable that it is very difficult to remove electrons from them or create holes in them. This implies that their energy band gaps are large. The energy band gap for the Perovskite oxides, such as BaTiO3, is around 3 to 4 eV. Even assuming electron mobility of 100 cm2V1s1,
(49)
where un and n are, respectively, the mobility and the concentration of electrons; and ui and ni are, respectively, the mobility and the concentration of vacancies. The electrons on Ta3+ or Ta2+ ions may hop to Ta4+ ions, contributing to an extrinsic ntype conduction. For pure BaTiO3 single crystals, electronic conduction is dominant for temperatures up to 500°C, but ionic conduction becomes significant at about 100°C. It is interesting to note that the activation energy for electronic conduction in BaTiO3 is considerably smaller in the polarized state than in the
Ferroelectrics, Piezoelectrics, and Pyroelectrics
KH2PO4Type Ferroelectrics Potassium dihydrogen phosphate (KH2PO4) is generally referred to as KDP crystals, with a tetragonal structure at room temperature. Ferroelectrics of the KH2PO4 type exhibit a much simpler behavior than other ferroelectrics because they belong to the uniaxial ferroelectric family. These materials polarize along only one
axis (up or down along the caxis) and undergo only one phase transition from a paraelectric into a spontaneously polarized state. The transition does not show a thermal hysteresis, implying that the transition is of the second order. In the paraelectric unpolarized state, the crystal assumes a tetragonal structure at T above Tc, with the ferroelectric axis along the caxis. The crystal is piezoelectric because it belongs to the noncentrosymmetric point group. At T below Tc, an orthorhombic phase exists, which is ferroelectric with spontaneous polarization due mainly to the displacement of K, P, and O ions in the direction of the polar caxis.34 The structure of KDP is quite complicated. Basically, it consists of two interpenetrating bodycentered lattices of PO4 tetrahedra and two interpenetrating bodycentered K lattices, with the PO4 and K lattices separated along the caxis. Every PO4 is linked to four other PO4 groups by hydrogen bonds, which lie perpendicular to the caxis. This arrangement gives rise to an ionic configuration of K+(H2PO4). The distribution of proton density shifts from the center of the bond at T above Tc to a localized asymmetric position below Tc. The direction of this shift reverses when the spontaneous polarization is reversed.34,35 The dielectric constant–temperature characteristics are shown in Figure 413, the data being from Busch,36 and the spontaneous polarization–temperature characteristics in Figure 106 Dielectric Constant
paraelectric state, possibly due to the big difference in dielectric constant, polarization, and lattice parameters between these two states. It should be noted that there is also a possibility of the oxide being oxygenrich (or metaldeficient). In this case, Ta4+ can give four electrons to oxygen atoms, but not all oxygen atoms can have two electrons each; some oxygen atoms can get only one each and become O ions. The O ions act as acceptors, creating holes in the crystals. These holes can migrate from O to O2 (equivalent to electrons hopping from O2 to O). Cations may also diffuse via vacancies, but the activation energy for cation diffusion in oxide crystals is always high. Thus, the extrinsic ptype conduction is dominant. However, both electronic conduction (ntype or ptype) and ionic conduction occur s in BaTiO3; the ratio of n depends strongly si on the purity and the fabrication process of the material, as well as the temperature. The breakdown strength of BaTiO3 single crystals is of the order of 0.5 MV cm1. For BaTiO3 ceramics, it is about 0.1 MV cm1. Generally, ceramics have a lower breakdown strength, partly because of their porosity. It should be noted that a high poling field may sometimes cause electrical breakdown, because the poling time is usually quite long (e.g., one hour). High field stressing coupled with long stressing time may be sufficient to overcome the interdomain stresses in BaTiO3. If impurities, pores, and other defects are present in specimens, as in ceramics, the breakdown strength will be strongly dependent on specimen thickness, electrode area, and temperature. For more details about the breakdown processes, see Electrical Breakdown in Chapter 8.
227
105 104
caxis
103 102
aaxis
10 1 50
100
150 200 Temperature (°K)
250
300
Figure 413 Dielectric constants of KH2PO4 as a function of temperature measured along the caxis and along the aaxis.
228
Dielectric Phenomena in Solids
5 Ps (mC cm–2)
KNaC4H4O6•4H2O (Rochelle Salt)–Type Ferroelectrics Rochelle salt is a potassiumsodium tartratetetrahydrate (KNaC4H4O6•4H2O) and belongs to the family of uniaxial ferroelectrics. This was the first material in which Valasek discovered the ferroelectric phenomenon in 1921, and from which he also introduced the term Curie temperature or Curie point for ferroelectrics. It is interesting to describe briefly the ferroelectric properties of this material. Rochelle salt has a rather poor mechanical strength and low disintegration temperature; it is also apt to absorb water. The crystal decomposes at a low temperature of about 55°C. However, the most interesting property of Rochelle salt is that it exhibits two Curie points, one at +24°C, called the upper Curie temperature, and the other at 18°C, called the lower Curie temperature. The nonpolar paraelectric phases for T > +24°C and for T < 18°C are orthorhombic. The polar ferroelectric phase, occurring at the temperature range between 18°C and +24°C, is monoclinic. The dielectric constant, measured along the aaxis with a small signal field of 1 kHz as a function of temperature, is shown in Figure 415. There is no thermal hysteresis at the transition points, indicating that the transition is of the second order. For temperatures from +24°C
104
103 er
414, the data being from Von Arx and Bantle.37 The Curie temperature Tc is +150°C (123 K). At T > Tc, the dielectric constant decreases with temperature, following closely the Curie–Weiss law with the Curie constant C being 3250°C.36,37 At T < Tc , the dielectric constant along the caxis drops sharply (but not abruptly) due to the dielectric saturation effect, which results in a decrease of dielectric constant with increasing spontaneous polarization. The dielectric constant along the aaxes also shows an anomaly at Tc, possibly due to the effect of dielectric cooperative action among the ions.38 The dielectric constant along the caxis is dependent on the applied DC biasing field. The bias tends to lower the dielectric constant and also to shift the peak of the dielectric constant toward higher temperatures.39 Figure 414 shows that the spontaneous polarization begins to rise at Curie point continuously, so the transition is of the second order. The coercive field Fc is temperature dependent. It is interesting to note that at a temperature of about 213°C, (60 K) there is a sharp break. At 120 K > T > 60 K, Fc is practically independent of temperature. But at T < 60 K, Fc increases rapidly with decreasing temperature.40 This phenomenon is probably caused by the hindered motion of domain walls at low temperatures. There are a number of crystals isomorphous with KH2PO4 that have a similar dielectric behavior, including KH2AsO4, RbH2PO4, CsH2PO4, etc. In this KDP family, hydrogen bonds play a vital role in the ferroelectric behavior.
102
4 3
10
2 1 0
100
105 110 115 Temperature (°K)
120
125
Figure 414 Spontaneous polarization of KH2PO4 as a function of temperature.
–200
–160
–120
–80
–40
0
40
Temperature (°C) Figure 415 Dielectric constant of Rochelle salt as a function of temperature.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
to about +50°C, the dielectric constant obeys the Curie–Weiss law, with the Curie constant C 2240°C. For the temperature range from 18°C to 28°C, the dielectric constant again follows the Curie–Weiss law, with a Curie constant of 1180°C. The decrease of the dielectric constant in the ferroelectric region is due to the effect of spontaneous polarization saturation, similar to BaTiO3 and KH2PO4. The temperature dependence of spontaneous polarization is shown in Figure 416. The coercive field for Rochelle salt depends on the specimen thickness and the magnitude and the frequency of the applied field, similarly to other ferroelectric materials. The data given in Figures 415 and 416 are from Hablutzel.41 Rochelle salt is like KDP; the hydrogen bond plays an important role in the ferroelectric behavior. This idea has led to the study of a deuterated Rochelle salt, prepared by dissolving ordinary Rochelle salt in highly concentrated D2O to make it thoroughly desiccated at higher temperatures, in order to replace hydrogen with deuterium, the isotope of hydrogen (heavy hydrogen consisting of a neutron and a proton in the nucleus). After this process, the Rochelle salt becomes a deuterated compound with a chemical formula of KNaC4H2D2O6. 4D2O. This compound has the Curie points at 22°C and +35°C, thus widening the region of
5
3
the stable ferroelectric phase and giving a higher spontaneous polarization, as shown in Figure 416.41,42 (NH2CH2COOH)3•H2SO4 Type Ferroelectrics Triglycine sulphate (TGS) is a uniaxial ferroelectric material, and its chemical formula is (NH2CH2COOH)3•H2SO4. This material exhibits ferroelectric properties at room temperature. The Curie temperature is 49°C. At T > Tc, the crystal structure is centrosymmetric and in the nonpolar paraelectric state with a monoclinic symmetry. At T < Tc, the crystal becomes polar and belongs to the polar group of the monoclinic system.39 Ferroelectric direction is along the baxis and the transition is of the second order. The dielectric constant–temperature characteristics measured at 1 kHz and 1 V cm1 are shown in Figure 417. The dielectric constant along the polar baxis shows a prominent anomaly in the vicinity of Tc. The dielectric constants along the a and caxes are practically independent of temperature, simply because this is a uniaxial polarized material. For T > Tc, er follows the Curie–Weiss law with a Curie constant C of 3200°C. The temperature dependence of the spontaneous polarization is shown in Figure 418. The experimental data are from Hoshino et al.43 Some crystals are isomorphous with TGS, such as triglycine selenate (NH2CH2COOH). H2SeO4
Deuterated
5 ¥ 103
Pure
103 5 ¥ 102
Dielectric Constant
Ps (10–7 C cm–2)
4
2
1
baxis
102 5 ¥ 10
aaxis caxis
10 5
0 –30
–160 –120
–20
–10 0 10 20 Temperature (°C)
30
40
Figure 416 Spontaneous polarization of Rochelle salt and deuterated Rochelle salt.
229
–80
–40
0
40
80
Temperature (°C) Figure 417 Dielectric constant of triglycine sulfate as a function of temperature measured along aaxis, baxis, and caxis.
230
Dielectric Phenomena in Solids 4.5
is shown in Figure 419.44 The Curie temperature Tc depends on the composition of the system. In this phase diagram, there are six major phase boundaries:
Triglycine Fluoberyllate Triglycine Sulfate Triglycine Selenate
4.0 3.5
Ps (mC cm–2)
3.0
1.
The cubic paraelectric–tetragonal ferroelectric (P–FT) phase boundary
2.
The cubic paraelectric–rhombohedral ferroelectric (HT ) (P–FR(HT)) phase boundary The tetragonal ferroelectric–rhombohedral ferroelectric (HT ) (FT – FR(HT)) phase boundary The rhombohedral ferroelectric (HT )– rhombohedral ferroelectric (LT ) (FR(HT)– FR(LT)) phase boundary The rhombohedral ferroelectric (HT )– orthorhombic antiferroelectric (FR(HT)–AFo) phase boundary The rhombohedral ferroelectric (LT )– orthorhombic antiferroelectric (FR(LT)–AFo) phase boundary
2.5 2.0 1.5
3.
1.0 0.5 0
4. 0
20
40 60 Temperature (°C)
80
5. Figure 418 Spontaneous polarization of triglycine sulfate, triglycine selenate, and triglycine flueboryllate as a function of temperature.
(abbreviated TGSe) and triglycine fluoberyllate (NH2CH2COOH)3H2BeF4 abbreviated TGFB), have similar properties to TGS with different Curie temperatures, as shown in Figure 418. Alloys of PbO, ZrO2, and TiO2 (PZT alloys)Type Ferroelectric Ceramics PZT alloys belong to the family of ceramics, which are alloys of lead oxide, zirconium oxide, and titanium oxide (PbO, ZrO2, and TiO2). The familiar Perovskite structure of BaTiO3 also appears in PZT alloys because there are equal numbers of divalent (Pb2+) and tetravalent (Zr4+ and Ti4+) cations. PZT alloys are in fact the alloys of two components: PbZrO3 and PbTiO3. This is why PZT alloys are similar to BaTiO3 in their ferroelectric properties. Thus, by controlling the composition and microstructure of the PZT alloys, it is possible to tailor their properties to suit particular applications. The general chemical formula is PbZr1xTixO3, with x as a fraction from 0 to 1. The phase diagram of ferroelectric ceramics is normally plotted in phase transition temperature as a function of the composition. A typical equilibrium phase diagram for the PZT system
6.
The phase is cubic paraelectric, implying that an applied field can distort the system and change it from unpolarized to a polarized state, but as soon as the field is removed, the system will quickly relax back to its original unpolarized state due to thermal agitation. Figure 419 has some prominent features worth mentioning. • The Curie temperature Tc for all compositions is higher than that for BaTiO3. The main reason is that the Pb2+ ion has two outer electrons beyond its last full shell, but the Ba2+ ion does not. These outer electrons can contribute to covalent bonding with neighboring oxygen ions. With this extra bonding, a greater thermal energy or a higher temperature is required to convert the polarized state into an unpolarized state. This results in a higher Tc for the PZT system. • The morphological boundary between the tetragonal and the rhombohedral phases occurs at x around 0.5. Since the PZT system is used mostly in piezoelectric devices, the PZT system with the composition near the morphological boundary has an advantageous crystal morphology. The efficiency
Ferroelectrics, Piezoelectrics, and Pyroelectrics
231
PbZrO3 Percentage of PbZrO3 in PbZrO3PbTiO3 System 100 500
90
230
Temperature (°C)
400 350
50
1
2
3
4
rie
Cu
AFT
FR(HT)
PS
Rhombohedral, Stable
AFO
re F
Cubic, Stable
100 50
20
10
0
s
ocu
AFO
190 0
200
30
PC
300 250
40
FR(HT)
210
150 PS
60
AFT
220
200
70
FR(LT)
tu era
p
Tem
ary ical Bound Morpholog
450
80
PC
PS Tetragonal, Stable
FT
Orthorhombic, Stable
0 10 20 30 40 50 60 70 80 90 100 Percentage of PbTiO3 in PbZrO3PbTiO3 System PbTiO3 Figure 419 The equilibrium phase diagram of the PZT system and microstructure of the unit cell for different phases.
of the conversion between electrical and mechanical energy depends strongly on crystal morphology. The piezoelectric coupling coefficient climbs to a maximum value at x around 0.5 because the shear transformation between the two types of structures is much easier. This is because there are six easy directions of polarization for the tetragonal unit cell and eight easy directions of polarization for the rhombohedral unit cell, which provide much easier mutual conformation. • For most PZT alloys, the rich Zr region with x below 0.1 is attractive because they have superior properties. In this region, the Curie temperature Tc is lower. At T < 200°C, there exists a boundary between the ferroelectric phase and the antiferroelectric phase. • The rhombohedral ferroelectric phase is subdivided into high temperature FR(HT) and low temperature FR(LT) phases. Simple rhombohedral unit cells appear in both hightemperature and lowtemperature regions. The basic difference between FR(HT) and FR(LT) is possibly due to the difference in the directions of the spontaneous polarization.45,46
• The Curie temperature in pure PbZrO3 is 230°C. Below this temperature, the crystal is in an antiferroelectric state, with the structure changing to orthorhombic one. But at or near the Curie temperature, the antiferroelectric phase assumes a tetragonal structure. The mechanism that causes this difference in structure at or near Tc is not certain; possibly it is due to the presence of foreign impurities.47 It is interesting to review the ferroelectric properties of lead zirconate PbZrO3 in the PZT system with x = 0. The dielectric constanttemperature relation for PbZrO3 ceramic is shown in Figure 420. The dielectric constant reaches a peak at the Curie temperature 230°C. Above Tc, the structure is cubic and er follows the Curie–Weiss law, with the Curie constant C equal to 1.6 ¥ 105 degrees. The results are from Roberts.48 Although the dielectric anomaly is similar to that in BaTiO3, no hysteresis loop has been observed for T < Tc, implying that there is no net spontaneous polarization. This indicates that the phase for T < Tc is antiferroelectric.49 In other words, all adjacent domains are oppositely polarized, so there is electrical ordering
232
Dielectric Phenomena in Solids 60
Fcrit (kv cm–1)
Dielectric Constant
3000
2000
40 P 20 F Fcrit 0 200
1000
0 0
100 200 Temperature (°C)
300
210 220 Temperature (°C)
230
Figure 421 The critical electric field Fcrit required to induce ferroelectricity in PbZrO3 as a function of temperature. Insert: the occurrence of a double hysteresis loop at the critical field.
Figure 420 Dielectric constant of ceramic PbZrO3 as a function of temperature.
but no net polarization (see Sections 4.2.3 and 4.2.5). However, in the vicinity of the transition temperature, a strong electric field can induce a ferroelectric phase. This means that the field can shift the phase boundary between AFo and FR, with the tendency of extending the ferroelectric region. A double hysteresis loop for pure PbZrO3 has been observed at temperatures below Tc.50 The ferroelectricity is induced in the antiferroelectric phase when the applied electric field reaches a critical value. A similar double hysteresis loop occurs in BaTiO3, but in that case the ferroelectricity is induced in the cubic paraelectric unpolarized region by a sufficiently high electric field and at a temperature slightly above Tc. Obviously, the origins of this doubleloop behavior for these two cases are different. In PbZrO3, the ferroelectric phase induced by the field has rhombohedral symmetry. The critical field is temperature dependent, as shown in Figure 421. The data are from Sawaguchi and Kittaka.50 It is difficult, if not impossible, to produce a PZT alloy PbZr1xTixO3 with 0 < x < 1 in single crystal form. The PZT alloys are ceramics, which are a solid solution. Generally, the three oxides—PbO, ZrO2, and TiO2—of selected purity and proportion, are ballmilled together
to produce a powdered mixture of very fine particle size. The chemical substance is then formed by calcining (fiercely heating) this mixture. This material is then ground up and artifacts made by compacting and sintering. Ceramics are quite different from single crystals. Ceramics are formed by many randomly arranged crystallites (grains) with unavoidable microvoids and impurities trapped in between. In fact, they are imperfect polycrystalline materials. So a polycrystalline ceramic that has not been subjected to static field stressing would behave like a nonpolar material, even though the crystallites composing it are polar. However, ferroelectric ceramics can be transformed into polar materials by an externally applied static electric field. This process is referred to as the poling process, which is reversible. To pole a specimen, the specimen must be brought to the saturation of the spontaneous polarization by a strong field and then allowed to relax back to the remanent condition. Poling is usually carried out at temperatures as hot as the Curie threshold temperature allows, and this poling condition is held for some hours. However, the Curie temperature is much lower than the ceramic sintering temperature, at which decent rates of transport between grains can occur, so it is inevitable that poled ceramics always carry some residual internal stress. A poled ceramic can be depoled
Ferroelectrics, Piezoelectrics, and Pyroelectrics
by the application of electric fields or mechanical stresses. A ceramic system consists of randomly originated grains (crystallites) intimately bonded together with grain sizes generally ranging from 1 mm to 20 mm. There are always pores (microvoids) and foreign impurities unavoidably present in the material during the fabrication process. It is obvious that both porosity and grain size affect dielectric and ferroelectric properties. The important factor leading to the effect is the variation in the dimensions of the grains and hence in the internal stresses during the change of temperature through the Curie point. The random directions of the crystallographic axes of the crystallites limit the extent to which spontaneous polarization can be developed. Due to the inhibition of the motion of domain walls by internal strains and other defects (such as impurities), the saturation value of the spontaneous polarization of BaTiO3 in ceramic structure is about half of the value for BaTiO3 single crystals. The hysteresis loop of BaTiO3 single crystals with a single domain is a square loop, like the one shown in Figure 45(a), having a spontaneous polarization Ps of about 26 mC cm2 and a coercive field Fc of about 1 kV cm1. The hysteresis loop for BaTiO3 ceramics is like a round loop, like the one shown in Figure 45(b), having Ps of about 7 mC cm2 and Fc of about 4 kV cm1. Of course, the latter figures depend to a great extent on the preparation of the ceramic specimens. One unusual feature of ferroelectrics is the aging phenomenon. A real crystal is never an ideal dielectric. It always contains imperfections, including vacancies, dislocations, impurities, etc., which disturb the uniformity of the polarization and depolarization. A ceramic material contains even more imperfections. The properties of ceramics change with time, even in the absence of external electric fields, mechanical stresses, or temperature changes. This aging phenomenon is associated with the continuous changing of the internal structure, which with time tends to reach a more stable arrangement—in other words, to lower the internal free energy. In fact, any poled ferroelectric ceramic is in a state of incessant depo
233
larization with time. However, the magnitude of the poling field and the poling temperature are important factors in determining the extent of the dipole alignment and hence the resulting ferroelectric properties. In actuality, the alignment is never complete. Depending on the type of the crystal structure and the poling condition, the thoroughness of poling can be quite high, approaching 83% (for the tetragonal structure) and 91% (for the orthorhombic structure) of that for single crystals.51 The aging process may be accelerated by exposing the poled ceramics to • Strong depoling fields • High mechanical stresses • Temperatures close to the Curie point A common rule of thumb to reduce the rate of depolarization (aging) is that the poled ferroelectric materials should not be exposed to temperatures higher than one half of the Curie temperature, since heat is the major factor that causes depolarization. However, aging is a complicated process that may be caused by several different mechanisms, such as • Gradual equilibration of domains toward the minimization of elastic and dielectric free energy • Segregation of impurities and vacancies on domain walls and grain boundaries • Ordering of impurities and vacancies inside the ferroelectric domains with respect to the polar axis52 Note that PZT ceramics are usually used with a dopant, modifier, or other composition in solid solution in order to improve or modify the properties of the basic PZT system for specific applications. A detailed discussion of many different compositional systems is beyond the scope of this chapter. However, a few significant examples will demonstrate the importance of additives in extending the variety of the applications of the PZT system. For the case of oxygenrich PZT, the conduction is mainly ptype extrinsic due to the holes produced by O ions. To reduce the ptype conduction, we can use donor dopants, such as
234
Dielectric Phenomena in Solids
Nb5+ or La3+, replacing Pb2+ in order to provide electrons required to convert O ions to O2, thus reducing the conductivity. It is important to reduce the conductivity because high conductivity makes it difficult to apply a high field for poling for a long period of time. The additives are usually compensated by Asite vacancies. (The Perovskite structure is expressed in the general formula ABO3. For BaTiO3, the vacancies created by missing Ba2+ are referred to as the Asite vacancies. Similarly, the vacancies created by missing Ti4+ are Bsite vacancies.) In this case, these additives will enhance domain reorientation and hence increase spontaneous polarization, dielectric constant, and piezoelectric constant; they will also lower the coercity and reduce the aging effect.53 One important compositional system, generally referred to as the PLZT system, is the PZT system modified by the lanthanum. This system can be formed by the complete miscibility of PbO, ZrO2, TiO2, and La2O3 in a solid solution; the amount of La can be adjusted on the basis of the general chemical formula Pb1yLay (Zr1xTix)1y/4O3 with the fraction y ranging from 0 to 1. Usually, the PLZT system is formulated so that La3+ ions replace mainly the Asite vacancies created by missing Pb2+ ions. In this case, the chemical formula can be expressed as Pb13y/2Lay(Zr1xTix)O3. Selected compositions within this system offer high electromechanical coupling coefficients for piezoelectric transducers.54–56 The PLZT system has also excellent electrooptic properties.57,59 Depending on its composition, the PLZT system exhibits one of three major types of electrooptic characteristics: memory, linear, or quadratic. Each of these three types can be used for different electrooptic devices.60 Another example is the Nb5+doped PZT system. It is well known that for the Pb(Zr1xTix)O3 system, a Zrrich system (i.e., small x)—for example with x = 0.05—exhibits an extensive phase boundary between the ferroelectric Fr and the antiferroelectric AFo phases, as shown in Figure 419. However, for x < 0.05, it becomes difficult to sinter to obtain a highdensity ceramic, compared to common PZT with higher x values. It is found that Nb5+
dopants can improve this situation.61,62 For the PbZr0.975Ti0.025O3 system doped with 1 wt% Nb2O5, the phase boundary at x = 0.025 occurs at room temperature. In general, the external electric field tends to broaden the region of the ferroelectric state, and the mechanical compression extends the antiferroelectric region. Thus, the AF–F boundary can be made to shift either by an applied field or by a mechanical compression. This implies that the stored energy due to spontaneous polarization in the ferroelectric phase can be released by a shock compression wave to convert the ferroelectric phase to an antiferroelectric phase. This principle can be applied for the generation of highenergy electric pulses.63 PVDF [(C H2  C F2)n]Type Ferroelectric Polymers The chemical formula for polyvinylidene fluoride (PVDF) is (CH2CF2)n. PVDF crystallizes from the melt below 150°C into spherulitic structures.64,65 In the melt, the polymer chains have randomly coiled shapes. Configurational defects can crystallize into regular conformations when cooled from the melt. This is accomplished by the torsional bond arrangements, in order to minimize the potential energy of the chains. The favorable arrangements are those having substituents at 180° between each other (called transor t) or having substituents at ±60° (called gauche± or g±), the actual torsional angles commonly deviating from these values. There are three known conformations of PVDF: alltrans, tg+tg, and tttg+tttg. The first two are by far the most common and most important ones,65–67 and they are illustrated schematically in Figure 422. In the alltrans conformation, all dipoles are aligned in the same direction normal to the chain axis. This yields the most highly polar conformation. The tg+tg conformation is also polar but has components of the dipole moments parallel and perpendicular to the chain axis. Depending on the temperature and the condition at which the material crystallizes, for most common polymorph PVDF produced by
Ferroelectrics, Piezoelectrics, and Pyroelectrics
235
H H
F F
F
H
t
F F
H H
H g+
F
H H H
t
H
F F
g–
F F H H
H g+
F
H
F
t
F
H
F
H H
g–
F
H g+
H H
H H
t
F F
F
(a) Alltrans
H
t
F F
F
F
H
t
F F
(b) tg+tg–
Figure 422 Schematic illustration of the two most common crystalline chain conformations in PVDF (a) alltrans conformation and (b) tg+tg conformation. The arrows indicate the projection of the CF2 dipole directions on planes defined by the carbon backbone.
melt–solidification, the unit cell consists of two chains in the tg+tg configuration and possesses dipole moments with components parallel and normal to the chain axis. So, the dipole moments of the two chains in the unit cell are antiparallel and the crystal does not exhibit spontaneous polarization. In this case, the unpolar phase of PVDF is referred to as the aphase. However, if the PVDF crystallizes at a temperature below 130°C and at a high pressure68 or in conjunction with a special epitaxial technique,69 the morphology of PVDF is changed to a structure oriented to the caxis, and the unit cell consists of two alltrans chains packed with their dipoles pointing in the same direction. This crystal structure renders PVDF the most highly polar phase, which is generally referred to as the bphase. The chains take on a planar zigzag (tttt) conformation. The chain
has a large dipole moment (uo = 7.06 ¥ 1030 Cm per monomeric unit).65 The degree of crystallinity for both aphase and bphase PVDF is approximately 50%. In the asdrawn bPVDF film specimens, the dipole moment is preferentially oriented along the stretched ± y direction in the film plane, since mechanical stretching (drawing) causes a breakdown of the original spherulite structure into an array of crystallites whose molecules are oriented in the direction of the stretching force. If electrodes are then deposited on the film surfaces and a strong poling field of about 0.5 MV cm1 is applied across the film specimen, the dipoles will reorient to align predominantly along the poling field in z direction perpendicular to the film plane. Ferroelectricity of PVDC has been established on the basis of the measured dielectric
236
Dielectric Phenomena in Solids
er
13
(a)
11 9 7
P (mC cm–2)
10
Pr
(b)
Fc 0
–10
–2
–1
0
Electric Field (MV
1
2
cm–1)
Figure 423 The variation of (a) dielectric constant and (b) polarization of bphase PVDF films with applied electric field. Initial poling, subsequent poling cycles.
constant of CF2 and the corresponding polarization as functions of temperature, as shown in Figure 423. The experimental data are from Takahashi, Date, and Fukada.70 A hysteresislike behavior of PVDF is good evidence that PVDF is a ferroelectric material. The Curie transition involves mainly intramolecular changes of polar orientation through the introduction of g± bonds that alter the polar alltrans conformation to a somewhat tg± and tt arrangement. As a result of this change, the Curie temperature for PVDF for the transition from the ferroelectric phase to a paraelectric phase would be around 205°C—about 20°C above its melting point.71 Although PVDF is ferroelectric, its dielectric constant is relatively small, around 10 to 15. But it exhibits strong piezoelectric and pyroelectric effects compared to other polymers, as first discovered by Kawai15 and Bergman et al.72
This material has been widely used for piezoelectric transducers and pyroelectric devices. 4.2.3 Thermodynamic Theory Classical thermodynamics deals mainly with the macroscopic behavior of materials. There are laws of thermodynamics that define the relationships between properties. To gain an understanding of the phase transitions and related effects, we need to understand the concept of free energy. One of the well known thermodynamic functions is the Helmholtz freeenergy function A, which is given by A = U  TS
(410)
where U is the internal energy, S is the entropy, and T is the temperature. There is also another wellknown function, called the Gibbs freeenergy function, which is given by
Ferroelectrics, Piezoelectrics, and Pyroelectrics
G = U  TS + pV
(411)
including a pV term. Most experiments in solids are performed at atmospheric pressure or pressures not far from it, which is so small that it makes the pV term negligibly small compared to other terms. Thus, by ignoring the pV term, the Gibbs function becomes Go = U  TS = A
(412)
The basic principle is the concept of the minimum free energy for the most stable system. If a system is allowed to have several alternative states, it will choose the one with the lowest free energy. To clarify the meaning of this principle, we apply it to a simple phenomenon. Based on Equation 412, a system can have the free energy at a lowest possible value if the internal energy U can be made as small as possible and the entropy S as large as possible. The internal energy U in a solid is primarily the potential energy, which is usually a negative quantity, implying that for a minimum potential energy all atoms (or ions) must rest at their lattice sites, that is, each atom (or ion) is resting at the bottom of its potential well. But this is a well ordered arrangement with very low entropy. Such an arrangement does not lead to a minimum free energy. Not all atoms (or ions) are at the bottom of the potential wells due to the thermal agitation, so the degree of order varies accordingly. At a given temperature T, the value of U and the degree of order S always tend to balance each other in order to reach a stable equilibrium state in which the free energy is the lowest. This is also why all atoms (or ions) in a solid are oscillating (vibrating) around their lattice sites. Statistically, entropy is a measure of disorder. The higher the disorder (or the lower the degree of order), the larger is the entropy. Based on thermodynamics, the entropy can be defined as dS = dQ T = Cp dT T
(413)
where dQ is the amount of heat absorbed by the system in a reversible process, and Cp is the specific heat at constant pressure. Based on
237
statistical mechanics, the entropy of a system is defined as S = k log q
(414)
where q is the number of microstates of the system. Disorder can be interpreted as the number of ways in which the particles inside a system can be arranged microscopically, so each different way can be considered a microstate or a thermodynamic state. Suppose that an alloy consists of two components: A and B. The total number of these two components is N per unit volume, of which n are of A type and the remaining Nn are of B type. Since the A components can be interchanged themselves in n! different ways and the B components in (N  n)! different ways, the number of different arrangements for N components (i.e., the number of microstates in the system) is q=
N! n!( N  n)!
(415)
Heat is one form of energy and energy cannot be created, it can only be converted from one form into other, different forms. The first law of thermodynamics states that the increase in internal energy dU is equal to the sum of the heat put in the system dQ and the work put in the system. When a solid body is subjected to an external electric field and mechanical stress, the internal energy will change accordingly. We can write dU = TdS + Xdh + FdP
(416)
where X and h are, respectively, the mechanical stress and the strain; and F and P are, respectively, the electric field and the polarization. F and P are vectors, and they have three components in x, y, and z directions. X and h are also vectors and have six components in x, y, and z, as well as shear directions on the plane normal to each of x, y and z, so the energy state of a crystal is specified by the values of nine variables plus the temperature. Thermodynamics can be used to describe the macroscopic behavior of the ferroelectric system by including external work done on the system. If the work put in the system is due to external mechanical stresses and electric fields, then the Gibbs function can be written as
238
Dielectric Phenomena in Solids
G = Go + Â Xi hi + Â Fj Pj i
(417)
j
The independent variables in the measurements of normal ferroelectric properties are the temperature T, the mechanical stress X, and the polarization P. Thus, it is convenient to discuss the G function as G (T, X, P). In the absence of mechanical stresses, X = 0 and at a constant T, Gibbs function can be simplified to G(T , P) = Go (T ) + Â j
Pj2 2e rje o
Ferroelectric Transition It should be noted that in Equation 418 both erj and Pj are temperature dependent and their behavior is anomalous and nonlinear near the transition point. Therefore, the behavior of the ferroelectric system can best be studied by expanding the energy in powers of the polarization. The Gibbs function for Perovskitetype ferroelectrics, formulated on the basis of the form of a power series by Devonshire73 and further developed by Huibregtse and Young,74 is given by
1 4 1 + 2 1 + 6 1 + 2 +
1 f2 ( Px2 + Py2 + Pz2 ) 2
f4 ( Px4 + Py4 + Pz4 ) f12 ( Py2 Pz2 + Pz2 Px2 + Px2 Py2 ) f111( Px6 + Py6 + Pz6 )
(420) where g2, g4, g6, etc., are new temperaturedependent coefficients. For the isothermal case, the electric field acting on the ferroelectric material, expressed in terms of P, can be obtained by F=
1 f123 Px2 Py2 Pz2 + . . . 6
g2 = b(T  Tc )
(421)
(422)
where b is taken as a positive constant and Tc may be equal to or close to the Curie transition temperature. The nature of the transition depends on the signs of the coefficients: g2, g4, g6, etc. The simplest case is that all coefficients, except g2, are positive, and P is continuous at the transition point, implying that the transition is of the second order. To find the values of P for which G is at the lowest value (minimum free energy), we differentiate Equation 420 with respect to P and set it equal to zero, that is, the values of P at F = 0. g 2 P + g 4 P 3 + g6 P 5 = 0
(423)
For simplicity, we ignore terms with the powers of P equal to and higher than 5. Then we have the values of P for the lowest G value as P=0
(419) where f2, f4, f12, f111, f112, f123, etc., are temperaturedependent coefficients. The series
dG = g2 P + g4 P3 + g6 P 5 . . . dP
At and near the Curie point, g2 can be approximated with a linear function of temperature.73 Thus, g2 may be written as
f112 [ Px2 ( Py2 + Pz4 ) + Py2 ( Pz4 + Px4 ) + Pz2 ( Px4 + Py4 )]
+
1 1 1 G(T , P) = Go (T ) + g2 P 2 + g4 P 4 + g6 P 6 2 4 6
(418)
where Go(T) is the Gibbs function under the unstressed and unpolarized conditions. The thermodynamic approach can be used to explain many ferroelectric properties. The following sections offer two transition processes as examples.
G(T , P) = Go (T ) +
does not contain terms of odd powers of P because crystals such as BaTiO3 in the unpolarized phase have a center of inversion symmetry. Supposing that the applied poling field is in the z direction (caxis of the cubictetragonal structure), then the polarization is also along the same z direction. By setting Py = PX = 0 and letting Pz = P for simplicity, Equation 419 can be simplified to
and P = ±( g2 g4 )1 2
(424)
Ferroelectrics, Piezoelectrics, and Pyroelectrics
The plot of G  Go as a function of P for three cases—g2 > 0, g2 = 0 and g2 < 0—is shown in Figure 424(b). It can be seen that for g2 = 0 (i.e., when T = Tc), P changes gradually from zero at T = Tc to a finite value at T < Tc. The transition in BaTiO3 is of the first order, but the energy of the Ti4+ ions in terms of their positions along the caxis takes the form of two potential wells. An applied electric field in the
239
direction opposite to the polarization may enable the Ti4+ ions to pass over the potential barrier between the two wells and reverse the direction of the polarity. If some coefficients other than g2 are negative, the situation becomes more complicated. For simplicity, assume that only g4 is negative and ignore all terms with powers of P higher than 6, then Equation 420 can be simplified to
G – Go
P
g2 > 0
0
P
g2
g2 = 0 g2 < 0
(a) FirstOrder Transition
G – Go
g2 > 0
P
g2 = 0 g2 < 0
0 g2
P
(b) SecondOrder Transition Figure 424 G–Go as a function of polarization at transition temperature and at temperatures just above and just below TC for (a) firstorder transition and (b) secondorder transition.
240
Dielectric Phenomena in Solids
G = Go +
1 1 1 g2 P 2  g4 P 4 + g6 P 6 2 4 6
(425)
For the minimum values of G, we have dG = g2 P  g4 P3 + g6 P 5 = 0 dP
dition that the free energy of the polar and the nonpolar phases are equal. This leads to 1 1 1 b(T1  Tc ) P 2  g4 P 4 + g6 P 6 = 0 (431) 2 4 6
(426)
The solution of Equation 426 yields
At the same time, the applied field is set equal to zero. This gives F=
P=0
dG = (T1  Tc ) P  g4 P3 + g6 P 5 = 0 dP
(432)
and 12
12 ¸ Ï 1 P = ±Ì g4 ± ( g4 2  4 g6 g2 ) ]˝ [ g 2 Ó 6 ˛
(427)
Figure 424(a) shows the value of G  Go as a function of P for g2 > 0, g2 = 0 and g2 < 0. For g2 = 0 (i.e., T = Tc), we have P = ±( g4 g6 )1/2. This implies that P changes discontinuously from P = ( g4 g6 )1/2 or P = +( g4 g6 )1/2 to P = 0 abruptly at T = Tc, and that the transition is of the first order. If the poling field is not high, we can use firstorder approximation by ignoring all terms with the powers of P higher than 2 in either Equation 420 or Equation 425. Then we have F=
dG = g2 P = b(T  Tc ) P dP
(428)
and P for T > Tc can be expressed as P = (e r  1)e o F = ce o F
(429)
Thus, from Equations 428 and 429, we obtain the Curie–Weiss relation c=
1 C = be o (T  Tc ) T  Tc
(430)
where C = (beo)1. This equation is similar to Equation 41. This thermodynamic approach can also be used to explain many ferroelectric phenomena related to the firstorder transition. Some of the common phenomena follow. The Difference between the Curie Temperature and the Actual Transition Temperature
The actual transition temperature T1 and the corresponding value of the spontaneous polarization can be calculated by imposing the con
From Equations 431 and 432, we obtain 12
È 3 Ê g4 ˆ ˘ P = ±Í Î 4 Ë g6 ¯ ˙˚ T1  Tc =
3 È g4 2 ˘ 16 ÍÎ bg6 ˙˚
(433) (434)
This indicates that the Curie temperature is lower than the actual transition temperature by 3 [ g4 2 bg6 ]. For BaTiO3, T1  Tc = 7.7°C.30 16 Thermal Hysteresis
On heating the crystal through the Curie point, the polarization changes discontinuously from P = 0 in the ferroelectric phase to P = 0 in the paraelectric nonpolar phase. In the firstorder transition, the crystal suddenly loses all the energy associated with the polarization at the Curie point, indicating a big change in its latent heat. We can calculate the actual transition temperature T2, above which the polar phase does not exist in the absence of electric field. In Equation 427, for the minimum freeenergy condition, there are several distinct values of P, for which G is a minimum. Above T2 there is only one value of P, corresponding to the condition g4 2  4 g6 b(T2  Tc ) = 0
(435)
Thus, T2 = Tc + g4 2 4bg6
(436)
In this case the Curie temperature is lower than the actual transition temperature by 1 [ g4 2 bg6 ]. For BaTiO3, T2  Tc = 10°C,30 4
Ferroelectrics, Piezoelectrics, and Pyroelectrics
Based on Equation 417, the differential form of the Gibbs freeenergy function can be written as i
(437)
j
Here we choose T, X, F instead of T, X, P as the independent variables. Under a constant stress condition with the applied field along one direction, Equation 437 can be simplified to dG =  SdT + PdF
(438)
At the Curie point, the free energy in the ferroelectric phase and that in the paraelectric nonpolar phase are equal. So for dG = 0, we have ∂T P = ∂F S
(439)
In this case, p and S are, respectively, the spontaneous polarization and the entropy at T = Tc. The discontinuous change in polarization at the Curie point causes a discontinuous change in entropy and hence the latent heat typical of a firstorder transition. The entropy can be expressed as S=
Ê ∂ Gˆ Ë ∂ T ¯ X, P
(440)
By differentiating Equation 425 with respect to T, and, for simplicity, ignoring all the terms with powers of P equal to or higher than 4 (because the coefficients of these highpower terms do not vary much with temperature), we obtain S=
1 ∂ g2 2 1 2 Ê ∂ Gˆ =P = bP Ë ∂ T ¯ X, P 2 ∂T 2
C 120.1°
15
(441)
Substituting Equation 433 for P into Equation 441, we obtain
122.2 125.3
10 5
0
ElectricField Dependence of the Curie Temperature
dG =  SdT + Â hi dXi + Â Pj dFj
20 P (mC cm–2)
indicating T2 > T1. In ferroelectrics with a firstorder transition, such as BaTiO3, the transition temperature is always at a slightly lower value when the crystal is cooling from the high temperature than when it is heating from the low temperature. This phenomenon is generally referred to as thermal hysteresis.
241
1
2
3 4 5 F (kV cm–1)
6
7
Figure 425 Hysteresis of BaTiO3 above the Curie point at three different temperatures.
∂T P 2 4 Ê g4 ˆ = = = ∂ F S bP 3b Ë g6 ¯
12
(442)
For BaTiO3, ∂T/∂F = 1.72 ¥ 103 °C cm V 1. This value agrees well with the experimental value, which is 1.43 ¥ 103 °C cm V1.30 The above argument indicates mainly that at temperature T > Tc, the crystal can be forced by an applied field to make a transition into a ferroelectric state and then return to the paraelectric nonpolar state when the field is reduced, producing a double hysteresis loop, as shown in Figure 425 for BaTiO3. The data for Figure 425 are from Meyerhofer.75 Antiferroelectric Transition A crystal is antiferroelectric if it exhibits paraelectric behavior, (i.e., the dielectric constant increases with decreasing temperature above the transition point) but does not show a net spontaneous polarization and the dielectric constant is considerably low below the transition point. A typical example is the PbZrO3 crystal (see Figure 420). This indicates that the transition involves a different mechanism for dielectric polarization. Xray analysis has revealed the existence of a superstructure below the transition point. The superstructure can be described in terms of two superlattices having equal but opposite polarization; above the transition temperature, the two superlattices are crystallographically equivalent and are unpolarized. In the previous section, we analyzed ferroelectric phenomena based on an appropriate
8
242
Dielectric Phenomena in Solids
thermodynamic free energy function G, which is expressed in powers of the polarization P. According to Kittel,76 the same approach can be applied to an antiferroelectric crystal if G is expressed in powers of the polarization Pa and Pb of the two superlattices. It should be noted that, unlike P for ferroelectrics (which can be detected), Pa and Pb for antiferroelectrics are not macroscopically observable quantities. However, following the same procedure for Equation 420, we can write G( Pa , Pb , T ) = Go (T ) + f ( Pa2 + Pb2 ) + gPa Pb + h( Pa4 + Pa4 ) + k ( Pa6 + Pa6 ) + . . .
(443) Whether the ferroelectric state (Pa = Pb), the antiferroelectric state (Pa = Pb), or the paraelectric state (Pa + Pb = 0) has the lowest free energy depends on the values of the coefficients. To deal with the antiferroelectric transition, it is convenient to transform Pa and Pb into the following parameters: P+ = Pa + Pb P = Pa  Pb
(444)
We can consider P+ as the total polarization and P as a measure of the antiferroelectric state. Substitution of Equation 444 into Equation 443 gives G( P+ , P , T ) = Go (T ) +
1 1 g2 P+2 + g4 P+4 2 4
1 g6 P+6 + . . . 6 1 1 + g2¢ P2 + g4¢ P4 2 4 1 6 + g6¢ P + . . . 6 1 + lP+2 P2 + . . . 2 +
(445)
where the coefficients g2, g4, g6, g¢2, g¢4, g¢6, . . . and l, etc., are related to the coefficients f, g, h, k, etc. Detailed analysis of antiferroelectric behavior is beyond the scope of this chapter. In general, an antiferroelectric state exists if G has a minimum for a finite value of P . Obviously, this condition depends strongly on the sign and
the value of the coefficients. Normally, the coefficient g¢2 decreases with decreasing temperature, and the antiferroelectric state is stable 1 at low temperatures. If the term lP+2 P2 is 2 positive and sufficiently large, then one kind of the state (e.g., antiferroelectric state) will prevent the formation of the other (e.g., ferroelectric state). The sharp decrease of the dielectric constant below the transition point is due to the saturation effect of Pa and Pb. Antiferroelectrics can be piezoelectric. Some antiferroelectric materials may also become ferroelectric under the application of a suitable electric field.77 It is not so obvious that domains would be formed in antiferroelectrics. However, optical observation has revealed the domain structure of PbZrO3 and NaNbO3 antiferroelectrics. The domains are nonpolar; therefore, their patterns should not be affected by external electric fields. For more details about antiferroelectric phenomena, see references.38,78 A twodimensional picture illustrating the basic difference among the ferroelectric, antiferroelectric, and ferrielectric states is given in Figure 4.26. In the ferroelectric state, there is polarization in the vertical direction and no polarization in the horizontal direction; in the antiferroelectric state, there is no net polarization in either the vertical or the horizontal direction; in the ferrielectric state, the crystal could be antiferroelectric in the vertical direction and ferroelectric in the horizontal direction. However, ferrielectric behavior is not really similar to its ferrimagnetic counterpart. It is a very strange behavior. An example of ferrielectric behavior is thiourea [SC(NH)2]. The reversal of the polarization in this crystal is related to relative displacements of entire molecules, rather than to the motion of single atoms or ions in the lattice, and its polarization phenomenon can be considered ferrielectric.79 4.2.4 Formation and Dynamics of Domains A single crystal or a system that is ferroelectric will undergo spontaneous polarization below the Curie temperature. If all the dipoles of the
Ferroelectrics, Piezoelectrics, and Pyroelectrics
(a)
(b)
243
(c)
Figure 426 Schematic illustration of the polarization in (a) ferroelectric structure, (b) antiferroelectric structure, and (c) ferrielectric structure.
polarization are pointing in one direction, the electrostatic energy of the system is extremely large and the system becomes very unstable. Naturally, a system always tends to minimize its potential energy by forming the socalled domains, which are actually regions in the crystal, each containing a large number of dipoles all aligned in the same direction. Domains are arranged in such a way that the polarization of different domains will compensate for each other and the net polarization of the whole crystal along any direction will vanish. Domains are separated by domain walls, which are the loci of the dipole orientation from one direction of the domain to another of the neighboring one. A single crystal may contain many domains with zero net polarization, but it can be changed to a single crystal with a single domain by a strong poling electric field, in which the dipoles of all domains must point in the same direction. In other words, all domains will join to form a large domain. For polycrystalline materials such as ceramics, single domain cannot be achieved because the crystal axes of the grains (crystallites) in the material are randomly arranged, which cannot be altered by the electric field. When a phase transformation begins, the domains will be nucleated at several places within the crystal, and the nuclei of domains will grow along the ferroelectric axes until the transformation of the new phase in the whole volume is completed. Ferroelectric domains are closely analogous to ferromagnetic domains. In uniaxial ferroelectrics such as TGS crystals, the domains can have only two possible dipole
directions, so the polarization will be in opposite directions in adjacent domains by twinning. In this case, the domain walls are called the 180° walls, as shown in Figure 427(a). For multiaxial ferroelectrics such as BaTiO3, domains can have more than two dipole directions. For example, in the tetragonal phase, polarization is along the caxis, that is, the elongated axis of the cubic structure. But in the ferroelectric phase, there are six easy directions deriving from the cubic structure, that is, the caxis can be in the ±x, ±y, and ±z directions. This implies that there are three pairs of antiparallel directions along the cube edges and that domains can have six directions of polarization. This gives rise to different types of domain walls: Those separating antiparallel dipoles are 180° walls, and those separating dipoles at right angles to each other are 90° walls, as shown in Figure 427(b) and (c). Similarly, for the ferroelectric phase with the unit cell in rhombohedral structure, the polarization is along the bodydiagonal directions. In this case, there are eight easy directions for spontaneous polarization. The angle between adjacent domains becomes 70.5° and 110°, so the domain walls are called the 70.5° and 110° walls. Some typical domain patterns in crystals are illustrated schematically in Figure 427. The electrostatic energy decreases with an increase in the number of domains formed due to the decrease in the depolarizing field. However, the domain formation process does not continue indefinitely, because a certain amount of energy is stored in the walls between different domains. For ideal crystals, when the
244
Dielectric Phenomena in Solids
(a)
(b)
(c) Figure 427 Schematic illustration of some domain patterns: (a) antiparallel domains with 180° walls, (b) domains with 180° and 90° walls, and (c) mixture of domains in c and a directions (a is perpendicular to c).
domain wall energy has increased to a certain critical value, at which it just balances the decrease in energy of the depolarizing field, the total potential energy of the crystal becomes minimal. Under this condition, the domain configuration has reached an equilibrium and stable state at the temperature considered. But for real crystals that are not completely
nonconductive and contain various defects, the domain configuration is hardly stable at any temperature because the charges induced by spontaneous polarization are partially compensated by the conducting carriers in the materials, and the uniformity of the polarization and the depolarizing field is disturbed by various defects. Because of such defects and the
Ferroelectrics, Piezoelectrics, and Pyroelectrics
conductivity of real crystals, the domain patterns do not always correspond to the absolute minimum of the free energy. This implies that the domain configuration is only metastable, resulting in the aging effect. The calculation of domain wall energy is very complicated, but the width of the domain walls is directly related to the total energy of the domain walls. The total wall energy is the sum of the energy due to dipole interaction and the anisotropy energy.22,39 Thus, the total wall energy Uwall can be written as Uwall =
A + Bd d
(446)
where d is the wall width and A and B are functions of the lattice constant, the spontaneous strain and the elastic constant. By minimizing the wall energy dUwall =0 dd
(447)
This leads to d = ( A B)1 2
(448)
Merz22 has estimated the wall width to be of the order of several lattice constants and wall energy of the order of 106 joule cm2, in contrast to the ferromagnetic domain walls whose width is of the order of several hundred lattice constants. In a ferromagnetic domain wall, the magnetization vectors must turn over gradually from one direction to the opposite one, which involves a change in exchange energy and anisotropy energy. This is why the ferromagnetic domain walls are much wider than the ferroelectric domain walls. The difference between the ferroelectric and the ferromagnetic domain walls is shown in Figure 428. In Equation 446, the first term A/d is the energy from dipole interaction due to the fact that the polarization changes from +P to P in the wall, and the second term Bd is the energy from the stress causing the strain changes from + strain to  strain in the wall. In ferroelectric materials, the first term (due to sideways interaction of adjacent dipoles) is small, whereas the elastic energy due to the changes of the strain is large. This is why the domainwall width is
Wall Width
(a)
245
Wall Width
(b)
Figure 428 Schematic illustration of the difference between (a) the ferroelectric and (b) the ferromagnetic 180° domain walls. The width of the domain walls is about several lattice constants for ferroelectrics and about several hundred lattice constants for ferromagnetics.
only several lattice constants. For ferromagnetic materials, the domain walls are a hundred times wider because the interaction energy of magnetic dipoles is large and the elastic energy is small. In general, strain energy is the dominant component in the ferroelectric domain wall energy budget, and the 180° and 90° walls are thus distinctly different in behavior. It is easy for the 180° walls to move under the influence of an applied electric field. The motion of the 180° wall merely requires the cations to move cooperatively toward the other end of their cages without involving the rotation of the polarization vectors or any change in the shape of the crystal. This implies that the domains with the polarization in the direction of the applied field expand sideways by moving the walls toward the domains with the polarization opposite to the field direction, making them shrink and eventually vanish. In other words, the two antiparallel domains will join or coalesce to form a big domain, with all dipoles aligned in the field direction. For the reversal of the polarization, an applied field should be normally higher than the coercive field Fc, and the time required for the complete reversal depends on the magnitude of the applied field following the relation ts = kF  n
(449)
where k and n are constants.30 It should be noted that when the applied field is small, the reversal may still occur, but a much longer switch
246
Dielectric Phenomena in Solids
ing time is required. This implies that the socalled coercive field Fc does not have a clear physical meaning, as fields much smaller than Fc still switch on the reversal, if the applied field is held for a sufficiently long time. For low fields, ts follows an exponential law is • exp (a/F), rather than a power law, given in Equation 449. The switching time is directly related to the velocity of the motion of domain walls. At high fields (>1 kV cm1), the sideways wall velocity follows the relation80 vs = hF m
(450)
where h and m are positive constants. It can be seen that vs is approximately proportional to the reciprocal of the switching time ts. However, when two 180° walls are sufficiently close, they do not move toward each other and there appears to be a repulsion between them. This repulsion results in the formation of a very narrow metastable region which suddenly disappears when an electric field is applied, creating Barkhausen pulses. The 90° walls are relatively difficult to move and usually require an applied electric field greater than a certain threshold value. In general, the motion involves the nucleation and growth of new domains with the polarization in the direction of the applied field. Thus, making the domains with polarization perpendicular to the applied field change to polarization along the field direction may sometimes cause the crystal to change shape. The process for a complete polarization in the direction of the applied field for a multiaxial ferroelectric could be quite complicated. Let us take a simple case as an example. For a singledomain crystal with the polarization along the caxis in the tetragonal phase, if an electric field is applied along the aaxis (perpendicular to the caxis), then a large number of needlelike new domains nucleate at the surface and are polarized in the direction of the applied field, growing in the form of wedges.81 The formation of new domains continues until the whole crystal is polarized in the same direction of the applied field. These newly formed domains originate at the surface of the crystal specimen (usually at the electrode
surface) and grow in the direction of the applied field with very little sideways motion of the walls. However, it can be imagined that the nucleation of new domains becomes more difficult because more nuclei are already present, due to more electromechanical interaction, particularly in multidomain crystals. Sideways motion of 90° walls in an applied electric field has been observed.39,81 Since the 90° wall width is only about several lattice constants, the activation energy for the wall motion is only a small fraction of the total wall energy. The critical field for the 90° wall motion is smaller than that for the nucleation and the growth of new domains. However, the motion causes a change in the shape of the crystal. For a more detailed discussion of the formation, structure, and dynamic behavior of domains, see references 22, 30, 38, 39, 78, and 80–86. 4.2.5 Ferroelectric Materials There are now many hundred materials that exhibit ferroelectric or antiferroelectric properties. In Section 4.2.2, the properties of some representative ferroelectrics were discussed. In this section, we will not list all the ferroelectric materials but summarize some important properties of some ferroelectrics with the potential for practical applications in Table 42. The most commonly used ferroelectrics have the Perovskite structure, with the chemical formula ABO3. The PZT system is a good example, consisting mainly of the alloy of PbTiO3 and PbZrO3. The general formula of the PZT system is PZ1xTx, so the ferroelectric properties can be tailored by varying the composition of Zr and Ti, that is, by varying the value of x. It is not always convenient to keep ferroelectric devices in an oven or a cryostat in order to maintain the required properties. Now, materials can be modified so that certain values of the required properties can be achieved at room temperature. The control of properties is possible by varying the composition in solid solution or by incorporating suitable additives.87 One good example is a ceramic formed by a solid
Ferroelectrics, Piezoelectrics, and Pyroelectrics
247
Table 42 General transition properties of some ferroelectric crystals.
Curie Temperature, Tc (°C)
Spontaneous Polarization Ps(mC m2) at [T (°C)]
Above Tc
Below Tc
Crystal Structure
Name (Abbreviation)
Chemical Formula
Barium Titanate
BaTiO3
120
26.0 [23]
Cubic
Tetragonal
Lead Titanate
PbTiO3
490
50.0 [23]
Cubic
Tetragonal
Potassium Niobate
KNbO3
435
30.0 [250]
Cubic
Tetragonal
Potassium Dihydrogen Phosphate (KDP)
KH2PO4
150
4.8 [177]
Tetragonal
Orthohombic
Triglycine Sulfate (TGS)
(NH2CH2COOH)3• H2SO4
49
2.8 [20]
Monoclinic (Centrosymm.)
Monoclinic (Noncentrosymm.)
PotassiumSodium TartrateTetrahydrate (Rochelle salt)
KNaC4H4O6•4H2O
24
0.25 [5]
Orthorhombic (Centrosymm.)
Monoclinic (Noncentrosymm.)
Antimony Sulfoiodide
SbSI
22
Orthorhombic (Centrosymm.)
Orthorhombic (Noncentrosymm.)
Guanidinium Aluminium Sulfate Hexahydrate (GASH)
C(NH2)3Al(SO4)2•6H2O
Trogonal
—
None
500 400 300 Tc (°C)
solution of PbTiO3 in BaTiO3, in which the transition temperature depends on the concentration of Pb in BaTiO3. In this case, all concentrations are possible and they are ferroelectric. An increase in Pb concentration causes the transition temperature Tc to increase from 120°C to 490°C. Similarly, the substitution of zirconium for titanium in BaTiO3 lowers the value of Tc, as shown in Figure 429. Iron, strontium, and calcium also tend to lower the value of Tc. For details about this subject, see references 39, 88, and 89. Ferroelectrics in ceramic forms are commonly used for practical applications because they have the advantage of being a great deal easier to prepare than their single crystal counterparts. Also, in many cases their ferroelectric properties approach quite closely those of the single crystal. As mentioned above, a wide range of ceramic compositions and additives can be used to adjust the properties of the material for different applications. Ceramics are generally prepared by grinding the material,
0.35 [23]
SrTiO3 BaZrO3 BaSnO3
PbTiO3
500 400 300
200
200
100
100
0
Tc (°C)
25.0 [0]
0
–100
–100
–200 –200 100 80 60 40 20 0 20 40 60 80 100 ABO3 Mole % of ABO3
BaTiO3
Mole % of PbTiO3 PbTiO3
Figure 429 The effect of various additives in BaTiO3 on the Curie temperature Tc.
together with any required additives, into powder. This reacted powder is usually ballmilled to increase homogeneity and particle reactivity. This may be processed with or without binder. Then the material is extruded or pressed into some shape and fired at a higher temperature (e.g., 1300°C), at which sintering occurs.44 This fabrication procedure produces a
248
Dielectric Phenomena in Solids
complicated polycrystalline material that has pores, some unavoidable impurities, and many crystallites of various sizes. Some properties of a ceramic may differ from those of the corresponding single crystal material because the crystallites in the ceramic are randomly oriented and some of them are under stresses even when no external force is applied; also, there exist grain boundaries and porosity. The ferroelectric properties of ceramics depend greatly on the grain (crystallite) size. In a ceramic with small grain sizes, a significant portion of the material volume is affected by grain boundaries. The important difference between grain boundaries and free surfaces is that in highdensity ceramics, the material close to the grain boundaries is elastically clamped by the neighboring grains at temperatures well below the sintering temperature. On cooling to the ferroelectric phase, large mechanical stresses may be developed by the anisotropic spontaneous strain, and these stresses may in turn affect the domain dynamics and configuration. If the grains are too small, the polarization may be completely clamped, preventing the action of domain reversal when the applied field is turned to the opposite direction. As the size of grains increases, domain reversal becomes possible, but the peak dielectric constant decreases, due mainly to the inhomogeneous distribution of the mechanical stresses and electric fields. If the polarization in the neighboring grains is not parallel, then the nonzero polarization at the boundaries creates depolarizing fields, tending to compensate free charges at the electrodes. The grain sizes of ceramics can be controlled to a certain degree during the fabrication processing by adjusting the sintering temperature and time, the composition of the material, and the additives. Most ceramics consist of grains with a range of grain sizes, and their crystallographic axes are randomly oriented. It can be imagined that the poling of a ceramic under an external electric field involves microscopic processes much more complicated than those for single crystals. Because of the grain boundaries, neither dielectric nor elastic relaxations under an alternating field within the bulk of
ceramics are possible. This is why the hysteresis loops are generally rounded, the spontaneous and the remanent polarizations are lower, and the coercive fields are larger; this is also why the aging effect is enhanced. As knowledge of ferroelectric ceramics progresses, new effects and new fabrication techniques, as well as new materials, will certainly be discovered. It is worth mentioning that ferroelectric thin films are very important for practical applications. For certain applications, ferroelectrics in thinfilm form are preferred. In general, the dielectric and ferroelectric properties are thickness dependent if the thickness of the films is below a certain value. For example, BaTiO3 films prepared by electronbeam evaporation or sputtering techniques exhibit normal dielectric and ferroelectric behavior if the film thicknesses are larger than 1 mm. Ferroelectric behavior becomes unstable for film thicknesses below 0.1 mm.90 But some investigators91 have reported that vacuumevaporated BaTiO3 films show well defined dielectric anomalies near 120°C for films with thicknesses down to 0.023 mm. For BaTiO3 films prepared by flash evaporation, the properties remain approximately similar to those of thick films down to a thickness of 0.1 mm.92 The discrepancy can be attributed to different techniques of film fabrication, which result in various structural and chemical defects. Defects aside, the interface between the film and the electrical contacts, the width of the depletion regions inside the film, and electronic conductivity also play important roles in the thickness dependence of the dielectric and ferroelectric properties of thin films. Although several film fabrication techniques (chemical vapor deposition, single or multiple target sputtering, multiple target ion beam, pulsed deposition techniques, etc.) have been put forward,58,93 none can be considered very satisfactory. However, the required degree of perfection varies according to the specific application; thus, the technique for film fabrication should be chosen accordingly. For example, for ferroelectric films used in small capacitors, we would want the films to have a high dielectric constant, low dielectric loss, and a minimal variation of these parameters with
Ferroelectrics, Piezoelectrics, and Pyroelectrics
249
temperature, applied field, and frequency. But for films used in optical devices, we would want the films to have a high optical quality. The trend of using ferroelectric films is ever increasing. The development of new techniques and the improvement of the existing techniques have to a great extent been motivated by various technical applications. It is certain that new experimental and theoretical results in this area will be available in the near future.
for practical applications. The most commonly used effects are the piezoelectric, pyroelectric, and electrooptic effects, which are discussed, respectively, in Piezoelectric Phenomena and Pyroelectric Phenomena in this chapter and Modulation of Light in Chapter 3. In this section, we shall briefly describe some applications related directly to the special features of ferroelectrics: mainly, spontaneous polarization, nonlinearity, and hysteresis behavior.
4.2.6 Applications of Ferroelectrics Based on the classification of crystals given in Figure 41 the following statements can be made:
Capacitors Capacitors are important elements in electrical and electronic circuits, performing various functions that include blocking, coupling and decoupling, ACDC separation, filtering, power factor correction, energy storage, etc. For a capacitor with the dielectric material of dielectric constant er and thickness d between two parallel metallic plates of area A, the capacitance is given by
• All ferroelectrics possess piezoelectric and pyroelectric effects. • All pyroelectrics possess piezoelectric effects, but not all are ferroelectric. • Piezoelectrics may have only piezoelectric effects, both piezoelectric and pyroelectric effects, or all three effects: ferroelectric, piezoelectric, and pyroelectric. Depending on the crystal structure, spontaneous polarization in a poled ferroelectric crystal can be varied to produce different effects by the application of an external force, such as a mechanical stress, an electric field, or a change in temperature. Figure 430 illustrates these effects. Each of these effects can be used
C = e re o
A d
(451)
If the working voltage is V, the average working field F is V/d, which must be lower than the breakdown strength of the dielectric material Fb by factor k. The volume efficiency of the capacitor is defined as h=
C e re o = 2 dA d
(452)
Mechanical Stress
Poled Ferroelectric Specimen
•Piezoelectric Effect (Due to change in polarization P ) •Piezocalorie Effect (Due to change in entropy S ) •PiezoOptic Effect (Due to change in strain h —elastic displacement resulting in change in refractive index)
Electric Field
Poled Ferroelectric Specimen
•Converse Piezoelectric Effect (Due to change in strain h ) •Electrocalorie Effect (Due to change in entropy S ) •ElectroOptic Effect (Due to change in polarization and hence in susceptibility)
Temperature Change
Poled Ferroelectric Specimen
•Pyroelectric Effect (Due to change in polarization P ) •Thermoelectric Effect (Due to change in strain h) •Heat Capacity Effect (Due to dQ = SdT )
Figure 430 The effects of a mechanical stress, an electric field, or a temperature change on the behavior of a poled ferroelectric specimen.
250
Dielectric Phenomena in Solids
The maximum permissible energy density stored in the capacitor is thus CV 2 e re o Fb2 = 2 Ad 2k 2
(453)
The value of erF 2b is a figure of merit for dielectrics. All dielectric materials have a finite value for DC resistivity. Thus, a charged capacitor will discharge gradually through its own resistance following Q(t ) = Qo exp( t t )
(454)
where Qo and Q(t) are, respectively, the initial charge and the charge remaining in the capacitor at time t; t is the dielectric relaxation time of the material, which is equal to ereor; and r is the resistivity of the material. A capacitor dissipates its stored energy through DC leakage resistance and, more importantly, the dielectric losses under an AC electric field. These account for the dissipation factor or the loss tangent tand (see section 2.2.3 in Chapter 2). It should also be noted that the leads and the electrodes always introduce an inductance L in the circuit. This is why a capacitor has a resonance frequency which may be very high, depending on the value of L. For general applications, it is important to keep the value of the unwanted stray inductance L as small as possible. However, from Equations 452 and 453, both the volume efficiency and the maximum energy stored in a capacitor increase proportionally with increasing dielectric constant. Thus, ferroelectric materials with high dielectric constants are obviously ideal materials for use in miniature capacitors. But the capacitance of the capacitors made of ferroelectric materials is dependent on temperature, applied electric field, and frequency. Usually, it is not so difficult to tolerate a small change in electric field and frequency, but the range of temperature variation is large under certain environmental conditions, and also the dielectric constant is strongly dependent on temperature, particularly at temperatures near the transition point. So for highpermittivity capacitors, it is necessary to choose a material with a small temperature coefficient of the capacitance (TCC), which is
TCC =
1 dC C dT
(455)
From Equation 451 we obtain 1 ∂ er 1 ∂ A 1 ∂ d + er ∂ T A ∂ T d ∂ T = TCD + a L
TCC =
(456)
where TCD is the temperature coefficient of the dielectric constant and aL is the linear expansion coefficient. So the change in capacitance due to a change in temperature is caused by the change of the capacitor’s dimension, which is usually not very significant, and by the change of the dielectric constant, which is significant, particularly at temperatures near the transition point. Ferroelectric ceramics are commonly used for capacitors. The Electronic Industries Association (EIA) in the United States has grouped ceramic capacitors into three classes: Class I: The materials have a low dielectric constant (ranging from 15 to 500), low dielectric losses (tand < 0.003), a low TCC, and a low rate of aging of the capacitance value. The working temperature range is 55°C to +85°C. Class II: The materials have medium to large dielectric constants (ranging from 500 to 20,000), with general properties primarily similar to BaTiO3 ceramics. The dependence of temperature, electric field, and frequency is stronger than for Class I, and the TCC value is higher. Class III: The materials consist of a conductive phase near the electrodes that reduces the effective thickness of the dielectric material. General properties are similar to those of Class II, but their working voltage is lower. The EIA has also introduced a scheme for specifying the variability of the capacitance with temperature in the range of practical interest for highpermittivity capacitors. Table 43 lists the EIA codes. For example, a capacitor of EIA code X7E implies that its capacitance may change by no more than ±4.7% in the range of temperatures from 55°C to +125°C.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
251
Table 43 The EIA codes for the specification of highpermittivity capacitors. EIA Code
Range of Temperature Variation (°C)
EIA Code
Change of Capacitance (%)
X7 X5 Y5 Z5
55 to +125 55 to +85 30 to +85 +10 to +85
D E F P R S T U V
3.3 to +3.3 4.7 to +4.7 7.5 to +7.5 10.0 to + 10.0 15.0 to +15.0 22.0 to +22.0 33.0 to +22.0 56.0 to +22.0 82.0 to +22.0
Dielectric materials with dielectric constants larger than 1000 are mainly ferroelectric materials, and they are very sensitive to temperature, electric field, and frequency. Obviously, the development of techniques for modifying the materials to improve stability and to retain the desirable high dielectric constant feature is very important. In fact, this work has been carried out continuously for about 50 years. In general, the dielectric constant is measured with a small AC signal. A bias of a large DC field will cause the value to decrease, but the field coefficient of the dielectric constant is normally small. Frequencies in the range of 0–100 MHz do not affect the dielectric constant to a great extent. The difference in dielectric constant between power and radio frequencies is only 5–10%, and for most ceramics based on BaTiO3 and its isomorphs, the dielectric constant does not vary greatly with frequency until it reaches the gigahertz range. The major concern is the temperature dependence of the dielectric constant. To reduce the temperature coefficient of the dielectric constant (TCD) is thus the goal that many researchers have attempted to reach. Highpermittivity ceramic capacitors are based mainly on ferroelectric BaTiO3, its isomorphs, and their solid solutions. According to Lichtenecker’s rule,94 the TCD of a ceramic formed by the mixture of several components will be equal to the volume average of the TCDs of its constituents, if there is no chemical reaction between constituents leading to the formation of new compounds. Following this rule, the dielectric constant of the mixture can be predicted approximately by Lichtenecker’s empirical formula
log e r = v fl log e rl + v f 2 log e r 2 + v f 3 log e r 3 + . . . n
= Â v fie ri
(457)
i =1
where eri and vfi are, respectively, the dielectric constant and the fraction of the total volume of the mixture of the ith constituent. In general, it is not possible to obtain a completely flattened er  T curve in a homogeneous ceramic having BaTiO3 as a major constituent. However, in the region below the peak, at temperatures below Tc, the value of the dielectric constant does not change much with temperature. This is due partly to the further change in crystal structure to rhombohedral and then to orthorhombic, and partly to the transition changing from first order to second order.95 Some ceramics with different compositions, which would provide usefully high permittivity–temperature characteristics, are given here as examples. Many similar mixtures have already been developed.58,95,96 BaTiO3 and Bi2 (SnO3)3 BaTiO3 and MgSnO3 BaTiO3, SrTiO3, and CaTiO3 BaTiO3 and MgF2 BaTiO3, CaSnO3, and CaO BaTiO3 and CaZrO3 BaTiO3 and CaSnO3
(er = 1000 at 25°C) (er = 2000 at 25°C) (er = 2000 at 25°C) (er = 3500 at 25°C) (er = 3500 at 25°C) (er = 5000 at 25°C) (er = 8000 at 25°C)
Furthermore, the locally inhomogeneous microstructure tends to broaden and flatten the er  T curve. This tendency is enhanced if the growth of grain sizes during sintering can be sufficiently inhibited. There is a large variety of ceramic capacitors, including thinfilm capacitors, thickfilm capacitors, and plate capacitors (based on the
252
Dielectric Phenomena in Solids
thickness of the dielectric material), singlelayer discrete capacitors in disk or wafer, or cylindrical tube form, or multilayer capacitors based on the construction shape. The design depends primarily on the requirements of the capacitors for certain specific applications. For more details about capacitors, see references 58, 59, and 95–98. ThermoAutostabilization Nonlinear Dielectric Elements (TANDEL) When a ferroelectric specimen is switched on to the ferroelectric phase with an alternating field, heat will be produced in the material each cycle, part of which is due to normal dielectric losses and part to hysteresis losses. As a result, the power dissipation WA in the material increases with temperature, reaches a peak at the transition temperature Tc, and then decreases rapidly for T > Tc, as shown in Figure 431. The value of WA increases also with increasing applied AC field. There is heat WB lost by the material through heat conduction and convection to the surrounding medium, which is proportional to temperature. Thus, at the intersection points (such as a, b, c), when the WA–T curve intersects with the WB–T curve, the heat produced in the material is equal to the heat lost from the material to its surrounding medium. So the points a, b, c
WA and WB
WB a c e
b
d
WA (F ) WA (F ¢) WA (F ≤)
f g Temperature
TC
Figure 431 The variation of the power dissipated in the ferroelectric specimen WA and the power lost by the specimen to its surroundings WB with temperature at the applied AC field F > F¢ > F≤.
represent the points of thermal equilibrium for ferroelectric materials. The material itself can stabilize its own temperature, such as point b near the transition temperature Tc where nonlinearity is high.99–101 The elements based on the changes in the dielectric constant, and hence the capacitance with the change of the applied AC field, can be used to replace varactors as circuit elements in frequency modulation, thermostat control, etc. HighEnergy Electrical Pulse Generators Ferroelectric ceramics possess a special feature of high spontaneous polarization and high dielectric constant, the latter being typically several hundred to several thousand, much larger than for organic solid insulators (usually below 10) and for inorganic solid insulators (below 20). Ferroelectric ceramics have already been used widely for energy storage capacitors.102 Ferroelectric ceramics also have a large piezoelectric constant, implying that the electric field produced per unit mechanical stress could be very large. For example, a compression stress of about 0.05 Gpa would generate an opencircuit field of about 5–15 kV cm1.44 The direction of the applied stress for such a piezoelectrically generated high voltage is parallel to the poling direction, and the depoling process is based on the linear piezoelectric effect. However, exploring piezoelectrically generated electric power beyond the linear limit of the linear piezoelectric effect, Neilson103 was the first to suggest that the remanent (or spontaneous) polarization of a poled ferroelectric material could be released by a shock wave of sufficiently high mechanical stress to cause the transition from the ferroelectric phase to an antiferroelectric one, thus resulting in the generation of highenergy voltage or current pulses. Since then, several investigators62,63,104,105 have studied further this method for the generation of highenergy power supplies actuated by a shock wave of mechanical compression through a poled ferroelectric ceramic material. The basic principle is simple. It is important to choose a material with its ferroelectric phase
Ferroelectrics, Piezoelectrics, and Pyroelectrics
very close to the boundary between the ferroelectric phase and the antiferroelectric phase. The phase diagram of the PZT system shown in Figure 419 shows that the PZT 95/5 material with x = 0.05 in the composition PbZr1xTixO3 should be suitable for this application. This material is in the ferroelectric phase (F) with the rhombohedral structure between 50°C and 220°C. It becomes antiferroelectric (AF) with an orthorhombic structure at temperature below 50°C. There is a phase boundary between the F and AF phases that is temperature dependent. However, external electrical field tends to broaden the ferroelectric phase, implying that the F–AF phase boundary tends to move toward the left side. This means that external electric field may convert the original antiferroelectric phase to a ferroelectric phase. A mechanical (compression) stress tends to extend the antiferroelectric phase region, implying that the FAF phase boundary tends to move to the right side. This means that a mechanical shock wave may convert the original ferroelectric phase to an antiferroelectric phase. A poled specimen is a specimen that has been polarized by a sufficiently high electric field F until the spontaneous polarization reaches the saturation value Pp (see Figure 44). Usually, the polarizing field is kept across the specimen for a period of time to ensure that all of the spontaneously polarized domains are aligned in the direction of the field before the field is
reduced to zero and then removed from the specimen. Thus, the poled specimen has a remanent polarization Pr with a bound charge Qb on the electrodes to balance the polarization charge in the specimen, thus keeping the whole system neutral, as shown in Figure 432(a). If a shock wave of compressive stress is now applied to the specimen in the direction perpendicular to the direction of the polarization, then the original ferroelectric phase will change to an antiferroelectric phase, in which Pr Æ 0, and the bound charge Qb on the electrodes will become free charge Q, ready to flow out of the system, as shown in Figure 432(b). Based on this principle, we can generate highenergy electric pulses by a mechanical shock wave. Let us consider a simple mechanical–electrical energy conversion system, as shown in Figure 433(a), with three sides xo, yo, and zo. The shock wave of the compressive stress travels in the z direction, perpendicular to the poling direction along the xaxis, with the velocity u. In this case, the operation is in the normal mode. It takes t = zo /u second for the wavefront to travel across the specimen of width zo. So, when the wave front has traveled for time t, the portion of specimen up to the dashed line in Figure 433(a) has already been depoled. The equivalent circuit of the system is shown in Figure 433(b). The system can be considered a current generator with an internal capacitance Co, resistance Ro, and inductance Lo. The value of Lo depends on the amount of
–Qb = –Pr A (Bound Charge) – – – – – –
+ + + + + + +Qb = +Pr A (Bound Charge)
(a)
253
–Q = –Qb (Free Charge) Metallic Electrode of Area A
– – – – – –
+ + + + + + +Q = +Qb (Free Charge)
(b)
Figure 432 (a) Poled ferroelectric ceramic specimen with a bound charge Qb on the metallic electrodes. (b) After the impact of a mechanical shock wave, the original ferroelectric phase changes to an antiferroelectric phase, and the bound charge on the electrodes is released and becomes a free charge.
254
Dielectric Phenomena in Solids
The current i(t) is thus
zo
(a)
i(t ) = dQ(t ) dt = Pr A t =0
ut
yo
ZL y o
+ Electrode
z XO
x
PS
– Electrode ZL
Shock Wave in z direction
(b)
i
CO RO LO
CL RL
leakage current flowing through the specimen. The external load impedance may consist of capacitance CL alone, CL in parallel with resistance RL, or CL in parallel with inductance LL. However, it is important to have CL always connected to the circuit to protect the system in case breakdown occurs during the phase transition. For a simple case, we can assume Ro = •, Lo = •, ZL consists of CL only and the permittivity of the specimen remains the same just after depoling. Then we have Co = e yo zo xo
(463)
The variation of V and i with time is shown in Figure 434 (solidline curves). However, the ideal case never occurs experimentally because there is always leakage current flowing through the specimen. So Q(t) should include a loss factor, and thus Q(t) should be expressed as Q(t ) = Pr A(t t ) (1  a t ) 0 £ t £ t = Pr A(1  at ) t>t
LL
Figure 433 (a) Schematic diagram of the mechanicalelectrical energy conversion system and (b) the equivalent circuit.
0 £t £t t >t
(464)
The variation of V and i will change accordingly. The dashedline curves shown in Figure 434 represent V and i for a nonideal case. We carried out a simple experiment to demonstrate how this type of highenergy pulse generator would perform. We used PZT with the composition of PbZr0.975Ti0.025O3 plus 1 wt% Nb2O5, because this material has the boundary between the F and AF phases at about room temperature. The phase diagram of this is shown in Figure 435(a). Its general properties are as follows63: • • • •
Density = 7.6 g cm3 Dielectric constant = 1600 (high field) Loss factor tan d = 3 ¥ 102 Curie temperature Tc = 215°C
(458)
0 £t £t
The charge released for t = 0 to t = t is V
Q(t ) = q(t ) in the system + qL (t ) in the load
and the voltage between the electrodes is V (t ) = q(t ) Co = qL (t ) CL = Q(t ) (Co + CL )
(460)
Since Q(t ) = Pr A(t t ) = Pr yo zo (t t ) = Pr A = Pr yo zo
Voltage or Current
(459)
i
0 £t £t t >t
(461)
0
t
Time t
so V (t ) = Pr A(t t ) (Co + CL ) = Pr A (Co + CL )
0 £t £t t >t
(462)
Figure 434 V and i as functions of time. Solidline curves are for the ideal case and the dashed line curves for a nonideal case.
100
FRH
50
AFOR
FRL
0 0.02 0.04 0.08 x (Fraction of Ti)
400 300 200 100 0
(a)
V (kV)
150 i (A)
Temperature (°C)
Ferroelectrics, Piezoelectrics, and Pyroelectrics
1
2 3 t (ms)
(b)
120 80 40 0
255
1 2 3 4 5 6 t (ms)
(c)
Figure 435 (a) Phase diagram of the PbZr1xTixO3 + 1 Wt% Nb2O5 system. (b) Shortcircuit currenttime curve. (c) Voltage–time curve.
• Electromechanical coupling factor kp = 0.1 • Piezoelectric coefficient d33 = 7 ¥ 1012 coulomb/newton The shock wave of the compressive stress was produced by an explosive system consisting of an initiating detonator, a plane wave generator, and a spacer to control the magnitude of the stress. The stress used for this investigation was about 3 Gpa, the shock wave velocity was 0.385 cm ms1, and the width of the wave was much longer than t. This compressive stress was sufficient to cause all remanent polarization (bound charge) to be released. Some typical results are briefly described as follows. ShortCircuit Current
We used specimens with xo = 0.5 cm, yo = 28 cm, and zo = 1 cm, so t = zo /u = 2.6 ms. Since Pr = 32.3 mC cm2, the total charge on the electrode is Qb = Pryozo = 904.4 mC. For this system, Co = ereoyozoxo1 = 8.4 ¥ 109 F. Thus, the charge Q(t) = Qbtt 1 and the current i = dQ/dt = Qbt 1 for 0 < t < t, and i = 0 for t ≥ t. The result is shown in Figure 435(b). The experimental value of 337 A for i is close to the calculated value of 904.4/2.6 = 348A. Voltage across Load Impedance Consisting of CL and RL
For this experiment we used specimens with xo = 4 cm, yo = 4 cm, and zo = 1 cm. In this case, Co = 1.5 ¥ 1010 F, we used CL = 9.75 ¥ 1010 F and RL = 39 kW. The result is shown in Figure 435(c). The experimental value of V across RL
is 107 kV, which again is very close to the calculated value of 111 kV. It should be noted that most ceramics are not good insulators. They consist of many pores and other defects, and generally they have a low resistivity and low breakdown strength. During depoling, a high voltage would be developed in the depoled section, which may enhance filamentary carrier injection from the electrodes, leading to local heating in certain regions. All of these factors may operate simultaneously to limit and affect the performance of the system.
Memories The bistable polarization of ferroelectrics can be used for binary memory systems in the same way as the bistable magnetization of ferromagnetics. The memory is nonvolatile and does not require a holding voltage. The idea of using ferroelectric bistable polarization for memories was first suggested by Anderson.106 The basic principle is simple. A ferroelectric matrix store is shown schematically in Figure 436 (a). The row and column electrodes are on opposite surfaces of the ferroelectric specimen. Thus, there are a number of square portions of the specimen having electrodes on both surfaces; each portion is one cell of the memory. The cell may have two remanent polarization states (+Pr or Pr). To write can be achieved by applying an electric field pulse Fx to the row electrode and a pulse Fy to the column electrode, both additively to produce a polarization of full magnitude 2Pr in the cell, and so it is dressed. To read, similar pulses Fx and Fy (but
256
Dielectric Phenomena in Solids
Fy :
Fx :
(a)
(b) P
Fy
Fy Fc 2
Pr
< F < Fc t
t Fc
FX
F
FX t
t
Writing
–Pr F
Reading
x
F x+ F y
(c)
(d)
Figure 436 (a) Electrode arrangement for a ferroelectric matrix store, (b) electrical circuit for the application of voltages (or electric field) pulses to the electrodes, (c) the polarities of electric field pulses for Writing and for Reading, and (d) the total polarization 2Pr attained by simultaneous application of Fx and Fy pulses additively.
with the polarities opposite to those for writing) are applied to the electrodes to depole the polarized cell, so the stored charge 2Pr will be released generating a current or a voltage pulse across a registered resistor. Figure 436 (b) through (d) illustrates this writing and reading process. It can be seen that the cells receiving a single pulse Fx or Fy are hardly affected; the two pulses must be coincident for both the writing and the reading. It should be noted that for a nondestructive readout, arrangements must be made to restore the original state of a cell after reading it. Fer
roelectric stores are similar to ferrite stores, but the former have some major shortcomings, mainly the low switching speed, the decay of the stored signal with repeated uses due to the inherent fatigue behavior, and the aging effect. Many suggestions have been put forward to deal with these shortcomings.107–110 For example, the combination of thin ferroelectric film technology with siliconbased memory technology offers the potential of combining nonvolatility with the fast read and write characteristics of dynamic random access memory (DRAM) and the small cell size of the
Ferroelectrics, Piezoelectrics, and Pyroelectrics
memory.108,110 For certain applications, such as for satellites, the radiation hardness of ferroelectric materials is a very attractive feature.108,109 Depending on the requirements of the particular application, ferroelectric memories have their own merit and deserve further development. By comparison, however, it appears that in some respects ferroelectric memories cannot compete with their well established magnetic and semiconductor counterparts. As a result, attention has been shifted to optical memories. For some excellent literature on optical memories, see references.98,111–114
4.3
Piezoelectric Phenomena
Crystals formed by polar molecules with a noncentrosymmetic structure (i.e., without a center of symmetry) will exhibit a piezoelectric effect. This implies that a mechanical stress applied to the crystal specimen will create an overall polarization and hence a voltage across it. The reverse of the stress direction will cause the reverse of the polarity of the polarization and hence the voltage. The piezoelectric effect is convertible. This means that an applied electric field will create a mechanical strain, expansion, or contraction, depending on the direction of the field. In general, an applied electric field always causes mechanical distortion in the geometric shape of the material, because matter is constructed of charged nuclei surrounded by a compensating electron cloud. The polarization induced by the applied field will cause changes in charge distribution and hence mechanical distortion. The strain resulting from the mechanical distortion is proportional to the square of the field, and this phenomenon, called electrostriction, is not inversive. This means that a mechanical stress acting on mass points cannot induce dipole moments from the neutral state of the material. Electrostriction occurs in all materials, although its effect, for most practical cases, is extremely or negligibly small. The direct effect of the piezoelectricity is the generation of electric polarization by a mechanical stress (acting like a generator), while the converse or inverse effect is the mechanical
257
movement actuated by an electric field (acting like a motor). There are two principal mechanisms for piezoelectricity. Based on the first mechanism, the dipole moments may just mutually cancel each other in the material under the unstrained condition. Piezoelectricity may occur if the crystal has no center of symmetry, and in this case the relation between the electric field and the mechanical strain is linear in the first approximation. This linear relation is sometimes referred to as the linear piezoelectric effect. However, based on the second mechanism, the dipole moment components may remain, but they add to a resulting moment along a polar axis of the unit cell, so the occurrence of piezoelectricity is accompanied by pyroelectricity, involving spontaneous polarization. Thus, for ferroelectric piezoelectricity, the variation of the mechanical strain with the applied electric field follows the change of polarization in the hysteresis loop, as shown in Figure 437. During the poling process, there is a small expansion of the material along the poling direction and a contraction in directions (lateral directions) perpendicular to it. So the strain along the poling direction is positive. In Figure 437, the solid line traces the poling strain from a virgin state 0 to saturation state C and remanent state D. The lateral strain is negative. Both the poling and the lateral strain–field relations form a butterflyshaped hysteresis. Figure 437 shows the basic differences among electrostriction, linear piezoelectricity, and ferroelectric piezoelectricity. In general, ferroelectric piezoelectrics, such as ceramics, have advantages for use in transducers because they have a large piezoelectric coefficient, especially near the transition temperature, and a high dielectric constant that allows the electromechanical coupling factor to approach unity. In comparison with nonferroelectric materials, ferroelectrics may have a high coupling constant, but they also have high dielectric losses. 4.3.1 Phenomenological Approach to Piezoelectric Effects Thermodynamically reversive interactions occur among the electrical, mechanical, and
258
Dielectric Phenomena in Solids Lateral Direction 0 F
Strain Strain
Strain
Strain
C
D
0
F
0
F
D
0
F
0
P
C
F
Poling Direction Electrostriction
Ideal Piezoelectricity
Ferroelectric Piezoelectricity
Figure 437 Schematic illustration of the variation of mechanical strain with electric field for electrostriction, ideal piezoelectricity, and ferroelectric piezoelectricity in poling and lateral directions.
thermal properties, as illustrated in Figure 438. The lines joining pairs of circles indicate that a small change in one of the variables causes a corresponding change in the others. The three direct relations are as follows. The relation between electric field F and displacement D defines the permittivity e D = eF
(465)
The relation between mechanical stress X and strain h defines the elastic compliance or elastic constant y (y = 1/Y, where Y is the modulus of elasticity or the elastic stiffness coefficients). h = yX
(466)
The relation between temperature T and entropy S defines the heat capacity Q S = QT 1
(467)
The lines joining the circles at different corners define the coupling effects. For ordinary solids, the properties follow Equations 465 through 467. But for piezoelectric materials, additional terms are required. For example, a mechanical stress causes not only a strain, but also electric polarization, even at a constant temperature.
Thus, the displacement induced by the stress can be expressed as D = dX
(468)
where d is one of the piezoelectric constants (or coefficients) whose unit is coulombs/newton. In the converse piezoelectric effect, we can also express the relation between electric field and the strain as h = dF
(469)
In this case, the unit for d is meters/volt. In fact, for both the piezoelectric and the converse piezoelectric effects, d is identical, so d=
D h = X F
(470)
In terms of the electric field produced by a mechanical stress, the relation becomes F = gX
(471)
In this case, g is another one of the piezoelectric constants. Its unit is [volts/meter]/ [newtons/meter2]. It can be expressed as g=
d d = e e re o
(472)
Ferroelectrics, Piezoelectrics, and Pyroelectrics
259
ELECTRICAL
lectr e Pi ezoe
cts ffe ic E ctr
Permittivity e
vers
ele zo
Con
ts
fec
loric iezoca
Effect
Therm
city
al Exp
P
He
at C api
y
Ela
Stress X
Ef
ty
tric
t
Entropy S
Strain h i stic
lec roe
ffec
ic E
Pie
Py
alor
Displacement D
troc
Elec
ic E ffect
Field F
ansio
Thermoelastic Effects
MECHANICAL
n
Q
Temperature T
THERMAL
Figure 438 The relations between the mechanical, electrical, and thermal properties for crystals with a noncentrosymmetric structure (without a center of symmetry).
There are two other piezoelectric constants, namely e and f, which are only occasionally used. Their relation is X = eF
(473)
F =  fh
(474)
Rigorous analysis and discussion of these piezoelectric constants (or coefficients) has been reported by Mason115 and Jaffe and Berlincourt.53 These four piezoelectric constants can be defined in partial derivatives as
d=
Ê ∂ Dˆ Ë ∂ X ¯ F ,T
g=
Ê ∂Fˆ Ë ∂ X ¯ D ,T
Ê ∂ Dˆ e= Ë ∂ h ¯ F ,T f =
(475)
Ê ∂ Fˆ Ë ∂ h ¯ D ,T
Similarly, the piezoelectric constants for the converse piezoelectric effects can be written as
260
Dielectric Phenomena in Solids
resulting from the direct piezoelectric effect, or
Ê ∂hˆ d¢ = Á ˜ Ë ∂ F ¯ X ,T
k2 =
Ê ∂h ˆ g¢ = Á ˜ Ë ∂ D ¯ X ,T
(483) (476)
Ê∂ Xˆ e¢ =  Á ˜ Ë ∂ F ¯ h ,T Ê∂Xˆ f ¢ = Á ˜ Ë ∂ D ¯ h ,T
Based on the thermodynamic argument, d = d¢, g = g¢, e = e¢, and f = f ¢. The interactions between the electrical and the elastic variables describe the piezoelectric effects. The equations of state relating the electrical and the elastic variables can be written in general form as D = dX + e X F
(477)
h = y F X + dF
(478)
where the superscripts denote the parameters held constant, so e X denotes the permittivity at constant stress X and y F denotes the elastic compliance at constant electric field F. For the ferroelectric piezoelectricity, the properties are nonlinear, so the equations of state should be written in differential form as d D = dd X + e Xd F
(479)
F
(480)
d h = y d X + dd F
The piezoelectric coefficients dependent. For example,
Mechanical energy from conversion Total input electrical energy
are
d = eX g e = eX f
inter
(481)
d31
Stress or strain direction normal to the field direction Field (or displacement) direction d33
To specify the overall strength of the piezoelectric effect, it is convenient to use the electromechanical coupling factor k, which can be considered the direct way to measure the ability of piezoelectric materials to convert one form of energy to another. This coupling factor k is defined as
resulting from the converse piezoelectric effect. Since the electromechanical conversion is always incomplete, k is always less than unity. Typical values of k are 0.1 for quartz, 0.4 for barium titanate, 0.7 for PZT, and close to 0.9 for Rochelle salt. In general, piezoelectric properties are dependent on orientational direction, so they must be described in terms of tensors. A convenient way to specify the directional properties is to use subscripts that define the direction and orientation, as illustrated in Figure 439. The subscript 3 refers to the polar axis (or poling axis); 1 and 2 refer to arbitrarily chosen orthogonal axes perpendicular to 3. Subscripts 4, 5, and 6 refer the shear planes of the mechanical stress and strain perpendicular to axes 1, 2, and 3, respectively. For example, subscript 4 indicates the change of angle of the stress or the strain between the two initially orthogonal axes 2 and 3 in the shear plane (subscript 4) normal to axis 1. Similar meaning is applied to subscripts 5 and 6. Stress and strain due to shearing action are referred to as the shear stress and shear strain. Piezoelectric coefficients are usually indicated with two subscripts denoting the direction of the properties. The first subscript refers to the direction of the electric field F (or the displacement D). The second subscript refers to the direction of the mechanical stress X (or the strain h). For example,
Stress or strain direction parallel to the field direction Field (or displacement) direction
Electrical energy from conversion k = Total input mechanical energy 2
(482)
In most cases, it can be assumed that the plane perpendicular to the polar axis is isotropic. This
Ferroelectrics, Piezoelectrics, and Pyroelectrics
261
+
3
– Polar Axis 6
2 –
5 –
+
+
4 1
Figure 439 Subscript symbols for the notation of the directional properties for poled piezoelectric materials.
implies that an electric field parallel to polar axis 3 interacts in the same way, with the mechanical stress either along axis 1 or along axis 2. Thus, d31 = d32, d15 = d24, y13 = y23, etc. It should be noted that shear can only occur when an electric field is applied at right angle to the polar axis, so there is only one shear piezoelectric coefficient d15 (since d15 = d24). There are also piezoelectric coefficients corresponding to hydrostatic stress. In this case, dh = d33 + d31 + d32 = d33 + 2d31. Similar notations are used for other piezoelectric coefficients, such as g33, g31, g15, gh, etc. Elastic properties can also be specified in terms of elastic compliance y, such as y11, y12, y13, y33, y44, y66, to denote the interaction of a strain and a stress under the condition of conF F stant field. Thus y should be written as y11 , y12 , F F F F y13, y 33, y 44, y66 (usually for F = 0). Each y relates to the application of a single stress in one direction; the other ys are kept fixed so that there is no lateral restraint. Stress and strain are interchangeable, so y13 = y31. The permittivity e should also be a tensor, but for most cases, the field has only one direction, oblique
components being negligible, so one subscript is sufficient. For example, e33 = e3, e31 = e1, e32 = e2, etc. indicating that e3 is the permittivity along the polar axis 3, and e1 and e2 are the permittivities along axes 1 and 2, respectively. Following the above conventions, Equation 481 becomes dij (∂ h j ∂ Fi ) X ,T = gij (∂ h j ∂ Di ) X ,T =
(484)
Ê ∂ Di ˆ = e Xi Ë ∂ Fi ¯ X ,T
For example, d33 x = e 33 = e 3x g33 d31 x = e 31 = e1x g31
Thus, Equation 479, due to the direct piezoelectric effect, becomes d D1 = d15d X3 + e1xd F1 d D2 = d15d X4 + e 2xd F2
(485) x 3
d D3 = d31 (d X1 + d X2 ) + d33d X3 + e d F3
262
Dielectric Phenomena in Solids
Equation 480, due to the converse piezoelectric effect, becomes d hi = y11F d X1 + y12F d X2 + y13F d X3 + d31d F3 d h2 = y11F d X2 + y12F d X1 + y13F d X3 + d32d F3 F d h3 = y13F (d X1 + d X2 ) + y33 d X3 + d33d F3 F d h4 = y44 d X4 + d15d F2
(486)
F d h5 = y44 d X5 + d15d F1 F d h6 = y66 d X6
4.3.2 Piezoelectric Parameters and Their Measurements The bestknown crystal showing a piezoelectric effect is quartz (SiO2). Lord Kelvin115 was the first to develop a model to explain this phenomenon. For a quantitative analysis of the piezoelectric effect, it is necessary to know first the piezoelectric and dielectric properties of the material. In the previous section, it was shown that piezoelectric properties are primarily governed by the electromechanical coupling coefficient k; the piezoelectric coefficients, mainly d and g; the elastic compliance y; and the dielectric constant er. These parameters are generally dependent on the crystal structure and the direction of the crystal axes, so it is important to know these parameters. The convenient way to determine these parameters is to use an equivalent circuit which consists of two portions: one involving an analog between mechanical and electrical quantities representing mechanical impedance, and the other representing the electrical impedance.4,116–118 The analog between mechanical and electrical quantities follows. Mechanical Quantity
Electrical Quantity
Elastic compliance: y Mechanical mass: m Viscous damping: G
Capacitance: Cm Inductance: Lm Resistance: Rm
First, we measure the resonance frequencies of the piezoelectric specimen under investigation with a sinusoidally varying electric field, as shown in Figure 440(a). By comparing the phase of the AC voltage with that of the AC current, it is easy to determine the frequencies at which Xs = XL  Xc > 0 or Xs < 0 or Xs = 0. The various frequencies are defined as follows:
fR: The resonant frequency at which Xs = 0 (XL = Xc); in this case, XL  Xc increases with frequency for frequencies below fR fA: The antiresonant frequency at which Xs = 0 (XL = Xc), but in this case, XL  Xc decreases with the frequency for frequencies around fA fp: The frequency at which the resistive component Rs is a maximum fs: The frequency at which the series arm of the upper portion of Figure 440(b) has zero reactance (Xm = 0) It can be seen from the equivalent circuit and its frequency response in Figure 440 that the piezoelectric specimen stores energy mechanically in one part of the cycle and feeds it back into the electrical portion in another part of the cycle. The specimen operates in sequence as an electromechanical transducer. It can be shown from the equivalent circuit Figure 440(b) and (c) that fR =
1 2p Lm Cm
fA =
1 2p
Cm + Ce Lm Cm Ce
(487) (488)
The ratio of fA /fR is related to the electromechanical coupling factor by the following equation119 2
8 k2 ˆ Ê fA ˆ = 1+ 2 Ê Ë Ë fR ¯ p 1  k2 ¯
(489)
Thus, from Equations 487 through 489, we obtain k2 =
f A2  f R2 Cm Ce + Cm f R2
(490)
Equation 490 gives good approximations, provided that the quality factor Q of the specimen is sufficiently high. Q is the ratio of the energy stored to the energy dissipated per halfcycle, which is equal to (tan d)1. For most dielectric materials, tan d is very small. For example, when tan d < 0.01, Q > 100. In Figure 440(b), we have already assumed Q > 100, so only the capacitance Ce is included in the electrical portion, the leakage resistance being ignored.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
263
Piezoelectric Specimen
Ls
Ammeter
Cs
Rs
Xs = XL – XC
AC Voltage Source
(a)
Mass
Cm
Rm Reactance
Lm
(c)
Compliance Damping
Capacitance
0
Frequency fR
fA
Ce
(b)
(d)
Figure 440 (a) A piezoelectric specimen under an alternating electric field, (b) equivalent circuit of (a) near the fundamental resonances (the top branch of the circuit represents the mechanical portion and the bottom branch represents the electrical portion), (c) the equivalent series circuit of the impedance of (b), and (d) frequency response near the fundamental resonances.
Once the parameter k has been determined, the other parameters can be determined easily. The mechanical energy stored in the specimen per unit volume is given by Um =
1 1 h2  X h= 2 2 y
(491)
and the electrical energy stored per unit volume is Ue =
1 1  D F= eF 2 2 2
(492)
Thus, we can write k2 =
Um d 2 = Ue ye
(493)
The relations between fR and fA and the elastic compliance y are given by fR =
1 2 l( ry F )1 2
(494)
fA =
1 2 l( ry D )1 2
(495)
Dielectric Phenomena in Solids
where r is the density of the specimen material and is the length of the specimen. The superscript F in yF means y measured at constant field, signifying that the specimen is shortcircuited, while the superscript D refers to y at constant displacement, signifying that the specimen is opencircuited. The permittivity e can be determined from the capacitance measured at a frequency well below resonance. Thus, from Equations 493 through 495, we can determine y, d, and g, since g = d/e. However, the piezoelectric parameters depend on the geometric shape and dimensions of the specimen. The geometry commonly used is a thin disc of diameter dia and thickness t, which is much smaller than dia. Metallic electrodes are deposited on both surfaces of the specimen, and the specimen is poled in a direction perpendicular to the surfaces. In this case, the planar (radial) electromechanical coupling factor kp is of a radial mode, excited through the piezoelectric effect across the thickness of the disc. kp is related to the resonant frequencies fp and fs, defined by the following relation k p2 f p  fs ˆ Ê = F Jo , J1 ,u Ë fs ¯ 1  k p2
(496)
where Jo and J1 are the Bessel functions of the orders of zero and one, respectively; and u is Poisson’s ratio. The other piezoelectric parameters d and g can be determined in the same manner as for the thick specimens, but the expressions for the thin disc are more complex.96 For more details about piezoelectric parameters, see references 44, 59, 96, 120, 121.
some special features of some piezoelectric materials. Quartz is a commonly used piezoelectric crystal, but crystals of the watersoluble type have a much larger electromechanical coupling factor k. For example, ammonium dihydrogen phosphate (ADP) has k 0.30. Still higher coupling can be achieved with ferroelectrics such as PZT (a PbTiO3 and PbZrO3 mixture). The PZT specimen, after being poled with a sufficiently strong electric field, exhibits high values of kp and d depending on the composition, as shown in Figure 441. This PZT system has been studied by several investigators.44,120–124 Aliovalent substituents would modify the properties of ceramics with a Perovskite structure. In order to achieve a given set of properties, PZTbased ceramics may require composition of more than one type of additive. One system that has been widely used for piezoelectric devices is PZT doped with lanthanum to form a new PLZT system. Such systems usually contain 3–12 mol.% La and 5–30 mol.% Ti. For the system with the composition of La : Zr : Ti=7 : 60 : 40, the values of kp and d33 have reached 0.72 and 7.1 ¥ 1010 m/V.125,126 Such high values of kp and d33 have been attributed to the compositions located within the boundary region between the rhombohedral and tetragonal phases.127–129 PLZT may also contain vacancies on B (as 160
0.40 0.35 0.30
Rhombohedral
kp
d33
0.20
100 80 60
0.15
40
0.10 0.05
140 120
kp
0.25
4.3.3 Piezoelectric Materials The most important piezoelectric materials are the ceramics consisting of crystallites of Perovskite structure, such as PZT and PLZT; the synthetic polymers, such as PVDF; and the ceramicpolymer composites. Table 44 lists the typical values of some important parameters of some commonly used piezoelectric materials. All ferroelectric materials are piezoelectric, but not all piezoelectric materials are ferroelectric. We will describe briefly
Tetragonal
d31
20
d ¥ 1012 (Coulombs/Newton)
264
0 0 PbTiO3 PbZrO3 Mole % Increasing PbTiO3 content Figure 441 The planar electromechanical coupling factor kp and piezoelectric coefficient d as functions of the composition of the PZT ceramics.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
265
Table 44 Selected properties of some piezoelectric materials: d = piezoelectric constant, k = electromechanical coupling factor, and r = density. Material (Abbreviation)
Chemical Formula
d (cm V1)
k
r (g cm3)
Silicon Dioxide (Quartz)
SiO2
2.25 ¥ 1010
0.099
2.65
PotassiumSodium TartrateTetrahydrate (Rochelle Salt)
KNaC4H4O6•4H2O
5.30 ¥ 109
0.78
1.77
Barium Titanate
BaTiO3
1.90 ¥ 108
0.38
5.70
9
0.29
1.80
0.12
2.31
—
1.69
0.42
4.45
0.035
4.64
0.10
7.46
—
7.12
0.66
7.70
—
1.40
Ammonium Dihydrogen Phosphate (ADP)
AH2PO4
2.46 ¥ 10
Potassium Dihydrogen Phosphate (KDP)
KH2PO4
1.07 ¥ 109 9
Triglycine Sulfate (TGS)
(NH2CH2COOH)3•H2SO4
5.00 ¥ 10
Potassium Niobate or Sodium Niobate
KNbO3 or NaNbO3
4.90 ¥ 109 10
Lithium Niobate
LiNbO3
0.85 ¥ 10
Lithium Tantalate (LT)
LiTaO3
3.00 ¥ 1010
Lead Titanate
PbTiO3
7.40 ¥ 10
10
Lead Zirconate Titanate (PZT)
Pb(Zr1xTix)O3
2.34 ¥108 10
Polyvinyl Chloride (PVC)
see Table 52
0.70 ¥ 10
Polyvinyl Fluoride (PVF)
see Table 52
1.00 ¥ 1010
0.03
—
see Table 52
10
0.12
1.78
well as on A) sites, providing a favorable way to change their polar states under the influence of applied fields. Polymer films have the following advantages: they are flexible and tough, they can be made very thin (<10 mm) and large in area, they can be shaped into any geometric forms, they have a low mechanical impedance, etc. Polymers, particularly PVDF, have been used widely for various transducers and sensors. For PVDF, the piezoelectric coefficient d and the pyroelectric coefficient p are closely related to the poling parameters. They increase linearly with increasing poling field Fp, poling temperature Tp, and poling time tp, as shown in Figure 442. The data are from Murayama et al.130,131 Apart from PVDF, other polymers, such as polyvinyl fluoride (PVF), polyvinyl chloride (PVC), PTFE, etc., also exhibit piezoelectric effects. PVC is a noncrystalline polymer but has relatively high piezoelectric and pyroelec
4.00 ¥ 10
110°C
15
90 70
d31 (10–12C/N)
Polyvinylidene Fluoride (PVDF or Kynar)
10 50 5 25 0 0
50 100 Poling Field (MV m–1)
Figure 442 The piezoelectric coefficient d31 of PVDF at room temperature as a function of poling field and poling temperature for the fixed poling time of 30 minutes.
tric coefficients when poled at high temperatures. It should be noted that the properties of polymers depend strongly on the preparation techniques and conditions.132
266
Dielectric Phenomena in Solids
To produce materials with optimal properties for a special application, we may choose a suitable ceramic–polymer composite. In general, a composite refers to a mixture in which ferroelectric ceramic particles are dispersed in a polymer matrix. The properties are largely determined by the choice of components, their relative composition, and the manner in which they are interconnected. The composites made by mixing PZT ceramic, PVDF polymer, and fluorinated rubber have a good piezoelectric coefficient, depending on the composition.133 Ceramic–polymer composites have been developed mainly to search for a suitable combination that can be adapted for piezoelectric or pyroelectric devices to be used in stringent environments, such as sonar devices in water, sensors for medical diagnostics, etc. 4.3.4 Applications of Piezoelectrics Both the direct and converse piezoelectric effects can be used for many practical applications, such as highvoltage generators, cigarette lighters, gas igniters, etc.; transducers for highintensity ultrasounds employed in ultrasonic cleaning, ultrasonic therapy, medical diagnosis, delay lines, etc.; resonators for filters and oscillators; microphones; various sensors; etc. The following sections use four simple and typical examples to demonstrate the importance of piezoelectric effects.
Force
– Spark Gap
P
+
P
–
Force Figure 443 Schematic diagram illustrating the principle of a gas igniter.
gradually would leak away through the leakage across the electrode, instead of building up to generate a high voltage across the spark gap. This is why igniters are of the momentary impact type rather than the slow squeeze type. Since most igniters have two pieces of poled ceramic elements connected back to back, we need consider only one for our analysis. Based on Equation 471, the voltage developed across the ceramic element when an impact force is applied is given by V = Fl = g33lX = g33l
Gas Igniters A schematic diagram of a poled piezoelectric ceramic igniter is shown in Figure 443, which is selfexplanatory. The principle is simple. When a force is applied to the poled ceramic, a voltage will be generated between electrodes. It is usual to use two pieces of poled ceramic elements connected back to back in order to double the charges released for the spark. On releasing the force, a voltage of about the same magnitude, but of the opposite sign, will be produced, yielding another spark across the gas gap. If the force were applied too slowly, no spark would occur because the charges released
Electrodes +
F A
(497)
where F is the force and and A are, respectively, the length and the area of the ceramic element. Ignoring all possible losses in the operation, the energy that may be dissipated in the spark is W=
1 A F 2 1 F 2l e 33 ÊË g33l ˆ¯ = d33 g33 2 l A 2 A
(498) If two elements are connected back to back (in fact, they are connected in parallel), the total energy available for the spark is two times that shown in Equation 498. PZT and PLZT are commonly used for gas igniters.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
Delay Lines The transmission of a microwave signal can be delayed by the following steps: 1.
2.
3.
The microwave signal is guided through a coupling network to a piezoelectric transducer, which converts it to an acoustic wave. This acoustic wave then propagates in a dielectric medium and reflects when it reaches the end. This reflected acoustic wave will be converted back to the original microwave signal by the transducer, as shown in Figure 444.
The major advantage of this type of delay line is the use of the transducer to convert the highspeed microwave signal to a lowspeed acoustic wave, and of the dielectric medium to produce the time delay. Since the speed of an acoustic wave is about 105 times slower than an electromagnetic wave, this type of delay line can be made much smaller in size and weight than a conventional one.134 However, for the design of such delay lines, it is important to consider the following factors: • The dielectric medium must have a low acoustic attenuation for the acoustic wave to propagate. • The transducer must have a high electromechanical coupling factor k and a high longitudinal mode acoustic wave velocity for its use at microwave frequencies. • The acoustic impedance matching between the dielectric medium and the transducer must be good, and the insertion loss must be low.
Piezoelectric Positioners and Actuators Piezoelectric positioners and actuators have been used widely in areas related to precision position controlling, vibration damping, relays, phonograph pickup, pressure sensing, etc.135–137 The basic principle is simple. A thin piezoelectric plate with metallic electrodes deposited on both surfaces can be used as a mechanical positioner or relay when the required movements are very small (e.g., a few micrometers or less). Figure 445 shows schematically a poled rectangular piezoelectric plate with the following dimensions: length a, width b, and thickness c, which are in the x, y, and z directions, respectively. When a DC voltage V is applied across the thickness in the z direction (which is also the poled direction), then the plate will expand or contract in the z direction, and contract or expand in the x and y directions, depending on the polarity of the voltage with respect to the poled direction. The magnitude of such movements can be easily calculated. From Equation 470, we can write
a c
V
P
Microwave Input
d
Acoustic Wave
c
a Microwave Output Figure 444 The structure of a microwave delay line; a: electrode A, b: electrode B, c: transducer, and d: dielectric medium.
b z
y x
(a) V>0
b
267
Dc /2
V=0 V<0
Da /2
(b) Figure 445 Schematic illustration of the deformation of a poled piezoelectric plate under an electric field: (a) the original shape of the plate at V = 0 and (b) the deformation at V > 0 and V < 0. (The deformation is exaggerated for clarity.)
268
Dielectric Phenomena in Solids
d33 =
h Dc c Dc = = F V c V
(499)
or
V
P P
Dc = d33V
This indicates that the change in thickness (i.e., the movement) depends on the piezoelectric coefficient d33 and the applied voltage V, but is independent of the thickness. For movements in the direction normal to the poled direction (for example, in the x direction), we have h Da a Ê c ˆ Da = = F V c Ë a¯ V a Da = Ê ˆ d31V Ë c¯
c
a
d31 =
(4100)
It can be seen that in this case, a can be made much larger than c if a >> c. For a very small adjustment in the position, we may use a small and more precise movement in the direction parallel to the poled direction. But for a larger movement, such as for relays, sideways movement in the direction normal to the poled direction may be preferable. Elastic compliance can be greatly increased by using long, thin piezoelectric strips or plates and mounting them as cantilevers. Bending such a strip or plate causes one half to stretch and the other half to compress, so there can be no net electrical response. However, if there are two such strips or plates with an intervening electrode and electrodes on outer surfaces to form a bimorph, as shown in Figure 446, then the bending will generate a voltage between the outer electrodes. By the converse piezoelectric effect, a bimorph will bend when a voltage is applied between the outer electrodes. The ∂h bending is governed by d ¢ = Ê ˆ (see EquaË ∂F ¯ tion 476). The applied field will also produce uniform strains along the length of the bimorph so that it will be in the form of a circular arc. Detailed analysis of the behavior of the bimorph under static conditions has been done by several investigators.138,139 The reflection at the free end of the bimorph cantilever is given by
V=0
DH V > 0 (+) Figure 446 Schematic illustration of the bending of a bimorph cantileverpiezoelectric actuator. (The bending magnitude is highly exaggerated for clarity.)
DH =
3 Ê a2 ˆ d31V 2 Ë c2 ¯
(4101)
In this case, DH is proportional to (a/c)2. This is why bending actuators are widely used for the applications requiring large movements, because they provide the largest movement (deflections) for a given applied voltage. It should be noted that bending bimorphs are not suitable for some applications because they have high mechanical inertia and cannot produce significant forces. Piezoelectric Transformers A transformer can be formed simply by a piezoelectric plate with electrodes deposited on half of its two flat surfaces and an electrode on the edge of the plate, as shown in Figure 447(a). One half of the plate is poled in the direction perpendicular to the surfaces, and the other half is poled in the direction parallel to the surfaces. The operation requires the application of an alternating voltage, like the conventional transformer, at a frequency that can excite a lengthmode resonance. In the first half of the plate, the input electrical energy through the input terminal is converted into mechanical energy, which results in oscillatory vibration. This mechanical energy is then converted back to electrical energy and picked up at the output
Ferroelectrics, Piezoelectrics, and Pyroelectrics
269
P
V input V output
P
(a) Stress Distribution
Halfwave Supporting Point
Supporting Points
Full Wave
(b) Figure 447 (a) Schematic illustration of a piezoelectric transformer and (b) the half and fullwave resonances.
terminal. It is important that the length of the plate be equal to a number of halfwavelengths of the acoustic wave to allow standing waves to form. In short, the mechanical oscillations in the first part are transmitted at resonance to the second part, which reconverts the mechanical energy into electrical energy, resulting in the generation of a higher voltage. The resonant frequency is determined by the acoustic velocity v in the piezoelectric material. If the total length of the transformer is 2, then for the transformer length equal to one full wavelength, the full wave resonant frequency is f =
v 2l
(4102)
For the transformer length equal to a halfwavelength, the halfwave resonant frequency is f =
v 4l
(4103)
Figure 447(b) shows that halfwave and the fullwave resonance. Since the operation of the transformer is based mainly on the resonance conditions, the location of the supporting points in the installation of such transformers is very important. In general, supporting points must be located at places where the oscillatory vibration is zero, as shown in Figure 447(b).
Based on the equivalent circuit shown in Figure 440, when the resonance occurs, the reactance due to Lm and Cm falls to zero and the overall impedance becomes very small if Rm is small. So the piezoelectric material can be used for wave filters to allow only a selected frequency band close to the resonance frequency to pass and to stop waves of other frequencies. The efficiency of such wave filters depends on the value of the electromechanical coupling factor k.
4.4
Pyroelectric Phenomena
Of 20 noncentrosymmetric crystal classes, 10 contain a unique polar axis under the unstrained condition. This implies that such crystals are already spontaneously polarized in a certain temperature range. Thus, they exhibit both piezoelectric and pyroelectric effects. For the latter, the crystal will develop free electric charges at the surfaces when uniformly heated because the polarization inside the crystal is changed by the heat. It should be noted that if a crystal specimen is heated nonuniformly (for example, with a temperature gradient along the specimen), then the temperature gradient will also develop a mechanical stress. So in this
270
Dielectric Phenomena in Solids
case, the specimen may have mixed piezoelectric and pyroelectric effects. However, under a uniform heating condition (i.e., a hydrostatic condition), the resultant piezoelectric effect vanishes. Since pyroelectricity results mainly from the temperature dependence of the spontaneous polarization of the polar materials, it occurs in ferroelectric materials whether they are singledomain crystals or poled ceramics. A change in temperature will cause a corresponding change in polarization and hence a change in the compensating charges on the metallic electrodes deposited on its surfaces. This change will produce a current in an external circuit. If the pyroelectric specimen is not connected to an external circuit and kept perfectly insulated from its surroundings, the surface charges on the electrodes released due to a change in temperature will flow inside the material through the intrinsic electrical conductivity of the material s, but it may take e/s time for the released charges to be neutralized. 4.4.1 Phenomenological Approach to Pyroelectric Effects The interactions between electrical and thermal variables are the direct concern of this section. A change in a crystal’s temperature can produce a number of electrical effects, which are referred to as pyroelectricity. These effects depend upon the thermal, mechanical, and electrical constraints on the crystal. The relation between D and T defines the pyroelectric coefficient (see Figure 438, the dashed line joining circle D and circle T ) or dD = p X dT dD pX = dT
circuited. However, a change in temperature will cause a change in the resultant dipole moment of all dipoles and hence a change in the spontaneous polarization. The surface charges will redistribute themselves to compensate for the new internal polarization, thus producing a flow of charges when the specimen is shortcircuited. Since D = e o F + Ptotal = e o F + ( Pinduced + Ps )
(4105)
where Pinduced and Ps are, respectively, the fieldinduced polarization and the spontaneous polarization. Pinduced is much smaller than Ps and less temperature dependent. So pX can be expressed as pX =
∂ Ps ∂T
(4106) X ,F
The pyroelectric coefficient under the condition of constant mechanical stress implies that the crystal is not clamped, that is, it is free to expand or contract thermally. Based on the relations between F, D, X, and T shown in Figure 438, we can write dh = y F ,T dX + d T dF + a F dT 123 123 123 Elasticity Thermal expansion Converse Piezoelectricity
(4107)
dD = d T ( dX ) + e X ,T dF + p X dT 123 123 123
Direct Pyroelectricity Piezoelectricity Permittivity
(4108) (4104)
The unit of p is coulomb m2K1. Pyroelectricity occurs only when the material exhibits spontaneous polarization. If the temperature of the specimen remains constant for a sufficient length of time, the charges accumulated on the surfaces will compensate for the internal polarization, so there will be no charge flow between the surfaces when they are short
where y, d, e, a, and p are, respectively, elastic compliance, piezoelectric coefficient, permittivity, thermal expansion coefficient, and pyroelectric coefficient. These equations should be written in tensor form, like those for piezoelectric effects, with subscripts to denote the direction and rotation of the vectors. For simplicity, we will ignore the complicated mathematical expressions and emphasize the physical concepts of the equations.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
Under the constraint condition of constant electrical field (i.e., dF = 0), from Equations 4–107 and 4–108, we obtain dX =
dh aF  F ,T dT F ,T y y
dD p X = T  T dT d d
(4109)
Under the condition of constant strain, dh = 0. This implies that the crystal is rigidly clamped, so expansion or contraction is not possible. Thus, from Equation 4109, we obtain pX =
∂D d Ta F + F ,T ∂T h y
= ph +
dTdF y F ,T
(4110)
Equation 4110 indicates that the total pyroelectric coefficient at constant stress pX consists of two components: • The pyroelectric coefficient at constant strain ph due to the primary pyroelectric effect • The secondary pyroelectric effect, which may occur when the crystal is free to react As shown in Figure 41, all pyroelectric materials are piezoelectric, but not all piezoelectric materials are pyroelectric, because the latter requires spontaneous polarization for its occurrence. For example, aquartz possesses three twofold axes, so a stress applied along any of these axes would cause a piezoelectric effect. But with heating, the material will expand equally along each of these axes. The angle between two adjacent axes is 120 degrees, so the pyroelectric effects tend to cancel each other. Hence, aquartz is not pyroelectric. Similarly, zinc blend ZnS (zinc sulfide) possesses four threefold axes and hence is piezoelectric and not pyroelectric. On the other hand, the hexagonal zinc sulfide or cadmium sulfide with a wurtzitetype structure possesses one sixfold axis, so it is piezoelectric and also pyroelectric. In general, pyroelectric materials also exhibit the piezoelectric effect under hydrostatic pressure, and pyroelectric materials have secondary pyroelectric and piezoelectric effects.
271
It should be noted that, theoretically, all ferroelectric materials are pyroelectric, but for applications only those with the secondorder transition at the Curie point are usable. From the Ps  T characteristics shown in Figure 49 it can be seen that the pyroelectric coefficient is high just below the Curie point for the case with a secondorder transition because dPs /dT is large. For example, TGS exhibits a secondorder transition and has a high pyroelectric coefficient just below the Curie point. The materials exhibiting a steep firstorder transition at the Curie point are not suitable for pyroelectric applications because they exhibit a thermal hysteresis and it is difficult in most applications to maintain a sufficiently constant temperature environment (see also Ferroelectric Phenomena in Chapter 4). The electrocaloric effect is the converse of the pyroelectric effect. The change of entropy can be expressed as dS = a F dX + p X dF +
1 dT Ty X , F
(4111)
Under the condition of constant entropy, which is an adiabatic process, dS = 0 and constant stress, dX = 0, then the electrocaloric coefficient qX can be written as qX =
dT dF
= Ty X , F p X
(4112)
S, X
The unit of qX is KmV1. 4.4.2 Pyroelectric Parameters and Their Measurements The major parameter is the pyroelectric coefficient pX since the electrocaloric coefficient is usually very small and scarcely used for the evaluation of pyroelectric effects. Several methods can be used for measuring pX. Here, we describe only two simple ones. One is the static method. In this method, the pyroelectric specimen is heated in a constant temperature chamber in which the temperature can be varied. Figure 448 shows the arrangement for measuring the charges developed on the pyroelectric specimen. These charges are then compensated by static charges induced on
272
Dielectric Phenomena in Solids
Pyroelectric Specimen
P
C
Electrometer
Adjustable Temperature Chamber Figure 448 Schematic diagram illustrating the static method for the measurement of pyroelectric coefficient p. For the dynamic method, capacitor C is replaced by a resistor R.
capacitor C, which can be measured simply by an electrometer. Based on Equation 4104, pX can be evaluated by pX =
Q2  Q1 A(T2  T1 )
(4113)
where Q2 and Q1 are the charges measured at temperatures T2 and T1, respectively, and A is the surface area of the specimen. The other method is the dynamic method. In this method, we can use the same arrangement shown in Figure 448 but with capacitor C replaced by a resistor R. In this case, the specimen is heated at a uniform rate of temperature rise, and it generates a current flowing through R measured also by an electrometer. We can write i=
dQ dD dD dT dT =A =A = Ap X dt dt dt dT dt
Thus, pX =
i A( dT dt )
(4114)
where i is the current and dT/dt is the rate of temperature rise. 4.4.3 Pyroelectric and Thermally Sensitive Materials Similar to piezoelectric materials, the most important pyroelectric materials are ceramics, synthetic polymers, and ceramic–polymer composites. In general, there are two types of pyro
electric materials: one is ferroelectric, and the other is not ferroelectric but possesses spontaneous polarization, which may not be reversed when the electric field is reversed. For poled specimens, the remanent polarization is temperature dependent and falls to zero as the Curie temperature is approached. This Ps  T relation below Tc is the cause of the pyroelectric effect. However, ferroelectric materials with the secondorder transition at Tc generally have higher pyroelectric coefficients than nonferroelectric ones, particularly at temperatures just below Tc. Table 45 lists the important parameters of some commonly used pyroelectric materials. The selection of pyroelectric materials for a special application should not be based solely on the figure of merit (see Equation 4138); other properties, such as chemical stability, mechanical strength, power handling ability, and fabrication processes, should also be considered. For example, triglycine sulfate (TGS) has a high figure of merit and is therefore a commonly used material for lowpower detection applications, but, it has its inherent shortcomings. It cannot be subjected to high heat—even sunlight may make it hot enough to depole. It is also mechanically weak and hygroscopic. However, the incorporation of alanine dopants into TGS greatly reduces its dielectric loss and dielectric constant, improving its performance as a radiation detector.140,141 Anyhow, this material is not suitable for devices to be used in an environment involving high vacuum or high humidity. Other materials with better mechanical strength and chemical stability than TGS, such as LiTaO3 and SBN, have already been used widely for pyroelectric devices. They are also insensitive to humidity. Lead zirconate (PZ)–based ceramics, such as PZT and PLZT, have a high value of pyroelectric coefficient and also of dielectric constant. It has been found that PZ doped with Fe, Nb, Ti, and U, such as Pb1.02(Zr0.58Fe0.20Nb0.20Ti0.02)0.994 U0.006O3 (PZFNTU), gives a higher pyroelectric coefficient and a lower dielectric constant.142 As mentioned earlier, pyroelectric polymers are now widely used for many applications
Ferroelectrics, Piezoelectrics, and Pyroelectrics
273
Table 45 Selected properties of some pyroelectric materials: p = pyroelectric coefficient at constant stress and electric field, and cp = heat capacity.
Material (Abbreviation)
Chemical Formula
p (C cm2K1)
cp (J cm3K1)
Temperature Range (K)
Triglycine sulfate (TGS)
(NH2CH2COOH)3•H2SO4
3.0 ¥ 108
1.70
273–321
Deuterated Triglycine Sulfate (DTGS)
(ND2CD2COOD3)•D2SO4
3.0 ¥ 10
8
2.40
243–334
Lithium Tantalate (LT)
LiTaO3
1.9 ¥ 108
3.19
273–891
8
2.34
248–303
Strontium Barium Niobate (SBN)
Sr0.6Ba0.4Nb2O6
8.5 ¥ 10
Lead Zirconate Titanate (PZT)
Pb(Zr0.52Ti0.48)O3
5.5 ¥ 108
2.60
298–523
8
2.57
—
Lanthanum Modified PZT (PLZT)
Composition Ratio: La/Zr/Ti = 6/80/20
7.6 ¥ 10
Barium Titanate
BaTiO3
3.3 ¥ 108
—
293–320
9
2.40
—
Polyvinyl Chloride (PVC)
see Table 52
0.4 ¥ 10
Polyvinyl Fluoride (PVF)
see Table 52
1.8 ¥ 109
2.40
—
see Table 52
9
2.40
—
Polyvinylidene Fluoride (PVDF or Kynar)
because of their ease of preparation in any shape and size. For example, polyvinyl fluoride (PVF) and polyvinylidene fluoride (PVDF) can be made extremely thin (< 2 mm). Although they have a low figure of merit, a low pyroelectric coefficient, and also a relatively high dielectric loss, they have a low heat conductivity and a low permittivity, facilitating both thermal and electrical coupling between neighboring elements. Their mechanical strength, thermal stability, and chemical stability are also good. Apart from pyroelectric materials, there are some materials whose resistivity is very sensitive to temperature based on other mechanisms and not pyroelectric effects. These materials are usually called negative temperature coefficient (NTC) materials, whose resistivity increases with decreasing temperature, or positive temperature coefficient (PTC) materials, whose resistivity increases with increasing temperature. Obviously, there are numerous applications of such materials with a high temperature coefficient of resistivity (TCR) in temperature indicators (e.g., thermometers), temperature
4.0 ¥ 10
controllers (e.g., thermostats, thermisters), currentlimiting devices, etc.
NTC Materials The most commonly used NTC materials are based on solid solutions of metallic oxides with a spinal structure, such as Fe3O4  ZnCr2O4 and Fe3O4  MgCr2O4, and also those based on Mn3O4 with partial replacement of Mn with Ni, Co, or Cu.96 On the basis of electrical conduction in semiconductors due to transport of charge carriers in the bands or hopping between localized states in the band gap, the temperature dependence of the resistivity follows the relation
r NTC (T ) = A exp
Ê Bˆ Ë kT ¯
(4115)
where k is the Boltzmann constant and A and B are constant. A is related to the resistivity at T Æ •, and B is the activation energy for the
274
Dielectric Phenomena in Solids
carrier movement. The negative TCR is a NTC =
1 dr NTC B = 2 r NTC dT kT
material increases with increasing temperature and reaches a peak at T > Tc, with the magnitude of several orders higher than that at Tc, as shown in Figure 449(a). This phenomenon is not observed in material with a single crystal structure. It occurs only in polycrystalline ceramics. Heywang144 has proposed that this phenomenon is caused by the Schottky barrier at the grain boundaries in polycrystalline structures. The energy band diagram near the grain boundary is shown in Figure 449(b). In the paraelectric phase, the band bending near the boundary is determined by the number of interface states Nint at the boundary. Similar to the Schottky barrier at the metal–semiconductor junction with the interface states at the metal–semiconductor interface, there is a
(4116)
PTC Materials The behavior of the DC electrical resistivity of ferroelectric ceramics is anomalous in the neighborhood of the Curie temperature TC. A typical example is BaTiO3 ceramic doped with 0.05 x 102 mol of Sn3+ or Nb3+. When the trivalent donor Sn3+ or Nb3+ substitutes for Ba2+, the extra positive charge in the material is compensated by an electron in the conduction band. The material behaves like a semiconductor, but electron mobility is also changed at the Curie temperature.143 As a result, the resistivity of the
Resistivity (ohmcm)
106
rmax
105 104 103 102
2rmin Tm
r25 10
rmin
1 0
Tmax
Tb
50
100
150
200
300
Temperature (°C)
Tmin
25
250
(a)
+ + +
+
+ Conduction Band + + + + + + +
+
+
Barrier Height f
+ +
+
+
+
+ + + + + + + Acceptor States
xd
Fermi Level Grain Boundary
(b) Figure 449 (a) The resistivity r as a function of temperature for BaTiO3 based PTC material and (b) the energy band diagram near a grain boundary of a polycrystalline material.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
depletion region xd and a barrier height f. Assuming that all donors are ionized, it can be shown that the barrier height is given by f=
q 2 N D xd2 2e re o
(4117)
where ND is the concentration of donors. The number of interface states at the boundary that accept electrons from the donors, acting as acceptorlike traps, must be Nint = NDxd. The barrier height depends on the size of grains because it affects the energy levels of the interface states.145 The resistivity of the ceramic material is determined by the magnitude of f. Thus, we can write Ê f ˆ r PTC • exp Ë kT ¯
(4118)
For temperatures T > Tc, the dielectric constant decreases with temperature following the Curie–Weiss relation (see Equation 41). So, from Equations 41, 4117, and 4118, we obtain B¢ Tc r PTC = A¢ exp ÈÍ Ê1  ˆ ˘˙ Î k Ë T ¯˚
(4119)
where A¢ and B¢ are constants related to doping concentration and structure of the material. It can be seen that for T > Tc the resistivity increases with increasing temperature. The TCR for this case is thus a PTC =
1 dr PTC B¢ Tc = r PTC dT k T2
(4120)
4.4.4 Applications of Pyroelectrics Pyroelectric materials respond to changes in temperature either by continuous heating or by the absorption of sinusoidally modulated radiation. Pyroelectric materials may be used for thermal detectors and calorimeters, but they do not respond to a temporally steady temperature or to radiation intensity. To obtain a response from a stationary temperature or radiation, it is necessary to make the heat or radiation periodically interrupted by a rotating chopper placed between the heat or radiation source and the pyroelectric element. Obviously, there are many applications of pyroelectric phenomena.
275
In the following sections, we discuss some typical cases as examples to illustrate the basic principles of pyroelectric devices. Pyroelectric Radiation Detectors Radiation detectors are mainly used for the detection of infrared radiation. A poled pyroelectric element is typically a thin plate of rectangular shape with metallic electrodes deposited on both surfaces. It is important that the element be very thin, so that it heats up quickly and uniformly, and that at least one of the electrodes is a good absorber of radiation, so that it can convert radiation energy to heat. Figure 450(a) shows schematically the basic arrangement for the detection of infrared radiation. Under a shortcircuit condition, there is a current flow due to the pyroelectricity, which is given by ip = pA
dT dt
(4121)
where p and A are, respectively, the pyroelectric coefficient and the area of the element. In the following discussion, the superscript x of pX is not shown for simplicity. The pyroelectric element behaves like a current generator with an internal resistance Ri and an internal capacitance Ci. The equivalent circuit to Figure 450(a) is shown in Figure 450(b). The detector also includes an amplifier represented by a shunt resistor Rd, a shunt capacitor Cd, and a voltmeter V. It is assumed that all incident infrared radiation energy is absorbed by the element in time dt and rapidly distributed throughout the whole volume of the element, so thermal diffusion can be ignored. The total power W incident to the element may be written as W = Wo + Wi exp( jw t )
(4122)
where Wo in the input power from the surrounding environment corresponding to temperature To, Wiexp (jwt) is the incident infrared power, and w is its frequency. When the element temperature is increased from To to T, part of the absorbed power will be lost to the surroundings by reradiation, conduction, or
276
Dielectric Phenomena in Solids
Incident Radiation
Measuring System Pyroelectric Axis
(a)
Current Generator ip = PAT
Ci
Ri
Rd
Pyroelectric Element
Cd
V
Measuring System
(b) Figure 450 (a) Experimental arrangement for infrared radiation detection and (b) the equivalent circuit of the radiation detector shown in (a).
convection at a rate of G per unit temperature rise in the element due to incident radiation. Thus, we can write the energy balance equation as dT hWi exp( jw t )  G(T  To ) = H dt
(4123)
dT + G(T  To ) = 0 dt
t T  To = (T1  To )expÊ  ˆ Ë tT ¯
(4125)
where tT is the thermal relaxation time, which is
where h is the fraction of the incident power that heats the element; H is the heat capacity of the element, which is equal to rcAL in which r is the density; c is the specific heat; and A and L are, respectively, the area and the thickness of the element. If the radiation is switched on at t = 0 and switched off at t = t1, then when t = t1, Wi = 0, Equation 4123 becomes H
Using the boundary condition (when t = 0, T = To and when t = t1, T = T1), the solution of Equation 4124 yields
(4124)
tT =
H G
(4126)
Assuming that the temperature of the element varies sinusoidally following the incident radiation frequency w, then the solution of Equation 4123 gives the continuous response of the pyroelectric element98,146 as follows: T  To = hWi (G 2 + w 2 H 2 )1 2 exp[ j(w t + q )]
(4127)
Ferroelectrics, Piezoelectrics, and Pyroelectrics
where q is the phase angle between the radiation and the temperature oscillation, which is given by
277
Ri Rd Ri + Rd
(4129)
From Equation 4127, T  To is independent of frequency for frequencies w << t T1 and decreases with increasing frequency for w >> t 1 T . From Equations 4132 and 4135, rv is maximal at the frequency w = (tTtE)1/2. Both ri and rv increase with increasing frequency for w < t T1 and decrease with increasing frequency for w > t 1 T .
CT = Ci + Cd
(4130)
The maximum value of rv occurs at w = (tTtE)1/2 and is given by
q = tan 1 (wH G)
(4128)
Based on the equivalent circuit shown in Figure 450(b), the total resistance RT and the capacitance CT are RT =
So the elementgenerated current ip due to the variation of temperature can be written as146,147 dT dV V = CT + dt dt RT w = hWi pAÊ ˆ [1 + w 2t T2 ]1 2 exp[ j(w t + q )] Ë G¯
ip = pA
(4131) The useful criteria for pyroelectric detectors are the current responsivity ri and the voltage responsivity rv, which are defined as follows: ri =
ip pAhw = (1 + w 2t T2 ) 1 2 Wi G
(4132)
From Equations 4129 and 4130, we can easily find the total admittance YT of the circuit. The voltage due to the change in temperature across Rd is given by V=
ip YT
= hWi pART
( wG )(1 + w t )
2 2 1 2 T
(1 + w 2t E2 ) 1 2
(4133) where tE is the electrical relaxation time, which is t E = RT CT
(4134)
Thus, the voltage responsivity can be expressed as rv =
V hpARTw = 2 2 12 Wi G(1 + w t T ) (1 + w 2t E2 )1 2
(4135) Assuming that the circuit parameters are independent of frequency, we can see the following features:
hpART G(t E + t T )
rv (max ) =
(4136)
For high frequencies, w2t T2 >> 1, w2t E2 >> 1 and Ci > Cd, so Equation. 4135 can be simplified to hpA wHCi hp = Awc pe
rv =
(4137)
where cp = rc. Since the sensitivity of the radiation detector increases with increasing rv, the p quantity in Equation 4137 may be used c pe as a figure of merit for the pyroelectric radiation detector Fv, which is Fv =
p c pe
(4138)
This is mainly a function of the material properties. In general, we would like the material to have a high pyroelectric coefficient and a low dielectric constant. However, all signal detectors encounter the effect of noise, which is always present in any detector circuit. So, the sensitivity of any detector is determined by the level of noise in the amplifier output signal. Therefore, the signaltonoise ratio must be made as large as possible. For pyroelectric detectors, the principal sources of noise are Johnson noise, thermal fluctuations, and amplifier noise. The noise level can also be described by the socalled noise equivalent power (NEP), which is defined as NEP =
DVN rv (Df )1 2
(4139)
278
Dielectric Phenomena in Solids
where DVN is a signal voltage equal to the noise voltage, produced by a necessary amount of power input to the detector, and Df is the bandwidth of the amplifier. It is often convenient to describe the minimum detective power of a detector by the socalled detectivity (D) which is defined as D=
1 NEP
(4140)
Pyroelectric Burglar Alarm Systems A blackbody at 300 K would radiate infrared rays of about 9.8 mm in wavelength. Human or animal bodies whose temperature is around 310 K are expected to generate infrared radiation of about 10 mm in wavelength. Thus, a moving intruder produces variable infrared radiation which, when reaching a pyroelectric detector, will switch on the alarm system. Figure 451 shows the arrangement of the pyroelectric elements and the alarm system. Since pyroelectric materials are also piezoelectric, they would produce electric charges due to external mechanical stresses caused by the expansion or contraction when the ambient temperature of the surroundings rises or falls. These stressinduced charges may interfere with the response of the active pyroelectric element to radiation. To prevent this interference, we need a dummy compensating element similar to the active element, but which does not respond to infrared radiation because the electrode facing the radiation is a reflecting electrode. The con
nection of this compensating element and the active element is back to back, so the response of the compensating element to the ambient temperature fluctuation will cancel that of the active element. In general, such compensation is essential for many applications. The basic principle is the same as that described in the previous section. The output voltage of the system is to switch on the alarm system. Pyroelectric Thermometry In contrast to radiation detectors, pyroelectric thermometers receive energy through conduction or convection. As a result, noise due to thermal fluctuations is low. The principle is simple.148,149 Based on the equivalent circuit shown in Figure 450, Equation 4131 can be rewritten as pA
P Compensating Element
(4141)
This equation indicates that pyroelectric thermometers can be used to measure the rate of temperature changes or the steps of steady temperature changes. Measuring the Rate of Temperature Changes
In this case, the electrical relaxation time must be small (i.e., tE = RTCT << 1), so the first term on the right side of Equation 4141 can be neglected. Thus, we have
Incident Radiation
Reflecting Electrode
dT dV V = CT + dt dt RT
Absorbing Electrode
dT V = dt pART
(4142)
FET
Rd
Alarm Unit
P Detecting Element
Figure 451 Schematic diagram of a pyroelectric burglar system alarm consisting of an active detecting element, a compensating (dummy) element, and an alarm unit.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
The thermometer directly measures the rate of temperature changes by measuring the voltage across the pyroelectric element. Measuring Steady Temperature Changes
In this case, the electrical relaxation time must be large (i.e., tE = RTCT >> 1), so the second term on the right side of Equation 4141 can be neglected. Thus, we have pA dT dV = CT dt dt
(4143)
Integrating Equation 4143 with the initial condition, V(0) = Vo and T(0) = To, we obtain T  To = (V  Vo )
CT pA
(4144)
The thermometer measures the steady temperature changes in steps by measuring V at T and Vo at To. For more about the limitations of this method and the factors involved in temperature measurements, see references 146–149. Pyroelectric Energy Conversion Thermal energy input to a pyroelectric element will cause changes in the spontaneous polarization and hence generate electric charges on the electrodes. If a load is connected between the electrodes, a current will flow through the load, and electrical energy will be consumed there. The energy conversion efficiency is defined as Electrical energy output Thermal energy input ipV = Wi = Wi rr i v
y=
(4145)
From Equations 4132 and 4135, y can be written as y=
Wi p2 RT (wt T )2 c L (1 + w 2t T2 )(1 + w 2t E2 )1 2 2 2 p
(4146)
When Ri << Rd, Ci >> Cd, Ci = eA/L and s = L/ARi = we¢, we obtain the internal energy conversion efficiency of the pyroelectric element as
y in =
279
p2 Ê Wi ˆ c (1 + w t )(e 2 + e ¢ 2 )wL Ë A ¯ 2 2 T
2 p
(4147) yin becomes a maximum for wtT = 1. Using the average temperature change given by Equation 4127, DT = T  To = Wi /cp A, we have y in =
p 2 DT 2(e + e 2 )cP 2
(4148)
In practice, e >> e1. So, we may consider p2/cpe as the figure of merit for energy conversion of pyroelectric materials. For typical values of tT = 1 s and Wi = 100 mW cm2 and the temperature change DT = T  To = 50°C, the internal conversion efficiency is yin 103. It has been found that p2/cpe does not vary much for most pyroelectric materials.98,150 So it is unlikely that the energy conversion efficiency would greatly exceed 103 under practical conditions, based on pyroelectric effects.
References 1. J. Valasek, Phys. Rev., 17, 475 (1921). 2. J. Valasek, Phys. Rev., 19, 478 (1922). 3. J. Valasek, Phys. Rev., 24., 560 (1924). 4. W.G. Cady, Piezoelectricity, (Dover, New York, 1964). 5. J. Curie and P. Curie, Compt. Rend., 91, 294 (1880) and 95, 1137 (1881). 6. Bunget and M. Popesco, Physics of Solid Dielectrics, (Elsevier, Amsterdam 1984), p. 383. 7. M. Born and K. Huang, Dynamical Theory of Crystal Lattices, (Clarendon, Oxford, 1954). 8. J.F. Nye, Physical Properties of Crystals, (Oxford University Press, Oxford, 1960). 9. C.S. Smith, “Macroscopic Symmetry and Properties of Crystals,” in Solid State Physics, Edited by F. Seitz and D. Turnbull, Vol. 6 (Academic Press, New York, 1958), p. 175. 10. K.R. Brain, Proc. Phys. Soc., 36, 81 (1924). 11. E.L. Kern and S.M. Skinner, J. Appl. Polym. Sci., 6, 404 (1962). 12. S.N. Levine, J. Appl. Polym. Sci., 9, 3351 (1965). 13. G.E. Hauver, J. Appl. Phys., 36, 2113 (1965). 14. E. Fukada, M. Date, and N. Hirai, Nature, 211, 1079 (1966).
280
15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38.
39. 40. 41. 42. 43.
Dielectric Phenomena in Solids
H. Kawai, Jpn. J. Appl. Phys., 8, 975 (1969). C.B. Sawyer and C.H. Tower, Phys., Rev., 35, 269 (1930). W.J. Merz, Phys. Rev., 76, 1221 (1949) W.J. Merz, Phys. Rev., 91, 513 (1953). E.J. Huibregtse and D.R. Young, Phys. Rev., 103, 1705 (1956). A.F. Davenshire, Phil. Mag., 42, 1065 (1951). H.H. Weider, Phys. Rev., 99, 1161 (1955), and J. Appl. Phys., 26, 1479 (1955). W.J. Merz, Phys. Rev., 95, 690 (1954). R. Landauer, D.R. Young, and M.E. Drougard, J. Appl. Phys., 27, 752 (1956). H.H. Weider, J. Appl. Phys., 28, 367 (1957). D.S. Campbell, J. Electronics and Control, 3, 330 (1957). W. J. Merz, J. Appl. Phys., 27, 938 (1956). V. Janovec, Czechoslov. J. Phys., 8, 3 (1956). W.J. Merz and J.R. Anderson, Bell Lab. Record, 33, 335 (1955). J.R. Anderson, G.W. Brady, W.J. Merz, and J.P. Rameika, J. Appl. Phys., 26, 1387 (1955). E. Fatuzzo and W.J. Merz, Ferroelectricity, (NorthHolland, Amsterdam, 1967). A.G. Chynoweth, Phys. Rev., 110, 1316 (1958). R.C. Miller, Phys. Rev., 111, 736 (1958). V.M. Rudyak, A.Y. Kudzin, and T.V. Panchenko, Sov. Phys.—Solid State, 14, 2112 (1973). G.F. Bacon and R.S. Pease, Proc. Royal Soc. London, A220, 397 (1953) and A230, 359 (1955). M. Tokunaga, Ferroelectrics, 1, 195 (1970). G. Busch, J. Helv. Phys. Acta, 11, 269 (1938). A. Von Arx and W. Bantle, J. Helv. Phys. Acta, 17, 298 (1944). W. Kanzig, “Ferroelectrics and Antiferroelectrics,” in Solid State Physics edited by F. Seitz and D. Turnbull, Vol. 4 (Academic Press, New York 1957) pp. 1–197. F. Jone and G. Shirane, Ferroelectric Crystals, (MacMillan, New York, 1962). H.M. Barkla and D.M. Finlayson, Phil. Mag., 44, 109 (1953). V.L. Hablutzel, J. Helv. Phys. Acta, 12, 489 (1939). A.N. Holden and W.P. Mason, Phys. Rev., 57, 54 (1940). S. Hoshino, T. Mitsui, F. Jona, and R. Repinsky, Phys. Rev., 107, 1255 (1957).
44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54. 55. 56. 57. 58. 59. 60. 61. 62. 63.
64. 65. 66. 67. 68. 69.
B. Jaffe, W.R. Cook, and H. Jaffe, Piezoelectric Ceramics, (Academic Press, New York, 1971). H.M. Barnett, J. Appl. Phys., 33, 1606 (1962). C. Michel, J.M. Moreau, G.D. Achenbach, R. Gerson, and W.J. James, Solid State Commun., 7, 865 (1969). E. Sawaguchi, J. Phys. Soc. Japan, 8, 615 (1953). S. Roberts, J. Am. Ceram. Soc., 33, 63 (1956), and Phys. Rev., 83, 1078 (1951). G. Shirane, E. Sawaguchi, and Y. Takagi, Phys. Rev., 84, 476 (1951). E. Sawaguchi and K. Kittaka, J. Phys. Soc. Japan, 7, 336 (1952). R. Redin, G. Marks, and C. Antoniak, J. Appl. Phys., 34, 600 (1963). G. Jonker, J. Am. Ceram. Soc., 55, 57 (1972). H. Jaffe and D. Berlincourt, Proc. IEEE., 53, 1372 (1965). K. Hardti, Ferroelectrics, 12, 9 (1976). L. Benguigui, Solid State Commun., 11, 825 (1972). K. Okazaki, Ferroelectrics, 35, 173 (1981). P. Thatcher, Appl. Opt., 16, 3210 (1977). R.C. Buchanan (Ed.), Ceramic Materials for Electronics, (Marcel Dekker, New York, 1986). L.M. Levinson, Electronic Ceramics, (Marcel Dekker, New York, 1988). G.H. Hacetling and C.E. Land, J. Am. Ceram. Soc., 54, 1 (1971). R.H. Dungan, H.M. Barnett, and A.H. Stark, J. Am. Ceram. Soc., 45, 226 (1962). Y.L. Wang, W.Z. Yuan, G.H. He, S.W. Lin, Y.H. Ling, C.F. Qu, and B.G. Wang, Ferroelectrics, 49, 169 (1983). Y.L. Wang and K.C. Kao, in Conference Record of the 2000 IEEE International Symposium on Electrical Insulation (IEEEDEIS, New York, 2000) pp. 58– 61. W.M. Prest, Jr. and D.J. Luca, J. Appl. Phys., 46, 4136 (1975). R. Hasegawa, Y. Takahashi, Y. Chatani, and H. Tadokoro, Polym. J., 3, 600 (1972). M.A. Bachmann and J.B. Lando, Macromolecules, 14, 40 (1981). A.J. Lovinger, Science, 220, 1115 (1983). J. Scheinbeim, C. Nakafukus, B.A. Newman, and K.D. Pae, J. Appl. Phys., 50, 4399 (1979). A.J. Lovinger, in Developments in Crystalline Physics, Vol. 1, edited by D.C. Bassett (Applied Sciences, London, 1982) Chapter 5.
Ferroelectrics, Piezoelectrics, and Pyroelectrics
70. 71. 72. 73. 74. 75.
76. 77. 78.
79. 80. 81. 82. 83. 84. 85. 86. 87. 88. 89. 90. 91. 92. 93.
T. Takahashi, M. Date, and E. Fukada, Appl. Phys. Lett., 37, 791 (1980). A.J. Lovinger, G.T. Davis, T. Furukawa, and M.G. Broadhurst, Macromolecules, 15, 323 and 329 (1982). J.G. Bergman, Jr., J.H. McFee, and G.R. Crane, Appl, Phys. Lett., 18, 203 (1971). A.F. Devonshire, Quarterly Supplement of Phil. Mag., Advances in Physics, 3, 85 (1954). E.J. Huibregtse and D.R. Young, Phys. Rev., 103, 1705 (1956). D. Meyerhofer, Technical Report 121, Laboratory for Insulation Research, Massachusetts Institute of Technology, 1957; also Phys. Rev., 112, 413 (1958). C. Kittel, Phys. Rev., 82, 729 (1951). L.E. Cross and B.J. Nicholson, Phil. Mag., 46, 453 (1955). P.W. Forsbergh, “Piezoelectricity, Electrostriction and Ferroelectricity” in Handbuch der Physik, Vol. 17, (SpringerVerlag, Berlin, 1956) pp. 264–392. G.J. Goldsmith and J.G. White, J. Chem. Phys., 31, 1175 (1959). H.L. Stadler and P.J. Zachmanidis, J. Appl. Phys., 34, 3255 (1963). E.A. Little, Phys. Rev., 98, 978 (1955). J.C. Burfoot, Ferroelectrics: An Introduction to the Physical Principles, (Van Nostrand, Princeton, 1967). J.A. Hooton and W.J. Merz, Phys. Rev., 98, 409 (1955). R.C. Miller and A. Savage, Phys. Rev., 112, 755 (1958); Phys. Rev. Lett., 2, 294 (1959); also J. Appl. Phys. 30, 808 (1959). R.C. Miller and G. Weinreich, Phys. Rev., 117, 1460 (1960). M. Hayashi, J. Phys. Soc. Japan, 33, 617 and 739 (1972). M. McQuarrie, Bull. Am. Ceram. Soc. 34, 170 (1955). G. Shirane and K. Sukuzi, J. Phys. Soc. Japan 7, 333 (1952). A. Glanc, V. Dvorak, V. Janovec, E. Rechziggel and V. Janouser, Phys. Lett. 7, 106 (1966). A.E. Feuersanger, in Thin Film Dielectrics, edited by F. Vratny (Electrochemical Society, New York, 1969), p. 209. Y.Y. Tomashpolski, M.A. Sevostianov, M.V. Pentagova, L.A. Sorokina, and Y.N. Venevstsev, Ferroelectrics 7, 257 (1974). J.R. Slack and J.C. Burfoot, J. Phys. C. Solid State, 4, 898 (1971). J.L. Vossen and W. Kern (Eds.) Thin Film Processes, (Academic Press, New York, 1978).
94. 95.
96.
97. 98.
99. 100. 101. 102.
103. 104. 105. 106. 107. 108. 109. 110. 111. 112. 113. 114. 115.
281
K. Lichtenecker, Phys. Z. 10, 1005 (1909) and 27, 115 (1926). K.W. Plessner and R. West “High Permittivity Ceramics for Capacitors,” in Progress in Dielectrics, Vol. 2, edited by J.B. Birks and J.H. Schulman (Heywood, London, 1960) pp. 165–192. A.J. Moulson and J.M. Herbert Electroceramics: Materials, Properties and Applications, (Chapman and Hall, London, 1997). J.M. Herbert, Ceramic Dielectrics and Capacitors, (Gordon and Breach, London, 1985). M.E. Lines and A.M. Glass, Principles and Applications of Ferroelectrics and Related Materials, (Clarendon, Oxford, 1977). S. Nomura and S. Sawada, J. Phys. Soc. Japan 6, 36 (1951); also ibid., 10, 108 (1955). A. Glanc, Z. Malek, J. Mastner, M. Novak, and J. Strajblova, J. Appl. Phys. 35, 1870 and 1875 (1964). J. Fousek, J. Appl. Phys. 36, 588 (1968). R. Koontz, G. Blookhina, S. Gold and A. Krasnykh, Annual Report of 1998 Conference On Electrical Insulation and Dielectric Phenomena (IEEE Publication 98CH362571, New York) pp. 23–26. F.W. Neilson, Bull. Am. Phys. Soc., 2, 302 (1957). P.C. Lysne and C.M. Percival, J. Appl. Phys., 46, 1519 (1975). W. Mock and W.H. Holt, J. Appl. Phys., 49, 5846 (1978). J.R. Anderson, Electrical Engineering, 71, 916 (1952). J.F. Scott and C.A. Araujo, Science, 246, 1400 (1989). J.F. Scott, C.A. Araujo, H.B. Meadows, L.D. McMillan, and A. Schawabkeh, J. Appl. Phys., 66, 1444 (1989). J.F. Scott, C.A. Araujo, and L.D. McMillan, Ferroelectrics, 116, 107 (1991). P.K. Larson, R. Cuppens, and C.A.C.N. Spierings, Ferroelectrics, 128, 265 (1992). L.K. Anderson, Ferroelectrics, 7, 55 (1974); also 3, 69 (1972). S.Y. Wu, W.J. Takel, and M.H. Francombe, Appl. Phys. Lett. 22, 26 (1973). S.A. Keneman, A. Miller, and G.W. Taylor, Ferroelectrics, 3, 131 (1972). P.P. Peercy and C. Land, IEEE Trans. Electron Devices, ED28, 756 (1981). W.P. Mason, Piezoelectric Crystals and their Applications in Ultrasonics, (Van Nostrand, New York, 1950).
282
Dielectric Phenomena in Solids
116. K.S. Van Dyke, Proc. IRE., 16, 742 (1928). 117. H.D. Megan, Ferroelectricy in Crystals, (Methuen, London, 1957). 118. D. Berlincourt, D. Curran, and H. Jaffee, in Physical Acoustics, edited by W.P. Mason (Academic Press, New York, 1964). 119. A.R. Von Hippel, Molecular Science and Molecular Engineering, (John Wiley, New York, 1959), p. 300. 120. J.M. Herbert, Ferroelectric Transducers and Sensors, (Gordon Breach, London, 1982). 121. J. Van Randeraat and R. Setterinoton (Eds.), Piezoelectric Ceramics, (Mullard, London, 1974). 122. G. Shirane, K. Suzuki, and A. Takada, J. Phys. Soc. Japan 7, 12 (1952). 123. G. Shirane and K. Suzuki, J. Phys. Soc. Japan 7, 333 (1952). 124. B. Jaffe, R. Roth, and J. Marzullo, J. Appl. Phys., 25, 809 (1954). 125. G. Haertling and C. Land, J. Am. Ceram. Soc., 54, 1 (1971). 126. S. Liu, S. Pai, and J. Kyonka, Ferroelectrics, 22, 689 (1978). 127. K. Hardti, Ferroelectrics, 12, 9 (1976). 128. K. Okazaki, Ferroelectrics, 35, 173 (1981). 129. M. Multani, S. Gokarn, R. Vijayaraghavan, and V. Polkar, Ferroelectrics, 37, 652 (1981). 130. N. Murayama, T. Oikawa, T. Katto, and K. Nakamura, J. Polym. Sci. Polym. Phys. Ed. 13, 1033 (1975). 131. N. Murayama and Hazhizume, J. Polym. Sci. Polym. Phys. Ed. 14, 989 (1976). 132. G. Pfister, M. Abkowtz, and R.G. Crystal, J. Appl. Phys. 44, 2064 (1973). 133. T. Furukawa, K. Ishida, and E. Fukada, J. Appl. Phys. 50, 4904 (1979).
134. 135. 136. 137. 138. 139. 140. 141. 142. 143. 144. 145. 146. 147. 148. 149.
150.
D. Liufu and K.C. Kao, J. Vac. Sci. Technol., A16, 2360 (1998). K. Uchino, Piezoelectric Actuators and Ultrasonic Motors, (Kluwer Academic, Boston, 1996). K. Uchino, Ferroelectrics, 91, 281 (1989). K. Uchino, “Ceramic Actuators: Principles and Applications,” (MRS Bulletin, April 1993), p. 42. J.G. Smith and W.S. Choi, IEEE Trans. Ultrason., Ferroelect., Freq. Contr. 38, 256 (1991). Q.M. Wang, X.H. Du, B.M. Xu, and L.E. Cross, IEEE Trans. Ultrason., Ferroelect., Freq. Contr. 46, 638 (1999). P.J. Lock, Appl. Phys. Lett. 19, 390 (1971). E.T. Keve, K.L. Bye, R.W. Whipps, and A.D. Annis, Ferroelectrics, 3, 39 (1971). R.W. Whatmore, Rep. Prog. Phys. 49, 1335 (1988). C.N. Berglund and W.S. Baer, Phys. Rev. 157, 358 (1967). H. Heywang, J. Mater, Sci. 6, 1214 (1971). N. Hirose and H. Sasaki, J. Am. Ceram. Soc. 54, 320 (1971). S.B. Lang, Sourcebook of Pyroelectricity, (Gordon and Breach, London, 1974). S.B. Lang and F. Steckel, Rev. Sci. Instru. 36, 1817 (1965). S.B. Lang, S.A. Shaw, L.H. Rice, and K.D. Timmerhaus, Rev. Sci. Instru. 40, 274 (1969). S.B. Lang, “Pyroelectricity: Its Phenomenology and Its Application to Temperature Measurements” in Heat Transfer, (Elsevier, Amsterdam, 1970), Section MT 1.6. J.D. Zook and S.T. Liu, Ferroelectrics, 11, 371 (1976).
5
Electrets The science of electricity is that state in which every part of it requires experimental investigation; not merely for the discovery of new effects, but the development of the means by which the old effects are produced, and the consequent more accurate determination of the first principles of action of the most extraordinary and universal power in nature. Without experiment, I am nothing. Michael Faraday
5.1
Introductory Remarks
Later, other types of electrets were discovered using special methods of creating real charges or polarization. In 1937, Nadjakov discovered photoelectrets.4,5 He found that charge separation occurred when a sulfur layer was subjected simultaneously to a visible light illumination and an electric field stressing. This photoelectric phenomenon later led to the development of xerography.6 This phenomenon was further studied by Kallmann et al.7,8 and Fridkin et al.9 There are many other ways to form electrets. For example, electroelectrets are produced by applying a strong electric field across the dielectric material between two metallic electrodes, causing polarization, injection of charge carriers, or both. Electrets formed by carrier injection can also be achieved by corona discharges or electron beams on the surface of the dielectric materials. Some kinds of electrets can be produced without the use of an electric field, such as magnetoelectrets produced by heating the dielectric material (e.g., polymethylmethacrylate) in a strong static magnetic field, and then cooling it slowly to the normal ambient temperature. This process makes the dielectric material become polarized due to the magnetic anisotropy of molecules, which tend to orient along with their dipole moments.10 Some electrets can be formed simply by a thermal process without involving either electric or magnetic fields. Such electrets are due mainly to charge separation through a phase transition on phase changes during solidification.11 Some electrets can be formed by applying a mechanical pressure to the dielectric material. In this case, surface charges can be
An electret can be considered a piece of dielectric material with the presence of quasipermanent real charges on the surface or in the bulk of the material, or frozenin aligned dipoles in the bulk. An electret behaves like a battery or acts as an electrical counterpart of a permanent magnet. A piece of poled ferroelectric material can also be an electret. The term quasipermanent implies that the amount of charges stored in the material does not remain the same permanently, but decays very slowly depending on the situation, and the decay time is normally much longer than the time period over which the electret is in use. In 1892, British scientist Oliver Heaviside was the first to introduce the term electret and to discuss its properties1. In 1919, Japanese scientist Mototaro Eguchi was the first to fabricate an electret by melting equal parts of Carnauba wax (extracted from the Brazilian Carnauba palm tree) and resin with a little beeswax and then lowering the temperature to allow the liquid mixture to become solidified while being subjected to an electric field of about 10 kV cm1.2,3 The internal polarization of the electret discs prepared by this method persisted for many years. In fact, electrets prepared by Eguchi’s method today are called the thermoelectrets, because they are formed mainly by a thermal process. Many materials can now be used to fabricate thermoelectrets, including organic materials such as ebonite, naphthalene, polymethylmethacrylate, and many polymers, and inorganic materials such as sulfur, quartz, glasses, steatite, and some ceramics. 283
284
Dielectric Phenomena in Solids
acquired simply by contact electrification, deformation, or friction without the application of an electric field.12 In this chapter, we shall discuss the formation of electrets and their related properties with emphasis on the basic physical concepts needed to identify important material parameters and to deduce guidelines for optimizing some desirable properties and predicting possible new applications.
5.2
Formation of Electrets
The electrical charges that can be created and stored in a dielectric material to form an electret have two major types: monocharges (also called real charges) and dipolar charges, which are in fact aligned dipoles and can be induced in dipolar materials containing dipolar molecules or in ferroelectric materials. Real charges may appear on the material surface, called surface charges, or in the bulk to form socalled space charges. Surface charges or space charges with the same polarity as that of the adjacent forming electrode are called homocharges, and those with the polarity opposite to that of the adjacent forming electrode are called heterocharges. Homocharges may appear as a result of charge carrier injection from the electrode into the dielectric material, followed by the capture of the injected carriers in traps near the injecting electrode. They may also appear due to the depositing of charge carriers resulting from the electric discharge in an air gap between the material surface and the forming electrode. Heterocharges are due mainly to the presence of aligned dipoles, to the displacement of the existing charge carriers (electrons or ions) in the material, or to the presence of residual impurities, which are apt to be ionized. Figure 51 depicts some common forms of electrets. In this section, we shall describe some of the most important methods for forming electrets. These methods are based mainly on the manner of charging or polarizing the dielectric material and on the structure of the material, whether it is dipolar or nondipolar.
5.2.1.
ThermoElectrical Method
Basically, this method is similar to the one originally used by Eguchi.3 It involves the simultaneous application of an electric field and heat to a dielectric material for a predetermined period of time and the subsequent cooling to normal ambient temperature while the electric field is still applied. Figure 52 shows three general electrode arrangements for forming thermoelectrets. One type has metallic electrodes vacuumdeposited on two surfaces of the dielectric material to form intimate contacts, as shown in Figure 52(a). Another type has only one surface with an intimate metallic contact; an air gap is between the other surface and a forming metallic electrode, as shown in Figure 52(b). A third type is without metallic contacts on both surfaces but with air gaps between the surfaces and the forming metallic electrodes, as shown in Figure 52(c). In the case with a dielectric material between two intimate metallic electrodes, the dipolar molecules (dipoles) are randomly arranged, as shown in Figure 53(a), but they will actively orient under an electric field and at an elevated temperature. In general, the temperature is higher than the glass transition temperature Tg, at which the material becomes very amorphous, homogeneous, and elastic, so the dipoles can orient easily in the direction of the applied field, as shown in Figure 53(b). After the poling period, the material is gradually cooled down to the normal ambient temperature To while the electric field is still applied. Finally, the applied electric field is removed and the material forms a thermoelectret consisting mainly of aligned dipolar charges, as shown in Figure 53(c). The temperatureapplied field time sequence for the poling process is shown in Figure 53(d), and the resulting polarization in Figure 53(e). After the removal of the applied field, the total polarization gradually decreases to a quasisteady level, which is mainly the remaining frozenin dipolar polarization associated with the difference in relative permittivity between Tg and To. At Tg the induced polariza
Electrets
285
Surface Monocharges –
– –
–
– –
–
– –
–
– –
–
– –
–
–
– –
– Space Monocharges
Metallic Electrode
+
+
+
+
+
+
+
+
Compensation Charges
– – – – – + – – – + – – – + – – – + + + – – – + + + – – – + + + + +
(a) Metallic Electrode
– + – + – + – –
Metallic Electrode
– + – + – + – +
Metallic Electrode
–
+
+
(d) Bound Charges
– + – + – + – +
–
–
–
–
–
–
–
+
+
+
+
+
+
+
Dipolar Charges Bound Charges
(b) Metallic Electrode
– –
– – – – – + – – – + – – – + – – – + + + – – – + + + – – – + + + + +
(e) – +
+ +
–
+
(c)
–
+ +
–
–
+ +
–
–
+ +
–
–
+ +
–
–
+ +
–
–
–
(f)
Figure 51 Schematic illustration of electrets involving (a) surface monocharges and space monocharges, (b) dipolar charges only, (c) dipolar charges and space monocharges, (d) surface monocharges, space monocharges, and dipolar charges, (e) deposited negative and positive surface charges, and (f) displacement of negative and positive real charges in the bulk.
tion is also a part of the total polarization under an electric field. As soon as the electric field is removed, the part due to induced polarization will gradually return to its randomized state. However, if the applied field is sufficiently high to cause carrier injection from the electrode to the dielectric material, but not high enough to cause internal discharge or breakdown, then the electret formed will consist of both frozenin aligned dipolar charges and injected space monocharges captured in traps, as shown in Figure 51(c). If the material is nondipolar, then we must produce real charge storage on the surface or in the bulk to form the electrets, as shown in
Figure 51(c) and (d). In doing so, we use the electrode arrangements with one or two air gaps, like those shown in Figure 52(b) and (c). When there is only one air gap, as shown in Figure 52(b), the system is basically a classical Maxwell–Wagner twolayer system. Assuming that the dielectric material is nonconductive with a relative permittivity er, then the electric field in the air gap Fo and that in the dielectric material Fe are given by Fo =
erV d + er s
(51)
Fe =
Fo er
(52)
286
Dielectric Phenomena in Solids
1 2 3
(b)
4
(a)
(c)
Figure 52 Three general electrode arrangements for forming thermoelectrets: (a) metallic electrodes deposited on both specimen surfaces, (b) a metallic electrode deposited on only one surface and the other surface bare, with an air gap between it and the forming metallic electrode, and (c) both surfaces bare with air gaps between bare surfaces and the forming electrodes. 1: Screening cage or heating chamber; 2: Upper metallic electrode; 3: Dielectric specimen; 4: Lower metallic electrode.
–
+
(a)
(b)
(c) F
T F (t )
Fp Tp Tg T (t ) To t0
t1
t2
t3
(d)
P
0
t1
t3
t
(e) Figure 53 Thermoelectrical electret formation processes: (a) prior to the application of an electric field, (b) during the poling process at a temperature T > Tg and a constant electric field, (c) alignment of dipoles in the electret after poling, (d) the temperature–time and electric field–time sequence in the poling process, and (e) the variation of polarization with time. Tp: poling temperature; Tg: glass transition temperature; To: normal ambient temperature; Fp: poling field.
Electrets
where V is the applied voltage across the system and d and s are, respectively, the material specimen thickness and the air gap length. For any applied voltage, the field in the air gap is Eg times larger than that in the material. The field required to cause electrical discharge in the air gap is about 30 kV cm1, and generally the field required to cause carrier injection from the electrode to the dielectric material is much larger (>100 kV cm1), depending on the potential barrier at the metal–dielectric interface. For this reason, it is easier and more convenient to use a system with one or two air gaps. When the applied voltage is large enough for Fo to reach the value to cause ionization in the air gap, real charges (electrons and ions) will be created and deposited on the material’s bare surface; electrons also may penetrate into the bulk and be trapped if the applied field is sufficiently high. This process should also be carried out at an elevated temperature to ensure that charges will penetrate to be trapped in deep traps in the material near the surface, ensuring the thermal stability of the electret. It is important to remember that the applied field must not be removed until the material has been cooled down completely to the normal ambient temperature. For the electrets of 5–10 mm in thickness, the air gaps are usually of the order of 0.1–1.0 mm. This method is simple and the electrets formed by it are stable, but it is a slow process and the lateral charge distribution in the electret is not uniform. When Eguchi made thermoelectrets in a Carnauba wax–beeswax mixture, the forming metallic electrodes were not in intimate contact with the material surfaces. There were tiny air gaps between the material surfaces and the adjacent forming electrodes. During the poling period with an electric field, the air gaps would break down, producing ions and electrons, which could be deposited as homocharges on the material surface. So, after the removal of the electric field and the forming electrodes, the charges on the electret surfaces were the sum of the heterocharges due to the frozenin aligned dipolar charges and the homocharges due to the electrical discharge in the tiny air gaps during the poling period.13–15 At the beginning, after the electret is formed, volume polarization is dominant. This is why
287
Eguchi observed the heterocharges appearing on the electret surface. But after a few days, he found that the polarity of the surface charges changed to the opposite of their original one, that is, homocharges appeared on the material surfaces. This was because the amount of dipolar charges decays with time, due to the continuous relaxation of the aligned dipoles to their randomized state. When such decay reaches a certain level, the deposited charges, which may have been trapped deep in the material just below the surface, may become dominant. This is why after a few days Eguchi observed homocharges appearing on the electret surfaces. 5.2.2 LiquidContact Method With this method, the bottom electrode of the dielectric material is either a vacuumdeposited metallic film or a simple metal plate, but the top forming electrode is generally made of fabric wetted with a conductive liquid, such as ethyl alcohol or water.16 Under an applied electric field between these two electrodes, the charges will be transferred from the top wetted electrode to the dielectric material surface, due to the interaction of the electrostatic and molecular forces at the interface during the contacting period, as shown in Figure 54. Since the top wetted electrode can be moved on the material surface, this method can be used to transfer charges over a large area of the material surface. It is also easy to control the charge density deposited on the surface and to make the lateral charge distribution comparatively uniform. Note that a certain time is required for the transfer of charges, so it is suggested to Deposited Charges Motion of the Top Metallic Electrode
Liquid Contact – – – – – + + + + + + + + + + +
Specimen Lower Metallic Electrode
Compensation Charges
Figure 54 Schematic illustration of the liquidcontact charging method.
288
Dielectric Phenomena in Solids
move the top electrode to one position and to leave it there for a short period (say, 10 to 20 minutes) to allow some time for the transferring process before moving it to the next position. The amount of charges or charge density on the surface depends on both the applied voltage and the poling time. 5.2.3 Corona Discharge Method With this method, the bottom electrode is a vacuumdeposited metallic film on the material surface, and the top forming metallic electrode is usually made of a metallic wire (e.g., tungsten wire), with one end polished to a sharp point so that voltage of only a few kV between the two electrodes is sufficient to create a field near the point electrode, exceeding the breakdown strength of the air in a region of a few millimeters around the point electrode. This is shown in Figure 55. Under this condition, corona discharge will occur, and negative and positive ions will be formed in the region near the point electrode, depending on the surrounding medium and the polarity of the point electrode. In air at one atmospheric pressure and humidity of 40–60%, negative ions such as CO3 and O2 are present when the point electrode is negative, and positive ions such as (H2O)nH+, NO+, and NO3+ are present when the point electrode is positive. For the negative point electrode, only negative ions can reach the dielectric material surface. These ions will then give up their attached electrons, becoming
Point Electrode Electret Material Metallic Electrode
Wire Grid
d1 d2
V1
V2
Screening Cage or Heating Chamber Figure 55 Schematic illustration of the corona discharge method.
neutralized, and return to the surrounding atmosphere, leaving a layer of negative trapped electrons just below the material surface. Similarly, when the point electrode is positive, positive ions, when reaching the material surface, will accept electrons from the material through the material–air interface, becoming neutralized, and return to the surrounding atmosphere, leaving a layer of positive trapped holes just below the material surface. Since the electric field distribution around a single point electrode is very nonuniform, with the field decreasing gradually with radial distance from the point, the distribution of the deposited charges on the material surface is also very nonuniform. To improve this situation, a metalwire grid can be placed between the point electrode and the material surface, as shown in Figure 55. The potential applied to the grid should be the same in polarity as, but lower in amplitude than, that of the point electrode. Some typical values are V1 = 8 kV, V2 = 0.5 kV, d1 = 4 mm, and d2 = 3 mm, the discharging time being about four minutes. With the grid, the distribution of the deposited surface charge is generally uniform if the discharging has reached such a level that the potential at the material surface approaches the potential of the grid. The corona discharge forming process can be carried out at normal ambient temperature, but the deposited surface charges may decay easily because the charges on the surface layer are mainly resting in shallow traps, so thermal stability is not very good. To remedy this situation, it is desirable to carry out the forming process at an elevated temperature. This may cause more charges to be captured in deep traps. Furthermore, the heating chamber also serves as a screening cage to prevent any exterior interference. The hightemperature corona discharge forming process also plays an indirect role in the annealing process to enhance the thermal stability of the electrets formed. The advantage of using a point electrode over a planar electrode, as shown in Figure 52(b), is that the applied voltage required to cause electrical discharge near the point electrode is much lower than that for the planar electrode, thus
Electrets
reducing the possibility of causing damage to the material surface from the bombardment of charged particles. It is worth mentioning that, if the surface potential and the current flowing to the bottom electrode to form compensating charges there can be measured continuously, then the surface charge density can be estimated during the charging process.17 5.2.4 ElectronBeam Method In order to produce real charges stored in the bulk of the material, we usually employ lowenergy electron beams with energy of the order of 10–50 keV, so that the range of the penetrating electrons is smaller than the dielectric material thickness. When this method is used to inject electrons into the material, the electrons will soon be trapped inside, forming negative trapped space charges. The energy of the electron beam should be controlled according to the structure and thickness of the material specimens to be used for forming electrets.18,19 For example, the energy of an electron beam of 10–50 keV is suitable for Teflon of 1–20 mm in thickness. A typical electron beam system is shown schematically in Figure 56. Beam scanning is required to control the uniformity of the distribution of the injected electrons. For a dielectric material specimen with a metallic electrode vacuumdeposited on the bottom surface and grounded, the energetic electrons from the beam, when striking the top bare surface, will generate electrons from the surface due to secondary emission, leaving a positively charged surface layer that is later neutralized by incoming slow electrons. The energetic primary electrons then penetrate into the bulk of the material and collide with molecules, creating electron–hole pairs, which may be quickly trapped but which will be occasionally released by thermal activation, contributing additional conductivity. This additional conductivity is generally referred to as radiationinduced conductivity (RIC). The magnitude of RIC depends on the dose and the energy of the electron beam, but in most practical cases, RIC is much larger than the intrinsic conductivity of the material.20 The original primary electrons, after one or more
Condenser Aperture
289
Electron Gun
Condenser Lens Scanning Coils Objective Lens Objective aperture
Backscattered Electrons Secondary Electrons
Absorbed Electrons
Figure 56 Schematic diagram of an electronbeam system.
collisions, lose most of their energy and are then trapped, forming negative charges located around the average range.20,21 The distribution of negative charges creates an internal field that tends to help the electrons to penetrate beyond the average range. In the RIC region, however, the electrons tend to move toward the interior of the material and the holes to move in the opposite direction. The motion of the electrons will gradually settle down to a thermal equilibrium state, resulting in a very stable distribution of negative charges and hence the formation of a negatively charged electret with high thermal stability. It has been found that for Teflon electrets formed by electron beam injection, the negative charge distribution is stable for a period of more than 10 years at normal ambient temperature (i.e., room temperature).22 The electronbeam method has the advantage of easily controlling the density, location, and lateral distribution of the injected negative charges. This is why it is widely adopted for forming electrets for research purposes and for practical applications. It should be noted
290
Dielectric Phenomena in Solids
that a similar ion beam technique, used for ion implantation in today’s semiconductor technology, is not normally used for injecting ions into a dielectric material for forming an electret. This is simply because much higher energy is required to inject ions than electrons into the same range in the material, so this technique would cause a lot of damage to the material. 5.2.5 Electromagnetic Radiation Method A dielectric material can be charged by the displacement of the charge carriers generated by various kinds of penetrating radiation, such as xrays or ultraviolet or visible lights, under an externally applied electric field. The electrets formed by xray radiation are generally referred to as radioelectrets. When ultraviolet or visible light is used, the electrets formed are generally called photoelectrets. The method is basically similar to that used by Vadjakov.4,5 The materials used for photoelectrets are generally photoconductive materials. A metallic electrode is usually deposited on one surface of the material specimen and a transparent electrode on the other surface, so that the light can illuminate the specimen through it. Sometimes it is desirable to have both electrodes transparent so that both the input light and the output light intensities can be measured, and hence, the photoelectron yield in the material can be determined. Under an electric field, the photogenerated carriers will be separated and will move toward the electrodes. These carriers may be trapped near the electrodes to create a space charge polarization. After the removal of the illumination and the electric field, this persistent polarization in the material forms a photoelectret, as shown in Figure 57. However, carrier trapping, detrapping, and retrapping occur continually during illumination. After the removal of the light, the charge distribution may become quasiequilibrium, but the polarization still decays gradually, even in the dark. Because the electrets formed by the photoelectric method are generally less stable than those formed by
other methods described here, this method is not widely used. The five methods described here are the major methods for forming electrets. Of course, they can be further improved by varying the performing ambients to suit the particular materials used for forming electrets. For example, for charging based on electrical discharge in air or other gas, we can change the pressure from the normal atmospheric pressure (760 torr) to a lower pressure (<100 torr) to produce electric discharge at a much lower voltage. The temperature during the forming process always plays an important role in the thermal stability of the electrets formed. An elevated temperature can provide a chance for the charges located in shallow traps to move to deep traps to stabilize the charge distribution, in other words, to improve the thermal stability of the electrets formed.
5.3 Charges, Electric Fields, and Currents in Electrets In general, electrets for practical applications are of the configuration shown in Figure 58. Such an electret is usually made of a thin dielectric material in sheet form or thinfilm form, with a metallic electrode deposited on the lower surface and the upper surface bare. Also, the upper floating planar metallic electrode is parallel to the bare surface with an air gap between them. The thickness of the electret is d and the air gap length is s. When the switch is on the A position, the specimen is being poled under a DC voltage V. Of course, we can use the thermoelectrical method described in Section 5.2.1. for the poling. If the poling voltage is sufficiently high to cause electrical discharge in the air gap, then after the poling period and the switch has been turned to the B position (open circuit), the electret formed will consist of quasipermanent trapped real charges on the bare surface, to form the surfacetrapped real charge density sr; quasipermanent trapped real charges in the bulk, to form the volumetrapped real charge density rr; and uniform
Electrets
291
– –
– – – – – – – – –
– +
(a)
+ + + +
–
–
–
+
(b)
+
+ +
+
–
– +
+
–
–
–
–
+ + + + + + + + + +
– – –
+ +
–
+ +
–
–
–
Light
+
+ +
(c)
Ip I
0
t1
t2
t
t2
t
(d) Fp F
0
t1
(e)
P
0
t1
t2
t
(f) Figure 57 Photoelectret formation processes: (a) prior to the application of light and an electric field, (b) displacement of photoinduced charges under light intensity Ip and electric field Fp, (c) charge distribution after poling, (d) the light intensity I–time t sequence, (e) the electric field F–time t sequence, and (f) the variation of polarization with time. Ip: light intensity at poling; Fp: poling field.
292
Dielectric Phenomena in Solids Upper Electrode x=d+s
sup +
+
+
+
+
Fo
sr sp
A x=d
x=0
– – – – + – – – – – + r – r + – + + +
– + – + – + – +
Lower Electrode
– – – – – + – – – – + Fe – + – + + + s1o
B
C
V
Figure 58 Arrangement of an electret and a floating upper electrode—the configuration most commonly used for applications. Switch on position A during poling period; switch on position B after being fully poled (open circuit); switch on position C under shortcircuit condition.
polarization P, composed of the quasipermanent frozenin dipolar polarization PP and the instantaneously induced polarization Pi, which follows the poling field F. Thus P = PP + Pi
(53)
where Pi = (e r  1)e o F
(54)
in which er is the dielectric constant of the electret material. PP may consist of not only the frozenin dipolar polarization, which is normally invariable with x, but also possibly a component due to charge displacement in the structural discontinuity. However, P would create a local volume charge with the local charge concentration given by r P =  dP dx
(55)
The polarization P also creates a bound surface charge density on the bare surface, which is given by s P = P
(56)
Assuming that the lateral dimensions (i.e., the y and z directions perpendicular to the x direction) are much larger than d and s, and that the lateral distributions of sr, rr and P are invariable with y and z, implying that they vary only with x; then after the poling (charging)
process, the electret can be characterized by the following two charge equations: s (d ) = s r (d ) + s P (d ) = s r  P
(57)
dP dx
(58)
r( x ) = r r ( x ) + r P ( x ) = r r 
In this section, we shall deal with two general cases. Case I: The Electret Has Only Surface Charges In this case we have r( x ) = O s (d ) = s r  P
(59)
When the switch is turned to the C position (shortcircuit), the voltage between the two electrodes is zero. In this case, the compensation charges on both electrodes will rearrange in such a way that the two electrodes shield all charges stored in the electret. The compensation charges on the lower and the upper electrodes, slo and sup, respectively, must satisfy the Gauss’s law. Thus, s lo + s up = s
(510)
Therefore, there is no current flowing through the short circuit because there is no potential between the two electrodes. So
Electrets
Fed = Fos
(511)
where Fe and Fo are, respectively, the electric fields inside the electret and in the air gap. Equation 510 can be rewritten in terms of Fe and Fo as e re o Fe + e o Fo = s
(512)
From Equations 511 and 512, we obtain Fe = 
ss (e r s + d )e o
(513)
Fo = 
sd (e rs + d )e o
(514)
and the voltage across the electret Ve and that across the air gap Vo as Ve = 
Vo = 
sd Êe + d ˆ e Ë r s¯ o sd = Ve Êe + d ˆ e r o Ë s¯
(515)
(516)
From Equations 510, 513, and 514, we obtain the relations between slo or sup and s, which are s lo = 
e r ss er s + d
(517)
s up = 
ds er s + d
(518)
It can be seen that with this configuration, even d is constant. Varying the air gap length s will cause a change in both Fe and Fo and hence in compensation charges on the electrodes slo and sup. The change in slo and sup implies that there will be a current flow through the short circuit. If there is a load (e.g., resistor) connected between the two electrodes instead of a short circuit, then an electrical signal will appear across the load when the air gap s is changed by an external force. Many applications of electrets are based on this simple principle. We shall discuss this more in Section 5.9. If we move the upper electrode to infinity (i.e., make s Æ •), we have the fields in the electret and in the air gap as
Fe = 
Fo = 
s s =e re o Êe + d ˆ e Ë r s¯ o s Ê e s + 1ˆ e Ë rd ¯ o
=
s d Æo e re o s
293
(519)
and the potential across the electret and air gap as Ve = Vo = 
sd e re o
(520)
which is independent of s. This is equivalent to saying that sup Æ 0, according to Equation 518. So, instead of moving the upper electrode to infinity, if we apply a voltage equal in magnitude but opposite in polarity to the potential Vo to compensate the potential across the air gap, then the voltage across the electret is still the same as that given in Equation 520. We can use this idea to determine the surface charge density. This is generally referred to as the compensation method and will be discussed in Section 5.4.
Case II: The Electret Has Both Surface Charges s(d) and Volume Charges r(x) The convenient way to deal with this situation is to convert the volume charges per unit planar area to an equivalent surface charges per unit area sr. This means that the effect of r(x) in the bulk is equivalent to that of sr on the bare surface. sr can be called the projected or the equivalent surface charge density, which is given by sr =
1 d xp( x )dx d Úo
(521)
Thus, the total surface charge density sT can be written as sT = s + sr = sr  P + sr
(522)
By replacing s with sT, all equations from Equation 513 to Equation 520 can be used for the evaluation of Fe, Fo, Ve, Vo, slo, and sup. However, to calculate sr, we must know the spatial distribution of r(x), which is difficult to find theoretically. It can, however, be deter
294
Dielectric Phenomena in Solids
mined experimentally. This will be discussed in Section 5.6. For practical applications, we always want Ve as large as possible to increase the sensitivity of the electret to respond to external signals. But the air gap s is a limiting factor, so s should be chosen so that Vo across the air gap is below the electrical breakdown voltage of the air gap. This directly limits the value of Ve. For example, with a Teflon electret of 20 mm in thickness (d) and the air gap of 40 mm in gap length (s), the breakdown voltage of the air gap at normal atmospheric pressure and temperature is 500 V for ps (gas pressure ¥ air gap length) equal to 40 mm ¥ 760 mmHg = 3.04 mm(Hg)  cm, based on Paschen’s law.23 This means that since Ve = Vo, the maximum value for Ve is 500 V. Normally, the allowable value for Ve in this case is about 200–300 V. Since sT = ereoVe /d, if we want a large Ve, we must make sT larger by producing more surface and volume charges in the electret. However, if sT is fixed, we can always adjust s to ensure that electrical breakdown will not occur in the air gap. In electrets, there always exist mechanical forces induced by the electric fields on the material. As discussed in Electromechanical Effects in Chapter 2, the mechanical forces per unit area acting on both the upper and the lower electrodes and tending to pull them toward the electret surface are given by Fo =
1 e o Fo2 2
(523)
pulling the upper electrode downward, and Fe =
1 e re o Fe2 2
(524)
pulling the lower electrode upward. All kinds of charges stored in electrets will give rise to a current flow, which may be due to a change of temperature, exposure to light, temporal variation of the electric field, decay of charges with time and so on. The parameters, P, sr, r, and Fe are not really time invariant. They are functions of time because they are always subjected to decay processes. In general, the current density in the electret can be written as
je (t ) = e re o
∂ Fe ∂ P + + jg ∂t ∂t
(525)
where the first term on the right side of equation 525 is the displacement current due mainly to the variation of s with time, the second term is due to the depolarization (dipolar relaxation), and the last term is due to intrinsic conductivity and the presence of thermally released trapped charge carriers (real charge decay processes).
5.4 Measurements of Total Surface Charge Density and Total Charges The total charges in the electret per unit planar area are given by d
QT = s + Ú r( x )dx o
(526)
and the total surface charge density is given by sT = s +
1 d xr( x )dx d Úo
(527)
There are several methods available to determine the total surface charge density sT, total charges per unit planar area QT, and the volume d charges Úo r(x)dx per unit planar area. This section reviews some commonly used methods for these measurements. 5.4.1 Total Surface Charge Density In this section we shall describe two methods for the measurement of the total surface charge density. Compensation Method In Section 5.3, we derived equations for the voltages across the electret and across the air gap for the electret with one surface metallized and one surface bare, and with a floating metal electrode above the bare surface and an air gap between them (see Figure 58 and Equations 515 and 516. When s Æ • we have Ve = Vo = 
sTd e re o
Electrets
295
Floating Upper Electrode +
+
+
+
+
Vo
s
Electrometer
– – – – – – – – – d + Lower Electrode
Ve
Electret +
+
+
+
+
Vibrator
+
+ Vo
Figure 59 Schematic illustration of the compensation method for the measurement of total surface charge density on the charged electret.
and so sT = 
e re o Ve d
(528)
Thus, by moving the floating electrode a large distance from the bare surface of the electret so that s >> d, sT can be measured simply by connecting a variable DC voltage supply between the lower electrode and ground, and an electrometer between the floating electrode and ground, as shown in Figure 59. Adjusting the applied DC voltage until it is equal to the electrometer reading, the electrometer reading is Ve, since the applied DC voltage has balanced out the voltage across the air gap Vo. This is why this method is called the compensation method. Knowing Ve, we can calculate sT from Equation 528. This method is simple, and it is independent of the air gap length s, so it does not involve the measurement of s. The sensitivity of this method can be improved by attaching a mechanical vibrator to the lower electrode to cause the electret to vibrate, as shown in Figure 59. The vibrator can be a simple loudspeaker. The vibration will cause the variation of s, and hence the voltage reading in the electrometer has an AC component. However, if Vo can be completely balanced out by adjusting the compensation voltage precisely, the AC component should disappear.24,25
Capacitive Probe Method For the electret with one metallized surface and one bare surface, we can use the capacitive probe method to measure the total surface charge density sT.26 With this method, a metal probe of area A is placed in parallel with the bare surface, with a relatively large air gap between them. The probe is connected to a large capacitor of capacitance C, much larger than the capacitance between the probe and the electrode, as shown in Figure 510. A shutter shields the probe from the field of the electret. When the shutter is removed and the probe is exposed to the field from the charged electret, a charge of Asup will flow into the capacitor C creating a voltage across it. Thus V=
As up C
(529)
The share of the induced charges on the lower electrode and the probe (i.e., the upper electrode) is similar to that under a shortcircuit condition. From Equation 518, s T = (1 + e r s d )s up = (1 + e r s d )
CV (530) A
The lateral charge distribution is usually different from the charge distribution in the bulk. If the probe can be made small enough, the lateral charge distribution can be determined by this capacitive probe method. This method can also
296
Dielectric Phenomena in Solids Movable Shutter Charged Electret Electrode
Metal Probe sT s – – – – – – – – – – d
Electrometer
C
Figure 510 Schematic diagram showing the capacitive probe method for the measurement of the total surface charge density in a charged electret.
be used for the electrets with both surfaces bare (nonmetallized). 5.4.2 Total Charges per Unit Planar Area QT In this subsection we shall describe two methods for the measurements of the total charge. Electrostatic Induction or Faraday Pail Method The Faraday pail method is a classic, basic electrostatic induction method for measuring total electrostatic charges in an electret with both surfaces bare (without metallic electrodes). To measure QT, we simply put the charged electret into a metallic Faraday pail, as shown in Figure 511. Based on the principle of electrostatic induction, the charges in the electret QT will induce +QT on the inner surface and QT on the outer surface of the pail. If the collective capacitance of the system and the electrometer is C and the voltage measured by the electrometer is V, then QT = CV
(531)
For electrets with both surfaces metallized, we must use the shaving technique to shave very thin layers of both metallic electrodes off the electret at low temperature to avoid any loss of the stored charges in the electrets. After the thin metallic layers have been removed, the same method can be used to measure QT. Thermal Pulse Method The total charges and the centroid of the charges can be measured by means of the
Negatively Charged Electret Metallic Faraday Pail –+ –+ –+ –+ –+ –+ –+ –+
– – – – – – – – – – – – – –
+– +– +– +– +– +– +– +–
C
Electrometer
Insulation Stand Figure 511 Experimental arrangement for the measurement of the total charges in a charged electret using a Faraday pail.
Sensing Guarded Electrode
Recorder Amplifier
x=d+s Air Gap
VoGuard Ring V y
x=d x=0
Charged Electret Ve Electrode Light Pulse
Figure 512 Schematic diagram showing the thermal pulse method for the measurement of the volume charge distribution in a charged electret.
thermal pulse method.27–30 The experimental arrangement for these measurements based on this method is shown schematically in Figure 512. The basic principle is to measure the change of the potential across the electret during diffusion of the thermal energy pulse generated by a short light pulse through the lower electrode at x = 0. Prior to the application of the thermal pulse, the voltmeter meas
Electrets
ures mainly the applied DC voltage V plus the voltage between the floating electrode and the lower electrode, which is, in fact, the difference between Ve and Vo. When a short light pulse illuminates the electret through the thin lower metallic electrode, the light energy will be absorbed by the electret material, generating a heat (thermal energy) pulse. The original potential at the bare surface is Ve = sT d/ereo. The change of this potential by DV is due to the effect of the thermal pulse, which results in thermal expansion of the material (change in d) and variation of the dielectric constant (change in er). Thus, by measuring the net change DV(t1) taken at time t1 immediately following the illumination, and V(t2) taken at time t2 after the change has reached its thermal equilibrium, we can write s T DV (tz ) = QT DV (ti )
(532)
since DV(t1) is related to sT due to the change of d and er, while DV(t2) is related to the diffusion of the volume charges from x = 0 to x = d. Therefore, to determine QT, we need two measurements: one to measure sT (from one of the methods given in Section 5.4.1) and the other to measure DV(t1) and DV(t2), using the thermal pulse method based on Equation 532. d The centroid of the volume charges Úor(x)dx measured from the lower electrode x = o is defined by d
Xo =
Ú xr( x )dx Ú r( x )dx o
d
(533)
o
If s is much smaller than the volume charges Údor(x)dx, then s can be ignored. Thus for this case, Equations 526 and 527 can be simplified to sT =
1 d xr( x )dx d Úo d
QT = Ú r( x )dx o
(534) (535)
From Equations 532 and 533, we obtain Xo DV (t2 ) = DV (t1 ) d
(536)
297
So, using the thermal pulse method, we can also determine the centroid of the volume charges and the total volume charges Údor(x)dx from Equation 536.
5.5 Charge Storage Involving Dipolar Charges In general, all electrets consist of both dipolar and real charges. But in dipolar materials, such as semicrystalline polyvinylidenefluoride (PVDF), the dipolar polarization is dominant. In this case, the small contribution from the real charges, if any, can be ignored in order to simplify the analysis. In this section, we shall deal with cases involving only dipolar charges. 5.5.1 Basic Poling Processes In Section 5.2.1, we discussed the thermoelectrical method of forming an electret by simultaneous application of an electric field and heat (at T > Tg). It should be noted that the average amount of the dipole moment per dipole aligning in the direction of the poling electric field F is less than uo, which is the permanent dipole moment of each dipolar molecule in the dipolar material. The value of uo is not affected by the field and the temperature. During the poling process, the polarization P increases with time because the amount of the dipole moments aligning in the direction of the field increases with time. Supposing that the material consists of only one type of dipoles, then the polarization P is governed by the Debye equation (see Electric Polarization and Relaxation in TimeVarying Electric Fields in Chapter 2) dP P e o (e rs  e r • )F + = tp dt t p
(537)
where ers and e• are, respectively, the static and optical dielectric constants and tp is the relaxation time of the dipoles, which is temperature dependent following an exponential relation t p = t po exp( H kT )
(538)
where H is the potential barrier height for the dipole orientation and the tpo is the average
298
Dielectric Phenomena in Solids
time required by an excited molecule to turn from one equilibrium direction to the other.31 For the isothermal poling condition and the initial boundary condition P(t = 0) = 0 at F = 0, the solution of Equation 537 gives P(t ) = e o (e rs  e r • )F[1  exp( t t p )]
(539)
When P(t) reaches saturation, as shown in Figure 53, P becomes P = e o (e rs  e r • )F
(540)
It should be noted that during the charging (poling) process, the dielectric constant er is a function of temperature. But for the present analysis, we assume that the variation of er with temperature is not appreciable and can be ignored. By doing so, the total charging current density can be written as jc (t ) = dP(t ) dt + g(T )F
(541)
where g(T) is the electrical conductivity of the material. Substitution of Equation 539 into Equation 541 yields jc (t ) =
P È t 1 t t p ˘ exp Í Ú e dt ˙ + g(T )F tp Î otp ˚
(542) The first term on the right side of Equation 542 is the charging current, which is due to the orientation of the dipoles toward the direction of the poling field, and the second term is the conduction current due mainly to the motion of charge carriers thermally generated inside the material. The charging (polarization) current follows a transient process, giving rise to a peak if the temperature increases continuously, but the conduction current always increases with increasing temperature. So by measuring the jc – T characteristics at a constant applied electric field, we can separate the contribution of these two components to the total current jc. After the poling temperature has been cooled to the ambient temperature To and the applied electric field F has been removed, P(t) will decay with time due to thermal relaxation at To. The decay process is governed by the following equation: dP(t ) P(t ) + =0 dt tp
(543)
In this case, the initial boundary condition is at t = 0, P(t = 0) = P (0) = Po = eo (ers  er•) F. Thus, the solution of Equation 543 is P(t ) = P( 0)exp( t t p )
(544)
Since tp is a function of temperature, the rate of the decay depends on temperature: The lower the temperature, the slower the decay process. At a constant temperature, the aligned dipoles are constantly subjected to thermal relaxation, resulting in a continuous depolarization in the electret. So the stored charges can be said to be only quasipermanent. 5.5.2 Relaxation Times of Dipoles and the Thermally Stimulated Discharge Current (TSDC) Technique In many materials, and particularly in polymers, there exist several relaxation times, implying that there are several types of dipoles that may be associated with side groups of the molecular chains and their mutual interactions. These can be measured by means of the thermally stimulated discharge current (TSDC) technique. This is a very powerful technique for determining the distributions of the relaxation times of dipoles and the energy levels of carrier traps, and for studying the charge decay processes.32,33 To measure the relaxation times of dipoles, we shortcircuit the poled electret and measure the discharge current as a function of temperature at a constant rate of increase in temperature, as shown in Figure 513. To start with, we make the electret a fully poled electret, following the thermoelectrical poling process described in Section 5.2.1. After that, we measure the shortcircuit discharge current jd, that is, TSDC, while the electret is heated gradually by slowly increasing the temperature at a rate of b = dt/dt (e.g., b = 1°C min1). At T = T0 during detention, jd = 0, since the compensation charges on both electrodes are bound charges compensating the polarization charges in the material. When the temperature rises, T > T0, the persistent polarization begins to decay, which means the average amount of dipole moments aligning along the direction of the poling field
Electrets
299
1 Electrometer
2
1. Heating Chamber 2. Upper Electrode 3. Dielectric Specimen 4. Lower Electrode
3 B
A 4
(a) T F (t ) Tp
T (t )
Tg
To
To t0
t1
t2
t3
t4
t
t3
t4
t
(b)
P
0 t1 (c) Poling
Storage
TSDC measurement
jd
To
Tm1
Tm2
T
(d) Figure 513 Schematic illustration of the experimental steps for the TSDC measurement: (a) arrangement for forming a thermoelectret—with switch on the A position, (b) the temperature–time and electric field–time sequence in the poling process, (c) the variation of polarization with time, and (d) the current jd as a function of the temperature during TSDC measurement—with switch on the B position.
300
Dielectric Phenomena in Solids
starts to decrease; hence, the amount of bound charges on the electrodes required for compensating the polarization charges also decreases. Some of the bound charges become released and free to contribute to the shortcircuit current jd. This discharge current is similar to the discharge current from a charged capacitor, which reveals the mechanism responsible for the polarization. From Equation 544, the discharging current density jd is given by (545)
jd (t ) = dP dt =  P(t ) t p
in which P(t) cannot be expressed in the simple form given in Equation 544 because P(t) during the TSDC process is also a function of temperature T and T is a function of t. For this reason, the appropriate expression for P(t) is33
and letting z = H/kT, the integration would be in the following form:
Úe
z
1 2! 3! 4! d Ê ˆ = e  z z 2 Ê1  + 2  3 + . . . ˆ Ë z¯ Ë ¯ z z z
(550) For most dielectric materials, z = H/kT > 40, and it is reasonable to truncate the series after the second term. However, this is still quite mathematically involved. So a reasonable approximation is needed in order to see easily the discharging process. An approximation in good agreement with experiments is given by jd (T ) = C2 È H ˘ C1 exp Íexp(  H kT )˙ 2 Î kT ( H kT ) ˚
(551) È t dt ˘ P(t ) = P( 0)exp Í Ú ˙ Î o t p (t ) ˚
(546)
If the temperature is raised linearly with time at the rate b (b = dT/dt), Equation 545 can be written as jd (T ) = 
P( 0) È 1 exp Ít p (T ) Î b
Ú
T
To
dT ˘ t p (T ) ˙˚
(547)
For a material having only one relaxation time, (i.e., only one type of dipoles), P(o) can be expressed as P( 0) = e o [e rs (T )  e r • ]F =
(548)
Nmo2 F 3e o kT
where N is the number of dipoles per unit volume. Since ers(T) is temperature dependent, P(0) is temperature dependent, but the temperature dependence of tp is much stronger than that of P(0). To simplify matters, we will ignore the temperature dependence of P(0) for the following analysis. Since tp = tpoexp(H/KT), the integral T dT ÚTo t p (T ) can be solved by partial integration, which leads to a solution in an asymptotic expansion.32,34 By expressing dT H ÚTo t po exp( H kT ) = kt po T
Ú
T
To
e
H k T
Ê 1 ˆ dÁ ˜ Ë H kT ¯
(549)
where C1 and C2 are adjustable constants.35–37 Equation 551 indicates that the thermally stimulated depolarization current starts out slowly, increases exponentially, and then reaches a peak value. After reaching the peak, it drops rapidly as the temperature is raised continuously, and then to zero when the arrangement of all dipoles becomes completely randomized. In Equation 551, the first term is dominant at low temperatures, that is, at T < Tm where Tm is the temperature for the occurrence of the peak current. Thus, the slope of the jd  T curve, based on Equation 551, at low temperatures would yield the value of H as follows: d[ln jd (T )] H =dT k
(552)
By differentiating jd with respect to T and setting it to zero, we would find the temperature Tm at which jd becomes maximal. Under this condition, we have the following relation dt p dT
=T =Tm
1 b
(553)
Substitution of Equation 538 into Equation 553 yields kTm2 =1 bHt p (Tm )
(554)
Thus, from Equation 552 we can determine H, the potential barrier height that the dipoles must
Electrets
Ê Hi ˆ t p = Â t pi = Â t poi expÁ ˜ Ë kT ¯ i i
(555)
10–10
a
r
b jd (A)
surmount in order to proceed with the orientation. From Equation 554 we can determine tp at Tm, which can be found from the TSDC thermogram ( jd  T curve). In dipolar materials the TSDC peak may arise from a single relaxation with one relaxation time or from a distributed relaxation with several relaxation times. When TSDC thermograms are measured under various poling conditions, the shape and the temperature for the occurrence of the current peak do not depend on the poling conditions if there is one relaxation time, but they do if there are several relaxation times. This is because the fastand slowrelaxing dipoles behave differently for different electret formation and storage times.32,33 A good example with a single relaxation can be found in ionic crystals, such as alkali halides, doped with divalent impurity ions, which coupled with their accompanying vacancies, will form the I–V dipoles.33 In many materials and particularly in polymers, however, there exist several relaxations, the most common ones being the g, b, a, and r relaxations. The g relaxation is associated with the motion of the dipoles within the side groups of the molecular chains, the b relaxation is due to the motion of the side groups themselves, and the a relaxation is caused by the joint motions of the side groups and the main chains. These three relaxations are directly related to the reorientation of dipoles, while the r relaxation is due mainly to the motions of real charges (space charges). Depending on the difference in activation energy DH between two types of dipoles, the two current peaks in the TSDC thermogram may merge to form one broad peak if DH is smaller than a few kT; otherwise, two separate peaks will appear. For PMMA (polymethyl methacrylate), four current peaks associated with the four relaxations can be monitored clearly, as shown in Figure 514. If the material possesses several groups of different relaxations, then Equation 538 must be written as the sum of a number of relaxations
301
10–11
g
10–12 –150 –100 –50 0 50 Temperature (°C)
100
150
Figure 514 Thermally stimulated discharge current (TSDC) thermogram (recorded at 5°C min1) of polymethyl methacrylate (PMMA) electret, specimen area being 19.6 cm2 and poled at 10 kV cm1 at 127°C for 30 min.33
where the subscript i specifies the ith group of dipolar relaxation. Each group will contribute to the polarization and the TSD current, so the total polarization or total TSD current is simply the algebraic sum of the contributions from all individual groups. It is also important to note that Equation 538 holds only for relaxations involving the reorientation of small dipoles. It becomes invalid for relaxations involving large dipoles in macromolecular materials such as polymers—particularly when the temperature reaches the glass–rubber transition state in which the motion of the large dipoles involves configurational rearrangement of parts of the long main chains because the motion of such bulky dipoles requires some unoccupied space. In this case, we must use the WLF empirical relation (WLF stands for Williams, Landel, and Ferry)32,33 instead of Equation 538. t r (T ) = t g exp[ Ca (T  Tg ) (Cb + T  Tg )] for T > Tg
(556)
where tg is the relaxation time in the glass state, Tg is the glass transition temperature, and Ca and Cb are constants. By approximation, Equation 556 may be reduced to a form similar to Equation 538, as follows t r = t w exp[ Hw k(T  Tw )]
(557)
where tw = tg exp (Ca), Hw = CaCb k, and Tw = Tg  Cb. This relation becomes invalid for T < Tg.
302
Dielectric Phenomena in Solids
5.5.3 Spatial Distribution of Dipolar Polarization
a r
jd /eoF (s–1)
If the poling field is uniform in the material specimen, the spatial distribution of the dipolar polarization is expected to be uniform. However, if volume space charges also exist inside the specimen, the charges will be separated: positive charges moving to the negative electrode and negative charges moving to the positive electrode, forming a space charge polarization. These heterocharges near the forming electrodes tend to lower the applied poling field near the center of the specimen, resulting in a smaller dipolar polarization in the center than that in the region near the electrodes, because dipolar polarization is field dependent. If the poling process also involves charge carrier injection, then the homocharges will cause the distribution of the field and hence the dipolar polarization will be nonuniform spatially in the specimen. The spatial distribution of dipolar polarization can be determined simply by the sectioning method, which is discussed in Section 5.6.1. For dipolar polarization measurements, thin metallic electrodes must be deposited by fast evaporation of gold on both surfaces of each slice cut out from the electret to avoid heating the specimen. Then we can measure the discharging current using the TSDC technique. The polarization can then be evaluated by integration of the TSDC spectrum based on P = • Ú o Jddt. If the electret is cut into many slices, the distribution of P(x) can be obtained by assembling the data from each slice. Let us take a PMMA electret as an example. The electret was cut into three slices: one near the center and other two near the electrodes. Figure 515 shows the TSDC thermograms of the slices cut out from the PMMA electret. The data of these curves are from Tounhout.32 It can be seen that the polarization near the center of the electret is significantly smaller than near the two electrodes, indicating clearly that the PMMA electret has heterocharges near the electrodes that cause the lowering of the poling field and hence the polarization near the center, since polarization increases with increasing
10–3
upper
10–4
lower middle section
10–5 20
60 100 Temperature (°C)
140
Figure 515 TSDC thermograms of three sectional slices of a PMMA electret showing the slices near the upper and lower electrodes having a higher polarization than the slice from the center. The specimen thickness was 4.8 mm and poled at 20 kV cm1 at 140°C for 1.5 hours; jd recorded at 0.5°C min1.32
poling field. This implies that the electret has not only the dominant dipolar charges but also real space charges. 5.5.4 Isothermal Polarization Decay Processes The retention of the dipolar charges depends on the structure of the material, which is directly related to tp and the operating and environmental conditions. In general, dielectric materials exhibiting good dipolar properties have a relatively high conductivity, due partly to their hygroscopic behavior. These materials, such as ceramic materials and some dipolar polymers, tend to absorb moisture from the surrounding environment. Dielectric materials with a low conductivity are usually not dipolar. The value of tp depends on the material parameters, such as the crystallinity and the arrangement of various dipolar groups (various types of dipoles), particularly for organic polymers, which are directly associated with the structure of the material38; the dopants, which are chosen to increase the potential barrier height responsible for dipolar relaxation so as to improve the
Electrets
retention time39,40; crosslinking for polymers; hygroscopic behavior, and so forth. The eff